Superconductivity Physics and Applications
Kristian Fossheim and Asle Sudbø The Norwegian University of Science and Tec...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Superconductivity Physics and Applications

Kristian Fossheim and Asle Sudbø The Norwegian University of Science and Technology Trondheim, Norway

c 2004 Copyright

John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex PO19 8SQ, England Telephone (+44) 1243 779777

Email (for orders and customer service enquiries): [email protected] Visit our Home Page on www.wileyeurope.com or www.wiley.com All Rights Reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning or otherwise, except under the terms of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London W1T 4LP, UK, without the permission in writing of the Publisher. Requests to the Publisher should be addressed to the Permissions Department, John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex PO19 8SQ, England, or emailed to [email protected], or faxed to (+44) 1243 770620. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the Publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. Other Wiley Editorial Offices John Wiley & Sons Inc., 111 River Street, Hoboken, NJ 07030, USA Jossey-Bass, 989 Market Street, San Francisco, CA 94103-1741, USA Wiley-VCH Verlag GmbH, Boschstr. 12, D-69469 Weinheim, Germany John Wiley & Sons Australia Ltd, 33 Park Road, Milton, Queensland 4064, Australia John Wiley & Sons (Asia) Pte Ltd, 2 Clementi Loop #02-01, Jin Xing Distripark, Singapore 129809 John Wiley & Sons Canada Ltd, 22 Worcester Road, Etobicoke, Ontario, Canada M9W 1L1 Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Library of Congress Cataloging-in-Publication Data Fossheim, K. (Kristian) Superconductivity : physics and applications / Kristian Fossheim and Asle Sudbo. p. cm. Includes bibliographical references and index. ISBN 0-470-84452-3 (alk. paper) 1. Superconductivity. I. Sudbo, Asle. II. Title. QC611.92.F67 2004 537.6 23 – dc22 2004002271 British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library ISBN 0-470-84452-3 Typeset in 10.5/13pt Times by Laserwords Private Limited, Chennai, India Printed and bound in Great Britain by Biddles Ltd, King’s Lynn This book is printed on acid-free paper responsibly manufactured from sustainable forestry in which at least two trees are planted for each one used for paper production.

Contents Preface

xi

Acknowledgements

I 1

BASIC TOPICS

1

What is superconductivity? A brief overview

3

1.1 1.2 1.3 1.4 1.5 1.6 1.7 2

xiii

Some introductory, historical remarks Resistivity The Meissner effect: perfect diamagnetism Type I and type II superconductors Vortex lines and flux lines Thermodynamics of the superconducting state Demagnetization factors and screening

3 6 10 13 17 18 23

Superconducting materials

27

2.1 2.2

27 27 27 29 31 31 34 35 35 37 37 40 41 42

2.3

2.4 2.5 2.6

Introductory remarks Low-Tc superconductors 2.2.1 Superconducting elements 2.2.2 Binary alloys and stoichiometric compounds Organic superconductors 2.3.1 Polymer and stacked molecular type 2.3.2 Fullerene superconductors Chevrel phase materials Oxide superconductors before the cuprates High-Tc cuprate superconductors 2.6.1 The discovery of cuprate superconductors 2.6.2 Composition and structure 2.6.3 Making high Tc materials 2.6.4 Phase diagrams and doping 2.6.5 Some remarks on the original idea which led to the discovery of cuprate superconductors 2.6.6 Thermal fluctuations of the superconducting condensate. A preliminary discussion

47 48

vi

CONTENTS

2.7 2.8 2.9 3

4

52 53 55

Fermi-liquids and attractive interactions

57

3.1 3.2 3.3 3.4

57 59 61 66 66 71 75

Introduction The non-interacting electron gas Interacting electrons, quasiparticles and Fermi-liquids Instability due to attractive interactions 3.4.1 Two electrons with attractive interaction 3.4.2 Phonon-mediated attractive interactions 3.4.3 Reduction of the effective Hamiltonian

The superconducting state – an electronic condensate 4.1 4.2 4.3 4.4 4.5

4.6

4.7

5

Heavy fermion superconductors MgB2 superconductor Summarizing remarks

BCS theory: a magnetic analogue Derivation of the BCS gap equation Transition temperature Tc and the energy gap Generalized gap equation, s-wave and d-wave gaps Quasi-particle tunnelling and the gap 4.5.1 Introductory remarks 4.5.2 The tunnelling principle 4.5.3 Single-particle NIN tunnelling 4.5.4 NIS quasiparticle tunnelling 4.5.5 SIS quasiparticle tunnelling BCS coherence factors versus quasiparticle-effects: ultrasound and NMR 4.6.1 Introductory remarks 4.6.2 Transition rates in ultrasound propagation and NMR 4.6.3 Longitudinal ultrasonic attenuation 4.6.4 Transverse ultrasound 4.6.5 Nuclear magnetic resonance relaxation below Tc The Ginzburg–Landau theory 4.7.1 Some remarks on Landau theory 4.7.2 Ginzburg–Landau theory for superconductors 4.7.3 Flux quantization

79 79 81 87 89 94 94 95 97 99 102 103 103 104 105 108 113 115 115 117 121

Weak Links and Josephson Effects

123

5.1

123 123 125 128 129 131

5.2 5.3

Weak links, pair tunnelling, and Josephson effects 5.1.1 Introductory remarks 5.1.2 DC Josephson effect: the Feynman approach AC Josephson effect 5.2.1 Alternative derivation of the AC Josephson effect Josephson current in a magnetic field

CONTENTS

5.4 5.5 5.6 5.7 5.8 6

London Approximation to Ginzburg–Landau Theory (|ψ| constant) 6.1

6.2

6.3 6.4 6.5 6.6 6.7

7

The London equation and the penetration depth λL 6.1.1 Early electrodynamics and the London hypothesis 6.1.2 Derivation of the London equation from the free energy The energy of a single flux line 6.2.1 Energy of a flux line: alternative derivation. An exercise Interacting flux lines: the energy of an arbitrary flux line lattice Self energy of a single straight flux line in the London approximation Interaction between two parallel flux lines Interaction between two flux lines at angle α General flux-line lattice elastic matrix in the London approximation

Applications of Ginzburg–Landau Theory (|ψ| spatially varying) 7.1 7.2 7.3 7.4 7.5

7.6 7.7 8

The SQUID principle The Ferrell–Prange equation The critical field Hc1 of a Josephson junction Josephson vortex dynamics Josephson plasma in cuprate high-Tc superconductors

The temperature-dependent order parameter |ψ(T )| The coherence length ξ 7.2.1 Relations between λ, ξ and Hc Two types of superconductors The structure of the vortex core The length ξ and the upper critical field Bc2 7.5.1 Isotropic systems 7.5.2 Bc2 , ξ , and λ in anisotropic superconductors Ginzburg–Landau–Abrikosov (GLA) predictions for Bc2 /Bc1 Surface superconductivity and Bc3

vii 134 136 138 139 140

141 141 141 146 148 151 154 160 162 164 166

171 171 172 174 175 180 182 182 184 188 190

More on the Flux-line System

199

8.1

199 199 200 201

8.2

Elementary pinning forces and simple models 8.1.1 The concept of a pinning force 8.1.2 Pinning force and flux gradient Critical state and the Bean model

viii

CONTENTS

8.3

8.4 8.5

8.6

8.7

II 9

Flux-line dynamics, thermal effects, depinning, creep and flow 8.3.1 TAFF, flow and creep: Definitions 8.3.2 Flux flow 8.3.3 Thermally activated flux creep: Anderson model Single particle TAFF FLL elasticity and pinning 8.5.1 Collective effects 8.5.2 Collective creep: inverse power law U (J ) 8.5.3 Logarithmic U (J ) 8.5.4 The vortex solid–liquid transition 8.5.5 Lindemann criterion and melting of a clean flux-line system 8.5.6 Modelling non-linear vortex diffusion Flux-line entry at Bc1 : thermodynamic and geometric restrictions 8.6.1 The critical field Bc1 8.6.2 The Bean–Livingston barrier 8.6.3 Geometric barriers Critical current issues 8.7.1 Critical current in the Meissner state 8.7.2 Depairing critical current 8.7.3 Reduction of Jc at grain boundaries 8.7.4 Relaxation of magnetic moment and the irreversibility line 8.7.5 How can Jc be increased?

204 204 205 206 207 208 208 212 213 215 218 224 228 228 229 232 233 233 234 235 236 242

ADVANCED TOPICS

247

Two-dimensional superconductivity. Vortex-pair unbinding

249

9.1 9.2 9.3 9.4 9.5 9.6 9.7

249 250 251 255 257 264 271

Introduction Ginzburg–Landau description Critical fluctuations in two-dimensional superfluids Vortex–antivortex pairs Mapping to the 2D Coulomb gas Vortex-pair unbinding and Kosterlitz–Thouless transition Jump in superfluid density

10 Dual description of the superconducting phase transition 10.1 10.2

Introduction Lattice formulation of the Ginzburg–Landau theory 10.2.1 Lattice Ginzburg–Landau model in a frozen gauge approximation

279 279 282 284

CONTENTS

10.3 10.4 10.5 10.6 10.7 10.8

Preliminary results Vortex-loops as topological defects of the order parameter Superconductor–superfluid duality in d = 3 Zero-field vortex-loop blowout 10.6.1 Definitions Fractal dimension of a vortex-loop tangle Type I versus type II, briefly revisited

III SELECTED APPLICATIONS

ix 286 289 295 298 299 306 309

315

11 Small scale applications 11.1 More JJ-junction and SQUID basics 11.1.1 Introductory remarks 11.1.2 RSJ – the resistively shunted Josephson junction 11.1.3 Further modelling of the Josephson junction 11.1.4 The autonomous DC SQUID 11.1.5 Simplified model of the DC SQUID 11.2 SQUID applications 11.2.1 Biomagnetism: neuromagnetic applications 11.3 Superconducting electrodynamics in the two-fluid model 11.3.1 Frequency dependent conductivity in the two fluid model 11.3.2 Surface impedance and AC loss 11.3.3 Surface resistance measurement 11.4 High-frequency radio technology 11.4.1 Microstrip filters and delay lines 11.4.2 Superconducting high-frequency devices

317 318 318 318 322 323 325 329 329 333 333 336 339 341 341 345

12 Superconducting Wire and Cable Technology 12.1 Low-Tc wire and cable 12.1.1 Introductory remarks 12.1.2 General design considerations 12.1.3 Basic superconductor properties 12.1.4 Design of technical superconductors 12.1.5 Stabilization 12.1.6 AC losses 12.1.7 Mechanical characteristics 12.1.8 Fabrication technology 12.2 High-Tc wire and cable 12.2.1 High-Tc wire and tape 12.2.2 Full-scale high-Tc cable 12.2.3 HTS induction heater 12.3 Magnet technology

349 349 349 350 350 353 355 358 359 359 362 362 363 364 366

x

CONTENTS

IV TOPICAL CONTRIBUTIONS 13 Topical Contributions 13.1 Spin-Triplet superconductivity, by Y. Maeno 13.2 π -SQUIDs – realization and properties, by J. Mannhart 13.3 Doppler effect and the thermal Hall conductivity of quasiparticles in d-wave superconductors, by N.P. Ong 13.4 Nanometer-sized defects responsible for strong flux pinning in NEG123 superconductor at 77 K, by M. Muralidhar and M. Murakami 13.5 Hybrid Magnets, by H. Schneider-Muntau 13.6 Magneto-Optical Imaging of Vortex Matter, by T.H. Johansen 13.7 Vortices seen by scanning tunneling spectroscopy, by Oystein Fischer 13.8 Resistivity in Vortex State in High-Tc Superconductors, by K. Kadowaki 13.9 Coated conductors: a developing application of high temperature superconductivity, by James R. Thompson, and David K. Christen References Chapter 13

V

HISTORICAL NOTES

369 371 371 374 376

378 380 385 388 392

395 397

399

14 Historical notes on superconductivity: the Nobel laureates Heike Kamerlingh Onnes John Bardeen Leon N. Cooper J. Robert Schrieffer Ivar Giaever Brian D. Josephson J. George Bednorz K. Alex M¨uller Alexei A. Abrikosov Vitaly L. Ginzburg Pierre-Gilles de Gennes Philip W. Anderson

401 401 402 403 404 405 407 408 410 411 413 414 415

References

417

Author index

423

Subject index

425

Preface Writing this textbook was motivated by the opinion of the authors that the time has come for an updated look at the basics of superconductivity in the aftermath of progress during the last couple of decades, both through the discoveries of new superconductors, and the ensuing theoretical development. High-Tc superconductor research since 1986 represents an almost unlimited source of information about superconductivity. This is an advantage in the sense that there is ample material with which to fill new books, but a disadvantage in the sense that only a very small fraction of all the efforts that were made, and the results that came out, can be discussed here. In this sense the situation is entirely new: The older texts, like those of de Gennes and Tinkham could discuss or refer to almost all aspects of superconductivity of importance in the 1960s and 1970s. With tens of thousands of papers published after 1986, there is no possibility to take such an approach any more. We apologize to the numerous researchers in the field whose work we could not mention. This situation leaves it even more to the taste of the authors to choose. First and foremost we have wanted to review the basics of superconductivity to new students in the field. Secondly, we wanted to allow those who take a serious interest in the subject at the PhD level, to follow the ideas to old heights like in the BCS theory, or to new heights like in the theory of the vortex system in high-Tc cuprates. Superconductivity is now a far richer subject thanks to the discovery of high-Tc cuprates by Bednorz and M¨uller. Suddenly, superconductivity became an arena for the study of critical behaviour in three-dimensional superconductors, an unthinkable situation in the low-Tc era. Our book seeks, among other things, to clarify this new aspect of superconductivity. In addition, we wanted to respect the wish of students to learn where physics meets the real life of applications. We have concentrated the material here to the central topics, basically how to describe and exploit the properties of Josephson junctions on the small scale, and on the large scale to give some insight into the makings of wires and cables. A special feature of this book is the inclusion of a chapter containing Topical Contributions from distinguished scientists in various areas of superconductivity research and development, from the smallest to the largest scale. Each of these scientists were invited to contribute their leading edge knowledge to give a clear idea of

xii

PREFACE

the state of the art in several important sub-fields as of September 2003 when the writing of this book came to a conclusion. Kristian Fossheim National High Magnetic Field Laboratory, Tallahassee, Florida and The Norwegian University of Science and Technology Trondheim, Norway Asle Sudbø The Norwegian University of Science and Technology Trondheim, Norway

Acknowledgements From Kristian Fossheim: My part of the writing was done in about equal parts during a sabbatical at the National High Magnetic Field Laboratory (NHMFL) at Florida State University, in Tallahassee, Florida during the academic year 2000/2001, and upon my return to Trondheim, Norway, at the Physics Department of the Norwegian University of Science and Technology (NTNU). I greatfully acknowledge the warm hospitality of the NHMFL, and in particular Jack Crow, Director, and Hans Schneider-Muntau, Deputy Director of the NHMFL. I also wish to express my thanks to my wife Elsa for her patience and her willingness to type, from day to day, my handwritten notes during our stay in Tallahassee. I also thank the Physics Department of NTNU, Trondheim for relieving me of some of my teaching duties during one semester of writing. In this book we also wanted to make Nobel laureates in the field more visible to the students, as human beings, and not just as scientific references. I therefore visited ten laureates, videotaping interviews with them. I want to thank them for the friendliness with which they all met me. It gave me some of the best moments of my scientific life to meet these great scientists and fine individuals in their own settings, and hear their own story told. In the Historical Notes, Chapter 14 a few and brief references to these encounters are mentioned. The rest of the material will have to be presented elsewhere. I also want to thank Ulrik Thisted, my PhD student who undertook the task of weeding out the mistakes in my drafts, and Torbjørn Hergum for various assistance, in particular for drawing the major part of the figures. I dedicate this book to the memory of my parents, Nikolina and Øyvind Fossheim. From Asle Sudbø : I thank the Department of Physics at the California Institute of Technology, and in particular Professor Nai-Chang Yeh, for warm hospitality during the initial stages of this project in the autumn of 2000, which I had the privilege of spending at CalTech on sabbatical leave. It gave me an opportunity to try out part of the material in this textbook on some of the brightest students one can possibly have. I also thank Professor Hagen Kleinert and the Department of Theoretical Physics at the Freie Universit¨at Berlin for their hospitality during 4 months of 2001, where part of the writing was completed. I also want to thank Dr Anh Kiet Nguyen, Dr Joakim Hove, and Dr Sjur Mo for several helpful suggestions and for making some of the material in their PhD theses available to me for this book. Having them as graduate students was truly a pleasure and

xiv

ACKNOWLEDGEMENTS

a privilege. Finally, I want to express my sincere thanks to Professor Zlatko Tesanovic, for the innumerable and inspiring discussions I have had with him over the years on the physics of strongly correlated systems. I dedicate this book to the memory of my good friend Anthony Houghton. The authors would like to extend their special thanks to scientific colleagues in the US, Europe and Japan for their topical contributions in Chapter 13: D. K. Christen, Ø. Fischer, T.H. Johansen, K. Kadowaki, Y. Maeno, J. Mannhart, M. Murakami, M. Muralidhar, N. P. Ong, H. Schneider-Muntau and J. R. Thompson.

PART I

Basic Topics

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

1 What is Superconductivity? A Brief Overview 1.1 Some introductory, historical remarks Progress in science in general, and in physics in particular, is characterized by many great discoveries both in theory and experiment. On superficial observation these sudden advances may look like a series of accidental occurrences. But in most cases such an impression would be wrong, in many cases even totally misleading. Very often discoveries occur when the time is ripe, i.e. when certain preconditions have been met, such as adequate technical capability, or attainment of a necessary intellectual and theoretical level. The discovery of superconductivity – the property of certain conductors to display zero DC electrical resistance – by Heike Kamerlingh Onnes and co-workers in 1911 illustrates the point [1]. It was a true discovery, and indeed a remarkable one, because there were no valid arguments around to predict such a phenomenon. Yet, to draw the conclusion that it was accidental would be unjustified. The necessary technical basis and opportunity for the discovery had been solidly established in the same group by the liquefaction of the inert gas helium in 1908. And research, both experimental and theoretical, on the electrical conductivity of metals at temperatures approaching the absolute zero, was ongoing and considered an important issue by leading physicists. They were even puzzled by an apparent similarity between the temperature dependences of electrical conductivity and heat capacity in metals. On travelling down the infinite road towards zero degrees Kelvin, new discoveries could and should be expected, since temperature is the most universal variable by which the (equilibrium) state of matter is defined. In fact, the absence of discoveries along this route should have been the real surprise. Even the cryogen itself, liquid helium, was later to offer a number of opportunities for important discovery. And many more were to come in other condensed matter systems below ambient temperatures. Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

4

WHAT IS SUPERCONDUCTIVITY?

Even the choice by Onnes of the metal to study, mercury, while appearing perhaps surprising today, was a judicial and natural one at that time: It was the metal that offered the most ideal conditions for the study of intrinsic properties of metals at low temperatures due to the purity at which it could be obtained. Purity was indeed a valid consideration, and would be even today, when studying electrical conductivity versus temperature. Research in the Leiden laboratory was carried out by coworkers and students of Onnes in a strictly systematic manner. Metal upon metal was measured, and the results contemplated. Gold was found to have almost immeasurably low resistance in the liquid helium range; but mercury became the first substance found to be superconducting, at a temperature near 4 K. The distinctive feature was a sudden drop of resistance by several orders of magnitude on lowering the temperature below what appeared to be a sharply defined temperature. Lead and tin were soon added to the list. Onnes dismissed the prevailing idea that electrons would ‘freeze to the atom’, and surmised instead that ‘the free electrons would remain free’ while the ‘vibrators’ (atoms) would become ‘practically immovable’1 . The timeliness of their research is also illustrated by the fact that thermal properties were much in focus, thanks to the blackbody problem, the early quantum theory of Planck, and the attempts by Einstein and others to explain low-temperature heat capacity, as well as by ongoing research on thermal and electrical conductivity of solids at lowtemperatures. The electron, a relatively recent discovery, had brought electrical phenomena to the forefront of research. The fact that the atomic nucleus was discovered that same year, 1911, makes this a truly remarkable year in the history of scientific discovery. The Leiden group attached considerable hope to the technological potential of superconducting coils for generation of magnetic field, foreseeing fields as high as 10 T. But they soon found an unexpected obstacle: An upper limit for current that would flow at zero resistance in lead or tin superconductors in the self field of the coil, what we today call the critical current Ic . This difficulty could not be circumvented until decades later, when it was realized, first through theoretical work, that a different kind of superconductor was needed. This new class of superconductors was to be labeled ‘type II’ as opposed to type I for Sn and Pb and similar conductors which had been studied in Leiden. Only upon discovering, understanding, and further developing type II materials could critical current density be raised to much higher, practical values. From the 1960s on a gradual development of superconductor technology has taken place, until today when superconducting magnets are commonplace in laboratories and hospitals all over the industrialized world. And the remarkable SQUID technology developed for measurement of small magnetic fields, has taken on a wide range of applications, and is showing promise in ever new fields by use of both old and new superconductors. 1 For

an account of early work on superconductivity, see Dahl [2].

SOME INTRODUCTORY, HISTORICAL REMARKS

5

Other great discoveries were to follow. The magnetic properties of superconductors attracted considerable attention through the 1920s and 1930s. A breakthrough came in 1933 when Meissner and Ochsenfeld [3] showed that in magnetic fields below a certain threshold value the flux inside the superconductor was expelled, and that this defined a new thermodynamic state and was not a consequence of infinite conductivity. The phenomenon became known as the Meissner effect, and laid the foundation for a thermodynamic treatment of superconductivity, later to be expanded when Abrikosov [4, 5] was finally permitted to report his theory of the magnetic properties of superconductors at a meeting in Moscow in 1957. That same year Schubnikow’s [6] important experimental work from the 1930s could also finally be recognized publicly and posthumously in the Soviet Union. This work had already established important magnetic properties of type II superconductors two decades earlier, and had shown promise for superconductors to carry larger current densities than materials previously studied by Onnes, and by Meissner and others. 1957 was also the year when the beautiful quantum theory, known as the BCS theory, was published by Bardeen, Cooper and Schrieffer [7], finally explaining the fascinating properties of superconductors from first principles. It had taken 46 years from the time of the discovery. A few years later Josephson’s [8] astonishing predictions regarding the physical properties of inhomogeneous superconductors were announced, soon followed by experimental verifications, and by a variety of applications as well as further theoretical development. It would take another 25 years before superconductivity made the transition from being mainly an exotic laboratory phenomenon, known mostly to physicists, to become almost a household word. That development was to take place by the discovery of a new class of superconductors, known as high-Tc cuprates, by Bednorz and M¨uller [9] at the IBM laboratory in R¨uschlikon near Z¨urich in 1986. This is an example of a great discovery made on the basis of systematic, goal oriented research. From then on the world outside of physics became fully aware of the almost magical properties of superconductors. The discovery started a race towards applications that is still ongoing, with great economic prospects. Equally intense was the desire to understand the mechanism. At the time of writing this book, that goal has not yet been reached. In the meantime, research has benefited greatly from the famous semi-phenomenological theories of the London brothers from the 1930s, and of Ginzburg and Landau [10] published in 1950, in particular. It has been estimated that well over 50 000 scientific papers have been published on superconductivity since the high-Tc discovery in 1986. A single book can only give a modest insight into this vast amount of knowledge and results. The present one aims to shed light on what the authors regard as the most central issues, with special emphasis on developments taken place during the last 15–20 years.

6

1.2

WHAT IS SUPERCONDUCTIVITY?

Resistivity

Two fundamentally important and intuitively startling properties are associated with superconductivity: • The transition from finite resistivity, ρn in the normal state above a superconducting transition temperature Tc , to ρ = 0, i.e. perfect DC conductivity, σ = ∞, below Tc . • The simultaneous change of magnetic susceptibility χ from a small positive paramagnetic value above Tc to χ = −1, i.e. perfect diamagnetism below Tc . These aspects are qualitatively illustrated in Figure 1.1. Actual measurements of resistivity as a function of temperature in a high-temperature superconducting material are shown in Figure 1.2. We shall return to the second of the above statements in Section 1.3. Let us now discuss the implications of the first statement. The traditional way to measure resistance is by balancing a Wheatstone bridge, using the sample as the fourth and unknown resistance. When balanced, the precision of the measurement is as good as that of the resistors used in the circuit, or possibly limited by the zero-readout accuracy of the galvanometer used in balancing the bridge. There is a limit to how low resistance one can claim to measure: Zero resistance is not accessible to direct measurement. By standard methods we can measure a reduction in resistance by many orders of magnitude, but we can never measure zero resistance in a strict sense. If we try to measure the inverse quantity, i.e. conductivity σ = 1/ρ, the impossibility

Superconductor r=0

0

Tc Temperature T

Susceptibility c(T)

Resistivity r(T )

Non-superconductor 0

−1

0

Tc Temperature T

Figure 1.1 Sketches of the two basic characteristics of a superconductor: The left figure shows the drop to zero resistivity, ρ = 0, at a temperature Tc , compared to a nonsuperconducting behavior. The right hand figure shows the corresponding drop in susceptibility to the ideal diamagnetic value of χ = −1 below Tc . The onset of the diamagnetic response corresponds quite closely to the point where ρ → 0 on the temperature axis. The figure also indicates that χ is positive but quite small above Tc .

RESISTIVITY

7

800

Resistance R(mΩ)

Tl-Ba-Ca-Cu-O 600 Superconducting phase

400

Normal phase

200 r=0 0

0

100

200

300

Tc Temperature T(K)

Figure 1.2 Experimental data on the resistance of a Tl-Ba-Ca-Cu-O ceramic sample from the early days (1988) of high-Tc discovery (unpublished data from the Trondheim group). As was often the case during the early days the material was not of precisely determined composition. The value of Tc indicates that the material was close to Tl2 Ba2 Ca2 Cu3 O10 composition.

remains. No method is available to measure an infinite quantity. For the discoverers of superconductivity this was a real dilemma. Kamerlingh Onnes held on to the belief that a ‘micro-resistance’ remained below Tc . It is, however, still possible to arrive at the reasonable conclusion ρ → 0, or equivalently σ → ∞, by inference from real measurements. Experiments have been devised for this purpose. In such experiments the magnetic field associated with an induced current has been found to remain constant during a time span as long as 1 year. This allows an estimate to be made of the lower bound of the decay constant, and of the upper bound of the resistance. The resulting analysis of such a measurement leads to the conclusion that the lower bound on the decay constant τ for the current in the superconductor is of the order of 100 000 years, implying that the total time for the current to die out completely would be millions of years. Let us see how such an estimate can be made. To be specific, we assume that a current I0 is set up by induction in a superconducting closed loop at time t = 0, at a temperature below Tc . Next, the associated magnetic field is monitored over a very long period of time over some area in the loop, as illustrated in Figure 1.3. As long as a resistance R exists in the superconducting loop, with inductance L in the presence of a current I = I (t), conservation of energy requires d 1 2 LI + RI 2 = 0 (1.1) dt 2 with the well-known solution

I (t) = I0 e−(R/L)t

(1.2)

8

WHAT IS SUPERCONDUCTIVITY?

a

B r

I(t)

V

I

R, L

Figure 1.3 Sketch of a simple setup to monitor the possible decay of current I (t) via its associated magnetic induction B(t) in a closed loop of inductance L and resistance R. The wire has a diameter a and a loop radius r. The field B is normal to the loop area. The magnetic sensor is a Hall probe.

where I0 was the initial current at time t = 0. The decay time of the current, as well as of the corresponding magnetic induction B, is τ = L/R. Now, if the B-field surrounding the loop is measured to be the same after a time t1 , say 1 year later, it appears to mean that I (t1 = 1 year) = I (t = 0) = I0 , and similarly for the corresponding B-field. However, this statement is not an exact one. The B-field we measure, resulting from the current I (t), can only be measured with a certain accuracy, determined by the instruments used. If we assume that the change of B-field can be detected with a relative instrumental resolution δB/B0 = 10−5 , an observation of ‘no change’ in reality only sets an upper bound on the possible decay δI of current and of field δB that may have occurred. What the measurement can determine is therefore only the maximum amounts by which the current I and the field B may have decayed. In reality the decay may have been much lower. Hence we can estimate

and

δI > I0 − I (t1 ) = I 0 (1 − e−(R/L)t1 )

(1.3)

δB > B0 − B(t1 ) = B0 (1 − e−(R/L)t1 ).

(1.4)

From this it follows that δI δB = > 1 − e−(R/L)t1 I0 B0 Solving for R, we find its upper bound δB δI L L = − ln 1 − R < − ln 1 − t1 B0 t1 I0 where all quantities on the right can be determined from the experiment.

(1.5)

(1.6)

RESISTIVITY

9

If we assume that we have used a single-loop inductor with a diameter a and loop radius r, and use the inductance formula for a single loop which applies for r a: L ≈ µ0 r ln(r/a), we find the expression for the upper bound on R as µ0 r ln(r/a) δB R 5.8 × 1013 s. Because 1 year is close to 3 × 107 s, the lower bound on the decay time is about 2 million years. This is a factor of 10 longer than the observations referred to above, so we were a bit generous. But we have to remember that the real observation was of no change. The instruments are the limitation, and we may not have overestimated the actual decay time at all. On the contrary, it might have been found to be much longer had instruments with higher resolution been used. The quest for an even better experimental verification of ρ = 0 in the superconducting state could be continued. If we had used a SQUID superconducting detector of the magnetic field (see Chapters 5 and 11), the detection limit for the small changes in magnetic field would be lowered by several orders of magnitude more, and the upper bound on resistance and resistivity might have been lowered correspondingly. The lower bound on the decay time τ = L/R would then be raised by many orders of magnitude above 1013 s that we have found so far. τ might even approach the lifetime of the Universe. This would be in accordance

10

WHAT IS SUPERCONDUCTIVITY?

with theoretical arguments in ideal situations. What better measure could we ask for to conclude that zero resistivity is physically possible? Having satisfied ourselves that ρ = 0 is an appropriate statement about the electrical resistivity in a superconductor, we must immediately caution against one particular misinterpretation: We have to keep in mind that this state of affairs only applies to DC resistivity. An applied AC electric field accelerates charge. We cannot avoid continually transferring energy to the electron system as long as we keep accelerating it, i.e. as long as we expose it to an AC electric field. We shall return to this question in detail in Chapter 11, and find that the resistance increases with the square of the frequency, but with a very small prefactor. Consequently, there is no abrupt change from DC to the AC resistivity in the superconducting state as we start increasing the frequency from zero. This loss becomes important only at very high frequencies. Still, because of the fact that in the actual technical construction of superconducting cables, normal metals unavoidably have to be used as part of the whole structure, there are losses, so-called coupling losses in the normal metal surrounding the superconductor even at standard electric grid frequencies, i.e. at 50 Hz or 60 Hz. In addition, losses caused by displacement of supercurrent vortices in a magnetic field are important in such cases, even in DC situations. These questions are treated in Chapters 8 and 12. That supercurrents in ideal situations can run without observable loss for years, indeed perhaps much more than 106 years as we found previously, is one of Nature’s most fascinating phenomena. It contradicts all experiences we have from physical systems in the macroscopic world, because it implies frictionless or lossless motion of matter, in this case charged matter, which is displaced relative to the ions. A classic analogue to electronic supercurrent transport in an electrical circuit could be that of sliding a pebble along a flat, icy surface. The pebble soon comes to rest because it spends all its energy working against friction. However, in the superconducting circuit the charged particles (current) continue to run, hence there is no friction. It is precisely because this situation is so contrary to all our experience with other real systems that superconductivity is such a startling and counterintuitive phenomenon. In fact, as we shall see, superconductivity is a pure quantum physics phenomenon on a macroscopic scale. Superconductivity has an additional property compared to the lossless motion of charged particles in atoms, namely phase coherence of the manybody wavefunction. Indeed one of the most remarkable feats of science was the development of a manybody quantum theory that finally explained superconductivity, and with predictive power.

1.3

The Meissner effect: perfect diamagnetism

From the discovery of zero electrical resistivity by Onnes in 1911, 22 years would pass until the next important discovery by Meissner and Ochsenfeld.

THE MEISSNER EFFECT: PERFECT DIAMAGNETISM

11

They found that the superconducting state possesses a second characteristic, defining property – perfect diamagnetism. Prior to this discovery there had been considerable debate regarding the magnetic properties, and the discussion had been based on an interpretation of the superconducting state with perfect conductivity as the (only) basic characteristic. Meissner and Ochsenfeld managed to escape this conceptual trap by observing that a magnetic field, which was applied above Tc would be expelled from the body of the superconductor on cooling below Tc , leading to B = 0 inside. Using the constitutive equation for a magnetic body we therefore have to write, in the superconducting state: B = µ0 (H + M) = 0

(1.9)

which means that in the superconductor M = −H.

(1.10)

Therefore, the susceptibility takes on the ideal value for a perfect diamagnet: χ=

dM = −1. dH

(1.11)

Because permeability is κ = 1 + χ we also have κ = 0 below Tc . These two ways of expressing the Meissner effect are of course equivalent, but the diamagnetic statement χ = −1 is perhaps physically more ‘descriptive’ and appealing. What happens is that shielding currents arise in the superconductor surface. These currents create a field both inside and outside the superconductor such that on the inside the applied and the induced fields exactly cancel, while outside they add. The result is that we observe expulsion of the B-field: zero B-field inside, and an increased field near the sample, on the outside. This is illustrated in Figure 1.4. While in the normal state Faraday lines would pass straight through the metal, practically as if there was only vacuum, in the superconducting Meissner state all lines are forced to pass on the outside. The highest H

B≠0

T > Tc c 0; k≈1 NORMAL

H

Cooling

B=0

T < Tc c = −1; k = 0 SUPERCONDUCTING

Figure 1.4 The Meissner effect in a superconductor.

12

WHAT IS SUPERCONDUCTIVITY?

density of flux lines is found near the equator, while near the poles there is a lower flux density than before the flux expulsion. That this situation represents a thermodynamic state is demonstrated by the experimental observation that the state is uniquely defined by the values of the thermodynamic variables, temperature T and applied field H , independent of how that state was reached. It is important in this context to observe that this is not possible if perfect conductivity was the only special property that the superconductor attained on passing below Tc . This can be confirmed by a simple thought experiment, as in the two sequences illustrated in Figure 1.5. Imagine (i) that a specimen which is originally at room temperature, is cooled in zero applied field to below a temperature Tc where it acquires zero resistance, ρ = 0. Now turn on an external magnetic field. Lenz’ law requires currents to arise in the specimen so as to screen out the applied field. As ρ = 0 this situation will persist forever, and no field will penetrate. Let us call this state I. Next, remove the field. Because the prevailing requirement from Lenz’ law is to allow no change of flux in the specimen, the currents in the sample will diminish to zero as the field is turned off. At the end of the sequence the sample is still free of magnetic flux inside. Call this state II. In the next sequence, (ii), start the experiment at room temperature, this time in an applied external field. This field penetrates the sample completely and almost totally undistorted due to the low paramagnetism of nonmagnetic metals. Now cool the specimen in the magnetic field to below the same temperature Tc as before. Although the sample, by assumption, acquired ρ = 0 on

Cooling

(a) Ha = 0; T > Tc

(b) Ha = 0; T < Tc

(d) Ha = 0; T < Tc (c) Ha > 0; T < Tc

Cooling

(e) Ha > 0; T > Tc

(f) Ha > 0; T < Tc

(g) Ha = 0; T < Tc

Figure 1.5 Cooling a hypothetical normal conductor with infinite conductivity in zero external field, and in a finite field, and comparing the resulting states of the material. The figure is explained in the text, and important conclusions are drawn from that discussion.

TYPE I AND TYPE II SUPERCONDUCTORS

13

passing through Tc , Lenz’ law requires the flux inside to remain perfectly constant. Call this state III. Next, remove the external field. Again Lenz’ law requires the flux to stay constant. This can indeed be implemented by a spontaneous current arising on the surface. Since by assumption ρ = 0, the situation will persist forever. Call this state IV. Now compare, in particular, state II and state IV. The thermodynamic variables T and H are the same, but the states are quite different as just described. The difference was unavoidable due to the assumption that the only new property that the specimen acquired on passing below Tc was perfect conductivity. However, on exposing real superconductors to precisely the same sequences the superconductor ends up in exactly the same state, namely one of total flux expulsion in both cases, and again the situation is persistent. We have two important conclusions to draw from these observations: • Superconductivity is more than just ρ = 0. • Superconductivity is a thermodynamic state, contrary to a state characterized by just ρ = 0. What happens in the Meissner effect is that spontaneous currents arise in the surface to exactly cancel the B-field inside. Diamagnetism is well known to exist in all matter, but usually the corresponding susceptibility is very small, typically χ = −10−6 in atomic and molecular diamagnetism. Perfect diamagnetism clearly is a totally different phenomenon. The reason for the large negative value is precisely the fact that currents encompass the entire body, and are not broken up into tiny currents circulating individual atoms. We might add that diamagnetism exists in metals in the normal state too, due to surface currents in a magnetic field. But this effect is more than overcome by the paramagnetism of the conduction electrons. In the discussions of the superconducting state we have so far assumed that currents and fields employed were below the threshold where superconductivity breaks down. In Chapter 8 we discuss the limits as to how large currents and fields a superconductor can tolerate before being forced to allow magnetic flux to penetrate. As long as the superconductor is at a field below such values, and χ = −1 is maintained, we say that the superconductor is in the Meissner state, or Meissner phase, as shown in Figure 1.6. These remarks point to the need of defining more precisely the thermodynamic range of superconductivity in the (H, T )-plane. This has been well established for a great number of metals and alloys, as well as high-Tc and other classes of superconductors. We return to this problem in the next section.

1.4 Type I and type II superconductors Superconducting materials have the ability, as we have seen, to exist either in the normal state or the superconducting state, depending on the external

14

WHAT IS SUPERCONDUCTIVITY? H Hc(0) NORMAL

Meissner phase SUPERCONDUCTING Tc

T

Figure 1.6 The Meissner phase of a superconductor. Under the curve, in the shaded area, the material is perfectly screened against an external magnetic field.

magnetic field they experience. It turns out that if we increase the magnetic field beyond a certain critical value Hc or Hc1 , which is different for different materials, the Meissner effect breaks down. That is to say, flux penetrates into the material. A sketch is shown in Figure 1.7. This figure shows the negative of the magnetization along the positive vertical axis. The slope of the line from the origin is then exactly 1 as long as the sample is in the Meissner state, corresponding to χ = −1. Let us here first discuss the ideal case which best brings out the underlying physics: Imagine we study a long, thin needlelike specimen, with the applied field parallel to its axis, in which case the demagnetization factor n = 0.2 A pickup coil can be used to measure the amount H Type I

Type II

Magnetization – M

I n≈0 ∆I ∝ ∆M

SM 0

N Hc (a)

SV

SM 0 Applied field H

Hc1

N Hc2

(b)

Figure 1.7 (a) shows the typical behaviour of a type I superconductor which switches abruptly from the Meissner state SM to the normal state N at Hc . (b) shows a different behaviour in a type II superconductor: At a lower critical field Hc1 the superconductor changes state from the Meissner state with complete screening, SM , to a state of vortex line penetration SV , and finally, at Hc2 , to the normal state N. The insert indicates that the magnetization development can be monitored by a coil around the rod-like sample (demagnetization factor n ≈ 0) such that the change of current I is proportional to the change of magnetization M. 2 We

refer to Section 1.7 for a discussion of demagnetization factors.

TYPE I AND TYPE II SUPERCONDUCTORS

15

of flux which penetrates the sample. Now turn on a magnetic field. At low fields the Meissner state, corresponding to complete screening, is found. But as the field increases further we will discover two distinctly different outcomes, depending on the materials we investigate. This will allow us to sort all known superconductors into two categories as follows: • Type I: The superconductor switches abruptly over from the Meissner state to one of full penetration of magnetic flux, the normal state, at a well-defined critical field, Hc . Examples of such materials are Hg, Al, Sn, In. Figure 1.7a shows a sketch of this behaviour. The ideal behaviour is only observed when n = 0. • Type II: The superconductor switches from the Meissner state to a state of partial penetration of magnetic flux, the mixed state, at a critical field Hc1 . Thereafter it crosses over continuously to full flux penetration, the normal state, at an upper field Hc2 . Examples: Nb3 Sn, NbTi, and all high-Tc cuprates. Figures 1.7b and Figure 1.8b illustrate this behaviour. The distinction between type I and type II turns out to be so important that hereafter we shall think of every superconductor we encounter as belonging to one class or the other. Several chapters of this book are occupied with aspects

Type II n ≠ 0: FILM

Type I n ≠ 0: DISC

a(H)

H

H

n=0

−M

Φ0 =

h 2e

−M

n≠0 Hc (a)

H

Hc1

Hc2

H

(b)

Figure 1.8 Illustration of flux penetration in cases when the demagnetization factor n = 0. In the (a) upper part, normal lamina penetrate the disc from the periphery when n = h arrange 0. In (b) vortices with flux lines carrying an elementary amount of flux 0 = 2e themselves in a hexagonal pattern in a field normal to a type II film. In the case of type I the laminar penetration is seen only when n = 0. When n = 0 the transition from the Meissner state to the normal state is abrupt, no lamina appear. In the case of type II superconductor the observed mixed state behaviour is inherent to the material, irrespective of the value of n.

16

WHAT IS SUPERCONDUCTIVITY?

related to their distinction, which turns out to be essential from a practical as well as a theoretical point of view. At this point we will limit the discussion to the descriptive level, and refer the more advanced discussion to later chapters. In order to see another difference between the two types of superconductors, let us relax the requirement on the demagnetization factor, and allow n to be non-zero. This forces flux to penetrate inhomogeneously even into a type I superconductor. Using various techniques to decorate and picture the flux distribution the following facts emerge, as illustrated in Figure 1.8a and b. In type I materials the flux penetrates in the form of continuous lamina, flat or meandering. The lamina are alternating normal and superconducting layers, parallel to the field, whose relative thicknesses depend on both temperature and applied field. The following constraints have been found to apply to these structures: Superconducting lamina are flux-free in a Meissner-like state, while the normal ones contain a magnetic flux density corresponding to the critical field, i.e. Bc = µ0 Hc . The relative thickness of normal and superconducting lamina is fixed by a combination of this fact, and by flux conservation. We refer to Section 7.3 for a further discussion. In type II materials, on the contrary, flux penetrates in tiny, precisely quanh tized units of flux 0 = 2e where h is Planck’s constant, and e is the magnitude of electronic charge. We call these objects flux lines or vortex lines, a distinction in terminology which will be made clear in the next Section. The density of such flux lines increases with increasing applied magnetic field, as is reflected in the M versus H diagram (Figure 1.8b). The magnetic energy density Hc2 /2µ0 required to break down the Meissner state completely at Hc in the type I case, with n = 0, measures directly the stability of the superconducting phase against that of the normal one. Hence this crucial information is obtainable by relatively simple measurements. Hc , it turns out, differs from one material to another, not a surprising fact considering that all metals have different electronic properties, like Fermi surfaces and band structures. If we study flux penetration into specimens of other shapes by allowing n = 0, we will find that when the Meissner state breaks down, the details of how flux penetrates and the precise fields at which it first occurs, and where it is completed, depend on the shape of the specimen due to the demagnetization effects alluded to above. An important point regarding these shape dependent effects is that whenever the demagnetization factor for a chosen combination of geometry and field direction is nonzero, the external field varies along the surface of the specimen. This causes flux to penetrate inhomogeneously whenever n = 0, unlike the case when n = 0. In the former case the transition from the Meissner state to the fully penetrated state is gradual when M versus H is measured even in type I. We underscore again the importance of the fact that partial flux penetration in type I superconductors, often referred to as the intermediate state, is very different from that of the mixed

VORTEX LINES AND FLUX LINES Type I

Type II

Hc Applied field H

17

Hc2 N

N SV Hc1

SM

SM Tc

Tc Temperature T

Figure 1.9 Phase diagram of type I (left) and type II (right). S = superconducting, M = Meissner phase, V = vortex phase, N = normal phase.

phase of type II. It is precisely this difference that makes type II superconductors useful on a large scale, while type I are not. Figure 1.9 illustrates the complete phase diagram for type I and type II superconductors in the H, T − plane.

1.5 Vortex lines and flux lines We want to stress a very important conceptual difference between what we call vortex lines and flux lines. Often, these terms are used interchangeably. This is permissible in most conventional type II superconductors, where the ratio between the upper and lower critical fields Hc2 and Hc1 , is not very large. In the cuprate high-Tc superconductors, however, this ratio is enormous. It then turns out to become important to distinguish between the concepts of flux lines and vortex lines. As already mentioned, Abrikosov predicted the existence of the so-called mixed phase, in what has become known as type II superconductors. The distinguishing characteristic of these, as we have seen, is their ability to allow magnetic field penetration in the form of magnetic vortices of quantized circulation. This cannot happen in type I superconductors. In the centre of each magnetic vortex superconductivity is destroyed, i.e. the density of superconducting electrons is zero, while outside the centre, it is non-zero. Hence, far away from the centre of the vortex the associated magnetic field goes to zero. As we will see in later chapters, the ratio of the penetration depth λ to the length over which a magnetic field destroys superconductivity, ξ , determines the extent to which a superconductor is type I or type II. When the ratio λ/ξ is small it is type I, and when the ratio increases roughly beyond one, the superconductor becomes progressively more type II. This situation is illustrated in Figure 1.10.

18

WHAT IS SUPERCONDUCTIVITY?

B(r) x : |y| < |y0|

l3 r

l2

l1

0

r

Figure 1.10 The parameters ξ of the vortex line and λ of the flux line. As explained in the text, the distinction between the concepts of vortex lines and flux lines becomes increasingly important as λ becomes greater and greater compared to ξ . λ measures the radius of circulation of supercurrent around the vortex core. The wavefunction is severely depressed for r < ξ , and goes to zero on the axis.

Flux lines are tubes of confined magnetic flux. They have a diameter given by the distance with which a magnetic field can penetrate into the superconductor. On the other hand, a vortex line is a line with a diameter given by the distance over which a magnetic field suppresses superconductivity. This length is conceptually different from the magnetic penetration depth. It is then easy to imagine that a thick line with a large diameter has a typical bending length which is much longer than a very thin line. Moderate (conventional) type II superconductors are characterized by the fact that the two length scales described above are roughly equal. In extreme type II superconductors, such as the highTc cuprates, this is not at all the case. The magnetic penetration length, i.e. the diameter of the flux line, is typically 100 times larger than the diameter of the vortex line. Hence, the vortex line resides deep inside the flux line and moreover fluctuates on a vastly different length scale than the flux-line. In essence, they therefore represent different degrees of freedom of the system. This will turn out to be of crucial importance in the theoretical treatment presented in Chapters 9 and 10. In these contexts, therefore, the conceptual distinction between flux lines and vortex lines is essential. In the extreme type II case, where flux lines no longer can be defined, basically being treated as infinitely thick objects, a vortex line is still perfectly well defined.

1.6 Thermodynamics of the superconducting state We have already pointed out that the superconducting state has a limited stability against application of a magnetic field. This became apparent in the discussion of the magnetization diagrams, M(H ), in Section 1.4. The M(H ) diagrams can

THERMODYNAMICS OF THE SUPERCONDUCTING STATE

19

be read as phase diagrams, and hence may be subjected to thermodynamic analysis. A very useful aspect of thermodynamics is as a tool to derive relationships between measurable quantities by analysis of free energies. We will now look into this possibility for superconductors. Let us first recall the so-called thermodynamic square, Figure 1.11, a useful mnemonic device from which one can quickly read out the basic relationships, in this case with respect to magnetic properties, of completely general validity. The starting point is the following square: −m0M

A

G

U S

Figure 1.11

T

E

H

Thermodynamic square.

Here M is magnetization, T is absolute temperature, A is Helmholtz free energy, U is internal energy, G is Gibbs’ energy, S is entropy, E is enthalpy, and H is the applied magnetic field. The idea here is that each free energy should be considered as depending on the two variables next to it. Following the suggestion of the arrows it may be used to read out thermodynamic derivatives. Going in the direction of the arrows generates a positive sign, going in the opposite direction generates a negative sign. Some examples: ∂G = −µ0 M ∂H T ∂G = −S (1.12) ∂T H ∂U =T ∂S M When discussing the superconducting state in an external magnetic field H , and the resulting magnetization, we should use the Gibbs’ energy G, and consider it dependent on T and H . We rewrite the first relation in Eq. 1.12 as dG = −µ0 MdH

(1.13)

This relation applies both in the normal and superconducting state. Next, integrate from zero to Hc at constant T in the superconducting state: 0

Hc

dGs = −µ0

Hc

Ms (T , H ) dH 0

(1.14)

20

WHAT IS SUPERCONDUCTIVITY?

Here M = M(T , H ), but varies only with H as T is constant during the integration. We now consider a type I superconductor. The Meissner state, in which we now carry out the integration, was found in Section 1.3 to be characterized by M = −H . Using this, Eq. 1.14 yields

Hc (T )

dGs = −µ0

0

Hc (T )

(−H )dH =

0

µ0 2 H (T ) 2 c

(1.15)

On the left-hand side we have

Hc

dGs = Gs (T , Hc ) − Gs (T , 0)

(1.16)

µ0 2 H (T ) 2 c

(1.17)

0

The result is: Gs (T , Hc ) − Gs (T , 0) =

We want to calculate the energy difference between the normal and the superconducting states, which addresses the question of stability of the superconducting state. To do that we recall first that χ for a normal metal is small, χ 1. This implies that a normal metal in a field Hc has practically the same Gibbs energy as in zero field. Hence we write Gn (T , Hc ) = Gn (T , 0)

(1.18)

This corresponds to saying that the integral

Hc

dGn = −µ0

0

Hc

Mn dH

(1.19)

0

taken in the normal state can be treated as zero. From the fact that the two phases coexist in the intermediate state of type I, with a field Hc in the normal lamina and zero in the superconducting ones, we conclude that Gn (T , Hc ) = Gs (T , Hc )

(1.20)

Comparing Eqs 1.18 and 1.20 we see that Gn (T , 0) = Gs (T , Hc )

(1.21)

THERMODYNAMICS OF THE SUPERCONDUCTING STATE

21

Putting this back into Eq. 1.17 gives: Gn (T , 0) − Gs (T , 0) =

µ0 2 H (T ) 2 c

(1.22)

The interesting aspect of this relation is that the difference in energy density between the (Gibbs’) energy in normal and superconducting states without a field present can be expressed by the characteristic energy µ20 Hc2 in the simple fashion of Eq. 1.22. From this relationship it becomes clear that Hc2 is in a deeper sense a measure of the ‘condensation energy’ of the Meissner state, or the stability of the Meissner state with respect to the normal one. The energy density is lower in the superconducting state by the amount µ20 Hc2 (T ). Alternatively we can write it as 2µ1 0 Bc2 (T ). We will later discover (Chapter 8) that the condensation energy can be found on a microscopic basis, leading to a relationship between Hc and the superconducting energy gap. It is useful at this point to calculate other thermodynamic aspects of the Meissner phase. Analytically this can be done if we can find an expression for Hc (T ). It turns out that experiments, to a good approximation, give a unanimous 2 answer, which we can use in the further analysis: Hc (T ) = Hc (0) 1 − TTc . This is a simple parabolic shape with the top of the parabola at Hc (0) on the vertical H-axis, and an approximately linear shape where it meets the Taxis. With the important result for the condensation energy and the functional expression for Hc in hand, we choose a relationship from the thermodynamic square, that for entropy: ∂Gs Ss = − (1.23) ∂T H We can now find the entropy change at the phase boundary by taking the temperature derivative of Eq. 1.22 directly and obtain: Sn (T , 0) − Ss (T , 0) = −µ0 Hc

dHc dT

(1.24)

We note here that the quantity −µ0 Hc dHc /dT is always positive, meaning that the entropy in the superconducting state is always lower than in the normal state. Hence, the superconducting state is characterized by greater order than the normal state. An entropy drop at (Tc , Hc ) accompanies the superconducting transition. The exception is when T = Tc , where Hc = 0. We see that in this case Sn = Ss , and there is no entropy drop. At this particular point the entropy is therefore continuous, characteristic of a 2nd order transition. There are two aspects of the superconducting state that show the increased order below Tc indicated by the thermodynamic analysis: Formation of Cooper pairs represent a partial ordering of the electron gas, and the superconducting wavefunction

22

WHAT IS SUPERCONDUCTIVITY?

shows an ordered phase of the wavefunction, or phase coherence. These facts are of course related. Another quantity closely related to entropy is the latent heat. Here we find L = T (Sn − Ss ) = −T µ0 Hc

∂Hc ≥0 ∂T

(1.25)

Again, this is a positive quantity as long as we are considering finite Hc . At Tc , where Hc = 0 we get L = 0, again characteristic of a second order or continuous transition. Finally, let us look at the heat capacity, which from thermodynamics is found by differentiation of the entropy CH ≡ T Taking the 2nd derivative of

µ0 2 2 Hc

∂S ∂T

(1.26) H

we find:

Cs (T ) − Cn (T ) = µ0 T

dHc dT

2

d2 Hc + Hc dT 2

(1.27)

which, at Tc becomes Cs (Tc ) − Cn (Tc ) = µ0 Tc

dHc dT

2 >0

(1.28)

T =Tc

We find a discontinuity at Tc , an upward jump on lowering the temperature through Tc as all quantities in the right-hand side are positive. Experiments have verified this aspect in every case it was measured in the low-Tc superconductors. In high-Tc materials the story is more complicated. There, fluctuations play a dominant role near Tc , and a different description altogether is necessary, as will be discussed in several chapters of this book. The discontinuity found in Eq. 1.28 is characteristic of mean-field theories and mean-field systems. The BCS theory, which eventually explained superconductivity in low-Tc materials, belongs to that class, and reproduces the experimental results nearly perfectly. Figure 1.12 illustrates examples of two different phase transitions. The left figure illustrates the BCS mean-field like behaviour, measured on a low-Tc material. The right figure illustrates the situation in a high-Tc material and shows a completely different form, with no jump, and with fluctuation contributions on both sides of Tc . We shall return to these questions which are of major importance in high-Tc materials, with a ratio λ/ξ 1, the so-called high-κ materials.

DEMAGNETIZATION FACTORS AND SCREENING

High Tc

Specific heat Cp

Low Tc

23

Tc

Tc Temperature T

Figure 1.12 Sketch of typical forms of specific heat curves measured from above the superconducting transition in a mean-field low-Tc metallic superconductor like Al (left), and in a substance with strong superconductivity phase fluctuations like the high-Tc compound YBCO (right).

1.7

Demagnetization factors and screening

When a specimen of ellipsoidal shape is subject to a homogeneous external field along one of its principal axes, it is well-known from magnetostatics (see for instance Jackson, 1975 [11]) that the internal fields B i and H i are both parallel to the applied field B a . The constitutive relation is B i = µH i = µ0 (H i + M) = (1 + χ )µ0 H i

(1.29)

As already discussed, in the Meissner state χ = −1, which leads to B i = 0. These two statements are equivalent, and consistent. For the applied fields we have similarly Ba = µ0 Ha (1.30) provided no magnetized matter is surrounding the magnetized body under study. These relations apply separately inside, and outside the measured body, and do not answer the question: what is the relationship between the applied field H a and the internal field H i ? This is not a trivial question. What complicates the relationship between the applied fields and the internal fields Bi , Hi , Ba , Ha is the so-called demagnetizing field. We refer to standard books on magnetostatics for a discussion of the theory of demagnetization effects. Here we will use the results without derivation. The word ‘demagnetization’ was originally coined for use in ferromagnets. It applies with opposite consequences in superconductors as compared to ferromagnets, but is equally important to consider here due to the fact that magnetization effects and demagnetization are very strong in

24

WHAT IS SUPERCONDUCTIVITY?

superconductors. The reason for this is that in superconductors the susceptibility χ = −1, the ideal and complete diamagnetism. Briefly stated, when a magnetic field H a is applied to a superconductor, the screening currents which appear near the surface, create an additional field in the specimen. This is called the demagnetizing field H D . We now have: Hi = Ha − HD

(1.31)

We will only address situations where the internal field is homogeneous, i.e. cases like those we mentioned in the introductory statement above. With this restriction we can still treat all ellipsoidal shapes. These all have a uniform field inside the body when exposed to a uniform external field. We may then write H D = nM

(1.32)

where n is the (scalar) demagnetizing factor, and M is the uniform magnetization of the body. We now have the relationship H i = H a − nM

(1.33)

In a superconductor M = −H i ; which, upon insertion in Eq. 1.33 leads to the important relationship Hi =

1 Ha 1−n

(1.34)

precisely the relationship which we pointed out was missing previously. To take a concrete example, let us examine the situation when a compact ellipsoidal body of superconductor is placed in an external magnetic field applied along one of the principal axes. At the surface of the superconductor the tangential component of H is continuous. The internal field is now parallel to the applied field which exists everywhere on the circumference of the extremal cross-section of the sample as viewed along the field direction. In case of a spherical body this circumference corresponds to the equatorial circle. This makes the field H a just outside the circumference equal to the field H i just inside. Eq. 1.34 now allows us to calculate the field just inside, and because this equals the field just outside, the field just outside is equal to Ha /(1 − n). We learn from this that a demagnetization factor n < 1 makes the field at the maximum circumference larger than the applied field Ha . Some important examples are the following, illustrated in Figure 1.13: • For a sphere, n = 13 , always giving a tangential field of 32 Ha at the equator. • In case the field is applied normal to a long rod of circular cross-section, n = 12 , and the tangential field is 2Ha .

DEMAGNETIZATION FACTORS AND SCREENING Ha

Ha

Ha

n = 1/3 3 H 2 a

(a)

25

n = 1/2

n=0

2 Ha

(b)

Ha

(c)

Figure 1.13 Demagnetization factors for different geometries with n given for each case. Horizontal arrows indicate the value of applied field at the surface in each case.

• With the field applied along the axis of the long rod, n = 0; no demagnetization occurs. The field along the entire surface of the rod is tangential to the (extremal) crossection, and equal to the applied field Ha . Demagnetization effects are very important in superconductors, where χ = −1 in contrast to normal metals where χ ≈ 10−4 or less. In practical cases, when the body under study is not ellipsoidal, one approximates the real geometry with an inscribed ellipsoidal surface which gives a best possible description of the real body, and uses the demagnetizing factor which applies to that ellipsoidal shape. This gives quite good results. A paradox : Having just proven that the field just outside the superconductor (usually) exceeds the applied field, one needs to consider what will happen when the applied field approaches Hc , the critical field of a type I superconductor. If we let the applied field Ha take the value (1 − n)Hc , then the internal field Hi becomes everywhere precisely equal to the critical field Hc . This looks like we now should expect the entire sphere to be driven into the normal state. However, this would cause M to become zero, since in the normal state this is the case with good approximation. This gives Hi = Ha < Hc , and we should conclude that we have a body driven into the normal state by a field H < Hc . This situation is an impossible paradox. Solution: What happens, is that the specimen allows some field to penetrate parts of the superconductor with normal lamina (type I), or vortices (type II). We have a coexistence of alternating normal and superconducting lamina in one case and vortices in the other. Such a thermodynamic coexistence of two phases is commonly found in nature. The situation is therefore normal, in agreement with the thermodynamic laws. The existence of such mixed normal and superconducting volumes is well documented in the scientific literature. Because of the effects discussed here, one finds in real situations that the transition from superconducting to normal state does not occur abruptly and

26

WHAT IS SUPERCONDUCTIVITY?

completely at the thermodynamic field, Hc , but rather over a certain range of fields, the width of which is determined by the demagnetization factor. We refer again to Figure 1.8 for an illustration of these points. With n = 0, as it is with the field along the axis of a long thin rod, the transition in a type I superconductor occurs abruptly at Hc , as we are led to expect from the foregoing, otherwise not.

2 Superconducting Materials 2.1 Introductory remarks After the initial discovery of superconductivity in an element of the periodic table, Hg, almost 20 years went by before research was undertaken in alloys. Another 40 years would pass before organic superconductors were synthesized in the 1970s. Then, another decade would pass before superconducting cuprates were discovered in 1986, followed by fullerenes shortly after. There is a line of progression of structures from the very simple to the quite complex. At the same time, Tc has increased by a factor of 40 from the beginning in mercury to the record Tc in cuprate perovskite; and there is a time span of 90 years between their discoveries. This seemingly slow development is governed by the general development of physics in a broader sense. Theoretical physics could not handle the manybody quantum theory necessary until the mid-1950s when the BCS theory was worked out. And the mechanism developed there was the only one to be relied upon until the superconducting cuprates were found 30 years later. Even today, 90 years after the initial discovery, there is a fierce debate about the mechanism for the high Tc cuprate superconductors. Superconductivity is still a subtle and very complex phenomenon.

2.2 Low-Tc superconductors 2.2.1

Superconducting elements

After superconductivity in Hg had been found, Sn and Pb followed suit. This brought Tc up from 4 K to 7 K. By the time the Meissner effect was discovered, several more elements of the periodic table had been added to the list. Meissner, among others, undertook studies of the transition elements with high melting point, called ‘hard’ metals. Discovery of superconductivity was announced in Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

28

SUPERCONDUCTING MATERIALS

Table 2.1 Ref. [12] Li F

Superconductors in the periodic table, including thin films. Adapted from

Be 0.03

Cs FP

Ba P

1

2

Tc = Superconducting transition F = Film P = Pressure applied Sc Ti 0.01 0.4

V 5.4

Cr F

Y P

Zr 0.6

Nb 9.3

Mo Tc 0.9 7.8

Ru 0.5

La Hi 4.9a 0.1 6.3b 3 4

Ta 4.4

W Re 0.02 1.7

Os 0.7

Ir 0.1

8

9

5

6

Eu F

Ce P Th 1.4

7

Pa 1.4

U P

10

11

Al Si 1.2 FP

P P

Zn 0.9

Ga 1.1

Ge FP

As P

Se P

Cd 0.5

In 3.4

Sn 3.7

Sb P

Te P

Hg 4.2

Tl 2.4

Pb 7.2

Bi FP

12

3

4

5

6

7

8

Lu 0.1

Am 1.0

tantalum in 1928 with Tc = 4.4 K, thorium in 1929, with Tc = 1.4 K, and Nb in 1930 with Tc = 9.2 K. The latter remains the highest Tc found in any element. Table 2.1 shows the elements with known superconducting Tc , a total of over 40 when observations of superconductivity under high pressure and in thin films are included. We notice in particular that superconductivity is neither found in the magnetic compounds, nor in the noble metals or copper. This indicates that superconductivity is incompatible with magnetism, and absent in metals with the highest electrical conductivity. Both of these rules will turn out to be understandable in light of the BCS theory; magnetism breaks up the Cooper-pairs, and is therefore a destructive influence; and excellent electrical conductivity is a signature of weak electron–phonon interaction, a property that reduces the effect of the electron–phonon mechanism for superconductivity in the BCS theory. In pure form the elements of the periodic table have provided excellent materials for scientific research in superconductivity. None of these pure elements have, however, contributed to applications of superconductivity on a large scale, like wires and cables for magnets. However, on a small scale Pb and Nb have been used for advanced development of Josephson technology. For SQUIDs (superconducting quantum interference device) niobium has been the best material overall, and is widely preferred in those particular low-Tc applications, to be discussed in Chapters 5 and 11.

LOW-Tc SUPERCONDUCTORS

2.2.2

29

Binary alloys and stoichiometric compounds

The earliest work on binary alloys has been largely forgotten, partly due to the overwhelming number of compounds that have been made and tested in later years. One person alone, Bernd T. Matthias, is said to have made some 3000 different alloys in his heroic attempt to achieve high-Tc superconductivity during the 1950s and 1960s. These efforts never succeeded, a fact which in itself gave strong impetus to go in totally new directions in more recent years. The history of the development of Tc is shown in Figure 2.1. The record shows [2] that research on binary alloys was started already in 1928 in Leiden by de Haas and Voogd. They found superconductivity in

180

160

* *

HgBaCaCuO 1993

Liq. CF4 140

TlBaCaCuO

120

BiSrCaCuO 1988 100 Tc(K)

YBCO (LBCO) 1987

80

60

Liq. N2

* = under pressure * LaBaCuO 1986

40

20

Liq H2

NbN NbC

Nb3Sn

Nb3Ge

V3Si Nb-Al-Ge Hg Pb Nb 0 Liq. He 1900 1920 1960 1980 1940 Year

Figure 2.1

*

History of Tc .

2000

30

SUPERCONDUCTING MATERIALS

A B

Figure 2.2

The A15-structure, A3 B.

SbSn, Sb2 Sn, Cu3 Sn, and Bi5 Tl3 . They noticed that the combination of a superconducting element with a non-superconducting one was successful. In Bi5 Tl3 , Tc was raised by a factor of 2–3 compared to pure Tl. What was even more interesting, was that the magnetic threshold for destruction of superconductivity in this material was much higher than in any of the elements known to be superconducting at the time. The material would remain superconducting up to 0.5 T at 3.4 K, and by extrapolation it was predicted to tolerate 0.9 T at 1.3 K. But soon they found an even more promising material; a Pb–Bi eutectic alloy with a critical field Bc = 2.3 T at 1.9 K. Unfortunately, the substance was so difficult to make and to handle that it never was to fulfill its promise as a material for wires, which might otherwise have made it an important material for superconducting electromagnets. After an intense period of research on binary alloys around 1930, not much happened in the materials area until Bernd T. Mattias and John K. Hulm started a new programme in the US in the early 1950s. Their ‘materials approach’ to superconductivity would bear rich fruit. A number of new compounds were made, with impressively high Tc and high critical fields. Throughout the 1950s the materials that were developed for use as superconductors included: solid solutions of NbN and NbC with Tc = 17.8 K; V3 Si with Tc = 17 K; Nb3 Sn with Tc = 18 K; NbTi with Tc = 9 K. Later (1973) Nb3 Ge was added to this list with the highest Tc of all, at 23.2 K, a record that lasted until 1986. We refer to Table 2.2 for some additional facts. The intermetallic compounds, just mentioned, belonging to the A3 B type of materials are classified as A15 compounds (Figure 2.2). They share a special feature, namely a softening of an elastic mode above Tc , a property which suggests relating their high transition temperatures to enhanced electron–phonon interaction caused by the softening. The two materials that have led to successful industrial production of low-temperature superconducting magnets are Nb3 Sn and NbTi. The first one is a stoichiometric, intermetallic compound, the second an alloy. These have paved the way for superconducting technology to

ORGANIC SUPERCONDUCTORS

31

Table 2.2 Some binary alloys and stoichiometric compounds. Values of Tc and Bc2 (0) may vary somewhat depending on precise composition Compound V3 Si Nb3 Sn Nb3 Ge V3 Ga NbTi VTi

Tc [K]

Bc2 (0) [T]

17 18 23.2 14 9 7

25 24 38 21 15 11

B

A e−

a

b e−

d+

d−

c

d

Figure 2.3 Predicted model substance for organic superconductor (Adapted from Little, 1964 [14]).

conquer the market for large laboratory magnets and magnetic resonance imaging magnets over the entire industrialized world. Behind this development lay great efforts in processing and materials science, as well as daring ventures into science-driven technological developments. Among the technical achievements were processing methods to make wires consisting of a large number of very thin filaments, a necessary procedure in order to stabilize the superconductor in a normal matrix.

2.3 Organic superconductors 2.3.1

Polymer and stacked molecular type

Research on electronically conductive organic materials dates back to the 1940s. High electrical conductivity was first discovered in 1954, in perylene bromine complex. Much later the discovery of a pronounced conductivity peak in (TTF)(TCNQ) near 60 K in 1973 [13] stimulated a lot of effort in the direction of low-dimensional systems, so-called charge transfer salts. Superconductivity in a polymer material was first found in (Sn)x in 1975. This was followed by the discovery in 1979 of superconductivity in a molecular salt,

32

SUPERCONDUCTING MATERIALS

Table 2.3 Some selected organic superconductors Material

Symmetry of counter molecule

(TMTSF)2 PF6 (TMTSF)2 ClO4 βL − (ET)2 I3 κ − (ET)2 Cu(NCS)2 κ − (ET)2 Cu[N(CN)2 ]Br α − (ET)2 RbHg(SCN)4 κH − (ET)2 Ag(CF3 )4 · TCE κL − (ET)2 Ag(CF3 )4 · 112DCBE κH − (ET)2 Au(CF3 )4 · TCE λ − (BETS)2 GaCl4

Octahedral Tetrahedral Linear Polymeric Polymeric Polymeric Planar Planar Planar Tetrahedral

TCE: 112DCBE:

1,1,2-trichloroethane 1,1-dichloro-2-bromoethane

H3C C

Se

Se C

C H3C

CH3 H2C

C

Se

Se

0.9 1.4 1.5 10.4 11.8 0.5 11.1 4.1 10.5 8

S

C C

H2C

CH3

Tc [K]

S

C

S C

C

S

S

TMTSF

S C

CH2

C S

C S

CH2

ET (BEDT-TTF) S H2C H2C

C

Se

Se C

C S

Se

S C

CH2

C Se

C S

CH2

BETS (BEDT-TSF)

(TMTSF)2 FF6 under 1.2 Gpa pressure, and with a Tc of 0.9 K [15]. Since then, a long list of organic superconductors have been synthesized, some of which are seen in Table 2.3. Tc remains low, although it has increased by a factor of more than 10 since the first discovery. In this sense progress has been remarkable. In another sense it has been disappointing, since predictions had been made for roomtemperature superconductivity in stacked organic structures. This prediction was set forth in 1964 by Little [14] in a paper where he suggested the possible existence of superconductivity in an organic substance consisting of a long unsaturated polyene chain, called the ‘spine’, with an array of side chain molecules attached at regular intervals (see Figure 2.3). He showed that even if the spine was initially an insulator because the valence bond was full and the conduction bond was empty, the addition of side chains could increase the effective electron–electron attraction to the point where it became energetically favourable to enter the superconducting state by mixing in states of the conduction band. It was concluded that superconductivity at room temperature could result. This paper in particular stimulated a worldwide effort to discover superconductivity in substances of appropriately stacked organic structures. The mechanism proposed by Little has later become known as the polaron mechanism. It is

ORGANIC SUPERCONDUCTORS

33

an alternative to the phonon mechanism, which was the one worked out in detail in the BCS-paper. Due to the higher energies involved in this new mechanism, Tc was expected to be much higher in the polaronic superconductors than in those with phonon-mediated pairing. Some of the organic superconductors are best described as a stack of twodimensional superconducting sheets with Josephson coupling between them. A good example is the so-called κ-type BEDT-TTF salts. They have different zero-degree coherence length ξ0 and ξ0⊥ in the stacking plane and normal to it, respectively. Table 2.4 shows Tc and coherence lengths for four different ET compounds, as determined by analysis of magnetic measurements. One finds the remarkable result that the interplanar coherence length ξ0⊥ is shorter than the interplanar distance by a factor of about 5. Supercurrent in the direction normal to the stacking planes must therefore be carried by Cooper pair tunnelling, so-called Josephson tunnelling. We refer to Chapter 5 for a discussion of the physics of Josephson tunnelling. What determines the important coherence length? Disregarding anisotropy for the moment, let us call this length ξ0 . A simple argument by means of the uncertainty principle leads to the following expression: ξ0 ≈

vF kTc

(2.1)

where is Planck‘s constant divided by 2π , vF is the Fermi velocity, and k is the Boltzmann constant. This indicates an inverse relationship between Tc and ξ0 , and proportionality between ξ0 and vF . Ideally we would want both ξ0 and Tc to be high, Tc for obvious reasons, ξ0 because a higher value provides better stability of the superconducting state. But clearly, a compromise is the best one can hope for. We see from the values in Table 2.4 that ξ0 in the 2D-plane is much longer than in the direction normal to the plains. This gives an indication for a ‘design-criterion’ for stacked superconductors. We shall encounter a similar situation in the inorganic high-Tc compounds in Section 2.5.

Table 2.4 Tc , and coherence lengths normal to the stacking plane ξ0⊥ , and parallel, ξ0 , for some ‘ET ’-compounds Material

Tc [K]

ξ0⊥ [nm]

ξ0 [nm]

κ − (ET)2 Cu(NCS)2

8.7 ± 0.2

0.31 ± 0.05

2.9 ± 0.5

κ − (d8 − ET)2 Cu(NCS)2

9.0 ± 0.2

0.32 ± 0.05

2.9 ± 0.5

κ − (ET)2 Cu[N(CN)2 ]Br

10.9 ± 0.2

0.58 ± 0.1

2.3 ± 0.4

κ − (d8 − ET)2 Cu[N(CN)2 ]Br

10.6 ± 0.2

0.57 ± 0.1

2.3 ± 0.4

After Ishiguro et al. [13].

34

SUPERCONDUCTING MATERIALS

2.3.2

Fullerene superconductors

The Buckminster fullerene C60 is a carbon molecule containing 60 atoms located at the vertices formed by the intersections of 12 pentagonal and 20 hexagonal faces, altogether forming a closed cage, as shown in Figure 2.4. We note that all atoms are in equivalent positions, where each is surrounded by one pentagon and two hexagons. One π electron and three σ electrons form a sp2 hybrid orbital. C60 condenses into an fcc structure, leaving room for introduction of small interstitial dopants like K and Rb. Other structures are bct K4 C60 and bcc K6 C60 . A significant transfer of electrons from K 4s orbitals to the C60 conducting band takes place. The electrical conductivity increases with dopant concentration, with a maximum for K3 C60 . The resulting substances have a well-defined Fermi surface. Superconductivity has been observed in a number of fullerene-based materials. The initial discovery was made in K3 C60 [16]. As shown in Table 2.5, transition temperatures go as high as 40 K. In Table 2.8 in the last section of this chapter a Tc as high as 45 K is indicated. Critical fields Hc2 are quite high, 28 T in K3 C60 and 38 T in Rb3 C60 . The fullerenes have been carefully studied with respect to isotope effects in Tc -values. The presence of significant Tc -dependence on atomic masses indicates electron–phonon mediated superconductivity. The presence of the Hebel–Slichter peak in nuclear magnetic resonance (NMR) (see Chapter 4) is considered definite proof that the BCS mechanism discussed in Chapter 3 is active.

Figure 2.4

Structure of C60-molecule (Buckminster ball).

OXIDE SUPERCONDUCTORS BEFORE THE CUPRATES

35

Table 2.5 Structure and Tc ’s of some fullerene type superconductors Material

Symmetry of the salts

Tc [K]

K3 C60 Cs2 RbC60 (NH3 )4 Na2 CsC60 Cs3 C60 NH3 K3 C60 Rbx (OMTTF)C60 (benzene)

fcc fcc fcc bct/bcc Orthorhombic

19.3 33 29.6 40 28 26

fcc = face-centered cubic, bct = body-centered tetragonal, bcc = body-centered cubic, OMTTF = octamethylenetetrathiafulvalene.

2.4

Chevrel phase materials

Superconductors referred to as Chevrel phase materials were discovered in 1971 (Figure 2.5) [17]. These are ternary molybdenum chalcogenides of composition MMo6 X8 , where X is one of the chalcogenes S, Se, or Te. M can be one of many different metals or rare earths. A most remarkable property of these compounds is the high critical magnetic field of some of them, as listed in Table 2.6. Figure 2.6 shows the temperature dependence of Bc2 (T ) for a number of low-Tc superconductors.

2.5 Oxide superconductors before the cuprates Superconductivity was found in 1964 in the perovskite oxide SrTiO3 [18], whose structure is shown in Figure 2.7. The following oxide compounds were found to exhibit superconductivity: doped SrTiO3−δ , NbO, and TiO. They had Tc ’s X = S, Se, Te Mo M

Figure 2.5

Structure of the Chevrel phase.

36

SUPERCONDUCTING MATERIALS

Table 2.6 Critical temperatures Tc , and critical fields Bc2 in some Chevrel phase materials Compound

Tc (K)

Bc2 (T)

SnMo6 S8 PbMo6 S8 LaMo6 S8

12 15 7

34 60 45

1) Nb3Ge 2) Nb79(AlGe)21 3) PbGd0.2Mo6S8 4) PbMo6S8 5) Nb0.3Ti0.7 6) Ti0.5V0.5 7) TaS1Se1 8) TaS2 (pyridin)

60 MxMo6S8

m0Hc2 (T)

50

40

30

20

Schicht

A-15

5) Nb-Ti 10

6)

V-Ti

8) 7) 0

2

4

6

1)

3) 4)

2)

8 10 12 14 16 18 20 22 T (K)

Figure 2.6 Upper critical field µ0 Hc2 versus temperature in various superconductors. After Fischer [19].

O Sr Ti

Figure 2.7

The cubic ABX3 structure. A prominent example is SrTiO3 .

HIGH-Tc CUPRATE SUPERCONDUCTORS

37

in the range 0.7 K to 2 K. In the years after 1964, bronzes were found to be superconductors: Kx WO3 , Kx MoO3 , Kx ReO3 . These had Tc ’s in the 4–6 K range. The 1970s brought discoveries of LiTi2 O4 and Ba(PbBi)O3 , both with Tc = 13 K. Naturally, they all had low carrier density. By now the results were encouraging, and the development pointed to oxide perovskites as a possibly promising class of materials. Some groups therefore pursued such a course.

2.6 High-Tc cuprate superconductors 2.6.1

The discovery of cuprate superconductors

The breakthrough to a new era in higher superconducting transition temperatures came in 1986 by the discovery of superconductivity in the La2−x (Ba,Sr)x CuO compounds by two scientists at the IBM Zurich laboratory, J. George Bednorz and K. Alex M¨uller [9]. Figure 2.8 shows the corresponding undoped mother perovskite La2 CuO4 . In their article in Zeitschrift f¨ur Physik they cautiously announced: ‘Possible high Tc superconductivity in the Ba-La-Cu-O system.’ Their material showed onset of superconductivity at about 30 K, well above previous records (see Figure 2.9). Initially the reaction from the scientific community was somewhat reluctant, but this changed to intense interest and competition, as soon as their results were confirmed by other groups, in Japan, in the US and China. The next important development occurred when the Houston group lead by Chu showed that external pressure could raise Tc substantially, going above 40 K under 13 kbar pressure [20]. An effect which is equivalent to application of

O La Cu

Figure 2.8 La2 CuO4 tetragonal crystallographic unit cell.

38

SUPERCONDUCTING MATERIALS

0.05

Resistivity r(Ω cm)

0.04

0.03

0.02

I = 0.50A/cm2

0.01

0

0

100 200 Temperature (K)

300

Figure 2.9 Resistivity versus temperature in La2−x Bax CuO. After the original publication by Bednorz and M¨uller, 1986 [9].

high pressure is achieved by replacing some of the ions with smaller ones having the same chemical properties. Thus, replacing Ba with the smaller ion Sr led to a Tc of 38 K. Naturally, one would think that a similar procedure ought to be tried at the La-site. The Huntsville group led by Wu proceeded in collaboration with the Houston group to replace both La and Ba, with Y and Sr, respectively. This suddenly brought Tc above 90 K [21].The news spread quickly all over the world. Soon the successful new compound turned out to be YBa2 Cu3 O7 (Figure 2.10). The discovery was made more or less simultaneously in several laboratories, in Tokyo, Beijing and at Bell Labs in the US. This breakthrough was of historic proportions. Tc had now moved well above the boiling point of liquid N2 at 77 K. The best values of Tc turned out to be in the range 91–93 K in YBa2 Cu3 O7−δ , depending on the value of δ (see Figure 2.11). The ensuing response from the scientific community was without parallel in the history of science. Suddenly, the efforts were joined by thousands of scientists and students around the world, trying to understand YBa2 Cu3 O7−δ and the other newly discovered compounds, and to push Tc even higher. Several new compounds with higher Tc were soon synthesized. With one exception, Ba1−x Kx BiO3 , all had one common feature: a quasi-2D network of CuO2 – i.e. they were all cuprate perovskites. The new materials are very different from traditional metals, being doped oxides. Their normal state properties are different from metals, and they are so strongly anisotropic that they could be shown in some cases to possess metallic-like conductivity in directions parallel to the CuO2 planes – although not free-electron like – while behaving

HIGH-Tc CUPRATE SUPERCONDUCTORS

39

Charge reservoir layer

Conduction layer

Cu O Charge reservoir layer

Y Ba

Figure 2.10 Structure of orthorhombic YBa2 Cu3 O7 . 100

Tc(K)

80 60 40 20 Normal 0 0.0

Superconductor 0.5 Oxygen content x

1.0

Figure 2.11 Tc versus x in YBa2 Cu3 O6+x . Data from Cava et al. (circles) [21] and from Jorgensen et al. (triangles) [22].

like semiconductors along the c-axis, normal to CuO2 planes. This profound anisotropy affects essentially all physical properties [23]. In the ensuing years huge efforts were spent on achieving superconductivity at still higher temperatures, even with the hope of reaching room temperature. This did not happen, but the efforts resulted in a long list of new superconducting compounds with complex structures and intriguing properties. A superconducting transition temperature as high as 163 K was eventually reported in the Hg-based HgBa2 Ca2 Cu3 O8 compound at a high external pressure. We refer again to Figure 2.1 which summarizes the main historical development of Tc

40

SUPERCONDUCTING MATERIALS

versus time. For further details about the historical record we refer the reader to Dahl [2].

2.6.2

Composition and structure

Referring now to Figure 2.10 showing the YBCO structure, one clearly sees the connection to the simple cubic perovskites. Essentially, YBCO is a stack of three perovskite unit cells where, compared to the basic model ABX3 (Figure 2.7), with atoms removed in some places and substituted in other places. The typical oxygen octahedra, so familiar in the ABX3 compounds like SrTiO3 have been split in two by a middle layer, and Ba replaces Y as the central atom in two out of three layers. We notice also that YBa2 Cu3 O7 is a modification of the structurally simpler compound YBa2 Cu3 O6 . Processing of high-Tc superconductors to single-phase material requires elaborate processes, which we will not go in details about here. Let us just remark that as far as YBCO is concerned the processing route usually goes via making the non-superconducting YBa2 Cu3 O6 first. This materials may be obtained under appropriate conditions in an oxygen atmosphere from a mixture of Y2 O3 + BaO + CuOx , heated to over 900 ◦ C. The resulting material is of tetragonal structure, with a lot of oxygen vacancies. On lowering the temperature to somewhere between 400 ◦ C and 500 ◦ C more oxygen is absorbed by the structure and a different oxygen ordering takes place, with Cu-O chains, as shown in Figure 2.10. The chain formation

Figure 2.12 Permanent magnet levitating above a chunk of high-Tc superconducting Y1 Ba2 Cu3 O7 .

HIGH-Tc CUPRATE SUPERCONDUCTORS

41

breaks the tetragonal structure with different lattice parameters along the a- and b-directions. A subsequent quenching of the material traps the oxygen in the structure. When all available oxygen sites are filled in this structure we have the YBa2 Cu3 O7 compound shown. Doping of SrTiO3 had been demonstrated to lead to superconductivity due to a reduction process, whereby oxygen was removed. The situation in YBCO is related, but more complicated, as can be seen in Figure 2.11. Starting with the YBa2 Cu3 O6+x structure at x = 0 and increasing the oxygen content via external oxygen supply at high temperatures the compound at first is an insulator, but becomes a superconductor at x-values grater than 0.4. From there on Tc increases until it goes through a maximum at x ≈ 0.93, and diminishes slightly until x = 1 is reached. Optimal doping (corresponding to the highest Tc ) of YBCO therefore is achieved in Y1 Ba2 Cu3 O7−δ with δ ≈ 0.07. On inspecting the resulting structure, one plane at a time, one finds that the orthorhombic YBCO structure consists of layers as do all high-Tc compounds. Beginning at the bottom and proceeding upwards they are: CuO, BaO, CuO2 , Y, CuO2 , BaO, CuO. The CuO2 layers are superconducting in YBCO like in all other high-Tc materials. But YBCO possesses the additional CuO chains, as mentioned. These can also be superconducting, depending on the degree of filling. In this respect YBCO is unique among high-Tc materials. Another aspect of this structure is that the oxygens are not in equivalent positions in the lattice, contrary to ABO3 type structures. There are four inequivalent O sites and two inequivalent Cu sites.

2.6.3

Making high Tc materials

High-Tc materials, being doped oxides, are made by heating a mixture of appropriate amounts of metal oxides in powder form to temperatures in the range 850–950 ◦ C. Materials that contain some percentage of superconductor are then easily obtained. But making materials of good quality, whether polycrystalline or single crystals is quite a different and highly non-trivial matter. Only quite elaborate procedures with attention paid to every detail of composition, temperature, pressure and atmosphere will bring out high quality materials. Regrinding, compressing and sintering repeatedly, is usually necessary. The resulting bulk material is then a fine-grained ceramic, brittle, and with high density of defects and grain boundaries. Making the big step towards single crystals is an even greater challenge. Growing large crystals of high quality has turned out to be extremely difficult. The main reason for this is to be found in the layered structure, which permits easy diffusion and growth along the (a, b)-planes, but allows only very slow diffusion and growth along the c-direction. Some of these materials end up quite ‘flaky’, like in the Bi-based materials where layer by layer may be peeled off quite easily. This is an intrinsic property of the material

42

SUPERCONDUCTING MATERIALS CuO

BaCuO2 Ba2CuO3

YBa2Cu3O7−d

Y2Cu2O5

YBa4Cu3O8.5 Y2BaCuO5−d

BaO

Y2BaO4

YO1.5

Figure 2.13 Isothermal phase diagram for the Y2 O3 -BaO-CuOx system at 900 ◦ C in 1 atm oxygen. Calculations by Rian [24]. Lines connect phases which exist in equilibrium at this temperature.

itself, reflecting the great anisotropy. Much of the difficulty in crystal growth and processing lies also in the fact that even the simplest of them are quaternary compounds. When 3 oxides are mixed, several different phases may result. Figure 2.13 shows a chemical equilibrium phase diagram relevant to YBCO. Matters grew even more complex when it turned out that the road to higher Tc went through compounds like Bi2 Sr2 Ca2 Cu3 O10+δ or Bi2 Sr2 Ca1 Cu2 O8+δ , with four metal ions, as can be seen in Figure 2.14, and several similar ones with Tl or Hg replacing Bi. In the process of making such substances a number of unwanted phases will normally be created. In this case perfection is practically impossible in bulk production, but single crystals may be grown. In order to study the intrinsic properties of new materials, access to single crystals is a necessity. Table 2.7 shows a list of high-Tc compounds, with corresponding Tc -values.

2.6.4

Phase diagrams and doping

Superconductivity in high Tc materials depends on appropriate doping; and the phase diagrams show a remarkable similarity: as a function of the appropriate doping parameter they all have an antiferromagnetic phase near zero doping, followed by an insulating phase, then the superconducting phase underneath a sort of metallic phase in a certain doping range, and finally Tc goes to 0 again. The typical situation is sketched in Figure 2.15, where the various phases

HIGH-Tc CUPRATE SUPERCONDUCTORS

43

BiO

BiO SrO CuO2 Ca CuO2 SrO BiO

BiO

SrO

Figure 2.14

Structure of Bi2 Sr2 CaCu2 O8 crystal.

are indicated. One finds the peculiar property that in every substance there exists a range of x-values, where superconductivity is observed, with optimal doping corresponding to the highest Tc , somewhere near the middle of that range. Above this dome-shaped curve is the ‘normal’ state, a kind of unconventional metallic region. To the left of the dotted line in Figure 2.15 is a region which is often referred to as that of a ‘strange’ metal, while to the right of the same line one finds more normal metallic properties. Much of the secret of highTc compounds may be found in these peculiar normal state properties. Often the question is asked: how can we understand high-Tc superconductivity if we don’t even understand the normal state? Anderson is the scientist who most relentlessly has pursued this question [25].

44

SUPERCONDUCTING MATERIALS

Table 2.7 Some representative examples of high-Tc cuprate superconductors and their Tc ’s. The reported values of Tc will vary somewhat, depending on the processing conditions and resulting oxygen content and other deviations from stoichiometry Compound

Tc [K]

Nicknames

39 92 84 110 90 110 125 91 116 122 95 122 133 25

LCCO or LaSCCO Y123 or YBCO Bi2212 or BiSCCO Bi2223 or BiSCCO

La1.85 Sr0.15 CuO4 YBa2 Cu3 O7 Bi2 Sr2 CaCu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 CuO6 Tl2 Ba2 CaCu2 O8 Tl2 Ba2 Ca2 Cu3 O10 TlBa2 CaCu2 O7 TlBa2 Ca2 Cu3 O9 TlBa2 Ca3 Cu4 O11 HgBa2 CuO4 HgBa2 CaCu2 O6 HgBa2 Ca2 Cu3 O8 Nd1.85 Ce0.15CuO4−y

Tl2223 or TBCCO

Hg1223 or HBCCO NCCO

300

T* TN

T (K)

200

Optimally doped metal (non-Fermi-liquid)

Pseudogap Underdoped insulator

100

Overdoped metal (Fermi-liquid)

AFM Tc Insulator Superconducting 0 0

0.10

0.20

0.30

x

Figure 2.15 Typical overall phase diagram with doping in high-Tc cuprate superconductors (AFM = antiferromagnetic phase).

HIGH-Tc CUPRATE SUPERCONDUCTORS

45

40

10 0

0.05

0.10

0.15 0.20 Doping x

Tetragonal

20

Orthorhombic

Tc(K)

30

0.25

0.30

Figure 2.16 Tc versus doping in La1−x Srx CuO4 . Data from Radelli et al. [26].

How doping is achieved, i.e. how the parameter x on the horizontal axis of Figure 2.15 is controlled, depends on the compound. In the case of the La-based, original high-Tc materials, the key is to replace trivalent La with divalent Ba or Sr (Figure 2.16). Because the basic compound La2 CuO4 is charge neutral, replacing La3+ with Ba2+ and still demanding charge neutrality results in a freed positive charge, donated to the valence band. On the other hand, in the case of oxygen depletion, removing an oxygen atom leaves behind two incomplete bonds, which upon completion free two positive charges, or holes. The charge structure of the cuprates can be described in a very simple block form by separating the superconducting atomic layers from the non-conducting ones, as shown in Figure 2.10 for the case of YBa2 Cu3 O7 . This case is special due to the existence of CuO chains. But the general charge structure scheme for all cuprate superconductors is as follows: A stack of alternating layers of charge reservoirs (like BaO or CuO) and conducting CuO2 layers that receive the mobile charges (usually holes) from the charge reservoirs. This internal redistribution of charge occurs in a fine tuned balance between the valences (affinities) of participating atoms. The undoped YBa2 Cu3 O6 has an insulating CuO2 layer where the d9 electrons of Cu2+ ions are antiferromagnetically bound. On admitting oxygen to YBa2 Cu3 O6 the chains are formed at the expense of taking away the necessary two electrons per atom from the CuO2 -plane. This is equivalent to doping the CuO2 plane with positive mobile charges, or holes. The result is a hole-like superconductor. The process is different in La2−x Bax CuO4 , where Ba2+ replaces La3+ , but the result is similar. When Ba is brought into the insulating La2 CuO4 unit cells, it delivers two negative charges to the bonds, but it needs one more to make up for three electrons donated by La, so an extra electron is taken from CuO2 to complete all bonds, and thereby a hole is released in the CuO2 plane, to give conduction. Although hole- doping is the rule in highTc superconductors there are some cases where the mobile charges are electrons. Figure 2.17 shows these possibilities for both types of carriers where the aspect

46

SUPERCONDUCTING MATERIALS Metallic

Insulating

Temperature T(K)

Electron-doped Nd2−xCexCuO4−y

Metallic

Hole-doped La2−xSrxCuO4−y

200

N-type

P-type 100

P-type

N-type

AFM SC

AFM

SG SC

0.3

0 Concentration x in Ln2−xMxCuO4−y

0.4

Detector output 1.0 mV

Figure 2.17 Comparison of electron-doped and hole-doped superconductor. The assignment SG refers to the possible existence of a spin glass phase.

0

100

200 Time (s)

300

400

Figure 2.18 These measurements of flux jumps in a superconducting ring gave the first verification of the flux quantisation according to 0 = 2e h in high-Tc superconductors. Adapted from [27].

of electron-hole symmetry is emphasized. Upon learning that these materials are dominated by hole carriers, one might ask: What about the pairing of carriers, is it still as we know it from the low-Tc metallic superconductors? The answer was found quite early by the Birmingham group [27] who demonstrated that flux quantization was intact in the new materials, and that the flux quantum was h 0 = 2e as before. In this sense it did not matter what the sign of the charge is. The measurements which provided proof of pairing in high-Tc superconductors are shown in Figure 2.18.

HIGH-Tc CUPRATE SUPERCONDUCTORS

2.6.5

47

Some remarks on the original idea which led to the discovery of cuprate superconductors

In spite of all efforts which have been spent on establishing a theoretical understanding of superconductivity in cuprate perovskites, a final conclusion on this matter has not yet been reached. It is nevertheless quite interesting to follow the reasoning which led Bednorz and M¨uller on the right track. We quote here a section taken directly from a paper given by M¨uller on the occasion of the celebration of the first 10 years of high-Tc superconductivity in 1996 [28]. (for simplicity we omit here the numerous references given): Strong electron-phonon interactions can occur in oxides, owing to polaron formation as well as mixed-valence states. This can go beyond the standard BCS theory. A phase diagram with a superconducting to bipolaronic insulator transition was proposed early by Chakraverty. A mechanism for polaron formation is the Jahn–Teller (JT) effect as studied by H¨ock et al. in a linear chain model. From it, one expects heavy polaron masses if the JT stabilization energy becomes comparable to or larger than the bandwidth of the degenerate orbitals, and thus localization. Intermediate polarons are expected if the JT energy is not too large compared to the bandwidth. We recall that the JT theorem states the following: A nonlinear molecule or a defect in a crystal lattice exhibiting an electron degeneracy will spontaneously distort in lowering its symmetry, thereby removing its degeneracy. Isolated Fe4+ , Mn3+ , Ni3+ and Cu2+ in an octahedral oxygen environment show strong JT effects because their incompletely occupied eg orbitals, transforming as 3z2 − r 2 and x 2 − y 2 , point towards the negatively charged oxygen ligands. Although SrFe4+ O3 is a distorted perovskite insulator, LaNiO3 is a JT undistorted metal in which the transfer energy bπ of the eg electrons of the Ni3+ is large enough to quench the JT distortion. On the other hand, LaCuO3 is a metal containing only the non-JT Cu3+ . Therefore, it was decided to investigate and ‘engineer’ nickel- and copper-containing oxides, with reduced bandwidth bπ , partially containing Ni3+ or Cu2+ states. The JT polaron proposed in 1983 was one envisaged to lead to a heavy mass of the particle; and intermediate, mobile polaron suited for superconductivity was not considered. However, in the ferromagnetic conductor La1−x Cax MnO3 , a giant oxygen isotope effect has been discovered most recently and ascribed to the presence of intermediate JT polarons due to the Mn3+ ions in the oxide. This important and new evidence for the existence of intermediate JT polarons is quite in favor of the new original concept. In R¨usclikon, there was a tradition of more than two decades of research in insulating oxides that undergo structural and ferroelectric transitions, which was a strong motivation to pursue the program. Furthermore, in 1979 the present author had started to work in the field of granular superconductors in which small Al grains are surrounded by amorphous Al2 O3 . In these systems Tc ’s have been reported to be as high as 5 K, compared to pure Al with a Tc of 1.1 K. In our laboratory, the search for superconductivity was initiated together with J. G. Bednorz in mid-summer of 1983. our efforts first concentrated on Ni3+ -containing perovskites, such as mixed crystals of LaNiO3 and LaAlO3 . In these unpublished efforts, the metallic behavior of the various synthesized double and triple oxides was measured, and at low temperatures

48

SUPERCONDUCTING MATERIALS

they exhibited localization upon cooling. This indicated the possible existence of JT polarons, however, without any signs of superconductivity. In Figure 2.9, results of these efforts are reproduced. In late summer of 1985, the efforts were shifted to copper-containing compounds, such as LaCuO3 . Because Cu3+ has two electrons in the eg subshell, the latter is half-filled. Thus, its ground state is not degenerate. It was clear that an oxide with mixed Cu2+ /Cu3+ or Cu3+ /Cu4+ had to be tried. At this stage, Bednorz became aware of a paper by Michael, Er-Rakho and Raveau on the mixed perovskite BaLa4 Cu5 O13.4 , exactly meeting the requirements of mixed valence. The French authors had shown that this mixed oxide, a metal at room temperature and above, contained Cu2+ and Cu3+ . Thus, we tried to reproduce it, at the same time continuously varying the Cu2+ /Cu3+ ratio by changing the Ba concentration on Bax La5−x Cu5 O5(3−y) , and we looked for superconductivity. A representative and concise account of the discovery of superconductivity in Bax La5−x Cu5 O5(3−y) and the relevant superconducting phase present appeared in the September 4, 1987, issue of Science and, in more detail, in the first of the two Nobel lectures in 1987, and would exceed the scope of this contribution.

2.6.6

Thermal fluctuations of the superconducting condensate. A preliminary discussion

Already in 1988 two more significant series of high-Tc superconductors were synthesized: one Bi-based, and one Tl-based. Later, a Hg-based series was also found. These series gave Tc ’s higher than the 93 K of YBCO, as could already be seen from Table 2.7. At the same time, however, their anisotropy was found to be much stronger than in YBCO, and the coherence length is very short, both a disadvantage and a challenge for their practical use. Why the coherence length is so short can be seen from Eq. 2.1, which can be obtained from the BCS theory, and may be assumed to hold approximately even in high-Tc . Equation 2.1 predicts a very short coherence length in high-Tc due to the combination of small Fermi surfaces with low vF , caused by the low concentration of holes, and the high Tc . The expression used here may also be derived from the uncertainty relation, and is not sensitive to the pairing mechanism. This prediction for ξ0 is approximately followed in real systems. While ξ0 = 1600 nm in Al, it is only of the order of 1 nm in the high-Tc compounds. This gives the thermal energy of kT a chance to create fluctuations of large spatial extent in the order parameter since they will occur in a typical volume ξ 3 . This volume is of the order of (1/1600)3 = 2.4 × 10−10 times smaller in high Tc materials than in aluminium. The energy barrier E against the creation of a fluctuation in the order parameter is proportional to the respective volumes ξ 3 in each case, and also proportional to the square of the thermodynamic field, i.e.

HIGH-Tc CUPRATE SUPERCONDUCTORS

E ≈

1 3 2 ξ Bc 2µ0

49 (2.2)

The ratio of condensation energies in a volume of ξ¯ 3 in the two materials is therefore

EYBCO (ξ¯ 3 Bc2 )YBCO =

EAl (ξ¯ 3 Bc2 )Al

(2.3)

where we have written ξ¯ 3 to indicate a geometric average of ξ1 ξ2 ξ3 for the anisotropic cases. A numerical estimate of the barrier ratio expressed by Eq. 2.3 gives 1.3 × 10−6 , favouring fluctuations enormously in YBCO as compared to Al. The ratio of probabilities for thermal fluctuations at a temperature T can be written as −

E kT YBCO

p1 e PYBCO = PAl − E kT Al p2 e

−

=

p1 e

ξ¯ 3 Bc2 2µ0 kT

−

p2 e

ξ¯ 3 Bc2 2µ0 kT

YBCO

(2.4)

Al

Let us try to gain some insight into the consequences of Eq. 2.4. Here the exponents are far more important than the unknown coefficients p1 and p2 . From measurement, Bc in aluminium is 0.02 T, and Bc in YBCO may be taken to be about 1.5 T. The ξ0 -values for YBCO and Al, can be estimated from Eq. 2.1. For Al, vF = 2.03 × 106 and Tc = 1.17 K which gives the estimate ξ0 = 2.2 × 103 nm. This is not too far away from the measured value, ξ0 = 1.6 × 103 nm. For YBCO, vF is about 100 times lower than in Al. This tells us that the ratio of coherence lengths ξAl /ξ¯YBCO should be about 104 , which is of the correct magnitude compared to measured values. Furthermore, the ratio between fluctuating volumes (ξAl )3 /(ξ¯YBCO )3 is about 1012 . So, not only is the fluctuating volume in YBCO a factor 10−12 smaller than in Al, but since the fluctuations take place at temperatures near 100 K in YBCO, versus 1 K in Al, the available energy to drive the fluctuations in YBCO is ≈102 greater. The effect of thermal fluctuations should therefore be expected to be hugely greater in YBCO than in Al. We can now estimate the exponents in Eq. 2.4 to gain an impression of the difference in probabilities for thermal fluctuations in the respective superconducting volumes of size ξ¯ 3 . For Al we find near Tc : ¯3 2 ξ Bc

E ≈ ≈ 4.0 × 107 (2.5) kT Al 2µ0 kTc Al

50

SUPERCONDUCTING MATERIALS

Clearly, this is an impossible barrier to overcome. Hence, thermally driven fluctuations in the density of Cooper pairs in a volume ξ¯ 3 in Al occur with practically vanishing probability. Let us now compare this with the situation on YBCO. We find

E kT

≈ YBCO

ξ¯ 3 Bc2 2µ0 kTc

≈1

(2.6)

YBCO

2 × ξ , and taken a rough average of In this estimate, we have written ξ¯ 3 = ξab c 3 −9 tabulated values to find ξ¯ = (1.5 × 10 m)2 × 0.5 × 10−9 m ≈ 2 × 10−27 m3 . With a resulting probability PYBCO ∝ e−1 the conclusion is that thermally driven fluctuations that suppress superconductivity in a ξ¯ 3 -volume must occur profusely. Conversely, the same argument says that in the normal state above Tc , fluctuations will occur with similar likelihood, in this case creating superconducting ξ¯ 3 -volumes in the normal matrix. In conclusion, the superconducting transitions in YBCO and other high-Tc materials, occur with such violent fluctuation of the superconducting wavefunction near Tc that the behaviour is bound to be non-classical, non-mean-field like, quite different from low-Tc physics. At this point one may even wonder how a substance with such violent fluctuations can sustain superconductivity at all near Tc . This is a very valid question indeed that will be dealt with in Chapters 9 and 10. Clearly, the superconducting phase transition in YBCO and other high-Tc superconductors is fundamentally different from low-Tc materials. The important question is how it is different. At this stage, let us also ask: What topological form will the fluctuations discussed above have? Will they always be in the shape of a ξ¯ 3 -volume as defined above? Not necessarily. There is sufficient thermal energy that the volume could be extended in one coordinate, for instance in a tubular shape, and still have a very good chance for the fluctuation to occur. As is now well established by computer-simulation there is firm prediction for a high rate of generation of thermally induced vortex loops. According to the prediction, this behaviour is accompanied by a vortex ‘blow-out’ phase transition within a vortex liquid phase [29, 30]. Figure 2.19 attempts to sketch such possibilities. These issues are discussed more precisely in Advanced Topics. It should be kept in mind for comparison, that on lowering the temperature of a high-Tc compound to liquid helium temperatures, fluctuations even in these compounds would occur with a low probability. It is the combination of high temperature, short coherence length and anisotropy which make the high-Tc compounds so different in terms of fluctuation properties at elevated temperatures. Figure 2.20 shows a highly unusual phenomenon in a high-Tc superconductor. The characteristic rule of superconductivity, that diamagnetic response is found only below Tc , is broken; diamagnetism is observed above Tc . The effect is explained by the presence of Cooper-pairs already formed above Tc .

HIGH-Tc CUPRATE SUPERCONDUCTORS

51

Figure 2.19 Sketch of possible configurations of thermally generated flux loops in high-Tc superconductors in the ordered phase as discussed by Tesanovic [31, 32], and Nguyen and Sudbø [29, 30].

1G 0

180 µG

c (emu/g)

−0.05

−0.1

−0.15

−0.2

−0.25 36

37

38

39 T (K)

40

41

42

Figure 2.20 Magnetic susceptibility in the superconductor La1.85 Sr0.15 CuO4 showing the presence of diamagnetic response (upper curves) even above Tc due to the presence of significant concentration of Cooper pairs above the superconducting phase transition. Tc is known to be 38 K from other independent measurements. The numbers given in the figure, 1 G and 180 µG, refer to the ac-field used in the measurements. Only of the lowest field did the weak superconducting resparse show up above Tc . After Thisted et al. [33].

52

SUPERCONDUCTING MATERIALS

2.7 Heavy fermion superconductors The term ‘heavy fermion superconductors’ refers to a class of superconductors characterized by very high effective electron mass, m∗ , 2-3 orders of magnitude larger than the free electron mass. The first discovery of such superconductors was made by Steglich and coworkers in 1979 [34]. The compound was CeCu2 Si2 . This discovery was later followed by UBe13 and UPt3 . The main characteristics of some of these superconductors are given in Table 2.8. Figure 2.21 shows the structure of the material where superconductivity was first discovered. Typical for these superconductors is that they contain elements like the rare earth Ce with two 4f electrons, and the actinide U with 5f electrons. When these f electrons mix or hybridize with conduction electrons a sharp band with high density of states D(E) arises at the Fermi energy. Since D(E) ∝ (m∗ )3/2 Table 2.8

Heavy fermion superconductor properties.

Superconductor

Tc (K)

Hc1 (mT)†

Hc2 (T)

λ(µm)

ξ (nm)

κ

m∗ /m0

UPt3

0.48

0.7

1.8//c 2.3//a, b 10.2 2.5//c 10.5//a 2.1//a 2.5//c

1

12//a, b 14//c 9.5 7.5//a 13//c

90

180

UBe13

0.87

6.7

URu2 Si2

1.2

0.2

CeCu2 Si2

∼1

∼2.5

∼1 ∼1 0.5

9

55

260

260

140 380

Reproduced from the website of Zbigniew Koziol http://www.iyp.org/vp/super/heavy/reference.html. † the value is estimated.

c = 9.94 Å

Si Cu Ce a = 4.10 Å

Figure 2.21

Structure of CeCuSi.

MgB2 SUPERCONDUCTOR

53

one ascribes the high density of states to the high effective mass. Hence the name referred to above. Clearly, this property carries over to other physical characteristics as well. The electronic specific heat is directly proportional to the effective mass. Hence the electronic specific heat is hugely increased compared to that of usual metals. In the superconducting state the penetration depth λ is proportional to (m∗ )1/2 . Hence this quantity is also very large, as seen in Table 2.8. Other heavy fermion superconducting compounds not included in the table are Ce3 Bi4 Pt3 , CeNi2 Ge2 , UPd2 Al3 and YBiPt. Recent research in heavy fermion superconductors indicate that they are a quite diverse group, showing distinctly non-universal behaviour. Some, like UPd2 Al3 exhibit coexistence of long-range antiferromagnetic order and a Landau Fermi-liquid phase in a range Tc < T < TN . Another group, like CeCu2 Si2 (see Figure 2.21), are intermetallics that show pronounced deviations from Landau Fermi-liquid behaviour, due to fluctuations in the local magnetization. For these and other reasons heavy fermion superconductors are still an active area of research. It is still not clear whether a generalized Fermi-liquid theory can be found to describe all superconductors in this class.

2.8

MgB2 superconductor

Magnesium diboride, MgB2 , is a metallic compound known since the 1950s. It is a hard and brittle material with a hexagonal structure, as seen in Figure 2.22, with magnesium located in the external corners and in the face centre positions of the upper and lower hexagon, and with boron located in the inner hexagon, rotated by 60◦ with respect to the Mg hexagons. Superconductivity in MgB2 was discovered as late as 2001 [35, 36], with Tc at 39 K, a record by far in an ordinary metallic compound. This value of Tc is close to what has been considered the maximum possible by pairing caused by electron–phonon interaction. MgB2 has several interesting physical properties.

B Mg

Figure 2.22 Structure of MgB2 superconductor.

A15-phase

Nb3 Ge Nb3 Sn V3 Si

Charge transfer salt Bechgaard salts, spin density wave

Non-cuprate perovskite

κ − (BEDT − TTF)2 Cu(NCS)2 (TMTSF)2 X X = ClO4 , PF6 , ReO4

Ba1−x KBiO3 ; x = 0.4

Perovskite high-Tc cuprate superconductors

Fullerene based

K3 C60 Rb3 C60 Pb2.7 Tl2.2 C60

La2−x Bax CuO4 ; x = 0.2 YBa2 Cu3 O7−δ Bi2 Sr2 Ca2 Cu3 O10 TbBa2 Ca2 Cu3 O9 HgBa2 Ca2 Cu3 O8+δ

Heavy fermion compounds

UPd2 Al3 CeCu2 Si2 UPt3

LaMo6 Se8

Chevrel phase: Mo-based chalcogenides

Layered non-cuprate

MgB2

PbMo6 S8

Category

Superconductor

30 93 110 123 133

Tc (K)

3.3 2.5 2.9 1.3

190

ξab

17–32 38

∼40 ∼2 1.9

5

60

39 24 23

19–40

Bc2 (T)

115 198

Bc2 (T)

30

8.7–10.5 0.9–1.4

19.3 29.6 45

0.46

2.0

11

15.2

23.2 17.9 17.0

39

Tc (K)

0.5 0.09

ξc

λab

500 480 3500

290 150 173 130

λc

980

240

∼3 ∼2 ∼1–10

600

215

90 65 60

85–180

λ(nm)

12–14

2.2

3 3 3

2–5

ξ (nm)

Table 2.9 Special properties of some superconductor categories

High Tc , high Bc2 , extreme Type II, anisotropic layered

Special properties

Record Tc for non-cuprate perovskite

Organic, quasi-2D Organic, quasi-1D

Organic, high Tc , molecular based

High carrier mass: m ∼ 102 me

High Tc , high Bc2

High Tc , lattice instability

Record Tc for BCS-type metal

Special properties

54 SUPERCONDUCTING MATERIALS

SUMMARIZING REMARKS

55

In addition to the high Tc -value, it has been found to have two quite distinct energy gaps caused by pairing involving electrons from different parts of the Fermi surface. The high Tc value is a compromise between the two gap values. The high Tc is favoured both by the light element boron and by strong covalent binding. The isotope effect reflected in the dependence of Tc on isotope mass is a strong indication of BCS type electron–phonon pairing mechanism. The most important phonon modes involved in the pairing are in the B-planes. The upper critical magnetic field Bc2 has not been determined with any accuracy yet. Values as high as 32 T have been reported, but much lower values have also been found. MgB2 shows promise for several applications including transport of high currents and Josephson junctions. Several other compounds of related composition have been found, but all with lower Tc than MgB2 .

2.9 Summarizing remarks In this chapter we have attempted to review some basic facts about the most important materials in superconductivity research and applications today. Necessarily such a review will be sketchy, considering the vast literature available on these subjects. Essentially, this chapter can only be an appetizer for a deeper look into this immensely rich area. Still, it is hoped that it may be sufficient for those students who want to get a broad overview, but who do not necessarily intend to pursue the subjects at a much deeper level. Finally, in Table 2.9 we summarize some special properties associated with different categories of superconductors, so that the reader can in one glance get an idea about how they differ in some important respects.

3 Fermi-Liquids and Attractive Interactions 3.1 Introduction In solid state physics, The Theory of Everything is given by a Hamiltonian of electrons moving more or less freely through a lattice of ions. Electrons and ions have a kinetic energy, and they interact with each other via the Coulomb interaction. This Hamiltonian is in some sense trivial, it is simply the sum of potential and kinetic energies. However, as we know, the amazing number of different phenomena taking place in condensed matter physics goes to show that trivial Hamiltonians need not exhibit trivial ground states. Superconductivity is an example of this. Another notable example is the fractional quantum Hall effect. The main difficulty is to be able to identify correctly the manybody renormalized low-energy excitations in various circumstances. This is what is non-trivial, and the excitations vary enormously, ranging from bosonic spinwaves in Mott–Hubbard insulators and quantum Heisenberg antiferromagnets to fermionic bogoliubons in superconductors via anyonic excitations with fractional charge in the fractional quantum Hall effect. These systems all have the same underlying microscopic Hamiltonian, and the diversity of the possible low-energy excitations basically reflect that they are emergent long-wavelength properties whose basic characteristics to some extent are a result of the initial conditions in which we have prepared the underlying electron-ion system. The grand unified theory of solid state physics is given by the Hamiltonian H = He−e + Hion−ion + He−ion

(3.1)

where He−e is the Hamiltonian for electrons moving through the solid, Hion−ion is the Hamiltonian for the ions in the solid, and He−ion is the Hamiltonian describing the coupling between the electrons and the ions. For electrons with Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

58

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

mass m and ions with mass M, we have He−e =

p2 e−e i + VCoulomb (ri − rj ) 2m i

Hion−ion =

i

He−ion =

i,j

Pi2 2M

+

e−ion VCoulomb (ri

ion−ion VCoulomb (Ri − Rj )

i,j

− Rj )

(3.2)

Here ri denotes an electron-position, while Ri denotes an ion-position. The dominant effect of the Coulomb interactions between the ions is to freeze them into a lattice. Once we have assumed the existence of this ion-lattice ion−ion ground state, VCoulomb (Ri − Rj ) has performed its principle task and we no longer need to consider it. In a perfect solid with no lattice defects and no lattice vibrations, the electrons may be considered as moving in an external periodic potential set up by the ions. Ignoring electron–electron interactions, this is basically a one-body problem of an electron moving in a periodic external potential. The exact eigenstates are Bloch-states. These states are adjusted to the perfect lattice and are not scattered at all, a perfect crystal is transparent to Bloch-electrons. Including lattice vibrations around equilibrium positions of the ions, but still no lattice defects, the Bloch-states will couple to the lattice vibrations, whose quantized excitations are bosonic phonons. We then need to include coupling of Bloch-electrons to phonons. Finally, we should include Coulomb-interactions between electrons. Hence, a sensible way of viewing the above Hamiltonian in the absence of lattice defects (we shall ignore such site-disorder) is that of Bloch-electrons with Coulomb-interactions coupled to phonons. This is the situation we shall consider. We start by describing electrons ignoring interaction effects altogether, then modify the description in the nece−e essary fashion when VCoulomb (ri − rj ), and finally include the electron-phonon interaction. In this chapter, we will give a brief introduction to the concept of Landau Fermi-liquid theory, which forms the cornerstone of our current understanding of ordinary metals. We will also present the effective Hamiltonian for phonon-mediated superconductivity, which forms the basis for the celebrated BCS theory of conventional low-temperature superconductivity arising out of good metals. The Fermi-liquid theory is a spectacularly successful framework which transforms the daunting problem of interacting electron systems into a theory which conceptually is almost as simple as the non-interacting electron gas. We will also give a brief review of why such a drastic simplification of the problem actually works, even in extreme cases like the heavy fermion compounds. The accepted theory of conventional phonon-mediated superconductivity we have available today for superconductivity (namely the BCS theory,

THE NON-INTERACTING ELECTRON GAS

59

named after the originators of the theory, Bardeen, Cooper, and Schrieffer [7]), basically assumes that the interacting electron gas forming the metal that ultimately becomes a superconductor, exhibits well defined electron-like excitations that can form Cooper-pairs. Theories for superconductivity based on metallic states which do not exhibit such electron-like excitations have been proposed, notably in the context of attempting to explain high-temperature superconductivity in copper oxides. None of them have so far achieved what the Fermiliquid-based BCS theory did in such a brilliant manner–to make predictions for a complicated many-body problem, with right numbers. The Fermi-liquid theory, and the BCS theory, which we will introduce the reader to in this chapter, are certainly two of the most successful theories in condensed matter physics ever.

3.2 The non-interacting electron gas The language we will use to formally describe manybody systems in this book, is second quantization, mainly due to its convenience in the context of manybody systems with non-definite number of particles. This is precisely the situation which is forced upon us for superconductors. The basic building blocks of this formalism, are the annihilation- and creation-operators for electrons with linear † momentum k and spin σ . The operator ck,σ creates a state of an electron in a plane-wave (or Bloch-state) and spin state with quantum numbers (k, σ ), while ck,σ destroys such a state. The fact that electrons are fermions obeying the Pauli principle is is taken into account by postulating anticommutation relations for these operators, namely † † ck ,σ + ck ,σ ck,σ = δk,k δσ,σ ck,σ

(3.3)

where the δ-symbols are Kronecker-deltas, δα,β = 1 if β = α, and δα,β = 0 otherwise. In this language, the operator that counts the number of electrons in a given state defined by the quantum numbers (k, σ ) is given by the operator † nk,σ = ck,σ ck,σ . The Hamiltonian of a non-interacting electron system of states (k, σ ) where the energy of such states is given by εk,σ , is simply the energy per state multiplied by the number operator of such states, and finally summed over all states. Normally, we assume that the energies are independent of σ , i.e. we have εk . Then, the Hamiltonian is given by H =

† εk ck,σ ck,σ

(3.4)

k,σ

The ground state of this system is given by filled states (k, σ ) up to the Fermimomentum kF , where we denote the energy of the uppermost filled state by εF .

60

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

This Fermi-sea is completely inert in the absence of interactions, and we will denote this ground state by |φ0 . It has the important property that nk,σ |φ0 = (εF − εk )

(3.5)

where the Heaviside step function has the property (x) = 1, x > 0, (x) = 0, x < 0. Physically, the above is simply a statement that in the ground state of the non-interacting electron gas, all levels below the Fermi-level are occupied with (maximal) occupation number equal to 1 per spin state in accordance with the Pauli principle, all states above the Fermi-level are unoccupied. An extremely important quantity in a many-particle system is the probability amplitude of finding a particle in a state (k , σ ) at time t , given that it was in state (k, σ ) at time t. This quantity is the so-called single-particle propagator, or Green’s function, of the system. For the non-interacting case we will denote it by G0 (k, k , t − t ) = G0 (k, t − t )δk,k

(3.6)

It plays a central role in describing the electronic structure of any manybody electron system. The right hand side of the relation above follows from the fact that in a non-interacting system, a particle cannot be scattered out of a planewave state defined by a wavenumber k. Note also that G0 only depends on t and t only via the combination t − t when H is time-independent. Mostly, it is convenient to work with the Fourier-transform of the above quantity, namely ∞ dteiωt G0 (k, ω) G0 (k, ω) = −∞

=

1 ω − εk + iδk

(3.7)

where δk = δsign(εk − εF ), and δ is an infinitesimal positive quantity. The pole in the propagator is given by ω = εk − iδk , which defines the spectrum of the single-particle excitations of the system. The imaginary part plays the role of a damping term for the excitations, i.e. an inverse lifetime. In the freeelectron case, this damping term is infinitesimal in the free-electron gas, i.e. the excitations of energy εk are infinitely long lived. The imaginary part of G0 (k, ω) gives the single-particle spectral weight 1 δk 1 A(k, ω) = − [G0 (k, ω)] = = δ(ω − εk ) π π (ω − εk )2 + δk2

(3.8)

which provides direct information on the occupation of a plane-wave state |k of energy ω. Hence, the momentum distribution n(k) of the free electron gas is given by A(k, ω) integrated over all frequencies ω, while the k-space sum of

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

61

A(k, ω) gives the density of states D(ω). At zero temperature n(k) is given by the Fermi-Dirac distribution function n(k) = (εF − εk ) Note that the magnitude of the step-discontinuity in this momentum distribution function is 1 at the Fermi-level. Going back to Eq. 3.7, we see that this value of the discontinuity happens to be the same as the value of the residue at the pole of the free-electron propagator. As we shall see below, this is not a coincidence.

3.3 Interacting electrons, quasiparticles and Fermi-liquids When spin-independent pairwise-interactions between electrons are taken into account (we ignore multibody interactions, as usual), the Hamiltonian includes a two-particle scattering term where two incoming electrons in states k, σ and k , σ are scattered to states k + q, σ and k − q, σ with a matrix element V which in principle depends on the initial scattering states and the momentum transfer q in the process. We assume that the two-particle scattering is elastic. Thus, we may under quite general conditions write the total Hamiltonian as follows † † H = εk ck,σ ck,σ + Vk,k ,q ck+q,σ ck† −q,σ ck,σ ck ,σ (3.9) k,k ,q,σ,σ

k,σ

A typical term in the interaction term of the Hamiltonian is illustrated in Figure 3.1. For such an interacting system, a rather remarkable fact is that we can again write down an exact expression for the single-particle propagator, denoted by G(k, t), i.e. the probability amplitude that if a particle is found in state |k, σ at time 0, it will still be found in this state at time t. This expression is known k + q, s

k′ − q, s′

q

k, s

k′, s ′

Figure 3.1 A typical two-body scattering event contributing to the interaction part of the Hamiltonian, Eq. 3.9. The dashed line connecting the electrons is an illustration of Vk,k ,q denoting some effective interaction, such as Coulomb-interaction, phonon-mediated electronelectron interaction, and soforth.

62

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

as Dysons equation, and is given by, when expressed in terms of the Fouriertransform of G(k, t) G−1 (k, ω) = G−1 0 (k, ω) − (k, ω)

(3.10)

where (k, ω) is the so-called one-particle irreducible self-energy. In general, this is a complex quantity. It has the following physical interpretation: The real part of (k, ω), R = ( (k, ω)), gives a reactive shift of the excitation spectrum of the interacting electrons, such that this spectrum is given by ε˜k = εk + R . The imaginary part, I = ( (k, ω)) essentially gives the inverse lifetime of the interacting electron in the plane-wave state k, σ , i.e. I ∼ τk−1 , where τk−1 is the lifetime of the electron in the state |k, σ . Let us work this out in more detail. Inverting Eq. 3.10, we have G0 (k, ω) 1 − G0 (k, ω) (k, ω) 1 = ω − εk − (k, ω)

G(k, ω) =

(3.11)

where we have ignored δk in the free electron propagator compared to the imaginary part of , which we anticipate to be finite. We now want to bring this onto a form such that it resembles, as much as possible, Eq. 3.4 for the free-electron propagator. We imagine that, in some sense, the interactions are not ‘too strong’, and write the complex self-energy on the form = R + i I , and assume that the imaginary part (the damping-piece) is small compared to the real part (the reactive-shift piece), | I |/| R | 1. The pole in G(k, ω) determines the exact single-particle excitation spectrum of the interacting system. This spectrum is therefore determined from the equation ω − εk − R (k, ω) − i I (k, ω) = 0

(3.12)

To zeroth order, we ignore the imaginary part of . This gives the self-consistency equation for the reactively shifted single-particle spectrum ω = ε˜k = εk + R (k, ε˜k )

(3.13)

Taking into account a small imaginary part of means that the frequency giving the pole in the propagator is shifted, and this in turn implies that we have to Taylor expand the real part of around the frequency ω = ε˜k , as is evident from Eq. 3.13. Thus, we consider the real part of Taylor-expanded to first order around ω = ε˜k , as follows

R (k, ω) = R (k, ε˜k ) + (ω − ε˜k )

∂ R |ω=ε˜k ∂ω

(3.14)

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

63

On the other hand, since we are computing to first order in I , we consider the imaginary part of evaluated at ω = ε˜k . Let us now insert these expressions into Eq. 3.12. We obtain ∂ R |ω=ε˜k − i I (k, ε˜k ) = 0 ω − [εk + R (k, ε˜k )] −(ω − ε˜k ) ∂ω =ε˜k

∂ R (ω − ε˜k ) 1 − |ω=ε˜k − i I (k, ε˜k ) = 0 ∂ω

(3.15)

We now define the lifetime τk of the interacting electrons in state |k, σ , as well as the quantity zk by the following equations

(k, ε˜k ) 1 =− R τk 1 − ∂

∂ω |ω=ε˜k zk =

1 1−

(3.16)

∂ R ∂ω |ω=ε˜k

Inserting all of this in the exact expression for G, we find G(k, ω) =

zk ω − ε˜k +

i τk

(3.17)

If we compare Eq. 3.17 with Eq. 3.7, we see that the main effects of interactions between electrons are to produce a shift of the single-particle spectrum as well as a finite lifetime for the interacting electrons in a given plane-wave state. In addition, the residue of the propagator, the quantity zk , is reduced from the value 1 which it had in the non-interacting case. This is seen directly from Eq. 3.16, as

R on physical grounds is expected to be a decreasing function of frequency: At high energies, the effect of interactions is expected to be smaller than at low energies, because rapidly moving electrons have less time to interact with their surroundings than slow electrons. Hence, ∂ R /∂ω < 0, and thus zk < 1. Roughly speaking, it is as if the electrons in the non-interacting case have been degraded in the interacting case, only a remainder (a residue) less than one remains. What we are particularly interested in, is if this residue is non-zero on the Fermi-surface, i.e. if there is anything left at all of the single-particle excitations we had in the free case. More precisely, are there any remnants at all left of the non-interacting electrons, at low energies close to the Fermisurface, once interactions have been turned on? If there is, i.e. if zkF > 0, then we have some amount of well-defined low-energy single-particle excitations similar to the ones that are exact eigenstates in the non-interacting case. Such free-electron-like excitations are called quasiparticles. An interacting fermionic system with such quasiparticles is called a Fermi-liquid. Such single-particle

64

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS nk

1

zkF

kF

k

Figure 3.2 The zero-temperature momentum distribution nk of an interacting electron system. The magnitude of the discontinuity on the Fermi surface is precisely the quasiparticle residue. The dashed line is the momentum distribution of the non-interacting system, which has a discontinuity of magnitude 1 on the Fermi-surface.

like excitations are no longer exact eigenstates of the system, since interaction terms permit scattering in and out of Bloch-states. However, in a Fermi-liquid the quasiparticles are nevertheless defined well enough at low energies, at least, to enable us to consider them as bona fide electron-like excitations of the system. The momentum distribution which we in principle may obtain from the quasiparticle propagator given in Eq. 3.17 is illustrated in Figure 3.2. The important feature to note is the discontinuity of magnitude zkF on the Fermi-surface, the hallmark of a Fermi-liquid. The concept of quasiparticles in interacting fermion systems was first introduced by Landau in 1950. It has proven to be an enormously successful and important paradigm, basically forming the cornerstone of our understanding of metallic systems. The basic idea which underlies the Landau Fermi-liquid picture is that there is a one-to-one correspondence between the quantum numbers of non-interacting electrons and those of interacting electrons. This means that we may imagine that we start out with some simple Hamiltonian like Eq. 3.4, of which we know the eigenstates and eigenexcitations, and then perturbatively introduce interactions in the problem. When this is done, the resulting quasiparticles of the theory are obtained adiabatically from the excitations of the non-interacting system, and in particular the quantum numbers of the excitations in the interacting and non-interacting case are in one-to-one correspondence with each other. Although this may naively seem like a hopeless approach, it turns out to be a surprisingly robust framework when considering metals. Even in heavy fermion compounds, where interaction effects are so strong that one gets a renormalization of the bare electron mass by factors of order 1000, one still has not obliterated completely the residue of the electrons that exist in the noninteracting case. Examples of systems that do not conform to the Fermi-liquid paradigm exist, however. Notably, quasi-one dimensional organic conductors are not Fermiliquids. This is because interactions in one-dimensional systems constitute a

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

65

singular perturbation to the free-electron case as a consequence of severely restricted Fermi-surface kinematics. As a result, forward scattering, which is innocuous in higher dimensions, is singular in one dimension and all vestiges of free-electron systems are destroyed as soon as interactions are switched on. The long-lived low-energy excitations in this case turn out to be bosonic in character, and are collective excitations in terms of the constituent electrons of the underlying system. Under such circumstances, there can be no one-to-one correspondence between the quantum numbers of the interacting case and of the non-interacting case. How can it be that an approximation that has all the appearances of a nonstarter, works so spectacularly well in most cases? Understanding the microscopics of the Fermi-liquid theory is not the main purpose of this book, so we mention it only briefly. It is however an important problem to understand, and for more details the reader is referred to the vast literature on the subject. What is absolutely crucial when one does any sort of perturbation theory, is to start with the right reference system. Why, then, is the non-interacting electron system a good and sensible starting point to perturb about, when the goal is to describe an interacting electron system? The reason is embedded in the Pauli principle. The number of states that an added particle to the system can scatter into, is severely limited by the Pauli principle, and this effectively suppresses the effect of switching on interactions. As a result, the free case is a good stable system to perturb around. It has the feature of having a finite compressibility in the ground state, and therefore collective modes, such as zero-sound, as well as thermodynamic quantities will change in a smooth manner when interactions are introduced. In contrast, this is not true for a bosonic system. For instance, noninteracting bosons do not support zero-sound, whereas the interacting system does. Hence, quantities do not evolve in a smooth manner as some interaction parameter is varied. Quite the contrary, the limit of zero interactions is a singular limit. So, the non-interacting boson system is not a good starting point to perturb around. The principal reason for why Fermi-liquid theory works is the kinematic restrictions imposed on the interacting system through the Pauli principle. This is all we shall have to say about this, for a more detailed exposition the reader may for instance consult the very nice review article by Varma et al. [37]. It should be emphasized here that in all of the above, we have assumed interactions to mean a repulsive interaction between electrons. This is very natural, in that the dominant interaction between electrons in condensed matter systems is the Coulomb interaction, whose Fourier-transform is given by a matrix element V of the type we considered in connection with Eq. 3.9, namely Vk,k ,q =

1 2π e2 4π ε0 q 2

(3.18)

In this case, V only depends on the momentum transfer q in the scattering process, not on the initial scattering states. However, as we shall see in the

66

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

next section, this is not the only source of interaction between electrons in a solid. For instance, electrons obviously interact with the ions of a solid as they move through it causing scattering of electrons and ions. These scattered ions may in turn interact with other electrons, thus mediating an effective electron–electron interaction. This phonon-mediated interaction turns out to be of a quite different nature than the photon-mediated Coulomb-interaction above. In particular, it has the property that in a thin energy-shell around the Fermi-surface, it is attractive. This feature alone suffices to produce an instability of the Fermiliquid. Attractive electron–electron interactions are singular perturbations to the non-interacting case.

3.4 Instability due to attractive interactions In the previous section, we established that the Fermi-liquid picture of interacting electrons is stable to repulsive interactions. In this section, we will start by investigating what happens to the Fermi liquid when an effective attractive interaction between two electrons is introduced as a perturbation to the noninteracting system. Later, we will show how a weak phonon-mediated interaction between electrons may produce a net attraction, even when the a priori dominant repulsive Coulomb interaction is accounted for.

3.4.1

Two electrons with attractive interaction

In this subsection, we will consider a rather artificial, but nonetheless extremely instructive problem, first considered by Leon Cooper. It exhibits in a lucid manner the dramatic effect an arbitrarily weak attractive interaction between electrons has, in stark contrast to a repulsive interaction. The Cooper problem is defined as follows. Consider the situation where we have an inert Fermi-sea, in which the electrons are treated as non-interacting. To this Fermi-sea we add two electrons above the Fermi-surface (by necessity). These two extra electrons do not interact with the inert Fermi-sea. They do however interact with each other, but in a very peculiar manner. The interaction is such that the two electrons attract if they both are within a small energy ω0 from the Fermi-surface, and on opposite sides of the Fermi-surface, otherwise they do not interact at all. In the absence of interactions, one electron occupies a plane-wave state |k, the other occupies the plane-wave state |−k. Let us denote the two-particle state of the two extra electrons in the absence of such a peculiar interaction by |k, −k, and in the presence of the interaction by |1, 2. Denoting the Hamiltonian of the system by H = H0 + Veff

(3.19)

H0 |k, −k = 2εk |k, −k

(3.20)

then we have

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

67

where εk is the single-particle excitation energy of the non-interacting fermion system (see Eq. 3.4). Note that due to the Pauli principle, we must have 2εk > 2εF in the presence of the inert Fermi-sea. This sea plays the role of providing blocking-factors for added states. Adding interactions, the exact Schr¨odinger equation for the (admittedly peculiar) two-particle problem defined above is given by H |1, 2 = E|1, 2

(3.21)

where E is the exact two-particle energy of the two electrons above the Fermisurface, in the presence of an attractive interaction. We assume that the states |k, −k form a complete set such that the exact two-particle eigenstate can be expanded in this basis, thus |1, 2 =

ak |k, −k

(3.22)

k

Our task is to obtain the expansion coefficients ak and finding the value of E. This will solve the Schr¨odinger-equation for the problem. Let us insert Eq. 3.22 into Eq. 3.21, obtaining (H0 + Veff )

ak |k, −k = E

k

ak |k, −k

(3.23)

k

We next project the resulting equation down on the adjoint states < k , −k |, where we have k , −k |k, −k = δk,k , in order to obtain a Schr¨odinger equation for the coefficients ak . Using the above orthogonality relation, we thus find ak [2εk − E] = −

ak k , −k |Veff |k, −k

(3.24)

k

The quantity k , −k |Veff |k, −k is basically a two-particle scattering matrix element for particles on opposite sides of the Fermi surface, from a two-particle state |k, −k to a two-particle state |k , −k . This scattering process is illustrated in Figure 3.3. So far, this is quite general, and we now specialize to the case where this scattering matrix element is of the somewhat peculiar nature described above, namely attractive in a thin shell around the Fermi-surface, and zero elsewhere. That is, we have k , −k |Veff |k, −k = −V ; |εk − εF | < ω0 = 0; otherwise

(3.25)

68

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

k

k′

−k′

−k

Figure 3.3 Scattering event of two particles maintained on opposite sides of the Fermisurface, scattered by the matrix element k , −k |Veff |k, −k which is operative in the thin shell around the Fermi-surface indicated by the dashed circles.

Then Eq. 3.24 takes the form ak [2εk − E] = V

ak (εk − εF )(ω0 − |εk − εF |)

(3.26)

k

The first -function ensures that the single-particle energies ε are above the Fermi-surface, the second one ensures that the effective attraction only is operative in a thin shell around the Fermi-surface. At this stage it is more convenient to go over to energy integrals instead of k-space integrals, by introducing the density of states D(ε), and viewing the expansion coefficients as functions of energy ε. Introducing the density of states D(ε) (the k-space sum of the spectral weight A(k, ε) obtained from G0 (k, ε) (see Eq. 3.8), as follows 1 δk 1 [G0 (k, ε)] = π π (ε − εk )2 + δk2 k k = δ(ε − εk )

D(ε) = −

(3.27)

k

where δ(ε − εk ) is a Dirac delta function, and we have used that limη→0 η/(x 2 + η2 ) = π δ(x). Noting that ak only depends on k via εk , we may write Eq. 3.26 as follows ∞ dε a(ε)δ(ε − εk )(ε − εF )(ω0 − |ε − εF |) a(εk )[2εk − E] = V =V

−∞ ∞ −∞

k

dεD(ε)(ε − εF )(ω0 − |ε − εF |)

(3.28)

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

69

We then obtain, upon renaming variables

εF +ω0

a(ε)[2ε − E] = V

dε D(ε )a(ε )

(3.29)

εF

The right hand side of Eq. 3.29 is seen to be independent of ε, and hence we immediately conclude that a(ε) must have the form a(ε) =

C 2ε − E

(3.30)

where C is some normalization constant. Its precise value will not be important, and we do not specify it further. Inserting the Ansatz Eq. 3.30 for a(ε) into Eq. 3.29, we find the self-consistent equation for the eigenvalue E 1=V

εF +ω0

εF

D(ε )dε 2ε − E

(3.31)

Utilizing the fact that we are considering a thin shell around the Fermi-surface, and assuming that the density of state D(ε) varies slowly, we may simply replace it by its value on the Fermi surface, D(εF ). Introducing the dimensionless coupling constant λ ≡ V D(εF ), we obtain 1=λ

εF +ω0

εF

dε 2ε − E

2(εF + ω0 ) − E = λ ln 2εF − E

(3.32)

We then introduce the energy difference between the states of two non-interacting particles on the Fermi-surface, and the exact energy eigenvalue E, i.e. = 2εF − E. In terms of this variable, Eq. 3.32 may be written 1 2ω0 = ln 1 + (3.33) λ Note that the way V is defined in Eq. 3.25, it is a positive quantity, hence λ is a positive quantity. Thus we see that in order for Eq. 3.33 to have a solution, > 0 is required. This means that E < 2εF ! This is a a quite dramatic result, since the basic starting supposition was that the inert Fermi-sea was completely filled up to the Fermi-level, and the two extra electrons lived above the Fermi-surface. Now, we have just reached the rather startling conclusion that an arbitrary weak attractive interaction leads to an exact two-particle state with a total energy lower than twice the Fermi-energy. What this indicates, is that the inert Fermi-sea is suffering some sort of collapse such that energy

70

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

states below the top of the Fermi-sea become accessible. At this stage, such an interpretation of the above result is merely a plausible conjecture. Confirmation of its physical soundness will have to await the analysis in the next chapter, where the full self-consistent treatment of all electrons in a thin shell around the Fermi-surface will be completed. Let us solve Eq. 3.33 for . We find =

2ω0 ≈ 2ω0 e−1/λ e1/λ − 1

(3.34)

where the last approximation follows if λ 1, i.e. if the effective electron– electron attraction is in some sense weak. Several remarks are now in order. First, we see that has an essential singularity as λ → 0. This means that the above result for could never have been obtained to any finite order in perturbation theory in λ. Hence, an arbitrarily weak attraction is a singular perturbation to a free electron gas. It destabilizes a Fermi-liquid. Secondly, we see that λ > 0 only if D(εF ) > √ 0. For a parabolic 2 2 band εk = k /2m in three dimensions, we have D(ε) ∼ ε. Hence, if the Fermi sea vanishes by draining electrons out of the system, λ → 0 and → 0. In other words, the tendency to pairing of electrons that we see above vanishes when the Fermi-sea vanishes. We should not expect a two-electron bound state for arbitrarily weak attraction in vacuum. Thirdly, if we were to reinstate in the problem, we would find = 2ω0 e−1/λ

(3.35)

This shows that the pairing is also a quantum effect, since the bound state energy gap vanishes when → 0, i.e. it vanishes in the classical limit. Last, but by no means least, we note that to the extent we choose to take the above results seriously (and we should), the fact that the two-electron bound state resides at an energy which apparently is prohibited by the Pauli principle, in a vague way hints at the fact that perhaps bound pairs of electrons are not as much slaves to the Pauli principle as are individual electrons. In fact, this is precisely true, as we will come back to in Chapter 4. By forming Cooperpairs, electrons can shed their fermion statistics. The resulting quantum fluid of Cooper-pairs is not as protected from interactions as are the Pauli principle loyal fermionic fluids. This is basically the root cause of why attractive interactions are able to destabilize the Fermi-liquid while repulsive interactions are virtually incapable of doing so in metallic states. Recall that when we briefly analyzed the microscopic foundations of Landau Fermi-liquid theory, we stated that the Pauli principle severely suppressed the effects of (repulsive) interactions, thus saving the electron-like quasi-particles from obliteration. For attractive interactions, the Pauli principle is essentially sidelined and no longer acts as a suppressor of interaction effects. This opens up the possibility of ground states qualitatively different from the free electron gas.

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

71

The resulting electron pair that we have described the genesis of in the above, is referred to as a Cooper-pair, named after Leon Cooper who had the audacity to consider the then outrageous problem of two electrons interacting attractively in the peculiar manner described above. Cooper’s calculation is truly remarkable in that when he performed it, there was no known mechanism by which electrons could interact attractively in solid states physics. As it turns out, the phenomenon of Cooper-pairing of electrons is at the heart of the phenomenon of superconductivity.

3.4.2

Phonon-mediated attractive interactions

In this section we will start with the Hamiltonian for electrons interacting with each other through the Coulomb interaction and add the coupling of electrons to phonons. A canonical transformation reduces this to an effective Hamiltonian with a modified electron-electron interaction that under certain circumstances could be attractive, despite the apparent complete dominance of the Coulomb-interaction compared to the weak electron–phonon couling. It is very much like David’s triumph over Goliath–intelligence and a sit of luck wins over brute force. Let us, before we start with formalities, give an intuitive picture of what is going on. The crucial point which facilitates the above rather remarkable result, is that heavy lattice ions are slow movers around their equilibrium positions compared to fast and light electrons. Hence, dynamic local lattice distortions arising from electron-ion collisions, remain long after the electron that caused them have passed. This phenomenon will be called retardation. A local lattice distortion gives rise to a small dipole moment that can interact with electrons. As a result, another electron in the vicinity of the local lattice distortion can be drawn towards it long after the initial electron has left the scene. As the electrons are far removed from each other, the repulsive Coulomb interaction is reduced. It is this ‘wait a little and see’ tactics that allows the electron–phonon coupling to circumvent the apparent insurmountable obstacles of the Coulombrepulsion. On the other hand, the second electron is not allowed to wait for a too long time before taking advantage of the local lattice distortion, since the latter eventually will decay as the ion settles around its equilibrium again. Hence the second electron has a limited amount of time at its disposal before moving in on the lattice distortion caused by the first electron. It therefore stands to reason that in order to reduce as much as possible the (for pairing purposes) adverse effects of the Coulomb-repulsion, the two electrons should put as much distance as possible between themselves per unit time. The best two-particle state for such purposes is a state where the two electrons occupy plane-wave states of opposite wavenumbers, i.e. they move in opposite directions. (Anybody who has ever been on an airliner between two major central European cities has experienced this by looking out the window of the aircraft and seeing another

72

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

airliner whizzing past in the opposite direction. They are out of sight in seconds, in contrast to those that fly in more or less the same direction, which can be followed for minutes.) This crude real-space picture already gives us a hint that Cooper’s calculation discussed in the previous subsection, while appearing quite artificial, in fact is precisely the right problem to consider. We now proceed to derive an effective electron–electron interaction, mediated by photons and phonons, which gives rise to the physics discussed above. The starting point is the second-quantized version of the interacting electron gas coupled to quantized lattice vibrations, or phonons. It is given by H=

† εk ck,σ ck,σ +

k,σ

Ve−ph =

k,k ,q,σ,σ

1 2π e2 † ck+q,σ ck† −q,σ ck,σ ck ,σ + Ve−ph 2 4π ε0 q

† † Mq (a−q + aq )ck+q ck

(3.36)

k,q,σ

where Mq is the matrix element for electron–phonon coupling. The operators (aq† , aq ) are creation and destruction operator for phonons, and satisfy the following commutation relations reflecting that phonons are bosons aq† aq − aq aq† = δq,q

(3.37)

Phonons are not material particles, and their number is not conserved in a solid. A typical electron-phonon scattering event is shown in Figure 3.4. In Eq. 3.36, we have assumed that one particular phonon-mode dominates the coupling to the electrons. Had we had several phonon-modes of equal coupling strength, we would have had to include a sum over phonon modes λ as well, in Ve−ph . The matrix element Mq may be expressed in terms of the eigenfrequencies ωq,λ of harmonic lattice vibrations and the Fourier-transform V˜e−ion (q) of k + q, s

q

k − q, s

Mq

M−q

k, σ

q

k, σ

Figure 3.4 Scattering events between electrons and phonons. In the left process, a phonon is absorbed by an electron causing recoil. In the right process, an electron emits a phonon causing recoil. In the latter case, the electron sets up a local dynamic lattice distortion. The vertex is denoted by a black dot and its strength is given by Mq .

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

73

the electrostatic electron-ion interaction as follows (when also a phonon-mode index λ is included) Mq,λ = i(q · ξ λ ) (3.38) V˜e−ion (q) 2Mion ωq,λ where Mion is the ion-mass and ξ λ is a unit vector giving the direction of the lattice-vibration mode λ. It is difficult to compute Mq,λ with any precision from first principles, and we will simply take this matrix element as some parameter. This coupling is much weaker than electron–photon coupling. Note also that limq→0 Mq,λ = 0. The fact that Mq,λ ∼ q reflects the fact that the electron-phonon coupling is a coupling between a point charge and a dipole moment. Let us see how we can transform the electron-phonon coupling into an effective electron-electron interaction in a fairly simple manner. Note that the interaction in Figure 3.1, when viewed as a Coulomb-interaction, may be considered as obtained from two scattering events as those depicted in Figure 3.4, but where the dashed lines are photons and not phonons, and where the scattering vertex has strength e, the electron charge, and not strength Mq . In Figure 3.1, we then interpret the dashed line between the electrons as a free-photon propagator. Since electrons are virtually at a standstill compared to photons, this interaction is non-retarded and we may ignore the frequency dependence of the photon-propagator. Under such circumstances, the photon propagator is nothing but the static Coulomb-interaction. We may proceed precisely along the same lines when phonons are involved. We obtain an effective electron–electron interaction by taking the two scattering events in Figure 3.4 and forming a two-particle scattering term as in Figure 3.1. We then interpret the dashed line connecting the electrons as a free phononpropagator. Free phonons have the Hamiltonian H = ωq aq† aq (3.39) q

where ωq is the eigenvalue of a phonon in a plane-wave state |q. The explicit expression for the free phonon-propagator D0 (q, ω), which has the same interpretation as the propagator for electrons, is given by D0 (q, ω) =

ω2

2ωq − ωq2 + iη

(3.40)

where η is a positive infinitesimal quantity. Using this, we obtain the phononmediated part of the electron–electron interaction Veff (q, ω) =

2|Mq |2 ωq ω2 − ωq2

(3.41)

74

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

In the above, q is the momentum transfer in the electron-electron scattering process, while ω is the energy transfer. Electrons are by no means at a standstill in solids compared to the velocity of sound waves. Thus, we cannot ignore the frequency dependence of this part of the electron–electron interaction. The result of all of the above is that Eq. 3.36 may be written on the form of a purely electronic system where the trace of the phonons is manifest in the additive contribution they give rise to in the electron-electron interaction, as follows H=

k,σ

V˜eff (q, ω) =

† εk ck,σ ck,σ +

k,k ,q,σ,σ

2|Mq |2 ωq 1 2π e2 + 4π ε0 q 2 ω2 − ωq2

† ck† −q,σ ck,σ ck ,σ V˜eff (q, ω)ck+q,σ

(3.42)

Note that when ω2 < ωq2 , the phonon-mediated piece of the electron–electron interaction is negative, i.e. it is attractive. This in itself does not mean all that much, the issue is if this attractive piece can overcome the manifestly repulsive piece originating in the Coulomb-interaction. In fact, it is easy to see that it can, at least for some momentum transfer and energy transfer. We note that as ω2 approaches ωq2 from below, the phonon-mediated piece of the interaction formally diverges! Hence, it does not matter how small |Mq |2 is, the phononpiece will always be able to overcome the Coulomb-piece. The physics of this is precisely what was alluded to in the introduction to the section. Namely, by waiting for a time which is of order the time-scale of the lattice vibrations, an electron may come in and be dragged towards a local lattice distortion caused by an electron passing the site at some earlier time. This minimum waiting time corresponds to the upper frequency cutoff. In Figure 3.5, a sketch of V˜eff (q, ω) is given as a function of frequency ω at fixed finite momentum q, the figure on the left. Note that when ω is close enough to typical phonon-frequencies ωq the total effective interaction is positive. For all ω2 > ωq2 it is repulsive, and this is also the case for too small ω2 . This latter fact is what we alluded to in the introduction to this subsection, namely that the electron can not wait for too long a time before taking advantage of the local lattice distortion. Thus, the effective attraction we see for not too small and not too large frequencies, is basically the Fourier-spacetime version of the “wait and see” tactics described at the start of the section. The figure on the right in Figure 3.5 is an idealized and simplified version of V˜eff (q, ω). We ignore entirely the repulsive part of the interaction, since we expect the effect of repulsive terms to be suppressed by the Pauli principle as discussed in the previous section. The attractive part is extended to all frequencies ω2 < ωq2 , and is moreover taken to be a constant independent of ω in this range. This simplification is the one that was originally considered by Bardeen,

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS Veff

Veff

w

−wq

75

wq

w

−wq

wq

Figure 3.5 The left figure shows V˜eff (q, ω) at fixed q as a function of ω. The right figure shows a much simplified version of it.

Cooper, and Schrieffer in their seminal 1957 work on phonon-mediated superconductivity [7]. It is an extreme simplification, but nonetheless yields results that are in spectacular agreement with experiments. While the agreement with experiments (to within a few percent for studiously chosen quantities) may have been a source of some surprise at the time, given the crudeness of the approximation of V˜eff (q, ω), we now understand why this is so. The point is that the simplified interaction contains the essential feature of the more realistic V˜eff (q, ω), namely attraction in a certain frequency range close to typical phonon-frequencies. What other details are left out are not all that important, the validity of the results obtained is virtually guaranteed by the principle of universality: Certain physical properties do not depend on tiny details of the microscopic Hamiltonian. All we need to do is to derive some effective description and compute properties from this, and we get the right results (if we focus on the right properties!). In the next chapter, we shall compute some results that come out right due to universality, and we shall also compute one notable quantity which definitely does not.

3.4.3

Reduction of the effective Hamiltonian

Let us next proceed to further simplifying the Hamiltonian Eq. 3.42. The simplifications we will make are expected to be sensible provided that the frequency range where V˜eff (q, ω) is attractive in a tiny energy range compared to the Fermi-energy, i.e. the shell around the Fermi-surface in Figure 3.3 is exceedingly thin compared to the radius of the Fermi-sphere. The implication of this is that when the frequency range of attraction is narrow, the phase-space for scattering such that the attractive interaction is felt, is maximized by having both the initial and final two-particle states within the thin shell. The energy transfer in the scattering process caused by V˜eff (q, ω) is ω = εk − εk+q = εk − εk −q . All energies (εk , εk , εk+q , εk −q ) must lie within a thin energy shell around the Fermi-surface if the initial and final two-particle states are to contain electrons that attract each other. What values of (k, k , q) in Eq. 3.42 will ensure

76

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

q

q k1 k2

k1 −q

k2

−q

Figure 3.6 Phase-space of two-particle scattering within a thin shell of the Fermi-surface. There is only one situation where both the initial and scattered states are within the thin shell, provided one of the initial and one of the scattered states are, and that is if the initial momenta are on opposite sides of the Fermi-surface.

this? The interaction term describes scattering of initial state |k, σ to state |k + q, σ > and scattering of the state |k , σ to state |k − q, σ . What relation between (k, k ) ensures that if |k + q, σ is a state within the energy shell, then so is |k − q, σ for all q? The answer is that this occurs if k = −k (see Figure 3.3), and this maximizes the phase-space for scattering of attractively interacting states. Hence, we will keep only such terms in Eq 3.42. The situation is also illustrated in Figure 3.6. Consider two electrons in momentum states k1 and k2 , both within a thin energy shell around the Fermisurface. Suppose one electron is scattered into momentum state k1 + q and the other into k2 − q. If the total momentum of the initial and scattered states is k1 + k2 = Q, then we see from the left figure that in general, one of the scattered states will not be within the thin shell even if the other is. There is only one situation that guarantees that both the scattered states are within the thin shell if one of them are, and that is if k1 + k2 = 0. This situation will tend to dominate the contribution to the scattering phase space, given that the twoparticle scattering matrix element is operative only if both of the initial and final states are within this thin shell. This domination becomes progressively more pronounced the thinner the shell is. If we dispensed with retardation altogether, and considered the scattering matrix element to be operative over the whole electronic band, then the above reduction into opposite momentum states is more questionable. Nonetheless, with the recent renaissance of purely electronic pairing mechanisms invoked in attempts of explaining such phenomena as superconductivity in high-Tc cuprates, the reduction is often used. Mostly out of old habit and with little or no justification. In the case of phonon-mediated attraction, the approximation is however on quite firm ground. Moreover, we expect the attractive interaction mediated by phonons to be of short range. Thus, electrons should be allowed to approach each other closely in space (although they avoid each other in time). Due to the Pauli principle, it is therefore plausible to suggest that the electrons that can approach each other in space most easily are such electrons that are in opposite spin states. Therefore, we also set σ = −σ . Setting k = −k, σ = −σ , and redefining k + q → k, k → k in the interaction term of the effective Hamiltonian, Eq. 3.42 may be

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

written on the form † † † H = εk ck,σ ck,σ + Vk,k ck,σ c−k,−σ c−k ,−σ ck ,σ k,σ

77

(3.43)

k,k ,σ

where Vk,k is an attractive two-particle scattering matrix element which is operative if both k and k are within a thin shell around the Fermi-surface. Eq. 3.43 is the celebrated BCS-reduced Hamiltonian forming the starting point for discussing phonon-mediated superconductivity. In Figure 3.7, we also provide a real-space illustration of a Cooper-pair of two electrons moving in a lattice, where we have in mind a phonon-assisted pairing mechanism (the only really known pairing mechanism to date). The electrons move approximately linearly in opposite directions and in opposite spin-states. Each electron leaves behind a trail of lattice distortions as it moves through the lattice, which the other electron can feel and be attracted towards via the matrix element Eq. 3.38. In order to maximize the attraction, it is advantageous for the electrons to move co-linearly, since this maximizes the time the electrons spend close to lattice distortions while at the same time being mobile. Moreover, moving in precisely opposite directions puts maximum distance between the two electrons per unit time, thus minimizing the adverse effects, for pairing-purposes, of the repulsive Coulomb-interaction. The above is a rough real-space version of the k-space arguments given in the previous paragraph. It clearly illustrates that Cooper-pairing is a k-space phenomenon, not a pairing phenomenon in real-space.

Electrons

Figure 3.7 Real-space representation of a Cooper-pair with phonon-mediated superconductivity. The black dots are lattice ions unperturbed by the motion of the electron through the lattice. The hatched dots are lattice ions that have been displaced slightly by the electrons passing close by. Since the ions are heavy and slow, the local lattice distortions remain long after the electrons have passed. An electron moving in precisely the opposite direction can now take full advantage of the extended line of distortions, more so than an electron crossing this line. Thus, phonon-mediated electron–electron attraction is maximized for electrons in opposite linear momentum states. Moreover, such states also minimize the adverse effects of Coulomb-repulsion, since the two electrons then put a maximum amount of distance between themselves in a minimum amount of time.

78

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

In metals, electrical resistivity has many sources, among them electron–phonon coupling, but also scattering of electrons off impurities. In very clean metals with low density of lattice defects or other sources of point-like or extended impurities, one might expect the electron–phonon coupling to dominate the contribution to the scattering. Provided the pairing mechanism we have described in previous sections is the source of superconductivity, the source of resistivity and superconductivity is basically one and the same scattering mechanism. This immediately gives some insight into a fact which seems to be borne out in most cases, namely that good metals become superconductors only at low temperatures. While mercury has a room temperature resistivity of 98 × 10−8 m and critical temperature of about 4.2 K, copper, the archetypical good metal, has a room temperature resistivity of 1.7 × 10−8 m and critical temperature which is in the millikelvin range. There really is no theory available to us that allows us to compute Tc from known experimentally accessible normal state properties with any great precisions. What we have, as we shall see in the next chapter, are rough estimates in terms of an electron–phonon coupling constant for which one has some crude estimate. It will turn out, however, that the critical temperature is exponentially sensitive to this couling constant, and hence great variation in Tc are expected. Paradoxically, therefore, we would expect the largest superconducting critical temperature in a poor metal! This goes to show that superconductivity is much more than just perfect conductivity. We already know this, of course, because the Meissner effect is a defining property of a superconductor which obviously has no counterpart in a perfect free electron gas with zero resistivity. The physical consequences of the Meissner effect have been mentioned, and will be elaborated on in much more detail in the chapters to follow.

5:48 pm, 6/26/05

4 The Superconducting State – an Electronic Condensate 4.1 BCS theory: a magnetic analogue We have seen in Chapter 3 that the effective Hamiltonian for electrons interacting attractively (by some mechanism) when two electrons are in opposite spin-states and states of opposite linear momentum, is given by the BCS reduced Hamiltonian † † † H = εk ck,σ ck,σ + Vk,k ck,σ c−k,−σ c−k ,−σ ck ,σ (4.1) k,σ

k,k ,σ

It is possible to recast the effective BCS Hamiltonian into a language reminiscent of what we are acquainted with for the Heisenberg model for magnetic insulators, using the so-called Anderson pseudospin formalism. Such pseudospin formalisms have subsequently been used extensively in the context of a number of physical phenomena, such as the bi-layer quantum Hall effect, to mention one example. We have seen in the previous chapter, that the effective Hamiltonian capturing the essentials of conventional phonon-assisted low-Tc superconductivity, is given by H =

k,σ

† εk ck,σ ck,σ +

k,k

† † Vk,k ck,↑ c−k,↓ c−k ,↓ ck ,↑

(4.2)

where the interaction term represents scattering of two-particle spin-singlet states on opposite sides of the Fermi-surface. We now recast this into the form of a (pseudo)spin-Hamiltonian, where it will become evident that superconducting off-diagonal long-range order is equivalent to pseudo-magnetic ordering, which is more familiar to us in that it at least has a classical counterpart. (Throughout Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

80

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

this chapter, we work with units such that = 1). We introduce the standard Pauli matrices τ1 , τ2 , τ3 , as well as the spin-lowering and raising operators τ ± = τ1 ± iτ2 . Next, we introduce the operators τk1 , τk2 , τk3 , as follows † † τk3 = ck,↑ ck,↑ − c−k,↓ c−k,↓ † † τk+ = 2ck,↑ c−k,↓

(4.3)

Inserting this into the effective Hamiltonian (Eq. 4.2), we obtain H =

k

εk (τk3 + 1) +

1 Vk,k (τk1 τk1 + τk2 τk2 ) 4

(4.4)

k,k

Note that this has the form of an XY-Heisenberg Hamiltonian of spins in an external magnetic field in the z-direction. However, it should be noted that the usual labels for spin-sites on a real-space lattice is replaced by indices in Fourier-space. This just underscores that point that Cooper-pairing is a k-space phenomenon. The point that enormously simplifies the treatment of the above pseudo-spin Hamiltonian is that the original effective interaction matrix element Vk,k is essentially a contact interaction in real-space, and hence a long-range potential in k-space. Thus, van der Waals type mean-field arguments can be brought to bear on the problem, and we expect that a mean-field decomposition of the pseudo-spin Hamiltonian will yield excellent results. With longer range interaction in real-space, and hence shorter range interactions in k-space, fluctuation effects are expected to become more prominent. Moreover, we have tacitly assumed that the majority of the two-particle scattering events take place between electron pairs of zero total linear momentum, an approximation that is expected to be excellent as long as the phase-space for attraction is limited to a thin shell around the Fermi-surface. Hence, Eq. 4.4 is expected to be an effective Hamiltonian which is reasonable for the case where the interaction responsible for Cooper-pairing is retarded. Spontaneous symmetry breaking in this pseudomagnet occurs for the case where the pseudomagnetic field vanishes, i.e. for the case where we ignore the kinetic energy term. This magnetic analog leads us to choose the magnetization to be oriented in the 1–2-plane, and thus define an order parameter as follows † † τk1 = ck,↑ c−k,↓ + c−k,↓ ck,↑

(4.5)

The task now will be to derive a self-consistent mean-field equation for this pseudomagnetic order parameter. Before doing this, let us make a few general remarks. Note that if the order parameter exists, it implies that the particle number is not conserved in the ground state of the system. Global conservation of particle number is reflected

DERIVATION OF THE BCS GAP EQUATION

81

by a global U (1)-symmetry of the original effective Hamiltonian. Thus, we see that superconductivity really amounts to breaking a global U (1)-symmetry in the ground state of the interacting electron gas. In physical terms, this means that the superconducting ground state is a coherent superposition of states with different number of particles, however with a majority of the states containing a number of particles which is close to the number of particles one would have in the U (1)-symmetric normal metallic state. Going back to the magnetic analogue, we see that superconductivity is equivalent to obtaining spontaneous pseudomagnetization in the 1–2-plane. It is as if an XY-magnet has ordered. For this reason, and since the symmetry group U (1) essentially is isomorphic to the symmetry group O(2), it is often said that the normal metal-superconductor transition is in the universality class of the XY-model. As we shall see later, while this statement is correct for the superfluid to normal fluid transition in H e4 , it is strictly speaking not correct in the case of a superconductor, which has a charged condensate. If the condensate has a charge, it means that it couples to an electromagnetic vector potential, a gauge-field. This elevates the symmetry of the system to a local U (1) symmetry, as opposed to the global U (1) symmetry of the XY model describing a superfluid. The presence of a gaugefield in the problem in principle alters the interactions, and hence also some critical properties. In many cases, the differences are, however, unobservably small. Not only is the normal metal–superconductor transition strictly speaking not in the XY-universality class, but depending on the value of the Ginzurg–Landau order parameter, the transition may not even be a critical phenomenon, but a first order phase transition! What will transpire is that the demarcation between first order phase transition and second order phase transition√is given by the tricritical value of the Ginzburg–Landau parameter κtri = 0.79/ 2. It also turns out that this value is the fluctuation-corrected demarcation between type-I and type-II superconductivity!

4.2 Derivation of the BCS gap equation In this section, we compute the free energy of the superconductor in the mean-field approximation. The superconducting gap is found by minimizing the expression for the free energy as a function of the gap-parameter. We first proceed by reducing the effective Hamiltonian to a self-consistent one-body problem by first introducing expectation values of the creation- and annihilation operators for Cooper-pairs. We have justified this mean-field procedure above, in the context of the pseudo-spin formalism. We first define the c-numbers bk = c−k,↓ ck,↑ † † c−k,↓ bk† = ck,↑

(4.6)

82

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

such that we have c−k,↓ ck,↑ = bk + c−k,↓ ck,↑ − bk .

(4.7)

δbk

We next insert this into the effective Hamiltonian and retain terms up to linear in δbk , ignoring terms of order O(δbk2 ). This gives † † † H = εk ck,σ ck,σ + Vk,k [bk† c−k ,↓ ck ,↑ + bk ck,↑ c−k,↓ − bk† bk ] (4.8) k,k

k,σ

This Hamiltonian is immediately simplified by introducing the superconducting gap-parameter, defined as follows Vk,k bk† †k ≡ − k

k ≡ −

Vk,k bk .

(4.9)

k

We the obtain an effective one-body Hamiltonian on the following form † † † † H = εk ck,σ ck,σ − [k c−k,↓ ck,↑ + k ck,↑ c−k,↓ − bk† k ] (4.10) k,σ

k

Note that because of presence of pair-production and pair-annihilation terms, Eq. 4.10 is not yet on the standard form of an effective non-interacting electron gas, and hence we cannot at this stage read off what the quasiparticle spectrum of Eq. 4.10 is. In order to achieve this, we perform a rotation of the basis to a set of new fermion operators that diagonalize this Hamiltonian, as follows. We introduce two new species of fermion annihilation operators (ηk , γk ) along with their corresponding creation operators, which are related to the original electron operators via the unitary transformation ck,↑ = cos(θ )ηk − sin(θ )γk † c−k,↓ = sin(θ )ηk + cos(θ )γk

(4.11)

and their corresponding adjoint operators. Inserting this into the Hamiltonian we obtain [εk + k bk† ] H= k,σ

+

[εk cos(2θ ) − sin(θ ) cos(θ )(k + †k )]ηk† ηk

k

−

k

[εk cos(2θ ) − sin(θ ) cos(θ )(k + †k )]γk† γk

DERIVATION OF THE BCS GAP EQUATION

−

83

[k cos2 (θ ) − †k sin2 (θ ) − 2εk sin(θ ) cos(θ )]ηk† γk k

† − [k cos2 (θ ) − k sin2 (θ ) − 2εk sin(θ ) cos(θ )]γk† ηk

(4.12)

k

We next proceed by choosing the value θ in such a way as to precisely diagonalize the Hamiltonian, i.e. such that only terms like ηk† ηk and γk† γk appear. This is achieved by choosing the following value of θ , upon ignoring phase-fluctuations in the complex order parameter entirely and setting k = †k tan(2θ ) = −

k εk

(4.13)

For such values of θ , we have 1 1− 2 1 cos2 (θ ) ≡ u2k = 1+ 2 sin2 (θ ) ≡ vk2 =

where Ek ≡

εk2 + |k |2

εk Ek εk Ek

(4.14)

(4.15)

Before we go further, it is appropriate to mention the factors vk2 and u2k which were introduced in Eq. 4.14. These are normally referred to as coherence factors. They play an extremely important role in the following sections where we will study ultrasound attenuation and nuclear magnetic resonance (NMR). Their existence was a prediction that came out of the BCS theory. It turns out that observed results for NMR and ultrasound attenuation in superconductors depend sensitively on these coherence factors, since in these two cases they conspire subtly and in entirely different ways. An even more subtle point is that, as we shall see, they conspire in different ways in transverse and longitudinal ultrasound attenuation! Bardeen, Cooper and Schrieffer [7] came up with predictions with correct numbers for these effects in a complicated manybody problem. This is undoubtedly one of the major triumphs of condensed matter physics of the 20th century. Using Eqs 4.14 in 4.12, we finally obtain the simple fermionic Hamiltonian which formally has the form of a free fermion quasiparticle gas H = [εk + k bk† ] + Ek [ηk† ηk − γk† γk ] (4.16) k,σ

k

The above Hamiltonian now has the form of a constant (mean-field) term H0 ≡ † k [εk + k bk ] plus the Hamiltonian for a spinless fermion system with two species of fermions, described by the operators (ηk† , ηk ) and (γk† , γk ), where

84

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

we can identify the quasiparticle excitation energies as (Ek , −Ek ) for the two species of fermions. Note that the two species of quasiparticle fermions are spinless since they are linear combinations of electrons and holes with opposite spins. Rather than having ↑-spin electrons and ↓-spin electrons as our degrees of freedom as in the metallic phase, we have two distinct linear combinations of particle-hole spin-singlets as our relevant degrees of freedom. Thus, the total number of degrees of freedom is conserved. The expression in Eq. 4.15 immediately provides a physical interpretation of k defined in Eq. 4.9. It appears as a gap in the quasiparticle spectrum on the Fermi-surface (where εk = 0), a gap which is present because the expectation value < c−k,↓ ck,↑ > is non-zero. This expectation value is essentially the order parameter of the superconducting state, as was made clear from the pseudo-magnet analog above, and hence we will refer to the gap k as the superconducting gap. Note that the gap strictly speaking is not precisely the same as the superconducting order parameter, by the definition (Eq. 4.9)! For one thing, the k-space structure of the two objects are different. However, they are both non-zero or zero simultaneously, and for this reason the gap in the quasiparticle spectrum may effectively serve as a bona fide order parameter, and in most cases this is in fact what is done. Since this now has the form of a free fermion gas, plus a constant term which does not contain fermionic degrees of freedom (the first term), it is elementary to write down the grand canonical partition function for the problem, which is given by

Zg = e−βH0 (1 + e−βEk )(1 + eβEk ) = e−βF k

H0 ≡ [εk + k bk† ].

(4.17)

k

This implies that the free energy F of the system is given by 1 F = H0 − [ln(1 + e−βEk ) + ln(1 + eβEk )] β

(4.18)

k

which has the form of a pure mean-field term plus the contribution to the free energy from a two-component effective non-interacting fermion gas. At zero temperature (β → ∞), the entropic contribution to the free energy vanishes, and Eq. 4.18 takes the form [Ek (−Ek ) + Ek (Ek )] F = H0 + k

= H0 +

[Ek (1 − (Ek )) − Ek (Ek )]

k

[εk + k bk† − Ek ] = k

(4.19)

DERIVATION OF THE BCS GAP EQUATION

85

where we have used the Heaviside step-function (x) = 1 − (−x), (x) = 0, x < 0, (x) = 1, x > 0. The gap k , which at this stage has the status of a variational parameter, is self-consistently determined by minimizing the free energy with respect to variations in k . We therefore demand that the following (equivalent) sets of equations be satisfied for the superconducting gap ∂F =0 ∂k ∂F =0 ∂†k

(4.20)

This mean-field requirement on the gap applies regardless of what the details of the k-space structure of the attractive interaction Vk,k is. One must remember that the above is a functional derivation such that only one term in the k-space sums are picked out when the derivation is performed. Applying the first of Eqs 4.20 to 4.18, we obtain bk†

∂Ek + ∂k

eβEk e−βEk − 1 + e−βEk 1 + eβEk

=0

(4.21)

or equivalently bk† = k

tanh(βEk /2) 2Ek

(4.22)

≡χ (k)

where χ (k) may be interpreted as a pair-susceptibility, i.e. the ability the system has to form Cooper-pairs. Using this explicit self-consistent relation between the order parameter bk and the gap parameter k in the definition (Eq. 4.9), we finally arrive at a self-consistent equation for k , namely the celebrated BCS gap-equation k = −

k

Vk,k k

tanh(βEk /2) 2Ek

(4.23)

As it is written here, it applies at the mean-field level to any superconductor, and as long as we do not specify the origin of the attraction, it is not limited to phonon-mediated superconductivity. Physically, we expect that in reality the detailed frequency spectrum of the ‘glue’-bosons does play some role in the phenomenon, but such details are left out of the above treatment. If we were to take such details into account, then we would arrive at a description which would be quite specific to the precise pairing mechanism we have in mind. The

86

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

lack of such details in the above mean-field theory is usually referred to as a weak-coupling approximation. The more sophisticated (but still mean-field!) description where the details of the specific spectra of the ‘glue’-bosons are taken into account, is usually referred to as Eliashberg theory, or strong coupling theory. We will not go into the details of this theory here, but simply state that the above picture of the superconductor as an electronic condensate is the basic picture in weak-coupling as well as strong-coupling theory. One remark is appropriate here. The phenomenon of Bose–Einstein condensation is well known, both in the context of cold dilute inert gases, as well as in the superfluid transition of H e4 . The basis for Bose–Einstein condensation even in ideal quantum gases is very much dependent on the fact that the basic constituents which condense are bosons that experience a statistical bosonic symmetry attraction. Electrons, on the other hand, obey the Pauli principle, which roughly may be viewed as a very brutal hard-core repulsion, rendering the pressure of even the ideal fermionic quantum gas finite at zero temperature, P = (4π 2 /3m)(3/8π )2/3 ρ 5/3 , where ρ is the particle density. How can electrons then condense? The answer lies in the fact that by first forming Cooper-pairs, which roughly may be considered to be bosons, the electrons effectively shed the shackles of the Pauli principle, and subsequently undergo a condensation into a superconducting condensate. Therefore, we reach the important conclusion that in principle, superconductivity arises as a result of some sort of condensation in a quantum fluid of Cooper-pairs. We will return to a more detailed description of precisely what this means, but it is important to understand that the formation of Cooper pairs occurs, in principle, at a temperature which is above the true superconducting transition temperature. It is only as a result of a mean-field approximation that we find that the temperature at which we get Cooper-pairs is the same as the temperature where superconductivity occurs. In three dimensional systems of good metals, fluctuation effects that lead to a separation of the Cooper-pair formation temperature and the superconductivity, are tiny and almost immeasurably low. However, in systems like high-Tc superconductors, which first of all are quasi-two-dimensional and secondly arise out of metals with very low carrier density, but nonetheless have very respectable transition temperatures, fluctuation effects are much more prominent, and ignoring them therefore becomes a much more dubious endeavour. The important fluctuations that destroy superconductivity, but do not dissociate Cooper-pairs, are transverse phase-fluctuations of the complex two-component superconducting gap function k . The stiffness of the phase of this gap-function, which is a measure of how difficult it is to excite transverse phase-fluctuations, is given by the superfluid density of the system, which is limited by the carrier density. Poor metals thus are expected to give rise to superconductivity where phase-fluctuations play a prominent role. Good metals are expected to give superconductivity where mean-field theory should work very well. In

TRANSITION TEMPERATURE Tc AND THE ENERGY GAP

87

superconductors, the Ginzburg–Landau parameter κ is determined by the super√ fluid density and the critical temperature, κ = λ/ξ ∼ Tc / ρs . Hence, in type-I and moderate type-II superconductors, we can ignore fluctuation effects. In extreme type-II superconductor, like the high-Tc compounds, they cannot be ignored. We will give a detailed description of phase-fluctuations of the superconducting order parameter in Chapters 9 and 10.

4.3 Transition temperature Tc and the energy gap The minimum of the free energy is determined self-consistently by having the gap-parameter satisfy the equation k = −

Vk,k k

k

tanh(βEk /2) 2Ek

(4.24)

At this stage, this is a mean-field equation with a quite general interaction matrix element Vk,k . Assuming that the potential is separable, i.e. Vk,k =

λη gη (k)gη (k )

(4.25)

η

where gη (k) are basis functions for the irreducible representations of the crystal symmetry group of the lattice which the electrons move through, then the gap can be written on the general form k (T ) =

η (T )gη (k)

(4.26)

η

The indices η denote symmetry channels that are represented in the total gapfunction. We will take a particularly simple form of this matrix element, namely Vk,k = −V

(4.27)

for such pairs of wavenumbers k, k that lie in a thin shell around the Fermisurface of thickness ω0 , and zero otherwise. The physical interpretation of ω0 is that it is an upper frequency cutoff on the spectrum of the bosons that provide the ‘glue’ between the electrons forming the Cooper-pairs. For phonon-assisted superconductivity, we have ω0 = ωD , where ωD is the Debye-frequency. Inserting this into the gap equation (Eq. 4.24), we conclude that the gap k is

88

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

k-independent, i.e. it is the simplest case of a gap which transforms as the identity under the allowed symmetry operations of the crystal which the electrons move through. Hence, the gap-equation can be written in the form

1=V

tanh(βEk /2) k

(4.28)

2Ek

There are two cases where this equation is easy to solve, namely T = Tc and T = 0, and we consider the former first. Letting T → Tc− , i.e. in the limit of a vanishing gap, the above equation simplifies in that we ignore the gap in the quasiparticle spectrum Ek . Moreover, we replace the k-sum by an energy integral by introducing the normal-state density of states Dn (ε). The k-space sum is by assumption limited to a narrow region around the Fermi-surface. We therefore need to consider the density of states near the Fermi-surface. Assuming that the Fermi-level is not located close to energies where Dn (ε) has a rapid variation, e.g. not located close to van Hove singularities, we may then simply replace Dn (ε) with Dn (0), i.e. the density of states at the Fermi-level when all energies are measured relative to the Fermi-surface. Finally, upon introducing the dimensionless coupling constant λ ≡ V Dn (0), we get the following equation determining Tc

1=λ

ωD

dε 0

tanh(βε/2) ε

= λ tanh(βωD /2) ln(βωD /2) −

βωD /2

dx 0

ln(x) cosh2 (x)

,

(4.29)

where we have performed a partial integration to isolate the logarithmic singularity in the integral. For phonon-assisted superconductivity (more generally, for weak-coupling superconductivity), λ 1. This means that in order to satisfy the above equation, we require that βωD /2 1. Hence, since the second integral above is rapidly convergent, the above simplifies to ∞ ln(x) βωD − dx 1 = λ ln 2 cosh2 (x) 0 π βωD − ln = λ ln 2 4eγ γ 2e βωD = λ ln π

(4.30)

89

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

m where γ ≡ limm→∞ l=1 1/ l − ln(m) = 0.5772156649 . . . is the Euler– Mascheroni constant. This equation may be solved to give kB Tc =

1 1 2eγ ωD e− λ ≈ 1.13ωD e− λ π

(4.31)

On the other hand, at T = 0, the gap-equation (Eq. 4.28) takes the form

ωD 1 dε 1=V =λ √ 2 2Ek ε + 2 0 k

ωD / ω dx D = λ sinh−1 =λ (4.32) √ 2 x +1 0 Again, when λ 1, this requires ωD / 1 for solution of the equation to exist, and hence sinh−1 (ωD /) ≈ ln(2ωD /). Thus we obtain 1

(T = 0) = 2ωD e− λ

(4.33)

Note that both Tc and (T = 0) depend sensitively on the coupling constant λ, and that both are functions of λ with an essential singularity as λ → 0. This reflects the fact that an attractive interaction is a singular perturbation to the free electron gas, in contrast to the repulsive Coulomb-interaction. There is no way we can obtain the above results for Tc and (T = 0) to any finite order in perturbation theory in the dimensionless coupling constant λ. Moreover, since the dimensionless coupling constant λ is not easy to compute reliably from first principles even in simple metals like aluminum, it is extremely hard to compute values of Tc and (T = 0) reliably. This reflects the fact that these quantities depend on all details of the system, and really should not be the focus of any computations, when the goal is to gain some qualitative understanding of the problem. This is actually a lesson that applies to all types of phase transitions. However, what was noted by Bardeen, Cooper and Schrieffer was the following remarkable fact. If we form the ratio of (T = 0) and kB Tc , then we obtain 2(T = 0) 2π = γ ≈ 3.52. kB Tc e

(4.34)

This is a universal amplitude ratio, all materials-dependent quantities precisely cancel out!

4.4 Generalized gap equation, s-wave and d-wave gaps As the BCS Hamiltonian is formulated in Eq. 4.1, it does not make specific references to any particular pairing mechanism, although originally the founders of

90

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the theory definitely had in mind a phonon-assisted pairing mechanism. What is central, is the idea that the basic physical phenomenon underlying superconductivity is pairing of electrons into Cooper-pairs, followed by a condensation of the electron system into a macroscopically phase-coherent matter wave. In a sense, superconductivity is the matter-wave counterpart of laser-light, which is basically a phase-coherent lightwave. The electron-pairing picture will be maintained. However, as a slight generalization of the above approach, we may ignore the issue of the origin of some attractive effective interaction between electron, leaving open even the possibility that it may not be phononic in origin, but could also be purely electronic. Thus, we may generalize the interaction to the case where it is not limited to be operative in a thin shell around the Fermi-surface, i.e. we include the possibility of a non-retarded attractive interaction. We also propose a slightly more complicated form of the matrix element Vk,k than what we suggested in the previous section, based on the physics of phonon-mediated attractive interactions between electrons. Assume that an electron moves through a crystal with some symmetry. Any physical quantity will ultimately reflect the symmetry of the crystal in some way. It can therefore be expanded in a complete set of functions that all reflect the particular crystal symmetry that the electrons experience. For instance, if the system is approximately isotropic we can expand any physical quantity in the complete set of the well-known spherical harmonics, if the crystal has simple cubic symmetry we can expand in the complete set of cubic harmonics, and so on. Let us denote the set of such complete basis functions by {gη (k)}, where η is an index that denotes which particular one of the basis functions is meant. Now, let us assume further that the matrix element Vk,k is factorizable. By this we mean that it can be factorized into two factors, where one factor only depends on k and the other one only depends on k. Now, since the set {gη (k)} is complete, by assumption, we may write λη gη (k)gη (k ) (4.35) Vk,k = η

where λη is the strength of the interaction in the η-channel. To be specific, consider an example. Assume that the lattice is square (twodimensional, with lattice constant set to unity) and that the electron-electron interactions are such that when two electrons are on the same site, on nearestneighbor sites (horizontal and vertical bonds), and on next-nearest-neighbour sites (diagonal bonds) they experience interactions U/2, 2V , and 4W , respectively. Fourier-transforming this to obtain Vk,k we find Vk,k =

U + 2V [cos(kx ) cos(kx ) + sin(kx ) sin(kx ) 2 + cos(ky ) cos(ky ) + sin(ky ) sin(ky )]

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

91

+ 4W [cos(kx ) cos(kx ) + sin(kx ) sin(kx )] × [cos(ky ) cos(ky ) + sin(ky ) sin(ky )]

(4.36)

Now, we would like to re-express this as a sum of factorized terms using the complete set of square lattice harmonics. As the interaction given above is of finite range, Vk,k has a finite number of terms and thus a finite number of square lattice harmonics will suffice to completely express the matrix element. It turns out that the five lowest order square lattice harmonics will do the job. They are given by 1 g1 (k) = 2π 1 g2 (k) = [cos(kx ) + cos(ky )] 2π 1 g3 (k) = cos(kx ) cos(ky ) 2π 1 g4 (k) = [cos(kx ) − cos(ky )] 2π 1 g5 (k) = sin(kx ) sin(ky ) (4.37) 2π Re-expressing Eq. 4.36 in terms of the above basis functions, we find an expression of the form of Eq. 4.35, with λ1 = 2U π 2 , λ2 = λ4 = 4V π 2 , λ3 = λ5 = 4W π 2 , and λη = 0, η ≥ 6. We note in passing the following fact, which will figure prominently in what follows. The symmetry group of the square lattice is C4v . What is important to note about the five basis functions listed above, is that the first two transform as the identity under all symmetry operations included in C4v . The latter three change sign under π/2 rotations. In this respect, they have common properties with l = 0 and l = 2 spherical harmonics functions that are the basis functions for the isotropic case. l = 0 spherical harmonics are commonly referred to as s-wave functions, while l = 2 spherical harmonics are referred to as d-wave functions. Hence, the first two basis functions above are s-wave basis function, g2 (k) is often called an extended s-wave function. The latter three are d-wave functions. Of these, g4 (k) is the most well-known one in the context of high-Tc superconductivity, since the gap in the cuprate superconductors to a very good approximation appears to be of the form k = 0 (T )g4 (k). Note that l = 1 square lattice harmonics do not enter in the above. The reason is that in all of the above, we have implicitly considered only such cases where we have spinsinglet pairing. This means that the spin-part of the Cooper-pair wave functions is antisymmetric so the space-part of it must be symmetric. This requires even-l basis functions. Spin-triplet pairing would be required in order to make use of odd-l basis functions.

92

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

Returning now to the general case, as far as the superconducting gap is concerned, it is clear that when Vk,k takes the form of Eq. 4.35, we obtain the gap-equation k = −

Vk,k k χk = −

k

=

5

5

λη gη (k)

η=1

k

gη (k )k χk

≡−η /λη

(4.38)

η gη (k)

η=1

which shows that the gap itself is also expressible as a linear combination of basis functions, as it should be, being a physical quantity. The coefficients η are not k-dependent, but do of course depend on temperature. Using the expansion of the gap in terms of basis function on both sides of the gap-equation, we find the set of coupled self-consistent equations for that gap in the different channels η η =

5 η =1

Mη,η = −λη

η Mη,η

gη (k)gη (k)χk

(4.39)

k

In general, these equations require numerical efforts in order to be solved. Considering, once again, the above square lattice example, and setting U > 0, V < 0, and W = 0, we find that there is no attraction in the λ1 -channel, and attraction in the λ2 -channel (extended s-wave) and the λ4 -channel (d-wave). Hence, we see that the gap function, which is closely related to the Fouriertransform of the Cooper-pair wave function, adjusts itself so as to be zero in channels where the wavefunction is non-zero for zero separation between the electrons. By choosing extended s-wave or d-wave, the electrons in the Cooper-pair avoid the onsite Coulomb interaction. Recall that in phonon-assisted Cooper-pairing, the electrons did not avoid each other in space, but used retardation to eliminate the adverse effects of Coulomb-interactions. I.e. they avoided each other in time. In the present non-retarded example, the electrons avoid each other in space, but not in time. Avoiding each other in space (higher-angular momentum pairing) or in time (retardation) are the basic two ways electrons can avoid the repulsive Coulomb-interaction. In the BCS gap-equation, the presence or lack of retardation effects is manifest in the presence or lack of an energy cutoff around the Fermi-surface. In the absence of such a cutoff, i.e. in the absence of retardation, the entire Brillouinzone contributes to the gap. Since (r) = k k eik·r , this means that (0) = k k . Hence, k must be chosen so as to obtain (0) = 0 in order to avoid

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

93

Coulomb-repulsion. Gaps of the form k = 0 (T )g2 (k), and in particular k = 0 (T )g4 (k), have this property. The latter gap-function has a form which is believed to be very close to the form of the gap-function in high-Tc cuprates. As an important application and in preparation for later sections, let us obtain the superconducting density of states Ds (E), which may now be found as follows. Imagine that we have some function g(k) that depends on k only through

Ek =

εk2 + 2k , and assume k to be independent of k. Then we have

g(k) =

k

dεDn (ε)g( ε2 + 2 )

=

dEDn (ε)

=

dε g(E) dE

dEDs (E)g(E)

(4.40)

√ dε , where Dn (ε) where we have introduced E = ε2 + 2 and Ds (E) = Dn (ε) dE is the normal state density of states. The above is exact provided we have Dn (ε) =

1 δ(ε − εk ) N

(4.41)

k

Here, N is the number of Fourier modes of the wave-number, equivalently the number of lattice sites in the problem. The normal state density of states is now assumed to be a slowly varying function of ε around the Fermi surface such that we approximate it by Dn (ε) ≈ Dn (0) when we measure energies relative to the Fermi surface energy. Implicit in this assumption is that sharp features in Dn (ε) are absent near the Fermi surface, i.e. there are no van Hove singularities near the Fermi surface. Then we have E Ds (E) =√ (E − ||) 2 Dn (0) E − 2

(4.42)

where (x) is the Heaviside step-function (x) = 1, x > 0, (x) = 0, x < 0. When the gap function k is not a constant in k-space, we derive a density of states more formally from the spectral weight A(k, ω) introduced in Section 3.2, as follows. Introduce, in analogy to Eq. 3.6, the Green’s function G(k, t) for the superconducting condensate. Formally, this Green’s function is given by + G(k, t; σ ) = −i0|ck,σ (t)ck,σ (0)|0

(4.43)

where |0 is the BCS superconducting groundstate. It is an eigenstate of the Hamiltonian Eq. 4.16. Moreover, we have

1 G(k, ω; σ ) = dteiωt G(k, t; σ ) (4.44) 2π

94

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

Without loss of generality we choose one spin direction, σ =↑ say, and find G(k, t; ↑) = −i0|(cos(θ )ηk+ (t) − sin(θ )γk+ (t))(cos(θ )ηk (0) − sin(θ )γk (0))|0

(4.45)

Now, using the fact that (ηk , γk ) diagonalize the BCS Hamiltonian, we have that 0|ηk+ γk+ |0 = 0 0|ηk γk |0 = 0

(4.46)

Hence, we obtain G(k, t; ↑) = −i cos2 (θ )0|ηk+ (t)ηk (0)|0 − i sin2 (θ )0|γk+ (t)γk (0)|0

(4.47)

Each bracket is now a free fermion propagator in the superconducting state, hence upon Fourier-transforming we find, introducing the coherence factors in Eq. 4.14, u2k vk2 + (4.48) ω − Ek + iδk ω + Ek + iδk where δk is infinitesimal. The spectral weight is therefore given by, using Eq. 3.8 G(k, ω; ↑) =

A(k, ω; ↑) = u2k δ(ω − Ek ) + vk2 δ(ω + Ek )

(4.49)

which should be compared to Eq. 3.8, and which is seen to be spin-independent. Due to the fact that we are considering spin-singlet pairing, we obtain the same result for σ =↓. Thus, we finally obtain the superconducting density of states per spin channel as 1 Ds (ω) = A(k, ω) N k

1 2 [uk δ(ω − Ek ) + vk2 δ(ω + Ek )] = N

(4.50)

k

which again is seen to be independent of the spin index σ due to the fact that we are here considering spin-singlet pairing.

4.5 Quasi-particle tunnelling and the gap 4.5.1

Introductory remarks

The field of superconductivity made two important steps forward at the experimental discovery of tunneling of single charge carriers (‘quasiparticles’) by Giaever in 1960 [38], and the subsequent predictions of tunnelling of Cooper pairs by Josephson in 1962 [8]. These discoveries set the stage for a new era in superconductivity on the small scale. Structures in which the thickness dimension was as small as a few nanometers could be manufactured in laboratories, and their properties controlled reproducibly. Avenues were opened for

QUASI-PARTICLE TUNNELLING AND THE GAP

95

entirely new research and insights, and for electronic devices of a kind that could not even in principle be achieved by conventional methods, all due to the unique properties of the superconducting state, and its wave-function. At the time of the discovery of these new phenomena quantum mechanical tunnelling was a well-established concept in atomic and nuclear matter, and had recently been demonstrated by Esaki to occur between semiconductors separated by a thin barrier. It took the curiosity of two young and independent student minds to divert from conventional thinking, and venture into the new landscapes: The scientific world was startled at the simplicity and profoundness of their discoveries. Giaever pointedly describes his discovery as a method of ‘measuring the superconducting energy gap with a voltmeter’. This apparent simplicity, and the importance of the results led to immediate acceptance. Josephson’s theory, on the other hand, met some initial skepticism. But within a year, experimental evidence began to accumulate in favour of Josephson‘s ideas, and further theoretical work by many groups expanded our understanding of the physics involved, and contributed to the foundation of present-day sophisticated devices, leading on to what we call today ‘Josephson technology’. Here again initial discoveries in pure physics found their way to applications in electrical engineering sciences and technical products.

4.5.2

The tunnelling principle

The tunnelling of a small particle through a barrier in vacuum is a standard problem in atomic physics books, and solvable by relatively simple mathematics using the Schr¨odinger equation, on requiring continuity of the wave-function through the barrier. Usually, the height of the barrier is an unknown parameter, which may eventually be determined by comparison of experiment and theory. When tunnelling is to take place between two conductors, separated by an insulating barrier, several possibilities arise. If we let N symbolize a normal metal, and S a superconductor, and have the substances separated by a thin insulator I, then we may combine these substances in various configurations: NIN, SIS, NIS, N1 IN2 , S1 IS2 etc. Some of these possible structures are illustrated schematically in Figure 4.1. The symbols φ, φl , φr in superconductors indicate the phases of the wavefunctions. In each case the tunnelling particle leaves the substance to the left, say,

N1

I (a)

N2

N

I (b)

S, f

S1, fl

I

S2, fr

(c)

Figure 4.1 Schematic illustration of various possible configurations for tunneling between two normal metals (a), between normal metal and superconductor (b), and between two superconductors (c).

96

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE E

f(E)D(E) EF

E

f (E)D(E)

f (E)D(E) EF

1

∆

2

EF

EF

N

S

f(E)D(E)

D(E)

D(E)

N1IN2 T ≠ 0, V = 0

NIS T ≠ 0, V = 0

(a)

(b)

I

I T>0 T=0 V (c)

∆ e (d)

V

Figure 4.2 (a) and (c) Illustrate tunnelling between two normal metals N1 and N2 through a thin insulating barrier I as seen in a density of states versus energy diagram, with the Fermi–Dirac function factored in. In (a) T = 0 and applied voltage V = 0. In (c) the I − V characteristic is shown as linear, as a consequence of displacing the electron distributions in (a) along the vertical axis by application of an increasing voltage. The right hand figures illustrate similarly the situation for tunneling between a normal metal and a superconductor with an energy gap , at T = 0 and V = 0 in (b), and that of varying voltage applied, in (d). The consequence of varying T is indicated in (d). Note the onset of tunnelling at V = /e.

where it occupies an allowed state in the conduction band of free carriers, and, after tunnelling enters into an allowed state in a band on the right side of the insulating barrier. These processes are restricted by the energy spectra and the statistics governing the bands from which they tunnel, and into which they arrive. Normal metals are well understood so that the appropriate mathematical description of the process between normal metals is straightforward. Furthermore, the BCS theory for superconductivity gave an accurate description of the energy bands in typical low-Tc metallic superconductors. Because this theory already existed by the time of the experimental work by Giaever and coworkers, the appropriate integrals could be written down. Figure 4.2 shows sketches of bands for two of the interesting cases. Figure 4.2a shows the N1 IN2 case, while Figure 4.2b illustrates the NIS case with no external voltage applied. Figure 4.2c and d illustrate the corresponding current–voltage characteristics for the NIN case (c), and the NIS case (d), respectively. None of these represent the Josephson case, however. In the Josephson effect the phase properties of

QUASI-PARTICLE TUNNELLING AND THE GAP

97

the wavefunction come into full play. This requires a different approach, as will be discussed later. The Giaever case is a simpler one. Let us look at the terms that contribute to the tunneling of single carriers, beginning with the NIN case where only normal electrons are involved.

4.5.3

Single-particle NIN tunnelling

For this discussion we refer to Figure 4.2a. The total number of electrons travelling across the barrier from left to right is proportional to the number of filled electron states on the left-hand side (l) and to the number of states that are unoccupied on the right-hand side (r). The tunnelling current il→r at a particular energy level E and in an interval dE is then il→r = Cn Dl (E)fl (E) × Dr (E)fr,h (E)dE

(4.51)

where fl and fr,h are the probabilities that the energy level E to the left is occupied, and that states at the same level to the right are unoccupied, respectively. According to quantum theory, when the transitions take place from left to right, i.e. when the transitions are completed as il→r , the unknown constant Cn may be written as Cn =

2π |Tn |2

(4.52)

where |Tn |2 is the tunnelling probability, given by the squared matrix element for the transition of an electron from the left electrode to the right electrode. We have, in addition, to factor in the number of available states (holes, h) to the right in the same energy interval by use of the relation fr,h (E) = 1 − fr (E)

(4.53)

The total tunnelling current, when adding processes taking place at all energy levels is then

∞ 2π ∞ |Tn |2 Dl (E)fl (E)Dr (E)(1 − fr (E)) dE Il→r = il→r (E)dE = −∞ −∞ (4.54) In equilibrium, of course, a similar integral applies to transitions from right to left. These transitions have to be subtracted to get the net current across the barrier. Finally, therefore: The net current ININ between two normal metals found upon subtraction of Ir→l from Il→r becomes:

2π ∞ |Tn |2 Dl (E)Dr (E)(fl(E) − fr (E)) dE (4.55) ININ = Il→r − Ir→l = −∞ In both equations above we have allowed integration from −∞ to +∞. This is permissible due to the difference term (fl (E) − fr (E)). The properties of these

98

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

functions makes the integrand extremely small outside a narrow energy window of order kT . Now, without a voltage applied, the difference (fl (E) − fr (E)) is simply zero, as may be seen from Figure 4.2a and b: No net charge transport can occur without an applied voltage. The claim that fl (E) − fr (E) = 0 may seem like an oversimplification if we consider two metals with different Fermi energies to the left and to the right. A very important condition has to be fulfilled for this equality to hold: The two electron gases must constitute one thermodynamic system. This requires particle exchange across the barrier, in fact vigorous tunneling must take place. It is a basic result of thermodynamics that two systems which come into equilibrium due to exchange of particles, will do so by spilling over particles until they have adjusted their chemical potentials to the same level. In the present context we will approximate the chemical potential µ by the Fermi-energy EF . So EF,l and EF,r become exactly equal at equilibrium. Now clearly fl (E) − fr (E) becomes zero since what really goes into the Fermi-functions is always the difference E − EF . This argument also points to the fact that initially there must be a current to establish equilibrium. But this process is fast, and happens during deposition of the films. We need not worry about such transient properties. We can break this symmetry by applying a voltage V , raising the electron band on one side with respect to the other side. Now current will flow since we have to put E + eV or E − eV as the argument in one or the other of the f -functions, and fl (E) − fr (E + eV ) becomes non-zero. The current is now ININ =

2π |Tn |2

∞

−∞

Dl (E)Dr (E + eV )(fl (E) − fr (E + eV ) dE

(4.56)

We may if eV Ef , to a very good approximation, make the following simplification for calculation of the integral for ININ : (f (E) − f (E + eV )) dE ≈ −

∂f eV dE ∂E

(4.57)

∂f Under the integral − ∂E acts like a δ-function; hence we obtain

ININ =

2π 1 |Tn |2 Dl (EF )Dr (EF )eV ≡ GNIN V = V RNIN

(4.58)

where GNIN is the normal conductance, or the inverse of the resistance RNIN of the entire NIN contact. We have taken Dl and Dr outside the integration, replacing them by the constants Dl (EF ) and Dr (EF ) since under normal circumstances E will be near EF where D(E) varies slowly with E. This result is shown in Figure 4.2c where the simple linear characteristic of one NIN contact is illustrated.

QUASI-PARTICLE TUNNELLING AND THE GAP

4.5.4

99

NIS quasiparticle tunnelling

The analysis given above proves that the NIN tunneling contact acts as an ohmic element in a circuit, a fact worth noting, but as such not particularly exciting or useful since for most purposes we have more practical ways of making resistors. However, the situation is substantially altered once we allow one, or both, of the metals to become superconducting. This can in many cases be achieved simply by cooling the contact. If the two metals were, for instance, Nb with a superconducting transition temperature Tc = 9 K and Pb with Tc = 7 K, we could implement the following contacts by lowering the temperature: N1 IN2 at all T > 9 K; NIS between 7 K and 9 K; and S1 IS2 below 7 K. What makes the NIS or SIS configurations so interesting, and useful, is (i) that they provide us with radically different, nonlinear current-voltage I–V characteristic both for single electron tunneling and for Cooper pair tunnelling, and (ii) that entirely new phenomena arise in SIS contacts in particular, reflecting deeper aspects of the superconducting wavefunction. These aspects are exceedingly interesting from a physics point of view, and harbor the promise for a multitude of important applications. On changing our system under investigation to an NIS-contact, as long as we are discussing single-particle tunnelling, the integrals introduced above do not change in principle, only the density of states Ds in the superconductor replaces one of Dn functions in the normal state. The Fermi–Dirac functions remain unaltered. Again we have to apply a voltage to set up a net current in one of the two directions (see Figure 4.3.) In Section 4.4 we have shown that the density of states of quasiparticles in the superconductor Ds (E) is related to the one in the normal metal Dn (0) near E N

E S

N

S

E FS + ∆ E FN

E FN

E FS E FS

E FS − ∆

V = 0; T ≠ 0; I = 0 (a)

∆ V = e ; T ≠ 0; I ≠ 0 (b)

Figure 4.3 (a) T = 0. Almost no electrons available for tunneling leads to very low tunnel current. (b) Bands displaced by eV . Optimal condition for quasiparticle tunnelling from N to S. In both cases EFN and EFS refer to Fermi energies of normal and superconducting metals, respectively.

100

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the Fermi energy by E ; |E| ≥ Ds (E) 2 = (E − 2 )1/2 Dn (0) 0; |E| <

(4.59)

where energy E is now measured from the Fermi-level EFS . On insertion of Ds (E) the current can be expressed as

∞ |E| 2π q 2 |Tn | Dl (0)Dr (EF ) INIS = 1 (f (E) − f (E + eV )) dE −∞,|E|> E 2 − 2 2 (4.60) where the superscript q reminds us that only quasiparticles (single electrons) are to be counted. The notation |E| > under the integral sign indicates that integration over the interval |E| > is excluded. On comparison with the NIN-case we discover q that INIS can be simplified to q

INIS =

GNIN e

∞

−∞

|E| 1 (f (E) − f (E + eV )) dE E 2 − 2 2

(4.61)

This integral can only be solved analytically in the T = 0 limit, giving 0; |eV | < q 1 (4.62) INIS = GNIN 2 (eV )2 − 2 ) ; |eV | ≥ e The quasiparticle current increases sharply from zero at V < e like the square root of the voltage in excess of e when V > e . A crucial point, which was eloquently exploited by Giaever and coworkers, is the ensuing relation for the differential conductance, defined as GdNIS = dINIS /dV (rather than GNIS = INIS /V used before). One quickly verifies that

∞ dINIS Ds (E) ∂f (E + eV ) = GNIN dE (4.63) GdNIS ≡ dV D ∂(eV ) −∞ n (EF ) Here the derivative of f approaches a δ-function when kT → 0. At finite values it assumes a form similar to a Gaussian distribution, and with a width of the order of kT . In the T = 0 limit the result is then exactly GdNIS = GNIN

eV (eV )2 − 2

1 = GNIN DS (E = eV ) 2

(4.64)

QUASI-PARTICLE TUNNELLING AND THE GAP

101

4

Relative conductance

(dI/dV)NIS (dI/dV)NIN

Pb/MgO/Mg ∆ = 1.34 × 10−3eV

3

T = 0.33 K

2

1

0

0∆

4∆ 8∆ 12∆ Voltage bias eV in units of ∆

16∆

Figure 4.4 Relative conductance of Pb/MgO/Mg contact in the NIS configuration relative to that of the corresponding NIN contact. The structure above the gap is caused by phonon processes during tunnelling. Adapted from Giaever et al. [39].

This means that a measurement of dINIS /dV , indeed a measurable quantity, probes the superconducting quasiparticle density of states function directly. Most clearly we see this in the experimentally accessible quantity GdNIS /GNIN = Ds (E = eV )

(4.65)

An example of an early manifestation of this relationship is seen in Figure 4.4, except for some additional phonon structure. The expected property that the relative conductance diverges like Ds at eV = , is therefore confirmed. A physical measurement can of course never truly measure a divergence in the strict mathematical sense. Neither should one take such a prediction literally in the real world. After all, we are talking about a model, the BCS theory, which has built into it certain idealizations that are not to be regarded as exact. Still, the model predicts a remarkably sharp onset of quasiparticle current vs. V that has been confirmed by experiments, even at temperatures well above T = 0, and the overall behaviour is very close to the BCS prediction. In the so-called excitation representation electron-like and hole-like excitations are depicted in a positive energy continuum above the superconductor gap energy . This is illustrated in Figure 4.5. The superconducting energy gap is introduced by joining the hole-like branch and the electron-like branch at a finite gap energy , and with consequences for the density of states, proportional to |∇E(k)|−1 .

102

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE E = |E′ − EF|

E′

E = |E′ − EF|

EF h

kF

k

0

(a)

e

kF (b)

h

k

0

e

kF

k

∆ (c)

Figure 4.5 (a) Usual free-electron gas representation of T = 0 in a normal metal; holes ◦ below EF , electrons • above. (b) Excitation representation of a normal electron gas at T = 0. Hole branch: ◦h, electron branch •e. (c) Excitation representation in a superconductor with −1 a gap . The two branches join at , and the density of states proportional to ∂E near ∂k the minimum point is strongly modified from that of the normal state in (b).

4.5.5

SIS quasiparticle tunnelling

With the construction of an a SIS contact the possibility arises to establish both a quasiparticle current and a Cooper-pair current between the two superconductors. Both of these can be treated fully by quantum theory, on a similar footing to that used in NIN and NIS contacts above. However, only the SIS-case is reasonably straightforward in the established language of single particle transitions. When Cooper-pairs tunnel the addition of matrix elements for the two constituent particles requires heavier formalism which belongs in a more advanced treatment. The familiar problem in quantum mechanics of adding before squaring comes in. We will attack this case with a different and simpler method in the next section. And, having established a method for calculation of NIS -quasiparticle current, one needs only extend that procedure to the S1 IS2 case directly. The resulting integral can be guessed on the basis of the earlier discussion: q ISIS

GNIN = e

∞

−∞

|E| |E + eV | ((f (E) − f (E + eV )) dE 2 2 E 2 − ((E + eV )2 − 2 ) 12 2 1 (4.66)

Again, it is understood that integration is not to be carried out in the gaps. This current can only be calculated numerically. Instead of working out this problem we resort to simple physical argument. In four successive sketches, Figure 4.6, a qualitative picture is developed for quasiparticle tunneling between two superconductors with different gaps, 1 and 2.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS E S1

103

E S2

∆1

∆2

S1

S2

eV = ∆2 − ∆1

∆1

∆2

EF1

EF2

V=0

V=

(a)

∆2 − ∆1 e (b)

E ∆1 EF

S1

I

S2 ∆2

1

EF

V=

∆1 + ∆2 e (c)

1 V Rnn

2

∆2 − ∆1 e

∆2 + ∆1 e

V

(d)

Figure 4.6 Qualitative illustration of quasiparticle tunneling between two superconductors with different gaps, (a), (b) and (c) at different values of bias field, (d) showing the resulting overall I–V characteristic to be expected.

4.6 4.6.1

BCS coherence factors versus quasiparticle-effects: ultrasound and NMR Introductory remarks

As we have seen in Section 4.2 the BCS theory predicts an energy gap (T ) = o (Tc − T )1/2 associated with the superconducting state due to an effectively attractive electron-electron interaction in the presence of an ionic lattice. This picture needs experimental confirmation. In the preceding section we already discussed a possible method, quasi-particle tunnelling. There are several other methods as well. In fact, specific heat measurements and infrared absorption had already shown, even before the BCS theory was worked out, that a gap had to be present. This was particularly evident well below Tc . In this sense the BCS theory explained already existing results. However, a more complete and satisfactory confirmation of the BCS theory requires measurement of both the gap size, the temperature dependence of the gap, the density of states, and

104

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

confirmation of more subtle effects like the so-called coherence factors. In this section we will illustrate both some theoretical approaches, and some experimental procedures that confirm central aspects of the BCS theory for metallic, low-temperature superconductors.

4.6.2

Transition rates in ultrasound propagation and NMR

Ultrasonic attenuation and NMR have turned out to be excellent tools for testing of the predictions from the BCS theory. Some experimental results for ultrasound appeared already in the BCS paper, and lent immediate support to this important work. Longitudinal phonons interact with the quasi-particles in the same way as with electrons in the normal state. The BCS theory for the attenuation of longitudinal phonons gives a very simple expression to test, as will be outlined below, with (T ) as the only unknown quantity. Early measurements at Brown University [40] showed overall consistency with the predictions of BCS, although the experimental data had low precision near Tc . We will now investigate how ultrasonic attenuation may be used to gain insight, possibly verifying more fully the BCS result. Let us follow the main line of reasoning leading to a prediction for ultrasonic attenuation and NMR relaxation rate. Up to a certain point these physical effects can be described by the same formalism. In quantum mechanical terms we need to calculate transition rates αs . These are the net transition rates between energy levels E and E + ω, in fact quite similar to tunnelling which we discussed previously, in Section 4.5. In the present context the energy ω refers to the exchange of a phonon in the case of ultrasound, and to the exchange of a quantum of electromagnetic radiation in the case of NMR. With the tunnelling effect as a reference, the expression for the desired quasiparticle transition rate in the superconducting state may be logically constructed as

αs = |M|2 C(, E, E + ω)Ds (E)Ds (E + ω) f (E) − f (E + ω) dE (4.67) Here, M is a matrix element for the appropriate electronic transition, the same one as in the normal state due to the close correspondence between quasiparticles and normal state electrons. The Ds -factors are the same density of states we used under the discussion of tunnelling in Section 4.5. However, there is a fundamental difference between the normal state and the superconducting state: In the latter case there is coherence between occupied one-electron states, making scattering events interdependent. This is an interference effect which is expressed by the coherence factors contained in the function C(, E, E + ω)1 . 1 See for instance de Gennes: Superconductivity of metals and alloys, Chapter 4. W. A. Benjamin, Inc. New York, 1966, for a thorough discussion of coherence factors in superconductivity.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

105

The choice of sign in the coherence factor is essential, and distinguishes two important cases. We quote here the form valid at low frequencies, ω . 1 E(E + ω) ∓ 2 2 1 = C(, E, E + ω) = 1 ∓ (4.68) 2 E(E + ω) 2 E(E + ω) Using previously developed expressions for Ds we now obtain the following integral for the transition rate in the superconducting state

∞ E(E + ω) ∓ 2 f (E) − f (E + ω) 2 2 αs = |M| Dn (0) dE (4.69) 1/2 −∞ (E 2 − 2 )1/2 (E + ω)2 − 2 The upper sign here refers to so-called case I processes, and the lower one to case II. The first of these involves a scalar potential as in longitudinal ultrasound, the second one corresponds to the presence of a vector potential A as in transverse ultrasound and in NMR. The notation for the integration limits has been simplified. It is understood that no integration is to be carried out in the range |E| < , since no quasiparticles are present there. Next, to normalize the superconducting scattering rate (Eq. 4.69), against the rate in the normal state we set = 0 to obtain αn corresponding to the normal state transitions rate. Integration of (4.69) gives αn = |M|2 Dn2 (0)ω.

(4.70)

Performing the normalization αs /αn we find an integral which subsequently may be worked out for different cases:

∞ E(E + ω) ∓ 2 f (E) − f (E + ω) 1 αs /αn = dE (4.71) 1/2 ω −∞ (E 2 − 2 )1/2 (E + ω)2 − 2 By calculating and measuring the ratio αs /αn the matrix element |M|2 drops out of the problem, as it did here, and we need not be concerned with its actual value; similarly for Dn2 (0).We are now in a position to discuss two distinct cases: ultrasound and NMR.

4.6.3

Longitudinal ultrasonic attenuation

The attenuation coefficient for ultrasound, α u , is the exponent by which the intensity of an ultrasonic wave at frequency ω decays with distance. Its value is measured in dB/m or in Nepers/m. The quantity α u is also closely related to the mechanical quality factor, the Q-factor, of the sample under study when treated as an acoustic resonator. It represents the ratio of dissipated energy to supplied energy. For this reason the normalized transition rate also corresponds to the normalized ultrasound attenuation, i.e. αsu /αnu = αs /αn . These relative rates can for instance be evaluated in the limit when ω approaches zero, an

106

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

approach which applies in the usual ultrasonic phonon energy range – typically at 100 MHz – where ω is very small, on the scale of the energy gap as well as on the scale of kT in most cases. Upon cancellation of the coherence factors against a density of states factor in Eq. 4.71 one finds an integral which can be simplified as follows in the low ω limit (ω → 0).

1 f (E) − f (E + ω) dE = − ω

∂f dE ∂E

(4.72)

Integration in the allowed range, i.e. excluding the range − to + by integration from −∞ to −, and from to ∞, one finds directly for longitudinal attenuation 2 αsl /αnl = 2f () = , (4.73) (T 1 + e )/kT a remarkably simple result, in form very similar to the Fermi–Dirac function. This result should not come as a complete surprise: Rather, the transition rate and therefore also the attenuation, should be expected to depend on the gap in this manner, since the Fermi–Dirac function determines the rate at which quasiparticles are created above the gap, and hence also the relative attenuation. In spite of this, the result (Eq. 4.73) is not entirely obvious. Without the accidental cancellation of a factor in the function C against a density of states factor in Ds , this simplicity would have been lost. Figure 4.7 shows data obtained on indium and analysed to give the limiting value of at low temperatures, (0) [41]. The early measurements quoted above, gave a good overall confirmation of the theory, but did not test this result fully, especially not near Tc where the temperature dependence is very strong, with a vertical tangent at Tc . Because this is also the region where the difference between the two-fluid model and the BCS model could be expected to be most distinct, ultrasound provides an important testing ground for the predictions of the combined effects of the energy gap and the coherence factors. In the case just discussed, only the gap remains as the controlling factor. This is quite different for transverse ultrasound, as will be discussed below. The BCS prediction for attenuation (Eq. 4.73), was tested by careful measurements using longitudinal ultrasound at 210 MHz very close to Tc in superconducting aluminium [42], (Figure 4.8). The agreement with BCS theory is seen to be remarkably good. We note the almost vertical slope in ultrasonic attenuation at Tc , and the fact that the attenuation drops by 25% over only 40 mK, all of this in full agreement with the BCS prediction. We conclude, that in the case of aluminium the BCS predictions for the temperature exponent of the gap, i.e. the exponent 1/2 in (Tc − T )1/2 , as well as its zero degree value, 0 = 3.52 kT , are in agreement with the experiment. Recalling that BCS is a mean field theory, this constitutes a demonstration that the BCS approach is good in typical low Tc superconductors even in the close vicinity of Tc . No traces of fluctuation effects are seen, in accord with the arguments given in Section 2.6.6.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

107

60 In

Attenuation [dB/cm]

50

an

q||e, q|| [001] 40

f = 270 MHz BCS theory, 2∆(0) = 3.1kT c

30

Datapoints as

20 10 0

1.0

1.5

2.0

2.5

3.0

3.5

4.0

Temperature (K) (a)

0.4

q||e, q|| [110] f = 150 MHz

0.2

In

2a n −1 as

−1

0.3

Slope → ∆(0) = 3.1 kTc 0.1

0

0

0.5

1.0

1.5

2.0

Temperature (K) (b)

Figure 4.7 (a) Measurements of attenuation of longitudinal ultrasound in indium in the normal and superconducting states. The normal state data were obtained by application of a magnetic field H > Hc . (b) Analysis of data at 150 MHz using the function (Eq. 4.73), leads to determination of (0)[41].

However, theoretical work by Halperin and colleagues [43], and later work by Bartholomew [44] and by Mo and co-workers [45], has shown that when κ = λ/ξ 1 the superconducting phase transition is expected to be first order. Aluminium is extreme Type I with a κ-value of order 10−2 , so the theory should apply in this case. Evidently the experiment quoted above would have to be carried out with even much higher than mK temperature resolution to reveal the predicted effect. Judging by the data presented here, the predicted first order jump has to be very small in Al, but its existence even here cannot be excluded on the basis of the presented data.

108

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE 1.00 q||e, q||[110] 0.95

Relative attenuation

210 MHz BCS theory

0.90

Error bars

0.85

a ls /a ln

Experiment

0.80 0.75

40

30 20 Temperature(T c − T ) (mK)

10

0

0.70

Figure 4.8 Measurements of the attenuation of longitudinal polarized ultrasound in superconducting Al, compared to BCS prediction in Eq. 4.73. Notice the temperature scale in mK. Adapted from Fossheim et al. [42].

4.6.4

Transverse ultrasound

The physics of scattering of transverse phonons in superconductors, as observed in experiments using transversely polarized ultrasonic waves, is distinctly different from the longitudinal case. This interesting fact has been largely overlooked in textbooks in superconductivity until now, in spite of the fact that the physics has been well described and understood. In early experiments [46] the attenuation of transverse acoustic waves in very pure metals was found to drop precipitously just below Tc . This effect became known as the ‘rapid fall’. It was somewhat erroneously considered to be due purely to Meissner screening of the fields associated with the transverse wave. It turns out, rather, that this difference offers an interesting possibility to test no less than a hallmark of the BCS physics, namely the coherence factors [47], cf. Eqs 4.14. With transverse waves these factors do not drop out of the transition rates as they did in the longitudinal case just discussed. An experimental test to reveal their possible presence is therefore a highly worthwhile enterprise. The difference referred to, is due to the different electronic responses to the ionic displacements of longitudinal and transverse acoustic waves in a conducting medium. In the presence of a longitudinal wave the electron gas is driven by the electrostatic fields created by the ‘piling up’ and ‘thinning out’ of positive ionic charge as the wave propagates through the lattice. This essentially electrostatic response is very fast, limited only by the plasma frequency, and therefore occurs completely in phase with the ionic motion. The interaction between the primary ionic wave and the electron gas is of a scalar nature, and independent of the direction of both electron spin σ and momentum k. The response of the electron gas is often described as that of maintaining (approximate) charge neutrality.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

109

The case of transverse waves is wholly different; there is no piling up or thinning out of charge in the transverse motion of the lattice. Charge neutrality, preexisting before injection of the acoustic wave, is preserved in the electronic response as well. In this case the transverse ionic current generates a time varying magnetic field, which in its turn drives an electronic current. The coupling between the ionic motion and the electron gas is therefore of electromagnetic nature and much slower than in the longitudinal case, involving the electronic skin depth δ. The presence of the induced magnetic field as an intermediary between ionic and electronic currents becomes extremely important when entering into the superconducting state. This necessarily leads to Meissner screening of electronic currents below Tc , an effect which is not present in the longitudinal case. Screening occurs in the entire range of the acoustic wave, in the bulk, contrary to how we previously encountered the Meissner effect, as a response occurring in a thin layer λ near the surface. As transverse wave propagation is easily generated at a single wavevector q at a time, this opens up for a determination of the superconducting penetration depth λ versus q in the bulk of the material. As was mentioned earlier, the coherence factors now appear in a different way: The interaction between a free charge and a magnetic field occurs via the product p × A = k × A, where A is the vector potential. This term is independent of spin, but changes sign on replacing k by −k. When evaluating the integrals discussed above this property turns out to require the opposite sign in the coherence factor function C introduced in Eq. 4.68. Although the coherence factors dropped out against a density of states factor in the longitudinal case, this clearly cannot happen here, and the coherence factors remain in the problem. Furthermore, screening has to be taken care of, and finite frequency electrodynamics enters in an important way. We now outline the approach which has been followed by Fossheim [42, 47]. The attenuation coefficient α for ultrasonic waves propagating in a conducting medium can be expressed as the energy dissipated per second divided by the energy input per second, both calculated per unit area of the wavefront. In the presence of induced current densities and fields this leads to the expression α=

1/2Re(j ∗ E) 1/2ρvi2 vs

(4.74)

Here we need an expression for the electronic current density j whose complex conjugate appears in Eq. 4.74, and the electric field E within the superconductor, which is by no means zero in this electrodynamic problem. Other factors in the above expression are the density of the material ρ, the ionic velocity vi and the velocity of sound vs . The quantity we have to express is primarily the field E, since the current density can always be written as j = σ E ≡ (σ1 + iσ2 )E. Here we have defined the complex frequency dependent conductivity σ as consisting

110

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

of a real part σ1 and an imaginary part σ2 . Next we express the electric field by these conductivities. For this purpose we combine Maxwell‘s equations ∂B ∂t ∇ × B = µ0 (j s + j i ) = µ0 (σ E + j i ). ∇×E =−

(4.75) (4.76)

Here we have introduced the magnetic induction B created by the ionic current density j i of the transverse acoustic wave, and the associated self-consistent electric field E generated by the time-dependent magnetic induction. We will assume the waveform to be exp i(qx − ωt) for all fields and currents in Eqs 4.75 and 4.76. To solve these equations for E we assume that the wave is traveling in the positive x-direction, generating the transverse ionic currents along the y-axis, and consequently the induction B is along the z-direction. In this plane wave scheme the spatial derivatives are nonzero only when taken with respect to x. We combine the two Maxwell equations by taking the curl of Eq. 4.75 and the time derivative of Eq. 4.76, and find ∇×

∂B ∂ = µ0 (σ E + j i ) ∂t ∂t

(4.77)

which is to be combined with ∇ × ∇ × E = −∇ ×

∂B ∂t

(4.78)

Recalling that for transverse waves there is no net charge accumulation, we have ∇ × E = 0 in the second of these equations. Using this to simplify Eq. 4.78, and after equating the right-hand side of Eq. 4.77 with the left-hand side of Eq. 4.78, we arrive at E=

iµ0 ω j q 2 − iµ0 ω(σ1 + iσ2 ) i

(4.79)

and eventually to

−σ1 + i E=

q2 µ0 ω

q2 + σ2 µ0 ω ji 2 + σ2 + σ12

(4.80)

This expression is fully valid in both the normal and the superconducting states. Referring to Eq. 4.74 we now normalize the attenuation coefficient in the superconducting state against that in the normal state, in both cases taking

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

111

the expression for the electric field from Eq. 4.80. The procedure is now to carry out σ1s |E s |2 Re(j s × E s ) αst = = αnt Re(j n × E n ) σ1n |E n |2

(4.81)

We have attached the suffixes s and n to the respective fields in the superconducting and normal states. To further develop Eq. 4.80 we introduce one simplifying aspect: the imaginary part of the normal state conductivity can be shown to be negligible in comparison with the real part at usual ultrasonic frequencies up to several hundred megahertz, hence σ2n is omitted hereafter. Note, however, that σ2s can by no means be neglected. After some algebra the final, normalized attenuation was found by Fossheim as [47] αst αnt

σ1s (qδ)4 + 1 σ1n = 2 2 σ2s σ1s 2 + + (qδ) σ1n σ1n

(4.82)

We leave it as an exercise to carry out the manipulations required to obtain this result from Eq. 4.81. In Eq. 4.82√we have introduced the parameter δ = (1/µ0 ωσ1n )1/2 . Except for a factor 2 this is the usual normal state skin depth for electromagnetic fields. We note from the way the skin depth appears together with the imaginary conductivity in the denominator of Eq. 4.82, that normal state screening plays a role. The product of skin depth δ and wavevector q – essentially the ratio of skin depth to acoustic wavelength – measures the effectiveness of the normal state screening since the term (qδ)2 adds to the term σ2s /σ1n which represents superconducting screening. The latter contains the Meissner effect. Thus in a subtle way Eq. 4.82 describes a continuous crossover between normal state screening and superconducting screening. What is being screened, of course, are the induced currents j , and B-fields that provide the coupling between the transverse lattice waves and the electron gas. And, as these are screened out, so is the electric field E. Therefore the whole coupling mechanism breaks down in a narrow temperature range below Tc . This eliminates a dissipation channel, and the acoustic attenuation drops dramatically, as mentioned above, the so-called ‘rapid fall’ which was referred to before. It is a phenomenon full of essential superconductor physics, as we demonstrate in more detail, next. Importantly, the coherence factors did not drop out of the problem, but are present in the conductivities. We proceed to discuss these aspects, making use of the transition rates again, i.e. Eq. 4.71, as was done originally by Mattis and Bardeen [48]. It is appropriate to associate the transition rate with the processes that determine σ1s since this is the loss part of the complex conductivity. The

112

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

resulting integral, still with the coherence factors intact, cannot be solved analytically, but an approximate analytic form was found by Cullen and Ferrell [49] 2 8 1 σ1s 2 ln − 8.42/π =1+ σ1n 2 kT eω kT

(4.83)

Mattis and Bardeen also gave σ2s /σ1n in integral form, but an analytic solution was only given under conditions which are outside of the accessible range in the experiments we are discussing here. The work of Fossheim [47] introduced instead a nonlocal modification of the London expression for σ2s /σ1n , as follows: σ2s 1 =2 λ−2 L (0) × T × K(qξ0 ) σ1n µ0 ωσ1n 2 δ =2 × T × K(qξ0 ) λL (0)

(4.84)

Here λL (0) is the zero degree London penetration depth, T = (Tc − T ), and K(qξ0 ) is the nonlocal Pippard kernel (see [47]). Since this term Eq. 4.84 appears not as a factor in the expression for αst /αnt , but added to the term (qδ)2 this approximation is not as essential to have in the correct BCS form as is the case with σ1s /σ1n , which contains the dominating effect of the coherence factors. That aspect is essential very close to Tc as it turns out that the presence of the coherence factors in σ1s /α1n dominate the behavior of the attenuation αst /αnt in the first few mK below Tc , below which it is overlapped and followed by the Meissner screening. And while at the transition the attenuation would have zero slope if the Meissner screening was the dominant effect, on the contrary, with the coherence factors present a sharp break occurs, with vertical slope. Perhaps no other phenomenon defines Tc as sharply as this in superconductivity. The issue is therefore whether experiments can confirm the latter prediction. Experiments in indium [47] and in aluminium [42] shown in Figure 4.9 provide substantial verification of the presence of the coherence factors, showing the predicted sharp break on the sub-millikelvin scale. In fact, in Ref. [47], Tc was resolved with ±2/10000 K resolution! In the aluminium results, there appeared a correction factor in the parameter λL (0) which was interpreted as an effect of electronic effective mass enhancement by about 1.5 due to electron–phonon interaction, also in accord with cyclotron resonance experiments. Again, evidence for the predicted first order transition [50] was not found. Evidently, even the already very high resolution of this experiment was not sufficient to see it. Calculations of the attenuation of transverse waves in several metals were carried out by [51], covering a wide range of frequencies. At frequencies of the order of 1 GHz, depending on the metal, it was found that the presence of the qδ-factor alters the sign of the initial slope of αst /αnt from a sharp downward break to an equally sharp upward break. This latter effect resembles very closely

1.0

147 MHz 206 MHz 245 MHz 285 MHz 305 MHz

0.8

Relative attenuation

q|| [110], e||[010]

0.6

113

ats /a tn

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

Theoretical curve, m = 1.4 0.4

0.2

30

25

20

15

10

5

0

0

Temperature T c − T (mK)

Figure 4.9 Attenuation of transversely polarized ultrasound in superconducting Al near Tc . Measurements by Fossheim et al. [42]. The continuous curve is a calculation based on theory by Fossheim [47]. µ is the mass enhancement factor mentioned in the text.

the behavior of the NMR relaxation rate at the superconducting transition. In essence, transverse ultrasonic experiments and NMR experiments contain the same information regarding the presence of BCS coherence factors, whether the ultrasonic frequency is high or low. It should be mentioned that the ultrasonic experiments referred to were carried out on ultra-pure 6N metals, where the electronic mean free path at low temperatures is of the order of millimetre length, making the product q 1, being the electronic mean free path. In this case the electronic attenuation in the normal state is temperature independent and proportional to q, and the rapid fall or rapid rise below Tc is a very strong and sharp effect.

4.6.5

Nuclear magnetic resonance relaxation below Tc

One of the earliest and most successful confirmations of the BCS theory was provided by the nuclear magnetic resonance measurements of the longitudinal relaxation rate 1/T1 in a superconductor by Hebel and Slichter [52]. The observed rise of the relaxation rate just below Tc , to a level above that in the normal state, confirmed a crucial aspect of the theory. A good idea of the expected behavior is obtained by use of the scattering rate already given in Eq. 4.71. By again introducing the derivative of the Fermi–Dirac function like before, and adding symmetric contributions from the ranges E ≥ and E ≤ − after allowing ω → 0, one finds the following integral expressing the relative NMR relaxation rate αs /αn in the superconducting state normalized against that in the

114

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

normal state as αs = −2 αn

∞

E 2 + 2 E 2 − 2

∂f ∂E

dE.

(4.85)

This integral diverges logarithmically. If ω had been allowed to retain a finite value, the divergence would be avoided, and the result would be of the order of ln(/ω), as discussed by Tinkham [53], of the order of 10 for typical cases. This is far larger than what is measured. Various schemes have been discussed in the literature to reduce this discrepancy. The main ones have been to take account of anisotropy of the energy gap, and to assume nonuniform lifetimes of quasiparticles over the Fermi-surface. What has become quite clear after the discovery of high-Tc superconductors is that the rise in relaxation rate below Tc is tied to the symmetry of the wavefunction. The relaxation peak is present in s-wave superconductors, as was worked out by BCS, but not in d-wave superconductors like the high-Tc cuprates. An example of a low-temperature measurement Superconductivity research during the first 75 years since 1911, was always a domain of low temperature physics, and a large part still is, in spite of highTc superconductivity. Figure 4.10 shows an example of an experimental setup which led to the ultrasonic data near Tc quoted previously in this section [42]. The measurements in aluminium required careful temperature control and measurements down to 1.1 K. This is just within the temperature range accessible by pumping away the evaporating gas from liquid helium 4 He, whose boiling point is 4.2 K at STP. The cylindrical chamber shown in the figure is immersed in helium, which at these temperatures (T < 2.2 K) is a superfluid, in a cryogenic glass Dewar and filled with superfluid through the tube indicated in the figure as the pumping line. Inside the chamber shown here, the sample is mounted onto the lower end of a quartz crystal acting as an acoustic delay line, centrally located in solid copper block for temperature stabilization. The use of superfluid helium in addition, offers excellent conditions for temperature stabilization since it is well known to sustain zero temperature gradients. This is ideal for the present purpose which requires a temperature stability better than 1/1000th of a degree. Other details of the physical attachments are shown in the figure. Note in particular the pumping outlet. It has a narrow constriction, 0.65 mm in diameter. While this arrangement still allows efficient pumping of gas from the chamber due to the short length of the hole, and the low density of the gas, it reduces substantially the flow of superfluid He film out of the chamber. If the superfluid is allowed to flow up along the inner wall of the pumping line over its full diameter, a phenomenon which is well known to occur, it will reach high enough temperatures to evaporate, thereby reducing the pumping efficiency sufficiently to prevent the lowest temperatures to be reached. The

THE GINZBURG–LANDAU THEORY

115

Pump Leads Signal

Spring Electrode Transoucer Delay rod Solid cu cylinder Cu chamber Ge S H

Sample Transoucer Electrode Spring

Figure 4.10 Experimental arrangement used to reach 1.1 K by pumping in liquid helium.

constriction reduced the film flow substantially, and the system worked exactly as planned, allowing 1.1 K to be reached. This as a good example of the type of know-how which is sometimes needed to perform good low-temperature measurements. The insert in the chamber is also equipped with a temperature sensor and heater for control of the temperature to submillikelvin level.

4.7 The Ginzburg–Landau theory 4.7.1

Some remarks on Landau theory

The Ginzburg–Landau theory [10] for superconductivity represents one of the most useful tools available for the theoretical description of superconductivity. It starts with a free energy expansion, completely in line with the general Landau theory [54] for condensed matter, with particular attention being paid to the term representing the gradient of the ordering quantity. In Section 4.1 we have referred to magnetic analogies to superconductivity for an intuitively simplified discussion of the quantum mechanical wavefunction. We begin here similarly with a brief discussion of the Landau free energy for a ferromagnet, where the ordering quantity is the spin. When spins, or the corresponding magnetic moments µi , are summed up and averaged over the volume they occupy, the magnetization may be expressed as M = i µi /V . M may take different orientations depending on symmetry, in order to minimize the total energy. Examples of such behaviour are commonly found in magnetic

116

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

domains in ferromagnets, where neighbouring domains may have the magnetization pointing in orthogonally different directions due to anisotropy. The domain walls between these small volumes are a kind of topological defects where the spins gradually change direction form one domain to the neighboring one, a configuration called Bloch wall, that costs extra energy to produce. This energy appears in the free energy expansion as the square of the gradient of M. This arrangement is still energetically favorable due to the resulting reduced field energy outside the material. Apart from this, the Landau expansion is permissible when assuming that we perform the calculation of the free energy relatively close to Tc , although not too close in case fluctuations might become important. The point here is that we can define a small parameter in this range, namely m = M(T )/M(0), which is the ratio between the actual magnetization M(T ), and the saturation value M(0) at T = 0. This quantity m(T ) may be used as an expansion parameter to whatever order is necessary. We have still one more aspect to take care of: There is always a background energy F0 (r, T ), which is independent of m. This can most easily be thought of as the entire free energy of the system at m = 0, for instance just above the magnetic ordering temperature Tc . The Landau free energy density is then: 1 1 F (r, T ) = F0 (r, T ) + αm2 + βm4 + c |∇m|2 (4.86) 2 4 Notice here that there are no terms of odd power in the m-expansion. Physically this is due to the obvious fact that the free energy in a ferromagnet must be independent of whether the spins point up or down. This constraint applies to most systems, whether magnetic or not, and is always caused by symmetry. We will now for simplicity confine the analysis to the interior of one domain where M and m are constant, and disregard the remaining terms. Minimizing the remaining free energy, requires

We find The solutions are:

∂F =0 ∂m

(4.87)

2αm + 2βm3 = m(α + βm2 ) = 0

(4.88)

m=0

and

m2 = −

α β

(4.89)

Generally, both α and β are themselves functions of temperature and are to be thought of here as the lowest order term in a temperature dependent expansion of the coefficients of Eq. 4.86. By studying the minimization conditions in more detail one finds that the expansion of α must have a zero’th order term equal to zero, so to lowest order α = α1 (T − Tc )

(4.90)

THE GINZBURG–LANDAU THEORY

117

where α1 is a constant. For β we find that the zero-order term β0 is finite, and we stop the expansion there. This adds up to α1 (Tc − T ) β0 1 1 α1 2 m= (Tc − T ) 2 β0

m2 =

(4.91)

So, the magnetization grows from 0 at Tc , like the square root of Tc − T . Above Tc its value is m = 0 in accordance with the first solution in Eq. 4.89. Both aspects are illustrated in Figure 4.11. What happens physically is that above Tc spins are totally disordered, producing m = 0. Below Tc , however, ordering increases gradually like the square root of temperature measured relative to Tc . Because of the gradual associated ordering taking place in the magnetic spins when T is lowered below Tc , the quantity m is called the ‘order parameter’ of the ferromagnetic transition. We also see that m is indeed suitable as a small quantity to expand in. The above gives an idea of the basic content of Landau theory, applicable to a wide range of systems where ordering takes place below a certain temperature. We have so far neglected the gradient term. This will often not be permissible, as we will see in superconductors.

4.7.2

Ginzburg–Landau theory for superconductors

Magnetization m(T )

The Landau approach works specially well in systems with long correlation length, called coherence length ξ in superconductors. We should measure this length on an atomic scale. Because ξ in low-Tc superconductors can be as long as thousands of interatomic distances (recall for instance Al, with ξ(0) = 1600 nm) superconductors offer a particularly suitable arena for the application of Landau theory, in that case called Ginzburg–Landau theory. As, on the other hand, ξ in high-Tc materials is only of the order of one, or a few, unit cell distances, one

1

(Tc − T ) 2

Tc Temperature T

Figure 4.11 Magnetization m(T ) versus temperature according to standard Landau theory described in the text.

118

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

should rightly be concerned about the validity of Ginzburg–Landau theory in such systems. Experience has shown that for many purposes it works quite well even there, when discussing equilibrium properties. However, one has to exercise great caution. For instance, as we have shown in Section 2.6 one should expect very vigorous thermal fluctuation in the order parameter, the superconducting wavefunction ψ, on approaching Tc . Indeed this causes immense complications in high-Tc as compared to low-Tc superconductors. Leaving those problems aside for now we proceed to develop the Ginzburg–Landau theory of superconductivity. We emphasize the following: The superconducting wavefunction ψ does possess the property required for an order parameter: Its equilibrium value is zero above Tc and increases gradually below Tc when written as 1

ψ = n 2 eiϕ = |ψ|eiϕ

(4.92)

where n is the density of Cooper pairs. Whether we refer to the BCS theory or use the language of the two-fluid model we know that the appearance of the factor n ensures that ψ has the required property. The phase ϑ is another quantity of great importance, and one that we shall dwell considerably on in later chapters. The next important step is to write the gradient term in the free energy expansion in a quantum mechanically appropriate manner. We have to define the momentum operator in a magnetic field, writing p = (−i∇ − 2eA)

(4.93)

where the symbols have their usual meaning in quantum mechanics, and we have introduced the charge −2e of a Cooper pair; and below we introduce its mass m. We are now ready to sum up the terms in the Ginzburg–Landau free energy density for a superconductor: β 1 1 2 |ψ|4 + |(−i∇ − 2eA)ψ|2 + B 2 2m 2µ0 (4.94) We remark here that since all the terms in Eq. 4.94 represent energy densities, the total free energy of the system is

d3 rFs (r, T ) (4.95) Fs (T ) = Fs (r, T ) = Fn (r, T ) + α |ψ|2 +

V

For the ensuing calculations we will define a vector G ≡ (−i∇ − 2eA), and we remind ourselves that the vector potential A is related to the magnetic induction B by B = ∇ × A. Next we carry out the minimization procedure for the free energy by making variations in ψ and ψ ∗ , i.e. by letting ψ → ψ + δψ, and ψ ∗ → ψ ∗ + δψ ∗ . The equilibrium condition δFs (T ) = 0 will then give us the Ginzburg–Landau

THE GINZBURG–LANDAU THEORY

119

equations, two equations of paramount importance in superconductivity. We can immediately write δFs (r, T ) = α(ψ + δψ)(ψ ∗ + δψ ∗ ) − αψψ ∗ β (ψ + δψ)2 (ψ ∗ + δψ ∗ )2 − ψ 2 ψ ∗2 + 2 1 G(ψ + δψ)G∗ (ψ ∗ + δψ ∗ ) − GψG∗ ψ ∗ + 2m

(4.96)

with G as defined above. Next we simplify: δFs (r, T ) = α(ψδψ ∗ + ψ ∗ δψ) + β(ψ |ψ|2 δψ ∗ + ψ ∗ |ψ|2 δψ) 1 + (GψG∗ δψ ∗ + GδψG∗ ψ ∗ ) (4.97) 2m The last parenthesis is GψG∗ δψ ∗ + GδψG∗ ψ ∗ = (−i∇ − 2eA)ψ(i∇ − 2eA) δψ ∗ + (−i∇ − 2eA) δψ(i∇ − 2eA)ψ ∗ (4.98) Summing up:

δFs (T ) =

d3 r (αψδψ ∗ + βψ |ψ|2 δψ ∗

V

1 (−i∇ − 2eA)ψ(i∇ − 2eA) δψ ∗ + c.c.) + 2m

(4.99)

After a partial integration we obtain, using ∇A = 0

1 3 2 2 ∗ δFs (T ) = (−i∇ − 2eA) ψ)]δψ + c.c. d r [(αψ + β |ψ| ψ + 2m V (4.100) Requiring δFs (T ) = 0 demands that the functions in front of δψ ∗ and δψ are zero, which means that we have GL-I:

αψ + β |ψ|2 ψ +

1 (−i∇ − 2eA)2 ψ = 0 2m

(4.101)

This is the first of the two Ginzburg–Landau equations, hereafter referred to as GL-I. Next, as a preparation for the derivation of the second Ginzburg–Landau equation, GL-II, we introduce Maxwell‘s equation ∇ × H = J which we use in the form ∇ × B = µ0 J . We write it out as µ0 J = ∇ × B = ∇ × (∇ × A) = ∇(∇ × A) − ∇ 2 A = −∇ 2 A

(4.102)

in the London gauge where ∇ × A = 0. When we later encounter the term − µ10 ∇ 2 A we will recognize this as the supercurrent J .

120

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

The procedure by which GL-II is obtained is to vary A in the free energy Fs (r, t), i.e. we let A → A + δA and find the corresponding variation in Fs (r, t). For this minimization of the free energy density Fs (T ) with respect to the vector potential A we need only retain the A-dependent parts of Fs (r, t). We write this as Fs (r, t, A). Next we take the variation δFs (r, t, A) = Fs (r, t, A + δA) − Fs (r, t, A)

(4.103)

In writing out the expression here we temporarily introduce the symbol p for −i∇ to simplify the mathematics. The proper operator is immediately reintroduced in the next step. We find 1 (p − 2e(A + δA))ψ (p∗ − 2e(A + δA))ψ ∗ 2m 1 (p − 2eA)ψ (p∗ − 2eA)ψ ∗ − 2m 1 + (∇ × (A + δA))2 − (∇ × A)2 2µ0 e iψ ∗ ∇ψ + iψ∇ψ ∗ + 4e |ψ|2 A δA =− m 1 + (∇ × δA)(∇ × A) (4.104) µ0

δFs (r, t, A) =

Now δFs (r, t, A) is to be integrated over the superconductor volume. We do the last term first:

1 1 3 (4.105) d r(∇ × δA)(∇ × A) = − d3 r∇ 2 A × δA µ0 µ0 Therefore, the entire δFs (T ) becomes

ie 4e2 1 2 3 ∗ ∗ 2 |ψ| A − δFs (T ) = d r (ψ∇ψ − ψ ∇ψ) + ∇ A δA = 0 m m µ0 (4.106) This requires the square bracketed term to be zero. Using the result from Eq. 4.102 the equation for the supercurrent is obtained: e 1 (4.107) (iψ ∗ ∇ψ − iψ∇ψ ∗ ) + 4e |ψ|2 A J = − ∇2A = µ0 m or GL-II:

J =

e ∗ ψ (−i∇ − 2eA)ψ + c.c. m

This is the second Ginzburg–Landau equation.

(4.108)

THE GINZBURG–LANDAU THEORY

121

c

B

Figure 4.12 Flux quantization. The larger area is the superconductor. The small hatched area illustrates a normal domain inside the superconductor where a magnetic flux penetrates a cross section of the sample. The contour c encloses this area completely.

To be precise, in deriving the GL equations so far we have omitted a surface integral:

(4.109) dψ ∗ (−i∇ − 2eA)ψdσ + c.c. This is correct to do if (−i∇ − 2eA)⊥ ψ = 0, i.e. when the normal component of the operator as applied at the surface gives zero. On inserting this condition into GL-II we find that it expresses the condition that no current is entering through the surface, J⊥ = 0. This is physically sound when the surface is a boundary to vacuum or an insulating material. We could turn the question around and ask what boundary condition on ψ would in general make J⊥ = 0. To answer this question, we apply the operator (−i∇ − 2eA)⊥ in GL-II and require J ⊥ = 0, i.e.: J⊥ =

e ∗ ψ (−i∇ψ − 2eA)⊥ ψ + c.c. = 0 m

(4.110)

We continue the discussion of this problem in Chapter 5.

4.7.3

Flux quantization

Imagine that some region of a superconductor is in the normal state due to magnetic flux penetrating it, as illustrated in Figure 4.12. Thus, we may think of the superconductor as a multiply connected domain described by a surface of genus one. In this case, given the order parameter ψ = |ψ|eiϕ the line integral of the gradient ∇ϕ around a closed contour encircling the normal domain has to be given by 2π N , where N ∈ Z. This follows since the order parameter must 2 be singled valued at any given point, and 1 dl∇ϕ = ϕ1 − ϕ2 independent of

122

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the path connecting the start-and endpoint. Thus we have ! dl · ∇ϕ = 2π N

(4.111)

Now, in the presence of a magnetic field, this is only slightly modified. The magnetic field couples to the superconducting order parameter via the vector potential A in such a way as to modify the phase of the superconducting order parameter by the usual minimal coupling scheme. The gauge invariant phase of the order parameter now has the gradient ∇ϕGI (r) = ∇ϕ(r) −

2e A

(4.112)

where we have used the fact that the charge of the Cooper pair is 2e. Such a modification is necessary in order to preserve gauge-invariance of the supercurrent, a physical observable. We have 2e/ = 2π/(h/2e) = 2π/0 , where the 0 = h/2e = 2.0679 × 10−15 T m2 . It is this gauge-invariant order parameter which now is subjected to the constraint ! (4.113) dl∇ϕGI = 2π N as the requirement of singled-valuedness must still hold. Hence, we obtain ! 2π dl × A = 2π N (4.114) 0 By using this in conjunction with Stokes’ theorem we have

! dl × A = dS∇ × A = dSB ≡ = N 0 C

S

(4.115)

S

where B = ∇ × A and is the magnetic flux through the surface S enclosed by the contour C. This flux is thus seen to be quantized in units of 0 . Note that the only place where any information about the superconducting state enters into this is in the statement that the charge of the superconducting condensate is 2e. Had we had a normal metal, we could apply precisely the same reasoning to the phases of the single-electron wavefunction which couples to a vector potential with the charge e instead of 2e. In that case, we would again get flux-quantization, but with twice the periodicity in magnetic field.

5 Weak Links and Josephson Effects 5.1 Weak links, pair tunnelling, and Josephson effects 5.1.1

Introductory remarks

When two superconductors are brought into contact in such a way that the critical current in the contact region is much lower than that of the individual constituents, the contact is called a ‘weak link’. Before contact is established the two superconducting constituents have independent wavefunctions, and therefore arbitrary and independent phases ϕ. Each superconductor wavefunction is characterized by its amplitude |ψ| and phase ϕ: = |ψ|eiϕ

(5.1)

After establishment of the weak link, coherence is established across the barrier, with a phase difference ϕ causing interference between the previously independent wavefunctions. When a Cooper-pair tunnels from the left side to the right of the junction, say, it probes successively the phases of both wavefunctions, the ‘left’ one with phase ϕl and the ‘right’ one with phase ϕr . More precisely, the system can be described as having one wavefunction as a whole. A typical realization of a weak link is a SIS tunnel junction, consisting of two superconducting films, separated by a very thin oxide layer, typically 1–2 nm thick. For low-Tc junctions the most commonly used superconductors are Nb and Pb. Niobium has turned out to be the best one overall. The critical current density of these junctions may be in the range 103 –104 A/cm2 , far below the typical critical current density of bulk superconductors. Transport across the barrier is a tunnel process, and this explains the low current. Tunnelling of Cooper-pairs naturally occurs with a probability far below that which could be expected for single particles. Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

124

WEAK LINKS AND JOSEPHSON EFFECTS

Josephson predicted in 1962 [8] that such a junction would have entirely new and unexpected properties: It should be able to sustain a supercurrent without application of a voltage; and if driven by an external current source to exceed its critical current, radiation of high frequency electromagnetic waves would appear. These predictions were soon confirmed experimentally, and moved superconductivity into a new era. A weak link system can be established in several ways (Figure 5.1). Instead of a thin oxide layer which was mentioned, other materials may be used, for instance a normal metal, corresponding to an SNS junction, in which case the metal layer can be much thicker. Another well established method is to create the whole system from a single superconductor, by splitting for example a continuous film into two regions, leaving just a narrow constriction between, of typical dimensions like the coherence length ξ . This latter construction is referred to as a Dayem bridge. In this case the critical current density is the same in the bridge and the bulk, but the overall critical current of the device is much lower than in the two parts. This is sufficient to make it a weak link. A recently developed method, specially suited for high-Tc superconductors, takes advantage of their very short, nanometre size coherence length ξ . In these superconductors a very narrow interruption of superconducting properties can be achieved by depositing a high-Tc film across a naturally occurring grain boundary in a substrate like SrTiO3 . The grain boundary forces the superconductor to develop a chain of defects along the length of the grain boundary. Above the grain boundary, therefore, there is a weak link between the two parts of the superconductor film. Such contacts are commonly referred to as grain boundary junctions or bi-crystal junctions. So-called break junctions and step junctions are variations on this method, where the topology of the substrate plays a role in creating the weak link. The observation already made, that the phase difference ϕ between the two sides of the junction provides the driving force for the transport of Cooper-pairs, is something we already could have seen from the Ginzburg–Landau equations. The two driving fields for a supercurrent were found to be the vector potential A ~x

I,N

GBJ Sl Sl

Sr

S

S

Sr

~x GB

(a)

(b)

(c)

Figure 5.1 Different types of weak links, (a) between superconductors Sl and Sr with normal (N) or insulating (I) barrier between; (b) narrow constriction; (c) grain boundary junction GBJ in a superconductor deposited in top of a substrate with a grain boundary (GB).

WEAK LINKS, PAIR TUNNELLING, AND JOSEPHSON EFFECTS

125

and the superconductor phase gradient ∇ϕ. In the case of a Josephson junction between two homogeneous superconductors the phase gradient becomes discretized, i.e ∇ϕr → (ϕl − ϕr )/d where d is the barrier thickness. So, already based on the GL-equations the physics community should not have been too surprised in 1962 by the prediction of a phase difference driven, voltage independent supercurrent across a thin barrier between two superconductors. Once the idea has been put forward one realizes the effect should be expected, provided Cooper-pair tunnelling can take place.

5.1.2

DC Josephson effect: the Feynman approach

The basic equation used in analysing the Josephson effect is the time dependent Schr¨odinger equation i

∂ = E ∂t

(5.2)

1

In a superconductor = ||eiϕ = ρs2 eiϕ , ϕ being the macroscopic superconducting phase and ρs the density of Cooper-pairs. However, when a coupling with overlap exists between the wavefunction to the left, l , and to the right, r , a term must be added to account for the ‘leakage’ of wavefunction so that l changes with time at a rate which is proportional to the amount of leakage from r into the left side. And similarly, a symmetric equation must exist for the rate of change of r . This results in the following modification of Eq. 5.2. ∂l = El l + Kr ∂t ∂r i = Er r + Kl ∂t i

(5.3) (5.4)

Here El and Er are the ground state energies of the unperturbed system when K = 0, i.e. with no transfer of charge. We do not need to know El and Er , but remark that the difference El − Er = −2eV is fixed by the potential difference V . We will take El = Er when K = 0, i.e. for a thick barrier. If we further choose the zero of energy to be midway between El and Er , we can share the potential energy difference between the two states symmetrically [55] by writing: ∂l = eV l + Kr ∂t ∂r i = −eV r + Kl ∂t i

(5.5) (5.6)

126

WEAK LINKS AND JOSEPHSON EFFECTS

The functions l and r may be written 1

1

l = ρl2 eiϕl ;

r = ρr2 eiϕr

(5.7)

i.e. each function is assumed to have a well-defined macroscopic phase, constant in space, and a well defined Cooper-pair density. This first limitation will have to be lifted later, but for the moment we can limit the discussion to a contact area that is very small, so that no spatial variation of ϕ is possible. We can now insert the wave functions with timedependent ρl and ρr into the differential equations (Eqs 5.5 and 5.6) and equate real and imaginary parts separately, a procedure which immediately leads to the following four relations, with γ ≡ ϕr − ϕl : K ∂ϕr =− ∂t ∂ϕl K =− ∂t

ρl ρr ρr ρl

1 2

cos γ +

eV

(5.8)

cos γ −

eV

(5.9)

1 2

1 2K ∂ρr =− (ρl ρr ) 2 sin γ ; ∂t

1 2K ∂ρl = (ρl ρr ) 2 sin γ ∂t

(5.10)

We note that variations of phase ϕ is due to the combined effects of the phase difference γ across the contact, and the potential difference V . Variations in pair density, on the other hand, are solely due to phase difference γ . The supercurrent across the contact is straightforwardly calculated by use of J = −2e

∂ρl ; ∂t

or

J = −2e

∂ρr ∂t

(5.11)

The time derivatives are already given above, so that we have: J =

1 4Ke (ρl ρr ) 2 sin γ

(5.12)

J = J0 sin γ

(5.13)

which we often rewrite as

a major result in the Josephson theory. It tells us that a supercurrent is driven across the thin barrier separating two superconductors simply by the superconducting phase difference across the barrier. The predictions from the theory outlined above have been extensively confirmed experimentally. An example of an IV-characteristic showing the DC Josephson current is seen in Figure 5.2. The data are from an S1 IS2 structure,

WEAK LINKS, PAIR TUNNELLING, AND JOSEPHSON EFFECTS

127

Figure 5.2 The I-V curve of a 0.7-µm square Nb/AlOx /Nb Josephson junction. The vertical scale is 20 µ A/div and the horizontal scale is 1 mV/div.[56]

with S1 = Nb and S2 = Pb. It shows the Josephson DC current at finite voltage which was discussed previously. Note that these measurements show the I-V curve for both positive and negative bias. The fact that a voltage is not needed to drive a supercurrent is something we already know well from the Meissner effect. In Chapter 6 we will find that the vector potential provides the driving mechanism. The Josephson effects established the phase of the wavefunction as a driving mechanism on equal footing with the vector potential, or magnetic field. The superconducting phase thereby took on a more firm and real existence. Observations of the corresponding physical effects followed, first few in numbers, then in abundance in the years after Josephson’s prediction. Superconductivity

Normalized current i

1.5

1

0.5

0

Figure 5.3

0

0.5 1 Normalized voltage, v

1.5

Quasiparticle current in intrinsic junction in Bi2 Sr2 CaCu2 O8 crystal [57].

128

WEAK LINKS AND JOSEPHSON EFFECTS 60

Current I (mA)

T = 68 K

0

−60 −0.15

0

0.15

Voltage (V)

Figure 5.4 I-V characteristic of (Pb0.2 Bi0.8 )2 Sr2 CaCu2 O8 crystal at T = 68 K showing intrinsic Josephson effect. After Kleiner et al. [58].

broadened its territory enormously by these discoveries, as mentioned before. In particular a range of unprecedented possibilities opened up in the area of electronic applications. An unusual realization of the Josephson effect was observed in a single crystal high-Tc superconductor Bi2 Sr2 Cu2 Cu3 O10 . This strongly anisotropic, layered structure consists of alternating superconducting CuO2 -layers separated by nonsuperconducting ones. The material can behave like a stack of SIN- and SISstructures. Hence, currents flowing along the c-axis normal to the layers have been observed, corresponding to either quasiparticle current or supercurrent, as seen in Figures 5.3 and 5.4 [57, 58].

5.2

AC Josephson effect

Josephson’s discovery included, however, another effect, one which even in hindsight may be seen as a surprising phenomenon an applied voltage across an junction would bring about an oscillatory variation of phase difference. We can find this fact from analysis of the time dependence of the phase difference by taking the difference between Eq. 5.8 and Eq. 5.9. This gives the Josephson frequency ωJ , when ρl = ρr , by ∂γ ∂ 2e = (ϕr − ϕl ) = ωJ = V ∂t ∂t

(5.14)

which is in an observable range, since V = 1 µV leads to fJ ≡ ωJ /2π = 483.6 MHz. We are speaking here of electromagnetic phenomena related to the movement of charge at elevated frequency: The Josephson contact emits electromagnetic radiation at the frequency ωJ .

AC JOSEPHSON EFFECT

129

Equation 5.14 for the Josephson frequency can be integrated to give the time dependence of the phase difference in zero magnetic field: γ = γ0 +

2e V t = γ 0 + ωJ t

(5.15)

Clearly then, as the Josephson current depends on sin γ , it will now be modified to J = J0 sin(γ0 + ωJ t)

(5.16)

It is this oscillatory Cooper-pair current which generates the microwave electromagnetic radiation. In the opposite case, when microwave radiation is incident )ωJ on the I-V curve. on the junction, steps appear at regular intervals Vn = n( 2e These steps, caused by absorption of n quanta of electromagnetic radiation at the Josephson frequency, are called Shapiro-steps after their discoverer. Figure 5.5 illustrates the I-V characteristic during illumination by electromagnetic radiation at ω = ωJ .

5.2.1

Alternative derivation of the AC Josephson effect

The simplified derivation of the AC Josephson effect did not explicitly bring out the role of the vector potential A, related to the B-field by ∇ × A = B. We therefore rederive the AC Josephson current in a manner which makes the role of A explicit. In so doing we have to use a gauge invariant form of the phase difference across the barrier. The necessity of doing this is seen in the PRF = 0

Voltage (µV)

600 300 0

PRF > 0

Increasing

4 Step number

3 2

2∆ In

1

−300 −600 I (arbitrary units)

Figure 5.5 Microwave-induced Shapiro steps in I-V curves of a Nb point contact Josephson junction at 4.2 K at different microwave power levels irradiating the junction at 72 GHz. I-V curves are shifted for clarity [59].

130

WEAK LINKS AND JOSEPHSON EFFECTS

GL-equations where the correct quantity to consider is ∇ϕ −

2e A

(5.17)

To bring out the phase difference between the two sides we integrate from left to right and get: γl→r

r r 2e 2π = A dl ∇ϕ − A dl = ∇ϕ − 0 l l

(5.18)

where it is understood that the integration starts on the left-hand side of the junction (see Figure 5.1a), at a point which is deeper than the penetration of magnetic field, and ends similarly on the right side. We have also inserted 0 for h/2e. Taking the vector potential Az (x) to be parallel to the direction of integration z, normal to the contact, corresponds to placing the B-field parallel to the contact plane, and pointing along the y-axis, with By (x) = ∂Az /∂x. On integrating we obtain γl→r

2π = (ϕr − ϕl ) − 0

r

Az dz

(5.19)

l

The phases ϕr and ϕl may be taken here to be fixed phases which exist in the absence of any AC current. Even though ϕ may not be well defined in the junctions, we may write the integral of the gradient as the difference between the endpoints and neglect a 2π × n contribution. When we take the time derivative z of this last relation we find, using Ez = − ∂A ∂t , r ∂Az ∂γ −1 −1 = −2π 0 dz = 2π 0 Ez dz = 2π −1 0 V ∂t ∂t l ∂γ 2e = V = ωJ as before. ∂t

(5.20) (5.21)

This derivation brings out explicitly the point that the AC Cooper-pair supercurrent across the contact is driven by a time-dependent vector potential, which again is created by a static electric field by the voltage V . A relevant question is now whether this current, being a Cooper-pair supercurrent, is lossless. A DC super-current can run forever as long as it is truly DC. But here, we are discussing time-dependent currents, i.e. accelerated mass and charge, and the process can only be sustained as long as we feed energy into the circuit. This will be the case in any super-current charge transport. In addition to this loss, observation shows that energy is radiated from the contact as a microwave electromagnetic field. Thus the Josephson effects are quite complex phenomena. The Shapiro steps (see Figure 5.5) in the I-V diagram

JOSEPHSON CURRENT IN A MAGNETIC FIELD

131

resulting from feeding microwave power into the contact is another manifestation of the energy exchange involving Cooper-pair super-current. More precisely, transfer of a Cooper-pair across the barrier costs an energy 2eV = ωJ , exactly the photon energy. Some of this energy is radiated, as mentioned.

5.3

Josephson current in a magnetic field

One of the truly remarkable and useful aspects of the Josephson contact comes about when its sensitivity to magnetic field is considered. Let the planar junction be placed in the xy-plane, with the magnetic field parallel to the y-axis. The GL-equations tells us that the DC supercurrent will be established according to ρe Js = (5.22) (∇ϕ − 2eA) m This current is the equivalent of the Meissner-effect according to London theory, but with the addition of a ∇ϕ driving term. Eq. 5.22 is easily rewritten as 2e m ∇ϕ = Js + A (5.23) 2e2 ρ Now choose an integration contour as shown in Figure 5.6, where the film thickness direction is along the z-axis, and the B-field along the + y-axis. We define the sum of length parameters λL + λR + δ = dJ . The length of the junction is L. Next, we perform an integration of Eq. 5.23 along the contours CL and CR in the superconductors, resulting in 2e m ϕRa (x) − ϕRb (x + δx) = A + 2 Js δl (5.24) CR 2e ρ 2e m A + 2 Js δl (5.25) ϕLb (x + δx) − ϕLa (x) = CL 2e ρ lR

lL CL

La

CR

Ra ∆x

L

By

x

Lb

z

Rb d dJ

Figure 5.6 A good choice of integration path.

132

WEAK LINKS AND JOSEPHSON EFFECTS

Now we exploit the following possibility: (i) The integration parallel to the junction may be performed so deep in the superconductor that screening current density is zero on both sides; (ii) that part of the integration which is done within the penetration depth of field and screening currents may be performed at right angles to that current. Figure 5.6 illustrates these two points. Forming now the phase difference ϕ(x + x) − ϕ(x) this can be achieved by manipulation of Eqs 5.24 and 5.25: ϕ(x + δx) − ϕ(x) ≡ ϕLb (x + δx) − ϕRb (x + δx) − ϕLa (x) − ϕRa (x) (5.26) 2e 2e ϕ(x + δx) − ϕ(x) = A · dl (5.27) A · dl + A · dl ≈ CL CR when we have taken λL + λR δ, which is a good approximation in most cases. Also the contribution from the two gaps will tend to be of opposite sign and equal size. Integration across the thickness δ can therefore be neglected. The result is that the phase difference across the barrier depends on x, as we get 2e ϕ(x + δx) − ϕ(x) = A · dl 2e = By (λR + λL + δ)δx = 2π −1 0 By dJ δx

(5.28)

which in integrated form becomes ϕ(x) = 2π −1 0 By dJ x + ϕ0

(5.29)

The shielding supercurrent density can now be written down using the standard Josephson relation Eq. 5.13. J = J0 sin(2π −1 0 By dJ x + ϕ0 ) 2π = J0 sin x + ϕ0 λϕ with λϕ =

(5.30)

0 By dJ

The interesting result is that the Josephson current across the barrier is a sinefunction, in other words varying in sign and amplitude along the direction perpendicular to the magnetic field, as illustrated in Figure 5.7. Looking at the whole pattern of super-currents in a Josephson junction in the presence of a magnetic field one recognizes the similarity with vortices

JOSEPHSON CURRENT IN A MAGNETIC FIELD

133

lj

Figure 5.7

A periodic pattern of supercurrent circulation in a Josephson junction.

penetrating a type II superconductor. In addition to the current crossing the barrier, charge conservation requires currents to flow along the contact in the direction transverse to tunnelling currents. This establishes a periodic pattern of supercurrent circulation, with the period λϕ defined previously (see Figure 5.7). The associated vortex patterns are called Josephson vortices. We note here that although similar to the usual vortices in type II superconductors, they are of a different nature since they have no normal core. Consequently, no upper critical field Hc2 is associated with the Josephson vortices. From Figure 5.7 one can immediately conclude (neglecting end effects) that a rectangular junction will obey a simple rule that the current is zero every time the relation L = nλϕ = n

0 By dJ

(5.31)

is satisfied, or at values of the magnetic field which obey: By = n

0 ; LdJ

n = 1, 2, 3 . . .

(5.32)

in other words every time an integral number of flux quanta is located in the junction. In case ϕ0 = 0 maximum current will appear at every field corresponding to the condition L = (n + 12 )λϕ

or

0 By = (n + 12 ) Ld ; J

n = 0, 1, 2 . . .

(5.33) (5.34)

The total current is found by integration of Eq. 5.30. Assuming we have a rectangular contact of area S = LW the current is found by integrating over the area S:

i λ2πϕ x−ϕ0 I = J0 sin ϕ(x)dS = e iJ0 e dS (5.35) S

S

where J0 is assumed to be constant, and dS = W dL

134

WEAK LINKS AND JOSEPHSON EFFECTS Ic

0

1

2

3

4

5

Φ Φ0

Figure 5.8 DC Josephson effect in magnetic field. Maximum zero-voltage current as a function of the magnetic flux.

The integration gives the following Josephson diffraction current: sin(π B /0 ) Imax = I0 (0) π B /0

(5.36)

Here we have removed a factor sin ϕ0 whose maximum is 1. Figure 5.8 shows a graph of I (B). Based on these results one can conclude that the principle for a sensitive detector of magnetic field has been established due to the sensitivity of the current in a Josephson junction to magnetic field. But the possible device described above is easily surpassed by a different design, which is far more sensitive. This is the SQUID, which we discuss next.

5.4

The SQUID principle

The SQUID (an acronym for superconducting quantum interference device), employs a design with two current paths in a loop-like structure. Current is fed into the loop on one side and collected on the other, in principle as sketched in Figure 5.9. In reality, the structure is usually made of flat layers of thin films, in a superconductor-insulating-superconductor sequence. Figure 5.9 can be thought of as a cross-section through such a structure. A complete contour is drawn inside the two superconductor branches, deep enough that we can regard the current as 2eA vanishingly small. In other words we assume: Js = ρe m (∇ϕ − ) = 0 which requires ∇ϕ = 2e A along the dashed contour C. We integrate this relation along C, and add also to this the integration across both junctions to make a complete closed contour, to obtain 2e (ϕr (a) − ϕl (a)) − (ϕr (b) − ϕl (b)) =

A · dl

(5.37a)

THE SQUID PRINCIPLE

135

a

I

l

r

I

Φ C

b

Figure 5.9

A double Josephson junction structure.

or 2e γa − γb =

A · dl =

2π 0

(5.37b)

where γa = ϕr (a) − ϕl (a); γb = ϕr (b) − ϕl (b). The total lumped current I can now be written as a sum of the currents across junction a and junction b:

resulting in

I = I0 sin(ϕr (a) − ϕl (a)) + I0 sin(ϕr (b) − ϕl (b))

(5.38a)

I = I0 sin γa + I0 sin γb

(5.38b)

π π sin γb + I = 2I0 cos 0 0

(5.38c)

by use of standard trigonometric relations for the addition of sine functions. The maximum current which the device can carry without dissipation is Imax = 2I0 | cos(π /0 )|

(5.39)

With this device a flux change B 0 can be detected. And since the area where the flux is felt by the SQUID (i.e. the whole loop) is much larger than the Josephson contact discussed previously, this shows that the SQUID can be many orders of magnitude more sensitive than a single contact in magnetic field measurements. This result is the basis for most applications of the SQUID. We shall return to that issue in Chapter 11. Calculation based on Eq. 5.39 for the resulting current through a two-point contact is illustrated in Figure 5.10. The flux introduced in the analysis above consists of two parts; the external flux e due to the applied magnetic field, and the flux LIscr due to screening currents Iscr in the loop with inductance L. In other words = e − LIscr

(5.40)

136

WEAK LINKS AND JOSEPHSON EFFECTS

Imax 2I0

1

0.5

0

1

2 Φ/Φ0

3

Figure 5.10 Maximum current which is possible to pass through a SQUID, as a function of the flux through it, measured in units of 0 .

Clearly, the maximum current Imax referred to previously is influenced by the presence of flux generated by screening currents, and the simple result given in Eq. 5.39 is strictly valid only when LIscr is negligible. In Chapter 11 we discuss the equations of motion for the DC SQUID in greater detail, and give references to extensive literature. A new and interesting development in SQUID physics and technology has taken place by the discovery of d-wave pairing in high-Tc cuprate superconductors. We recommend reading about the outstanding work described by Mannhart in the a topical contribution to this book, in Chapter 13.

5.5

The Ferrell–Prange equation

What happens to screening currents in a Josephson junction exposed to an external magnetic field? We now address this question, referring to Figure 5.11, a sketch of the situation we discuss. We recognize the main structure as that of a Josephson junction of length L in the x-direction and with an external field applied along the y-axis. In the presence of the applied B-field screening currents are generated. In the superconductor these penetrate to a usual depth λ. However, where the screening current crosses the insulator barrier, the density of Cooper-pairs is much lower than in the superconductor bulk or film. Hence the screening length is much larger in the junction. This length is usually called the Josephson penetration depth λJ . The previously defined lengths dJ and δ are also indicated in the figure. Our task is now to express λJ in terms of other known parameters. We can now repeat the procedure previously adopted, i.e. integrating the relation ∇ϕ = 2e A along a closed contour crossing the junction at distances dx like before. 2e γ (x + dx) − γ (x) = A · dl (5.41)

THE FERRELL–PRANGE EQUATION λ

137

dJ

λJ

B

δ

L

x

z

Figure 5.11 Illustration of geometries relevant to derivation of the Ferrel–Prange equation.

The right-hand side becomes 2e d 2e A · dl = d = 2π 0

(5.42)

where d is the flux enclosed within the contour, between the contour crossings at x and x + dx. The integration on the left side of Eq. 5.41 at x and x + dx leads to dγ = γ (x + dx) − γ (x) = 2π

d 0

(5.43)

in the same notation and by the same argument as before. We can write this as dγ 2π d = dx 0 dx

(5.44)

We can now introduce the magnetic field instead of the flux by observing that B=

d dJ dx

(5.45)

Introducing this into Eq. 5.44 gives us 2π dj d 2π dJ dγ = = B dx 0 dJ dx 0 0 dγ B= 2π dJ dx

(5.46)

138

WEAK LINKS AND JOSEPHSON EFFECTS

From Maxwell‘s equations we get the supercurrent density Js = ∇ × H = µ0 ∇ × B = µ0 dB dx along the z-axis. When this is inserted into Eq. 5.46 together with J = J0 sin γ we find: 2π J0 µ0 dJ d2 γ = sin γ 2 0 dx

(5.47)

1 d2 γ = 2 sin γ 2 dx λJ

(5.48)

which is usually written

This is the Ferrell–Prange equation [60] which predicts how the screening field penetrates into and parallel to the Josephson junction, with λJ =

0 2π dJ µ0 J0

1 2

(5.49)

When the phase difference γ is very small sin γ can be approximated by γ . In this case we get 1 d2 γ = 2γ 2 dx λJ

(5.50)

γ (x) = γ (0)e−x/λJ

(5.51)

which is easily solved as

Using this in the previously found relation for B, Eq. 5.46, we obtain B(x) = B(0)e−x/λJ

(5.52)

The Josephson penetration depth can be estimated on the basis of typical values for the parameters entering in Eq. 5.49. With J0 ∼ 102 A/cm2 and dJ ∼ 10−5 cm, one finds λJ ∼ 0.1 mm. The result is that λJ is much larger than λ, as we argued from the outset.

5.6

The critical field Hc1 of a Josephson junction

What field could we guess is required to force Josephson vortices into a Josephson junction using an external field? For this question we already have a relevant reference: The argument leading to an expression for Hc1 in bulk superconductors. In the bulk we expect Hc1 to be determined by distributing one quantum

JOSEPHSON VORTEX DYNAMICS

139

of flux 0 over the characteristic area for penetration of flux in the presence of the Meissner effect, i.e. π λ2 . This leads to the approximate expression Hc1 ≈ 0 /π λ2 in bulk superconductors. In the case of a Josephson junction there are two characteristic lengths, one along the junction, λJ , and one transverse to it, dJ , as introduced before. We should therefore expect Hc1 in the junction to be approximately given by Hc1 ≈

0 dJ λJ

(5.53)

which is indeed correct to within a numerical factor of order unity. The precise expression turns out to be Hc1 =

5.7

2 0 . π 2 dJ λJ

(5.54)

Josephson vortex dynamics

We have only discussed static vortices above. A lot of interesting physics is connected with dynamic phenomena, i.e. Josephson vortices in motion. Because of the fact that these do not have a normal core, as mentioned, they can move extremely rapidly and with minute losses within the junction. Vortex dynamics is described by the Sine–Gordon equation. In deriving the Josephson penetration depth λJ via the Ferrell–Prange equation we came close to this problem. One only needs to add a dynamic term to the equation, namely the acceleration 2 term ∂∂tγ2 to change the validity from that of a static to a dynamic description, resulting in ∂ 2γ ∂ 2γ 1 + = 2 sin γ ∂x 2 ∂t 2 λJ

(5.55)

The solution of this equation is solitary-like, i.e. representing the Josephson vortex as a solitary wave in a non-linear medium. Figure 5.12a shows the location of the vortex in the junction, and Figure 5.12b shows a representation of the solitary wave in more detail. This solitary wave moves along the junction with a speed close to that of the speed of light due to its low dissipation in the absence of a normal core. Moreover, high frequency radiation is generated from the junction as the solitons reach the surface in rapid succession. The solitary waves can be driven by a current source or a voltage source applied to the junction.

140

WEAK LINKS AND JOSEPHSON EFFECTS Φ0

ity

c Velo

x

z

By magnetic field

J supercurrent

y (a)

Figure 5.12

(b)

The Josephson vortex as a solitary wave. After Pedersen [61].

A practical problem arises in the use of these junctions as high-frequency radiation sources due to the great mismatch of impedance between the junction and the surrounding vacuum. This mismatch is caused by the difference in wave velocities. In the case of solitary wave analysis it is necessary to consider an extended or long junction, with a length L λJ . In a long junction one includes the effects of the self field in addition to the externally applied magnetic field. This corresponds to taking into account the screening currents in the SQUID, a possibility we already pointed out. For a general introduction to soliton physics in Josephson junctions, see reference [61].

5.8 Josephson plasma in cuprate high-Tc superconductors An interesting development related to the Josephson effects was the prediction [62] and observation by numerous groups, among them Matsuda and coworkers [63], of plasma effects in Bi2 Sr2 CaCu2 O8+δ . Neighbouring superconducting CuO2 layers are coupled by the Josephson effect through the block layers between the CuO2 layers, and the Josephson plasma is generated by the coupling between the Josephson current flowing along the c-axis and the electromagnetic field, leading to current oscillations at frequencies well below the superconducting gap frequency, in the GHz to THz range. Longitudinal and transverse plasma waves propagating along the c-axis and in the ab-plane are of quite different nature. These phenomena have already been developed to an advanced stage, and it has become possible to make devices that emit electromagnetic waves in the THz range. Another, related phenomenon is the interaction between the plasma and vortices. This leads to strong dependencies of the plasma frequencies on the state of the vortex matter created by an external magnetic field. Furthermore, the static interaction between pancake vortices and Josephson vortices has led to new insight into so-called crossing lattices of vortex matter.

6 London Approximation to Ginzburg–Landau Theory (|ψ| constant) 6.1 The London equation and the penetration depth λL 6.1.1

Early electrodynamics and the London hypothesis

Figure 6.1 describes an essential property of Meissner screening: The interior of a superconductor is shielded against a static magnetic field, a phenomenon we already discussed briefly in Chapter 1. We will now discuss the physics of this effect and its history. Already years before the discovery of Meissner screening, speculations had been made by Onnes among others, that the current in a superconductor might involve surface currents. The discovery made by Meissner and Ochsenfeld [3] in 1933 proved that this was correct, in the case of diamagnetic response to an external magnetic field. Logically the magnetic field could be expelled from the interior only by setting up a surface current. But the current could not exist only in the surface. It would have to penetrate to a certain depth called λ. If this were not so, a finite current should exist in a layer of zero thickness, which would imply an infinite density of free charge. Since there is of the order of one free charge pr metal atom, the penetration depth must be finite, and its length must be controlled by the free electron number density ne . The more electrons are present per volume, the more effective is the screening, and the shorter must λ be. The prediction for an electrodynamic screening length λ had already been made by de Haas Lorentz [64] in 1925. In modern SI units it reads 1 λ = (mq /µ0 ns q 2 ) 2 (6.1) where q is the charge of the carriers in the superconducting state, mq their mass, and ns their number density. This is the same formula that we use for screening Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

LONDON APPROXIMATION TO G–L THEORY

Penetrating field B(x)

142

Ba Bae−x/l l ~ 100−1000 nm

l Distance from surface, x

Figure 6.1

Meissner screening.

of a static magnetic field today. The prediction would give a penetration depth of about 50 nm in typical metals, a value which later has turned out to be in good agreement with observation. The derivation of the result for λ goes as follows: Near the surface of a superconductor an electric field can exist, accelerating the superconducting electrons frictionlessly according to mq v˙ = −qE

(6.2)

where, v is the carrier velocity and E the electric field. Time derivative is indicated by the dot. Since current density can be written as J = −ns qv this gives an expression for E: E=−

mq v˙ µ0 mq J˙ = = µ0 λ2 J˙ q µ0 ns q 2

(6.3)

Taking the curl on both sides we obtain ∇ × E − µ0 λ2 ∇ × J˙ = 0

(6.4)

Using ∇ × E = −B˙ we find µ0 λ2 ∇ × J˙ + B˙ = 0

(6.5)

Applying Maxwell’s equation ∇ × B = µ0 J leads to λ2 ∇ × ∇ × B˙ + B˙ = 0

(6.6)

˙ hence The first term is equal to −∇ 2 B, ∇ 2 B˙ =

1 ˙ B λ2

(6.7)

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

143

˙ from the surface towards the interior, The solution is an exponential decay of B over the characteristic distance λ Note that this is proposed as the electrodynamics of a superconductor. It is fundamentally different from the skin depth of a metal since we assumed frictionless motion of charge. Heinz and Fritz London [65] observed that on performing the time integration of Eq. 6.7 one is left with an equation between a static magnetic field B and a stationary current J , with an additional unknown integration constant. Setting the constant of integration equal to zero, they obtained B = −µ0 λ2L ∇ × J

(6.8)

Here we have renamed the parameter λ as λL . Equation 6.8 is the famous (second) London equation, which correctly describes the Meissner effect mathematically. Furthermore, on introducing the vector potential A via ∇ × A = B, we obtain the profound relationship between the vector potential and the supercurrent J =−

1 µ0 λ2L

A = −A

(6.9)

Notice that this equation is analogous to Ohm‘s law: J = σ E. Hence, in a superconductor exposed to a static magnetic field it is the vector potential A that drives a stationary supercurrent J . The factor is a response function, analogous to the conductivity σ in a normal metal. Although this equation seemed to express the Meissner effect correctly, and as such was a major achievement, its justification on microscopic grounds remained unknown since the London treatment is purely phenomenological. To justify the result from first principles remained a challenge for more than 20 years, until the famous BCS paper of 1957 [7]. In any case, the phenomenological basis for the important length parameter λL , the London penetration depth, had now been established and a prediction made for the screening length of a static B-field. It is mathematically the same parameter as was originally found by de Haas Lorentz, a fact which has gone largely unnoticed in the scientific literature. For completeness we repeat the simple steps leading to the Meissner effect as a consequence of the finite screening length λL for static magnetic fields. Our starting point is now the London Eq. 6.8, which we rewrite as B + λ2L ∇ × ∇ × B = 0

(6.10)

The simplest situation is the 1-dimensional case with the field applied parallel to the z-axis along the surface of a superconductor of long length along y, and with the x-axis measuring the distance from the surface into the superconductor, as already depicted in Figure 6.1. Equation 6.10 may be reformulated into B = λ2L ∇ 2 B

(6.11)

144

LONDON APPROXIMATION TO G–L THEORY

with the solution in the 1-dimensional case − λx

B(x) = Ba e

(6.12)

L

Ba is the externally applied induction field related to the applied field Ha by Ba = µ0 Ha . The solution of the London equation shows the significance of the parameter λL as the screening length over which the applied field is reduced to Ba /e. The length λL is mainly controlled by the superfluid density ns . BCS theory showed later that due to pairing of electrons the mass mq and charge q are twice that of the normal electron gas, and the full value of ns is half of the density n in the normal state. We could introduce factors of 2 in the mass, charge and particle density, but the end result is the same for λL . These factors cancel out, and the zero degree value of λL acquires the same value by either choice. In the case of pure metals the main variations in ns from one metal to another come from different valency. The typical values of the calculated λL lie in the range 40–50 nm in metallic superconductors such as Al, Sn and Pb. Because there is an effective mass involved, as well as different band structures, deviations from the ideal values are to be expected. In doped superconductors on the other hand, ns is of course determined by the doping level rather than by band structure effects. The solution (Eq. 6.12) precisely describes the Meissner effect: when an external static magnetic field is applied to a superconductor, supercurrents arise spontaneously in the surface layer to a characteristic depth λL so as to create an opposing field in the sample, exactly cancelling the applied field inside. It depends on the shape of the superconducting sample how the currents run, and whether the screening is complete or not (Figure 6.2). A partial deeper penetration of field will often occur, depending on the demagnetization factor of the sample with respect to the direction of the applied field. We refer back to Section 1.7 for a brief discussion of this point. Experimental values for the relative penetration depth λ were determined in Ref. [66] which reported on the temperature dependence of the quantity λ/λ0 where λ0 is the value near 0 K. It showed a steep descent of λ/λ0 below and

Js

Js

Js Ha Ha

Figure 6.2 field.

Ha

Some examples of sample shapes and screening currents in an external magnetic

145

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

away from the transition temperature Tc . This corresponded well with the two 2 fluid model of Gorter and Casimir [67], which would give λλ0 = 1−[T1/T ]4 . c These authors had introduced the idea that the electron gas in the superconducting state consists of a uniform mixture of two electron fluids, one being the normal component and having properties like in the normal state, the other one being the superfluid component observed only below Tc , and being responsible for the superconducting properties. In the two-fluid model they argued that a fraction w of superconducting electrons would condense into an ordered state, and vary from zero at T = Tc to unity at T = 0 according to 1 − (T /Tc )4 . When this was put into the expression for λ the experimentally observed behavior would result. Figure 6.3 shows data by Schawlow [68] confirming that this form even agrees well with BCS theory. After World War II, Pippard [69] performed measurement of the surface impedance of metals at radio-frequencies up to 1200 MHz. In the normal state the penetration is the familiar classical skin depth δ, which, upon passing below Tc becomes λ. The wave-vector dependence had not yet been sorted out; the possibility remained therefore that the measured λ could be different from the λL which had been predicted for the DC case. Even so, the data seemed in harmony with the predictions of the two-fluid model. Further measurements of λ in the presence of a static magnetic field led Pippard to propose the existence of a new length parameter, the superconducting coherence length ξ , which would cause the observed entropy change in pure tin at the superconducting transition to be distributed to a depth as much as 20 times the penetration depth λ. 1400 1200

− BCS theory Experimental data

dy

dl ˚ (A)

1000 800 600 400 200 0

1

2

3

4

5

1 y= √1 − t4

Figure 6.3 Early results on the temperature dependence of λ in a type I superconductor [68].

146

LONDON APPROXIMATION TO G–L THEORY

A decisive step was taken when Pippard showed that, contrary to the prediction of the London theory, λ depended very sensitively on impurity scattering. With the addition of only 3% indium to tin λ changed by a factor of 2, while at the same time the changes in Tc and Hc were insignificant. In the London theory λ depended only on m/n, offering no hint at an explanation. Figure 6.4 shows data demonstrating the effect of the mean free path l on penetration depth λ. Pippard realized that the key point was a breakdown of the underlying assumption of local response in the London theory. We shall return to Pippard’s analysis in Section 7.3.

6.1.2

Derivation of the London equation from the free energy

The London equation applies in the presence of a magnetic field, giving rise to both a kinetic energy density Fk and a magnetic energy density Fm . The superconductor is already at a temperature T < Tc when the London equation takes effect, so the total energy includes also the condensation energy density Fs . The total energy density F for the problem is found by integrating the three densities over the volume V : 3 3 F = Fs (r)d r + Fk (r)d r + Fm (r) d3 r (6.13) V

V

V

We may regard the condensation energy density as unaffected by the application of a magnetic field. Then Fs (r) d3 r = Fs may be regarded as a constant

106 l (cm)

10

5

10

20

30

40 106l (cm)

50

Figure 6.4 Pippard non-local behaviour as evidenced by mean free path dependent penetration depth. After J. Waldram, thesis 1961 [70] and Lynton, 1962 [71].

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

147

background term. The kinetic energy is

1 2 mv (r)ns d3 r Fk (r)d r = 2 s µ0 λ2L J 2 (r) d3 r = 2

Fk =

3

(6.14) (6.15)

which is obtained on writing J = −ns ev s . The magnetic energy is Fm =

Fm (r) d3 r =

1 2 b (r) d3 r 2µ0

(6.16)

In Eq. 6.16 we have introduced the vector b allowing it to represent local induction on a scale smaller than λL . For later treatment of the physics of the flux lines this allows a distinction between induction on scales larger than λL represented by B and on scales smaller than λL . Hereafter we write λ for λL . After combining all three terms, introducing b, and using the Maxwell equation µ0 J = ∇ × b we find F = Fs +

1 2µ0

λ2 (∇ × b(r))2 + b2 (r) d3 r

(6.17)

We want to vary b(r) an amount δb(r) and find the corresponding δF , i.e. we replace b(r) with b(r) + δb(r) and take the difference in F before and after the operation. The resulting δF to lowest order in δb is found to be 1 δF = 2µ0

2bδb + 2λ2 (∇ × b)(∇ × δb) d3 r

(6.18)

To obtain the condition under which the free energy is minimized we set δF = 0. We find that this requires b(r) + λ2 ∇ × ∇ × b(r) = 0

(6.19)

Here we have recovered the London equation. The physical meaning of the London equation is therefore to express the minimization condition for the free energy of the superconductor in the presence of a magnetic field. This is a result worth contemplating. It takes some of the mystery out of the London equation. There is a good, understandable reason for this equation, which was originally postulated without proof.

148

LONDON APPROXIMATION TO G–L THEORY

6.2 The energy of a single flux line Upon subjecting a type II superconductor to a field higher than Hc1 the Meissner screening breaks down, and individual flux quanta penetrate the superconductor. An important problem with regard to the physics of the vortex state, referred to as the mixed state between Bc1 and Bc2 , is the determination of the energy contents of a flux line. We will calculate this quantity as the energy per unit of length. We begin by deriving an expression for b(r), and then integrate the energy density associated with the field and currents in a flux line. The aim of the calculation will be to find, in the London approximation, the sum of kinetic and magnetic energies whose densities were already given in Eqs 6.15 and 6.16, respectively. The background energy Fs is of no interest in this context. We find F =

1 2µ0

b2 (r) + λ2 (∇ × b(r))2 d3 r

(6.20)

r>ξ

The limit of integration is a reminder that we cannot include the vortex core, of radius ξ , in this derivation because the London equation does not apply when ns varies in space. The justification for this approximation is that ξ λ in most type II superconductors, notably in all high-Tc materials. The energy associated with the vortex core is therefore quite small. The energy F is also often referred to as the line tension. It tells us how much energy is required to create extra length of flux line. Flux lines are not like rubber bands, there is no elastic energy associated with stretching a straight flux line. However, it does require extra length to bend a flux line in a superconductor, either uniformly or locally, and the energy per unit length required to achieve this elongation is the line tension. A practical way of approaching this problem was discovered by the Russian physicist Abrikosov1 (1957) [4, 5]. We replace the singularity inside r < ξ when we let ξ → 0 by a 2D delta-function δ2 (r). Let us first discuss that aspect. The London equation now takes the form: b + λ2 ∇ × ∇ × b = 0 δ2 (r)

(6.21)

Notice that higher order terms in δb in Eq. 6.18 are neglected. The deltafunction represents a solution where b(r) is not smooth. In Eq. 6.21 0 is a vector along the direction of the induction normal to the surface, where 0 is the flux associated with an area of radius |r| ∼ λ. 1 It was not immediately obvious that the approach of Abrikosov was correct. It is known that Landau rejected it when Abrikosov first presented it to him. This delayed the publication of Abrikosov’s theory by years. The consequences of Abrikosov’s idea were far-reaching, however, leading to the prediction of a flux line lattice, a truly remarkable result which was later to be confirmed experimentally.

THE ENERGY OF A SINGLE FLUX LINE

Integrating Eq. 6.21 immediately gives 2 b + λ ∇ × ∇ × b dσ = 0 × δ2 (r) dσ = 0

149

(6.22)

where dσ is a surface element, and we integrate over the plane perpendicular to the flux line. The last relation is obtained since 0 and dσ are parallel, and by the properties of the 2D delta-function. Next we carry out λ2 [∇ × (∇ × b)]dσ = λ2 (∇ × b)dl = λ2 µ0 J dl ≈ 0 (6.23) r=R

r=R

The last form approximates zero because we take the line integral at such large distance, R λ, that the current associated with the flux line vanishes. From Eq. 6.22 we are now left with a relation which determines the total flux associated with a single flux line: (6.24) bdσ = 0 We have proved that 0 is the flux associated with the local field b of a single flux line when ξ can be regarded as vanishingly small compared to λ. This corresponds to insisting that δ |ψ| = 0, which is the overall approximation made in the present chapter. We can now go back to solving (6.22) for the region ξ < r λ. We first rewrite it approximately as 2 bdσ + λ (∇ × b)dl = 0 (6.25) ξ ξ . This corresponds to a cut-off k⊥ < 1/ξ . The integration over kx and ky is simplified by transforming to polar coordinates. 2 1 F = 0 Lz 2µ0 2π

1 ξ

dk

0

2 1 = 0 2µ0 (2π )2

0

2π k 1 + λ2 k 2

λ2 ξ2

du 2π k 2λ2 k 1 + u

where

u = λ2 k 2

(6.99)

162

LONDON APPROXIMATION TO G–L THEORY

The final result is 20 F = ln κ Lz 4π µ0 λ2

κ=

λ ξ

(6.100)

The problem is now solved for the free energy per length of a straight flux line in the London approximation for the isotropic case.

6.5

Interaction between two parallel flux lines

We discuss next a simple application of the expression for the interaction energy between flux lines, specified to two parallel, straight flux lines along the z-axis, with flux line no 1 at r 1 = (x1 , y1, z1 ), and no 2 at r 2 = (x2 , y2 , z2 ), as shown in Figure 6.7. This is an important example, as it can be viewed as the beginning stage of studying the forces at work in the flux line lattice. We already derived the general energy expression we have to start from; which we now specify for two parallel flux lines: 2 U12 = 0 (6.101) dr 1 dr 2 V (r 1 − r 2 ) µ0 d3 k ei k (r 1 −r 2 ) (6.102) V (r 1 − r 2 ) = (2π )3 1 + λ2 k 2 V (r 1 − r 2 ) is the potential energy between two arbitrary line elements dr 1 and dr 2 , and is valid whatever configuration the two flux lines assume. Carrying out the integral (Eq. 6.102) gives V (r 1 − r 2 ) =

1 e−|r 1 −r 2 |/λ 1 e−r/λ = 2π λ2 r 2π λ2 |r 1 − r 2 |

(6.103)

FL2 FL1 dr2 r2 z (r2 − r1) r1

dr1

x

y

Figure 6.7 Coordinates used in calculating the interaction energy between two parallel, straight flux lines.

INTERACTION BETWEEN TWO PARALLEL FLUX LINES

163

This is essentially the well-known Yukawa potential. Since the vortices are ˆ dr 2 = dz2 kˆ where kˆ is a unit vector parallel to the z-axis, we have dr 1 = dz1 k; along the positive z-axis. We introduce for the distance |r 1 − r 2 | : 1 2 |r 1 − r 2 | = (x1 − x2 )2 + (y1 − y2 )2 + (z1 − z2 )2 1 1 2 2 2 = ρ 2 + (z1 − z2 )2 ≡ ρ 2 + z2

(6.104)

where z2 = z2 − z1 , and ρ 2 = (x1 + x2 )2 + (y1 − y2 )2 . Inserting this expression into the integrand of Eq. 6.101 results in

U12

2 = 0 µ0

∞ −∞

20 = 2π µ0 λ2

dz1

1 2 2

1 e−(ρ +z2 ) /λ dz2 × 2π λ2 (ρ 2 + z 2 ) −∞ ∞

2

2

∞

−∞

dz1

∞

−∞

dz2

1 −(ρ 2 +z 2 ) 2 /λ

e

(ρ 2 + z2 2 )

(6.105)

The integral over dz1 gives the length of vortex line no 1. We divide it over to the left-hand side and get the energy pr unit length U12 . The integral over z2 gives U12 =

ρ 20 K 0 λ 2π µ0 λ2

(6.106)

where ρ is the distance between the flux lines in the (x,y) plane, and K0 ( ρλ ) is a modified Bessel function. We find that the result can be written as the product of the flux 0 times the field h(ρ) at distance ρ. U12 = 0 h(ρ);

h(ρ) =

1 b(ρ) µ0

(6.107)

The total energy of two interacting, parallel flux lines is therefore: tot U12 = 2F + 0 h(ρ)

(6.108)

We can now find the force between the two filaments in the x-direction: f2,x = −

∂U12 ∂(2F ) ∂h(ρ) − = −0 ∂x2 ∂x2 ∂ρ

(6.109)

164

LONDON APPROXIMATION TO G–L THEORY

The interaction force is repulsive. If we introduce the current jy , by Maxwell‘s ∂ h, where jˆ is the unit vector along y, we find equation; j y = −jˆ ∂ρ f2,x = jy 0

(6.110)

We notice in particular that the force in the x-direction on a flux line is zero only when the superfluid current (and velocity) at that point is jˆy = 0. This corresponds well with the Lorentz force on a charge e, F = ev × B. The whole situation of two interacting vortices can be easily illustrated by letting the currents and fields of the two overlap. One finds repulsive interaction when the vortices are parallel, and attractive when they are anti-parallel as is also implied by the mathematical analysis. Interestingly, when two flux lines of opposite rotation are made to coincide, they annihilate, since the sum of all currents must everywhere be zero. Clearly, the situation of anti-parallel flux lines is an extremely unstable one. See also Chapter 8, Figure 8.1.

6.6

Interaction between two flux lines at angle α

In high-Tc materials the consensus is that a flux line liquid exists above a certain flux line lattice (FLL) melting temperature Tm . A situation, which has been predicted to exist between Tm and Tc (H ) is that of an entangled flux line fluid. The behaviour of this fluid will be quite dependent on whether the flux lines are stuck in their entanglement, or are able to disentangle and straighten out. The answer to this question should be sought in the flux-line–flux-line interaction energy. In the case of parallel flux lines there is distinct repulsion, as we have seen in Section 6.5. But in a liquid state we can envisage flux lines which are softly bending and interwoven between each other, as shown in Figure 6.8. The flux lines at positions of closest spatial approach interact at some angle α, which is different from one place to another. One interesting question which arises here

Figure 6.8 Flux lines in a rigid Abrikosov vortex lattice (left), and a putative entangled flux-line system in the molten phase (right).

INTERACTION BETWEEN TWO FLUX LINES AT ANGLE α FL1

165

FL2 z

d y

x

a

Figure 6.9 Coordinates for calculation of interaction between two flux lines at an angle α. Both flux lines are located in the (y, z)-plane, one displaced a distance d along the x-axis from the other. Hence the distance of closest approach is d. The angle they are splayed is denoted by α, in the present case the splaying is symmetric around the z-axis.

is the following: What is the energy cost of moving two nearly intersecting flux lines across each other to disentangle? This situation may be closely modeled by letting two flux lines be placed at a crossing angle α, like in Figure 6.9. To calculate the interaction energy we can again revert to the general formalism employed before. The difference between this case and the one treated in Section 6.5, is that the interacting line elements are at an angle α, and at a distance d, which means that the line elements dr 1 and dr 2 are at such angle, wherever their location is on line 1 and line 2. The integral to work out is now: dr 1 dr 2 V (r 1 − r 2 ) (6.111) U1,2 (α) = F L1

F L2

The integration over the variables in parallel position was carried out in Section 6.5. Taking advantage of that integration result, and inserting the cos α for the vector product of dr 1 × dr 2 , where |dr 2 | = dy/ sin α, and after dividing by the length of line 1 on both sides, we get 20 U1,2 (α, d) = 8π 2 λ2

∞

−∞

dy cos αK0 sin α

1

(d 2 + y 2 ) 2 λ

(6.112)

where K0 is again the same Bessel function encountered in Section 6.5. We find U1,2 (α, d) =

20 cot αe−|d|/λ 8π λ2

(6.113)

In fact, if we consider the fact that the systems also may be uniaxially anisotropic, then we may parametrize this in the London model by introducing two penetration

166

LONDON APPROXIMATION TO G–L THEORY

lengths, namely λab which is the penetration length in the (a, b)-plane ((x, y)plane) for a magnetic field oriented along the c-axis (z-axis), and λc which is the penetration length along the (a, b)-plane for a screening current along the c-axis. Eq. 6.112 then generalizes to U1,2 (α, d) =

20 −|d|/λab −|d|/λc − tan(α/2)e cot(α/2)e 4π λ2

(6.114)

as was shown by Sudbø and Brandt [77]. This is seen to reduce to Eq. 6.113 when λab = λc . Note how the angle at which flux lines do not interact (electromagnetically) in fact increases when the anisotropy ratio λc /λab increases. For the isotropic case, the interaction changes sign at α = π/2. When λc /λab → ∞, the interaction never changes sign, but approaches zero as α → π . The neutrality angle where the electromagnetic interaction between two rigid flux lines vanishes therefore increases with anisotropy.

6.7 General flux-line lattice elastic matrix in the London approximation As a final application of Eqs 6.83 and 6.91, let us use them to derive an expression for the general elastic fluctuation matrix of a flux-line lattice in an arbitrarily tilted external magnetic field, valid beyond the continuum approximation for the flux-line system. This means that we explicitly take into account the underlying Abrikosov lattice structure when deriving the fluctuation Hamiltonian for flux lines around their ground state configuration. The continuum approximation is a special case of the result we will derive, and as a byproduct we will obtain expression for the flux-line liquid elastic moduli in this limit when the external magnetic field is tilted an arbitrary angle with respect to the crystal c-axis. ˆ The exposition here closely follows that of Sardella [78] and Nguyen and Sudbø [76]. The starting point is Eq. 6.83 20 F = dr αi dr βj Vαβ (r i − r j ) 2µ0

(6.115)

ij

We now rewrite this by being slightly more explicit in writing the line integrals that are involved. The line integrals are along directed flux lines, the average direction of the flux lines is the z-axis, and hence we have dr αi = dz(dr αi /dz). We now insert this into Eq. 6.115 and obtain 20 drβj drαi F = Vαβ (r i (z) − r j (z )) dz dz 2µ0 dz dz ij

(6.116)

GENERAL FLUX-LINE LATTICE ELASTIC MATRIX

167

where the information on the shape of the flux lines is encoded in drβj /dz. We now imagine that the ground state of this system is the Abrikosov fluxline lattice, and expand the free energy in fluctuations around this ground state, keeping terms up to quadratic order in the displacements sj (z) around the ground state, where we have ri (z) = Rj + sj (z)

(6.117)

where Rj denotes the positions of flux lines in the ground state Abrikosov vortex lattice, and sj (z) denotes the fluctuations around these positions. The first thing to notice is that drβj (z)/dz = 1 if β = z, and drβj (z)/dz = dsj (z)/dz if β = (x, y). Let us now expand the tensor Vαβ (ri (z) − rj (z )) up to quadratic order in the displacements sj (z), obtaining Vαβ (ri (z) − rj (z )) = Vαβ (Ri − Rj ) + [si (z) − sj (z )]∇Vαβ (r)r=Ri −Rj 1 + [si (z) − sj (z )]n [si (z) − sj (z )]m 2 × ∇n ∇m Vαβ (r)r=Ri −Rj + . . .

(6.118)

Inserting this back into the expression for the energy, Eq. 6.116, we obtain, upon collecting terms up to quadratic order and noticing that terms that are linear by necessity must vanish since we are expanding around a minimum, we have for the elastic energy F = F − F0 , where F0 is the total energy of the ground state Abrikosov flux-line lattice (NB We must keep terms that are linear in displacements when expanding the tensor Vαβ (ri (z) − rj (z ))!) 20 dsαi dsβj F = Vαβ (Ri − R) dz dz 2µ0 dz dz ij

1 + [si (z) − sj (z )]n [si (z) − sj (z )]m ∇n ∇m Vαβ (r)r=Ri −Rj 2 dsαi [si (z) − sj (z )]β ∇β Vzα (r)r=Ri −Rj +2 (6.119) dz where (α, β) ∈ (x, y). The next step is to express this in terms of the Fouriermodes of the displacement vectors si (z). Now, because we are assuming an underlying Abrikosov lattice which gives rise to a Brillouin zone, the wavevectors of the displacement vectors are only defined up to an arbitrary reciprocal lattice vector Q. Hence, when we Fourier-expand the displacement vectors sj (z), we express the Fourier transform through a sum over reciprocal lattice vectors

168

LONDON APPROXIMATION TO G–L THEORY

Q of the Abrikosov vortex lattice and an integral over the wavevector k that runs over the first Brillouin zone. This means that we can write F =

1 sα (−k)αβ (k)sβ (k) 2

(6.120)

k

which defines the elastic matrix αβ (k). In the above expression, k runs over the first Brillouin zone. Such an expression is arrived at by partial integrations in Eq. 6.119, and then introducing the Fourier transforms of sj (z) as follows si (z) =

d3 k sβ (k) eikRi (2π )3

(6.121)

Moreover, because of the underlying Abrikosov flux-line lattice we must take into account that the wavevectors k are only defined up to reciprocal lattice vectors of the Abrikosov lattice, whence

eikRi = (2π )2

B δ2 (k − Q)eikz z 0

(6.122)

Q

i

where δ2 (k − Q) is a two-dimensional Dirac δ-function. Inserting all of this into Eq. 6.119, we find Eq. 6.120 with αβ (k) =

B2 fαβ (K) − fαβ (Q) 2µ0

(6.123)

Q

where we have introduced the function fαβ (k) = kz2 V˜αβ (k) + kα kβ V˜zz (k) − kz kβ V˜zα (k) − kz kα V˜zβ (k) (6.124) and where V˜αβ (k) is the Fourier transform of Eq. 6.91, namely V˜αβ (k) =

2 qα qβ 1 δαβ − 1 + 1 k 2 1 + 1 k 2 + 2 q 2

(6.125)

In Eq. 6.123, we introduced K = Q + k and moreover symmetrized the tensor fαβ (k). From Eq. 6.119, as it stands, we would have obtained fαβ (k) = kz2 V˜αβ (k) + kα kβ V˜zz (k) − 2kz kβ V˜zα (k)

(6.126)

However, for numerical purposes, when computing elastic modes of the flux-line lattice, it is often convenient to use the symmetrized form since it guarantees positive definite eigenvalues of the elastic matrix. The expression Eq. 6.123 is very useful, among other things it directly lends itself to a computation of the

GENERAL FLUX-LINE LATTICE ELASTIC MATRIX

169

elastic shear moduli of the Abrikosov flux-line lattice, of which there are several when the magnetic field is tilted away from the c-axis. ˆ The continuum limit of the elastic description of the Abrikosov flux-line lattice is obtained by omitting all terms in the sum over Q except Q = 0. Since the underlying lattice is not taken into account, this is basically an elastic description of a flux-line liquid, so the shear moduli are not accessible in this approximation. The bulk and tilt moduli are, however. Let us see how we can extract them from what we have derived above. In the flux-line liquid limit, taking only the Q = 0 terms and using that fαβ (k = 0) = 0, from Eqs 6.120 and 6.123 we simply have the elastic free energy given by F =

B2 sα (−k)fαβ (k)sβ (k) 2µ0

(6.127)

k

When the external magnetic field is tilted away from the c-axis ˆ by an angle θ we have four distinct elastic moduli of the flux-line liquid, such that the elastic description on symmetry grounds is given by the expression F =

1 ⊥ (k)(kz sx )2 + c44 (k)(kz sy )2 c11 (k)(ks)2 + c44 2 k +2c14 (k)(kz sx )(ks)

(6.128)

The elastic moduli that enter her can be obtained by comparing Eq. 6.128 with Eq. 6.127, and they are found to be given by Refs [73, 76, 78] ⊥ c44 (k) =

1 + [λ2ab + (λ2c − λ2ab ) sin2 θ ]k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

c44 (k) =

B2 1 2 2 4µ0 1 + λab k + (λ2c − λ2ab )q 2

c11 (k) =

1 + [λ2ab + (λ2c − λ2ab ) cos2 θ ]k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

c14 (k) =

(λ2c − λ2ab ) sin θ cos θ k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

(6.129)

⊥ (k) and c (k) are known as tilting moduli. Here, the set of moduli given by c44 44 When the flux lines on average are directed away from the symmetry c-axis, ˆ there appear two tilting moduli in the problem. The reason is that when the system is layered and the z-axis is tilted an angle θ away from the c-axis, ˆ we have a hard and a soft tilting mode depending on whether the tilting away from the z-axis is parallel to the crystal ab-plane, or out of the crystal ab-plane.

170

LONDON APPROXIMATION TO G–L THEORY

(Similar effects are present in the shear moduli of the flux-line lattice, which do not concern us here since we are considering the flux-line limit). Notice that for ⊥ (k) = c (k). The third of the four elastic moduli c (k) is θ = 0, we have c44 11 44 the bulk modulus, or compressional modulus, of the flux line liquid. The fourth of the elastic moduli, namely c14 (k) does not have a counterpart in an isotropic superconductor, nor in an anisotropic superconductor when the magnetic field is parallel to the c-axis. ˆ The new elastic modulus appearing is a mixed tiltand bulk-modulus, suggesting that in a tilted magnetic field, the elastic tilting and compressional modes of the flux-line liquid interact with each other. These mixed elastic moduli vanish in the limit when k → 0. (For the shear moduli, we have a similar situation. We get a hard and a soft shear mode, as well as a mixed shear-tilt mode). Note how all of the other elastic moduli, bulk as well as tilting moduli, take the value B 2 /µ0 when k = 0. Mass anisotropy is not seen at all in this socalled local limit. Moreover, the elastic properties of the flux-line liquid are oblivious to the value of λ (or κ) in the local limit. At finite k-vectors, the flux-line liquid softens considerably as the degree to which a superconductor is type II, increases. But the effect of mass anisotropy and the hardness of the superconductor (degree of type II) only influence the elastic properties of the flux-line lattice provided a non-local elastic theory is used. We shall come back to this point in Chapter 8, when we consider the Lindemann criterion for melting of the flux-line lattice.

7 Applications of Ginzburg–Landau Theory (|ψ| spatially varying) 7.1 The temperature-dependent order parameter |ψ(T )| As a first application of the Ginzburg–Landau (GL)-equations we derive the temperature dependence of the order parameter ψ. This can be done under the simplest possible conditions, with B = 0, and under homogeneous conditions ∇ψ = 0. The free energy now reduces to F (T ) = F0 (T ) + α |ψ|2 +

β |ψ|4 + · · · 2

(7.1)

Taking the derivative leads to the equilibrium condition δF = 0 ⇒ (α + β |ψ|2 ) |ψ| = 0 δ |ψ|

(7.2)

One solution is that |ψ| = 0, which is correct for the superconducting wavefunction above Tc . The other alternative is α + β|ψ|2 = 0. This gives α |ψ|2 = − (7.3) β Since α = α1 (T − Tc ) where α1 is a constant ,we find to a useful approximation, like in the magnetic case |ψ|2 =

α1 (Tc − T ) β

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

172

APPLICATIONS OF GL-THEORY 1 2

|Ψ|

|Ψ| ~ (Tc − T )

|Ψ| = 0

Tc

T

Figure 7.1 Temperature dependence of the order parameter |ψ|.

or |ψ| =

α1 β

1 2

1

(Tc − T ) 2

(7.4)

as sketched in Figure 7.1. Since the interpretation of |ψ|2 is that it represents the superfluid density ns , we have ns ∝ (Tc − T )

(7.5)

Some important remarks on the limitation of GL-theory are in order here. The last two results are both typical mean-field-like, a consequence of the tacit assumption of the GL-approach that fluctuations of ψ are to be neglected. In real cases, the temperature exponent 1/2 is good in the low-Tc materials, but not expected to hold in high-Tc materials. The difference comes from the properties we discussed in Section 2.6, that the coherence length is quite long in lowTc and quite short in high-Tc materials, making fluctuations important in the latter case. According to the results above, the superfluid density ns – corresponding to the density of Cooper-pairs – vanishes at Tc . Again, this mean-field like prediction is correct for long ξ , low Tc materials. In these the Cooper-pairs do start to condense at Tc , and the superfluid density ns and wavefunction ψ build up as the temperature is lowered below Tc . The lower the temperature, the more Cooper-pairs are created. However, again the situation does not prevail in high-Tc materials. It turns out that in those materials the wavefunction amplitude |ψ| is not zero above Tc . We return to these profound problems in Chapter 10.

7.2

The coherence length ξ

The coherence length ξ is a temperature-dependent as well as a materialdependent quantity. We will now demonstrate how it may be derived from

THE COHERENCE LENGTH ξ

173

the GL-theory, even without a magnetic field present. In this case the GL-I equation immediately becomes α(T )ψ + β |ψ|2 ψ +

1 (−i∇)2 ψ = 0. 2m

(7.6)

This is a differential equation for spatial variations of the order parameter. In geometries where 1D calculation may be used for simplicity, it reads −

2 d2 ψ + α(T )ψ + β |ψ|2 ψ = 0. 2m dx 2

(7.7)

On dividing through by the parameter α we observe that an operator defined 2 d2 in the first term of Eq. 7.7 must be dimensionless. Therefore, the as 2mα dx 2 quantity ξ defined by ξ≡

2 2mα(T )

12 (7.8)

must have the dimension of a length. Such a finding is significant, and suggests that this is to be understood as a characteristic length of the system. Indeed, this is the temperature-dependent GL coherence length ξ . Its temperature dependence is predicted to have the classical exponent ν = 1/2, according to 1 (T /Tc − 1)− 2 ; T > Tc (7.9) ξ(T ) = ξ0 1 (1 − T /Tc )− 2 ; T < Tc 1

where the length ξ0 is /(2mα1 Tc ) 2 . The length ξ(T ) is of fundamental importance in superconductivity, representing the coherence length of the wavefunction. We may regard this as the shortest distance over which the wavefunction is allowed to vary without generating pair breaking kinetic energy. We notice in particular the important aspect that ξ(T ) diverges towards Tc , from below as well as from above. This means that when the wavefunction is perturbed by for instance a magnetic field, or by normal inclusions in the superconductor, the length ξ(T ) is the healing length over which ψ recovers its full value. Clearly, this situation also exists when flux lines or vortices penetrate a type II superconductor, where, as we know, ψ → 0 at the centre. ξ(T ) is then the effective radius within which the Cooper-pair density is suppressed, a fact which allows the calculation of the energy cost of breaking the Cooper-pairs in a radius ξ around the vortex centre. A similar role is played by ξ(T ) at a superconducting to normal interface in the laminar structure of type I superconductors. Here ξ defines the wall thickness, quite analogous to domain walls in systems like ferromagnets, ferroelectrics, etc. All results of the GL-theory are purely phenomenological. The coefficients of the energy expansion, α1 ,β and c are unknown. However, they can be determined

174

APPLICATIONS OF GL-THEORY

by relating them to measurable quantities, like ξ , λ and Hc . The consistency of data taken by independent methods may then be checked, with the prospect of asserting the overall picture, as well as imposing a quantitative control on the expressed relations between experimentally determined quantities. The penetration depth λ is the other length parameter of particular importance in superconductivity. How can it be expressed by use of the GL-equations? Since λ is a measure of the depth of supercurrent response to a magnetic field, this suggests looking at the second GL-equation. In situations where the Cooper-pair density remains unperturbed, like when a magnetic field penetrates to depth λ in the Meissner state, we can simply neglect the gradient of ψ in GL-II. What remains is J =

e ∗ ψ (−2eA)ψ + c.c. m

=−

4e2 |ψ|2 A m

(7.10) (7.11)

From the London equation we have J = −(1/µ0 λ2 )A. This gives the relation 4e2 |ψ|2 = µ 1λ2 . Here we must have |ψ|2 = ns for consistency of these indepenm 0 dent derivations. The result clearly is in accord with the BCS-picture since it leads to the conclusion that λ2 =

m (2e)2 µ0 |ψ|2

(7.12)

This offers a somewhat more precise definition of the length λ, where 2e corresponds to the magnitude of the charge of a Cooper-pair, and m is the corresponding mass. By now we have obtained results for ξ and λ, and can also express the quantity κ = λ/ξ , which is of fundamental importance in superconductivity.

7.2.1

Relations between λ, ξ and Hc

So far we have used the GL free energy expansion and the GL-equations to gain insight into the characteristic lengths of the superconductor. Next, we look for relations between these and the important thermodynamic quantity Hc . We consider again a homogeneous superconductor in the absence of a magnetic field. The free energy is Fs (T ) = Fn (T ) + α |ψ|2 +

β |ψ|4 + · · · 2

(7.13)

TWO TYPES OF SUPERCONDUCTORS

175

Using |ψ|2 = − βα we find Fs (T ) = Fn (T ) −

α2 2β

(7.14)

This must agree with the difference in Gibbs’s energy between the normal and superconducting states derived in Chapter 1, hence µ0 2 α2 = H 2β 2 c

(7.15)

We can also find expressions for α and β from the preceding relations. Using µ0 Hc2 = −α |ψ|2 ;

α |ψ|2 = − ; β

and

−4e2 µ20 Hc2 1 = αm λ2

(7.16)

we find −4e2 µ20 Hc2 λ2 m

(7.17)

(4e2 )2 µ30 Hc2 λ4 α2 = µ0 Hc2 m2

(7.18)

α= and β=

By combining the equations containing Hc , ξ and λ we obtain the interesting result that Hc λξ =

0 √ 2π 2µ0

(7.19)

Since the right-hand side is a constant, we see that on varying the temperature, the three quantities Hc , λ and ξ are predicted to vary in such a way that their product remains fixed. Equally interesting and useful is the combination λ(T )ξ(T ) =

7.3

0 2π 2µ0 Hc (T ) √

(7.20)

Two types of superconductors

In complete analogy with Ohm’s law, J = σ E, which we pointed out is formally equivalent to the London equation, Pippard [69] adopted the corresponding

176

APPLICATIONS OF GL-THEORY

non-local version of Ohm’s law from Reuther and Sondheimer [79] for the so-called anomalous skin-effect, 3σ J = 4π l

r(r · E)e−r/ l 3 d r r4

(7.21)

Non-locality enters the problem when the response to a field can only be determined correctly by integrating over a volume of the size of l 3 (3D case), where l is comparable to or longer than the distance δ, the depth over which the E-field varies. Consequently, in the London equation ξ would have to be introduced whenever the coherence length ξ is greater than λ, since λ is the penetration distance of B whose vector potential drives the current. From experience in studies of the anomalous skin-effect in pure, normal metals Pippard saw the analogy for the superconductor in the simplest case to be J =−

ξ(l) A ξ0

(7.22)

where ξ0 is the value of ξ(l) in the limit of large l, i.e. for the pure case, and = (µ0 λ2L )−1 . Clearly, this equation predicts a reduced response when ξ(l) is reduced by impurities. Because experimentally λ is found to increase with decreasing l, ξ(l) must decrease as l decreases, as can be seen from Eq. 7.20. Eq. 7.22 can be viewed as one which applies when ξ λ, which we may call the London limit. It is also a limiting form of the general Pippard non-local relation, which he constructed on the basis of the combined insight from Eq. 7.22 and the Reuther–Sondheimer integral. The whole chain of arguments led Pippard to propose for superconductors, in complete analogy with the non-local response to an electric field in a normal metal 3 r(r · A)e−r/ξ 3 J =− d r (7.23) 4π ξ0 r4 where ξ(l)−1 = ξ0−1 + l −1 . Limiting cases which can be worked out are: λ = (ξ0 /ξ )λL √ 1 3 3 λ= ξ0 λ2L 2π

for

ξ λ

(London limit)

for

ξ λ

(Pippard limit)

where we used the symbol λL for the original London value of λ. These expressions have been verified experimentally. It is remarkable that the microscopic BCS theory [7] later confirmed the essential correctness of Pippard’s bold adaptation of non-local electrodynamics

TWO TYPES OF SUPERCONDUCTORS

177

from normal metals to superconductors. The BCS theory also gave an expression for the ξ0 -parameter: ξ0 = 0.18vF /kTc , where vF is the Fermi velocity, and k = 1.38 × 10−23 J /K is Boltzmann’s constant. Essentially the same answer is obtained using the uncertainty principle. In that case the idea is to relate the coherence length to the energy gap. The introduction of the coherence length lead to the extremely important distinction between two types of superconductors, i.e. those with ξ > λ versus those with ξ < λ, called type I and type II superconductors, respectively. A precise expression for this distinction is derived later in this chapter. At this point a semiquantitative, less stringent argument, proves the main point (see Figure 7.2). In both the parts of Figure 7.2 we are faced with a situation where a change takes place between a point at the origin, r = 0, where the normal state with B = Bc ends, followed by a region where superconductivity recovers over a distance ξ , while screening extends over the distance λ. We refer first to the left figure, where the situation is sketched from the NS-interface into the superconducting region. Here B(r) falls off from r = 0 according to B(r) = Bc e−r/λ . Next, the superconducting wavefunction is suppressed over a much wider range, i.e. over the coherence length ξ . The energy argument now goes as follows: To expel the magnetic field from the volume of the superconductor costs the energy 2µ1 0 Bc2 per volume. However, a volume equal to the product Aλ of laminar interface area A and penetration depth λ, is not screened against Ba , amounting to a total energy E1 = λA

1 2 B 2µ0 c

(7.24)

saved in setting up the laminar structure, compared to what it would cost to have a totally sharp boundary between normal and superconducting volumes, i.e. if λ = 0. On the other hand, the density of Cooper-pairs ns is suppressed since the proximity to the normal interface forces the superconducting wave-function ψ Type I

Type II B (r)

B (r)

l

NS interface

|y(r)|2

|y (r)|2

x

l x

Vortex center

Figure 7.2 Variations of magnetic field B and wavefunction ψ at the normal-superconducting interface.

178

APPLICATIONS OF GL-THEORY

to go to zero at the normal boundary where B = Bc . The distance over which ψ is suppressed from full equilibrium value ψ0 to zero, is precisely the length ξ that we introduced in Eq. 7.8. In the volume defined by the total laminar wall area times ξ , superconductivity is essentially destroyed. This costs an amount of energy corresponding to breaking the majority of Cooper-pairs in this volume, E2 = ξ A

1 2 B . 2µ0 c

(7.25)

So the net energy E gained by setting up the laminar walls is given by the difference E = E1 − E2 . For the situation to be stable E must be positive:

E = ξ A

1 2 1 1 2 Bc − λA Bc = ABc2 (ξ − λ) > 0 2µ0 2µ0 2µ0

(7.26)

We can regard this condition as the defining one for type I superconductivity, and note that it corresponds to the√simple statement that ξ > λ, not very different from the exact condition: κ < 1/ 2 to be shown later. The fact that the interface energy is positive in type I, makes the system want to establish as small an interface area as possible. It does so by setting up the laminar structure shown in Figure 7.3. We note from the picture that the lamina are not flat, but show a meandering structure as long as the field is directed normal to the flat sample surface. Experiments have shown that the laminar structure can be straightened out and stabilized by a magnetic field tilted in the plane of the laminar direction [80, 81], as sketched in Figure 7.4. With a flat geometry and a tilted field, as shown in Figure 7.4, the laminar structure acquires a thickness period where normal lamina thickness dn and superconducting lamina thickness ds add up to a total thickness d = ds + dn . In the normal lamina B is everywhere Bc , and in the superconducting lamina we take B = 0. Furthermore, if we assume that the lamina extend across a length L of a plate-like rectangular slab structure, there is a simple flux-conserving relationship between the laminar geometry, the thermodynamic field Bc and the applied field Ba . Conservation of total flux a applied to the specimen requires that a = Ba Ld = 0 × Lds + Bc Ldn ⇒ dn =

Ba a = d Bc L Bc

(7.27)

Here we have disregarded the small tilt of B a with respect to the surface normal. Since dn + ds = d we find also Ba Ba d + ds = d ⇒ ds = 1 − d (7.28) Bc Bc

TWO TYPES OF SUPERCONDUCTORS

179

Figure 7.3 Meandering laminar structure with alternating normal and superconducting regions, typical for type I superconductors with the magnetic field applied normal to a flat slab. From [82]. Reproduced with permission of the Royal Society.

Ba

dn

ds

d

L

Figure 7.4 Sketch of laminar structure in type I superconductor, straightened by tilting the applied magnetic field Ba [80].

180

APPLICATIONS OF GL-THEORY

This shows how the laminar thicknesses dn and ds vary with applied field and temperature through the dependences of ds and dn on Ba and Bc (T ). This result applies as long as the total d is a constant. Original work in this area was done by Landau [83, 84]. Next we discuss the second alternative, κ > 1. The energy argument we used before, pertaining to the interface energy, applies again, but due to the condition ξ < λ the energy E required to create the interface is now negative: 1 2 B A(ξ − λ) < 0 2µ0 c

(7.29)

√ So, to within a factor 1/ 2 as before, λ > ξ is the condition for type II superconductivity. Therefore now, the larger the interface area can be made, the more energy is gained. Can this go on without limit? Clearly no, because, as we have seen, flux is quantized in elementary units 0 = h/2e. This is how far the division of flux can and will go. These flux quanta are established by circulating superfluid currents, vortices of Cooper-pair flow that will go on forever once created, provided the temperature is held below Tc . Because of the smallness of the flux quantum, there will be a huge number of these in a finite field. A field of 1 T in a sample with 1 cm2 cross-section will cause the sample to be penetrated by more than 1011 vortices! We shall later study the physics of these in greater detail. As a consequence of ∇B = 0 we can immediately conclude that any such quantized vortex, once created, must extend continuously all the way through a homogeneous superconductor or form closed loops. The physics of vortices constitutes the central issue in the science of superconductivity in type II superconductors. We return to this subject in several later chapters of this book.

7.4 The structure of the vortex core In Chapter 6 we derived, as a byproduct of finding the line energy, the radial dependence of the local field from a vortex: 0 λ b= + b0 ln (7.30) r 2π λ2 This was obtained as an approximation when integrating curl b × dl for ξ < r λ. The rigorous result is r 0 b(r) = (7.31) K 0 λ 2π λ2 where K0 ( λr ) is a zero’th order Bessel function [72]. This form flattens the dependence on r within a radius ξ , the ‘hard core’. For convenience we repeat

181

THE STRUCTURE OF THE VORTEX CORE

the limiting forms: 0 λ b(r) = ln ; rλ 2 r 2π λ 1 0 π λ 2 −r/λ b(r) = e ; r λ 2 2r 2π λ

(7.32)

(7.33)

The structure of the vortex, therefore, is an inner volume of radius ξ where the field locally is high enough to destroy superconductivity by breaking most of the Cooper-pairs, i.e. ns approaches zero. This means also that the wavefunction ψ must likewise approach zero. It is equal to zero only at the centre. How can we prove that ns is so suppressed? Physically the upper critical field where the superconductor crosses over to the normal state, can be estimated by Bc2 ≈

0 πξ2

(7.34)

This implies that superconductivity is destroyed when the cores start to overlap. The reason why this leads to a normal state, is that at Bc2 cores with ns ≈ 0, overlap. This argument is also bears on ψ, since |ψ|2 = ns . Figure 7.5 shows a sketch of a cut through the vortices, represented by ns and b(x). Figure 7.6 b (x) ns = |y|2

x

Figure 7.5

Cut through the centre of neighbouring vortices, showing b(x) and |ψ|2 (x).

|y|2

Bc1 < B Bc . κ >

√1 2

2 . 2mξ 2

(7.42) √1 2

we have

is the exact condition for the appearance of a vortex phase

in type II superconductors. When κ < √1 we get Bc2 < Bc . In that case, as we 2 lower the field from above, we meet the Bc field before Bc2 . Here the Meissner effect sets in, and the mixed phase will not appear. We have type I behaviour. The importance of the value of κ = λ/ξ is apparent. We have two types of superconductors: κ

Bc when n = 0.

κ>

√1 : 2

type II with vortex state at Bc1 < B < Bc2

The laminar structure of field penetration in type I is amply documented. It occurs when an inhomogeneous field surrounds a sample with demagnetization factor n = 0. The field may then exceed Bc in some areas, and some flux is allowed to penetrate the sample in order to lower the total energy. On penetration, the laminar structure appears as the device by which the sample avoids being exposed to a field B > Bc anywhere. At this point it may be interesting to ask for an exact expression for Bc1 too. A rigorous argument, which avoids use of thermodynamics, and only relies on geometric consideration, disregarding any finite core effects, is the following. Bc1 is defined as the field at which the first vortex enters the

184

APPLICATIONS OF GL-THEORY

superconductor. That being so, let one flux quantum be in the superconductor at the field Bc1 . Let us for this purpose work in the London approximation where the normal core radius is set equal to zero. The flux quantum 0 is now allowed to occupy the whole specimen, the field being distributed according to the function e−r/λ . The critical field Bc1 at which one flux quantum has entered can then be computed by weighting each area dA = 2π r dr by the distribution function e−r/λ . The field is the total flux divided by effective area as follows: Bc1 =

∞

0 − λr

e

2π r dr

=

0 2π λ2

(7.43)

0

which is the exact answer in the London approximation with |ψ| constant.

7.5.2

Bc2 , ξ , and λ in anisotropic superconductors

So far we have discussed superconductivity in isotropic systems. However, for layered, highly anisotropic high-Tc compounds there is a need to develop methods to treat such cases. This is achieved by the Lawrence–Doniach (LD) theory [85, 86]. In a simple model picture, let us assume that the superconductor can be described by a state of alternating superconducting and insulating layers, of type SISISI, where S = superconductor and I = insulator, or SNSNSN, where N is a normal layer. In such systems, if the contact between S-layers is poor, the main charge transport between S-layers may take place by tunnelling, both for normal carriers and for Cooper-pairs. Among high-Tc materials the Bi-based compounds are good examples of such behaviour. In such a layered structure, let the x, y axes lie in the ab-plane, and the z-axis along the normal to the ab-plane. We will assume for simplicity that a- and b-axes are equivalent, corresponding to a tetragonal symmetry. In the high-Tc cuprates the orthorhombic structure is usually realized, but the distinction between a and b is far less significant than the difference between c and a, b. An immediate consequence is that the effective mass along a, b, called mab may be quite different than mc . In this situation the inverse mass appears as a tensor quantity in transport problems and in summing up energy terms. The free energy for a stack of superconducting planes with restricted contact between layers can be written down as

F =

n

1 d2 r α |ψn |2 + β |ψn |4 2 2 ∂ψn 2 ∂ψn 2 2 + + + ∂y 2mab ∂x 2mc

∂ψn 2 ∂z

(7.44)

THE LENGTH ξ AND THE UPPER CRITICAL FIELD Bc2

185

The summation is over all planes, and integration is in each plane, in two dimensions. The distinction between the ab- and c-directions is most manifest in the coherence length, which is often much shorter in the c-direction than in the ab-plane, even shorter than the S-S-plane distance s in high-Tc cuprates. Here one may choose to discretize the last derivative in extreme cases of layeredness. This term would take the form 2 |ψn − ψn−1 |2 2mc s 2

(7.45)

and by the summation, each layer n will be found to interact with one nearest neighbour on each side. On writing ψn = |ψn |eiϕn , and ψn−1 = |ψn |eiϕn−1 assuming identical layers, one finds by insertion in Eq. 7.44 that the energy for two adjacent planes is 2 |ψn |2 (1 − cos(ϕn − ϕn−1 )) mc s 2

(7.46)

This expression bears a striking resemblance to the Josephson coupling energy1 , as it ought to since the physics is the same when charge transport between layers takes place by tunnelling. On the other hand, in case we stick with the continuum version of derivation even along z, within some distance from Tc , due to the divergence of ξ(T ) we can instead use the continuum GL-equation found before, ↔−1 but with the modification that inverse mass is now a tensor expressed as m ; i = a, b, c. The only change from the isotropic case, is that we have to write the product of the kinetic operator and the inverse mass tensor in a new form. ↔−1 As the kinetic operator is squared, the way to write the product is to place m between the two operators. The GL-equation for the anisotropic, continuous case is called the LD-equation and now reads 2 αψ + β |ψ| ψ − 2 2

2e 2e ↔−1 ∇−i A · m · ∇−i A ψ =0

(7.47)

The inverse mass tensor has principal values: m1ab , m1ab , m1c . The anisotropy encountered here is extremely important in the high-Tc cuprates, and its consequences must be dealt with realistically in any serious approach. We immediately come upon this fundamental issue in the description of the coherence length, ξ . Clearly, we now have to write the relationship 1 The Josephson coupling energy expresses the energy stored in the junction, and can be determined by

up the electrical work which the current source does in changing the phase ϕ, i.e. by

integrating Is V dt = Is (/2e)d( ϕ).

186

APPLICATIONS OF GL-THEORY

between ξ and the parameter α in a new form, with corresponding labels i on ξ and m: 2 ξi2 = (7.48) 2mi α(T ) And since ξi is anisotropic, so is λi as expressed by 0 ξab λab = ξc λc = ξi λi = √ 2 2π Bc

(7.49)

Thermodynamic quantities like Bc , of course, should have no anisotropy label. The inverse relationship between ξi and λi is noteworthy. Remembering that the index i on ξi represents the direction of the corresponding axis and the direction of movement of the mass mi , the index i on λi takes a different meaning: It refers to supercurrent shielding by currents flowing in the plane normal to the i-th axis. The anisotropy was introduced above through the masses mi , and these are different by a factor of the order of 10 in high-Tc compounds. The lattice anisotropy has a direct influence on masses mi , and via the mass it propagates to all other directionally distinguishable quantities. One other notable consequence is in the critical fields, where we now have c

Bc2 =

0 2 2π ξab

;

ab

Bc2 =

0 2π ξab ξc

(7.50)

The reason why we have to divide by the product ξab ξc in the second case is that the currents defining the vortices and flux lines flow around the axis lying in the ab-plane and therefore flow both in the ab-plane and in the c-direction. c ab Since ξab ξc we get Bc2 < Bc2 . To summarize, the anisotropy factor γ can be written as 1 ab Bc2 ξab λc mc 2 = = = c (7.51) γ ≡ mab ξc λab B c2

An illustration of the definitions of the length parameters λ and ξ in anisotropic superconductors of the type discussed above is given in Figure 7.7. In Figure 7.8 we have illustrated how the vortices created in a layered superconductor are broken up into a stack of ‘pancakes’. When the field is tilted, the pancakes are connected by horizontal Josephson vortices, shown in the figure only as horizontal lines. An important distinction is the fact that pancakes have a normal core, while the Josephson vortices have no such core. To study Hc2 , or Bc2 in the strongly anisotropic case we return to the discretised version Eq. 7.45, but with appropriate terms included to allow a magnetic field through a vector potential A. We choose to let Az = Bx, where B is along the y-axis, in the ab-plane.

THE LENGTH ξ AND THE UPPER CRITICAL FIELD Bc2

187

z

lb xc y

xb

lc

Figure 7.7 Sketch of a vortex of elliptical cross section aligned parallel to the a axis in an anisotropic superconductor described by the anisotropic Ginzburg–Landau theory.

(a)

(b)

(c)

Figure 7.8 Stacks of 2D pancake vortices: (a) straight stack, the configuration of lowest energy at zero temperature, and (b) disordered stack, which occurs at higher temperatures. (c) Sketch of a tilted stack of pancake vortices in successive superconducting layers, connected by interlayer Josephson strings.

We will now express the contribution to the LD-equation in the n’th superconducting plane by the continuous model as 2 αψn + β |ψn | ψn − 2mab 2

2 2e ∇ − i A ψn

(7.52)

A contribution must be added here to include the effect of coupling to planes n − 1 and n + 1. Since ψn has neighbours ψn−1 and ψn+1 the phases relative to these with respect to the phase of ψn must be expressed explicitly. The three terms in the summation over three planes ψn+1 , ψn , ψn−1 must be modified to take account of the phase contribution from the vector potential A. The phase difference to look for is indicated by the second term in the operator (∇ − i 2e A). 2e Here i A is equivalent to the derivative of the phase difference, so it must be multiplied by the distances between planes to give the phase difference.

188

APPLICATIONS OF GL-THEORY

And finally, the difference between wave functions on the corresponding two neighbouring planes has to be divided by s 2 to give the discretized second derivative. Upon adding these terms to those written down before, recalling also the direction of the field we have chosen, we find αψn + β |ψn |2 ψn − −

2 ∇ 2 ψn 2mab x,y

2ieA s 2ieAz s 2 − z e − 2ψ − ψ e ψ =0 n+1 n n−1 2mc s 2

(7.53)

This equation can be simplified enormously by linearization, i.e. by removing β |ψn |2z ψn , and by having A = (0, 0, Az ), and finally by writing the last parenthesis in the form of a coupling energy. Also, here again we make the perfectly reasonable assumption that all superconducting planes are physically equivalent. We can now omit the index n on the various ψ-functions. We find 2 ∂ 2 ψ 2 2eAz s αψ − − ψ =0 (7.54) 1 − cos 2mab ∂x 2 2mc s 2 Inserting the expression α =

2 2 mab ξab

and Az = Bx, and expanding the cos-func-

tion for small argument, corresponding to small s we find the equation d2 ψ mab 2π Bx 2 1 + − 2 ψ =0 (7.55) mc 0 dx 2 ξab (T ) Using a trial solution of the form ψ = eiky y eikz z f (x) one finds Bc2 =

0 2π ξab ξc

(7.56)

7.6 Ginzburg–Landau–Abrikosov (GLA) predictions for Bc2 /Bc1 The most important parameters to be determined by measurements in type II superconductors are the lower and upper critical fields, Bc1 and Bc2 , and the ratio κ = λ/ξ . Difficulties were always connected with the determination of the lower critical field Bc1 , because of the presence of pinning, which can mask completely the predicted sharp drop in the magnetization at Bc1 . Therefore, experimental data on Bc1 are often quite uncertain. The test of consistency with GLA theory is usually to compare data according to the relation (Bc1 Bc2 )1/2 /Bc = ln κ. Due to the ln κ factor, this is a quite insensitive test of the consistency of data on

GINZBURG–LANDAU–ABRIKOSOV (GLA) PREDICTIONS FOR Bc2 /Bc1

189

critical fields and κ. A much more sensitive test can be made by taking the ratio of critical fields Bc1 and Bc2 rather than their product, as we will now show. By deriving the well-known formula for Bc1 Bc1 =

0 (ln κ + ε) 4π λ2

(7.57)

one has in reality derived the κ-dependence of the ratio Bc2 /Bc1 , or the inverse thereof. This is easily shown by writing Bc1 in the form Bc1 =

0 (ln(λ/ξ ) + ε) 2 2π ξ 2λ2 /ξ 2

=

0 (ln κ + ε) (ln κ + ε) = Bc2 (7.58) 2 2 2π ξ 2κ 2κ 2

We define the function K(κ) by the relation 2κ 2 Bc2 ≡ K(κ) = Bc1 (ln κ + ε)

(7.59)

Taking the first and second derivatives of K(κ) one finds this function to have a minimum, occurring at a κ-value κe1/2−ε . In order to carry out a test procedure, we need to distinguish between isotropic systems, where Eqs 7.57, 7.58 and 7.59 are the predictions, and layered structures as in the high-Tc cuprate materials. The results are remarkably simple [12]: The K(κ)-functions have precisely the same form as in Eqs 7.58 and 7.59. With the field along the c -axis one obtains c c Bc2 /Bc1 =

2κc2 ≡ K(κc ); (ln κc + ε)

κc = λab /ξab

(7.60)

With the field in the ab-plane we get ab ab Bc2 /Bc1

2 2κab ≡ K(κab ); = (ln κab + ε)

κab

λab λc = ξab ξc

12 (7.61)

We then have K(κ) = K(κc ) = K(κab ) = 2κ 2 /(ln κ + ε)

(7.62)

Therefore, in all these cases the same maximum of Bc2 /Bc1 is predicted to exist, given by the criterion κ = e1/2−ε . Data in the literature on independent measurements of all parameters Bc1 , Bc2 , λ, and ξ turn out to be rather scarce. It is common practice to use the GLArelations to calculate for instance the coherence length on the basis of a measurement of Bc2 , using the relation we have found in Section 7.5.1. Figure 7.9 shows a plot of the function K(κ) given in Eq. 7.62.

190

APPLICATIONS OF GL-THEORY

10−1

K −1 (k)

10−2

10−3

10−4

1

10

100

k

Figure 7.9 = 0.13.

The function K −1 (κ) = Bc1 /Bc2 derived in Eq. 7.62 from GLA theory, with

GLA theory has been an enormously powerful tool by which to work out the physics of the vortex state of superconductors, even well beyond the limits of expected applicability.

7.7 Surface superconductivity and Bc3 So far our treatment of the Ginzburg-Landau equations at the mean-field level has not taken into account the surface of the sample. It has been implicitly assumed that we are working in the bulk. At the surface of the superconductor, however, some additional boundary conditions need to be imposed on the solutions, since one can quite reasonably expect the presence of an interface between the superconductor an a non-superconducting material such as a normal metal or an insulating material, to affect the nucleation of superconductivity in the material. For the purposes of studying the nucleation (i.e. onset) of superconductivity, it suffices to consider the linearized version of the first Ginzburg-Landau equation, namely

or equivalently

1 (−i∇ − 2eA)2 ψ = −αψ 2m

(7.63)

2 2mα 1 2e −i∇ − A ψ = − 2 ψ ≡ 2 ψ ξ

(7.64)

SURFACE SUPERCONDUCTIVITY AND Bc3

191

where we have introduced the characteristic length ξ2 ≡ −

2 2mα

(7.65)

We now make a couple of simplifying assumptions. a) We consider ξ to be small compared to the bulk dimension of the sample. b) We assume that the surface is such that the local radii of curvature of the boundaries are large compared to ξ . This allows us to consider the problem of a plane boundary. We first take the external magnetic field to be parallel to the surface, which is located in the (y, z )-plane, with magnetic field B = B zˆ . The superconducting sample is located in the half-space x > 0, while we take the non-superconducting material to be located in the half-space x < 0. The latter material is here chosen to be either vacuum or an insulating material, we will only briefly consider the case of a metallic coating of the superconductor, where the boundary conditions to be imposed are different. Then, the boundary condition to be imposed is that the component of the gauge-invariant supercurrent normal to the surface is zero, i.e. ∂ −i − 2eAx ψ|x=0 = 0 (7.66) ∂x We choose to work in the gauge A = Bx yˆ and look for a solution to equation of the form ψ = f (x)eiky

(7.67)

Inserting this Ansatz into the GL-equation and the boundary condition we find −

2 d2 f 1 (k − 2eBx)2 f = −αf + 2 2m dx 2m

(7.68)

with the constraints that df/dx = 0 for x = 0 and x = ∞. The above equation is the Schr¨odinger equation for a harmonic oscillator with frequency ω=

2eB m

(7.69)

and with a minimum of the quadratic potential located at X0 =

k 2eB

(7.70)

The complication arises because the boundary condition states that the solution must be flat at a position x = 0 while the minimum of the potential is located at x = X0 . If X0 = ∞ or X0 = 0, this is simple, because when the minimum of

192

APPLICATIONS OF GL-THEORY

the potential is located very far from the surface (X0 = ∞) we can ignore the boundary condition, and when X0 = 0 the boundary condition is satisfied by the standard solution to the Schr¨odinger equation in terms of a Gaussian multiplied by Hermite polynomials with Eigenvalues 2eB 1 1 = n+ ; n = 0, 1, 2, . . . (7.71) −α = ω n + 2 m 2 The lowest Eigenvalue for these two cases (X0 = (0, ∞)) quite clearly corresponds to the case where nucleation of superconductivity is energetically most favourable (for X0 = (0, ∞)), and corresponds to 2eB 1 2 = −α = m 2 2mξ 2 (h/2e) 0 B= = = = Bc2 2eξ 2 2π ξ 2 2π ξ 2

(7.72)

Hence, we rederive the well-known result that when the surface of the boundary does not constitute a complicating factor in the GL equations (which happens deep in the specimen or right at the surface) then superconductivity is nucleated at the upper critical magnetic field Bc2 . (But note that this type of sharp onset of superconductivity at a sharply defined field is an artifact of mean-field theory! In reality, Bc2 is a crossover line). Hence, we reach the conclusion that the surface has consequences for the solution to the GL equations only at intermediate values of X0 . Let us first see precisely what we mean by this statement. We start by considering the lowest energy solution for X0 very large, which is given by the well-known harmonic oscillator function for n = 0, namely mω (x − X0 )2 f (x) = A exp − 2 x − X0 2 = A exp − (7.73) ξ Thus, we see that the solution is located within a distance ξ of the position X0 . Hence, we conclude that within a sheeth of thickness ξ of the surface of the sample, nucleation of superconductivity is altered by the presence of a surface. We must now think of the Schr¨odinger equation −

2 d2 f 1 (k − 2eBx)2 f = −α(X0 )f + 2 2m dx 2m

(7.74)

as en Eigenvalue problem where the Eigenvalue is X0 -dependent, and our task is to minimize this with respect to X0 subject to the boundary condition on f at the

SURFACE SUPERCONDUCTIVITY AND Bc3

193

surface. This may in principle be done by writing down the general solution to this equation in terms of a linear combination of two degenerate hypergeometric functions, finding the expansion coefficients from the boundary conditions at the surface and at infinity, thus determining the lowest eigenvalue. This requires numerical work. We proceed by a different analytical method which yields the correct answer to within 2%. We start by rewriting the equation as mω 2 d2 f 2mα(X0 ) + (x − X0 )2 f = − f (7.75) 2 dx 2 √ √ Introducing z = mω/x, z0 = mω/X0 , and β = −2α/ω, we find −

−

d2 f + (z − z0 )2 f = βf dz2

(7.76)

where the task now is to find the lowest possible value of β subject to the boundary conditions df/dz = 0 at z = (0, ∞). This problem may be phrased as the following variational problem of minimizing the functional ∞ 2 df 2 2 dx + (z − z0 ) f dz 0 ∞ β= (7.77) dxf 2 0

with respect to variations in f. The Euler-Lagrange equation for this variational problem is precisely the above scaled differential equation. To do the minimization, we use a trial wavefunction of a form similar to the lowest eigenvalue state of the harmonic oscillator, but now shifted with respect to the minimum of the oscillator potential 1 2 f = exp − bz (7.78) 2 which we note satisfies the correct boundary conditions. It is a simple matter to perform the necessary integrals, and we obtain β=

1 2z0 b + −√ + z02 2 2b πb

(7.79)

This is now to be minimized with respect to b, which yields b in terms of z0 . This particular value of b is then to be substituted back in the expression for β, which then is minimized with respect to z0 . One may just as well do the minimization in reverse order, first minimize with respect to z0 and then with respect to b. We choose the latter. 2 ∂β + 2z0 = 0 = −√ ∂z0 πb

(7.80)

194

APPLICATIONS OF GL-THEORY

√ yielding z0 = 1/ π b. Substituting this back in β and minimizing with respect to b, we find ∂β 1 1 1 = − 2+ =0 ∂b 2 2b π b2 which yields b =

√

1 − 2/π . Substituting this back into β yields 2 βmin = 1 − π

(7.81)

(7.82)

We now go back to the definition of β = −2α/(ω), and reintroduce the characteristic length 1/ξ 2 = −2mα/2 as well as the frequency ω = 2eB/m to find 2 h/2e Bc2 (7.83) = = βmin = 1 − = 2 2 π B 2eBξ 2π ξ B Hence, we find that in the presence of a surface, i.e. when nucleation of superconductivity occurs within a length ξ from the surface plane, the upper critical field at which it starts to nucleate as the field is lowered from above, is given by 1 B = Bc3 = √ Bc2 = 1.66Bc2 1 − 2/π

(7.84)

A more careful numerical analysis based on hypergeometric functions yields the slightly larger value for the surface nucleation field Bc3 = 1.69Bc2

(7.85)

We see that our analytical estimate is in excellent agreement with this, differing by less than 2%. It is straightforward, but a bit tedious, to obtain essentially perfect agreement with the numerical result if we use a slightly refined variational function f (x) = (1 + cz2 ) exp(−bz2 /2). Physically, the boundary condition df/dx = 0; x = 0 means that the order parameter ψ is enhanced at the surface, since the solution to the problem ignoring boundary conditions has a negative derivative. Thus, we may view this as pinning of Cooper-pairs to the surface of the sample. We should, however, be cautious about regarding Bc3 as some sort of critical field, it is after all a surface phenomena we are talking about, and superconductivity with long-range order in the superconducting order parameter does not exist at any finite temperature in two dimensions, as we shall see in Chapter 9. Moreover, as the above results show, Bc3 is tied to the notion of the bulk upper critical field Bc2 , which itself is not a critical field either, but rather defines a crossover line. Bc3 is therefore best thought of as a surface enhanced crossover line where one sees the first nucleations of locally superconducting islands in the system. The main point

SURFACE SUPERCONDUCTIVITY AND Bc3

195

about the above results, is that when superconductivity occurs in a system, it tends to nucleate at the surface of an ideal (defect-free) sample, not in the interior of it. Alternatively, if we have material defects in the interior of the system, superconductivity may nucleate in the vicinity of such defects as well. Let us also consider the case of an inclined magnetic field with respect to the sample surface. We imagine tilting the field in the (x, z ) plane and angle θ with respect to the sample surface located in the (y, z )-plane. hence we have B = B cos(θ )ˆz + B sin(θ )xˆ

(7.86)

We now work in a gauge such that the vector potential is given by A = B[x cos(θ ) − z sin(θ )]yˆ

(7.87)

The first Ginzburg-Landau equation now becomes 2 2 ∂ 2 ψ ∂ 2eB 2 ∂ 2 ψ 2 − i + [x cos(θ ) − y sin(θ )] ψ = −αψ − + 2m ∂x 2 2m ∂z2 2m ∂y (7.88) √ 2 2 Again, introducing √ √ 1/ξ = −2mα/ and new coordinates ζ = mω/x, η = mω/y, ρ = mω/z with ω = 2eB/m, and defining β = −2α/(ω) the equation may be written on the form 2 ∂ 2ψ ∂ 2ψ ∂ − 2 − + [ζ cos(θ ) − ρ sin(θ )] ψ = βψ + i ∂η ∂ζ ∂ρ 2

(7.89)

We now try a solution of the form ψ(ζ, η, ρ) = g(ζ, ρ) exp[iζ0 η]

(7.90)

and obtain the following differential equation −

∂ 2g ∂ 2g − 2 + [ζ cos(θ ) − ζ0 − ρ sin(θ )]2 g = βg ∂ζ 2 ∂ρ

(7.91)

This equation is the Euler-Lagrange equation for the variational problem of minimizing the following functional 2 2

∞ ∞ ∂g ∂g 2 2 + ∂ρ + (ζ cos(θ ) − ζ0 − ρ sin(θ )) g 0 dζ −∞ dρ ∂ζ

∞ ∞ β= 2 0 dζ −∞ dρg (7.92)

196

APPLICATIONS OF GL-THEORY

Here, we follow the strategy of the previous treatment and try a variational Ansatz of the form 1 2 1 2 g(ζ, ρ) = exp − aζ − bρ (7.93) 2 2 Performing the necessary Gaussian integrals, we find 1 1 1 2 1 2ζ0 2 2 2 β= b + cos (θ ) + a + sin (θ ) + cos (θ ) ζ0 − √ 2 b 2 a πb (7.94) Minimizing this with respect to a, b, and ζ , we find 2 β = cos(θ ) 1 − + sin(θ ) π 2 (7.95) b = cos(θ ) 1 − π √ with a = sin(θ ) and ζ0 = 1/ π b. Now, in analogy with the θ = 0 case, where we had Bc2 2 βmin = 1 − = (7.96) π Bc3 (0) we may define β=

Bc2 Bc3 (θ )

(7.97)

which leads to 1 1 1 sin(θ ) = cos(θ ) + Bc3 (θ ) Bc3 (0) Bc2

(7.98)

or equivalently Bc3 (θ ) =

Bc3 (0) cos(θ ) +

(7.99)

√sin(θ ) 1−2/π

Hence, we see that when the field is perpendicular to the surface, Bc3 = Bc2 , and the variation in Bc3 is smooth in between the limiting cases θ = 0 and θ = π/2. In particular 1 dBc3 Bc3 (0) 1 − |θ =0 = = = 1.66 (7.100) Bc3 dθ Bc2 1− 2 π

SURFACE SUPERCONDUCTIVITY AND Bc3

197

A more careful numerical analysis of the problem of tilted magnetic fields yields for the above slope the result 1.35, which is not too far away from our analytical estimate. A more accurate variational result may be obtained by refining the variational function, to a form like g(ζ, ρ) = (1 + cζ 2 + dρ 2 ) exp(−(aζ 2 + bρ 2 )/2). In the case of a metallic coating of the superconductor, a current can in principle go across the interface at x = 0, such that the boundary conditions are different. Consider again the case of a magnetic field parallel to the surface, with the vector potential given by A = Bx y. ˆ The boundary condition to be used is then given by, crudely dψ ψ |x=0 = − dx l

(7.101)

where l is some characteristic length that provides a proximity effect of superconductivity into the metal. This reduces the flatness of ψ at the surface, i.e. the pinning of Cooper pairs to the surface is reduced. Hence one can expect Cooper pairs at the surface to diffuse into the metal and be destroyed. A metallic overlayer thus acts as a pair-breaker and this will impede surface nucleation of superconductivity and suppress surface superconductivity above Bc2 . Finally, a cautionary remark is in order concerning hard superconductors, i.e. those with large bulk values of κ. The treatment in this section has been exclusively at the mean field level. As the surface of the superconductor is approached from within one must expect a continuous depletion of superfluid density. As we shall demonstrate in Chapters 9 and 10, the superfluid density is connected to the phase-stiffness of the order parameter. This will also reduce the correlation length ξ , since this is basically a measure of the length over which the local phases of the order parameter are correlated. A reduction in ξ would lead to an increased estimate for the upper critical field compared to the bulk value.

8 More on the Flux-line System 8.1 Elementary pinning forces and simple models 8.1.1

The concept of a pinning force

We have previously derived the force per unit length from one vortex, labelled as number 1, on another parallel vortex labelled as number 2, in Chapter 6. This situation is illustrated in Figure 8.1. We found in Chapter 6: f2,x = jy 0

(8.1)

f 2 = J 1 × 0

(8.2)

which we can rewrite as

where J 1 is the supercurrent density from vortex number 1 at the position of vortex number 2. If there is a current from other vortices, or an additional external current, giving a total current density J s , this will determine the total force per length, f on the reference vortex, i.e. f = J s × 0 .

(8.3)

f becomes a volume force, F , if we divide both sides by unit area, and we have F = Js × B

(8.4)

This force will, if acting alone, cause a continuous displacement of flux lines as long as the force F is acting upon the flux line lattice. This is a basic problem encountered when a type II superconductor is to be used for current and energy transport. The forced motion of the vortices against the friction of the electron gas, normal and superfluid, causes dissipation of energy, and the superconductor Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

200

MORE ON THE FLUX-LINE SYSTEM

2

1

Figure 8.1 Two interacting flux lines, repulsive forces shown.

behaves essentially like a normally conducting material. To stop or prevent this motion, a pinning force F p of magnitude at least equal to F is necessary. When |F | < Fp the flux-line lattice will be at rest; whereas the lattice will move if |F | > Fp . The precise value of F corresponding to the volume pinning force Fp is specially significant. When the applied force density is equal to Fp the corresponding current density is defined as the critical current density, Jc . We now have Fp = Jc B or Jc ≡ Fp /B

(8.5)

This is the conceptual definition of Jc . How it is to be determined is not obvious. Fp is not usually measured directly. Rather, by judicious choice of a criterion for determination of Jc , one can calculate the pinning force based on that definition.

8.1.2

Pinning force and flux gradient

Equation 8.4 could equally well be written by means of Maxwell‘s equation ∇ × H = J , as F = (∇ × H ) × B

(8.6)

This points to the significant fact that a current corresponds to the existence of a gradient of H . We have here the curl of H , ∇ × H , but in well defined cases

CRITICAL STATE AND THE BEAN MODEL

201

ˆ along the z-axis and this is just a negative gradient. Take for example H = kH ˆ ˆ ˆ the current along the y-axis. We get, using i, j , k as unit vectors J = ∇ × H = −jˆ

∂ H = Jy jˆ ∂x

(8.7)

The volume force acting on the flux lattice is now, on introducing the B-field |F | =

B ∂B µ0 ∂x

(8.8)

This relation provides a basis for a definition of critical current density Jc in the Bean model.

8.2 Critical state and the Bean model The critical current density Jc will in general depend on both r and B. This should be regarded not only as a possibility, but as a reality under usual conditions. This fact tends to complicate the analysis of the critical current condition substantially. Even so, simplified models are quite often useful. Bean [87] suggested to model Jc as a constant value corresponding to regarding Jc = µ−1 0 (dB/dx) as constant. Figure 8.2 shows sketches of the correspondence between Jc and the flux gradient ∂B/∂x in several situations, including the reversal of flux gradient on reducing the applied field Ba after it has been raised to a maximum value Bm , larger than B ∗ , which is the field where the flux first penetrates to the center. In all these sketches |Jc | is taken to be a constant value in space and time. This demonstrates the properties of the simplest form of Bean model. The situation where the flux front reaches the center, and the current density is Jc everywhere, is the Bean critical state. It allows a simple and often quite useful analysis of what is going on in the sample under varying external applied field. The Bean model, as shown in Figure 8.2, takes Jc to be independent of B. This is a condition which is never quite correct. In cases where the pinning force is independent of B, Jc will be proportional to B −1 . We have also to keep in mind that higher temperatures necessarily will influence Jc negatively, and that a spatial dependence of Jc is also present unless the material is perfectly homogeneous with regard to pinning force. Experience tells us that relatively simple modifications of the Bean model may be sufficient to account for more complicated situations. One modification, often referred to as the Kim–Anderson model [88], is described by the following expression for Jc Jc (T , B) =

J0 (T ) 1 + B/B0

(8.9)

202

MORE ON THE FLUX-LINE SYSTEM Bm

B(x)

B(x)

B*

(3) Ba

B(x)

(1)

Ba

(2) (2)

(1) x

−d/2

d/2

+Jc

x

−d/2

d/2

+Jc

x (1)

(1)

(1)

(2,3)

−Jc (a)

d/2

+Jc (2,3)

−Jc

x

−d/2

x

x −Jc

(b) +Jc (2)

−Jc (c)

Figure 8.2 Bean model. (a) Flux distribution (upper part) and corresponding current distribution (lower part) after application of an external field Ba which is subsequently kept constant. (b) Similar to situation (a), labelled as (1); then (2) after raising Ba to B ∗ where the flux front reaches the centre of the sample, the situation referred to as the critical state, and (3) after increasing Ba to Bm above B ∗ . (c) Shows the effect of lowering the applied field, case (1) and case (2), by different amounts.

which has been shown to agree well with experimental results in some cases. Here J0 (T ) is the critical current density at zero field and B is the local flux density. B0 is a model parameter to be determined by experiment. Next we derive a simple relationship between Jc and the magnetization, implied to exist in Figure 8.3. Imagine that we have measured a complete magnetization curve M(H ), looking like the one sketched in Figure 8.3a. In Figure 8.3b we indicate how the area A represents the difference in magnetisation of the sample at point (1) and point (2) in Figure 8.3a. The total magnetization difference at H1 is M = M↑ − M↓ = M(H1 ), where we have once arrived at H1 from lower field (1), and once from higher field (2), as illustrated in Figure 8.3b. The two approaches to H1 result in different magnetisations M↑ and M↓ , and with a difference M↑ − M↓ . This construction can also be made via graphical display of the Bean model. Now,

CRITICAL STATE AND THE BEAN MODEL

203

−M

(1) ∆M H1 (2)

Hc2

H

(a)

(2)

H

A ∝ ∆M × d (1)

(b)

− d2

d 2

x

Figure 8.3 (a) is a sketch of magnetization versus field H in a type II superconductor with pinning. Magnetization starts out from zero. Points (1) and (2) refer to the same magnetic field with different magnetization. The dotted line is the magnetization without pinning. In (b) we sketch how the magnetisation difference M is obtained.

since Jc =

M(x) x ,

we have M(x) = Jc x in the Bean model. We calculate 1 M↓ = − d/2

d/2

0

1 Jc x dx = − Jc d 4

(8.10)

Correspondingly we get M↑ = 14 Jc d. The difference is then M = M↑ − M↓ = 1 2 Jc d, or Jc = 2

M d

(8.11)

This allows an estimate of Jc from a half cycle measurements of M(H ), (‘Magnetization Jc ’). In other sample geometries, a numerical, geometry dependent factor of the order of unity will modify the right-hand side of Eq. 8.11.

204

MORE ON THE FLUX-LINE SYSTEM

The simple, and very useful rule we glance from this, is that the wider the magnetization loop is, the higher is Jc . This kind of data analysis is widely used to obtain Jc . Before computing the Jc -value, one should also attempt to remove the equilibrium part of the magnetization curve, i.e. the M(H ) curve which is obtained without pinning. This magnetisation method for measurement of Jc is often easier to use than the transport method.

8.3 Flux-line dynamics, thermal effects, depinning, creep and flow 8.3.1

TAFF, flow and creep: Definitions

Current transport measurement are always central in the study of superconductivity. In Figure 8.4 we have sketched measured voltage V versus current I , (alternatively electric field E versus current density J ) in the presence of an external magnetic field which has created a certain vortex density in the superconductor. The definitions which apply to the 3 different parts of the I–V curve are: ‘thermally assisted flux flow’ (TAFF) in the low current end, ‘flux flow’ in the high current region, and ‘flux creep’ in the transition region between the two. While the latter two terms were commonly used in low-Tc research, the new term, TAFF, was coined for this new aspect of high-Tc , I–V characteristics. The particularly important feature of this plot is the highly nonlinear region, where the critical current Ic is marked in the region crossing over between TAFF and flux flow. What has been agreed on as a practical measure is to define Ic at the point where V = 1 µV, or similarly, E = 1 µV/cm. The point is that

E, V

Flux flow

Flux creep 1 µV

TAFF Jc, Ic

J, I

Figure 8.4 A sketch for the definition of Ic or Jc by transport measurement. This curve has a linear V versus I at low I , followed by a highly nonlinear region at intermediate values of I , and finally a linear relation again. The effective resistance is quite different in the two regions where ohmic behaviour is found. The plot can be read either as an E –J characteristic or as an I –V characteristic.

FLUX-LINE DYNAMICS, THERMAL EFFECTS, DEPINNING, CREEP AND FLOW

205

there is no way to define sharply what Ic is. One has to agree on a criterion related directly to measurements. However, it should be noted that flux flow is a phenomenon which arises when the current is high enough to essentially tear loose the whole flux lattice, and set it in sliding motion. It is then quite reasonable and conceptually sound to define Ic and the corresponding Jc as the point where this flux motion is just about to begin. All of the above implies the presence of various kinds of flux line dynamics present during the measurement.

8.3.2

Flux flow

If the superconductor is pin-free, or if the Lorentz force is so strong that it exceeds the pinning force, the vortex velocity v is limited by the viscous drag exerted by the surrounding medium, through the force balance 0 J = ηv giving v=

1 0 J η

(8.12)

Multiplying the above equation with B gives the E-field E = Bv =

B 0 J = ρff J η

(8.13)

with a flux flow resistivity ρff =

1 B0 η

(8.14)

The most widely accepted theory of flux-flow was worked out by Bardeen and Stephen [89]. They considered a vortex core of radius ξ , which can be treated as if it were in the normal state. When a vortex is set into linear motion the moving flux pattern will generate an electric field in its surroundings, the vortex core included. The induced resistive currents in the vortex core creates a loss W = ρff J 2 , and thereby a flux-flow resistivity. The result is ρff = ρn

B Bc2

(8.15)

where ρn is the normal state resistivity. It is not difficult to guess such a relation: when B reaches Bc2 , ρff becomes ρn as it should. When B goes to zero, ρff goes to zero as it should, and in between the factor B/Bc2 is simply the fraction of the material occupied by the vortex cores. ρff is therefore equal to ρn times this fraction. The result is the same as if a uniformly distributed current were passed through the material and losses would appear from the fraction of the current which passed through the core regions.

206 8.3.3

MORE ON THE FLUX-LINE SYSTEM

Thermally activated flux creep: Anderson model

Random thermal forces may induce escape of a vortex from its potential minimum at the pinned position. Depinned vortices will move, or ‘creep’ in order to relax the critical state field gradient. We outline the theory of flux creep which was put forward by Anderson and Kim [88]. The escape rate R from pin sites is determined by the Boltzmann factor, R = ν0 e−U/kT

(8.16)

where U is the height of the activation barrier and ν0 is some microscopic attempt frequency, typically of order 10−8 − 10−10 s−1 . As indicated in Figure 8.5, the effective height of the barrier will be reduced with increasing current. We can model this by writing U = U0 (1 − J /Jc ). Here Jc is the critical current density, and is proportional to the maximum energy gradient dU/dx. The decay of a finite (non-equilibrium) magnetization as well as its associated current density J , proportional to R, for forward jumps is U0 dJ ∝ e− kT (1−J /Jc ) dt

(8.17)

J=0

J < Jc

J ~ Jc

Figure 8.5 force.

Energy landscape for a flux line in a pinning environment and a uniform external

SINGLE PARTICLE TAFF

207

with the long-time solution J (t) ∝ const. − ln(t).

(8.18)

Hence, at long times the magnetization current and therefore also the magnetic moment decay proportional to ln t. In a transport measurement the E –J characteristics will be exponential, since the force equation eE = ev × B can be written as U0

E = Blν0 e− kT (1−J /Jc )

(8.19)

where l is the effective jump distance. This equation is of course the equivalent of an I–V characteristic. It is highly non-linear as required by experimental observation sketched in Figure 8.4, and the model contains simple creep behaviour. The flux-creep theory described here is a single particle model, i.e. depinning events occur by escape of individual vortices, independently at individual pins. The simplest way of accounting for collective dynamics is to assume that bundles of correlated flux-lines move simultaneously. Anderson suggested that all fluxlines within a distance λ would constitute a correlated flux bundle. However, the bundle concept does not introduce truly new dynamics, as its effect can be shown to alter only phenomenological parameters like U , Jc , l etc. A more advanced approach to collective dynamics is the theory of collective creep, a subject we return to below.

8.4 Single particle TAFF The creep rate as given above has a finite value even for J = 0. This unphysical result occurs because we did not take into account the asymmetry of forward and backward flux jumps. If one subtracts jumps in the backwards direction from forward jumps in the rate equation, one obtains the E-field, U U − kT0 (1−J /Jc ) − kT0 (1+J /Jc ) E = Blν0 e −e −U0 /kT

= 2Blν0 e

U0 J sinh kT Jc

(8.20)

which gives the same result as earlier at large currents, J Jc kT /U0 , but at low current it gives a linear resistance, the so-called TAFF resistance (thermally assisted flux flow) E = 2Blν0

U0 J = ρTAFF J Jc kT

(8.21)

208

MORE ON THE FLUX-LINE SYSTEM

According to this analysis, magnetization current and magnetic moment will decay exponentially with time in a way analogous to skin effect in normal superconductors. Linear resistance has been found at low current densities in a large range of temperatures below the transition. The relevance of the TAFF diffusive dynamics for this regime was discussed by Kes and coworkers [90].

8.5 FLL elasticity and pinning 8.5.1

Collective effects

Among the more important recent developments is a deeper insight into the wavevector dispersion of the elastic constants, which is important for melting as well as for pinning of the flux line lattice. In this Section we give an elementary discussion of pinning effects based on the elasticity theory worked out before in Chapter 6. An elastic energy is always written as (1/2)cε2 , where c is an elastic constant, and ε is a corresponding elastic strain. This is the case whether the strain is applied to the crystal lattice as well as to the flux line lattice. What concerns us in the following is the flux line lattice. To visualize the meaning of typical strains and elastic constants in the FLL, we refer to Figure 8.6 which illustrates the three important strains, with corresponding elastic constants c11 for a strain ε1 , c44 for a strain ε4 , and c66 for a strain ε6 . Calculations in Section 6.7 show that an important k-vector dispersion occurs at high k due to non-local response. By high k we mean k-vectors that are comparable to the inverse screening length λ−1 . We have three lengths to com√ 1 pare: (i) The lattice constant of the FLL, a = [(2/ 3)0 /B] 2 , (ii) the screening length λ and (iii) the wavelength λε of the strain. Due to the high density of vortices giving a short length a at a typical magnetization, we usually have λ a except very close to Bc1 . What is important for the elastic response under such conditions is whether the applied strain has a k-vector which is of the order of λ−1 or greater. Under such conditions the flux line interactions are substantially weakened, since the denominator in the expression for cii typically goes like 1 + k 2 λ2 , with an exception for c66 . We refer to Chapter 6 regarding the elastic properties of the FLL. In the isotropic case the results are: c11 (k) ≈

B2 ; µ0 (1 + k 2 λ2 )

c44 (k) ≈ c11 (k) + 2c66 ln

c66 ≈

B 0 BBc1 · ≈ ; 2 8µ0 2π λ 8µ0

κ2 1 + kz2 λ2

(8.22)

We notice that c66 is non-dispersive and very small compared to the two others. In high-Tc superconductors where λ is very long (≈150 nm) the softening of the

FLL ELASTICITY AND PINNING

209

e1; c11

e4; c44

e6; c66

Figure 8.6 Elastic strains ε1 , ε4 , and ε6 of a flux line lattice under homogeneous strain, i.e. k = 0. Corresponding elastic moduli are indicated in each case.

FLL becomes important at k-vectors with wavelength even larger than 150 nm, and all shorter wavelengths. The lattice constant a at 0.2 T is about 100 nm. From there on up in field, screening currents from surrounding flux lines overlap more and more, with the gradual breakdown of net screening, and accompanied by softer and softer FLL. Let us estimate the effects on thermal phonons at the Brillouin zone boundary of the crystal lattice. These have a k-vector in the ab-plane of approximately π(nm)−1 . The product kλ is then about 300. This means that the elastic constants c44 and c11 for tilt and compression are two orders of magnitude softer as seen by Brillouin zone phonons than by zone centre, k = 0 modes. In other words, acoustic waves with low wavevector will propagate faster in the presence of a magnetic field, while at the zone boundary it makes almost no difference. (Recall here that the elastic constant of the FLL is to be added to that of the crystal lattice.) We note that at k = 0, c66 typically is weaker than c11 and c1 c44 by a factor 18 BBc1 as seen from the approximation c66 ≈ BB 8µ0 . The above discussion underscores the susceptibility of the FLL of high-Tc materials to thermal fluctuations.

210

MORE ON THE FLUX-LINE SYSTEM

We refer here for completeness the results for c44 and c66 in the anisotropic case with the field along the c-axis, from which c11 can also be found. c44 (k) ≈ c66 ≈

B2 κ 2 2 2c66 ln + 2 µ0 (1 + (kx2 + ky2 )λ2c + kz2 λ2ab ) 1 + kz2 λ2ab

(8.23)

B 0 × 8µ0 2π λ2ab

(8.24)

Here κ = λab /ξc and = λc /λab = ξab /ξc . Except for differences arising in symmetry properties, we recognize the results from the isotropic case: c66 remains low and non-dispersive, and its magnitude relative to c44 is still of the order of Bc1 /8B; more precisely (0 /2π λ2ab )/8B. The key idea in collective weak pinning is to describe the distortion of the vortex lattice in terms of a correlation volume, Vc = Rc2 Lc where Rc and Lc are the transverse and longitudinal correlation lengths, respectively. A correlated volume may be thought of as a volume Rc2 Lc , which appears approximately like a piece of regular flux-line lattice, but with an average lattice constant which may be slightly different from that of the unpinned lattice. The whole flux-line system may be thought of as a collection of such correlated volumes, and Rc and Lc are average lengths defining the typical correlation volume Vc . The underlying energy principle which determines the positions of flux lines, and hence the distortions in each correlation-volume, is the balance between the elastic energy cost of deforming the flux-line lattice locally within Vc versus. the energy gained by letting the flux lines pass through several point pins within Vc . The collective pinning theory was originally developed by Larkin and Ovchinnikov [91]. For a brief analysis of these effects on Jc , following Tinkham [53] we disregard the strain ε1 . To calculate the increased elastic energy connected with strains ε4 and ε6 we need to estimate δFe = 12 c44 ε42 + 12 c66 ε62

(8.25)

Here we can divide the range ξ of the pinning force by the corresponding correlation lengths to obtain the strains. ε4 =

ξ ; Lc

ε6 =

ξ Rc

(8.26)

This gives 2 2 1 1 ξ ξ δFe = c44 + c66 2 Lc 2 Rc

(8.27)

Next we consider the pinning energy δFp . When N elementary pinning forces 1 f are added randomly in a volume Vc , the total force is N 2 f . Here N = nVc ,

FLL ELASTICITY AND PINNING

211

where n is the number of forces f per volume, and Vc is the correlation volume. This force acts, on the average, over a distance ξ , after which it becomes random. The potential energy is force times distance: 1

1

1

1

1

δFp = ξ N 2 f/Vc = ξf n 2 /Vc2 = ξf n 2 /Lc2 Rc

(8.28)

The total energy δF = δFe + δFp is 1 δF = c44 2

ξ Lc

2

1 + c66 2

ξ Rc

2

1

−

ξf n 2 1

(8.29)

Lc2 Rc

By the minimisation of δF one finds approximate expressions for Lc , Rc , Vc , as functions of c44 , c66 , ξ, n, f . The minimum of δF is found [53] to be δFmin = −

n2 f 4

(8.30)

2 ξ2 8c44 c66 1

On equating the pinning force per unit volume f (n/Vc ) 2 with the maximum Lorenz force density Tinkham found for the critical current density: Jc =

n2 f 4 2 ξ 3B 2c44 c66

(8.31)

This expression has implications borne out by experiment: Jc increases with softening of the lattice, i.e. with smaller elastic moduli, because the flux line system can more easily adjust the positions of individual flux lines to fit the random position of pins. This is often observed near the melting temperature of the flux-line lattice. It is interesting to imagine the opposite extreme; that of a completely rigid FLL in a random arrangement of (weak) pins of high density. In this case the pinning force will be zero: The total pinning energy Vp is in this case necessarily independent of the position of the FLL. The force is given by the negative of the gradient of U , and since U does not vary with position, the force must be zero. This sends a message that the density of pins should be high enough to contain a wide k-spectrum in the Fourier expansion n(k) of the pin density n(r), to take advantage of the wide range of k-values where the elastic constants c11 and c44 are soft. A Fourier density peaking at the FLL Brillouin zone boundary wavevector might seem ideal. This corresponds to a pinpoint density with an average distance like the FLL lattice constant. However, this would be ideal for that particular field only. If pinning is to be effective over a wide range of fields, there has to be a broad variation in pin distance, even for the use of the Brillouin zone boundary matching criterion to be good. Hence we end up,

212

MORE ON THE FLUX-LINE SYSTEM

again, with a broad spectrum of Fourier density k-values as a good guideline. Only when optimizing pinning for a particular value of the magnetic field, i.e. a particular FL density, can a pin distance corresponding to the Brillouin zone wavelength or its vicinity, be the optimal solution.

8.5.2

Collective creep: inverse power law U (J )

From the previous discussion of collective pinning it becomes evident that a full description of creep phenomena needs to take into account collective effects. This has been attempted [91, 92], and has led to interesting new predictions for collective creep, i.e. for the behaviour of an elastic flux line lattice in the presence of random, weak point-pin sites. In this theory the collective creep regime is characterized by diverging time and length scales in the limit of zero driving force which is also the signature of so-called vortex glass behaviour. We review here only briefly some aspects of collective creep theory without full justification, and refer to the original literature for details. The correlated volume Vc = Rc2 Lc was defined in the previous subsection as the characteristic volume which maintains the quality of a regular flux-line lattice even in the presence of distortions due to the interaction with a high density of point pins. Theory predicts that the volume Vc grows with the displacement ω of flux lines, raised to the power D, the dimensionality of the correlated volume, divided by the so-called wandering exponents ξ . In other words Vc ∝ ωD/ξ . Here D = 0 for single pancake vortices, considered as point vortices, D = 1 for a single vortex line, D = 2 for a bundle of point vortices (pancakes), and D = 3 for a bundle of vortex lines. The wandering exponent ξ is determined by equating the energy of the elastic vortex lattice deformation to the fluctuation in pinning energy. The next requirement is that both these energies should be of the order of the energy gain due to the driving force j BVc ω, the Lorentz force density multiplied by volume and displacement. Through this requirement the correlated volume becomes current dependent, and results in a current-dependent flux creep activation barrier U = Uc

Jc J

µ (8.32)

with µ = (D + 2ξ − 2)/(2 − ξ ) > 0. It has the surprising and important consequence that as J → 0, the activation energy U → ∞. This leads to vanishing of both flux motion and linear resistance in that limit. In the single vortex regime in three spatial dimensions µ = 1/7, and the divergence of U is weak (near logarithmic). As the current density decreases one crosses over from single vortex regime to a regime of small bundles with µ = 5/2, then to larger bundles with µ = 1, and finally to large bundles with

FLL ELASTICITY AND PINNING

213

µ = 7/9. Other values of the exponent µ are obtained when a layered structure becomes dominant like in some high-Tc cuprates. The collective creep theory applies at current densities much lower than the critical one, i.e. J Jc . However, U is expected to go to zero at J = Jc (in the Anderson–Kim model as U0 (1 − J /Jc )). To incorporate this into the collective creep model one often rewrites Eq. 8.32 as U (J ) = Uc [(Jc /J )µ − 1], where Uc = U0 /µ [92]. This provides an interpolation between the low current (‘glassy’) phase and the high current (linear A-K) phase.

8.5.3

Logarithmic U (J )

The various models used for U (J ) have often turned out to be difficult to distinguish on the basis of experimental data. This situation is compounded by the discovery that in many cases a logarithmic U (J ) is found to give the most adequate interpretation of data, i.e. U (J ) = Uc ln

Jc J

(8.33)

Due to the short coherence length and the strong anisotropy of high-temperature superconductors, pinning energies are small, and thermally activated flux motion is a significant source of dissipation in the current carrying state, even when the Lorentz force on the vortices is less than the depinning force. The resulting decay of a screening current corresponds to a decay of the induced magnetic moment. For this reason, measurement of the magnetic relaxation serves as a powerful tool to investigate the dynamics of vortices in superconductors. In the thermally activated regime of flux creep the decay rate of the magnetisation current density is given by the rate equation, dJ U (T , B, J ) = −A × exp − dt T

(8.34)

Where A is a constant. In Figures 8.7, 8.8 and 8.9 [93], [94] we illustrate the procedures involved in analysing magnetization current decay data for possible logarithmic activation energy. The substance studied was HgBa2 CaCu2 O6+x (Hg-1212) with a Tc = 127 K. In Figure 8.7 the time dependence of magnetisation was measured over two decades in time in 1 T magnetic field parallel to the c-axis using a SQUID detector. The magnetic moment due to screening currents caused by the flux gradient set up by application of the external field is shown here. Notice the great differences observed at different temperatures. Data have been corrected for the equilibrium magnetisation which would be present without pinning.

214

MORE ON THE FLUX-LINE SYSTEM

5K

m − meq

0.06

10 K

0.04

15 K 20 K

0.02

0.00 0

100

1000

25 K 30 K 35 K 40 K 60 K 10000

Time (s)

Figure 8.7 Typical relaxation curves in Hg-1212 of the non-equilibrium magnetic moment in a field of 1 T, at different temperatures as indicated by the numbers. The magnetic field is along the c axis. After Gj¨olmesli et al. [94]. 2500

2000

U (K)

1500

1000

500

0

0.1 T 0.5 T 1T 2T 4T 1 × 10−3

1 × 10−2

1 × 10−1

J a mJ (emu)

Figure 8.8 The barrier energy of Hg-1212 as calculated from Eq. 8.35. Each curve consists of data sets obtained at the temperatures indicated in Figure 8.7. The numbers indicate the values of the external magnetic fields, in tesla. B parallel to the c-axis. After Gj¨olmesli et al. [94].

In Figure 8.8 data were analysed by the Maley method [95]. This consists first in inverting Eq. 8.34, to write it as dmJ U (T , B, mJ ) = T ln A − ln (8.35) dt

FLL ELASTICITY AND PINNING

215

1200

Uc (T )

800

400

0

0

1

2

3

4

B (T)

Figure 8.9 Resulting Uc versus T from the analysis of data in Figure 8.8.

after replacing current J in Eq. 8.34 with the associated magnetic moment mj = m − meq . Here, the quantity meq is determined from the experimental data by the asymmetry in the magnetization during increasing versus decreasing field. Next, all measurement taken at different temperatures in the same magnetic field are regarded as giving access to different segments of U (J ) since J associated with any magnetisation is proportional to that magnetisation. The data in Figure 8.8 immediately attests to a current-dependent activation energy close to logarithmic in its dependence on J , according to Eq. 8.33. The experiment also gives further information about the B-field dependence of the activation energy, while it was not necessary to assume T -dependence of U . A logarithmic U (J ) could possibly be expected from a model [96] in which a logarithmic spatial variation of pinning energy is involved. Alternatively, it can be a special case of collective creep for 2D pinning in the extreme lowcurrent limit [97]. Alternatively again, it may be viewed as a special case of the inverse power law Eq. 8.32 with vanishing µ. Furthermore, in the critical region near a vortex glass transition (see later), power law E–J curves are expected for intermediate currents, irrespective of the value of µ, often referred to as the vortex glass exponent. Such power-law E–J would suggest logarithmic U (J ) for intermediate currents, and could fill the gap between the low current limit and high current limit in the interpolation formula for the collective creep. We note finally, that the experiment just described gave indication of a different type of creep at very low temperatures, a temperature independent limit creep due to quantum mechanical tunnelling between pin sites.

8.5.4

The vortex solid–liquid transition

A much debated subject in the scientific literature on the properties of the vortex system in superconductors, and in high-Tc superconductors in particular,

216

MORE ON THE FLUX-LINE SYSTEM

is the question regarding the nature of the transition between a vortex liquid and a vortex solid, following the works of Gammel and Bishop [98], Nelson [99], and Fisher et al. [100]. Two views have been advocated, that the solid phase may be in the nature of a vortex glass, or that it may be a more regular vortex lattice. In the first case a continuous transition is expected, in the latter a first order discontinuous one. Over the years the conclusion has been reached that both are possible. Depending on the amount of pinning, at low pin density freezing of a regular lattice may occur. We refer here to the Topical contribution of Kadowaki (Section 13.8) showing in a convincing manner that a first order transition to a regular vortex solid can indeed take place. At high density of pins the “vortex matter” is sufficiently distorted from a regular lattice that it freezes into what has become known as a vortex glass state. The analysis of this state was made earlier than the first order transition, largely due to the difficulty of obtaining superconducting material with low pin density. The fact that the frozen vortex system may appear as a regular lattice has been amply demonstrated by various decoration and imaging techniques. We refer to Figure 8.10 for an example. The other alternative, the vortex glass, was concluded to exist from very detailed I–V (or E–J) characteristic measurements [102] in YBCO thin film (see Figure 8.11 [103]). The glass line (Tg -line) in the phase diagram may be determined by scaling of E–J data. Just at Tg the current–voltage characteristic is expected to show

Figure 8.10 Magnetic decoration techniques allows imaging of nearly perfect triangular vortex lattice. After Tr¨auble and Essmann [101].

FLL ELASTICITY AND PINNING

217

1

3

log E

0

−1

Tg 2

−2 1 −3

4

5

6

7 log J

8

9

10

Figure 8.11 Schematic I–V isotherms of an YBCO single crystal in a magnetic field applied parallel to the c-axis. The dashed line marks the glass transition temperature below which the curves decrease exponentially. The temperature decreases in equal steps from top to bottom or from left to right. Region 1 marks the linear I–V behaviour, region 2 indicates non-linear behavior above Tg and region 3 is when d(log E)/d(log I ) = 3 both above and below Tg . [103]. Simplified from Blatter et al. [97].

power law behaviour, E ∝ Jα

(8.36)

with α = (z + 1)/(D − 1), where z is the dynamic exponent with typical value 4–5, and D is the relevant spatial dimension. Above Tg the characteristic should change from ohmic ρ(T ) ∝ (T − Tg )ν(z+2−D)

(8.37)

at very low J where ν is the temperature exponent for the coherence length, to power law at high J . Below Tg a glass-type response at small current densities is expected as U0 Jc µ E ∝ exp − kT J

(8.38)

Again a power law critical behaviour is expected at high current densities. The crossover between the two regimes of power law at small scales and large current, and liquid/glassy state at small scales (probed by low current density) scale as Jx± ∝ |T − Tg |ν(D−1)

(8.39)

218 8.5.5

MORE ON THE FLUX-LINE SYSTEM

Lindemann criterion and melting of a clean flux-line system

In this subsection, we will present a calculation that determines the rough position of the line in the (B, T ) phase-diagram where the flux-line lattice may be expected to melt into a liquid state, i.e. the transition line from an Abrikosov flux-line lattice to a vortex state with zero shear stiffness. Crucial in our considerations will be the observation that conventional melting of a three-dimensional solid is expected to be a first order phase transition. This means that longwavelength fluctuations do not occur at the point of the transition, unlike in a second order phase transition. Under such circumstances, short-wavelength fluctuations are the ones responsible for inducing the transition from the solid to the liquid state. For our purposes this may be rephrased as follows. The Fourier modes of the fluctuations that dominate at the transition point are those that live at the boundary of the first Brillouin zone of the vortex lattice, i.e. those Fourier modes of fluctuations that have the largest wave vectors. Thus, it is reasonable to conjecture that when we want to estimate the position of the melting line using a description of the vortex lattice in terms of elasticity theory, we need to consider wave-vector dependent elastic moduli, i.e. non-local elastic moduli. In fact, as we shall see, this is absolutely crucial in order to obtain a reasonable estimate of the location of the melting line, since it will turn out that the elastic moduli of the flux-line lattice soften significantly as the wave vectors increase, and this dramatically enhances the susceptibility of the flux-line system to thermal fluctuations. Moreover, the variation of the position of the melting line with degree of layeredness of the material, can only be brought out through a non-local formulation. Before we go into the details, let us outline the structure of the the calculation that determines the position of the melting line, Tm (B). We consider a situation where we have an external magnetic field along the zˆ -direction, and we consider also the case where we have uniaxial anisotropy. This will make our results directly applicable to the study of the melting transition in the high-temperature cuprates, where the issue of flux-line lattice melting was first seriously considered as an experimental reality. (Many years earlier, Eilenberger had considered the melting of the flux-line lattice theoretically in moderate type II superconductors, and concluded that a melting line would be practically indistinguishable from the upper critical field line Hc2 (T )) [104]. The ground state of the system is the hexagonal Abrikosov vortex lattice, and we now consider the Hamiltonian that governs the elastic fluctuations around this ground state. Hence, we write the positions of the flux lines as rν = Rν + sν (z) Here, Rν is the position of flux line number ν, while sν (z) = (sxν (z), syν (z), 0) is the displacement of the νth flux line away from its position in the perfect

FLL ELASTICITY AND PINNING

219

Abrikosov flux-line lattice. Note how this displacement vector has two components, which vary with the distance along each flux line. In order to consider the fluctuations of the flux-line lattice in the continuum limit, we define an effective elastic Hamiltonian governing these fluctuations. For an ideal triangular lattice the Hamiltonian in the harmonic approximation takes the simple form

1 2 H = si (−k) cL (k)ki kj + δij c66 (k)k⊥ + c44 (k)kz2 sj (k) (8.40) 2 k

Here, cL , c66 and c44 are bulk-, shear-, and tilting elastic moduli, respectively, and si (k) are the Fourier modes of sν (z). Given the Hamiltonian Eq. 8.40, the elastic propagator can be written in the form

PT PL (8.41) + Gij (k) = kB T 2 + c (k)k 2 2 + c (k)k 2 c66 (k)k⊥ c11 (k)k⊥ 44 44 z z 2 is the transverse where c11 (k) ≡ cL (k) + c66 (k). Moreover, PT = δij − ki kj /k⊥ 2 is the longitudinal projection operator. projection operator, while PL = ki kj /k⊥ To examine the stability of the flux-line lattice against thermal fluctuations we will determine the mean square displacement of the flux lines from their equilibrium positions d2 (T ) = sν2 = TrGij (k) (8.42) ν

k

Here .. indicates a thermal average with respect to the Hamiltonian Eq. 8.40. Using Eq. 8.41 in Eq. 8.42

∞

d (T ) = kB T 2

×

0

dkz 2π

0

2

2 dk⊥ 2π

1 2 + c (k)k 2 c66 (k)k⊥ 44 z

+

1 2 + c (k)k 2 c11 (k)k⊥ 44 z

(8.43)

The Lindemann criterion now states that the flux-line lattice will melt when thermal fluctuations are such that the thermally induced root mean square displacements of each flux line is some fraction of the intervortex distance in the ground state of the Abrikosov vortex lattice, i.e. the melting criterion is given by d(T ) = cl, where l is the lattice parameter of the flux-line lattice, and c is some fraction typically of order c = 1/10. In the triangular Abrikosov vortex lattice, √ we have 3l 2 /2 = 0 /B, i.e. l is determined by a flux quantization condition. In the above expression, we have approximated the k-space integral over the first Brillouin-zone by assuming a circular Brillouin-zone of radius , where 2 , and b = H /H . Here H is the spatial average of the field, 2 = 2b/ξab sp c2 sp

220

MORE ON THE FLUX-LINE SYSTEM

averaged over the sample, and Hc2 is the upper critical field. Moreover, ξ⊥ is the ab-plane coherence length. The k-dependant elastic moduli can only be obtained from the full Ginzburg– Landau theory after a very arduous and lengthy calculation, there really appears to be no easy way of obtaining them. However, a detailed derivation may be found in the paper by Houghton and colleagues , [105], and the interested reader is referred to this paper, see also the work of Sardella [106]. The expressions for the elastic moduli, despite their involved derivations, are relatively simple and given by

B 2 mab 1 1 c44 (k) = (8.44a) ω0 2 + µ0 mc k⊥ + (mab /mc )(kz2 + ω0 ) 2bκ 2 B2 k 2 + (mab /mc )ω0 c11 (k) = ω0 2 + (m /m )(k 2 + ω )) µ0 (k 2 + ω0 )(k⊥ ab c 0 z

1 (8.44b) − 2 k⊥ + (mab /mc )kz2 + kψ2 2 . Compare these expression with those given in where kψ2 = 2(1 − b)/ξab Eq. 6.129 in Chapter 6, for the case where the magnetic field is parallel to the c-axis. ˆ These expressions are a bit more precise than those given there and in Subsection 8.5.1, in that they explicitly also incorporate the core-contribution to the elastic moduli. Generalization of the above Eqs 8.44a and 8.44b for parallel flux lines (kz = 0) for the case where the magnetic field is tilted away from the c-axis ˆ was given by Sardella [106]. The corresponding generalization of Eqs 8.44a and 8.44b for the case kz = 0 has not yet been achieved. In the above, ω0 is the spatial average of the square of the Ginzburg–Landau function in the ground state of the Abrikosov flux-line lattice. Since we will not need an explicit expression for this quantity here, we do not specify it further. Moreover, the uniaxial anisotropy is manifest through the parameter mc /mab , where mc is the normal-state quasiparticle mass in the z-direction, while mab is the quasiparticle mass in the ab-plane. Another way of writing this is mc /mab = λ2c /λ2ab . The shear modulus of the Abrikosov flux-line lattice is for all practical purposes k-independent. In the present geometry, where the external magnetic field is directed along the axis of uniaxial anisotropy, the shear modulus will be that of an isotropic superconductor, since only shearing in the ab-plane makes any physical sense in this case. Thus, the shear modulus is given by

c66 =

Bc2 b(1 − b)2 µ0 8κ 2

(8.45)

FLL ELASTICITY AND PINNING

221

Several things are worth noting about these expressions. First of all, when k → 0, all effects of uniaxial anisotropy, manifest through the parameter mc /mab , vanishes. Note also that when k = 0, the maximum value of c44 and c11 occurs at the upper critical field, as a function of magnetic field. Using the dimensionless wavevector q = k/, the above expressions for c44 and c11 may be written

1 B 2 (1 − b) mab 1 c44 (q) = (8.46) + 2 + (m /m )(q 2 + m2 ) µ0 2bκ 2 mc q⊥ 2bκ 2 ab c z λ q 2 + (mab /mc )m2λ B 2 (1 − b) c11 (q) = 2 + (m /m )(q 2 + m2 )) µ0 2bκ 2 (q 2 + m2λ )(q⊥ ab c z λ

1 (8.47) − 2 q⊥ + (mab /mc )qz2 + m2ξ where we have introduced the ‘mass’-parameters m2ξ = (1 − b)/b and m2λ = (1 − b)/2bκ 2 . Now, another interesting feature of the wave-vector dependant moduli becomes evident. For finite k(q), they vanish at the upper critical field, in contrast to the k = 0 moduli, which acquire their maximum at that value of the magnetic field. This means that those Fourier modes that are most relevant for melting the flux-line lattice, become particularly soft as the magnetic field approaches the upper critical field limit. This is true for the case of uniaxial anisotropy, as well as for the isotropic case. It substantially contributes to melting the flux-line lattice well below the upper critical field line, and is a key feature which leads to a suppression of the melting line below the upper critical field even for moderately small Lindemann parameters c. To determine d2 (T ) from Eq. 8.42, we have to integrate over the entire circularized Brillouin-zone 0 < q⊥ < 1. Therefore, it is evident that a fully non-local theory, i.e. an elastic description with wave-vector dependant moduli, is essential. For arbitrary field and temperature, the necessary integrals in Eq. 8.42 can only be done numerically, however with some limitations (that turn out to be not very restrictive in strong type II superconductors), analytic results can be obtained that provide key insights into the main physical parameters controlling the position of the melting line. We proceed by writing d2 (T ) = d21 (T ) + d22 (T )

(8.48)

where d21 (T ) is the contribution to Eq. 8.42 containing the shear modulus, while d22 (T ) is the contribution to Eq. 8.42 containing the bulk modulus. For b > 1/2κ 2 we find

2 kB T mc 2bκ 2 √ d21 (T ) = ( 2 − 1) (8.49) 0 c0 4π c44 mab 1 − b 66

222

MORE ON THE FLUX-LINE SYSTEM

while under the condition b > 1/2κ 2 and (1 − b)/b 1 we find

kB T 2 mc bκ 2 2 d2 (T ) = 0 c0 4π c44 mab 1 − b 11

(8.50)

0 and c0 are the elastic moduli given above taken at k = 0. The factors Here, c44 11 in square brackets in each term is what we would have obtained had we used k-independent elastic moduli in the calculation. The other factors enter into the expressions only because the k-dependence of the elastic moduli is taken into account. Note that if we had ignored the k-dependence, the enhancement factors both coming from the large value of κ in extreme type II superconductors, as well as the enhancement factor coming from the mass anisotropy, would have been missed. Below, we shall identify a dimensionless parameter that explicitly shows how dramatic the effect of including non-local elastic moduli really is. 0 and c0 , thus finding To see this, we introduce explicit expressions for c44 11 √ √ 4( 1 m t b 2 − 1) c (8.51) d2 (T ) = + 1 l2 √ √ 2π mab 1 − t 1 − b 1−b

Hence, the Lindemann melting criterion is given by √ √ t 4( 2 − 1) b mab 2 c ≡α + 1 ≥ 2π √ √ mc 1−t 1−b 1−b Here, we have introduced the Ginzburg criterion parameter 2 kB Tc µ0 x 2 = 02 ξ 4π Bc2 ab and t = T /Tc . The dimensionless parameter α is given by 0 B c2 mab 1 α = 2 × 107 c2 mc κ 2 Tc2

(8.52)

(8.53)

(8.54)

This parameter essentially controls the position of the melting line in the (B, T ) phase diagram. In Eq. 8.54 we have again singled out in square brackets what we would have obtained for α had we only used local elastic moduli, the other two factors involving the mass ratio and the Ginzburg–Landau parameter κ appear exclusively due to non-locality in the elastic description of the flux-line lattice. If α is very large, it is clear from Eq. 8.52 that t and b need to be very close to unity for the melting criterion to be satisfied. A reduction in α facilitates a suppression of the melting line below the upper critical field line. In conventional supercon0 = 1 T, T = 10 K, and m /m ≈ 1. If ductors, typically we have κ ≈ 1, Bc2 c c ab

FLL ELASTICITY AND PINNING

223

we set c = 0.1, we have α ≈ 104 . In high-temperature superconductors, on the 0 = 100 T, T = 100 K, and m /m ≈ 100. other hand, we have κ ≈ 100, Bc2 c c ab −1 This gives α ≈ 10 , which is a reduction of nothing less than five orders of magnitude. Notice that the factor in square brackets in the expression for α is about the same in conventional moderate type II superconductors and extreme type II high-temperature superconductors, namely of order 107 c2 . The reduction in α originates exclusively in mass anisotropy and large value of κ. It is therefore an intriguing fact that the enhancement of Tc in high-temperature superconductors compared to conventional low-temperature superconductors in itself does not contribute substantially to suppressing the melting line below the Bc2 line, since the enhancement of Tc is cancelled by the enhancement of 0 . Bc2 However, once non-locality is included and mass anisotropy and large values of κ explicitly come into play, then the melting line is suppressed well below the upper critical field line, and the liquid phase of the flux-line system should be easily experimentally accessible. The one dominant feature which makes this possible, is not first and foremost the mass anisotropy, but rather the large value of the Ginzburg–Landau parameter κ, notice how it is the square root of the mass anisotropy that enters in the melting criterion while it is the square of the Ginzburg–Landau parameter which is relevant. Once more, it is the use of a nonlocal elastic theory of the flux-line lattice which brings out the dependence of both the mass anisotropy and the Ginzburg–Landau parameter. It is in particular the factor 1/κ 2 which brings the melting criterion above in reasonable agreement with experiments [98] for a sensible Lindemann parameter c ≈ 0.4, and the √ factor mab /mc which distinguishes between flux-line lattice melting in YBCO and BSCCO in a manner consistent with experiments [98]. In a deep sense, the sensitivity of the melting criterion to κ reflects the softness of phase-fluctuations of the superconducting order parameter in strong type II superconductors. This is because large values of κ are due to small values of the superfluid density in these compounds. On the other hand, the superfluid density is nothing but a measure of the stiffness of phase fluctuations. We shall have much more to say about such fluctuations in Chapters 9 and 10. In closing this subsection, we emphasize that the above is not a theory of melting of the flux-line lattice, the Lindemann criterion is after all just that, a criterion. It does however provide useful insight into what parameters that determine the position of the melting line, provided the assumption of a first order melting transition is correct. In fact, numerous Monte Carlo simulations and experiments now strongly indicate that this is indeed so. See for instance the work of Hetzel and co-workers [107] for the first demonstration through large-scale Monte Carlo simulations that the Abrikosov vortex lattice melts in a first order melting transition, and the contemporary experimental work of Safar and colleagues [108], showing pronounced hysteresis in resistivity data at what was interpreted as a melting transition of the flux-line lattice.

224 8.5.6

MORE ON THE FLUX-LINE SYSTEM

Modelling non-linear vortex diffusion

The voltage–current characteristics in many high-Tc superconductors are well described by a power-law over many orders of magnitude in the electric field. This has been found directly from transport measurements, and indirectly from the magnetic relaxation. It seems to be the general behaviour for YBCO- and BISCCO-based compounds, as well as for the Hg-based cuprate superconductors. As pointed out before, the power-law E–J-characteristics is most commonly interpreted as a result of thermally activated flux creep with a pinning barrier diverging slowly as the current vanishes, i.e. U (J ) ∝ log(Jc /J ) or U (J ) ∝ (Jc /J )µ , with µ small. Although there is evidence for some curvature in log(E) versus log(J ), the power-law may still serve as a first order approximation and as a model description of the voltage–current characteristic of high temperature superconductors. An analysis of the magnetic relaxation due to a power-law, with static boundary conditions, has been given by Vinokur and Feigel’man [109] and by Gilchrist and van der Beek [110]. Analysis of the AC-losses due to a power-law has been given by Rhyner [111] who considered an AC magnetic field at the surface of a superconducting semi-space. Such a configuration would apply to a real sample when the characteristic penetration depth of the field is small compared to the sample thickness or radius. In the following we consider the situation from zero to full penetration of a cylindrical sample, infinite in the axial direction. The boundary condition is a sinusoidally time-varying magnetic field applied at the surface, and the AC-susceptibility is calculated for different n-values. The numerical results are compared to experimental susceptibility data on a YBCO single crystal. The power-law can be written in dimensionless units as n E J = (8.55) E0 J0 By letting n vary from n = 1 to n = ∞, one covers a full class of cases ranging from ohmic with ρ = E0 /J0 , to the ideal critical state superconductor with a well-defined critical current density Jc = J0 , as illustrated in Figure 8.12. In terms of vortices and vortex dynamics, the limit n = ∞ represents the static critical state in which the vortex density gradient is balanced by the pinning force Fp = J0 B. When n has some finite value, this is equivalent to a relaxation of the critical state, e.g. by thermally activated creep. Now consider an infinitely long cylindrical sample of radius a in an axial magnetic field B = Bac sin(ωt). Maxwell’s equations for the field in the sample in cylindrical coordinates read ∂B 1 ∂ (rE) = − r ∂r ∂t ∂ B = −µ0 J ∂r

(8.56) (8.57)

FLL ELASTICITY AND PINNING

225

1.0

0.8

E/ E0

0.6 n=1 0.4 n=4 0.2 n = 20 0.0 0.0

Figure 8.12

0.2

0.4

0.6 J / J0

0.8

n=∞ 1.0

1.2

Power-law curves for different n-values from Eq. 8.55.

where E and J are azimuthal field and currents, while the B-field is in the axial direction. Next we introduce the dimensionless variables b = B/Bac , ζ = r/a and τ = ωt/2, and aualyze the above equations with respect to the reduced magnetic field b, obtaining n

∂b a n+1 ∂b ∂b 1 ∂ ζ = × sgn ζ ∂ζ ∂ζ δ ∂τ ∂ζ

(8.58)

Here sgn denotes the sign function, and the characteristic length-scale δ represents a generalized penetration depth which can be written as (n−1)

2

(n+1) δ = δcl(n+1) × δBean

(8.59)

where δcl = 2E0 /µ0 ωJ0 is the classical skin depth in the linear limit (n = 1) and δBean = Bac /µ0 J0 is the Bean penetration depth in the critical state (static) limit (n = ∞). The combined depth δ reduces to its appropriate limits δ = δcl and δ = δBean when n = 1 and n = ∞ respectively. The total magnetic flux in a cylindrical sample of radius a is (t) = 2π

a

B(r)r dr,

(8.60)

0

and the complex susceptibility, χ = χ + iχ , is a measure of the first harmonic Fourier components of the spatially averaged flux density,

226

MORE ON THE FLUX-LINE SYSTEM

χ + 1 = χ =

1 2 π a Bac 1 π a 2 Bac

2π

(t) sin ωt d(ωt) ωt=0 2π

(t) cos ωt d(ωt).

(8.61)

ωt=0

The susceptibility can be calculated exactly in both the linear [112] and the critical state [113] limits. In the linear limit one finds 1 + χ = 1 + χ + iχ =

2J1 (ka) kaJ0 (ka)

(8.62)

with k = (1 + i)δcl and J0 (ka) and J1 (ka) denote Bessel functions of zero’th and first order respectively. (For a London superconductor k = 1/λ, which results in loss-free screening currents and χ = 0.) In the limit n = ∞ Eq. 8.58 reduces to the critical state equation, ∂B/∂r = ±µ0 J0 [111]. The susceptibility can then be found by calculating the critical state profiles for a cycle of the surface field and integrating over space and time. This has been done by Clem [113], and the solution reads χ = g1 (x) χ = g2 (x)

(8.63)

where x = Bac /B ∗ = Bac /µ0 J0 a, and g1 (x) and g2 (x) are known polynomials of x and sin−1 (x −1/2 ). In the linear case the susceptibility will depend on the frequency of the AC field, but not on the amplitude, while in the critical state limit the situation is the opposite, a behaviour which is also reflected in δ. Moreover, in the linear limit the response is purely harmonic while for n > 1 the response is anharmonic, resulting in an infinite set of higher order susceptibility terms. The AC susceptibility can be measured over a wide range of penetration, often by varying either the temperature or the static background magnetic field, or both. A maximum in the loss component χ is observed when the penetration depth is of the order of the sample radius, i.e. when 2

(n−1)

(n+1) ∼a δcl(n+1) δBean

(8.64)

or

2E0 µ0 J0 ω

1 (n+1)

Bac µ0 J0

(n−1) (n+1)

∼a

(8.65)

In the exact limits the conditions for a peak maximum in χ is δBean = a and δcl a/1.77, respectively. By taking the differential of Eq. 8.65 we find the

FLL ELASTICITY AND PINNING

227

relation d ln(ω)/d ln(Bac ) = n − 1. These differentials can be found experimentally by measuring the shift in the loss maxima (e.g. with temperature) as a function of both amplitude and frequency of the AC field. Such experiments may therefore be used to obtain the value of n directly. Numerical values of χ and χ were calculated [93] for different values of n by letting the ratio δ/a vary from zero to some large number 1. B(r, t) was found by solving Eq. 8.58 by means of finite differences, and χ and χ were found by integrating in space and time according to Eqs 8.60 and 8.61. A convenient way of plotting susceptibility results is the Cole–Cole plot, in which χ is plotted as a function of χ . We now make a comparison of the numerical results with experimental susceptibility data obtained on a single crystal YBCO. The data used here are only a small subset from a wider experimental study [114]. The crystal sample was cubic with sides 1 mm, and due to such a non-ideal sample shape, a comparison is only of a semi-quantitative nature. The susceptibility was measured as a function of temperature in different DC fields ranging from 1 to 8 T and with an AC field of amplitude 10−4 T, and frequency 121 Hz. The measured χ (T ) and χ (T ) are shown in Figure 8.13 and in a Cole–Cole plot in Figure 8.14. The data collapse in Figure 8.14 shows that the same process is governing the susceptibility behaviour for all curves, occurring at different temperatures 1.0

1 + c′

0.8 0.6 8T

7T

5T

4T

3T

2T

1T

0.4 0.2 0.0

)

c′′

0.2

0.1

0.0 70

75 Temperature (K)

80

85

Figure 8.13 AC susceptibility data on a single crystal YBCO, with Bc at 121 Hz. Applied fields have corresponding values in the upper and lower panel. After Gj¨olmesli [93] and Karkut et al. [103].

228

MORE ON THE FLUX-LINE SYSTEM

c′′

0.3

n=1

0.2 n→∞ 0.1 B||c Bac = 10−4 T DC fields 1, 2, 3, 4, 5, 7, 8 T

0.0 0.0

0.2

0.4

0.6

0.8

1.0

1 + c′

Figure 8.14 Cole–Cole plot of the susceptibility data shown in Figure 8.13. The plotted data follow the n = 1 curve at the highest values of 1 + χ , corresponding to the highest temperatures. But at some point they switch over to a non-linear domain with n 1. This is the freezing point of the lattice. Data Aualysis: Ref [93] from Karkut et al. [103].

determined by the DC field. In other words, the susceptibility can be written as a function of a single variable which changes monotonically with temperature and field. At large penetration, χ + 1 1 the data follow closely the linear curve n = 1. Then at some particular value 1 + χ 0.95 and χ 0.2, the curve makes a small jump into the non-linear region with n > 1. Moreover, the linearnonlinear jump is rather sharp, occurring over less than 0.2 K, indicative of a phase transition of the vortex state, possibly from a vortex liquid to a vortex glass [93]. We conclude that the non-linear diffusion due to a power-law E–J-characteristic gives a generalized penetration depth δ which reduces to the classic skindepth and to the Bean penetration depth in the appropriate limits. The peak shift in χ with respect to amplitude and frequency can be used to determine the value of the exponent n. The non-linear diffusion equation was solved numerically and the complex magnetic susceptibility was calculated, in order to be compared to experimental data. By plotting χ versus χ the experimental data collapse occurred, with indications of a sharp transition from a vortex liquid state with linear dynamics into a state of non-linear dynamics, possibly a vortex glass.

8.6 Flux-line entry at Bc1 : thermodynamic and geometric restrictions 8.6.1

The critical field Bc1

The mixed state of a superconductor is one where the superfluid phase coexists with the flux-line lattice, a vortex glass, or with the flux-line liquid. When

THERMODYNAMIC AND GEOMETRIC RESTRICTIONS

229

an applied magnetic field is increased from zero, the superconductor is first in the Meissner phase, with complete shielding. At a certain value of the applied field Hc1 = µ10 Bc1 it becomes energetically favourable to have flux-lines created near the surface, and for these to penetrate the body of the superconductor. A thermodynamic analysis to determine Hc1 starts by writing down the Gibbs free energy G when n vortices per area are inside and far apart so that their mutual interaction can be neglected. We now have: G = nF − BH

(8.66)

where F is the vortex line energy previously determined in Chapter 6. This is an excellent approximation very near Hc1 where in principle even a single flux-line can penetrate alone. Since the average field is B = n0 , we make this substitution, and find F −H (8.67) G=B 0 The lowest value for G as long as the expression in the parenthesis is positive, is G = 0, corresponding to B = 0, as expected for a system in the Meissner phase. A simultaneously positive value of the expression in parenthesis signifies stability against vortex entrance, consistent with Meissner screening. However, when the expression in the parenthesis is negative, i.e. when H > F /0 , G can be lowered below the Meissner-state value G = 0 by B = 0. A finite B means that flux has entered, and that the energy G is lower than in the Meissner state, which is consistent with instability towards flux penetration. The critical field at which the instability occurs clearly is F 0 λ Bc1 = +ε (8.68) = ln 0 ξ 4π λ2 as derived before.

8.6.2

The Bean–Livingston barrier

When a vortex is created near the surface of a superconductor in the Meissner state two opposing forces act on it. The screening currents create a Lorentz force normal to a flat surface, attempting to move the vortex into the material according to fx,L = 0 jy

(8.69)

230

MORE ON THE FLUX-LINE SYSTEM

as shown in Eq. 6.110. We can write this as fx,L = 0

H −x e λ λ

(8.70)

reflecting the decay of the screening current into the superconductor. The second force is the image force attracting the vortex to the surface. Using the result in Eq. 6.106 where the distance between the vortex and its image is 2x, the interaction energy which is now negative, becomes U12

20 2x =− K0 λ 2π µ0 λ2

Taking the derivative, and making use of the relation these Bessel functions the resulting image force is fx,im

(8.71) d dx K0 (x)

= −K1 (x) for

20 2x =− K1 3 λ 2π µ0 λ

(8.72)

We now evaluate the force at x = ξ , since this is as close as we can approach the surface using the vortex model. The sum of opposing forces is fx = fx,L + fx,im

20 H −ξ/λ 2ξ = 0 e − K1 3 λ λ 2π λ

(8.73)

The total force is zero at field ξ 0 2ξ eλ K1 Hsb = 2 λ 2π µ0 λ

(8.74)

which is called the surface barrier field for obvious reasons. Furthermore, using the property of the Bessel function lim K1 (x) =

x→0

1 x

(8.75)

for ξ λ one finds lim Hsb =

1 0 = √ Hc 4π µ0 ξ λ 2

(8.76)

This is the surface barrier field at which the net force against flux entry is zero. This barrier field has important implications. As an example, in microwave applications where flux entry would represent a loss factor it is important that Hc in type II superconductors like Nb is much greater than Hc1 . To take full advantage of this situation the surface should be smooth, at least on the scale of λ,

THERMODYNAMIC AND GEOMETRIC RESTRICTIONS

231

∆G

H > Hsb 0

x

(c)

Figure 8.15 Sketch of the Gibbs energy from which the two opposing forces active in the Bean–Livingston barrier are derived. At H = Hsb the slope of the curve at the origin will be zero, providing free entry of flux.

since the force found above is calculated under the assumption of a flat surface. Figure 8.15 shows how the Bean–Livingston barrier [115] can be viewed and understood to operate. In most real situations sample shapes and surface conditions will allow flux entry of static fields near Hc1 . Normally Hsb will be the entry field only when special precautions are taken.

232 8.6.3

MORE ON THE FLUX-LINE SYSTEM

Geometric barriers

The concept of a geometric barrier was introduced by Zeldov and coworkers [116] and discussed also extensively by Brandt [117]. This is a shape dependent barrier which can be explained qualitatively by reference to the sketch in Figure 8.16. A sample S of thickness d, with sharp corners is placed in a magnetic field. Near the sharp corners the local field is enhanced considerably compared to the applied field H , and therefore penetrates first at these points. This undermines the opposing forces due to the Bean–Livingston barrier. However, for the flux line to enter, the length of flux line Lf as seen in the figure, has to be considerably longer than just Ls = d, which would be the length corresponding to penetration along the flat outer surface. If we approximate the length Lf by a half circle at the point when it just leaves the surface we estimate that Lf ∼ π d2 . The flux line therefore was stretched by an amount L = Lf − Ls ≈ (π − 2)

d d ∼ 2 2

(8.77)

compared to the length it would have in the centre of the specimen. Notice also that Figure 8.16 indicates that a vortex line has jumped directly to the centre of the sample once it entered. This is because here again the length inside the sample is only equal to d. Alternatively we may say that the flux line was driven to the centre by the Meissner currents discussed before. Hence it is energetically advantageous to travel all the way to the centre in case of no pinning. The energy cost of creating the flux line near the surface is therefore raised by ∼50% due to sample geometry in this simple estimate. Consequently we may expect the flux entry field to be raised by an amount which is of the same order of magnitude as Hc1 itself. Obviously, the effect is strongly shape dependent, hence its name. In case of elliptical crossection it may be shown that there is no geometrical barrier.

d 2 S

Lf

d

d 2

Figure 8.16

Sketch illustrating flux entry in the presence of a geometrical barrier.

CRITICAL CURRENT ISSUES

233

This effect also has an associated hysteresis, since there is no corresponding barrier against flux exit. The geometric barrier therefore is recognized experimentally by hysteresis in magnetisation experiments even in the absence of pinning. The additional effect of pinning was discussed by Brandt [117].

8.7 Critical current issues 8.7.1

Critical current in the Meissner state

According to the London equation there is a relation between the supercurrent density and the magnetic field at any point in the superconductor. In the Meissner phase, due to screening, the current and field can only penetrate to a depth measured by λ. Due to the correspondence between J and H it does not matter whether J is the sum of a transport current and a screening current. Experiments show that there is a critical current density Jc above which screening and superconductivity break down. Due to the equivalence of transport current and screening current it is to be expected that superconductivity breaks down when the total current density–the sum of transport and screening current–exceeds the critical current density Jc . The famous Silsbee hypothesis states the converse: A superconductor looses its state of zero resistance when the total magnetic field strength due to transport current and the applied field exceeds the critical field strength Hc . Mainly because of large variations in charge density, λ may vary by an order of magnitude, from ≈15 nm in good polyvalent metals to 150 nm in YBCO. What we have then, in a surface layer of thickness 15–150 nm, is a decaying screening current and an associated magnetic field which are locally related in the London approximation. With a field H created by a current J along a cylindrical rod, the H -field is circular in the plane normal to the rod with radius ∂ a. We get ∂r Hθ (r) = J from Maxwell’s equations ∇ × H = J , leading to J =

Hθ (a) λ

(8.78)

where Hθ (a) is the value of Hθ at the surface. Now, if we allow J to reach Jc , this corresponds to Hθ (a) = Hc . In other words: Jc =

Hc λ

(8.79)

This is the relation which holds in the Meissner state, and therefore is valid in type I as well as type II superconductors. It is worth noting that this rule is very similar to the one we derived for Jc in the Bean critical state. In that case Jc was also given by a field divided by a length, namely M/d. Since H and

234

MORE ON THE FLUX-LINE SYSTEM

M are in the same units, what these expressions have in common, is that the gradient of the field gives the critical current. Does the relation Jc = Hc /λ reconcile with a calculation based on Ampere’s law? If the superconducting rod is of radius a, and the total current is I , the field at the surface, Hθ (a) is given by I = 2π aHθ (a)

(8.80)

or, if the current is strong enough to reach Hc : Ic = 2π aHc

(8.81)

Equation 8.81 looks different from Eq. 8.78. But for real comparison we have to introduce the current density, J = I /Aeff = I /2π aλ;

I = 2π aλJ

(8.82)

Here, the effective area was written as Aeff = 2π aλ, since a λ. We now find 2π aλJc = 2π aHc , which leads to Jc =

Hc λ

(8.83)

and we have recovered the answer we had before, in Eq. 8.79.

8.7.2

Depairing critical current

Calculations of critical current density can be carried out using Ginzburg–Landau as well as BCS theory. Except for a numerical factor they come out with essentially the same result: Jc ≈

Hc λ

In Ginzburg–Landau-theory the exact result is √ Hc 2 2 Hc Jc = √ 0.54 λ 3 3 λ

(8.84)

(8.85)

In BCS theory the kinetic energy added to the system by turning on a current J , has to be compared to the energy gained by forming the Cooper-pairs. When the kinetic energy equals the pair condensation energy we have the critical current

CRITICAL CURRENT ISSUES

235

density. The condensation energy can be expressed on the basis of thermodynamics as ( 12 µ0 )Hc2 , and from BCS theory as 12 N (0)2 , where N (0) is the normal density of states at the Fermi level, and is the BCS energy gap. This would give Hc2 = µ0 N (0)2 Using Jc = Hλc we find Jc = nomenology and BCS.

(8.86)

√

µ0 N (0)2 λ

as a mixed expression between phe-

Example Measurements in a 1-mm diameter wire have given critical current at 0 K: Ic = 75 A. With a = 0.5 mm, λ = 5.1 × 10−6 cm; Jc (0) = 2πIcaλ = 4.7 × 107 A/cm2 . A simple estimate of Jc based on the basic formula Jc = Hc /λ gives typically, with µ0 Hc ≈ 0.1 T and λ ≈ 100 nm: Jc =

Bc = 1012 A/m2 µ0 λ

Often such values are quoted in A/cm2 , in this case: Jc ≈ 108 A/cm2 . This is the maximum ideal current density the superconductor can sustain under any circumstance. There are many reasons why one does not reach this value in practical cases. The most important obstacles are typically flux motion and grain boundary problems, particularly in high-Tc cuprates. Yet, often one finds that real materials can come within a factor of 2–3 of this pair-breaking current.

8.7.3

Reduction of Jc at grain boundaries

So far we have discussed the idealized situation as far as critical current density Jc is concerned. These considerations give a good idea of what maximum of critical current density we can expect in a superconductor. However, there are many mechanisms by which Jc may be reduced, even substantially. Of course, if in a granular material the grains do not join together well, for instance due to a transition layer of different composition between the grains, this has a strongly derogative effect. High-Tc materials are known for their short coherence length ξ . In a transition layer the wavefunction ψ may be depressed over a distance ξ without bridging properly across the boundary, in which case little current can pass across the interface, except by tunnelling which may be very weak. In addition, due to the dx 2 −y 2 character of the wavefunction in high-Tc cuprates several misorientation effects at the microscopic level are possible, each representing an obstacle to current transport, and hence to reduction of Jc [118]. These mechanisms are illustrated in Figure 8.17. Referring to this figure

MORE ON THE FLUX-LINE SYSTEM

+

+

−

|∆|

x

x

+

−

−

+

+

−

(b)

+ −

Large Jc

j = ∆j

+

−

−

+

Small Jc

+ −

− +

I

+ −

j = ∆j + p

+

− +

+

− +

−

Position

−

(a)

(c)

+

−

− +

−

236

− +

Figure 8.17 Illustration of different mechanisms by which Jc may be reduced at grain boundaries in high-Tc dx 2 −y 2 type superconductors. After Hilgenkamp and Mannhart [118].

the mechanisms are from top down: In Figure 8.17a two adjoining grains are differently oriented, causing a depression of the wavefunction over a distance ξ due to frustration caused by misorientation of CuO2 -planes. In Figure 8.17b one sees a case of alignment of the lobes of the dx 2 −y 2 function allowing a high Jc , and a misalignment causing a small Jc . Finally in Figure 8.17c a faceted grain boundary facilitates the current in one channel, and opposes it in the other. The result is lower Jc .

8.7.4

Relaxation of magnetic moment and the irreversibility line

Soon after the discovery of high-Tc superconductors by Bednorz and M¨uller, the IBM team also found an important difference between low-Tc and high-Tc

CRITICAL CURRENT ISSUES

237

superconductors when exposed to a magnetic field [119]. Essentially the discovery was that in a broad temperature region below Tc (H ) the superconducting properties were reversible, corresponding to critical current Jc = 0. Only below a much lower temperature Tirr (H ) did the behaviour shift to irreversible, corresponding to Jc = 0. This created a dividing line in the (H, T )-plane, later called the irreversibility line. Furthermore, this line was not a fixed line, determined once and for all for a given material. Rather, in a given sample the experimentally determined location of the irreversibility line Tirr (H ) depended on the characteristic measuring time of the experiment, and in samples of the same nominal composition it would depend also on sample history. These effects are present to some extent in all superconductors, but to a far less degree in low-Tc than in the cuprate high-Tc materials. What is going on can briefly be described as follows: After a certain arrangement of vortices has been established, typically after application of a magnetic field, and subsequent removal of the field to observe the vortex dynamics, vortices will leak out of the sample, leaving the most shallow pinning sites first. As time passes, the depinning process goes slower since the vortices have to climb higher and higher barriers in order to leave their pinning sites. The process goes on indefinitely, all the time at a slower rate. This effect is most clearly demonstrated by observing the decay of the magnetic moment m(t) originally present as mi at a time ti when the field is switched off, and then monitoring the relaxation process over decades of time. The observed time-dependent magnetization is typically such that the magnetic moment, when plotted versus time on a double logarithmic scale, decays linearly, i.e. the functional dependence is a power law. Due to the relatively strong decay observed in high-Tc materials the behavior in these was termed ‘giant flux creep’ [120]. In Figure 8.18 we give an example of magnetization decay measurements at several temperatures in a wide range, observed in a thin film of Bi2223. The decay was monitored by a squid, located in a superconducting chamber, shielded against outside signals except for the signal picked up by a gardiometer coil surrounding the sample. Measurements started immediately after switching off a 10 mT field from a small solenoid surrounding the sample, starting the flux leakage from the sample [121]. Below 50 K the decay is seen to be quite linear in the double logarithmic plot over 4 decades in time, except for a small deviation in the long time limit (t ≥ 100 s) at the highest temperatures. The dominating decay behaviour may be expressed simply as −S t m = mi (8.87) ti where the exponent S is S = ∂(ln m)/∂(ln t). For temperatures T ≥ 50 K a crossover to faster dynamics is apparent, as would be expected in a crossover to vortex liquid. In this range the data are relatively noisy, due to the low magnetic moment.

238

MORE ON THE FLUX-LINE SYSTEM 10 20 K

m (a.u.)

1

10−1 47.5 K 55 K 10−2 50 K 60 K 10−3 10−1

1

102

10

103

104

t (s)

Figure 8.18 Relaxing irreversible magnetic moment in a Bi2223 film after a field step of −10 mT is applied at different temperatures. The flux is leaving the sample, and shielding currents decay proportionally to the decrease of the magnetic moment. The temperatures are from top to bottom: 20, 25, 30, 35, 37.5, 40, 42.5, 45, 47.5, 50, 55, and 60 K. The c-axis oriented thin film with Tc = 97 K was grown by metalorganic chemical vapor deposition (MOCVD) by Endo and coworkers at the Electrotechnical Laboratory in Japan. The measurements are by Tuset et al. [122].

The above experiment makes very clear why the so-called irreversibility line depends on the timescale of the experiment: The longer timescale is allowed in a given experiment, the more of the magnetization decay is integrated into the observation. To illustrate the consequences of this, we refer to Figure 8.19 where the position of the peak in the loss component of the dynamic susceptibility was measured as a function of temperature at different frequencies and field directions. The excitation field was parallel to the static magnetic field. Figure 8.19 shows the irreversibility line as measured by AC susceptibility in YBCO crystal at a range of frequencies. Here the line is determined as the locus of points where the loss peak in the imaginary part of the susceptibility χ appears in the (H, T )-plane. We clearly see the effect of changing the time-scale of the experiment: With increasing frequency the Tirr (H ) line moves up in temperature. The question is now how this line can be described quantitatively, or at least semiquantitatively. A crude argument which gives some insight, but without taking into account the collective effects we discussed before, goes as follows: Assuming that pinning occurs at pin points of volume Vc , the energy gained by having a flux line pass through this volume is equal to the condensation energy U = 12 µ0 Hc2 (T )Vc

(8.88)

CRITICAL CURRENT ISSUES

8

239

H⊥c H||c

m0 Hdc (T)

6

4

f (Hz)

2

12.1 121 1.21 k 12.1 k 121 k

0 70

75

(a)

80 T (K)

85

90

0T

90

0.4 T 1.5 T T (K)

85

4T

80

6T 75

8T

10 (b)

H||c 102

103 f (Hz)

104

105

Figure 8.19 Irreversibility line measurements (a) at various frequencies in YBCO with H c-axis and H ⊥c-axis. The bottom, (b), figure shows how the irreversibility line with H c is shifted to higher temperature with increasing frequency. After Karkut et al. [103].

Assume further that Vc may be written as a02 ξ(T ) where a02 is the correlation area in the transverse direction given by the flux-line lattice constant. The critical field has almost linear temperature dependence in the field range we are discussing 1 in high-Tc materials, i.e. Hc ∝ (1 − T /Tc )1 and ξ(T ) ∝ (1 − T /Tc )− 2 in the mean field approximation, as in Ginzburg–Landau theory. The result is, when inserting the expression for a0 = 1.075(0 /B)1/2 that

240

MORE ON THE FLUX-LINE SYSTEM

U=

U0 1 − B

T Tc

n ;

n = 1.5

(8.89)

In order to test this line of thinking, Sagdahl [123] analysed a relaxation model for the permeability, writing the two components on the usual Debye form 1 1 + (ωτ )2 ωτ µ = 1 + (ωτ )2 µ =

(8.90) (8.91)

The relaxation time is expected to be τ = a/Rl where l is the typical jump distance, R is the flux jump rate and a is a macroscopic distance describing the total depth of penetration of flux. We rewrite this as τ = (a/f0 l) exp(U/kB T )

(8.92)

Here f0 is an attempt frequency, and U is the pinning potential already introduced. The maximum in µ occurs at ωτ = 1, setting the criterion for B and T to be on the irreversibility line as B ∗ and T ∗ at a selected frequency and AC amplitude. Using this criterion we arrive at the following condition for the irreversibility line: U = − ln(ωτ0 ) kB T ∗

(8.93)

where τ0 = (a/f0 l). Next, inserting the expression for U arrived at previously we find that Eq. 8.93 converts to U0 (1 − T ∗ /Tc )n /kB T ∗ B ∗ = − ln(ωτ0 )

(8.94)

where Aj is a parameter which we leave undetermined. Finally, we rewrite Eq. 8.94 as B ∗ = C(ω)(1 − T ∗ /Tc )n /T ∗

(8.95)

where C(ω) = −(U0 /kB ) ln(ωτ0 ). This constitutes an expression for the irreversibility line in the present analysis. In [123] this expression was tested, and found to agree with experiments, with n = 1.5 at the fields above 1.5 T, while n = 1 below. Furthermore, in fitting the expression the parameter Tc had to be taken with a value well below the zero-field value Tc (0). This shows that the model does not apply in the vicinity of Tc (0). The irreversibility line was found

CRITICAL CURRENT ISSUES

241

to be almost flat over several degrees below Tc (0). In other words very weak irreversibility was found in that temperature interval. Clearly pinning very close to Tc (0) at very low fields is quite different from that at high fields. This can at least partly be argued to be caused by twin boundaries taking a more prominent role as pinning centres when the flux line density is low, in which case the flux line dynamics may be altered substantially. It turns out that Eq. 8.89 agrees surprisingly well with experiments, considering the simplicity of the model, and the complexity of the real problem. Figure 8.20 gives an example of such overall agreement. Part of the reason should be ascribed to the fact that point pinning is important in YBCO due to the presence of oxygen vacancies as pinning sites. In the vicinity of the melting line the softening of the FLL strengthens the role of individual pinning. The irreversibility lines of high-Tc compounds are located well below the Hc2 line, and the difference is larger the more 2D-character the material possesses. This has represented a great challenge in the search for material processing methods suitable for attainment of high-Jc at reasonably elevated temperatures and in high magnetic fields. It is natural to ask how the irreversibility line is related to the melting line. The answer is that these are of different origin and largely independent, but not unrelated. The irreversibility line is determined for the decay of magnetisation current, in other words governed by flux line dynamics, while the melting line is a thermodynamic line and as such an equilibrium phase boundary, fixed in the (H, T )-plane for a given piece of material. The position of the melting line should be expected to depend somewhat on pinning 8

B* (T)

6

4

2

0

65

70

75

80

85

90

T* (K)

Figure 8.20 The irreversibility line B ∗ (T∗ ) in the field range 0 to 7.5 T (H c) determined from AC permeability measurements on an YBCO single crystal with f = 121 Hz and Bac = 3 × 10−4 . The solid and dashed lines represent theoretical fits using Eq. 8.95, with exponents n = 1.5 for fields higher than 1.5 T and n = 1 for fields lower than 1.5 T. After Sagdahl [123].

242

MORE ON THE FLUX-LINE SYSTEM

properties of the material. However, melting can only be observed in materials with relatively low density of pins. In pin-free materials each superconductor should possess a unique melting line. The irreversibility line is highly anisotropy dependent, as is the melting line as was shown in Figure 8.19 in two directions in YBCO. Clearly, both flux line dynamics and melting properties should be expected to be different in the two cases: When flux lines are along the c-axis they are free to displace sideways in two directions, while in the ab-plane they are packed parallel between superconducting CuO2 sheets and can only move sideways parallel to the ab-plane. This means that a thermal energy kB T has much less influence on the configuration of flux lines when the field is in the ab-plane than when it is along the c-axis. Therefore it is much harder to melt the FLL with the field in the ab-plane than along the c-axis. The melting line for field in the ab-plane is therefore much higher than with field along the c-axis. The statement made above that the irreversibility lines are independent but not unrelated can now be given more content: We see from Figure 8.19 that the irreversibility line is much steeper and higher up in temperature with field in the ab-plane than when it is in the c-direction. In this sense they are clearly related. But the irreversibility lines move as a function of frequency of the AC field, in this sense they are independent. The relationship between the two types of lines is due to the fact that time constants near phase boundaries depend stronger on temperature relative to T (H ) and tend to diverge at the phase boundary. A wide range of time constants is therefore available in the vicinity of the Tm -line. As it turns out the experimentally accessible time constants are in that same range. Hence the irreversibility line will appear not too far away from the Tm -line. A sketch of this is given in Figure 8.21.

8.7.5

How can Jc be increased?

The irreversibility line problem in high-Tc materials has been a serious obstacle against the development of wires and cables for many kinds of superconductor B Tm

Tirr

Bc2

Reversible

Irreversible Tc

T

Figure 8.21 Sketch of the irreversibility line Tirr and the melting line Tm .

243

CRITICAL CURRENT ISSUES

applications. Huge research efforts have been made to overcome it. The improvements which have been achieved are very impressive. Compared to the critical current densities obtained in the early stages of high-Tc research these systematic efforts have led to increased critical current density by many orders of magnitude. For a good example we refer to the topical contribution by Muralidhar and Murakami (Section 13.4) on a modification of YBCO-type material, where extremely strong magnetic fields may be stored in bulk material. The highest fields reached are so strong as to challenge the physical strength of the material itself due to the strong forces that the pinned vortex lattice causes on the structure. In the following we give some some more examples of results where the improvements are substantial. The first example is from the work of Krusin-Elbaum and coworkers [124]. In this case the mercury-based superconductor HgBa2 Ca2 Cu2 O6+δ , also referred to as Hg-1212, was subjected to 0.8 GeV proton bombardment which induced fission processes in Hg, leaving tracks in the material. These tracks created what is often referred to as ‘columnar defects’ in a ‘pinning landscape’ which reduced the vortex motion (creep) substantially. Figure 8.22 shows the resulting improvements in critical current density, as well as a big shift of the irreversibility line,

1.0 0.8

−0.1 T −1.0 T −2.0 T

R/RN

10

5

1.52 × 1017 cm−2

4

mo H( T)

J (106 A/cm2)

Unirr

0.4 0.2

1

Hg-1212

0.6

mo H = 2 T Irr

0.0

3

80 ∆Tirr

2

100 T (K)

0T 120

Irradiated

0.1 Unirradiated

1 Unirradiated

Hg-1212 0.01

0 0

20

40

60 T(K)

80

100

60

70

80

90

100 110 120

T(K)

Figure 8.22 The effect of proton bombardment at 0.8 GeV, with resulting fission fragments creating columnar defects in superconducting HgBa2 CaCu2 O6+δ . On the left the improvement of critical current is shown at various fields, with open and closed symbols showing the results before and after irradiation, respectively. The proton fluence of the irradiation was 1.52 × 1017 cm−2 . The figure on the right shows the corresponding shift of the irreversibility line, with the insert giving simultaneous resistivity changes [124].

MORE ON THE FLUX-LINE SYSTEM

500 nm

244

5 4 3

0

1

2

2 3

1

4

(a)

5 −H4

−H3

−H2 −H1

0

µm H1

H2

H3

H4

3 Pb/Ge 2

With antidot lattice

M(10−4 emu)

1 Without antidot lattice 0

−1

−2 T=6K −3 (b)

−96

−72

−48

−24

0 H(G)

24

48

72

96

˚ film with a square lattice of subFigure 8.23 (a) An AFM picture of a single Pb (500 A) micron antidots (periods d = 1 µm, radius r = 0.2 µm. (b) Magnetization loop M(H ) at ˚ ˚ 2 multilayers with and without the triangular antiT = 6 K of a (Pb (100 A))/(Ge (50 A)) dot lattice (d = 1 µm). The solid line is a fit following the logarithmic dependence of the magnetization between the matching fields Hm and Hm+1 . The dashed line is demonstrating the validity of the linear behaviour of M(Hm ). The loops were measured for M > 0 and symmetrized for clarity for M < 0 [125].

CRITICAL CURRENT ISSUES

Jc (106A/m2)

1.0

245

TP

0.5

TP1 0

Figure 8.24

3.5

4.0 Temperature (K)

4.5

Tc

4.8

The ‘peak effect’ demonstrated in NbSe2 [126].

moving it up by about 20 K at the highest field employed [124]. Since the irreversibility line is a borderline between regions where Jc = 0 and Jc = 0 this means that a much larger area of the (H, T )-plane is potentially useful after the irradiation. A different strategy was followed by Fossheim and coworkers [127] who were able to embed carbon nanotubes into Bi2 Sr2 CaCu2 O8+x . Due to the small diameter of the nanotubes, in the 10 nm range, they are suitable as columnar defects and can provide strong pinning. The next example, Figure 8.23 is from a thin film superconductor by V. Moshchalkov and coworkers [125]. In this case a thin film superconductor was modified by making a large number of holes, “antidots”, in the films, creating a regular lattice of holes. Each hole is capable of pinning one or more vortices. The measurements shown are magnetization vs. applied field in both the positive and the negative directions. The narrow inner curve shows, for comparison, the magnetization before making the holes in the film. The magnetization is very low, corresponding to a very low critical current density. In the upper curve, corresponding to measurements in the film with pinning arrays, the situation has changed dramatically: As the magnetic field is turned on, one finds a magnetization which is orders of magnitude higher than in the intrinsic case. In addition, some structure appears. The first peak corresponds to a matching of the number of holes with the number of vortices available for pinning, at the so-called ‘matching field Bφ ’. On further increase of the applied field, new matching conditions are found, representing two, and three vortices per hole, etc. A number of different geometries and variations in pinning strategies have been investigated. An interesting effect which arises in many superconductors when the temperature approaches Tc from below, is the appearance of a sharp maximum in the critical current density just before it goes to zero at Tc . This is the so-called ‘peak effect’, and is ascribed to collective pinning. It arises because the flux

246

MORE ON THE FLUX-LINE SYSTEM

line system softens on approaching Tc , as can be seen from the analysis we have done of the elastic properties of the FLL previously in this chapter. Since a softer vortex lattice is able to adjust more easily to the random positions of pinning centra, the vortices are now better pinned. However, as Tc is approached further, the Cooper pair density and the wavefunction diminish even more, and pinning vanishes altogether. Jc then must go to zero. The example given in Figure 8.24 is from Kes and coworkers on NbSe2 [126], with Tc = 7.1 K. Three characteristic temperatures are indicated in the figure, representing the minimum of critical current density reached below the peak temperature, the position of the maximum, and finally Tc where Jc goes to zero.

PART II

Advanced Topics

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

9 Two-dimensional Superconductivity. Vortex-pair Unbinding 9.1 Introduction In this chapter, we will go through the case of how superfluidity is destroyed in thin film superconductors or thin films of superfluids with a scalar order parameter. The starting point is the Ginzburg–Landau theory, now applied to two-dimensional systems. In this case, the distinction between superconductors (charged condensates) and superfluids (neutral condensates) vanishes. The reason is that in the case of superconductors, the effective London penetration depth is given by the bulk penetration depth λ and the thickness of the film d as follows λ λeff = λ d mq λ= µ0 ns q 2

(9.1)

where q is the charge of the carriers in the superconducting state, mq their mass, and ns their number density. We may thus write the effective penetration depth in the form mq λeff = . (9.2) 2 µ0 ns qeff Thus, when d → 0, this is equivalent to letting qeff → 0, and we thus effectively have a neutral condensate in this case. The physics of this is simply that in the case of an infinitely thin film λeff → ∞, thus precluding gauge-field fluctuations in the interior of the film. We therefore can ignore the vector potential A as an independent fluctuating variable in the action. In the presence of an external Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

250

TWO-DIMENSIONAL SUPERCONDUCTIVITY

field inducing vortices in the thin film, this would simply enter as appropriately twisted, but non-fluctuating, boundary conditions on the sample. Here, we shall for the moment ignore an externally imposed magnetic field.

9.2 Ginzburg–Landau description The Ginzburg–Landau theory in the two-dimensional case, regardless of the charge of the condensate, takes the form Fs (r, T ) = Fn (r, T ) + α |ψ|2 +

β 2 |ψ|4 + |∇ψ|2 2 2m

(9.3)

where ψ(r) = |ψ(r)|eiθ (r) is the complex scalar order parameter of the condensate. For the subsequent discussion, we will find it convenient to regularize this continuum theory by placing it on a lattice, i.e. we introduce a short distance cutoff in the problem, which in physical terms is taken to be of the order of the coherence length ξ . Moreover, we ignore the normal state free energy, measuring free energies in the superconducting state relative to the normal state. Such a lattice regularization is tantamount to introducing finite differences instead of gradients everywhere. Also, the order parameter will now be defined on lattice sites with labels given by the set {i}, which runs through 1, . . . , N = L2 , where L is the length of the sample in each direction. Ultimately, the L → ∞ limit needs to be taken. Note that in the end, it is really the continuum version of the Ginzburg– Landau theory we will be interested in, more precisely the continuum version at the critical point of the theory. When a phase transition happens to be a critical phenomenon, this means that there is a diverging length scale (ξ ) in the problem. We shall identify this length in the present chapter. Under such circumstances, the physics we are interested in are critical fluctuations on a length scale set by the diverging length. Hence, the lattice constant in our regularized theory is an irrelevant variable and the physics at the critical point of the lattice superconductor is expected to capture the physics of the continuum theory. Lattice regularizations, however, do require a bit of caution whenever they are applied, since it is not in any way obvious that such discretizations of space are not singular perturbations. Moreover, even if the lattice constant ‘disappears’ from the problem in this case, it does not necessarily leave the scene quitely, but may endow the system with an exponent η. The lattice regularized Ginzburg–Landau theory for a two-dimensional lattice superconductor takes the form 2 β 2 Dµ ψ Fs = α |ψi |2 + |ψi |4 + 2 2m µ=x,y i

Dµ ψ = ψi+µ − ψi

(9.4)

CRITICAL FLUCTUATIONS IN TWO-DIMENSIONAL SUPERFLUIDS

251

where ψi+µ is the order parameter evaluated at a lattice site which is shifted one lattice constant (set equal to unity) in direction µ. Expressing the above in terms of the amplitude and phase of the order parameter we find 2α(T ) 2 4 ψ + ψ Fs = J1 i i α(0) i ξµ2 + |ψi+µ ||ψi |(1 − cos(µ θ )) (9.5) 2 a µ=x,y µ where µ θ = θi+µ − θi J1 = 2α(0)β ψi ψi = α(0) β

(9.6)

9.3 Critical fluctuations in two-dimensional superfluids In principle, this formulation allows for both amplitude and phase fluctuations. However, we will ignore the amplitude fluctuations in the following. We simply set the amplitudes |ψi | = 1. This is very much like what we do in spin models where the length of the spin is taken to be frozen, and only the direction of the spin is taken to be important in investigating whether the magnet orders or not. Although we will not go into the details here, it is by now very well established that phase-only approximation to the fluctuations in ψi is on solid ground. This means that we can write the energy for latticized two-dimensional superconductor/superfluid on the form 1 − cos(µ θ ) Fs = J0 i,µ

J0 = J1

ξµ2 aµ2

(9.7)

when all constant terms are ignored. This is the well-known two-dimensional XY-model. It may be recast slightly into the following form (in addition, we introduce H as the Hamiltonian instead of Fs ) 1 − cos(θi − θj ) (9.8) H = J0 i,j

Here, i, j denotes nearest neighbour coupling, which emerges naturally by putting gradient terms in the Ginzburg–Landau theory on the lattice, and i runs

252

TWO-DIMENSIONAL SUPERCONDUCTIVITY

over all lattice sites in the problem. The entire Ginzburg–Landau theory is now expressed solely in terms of the phase of the superconducting order parameter, and the resulting statistical mechanics is entirely governed by phase fluctuations. Phase differences between lattice points are expressed as lattice gradients of the phase. Let us for simplicity denote them by ∇θ , which is a vector. A vector may always be split into a transverse part and a longitudinal part. The transverse part is divergence free, the longitudinal part is curl-free, hence we have ∇ · (∇θ )T = 0, ∇ × (∇θ )L = 0

(9.9)

Consider first this model at low temperatures. We then expect that thermally generated fluctuations in θ are, in some sense, small. The situation we have in mind in this case is depicted in Figure (9.1). This means that we can expand the cosine-term to leading order in the phasegradients, arriving at H=

J0 (θi − θj )2 2

(9.10)

i,j

where J0 now can be identified as a bare spin-wave stiffness parameter. The correlation function that probes the phase-coherence in the system is (r) = eiθi e−iθj

(9.11)

Figure 9.1 Spin-wave configurations, or equivalently longitudinal phase-fluctuations, in the two-dimensional XY -model on a square lattice. The arrows indicate values of θi , analogous to an XY spin direction, on the lattice points where the order parameter is defined.

CRITICAL FLUCTUATIONS IN TWO-DIMENSIONAL SUPERFLUIDS

253

where r = i − j. At low temperatures, the statistical average can safely be computed using the Hamiltonian Eq. 9.10. Since this is quadratic in the phase fluctuations, the average may be evaluated exactly. First of all, this leads to the simplification that (r) = e−(θ (r−θ (0))

2 /2

= e−(θ (r)−θ (0))

θ (0)

(9.12)

Here, r is the lattice vector between points i and j . In the last equality above, we have used the fact that the system is assumed to be translationally invariant. This means that we are neglecting effects of disorder in what follows. Thus, we are faced with the task of computing the correlation function G(r) ≡ [θ (r) − θ (0)]θ (0)

(9.13)

The computation of this quantity is facilitated by the equipartition theorem applied to Eq. 9.10, expressed in terms of the Fourier-modes θq of the phasefluctuations as follows H=

J0 2 q θq θ−q 2 q

(9.14)

This is quadratic in each of the Fourier modes and thus we have, by the equipartition theorem kB T J0 2 q θq θ−q = 2 2

(9.15)

which implies that the Fourier transform of the correlation function φ(r)φ(0) is given by θq θ−q =

kB T 1 J0 q 2

(9.16)

d2 q eiq·r − 1 (2π )2 q2

(9.17)

Thus, we get kB T G(r) = J0

Note how the phase-fluctuations vanish when T → 0. This means that phasecorrelations become truly long-ranged when T = 0, so at least in this limit we have established long-range order. What happens as we switch on T ? The above Fourier-integral may be evaluated straightforwardly, to obtain G(r) = −

r kB T ln 2π J0 a

(9.18)

254

TWO-DIMENSIONAL SUPERCONDUCTIVITY

√ where a is some short-distance cutoff a = e−γ /2 2 and γ = 0.577 . . . is the Euler–Mascheroni constant. Inserting this back into Eq. 9.12, we get (r) =

r −η a

(9.19)

where η = kB T /2π J0 . Note how this correlation function fits in with a general Ansatz for the two-point correlator 2 (r) close to a critical point, which on general grounds may be written as 2 (r) =

1 r d−2+η

G(r/ξ )

(9.20)

where ξ is some correlation length of the problem, d is dimensionality, G is some scaling function, and η is a so-called anomalous scaling dimension of the superfluid matter field ψ. Eq. 9.20 is of the form of Eq. 9.19, provided we set d = 2 and ξ = ∞. The latter is the hallmark of a system which is critical. Thus, what we learn from this is that a two-dimensional superfluid/superconductor has an entire low-temperature phase, which is critical. This is also reflected in the anomalous scaling dimension η = kB T /2π J0 , which is non-universal. Critical exponents associated with critical points are universal. Non-universality of exponents means that we are dealing here with a critical line, not a critical point. An important feature of (r) is that limr→∞ (r) → 0 provided η = 0, i.e. as soon as T = 0. Hence, there is never true long-range order at finite temperature in a two-dimensional superfluid/superconductor. In other words, the U (1) symmetry that is spontaneously broken in the three-dimensional case is never broken at finite temperature in two dimensions. This is a specific example of a somewhat more general statement, namely the Hohenberg–Mermin–Wagner theorem that states that at finite T , no continuous symmetry can be spontaneously broken in dimensions d ≤ 2[128, 129]1 . What we at most can have is power-law decay (which is much slower than exponential decay characteristic of shortrange order). Power laws mean that there is no length scale in the problem any longer, ξ → ∞ in Eq. 9.20. The system is thus scale-invariant, which is exactly the hallmark of criticality. This is often referred to as quasi-long-range order. The above result is based on the presumption that we can define local order of the phase-fields, and expand in small fluctuations around local order. A minute or two of reflection reveals that this cannot possibly be correct at high temperatures. It is obvious that in the high-temperature limit, even short range order must break 1 Often just referred to as the Mermin–Wagner theorem. Both the papers of Hohenberg and of Mermin and Wagner demonstrate the absence of long-range order in low dimensions for systems with continuous symmetries. Hohenberg considers neutral superfluids, Mermin and Wagner consider ferromagnets. Ironically, the title of the paper by Hohenberg is nonetheless Existence of long range order in one and two dimensions! A humorous remark by Halperin at Hohenberg’s 60th birthday suggested that perhaps the title is the reason for the much more frequent reference to Mermin–Wagner, rather than Hohenberg–Mermin–Wagner! Let it be said at once that both papers arrive at correct conclusions.

VORTEX–ANTIVORTEX PAIRS

255

down, and the above analysis is invalid. What have we missed? The process of elimination reveals the answer. Our starting point only has phase-fluctuations to begin with. The smooth phase-fluctuations we have included so far correspond to longitudinal phase-fluctuations. What we have left out, are transverse phasefluctuations. Their inclusion in the description, and their physical consequences, will be the topic of the next sections. We conclude this section by emphasizing that what we have demonstrated here, is that smooth phase-fluctuations (analogues of spin-waves in magnetic systems) suffice to destroy long range order in two dimensions and render the system critical, at any finite temperature. Spin-waves are therefore critical fluctuations in two dimensions (spin waves are not critical in three dimensions). Nonetheless, this does not mean that it does not cost energy to ‘twist’ the phase of the superconducting order parameter at low temperatures. Even if the system does not exhibit true long-range phase order, it still has a phase stiffness associated with it. On the other hand, at very high temperatures, phases are randomly oriented relative to each other even on the shortest length scales, and a local twist is expected to come at no cost in the free energy. Hence, somewhere in between low and high temperatures some phenomenon must occur such that the phase stiffness vanishes. If this happens at a finite temperature, then this phenomenon must in fact be a phase-transition, not a crossover. This is because a finite phase stiffness cannot be brought to precisely zero on a finite temperature interval in an analytic manner. It must therefore vanish in a phase transition. That this putative phase transition must be a subtle one, is clear from the simple observation that it cannot be a phase transition from an ordered low-temperature state to a disordered high-temperature state. It must be a phase transition from a quasi-ordered state to a disordered state. Under such circumstances we do not have the luxury, as we have in three dimensions, of probing the phase transition by monitoring the expectation value of a local ordering field (a local order parameter) and asking when it vanishes. In fact, when we are dealing with systems with a continuous symmetry in two dimensions we are forced to invoke a much more general (but often unnecessary) method of detecting a phase transition: We must identify a generalized stiffness of the system, which is a global quantity, and investigate when this stiffness vanishes through a proliferation of topological defects facilitated by entropy production in the free energy. In fact, this is a method we can always use, also in three dimensions, to detect phase transitions. We shall rephrase the three-dimensional superconductor to normal metal transition in this language in the next chapter.

9.4

Vortex–antivortex pairs

Transverse phase fluctuations are more violent than the smooth longitudinal ones considered in the previous section. Consider the quantity ∇θ and imagine

256

TWO-DIMENSIONAL SUPERCONDUCTIVITY

integrating this around some arbitrary closed contour in the plane. The vorticity q of the phase-distribution is measured by the quantity

dl × ∇θ = 2π q

(9.21)

Here, q ∈ Z. It is impossible to continually deform a phase distribution with q = 0 where only longitudinal, smooth phase fluctuations are excited, into a distribution where q = 0. Those phase distributions where q = 0 and those where q = 0 are topologically distinct. A vortex with a vorticity q is a topological defect superimposed on the phase distribution where no vortices are present. It is obvious that for high enough temperatures, transverse phase fluctuations will be excited thermally, not only smooth longitudinal ones. Vortices will therefore be generated spontaneously at high enough temperatures since this will increase the configurational entropy of the system, thereby lowering the free energy. Vortices are topological defects of the superconducting ordering field eiθ (r) . When they proliferate, the phase stiffness of the system vanishes, and this defines the phase transition. In Figure 9.2, we illustrate a vortex configuration in the twodimensional XY -model on a square lattice, while in Figure 9.3 we illustrate a vortex–antivortex pair. Note that for a charged superfluid, ∇θ gives rise to an electric current. The curl of this current is a magnetic field, and by Eq. 9.21 we thus see that q

Vortex

Antivortex

Figure 9.2 Four examples of vortex configurations, or equivalently transverse phasefluctuations, in the two-dimensional XY -model on a square lattice. Notice how each vortex corresponds to a collective phase-mode. The black dot in the centre is meant to illustrate the core of the vortex in this particular configuration. Thermally excited transverse phase fluctuations always give a vortex and an antivortex. The arrows indicate values of θi , analogous to an XY spin direction, on the lattice points where the order parameter is defined.

MAPPING TO THE 2D COULOMB GAS

257

Figure 9.3 An example of a vortex–antivortex pair. If we encircle one of these vortices along one of the small paths, we pick up a phase-difference ±2π. The phase-difference along the large path is zero. The fluctuations outside of this path correspond to spin waves.

may be interpreted essentially as the quantum of a magnetic field penetrating through an area enclosed by a contour C which the integral in Eq. 9.21 is taken around. It is intuitively perhaps obvious that no net magnetic field can be generated throughout the system by thermal fluctuations. Hence, vortices must always be generated in pairs of opposite vorticity, a vortex–antivortex pair. At low temperatures where vortices are expected to be unimportant, the above statement of the existence of vortex–antivortex pairs translates into a statement that at low temperatures only very tightly bound pairs exist. The proliferation of free topological defects at high temperatures, responsible for destroying the phase stiffness of the system, is equivalent to saying that the vortex–antivortex pair has dissociated into two free vortices of opposite vorticity. As we shall see, the above may be precisely rephrased into the language of a metal-insulator transition in a two-dimensional Coulomb gas, where the low-temperature phase corresponds to an insulating dielectric phase and the high-temperature phase corresponds to a metallic plasma phase.

9.5

Mapping to the 2D Coulomb gas

When vortex configurations are thermally excited in the two-dimensional superfluid, this is equivalent to generating a set of fluctuating ‘charges’ {qi } with overall charge-neutrality imposed, i qi = 0. The loss of phase-stiffness in the system, which we have argued above to be the phase-transition, must be related somehow to the statistical mechanics of this ensemble of charges. This follows

258

TWO-DIMENSIONAL SUPERCONDUCTIVITY

from the fact that these charges are manifestations of transverse phase fluctuations in the superconducting ordering field, and that the longitudinal phase fluctuations are incapable of driving the system into the high-temperature phase. What we need to do, is to include explicity the feature that the phases of the order parameter are angular variables defined on the interval θi ∈ [0, 2π . For the purposes of studying the phase transition in the two-dimensional superfluid on a lattice, i.e. where we have introduced a short-distance cutoff in the problem, we will perform a number of standard steps essentially amounting to what is called a duality transformation. Such a transformation is basically the following. When we focus on studying the critical properties of a system exhibiting a critical phenomenon, we try to identify precisely the thermal excitations that are responsible for destroying order in this system. These excitations may be viewed in general as topological defects in some ordering field, in our case the superfluid/superconducting condensate wave function ψi . Next, we attempt to express the partition function, more precisely the part of the partition function giving a singular contribution to the free energy, in terms of these topological defects. When this has been done, we have effectively executed a duality transformation. Strictly speaking the final step in the duality transformation is to write down a field theory for the action appearing in the partition function when it is written in terms of the topological objects of the original system. This field theory is the dual to the original field theory we started from. In this context, let us make an important remark on duality before we start doing computations in earnest. Suppose we have arrived at some dual field theory starting from an original theory such as the Ginburg–Landau theory of the two-dimensional superfluid. This dual theory itself has topological defects in its (dual) ordering field, which in principle we may identify. The partition function for the dual model may thus also be written in terms of the topological defects of the dual ordering field, and a field theory can be written for the corresponding action. This field theory is the dual of the dual model, and must in fact correspond to the original starting model. Duality squared must be equal to one. This is a statement which holds for all systems with only one phase transition. It is much weaker than the statement of self-duality, which means that the dual model has an identical form as the original model (but with inverted coupling constants). For instance, the dual model of the two-dimensional XY model does not have the same form as the two-dimensional XY model. The dual of the dual of the two-dimensional XY model is the XY model itself. However, the two-dimensional Ising model is selfdual, while the dual of the three-dimensional Ising model is a three-dimensional Ising gauge-theory, i.e. a lattice model with a local Ising theory. This is probably the simplest example where two models with the same symmetry, but where one has a global symmetry and the other has a local one, are related by a duality transformation. As it turns out, a similar situation is true for three-dimensional systems with local and global U (1) symmetries, which we will consider in the next chapter.

MAPPING TO THE 2D COULOMB GAS

259

The model with a global U (1) symmetry is a description of a three-dimensional charge-neutral superfluid, while the model with a local symmetry is a model of a three-dimensional superconductor. Hence, three-dimensional superfluids and superconductors are duals of each other. The partition function for the system is a priori given by

ZXY = Dθ e−βHXY HXY = J

1 − cos(θi − θj )

(9.22)

i,j

We next ignore the constant term in the Hamiltonian, and introduce the Fourier expansion of eα cos(x) as follows ∞

eα cos(x) =

In (α)einx

(9.23)

n=−∞

where In (α) is a Bessel function of order n. Inserting this in Eq. 9.22, we get ZXY =

∞

Dθ exp

Inµj (β)

(inµj µ θj )

(9.24)

n=−∞

Carrying out the angular integrations yields a constraint on the integer-valued field n given by µ nµj = 0

(9.25)

This is solved by introducing the two-dimensional curl nµj = εµν ν φj

(9.26)

where εµν is the two-dimensional Levi–Civita tensor, and φj is some scalar integer-valued field, which constitutes the actual degrees of freedom of the system. Up to now, everything is exact. The partition may now be written in terms of our new degrees of freedom, {φj }, as follows Iφj (β) (9.27) Z= {φj }

This may be approximated, using standard properties of the Bessel functions, as follows 1 (9.28) exp − [µ φj ]2 Z= 2β {φj }

j,µ

260

TWO-DIMENSIONAL SUPERCONDUCTIVITY

which we now want to write in a form that explicitly exhibits the topological excitations of the theory. Strictly speaking, the approximation we have made in passing from Eq. 9.27 to Eq. 9.28 is quantitatively useful at large values of β, i.e. it is naively expected to be a good low-temperature approximation. However, it is also qualitatively useful outside of the low-temperature domain. First, the symmetries of the exact partition function Eq. 9.27 and the approximate partition Eq. 9.28 are the same. This means that that the topological excitations of these two objects are the same. Hence, we expect that for the purpose of studying the critical properties of the system, these two objects essentially produce results which are in the same universality class. Less important details, such as the exact value of the critical temperature, will of course differ. To proceed further, we first introduce the Poisson-summation formula ∞

f (n) =

n=−∞

∞

∞

k=−∞ −∞

dz f (z)ei2π kz

(9.29)

Thus, the partition function is written in the following form, when we introduce a scalar auxiliary field pi Z=

{pi }

1 2 D{φ} exp − [µ φj ] + i2πpj φj 2β

(9.30)

The next step is now to perform the φj integrations, which gives Z = Z0

exp −4π 2 β

{pi }

pi D(|i − j |)pj

i,j

−2µ D(|i − j |) = δij

(9.31)

where Z0 is the partition function for spin waves. Note how the partition function factorizes (in the approximation of Eq. 9.28) in the product of a spin-wave part and a part which is isomorphic to the partition function of a two-dimensional Coulomb gas. We will see below that the quantities pj may be thought of as vortices in the original phase fields θi . The above factorization shows that spin waves and vortices do not interact within the approximation made in Eq. 9.28. Explicitly, we have

D(|i − j |) =

π

−π

dqx 2π

π

−π

dqy eiq·(i−j) 2π 2 µ 1 − cos(qµ )

(9.32)

which is just the Coulomb-potential on the two-dimensional lattice. It has the asymptotic value D(|i − j |) ∝ ln(|i − j |) as |i − j | → ∞, moreover the only

MAPPING TO THE 2D COULOMB GAS

261

allowed vortex configurations are those where i pi = 0. This ‘charge-neutrality’ condition follows from the fact that the above describes a Coulomb system with no screening, and hence it is incompressible. This means that any finite charging of the system will cost an infinite amount of energy in the thermodynamic limit such that configurations with i pi = 0 are suppressed. Let us now see how the fields pi correspond to vortex configurations of the original phase fields. In order to interpret the pi -excitation in as easy a fashion as possible, it is convenient to retrace our above steps, using the following approximation for the exponential of the cosine-potential in the XY action eβ cos(x) ≈ eβ

β exp − (x + 2π n)2 2 n=−∞ ∞

(9.33)

where we allow x to vary on the interval −∞, ∞ on the right-hand side. This approximation is usually referred to as the Villain-approximation, and is extremely useful in the current context (as well as in higher dimensions, as we shall see in Chapter 10). Essentially, the partition function for the XY -model is approximated by the partition function for a 2π periodic Gaussian model as follows

β Z= (µ θj − 2π aµ,j )2 Dθ exp − (9.34) 2 {aµ }

µ,j

where aµ,j is an integer-valued field, and we are instructed to sum over all such integers. The next step is to introduce the Fourier transform for each of the exponentials appearing in the partition function using

∞ β 1 1 exp − (x + 2π n)2 = √ dy exp − y 2 + iy(x + 2π n) (9.35) 2 2β 2πβ −∞ Thus we get, up to multiplicative factors which do not contribute to singular parts of the free energy,

1

2 − vµj + ivµj (µ θj + 2π aµ,j ) (9.36) Dθ Dvµ exp Z= 2β {aµ }

µ,j

The next step is to carry out the integrations over the phase-field θj , thus producing the constraint µ vµ,j = 0 (9.37) which is satisfied provided vµ,j = εµν ν φj

(9.38)

262

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Let us insert this representation into the partition function Eq. 9.36. Upon a partial integration in the exponent of Eq. 9.36, it may be written on form

Z=

{aµ }

1 2 − vµj − 2π iεµν µ aν,j φj Dφ exp 2β

(9.39)

µ,j

Now, comparing this with Eq. 9.30, we see that it has an identical form to Eq. 9.39, but we can identify the p-fields, namely pj = εµν µ aν,j . If we now think of aµj as the integer part of the phase-difference µ θj , which we may think of as a current, then we see that pj represents the vorticity of the original fields. It is also useful to rederive all of the above in a continuum version using a particular representation of the gradients of the phase which also takes into account the singularities arising from the fact that the phase is an angular variable, i.e. is defined with compact support, θi ∈ [0, 2π . We write the gradient of the phase (a vector) as a longitudinal and transverse part, cf. Eq. 9.9. The longitudinal part, corresponding to spin waves, is non-singular, while the transverse part gives rise to vortices. Moreover, since they are orthogonal components of the phase gradient, we have (∂θ )2 = (∂θL )2 + (∂θT )2

(9.40)

Recall also the equation relating ∂θT to vorticity, namely Eq. 9.21, which we may also write, using Stoke’s theorem, as ∂ × (∂θT ) = 2π q or equivalently εµν ∂µ ∂ν θT = 2π q(r)

(9.41)

where q(r) is the local vortex density. This equation is satisfied if the following representation is used for (∂ν θ )T

(∂ν θ )T = −2π εµλ ∂λ

d2 r G(r − r )q(r )

provided that the function G(r − r ) satisfies the Laplace equation −∂ 2 G(r) = δ(r)

(9.42)

MAPPING TO THE 2D COULOMB GAS

263

From this, we obtain

d r1 d2 r2 ∂λ G(r − r1 )∂ρ G(r − r2 )q(r1 )q(r2 ) (∂ν θT ) = (2π ) ενλ ενρ

= (2π )2 δλρ d2 r1 d2 r2 ∂λ G(r − r1 )∂ρ G(r − r2 )q(r1 )q(r2 )

2 2 = −(2π ) d r1 d2 r2 G(r − r1 )[∂ 2 G(r − r2 )]q(r1 )q(r2 )

2 (9.43) = +(2π ) d2 r1 q(r1 )G(r − r1 )q(r) 2

2

2

Here, we have used a property of the two-dimensional Levi–Civita tensor, namely that ενλ ενρ = δλρ . If we now write the XY model in the continuum limit as follows

K H= d2 r(∂θ )2 2

K d2 r[(∂θL )2 + (∂θT )2 ] = 2

(9.44)

and then utilize Eq. 9.43, we obtain K H = 2

d r(∂θL ) + 2π K 2

2

2

2

d r

d2 r q(r)G(r − r )q(r )

(9.45)

which again describes a spin-wave system and a Coulomb gas in two dimensions, since G is the Green’s function for the electrostatic potential between point charges in two dimensions. Again, note how spin-waves and vortices decouple in Eq. 9.45, which in this derivation is a consequence of expanding the cosine of the gradient up to quadratic order only. Coupling between spin waves and vortices is seen to be an effect due to higher order gradient terms, and is therefore irrelevant in renormalization group sense. To summarize this section, we have shown that the physics of the twodimensional XY model, i.e. that of a two-dimensional superfluid or superconductor, corresponds to that of a spin wave system coupled to vortex configurations of the XY model. In one particular approximation the spin waves and vortices decouple. Since the spin waves render the system critical at any finite temperature, but do no suffice to induce short-range phase correlations, it follows that the phase-transition from quasi-long range order to short-range order must be encoded in the Coulomb-piece of the partition function. Precisely what sort of phase transition such a system is capable of sustaining, will be the topic of the next section.

264

TWO-DIMENSIONAL SUPERCONDUCTIVITY

9.6 Vortex-pair unbinding and Kosterlitz–Thouless transition In this section, we study the phase transition in the two-dimensional Coulomb gas. We emphasize that we will be using nomenclature appropriate for a system of charges, but want to stress that the connection between the two-dimensional Coulomb gas and the two-dimensional XY model presented in the previous section (i.e. phase-only approximation to the Ginzburg–Landau theory of a two-dimensional superfluid) must always be kept in mind. We will ignore the spin wave part of the partition function, Z0 , since it gives no singular contributions to the free energy. The two-dimensional Coulomb gas has the feature of having an internal energy which consists of contributions that are logarithmic in the separation between the charges of the system. This is a feature which will be of utmost importance in what follows, since it implies that the internal energy and the entropic contribution to the free energy will behave precisely in a similar manner as a function of separation of vortices in a vortex–antivortex pair. Since we have that F = U − T S, we tentatively conclude that due to the logarithmic interaction, the internal energy U and the entropic term T S compete on an equal footing such that at high enough temperatures T , the entropy wins. This means that in the Coulomb gas language, a low-temperature dielectric phase of a system of charges consisting of tightly bound dipoles is converted, at some temperature, into a plasma of dissociated dipoles. In other words, the twodimensional Coulomb gas is capable of sustaining a metal–insulator transition. This would not happen in the one-dimensional Coulomb gas, which is always in the dielectric phase because the internal energy is linear in separation of charges, while the entropy is logarithmic, and hence the former dominates for large separations. Nor would it happen in the three-dimensional Coulomb gas which is always in the metallic phase, due to the fact that the internal energy is inversely proportional to separation between charges, while the entropy is logarithmic, the latter always wins for large separations. So the two-dimensional case is quite special, and it is the logarithmic character of the Coulomb-interaction between charges which is the central point. Coulomb-potentials (in any dimension) also have the special property that they are not screened by dipoles. A cautionary remark to begin with is absolutely necessary. One-dimensional superfluids do not map onto the one-dimensional Coulomb gas, and threedimensional superfluids do not map onto the three-dimensional Coulomb gas! The three-dimensional case will be dealt with in Chapter 10 by similar techniques as in the two-dimensional case, but the result will not be a system of point charges interacting with a Coulombic potential in three dimensions. The topological defects of the three-dimensional superfluid turn out to be vortex-lines, not point-vortices. Therefore, although a three-dimensional Coulomb gas does not have a finite-temperature phase transition, a three-dimensional superfluid

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

265

certainly does! When the two-dimensional Coulomb gas transitions from a dielectric phase to a metallic phase, it is the screening properties of the system which are altered in a non-analytic fashion as a function of temperature. We now follow the pioneering work of Kosterlitz and Thouless [130, 131], with only slight modifications due to Young [132], and Jos´e and co-workers [133]. The approach basically amounts to setting up a self-consistent description of a charge-neutral system in terms of scale-dependent electrostatics. The interested reader may also find it useful to consult the excellent review article on the two-dimensional Coulomb gas by Minnhagen [134]. Imagine that we have a system with a low density of charges, such that an asymptotically exact low-density approximation to its dielectric constant is given by the following expression ε = 1 + 2π nd α

(9.46)

where α denotes the polarizability of the medium. In the following, we will work in arbitrary dimensions d, and specialize to the d = 2 case at the end. The following closely follows the treatment of the problem by Kleinert et al. [135], which again builds on the approach of Young to the problem. In arbitrary dimensions, we assume that the point-charges of the system interacts with an interaction of the following form d − 2 − ηA |x| 2−d+ηA 2 V (x) = −1 (9.47a) 2 + ηA a η d/2 A 2 (4π ) 2 where the -function is defined by

∞

(x) =

dt t x−1 e−t

(9.47b)

0

This is a generalized potential which will correspond to precisely a logarithmic interaction when 2 − d + ηA = 0. Here, ηA is some parameter that describes deviations from standard Coulomb interactions in d dimensions. The standard Coulomb case for arbitrary d corresponds to ηA = 0, and we thus get a logarithmic interaction for the Coulomb-case if and only if d = 2. In this section, we will derive to lowest order in the fugacity the recursion relations for a scale-dependent stiffness parameter K(l) and a scale-dependent fugacity y(l) for a d-dimensional plasma where the bare pair-potential is given by Eq. 9.47a. This potential reduces to a logarithmic interaction when d = 2, and ηA = 0. As will become clear below, the stiffness parameter is basically the inverse of a scale-dependent dielectric constant. The scale-dependent fugacity y(l) basically gives the density of free unbound charges in the system, provided the density is low. Thus, when liml→∞ y(l) → 0, we have no free charges in the

266

TWO-DIMENSIONAL SUPERCONDUCTIVITY

system, only tightly bound dipoles. On the other hand, when liml→∞(l) y(l) → ∞ this is an indication that vortex–antivortex pairs dissociate and free charges appear in the system. Hence, we will look for changes in the scaling of the fugacity as the hallmark of the phase transition in the system. The starting point will be a low-density approximation for a dielectric constant of this system. Introducing the solid angle in d dimensions d = 2π d/2 / (d/2) and the density of dipoles in the fluid by nd , a low-density approximation for the dielectric constant is given by ε = 1 + nd d α

(9.48)

where a standard linear-response analysis gives α = 4π 2 Ks 2 /d for the polarizability, and s 2 is the mean square of the dipole moment in the system. To compute this, we need the low-density limit of the pair-distribution function n± (r) of the plasma, which is readily obtained from the grand canonical partition function expanded to second order in the bare fugacity ζ , and replacing the thermal de Broglie wavelength by a short-distance cutoff r0 , as follows n± (r) =

ζ2 r02d

e−4π

2 KV

(9.49)

In this way, we may now go on to express a scale-dependent dielectric constant as follows

4π 2 d K r ds s d+1 n± (s) (9.50) ε(r) = 1 + d r0 Note, however, that in Eq. 9.50, a mean-field approximation is understood to be used by replacing the bare potential V in n± (r) by an effective potential U (r). This effective screened potential must be selfconsistently determined by demanding that it gives rise to an electric field in the problem given by ∂U K f˜(d) = E(r) = ∂r ε(r) r 1−ρ

(9.51)

ρ = 2 − d + ηA

(9.52)

where and f˜(d) is defined by

d − 2 − ηA (d − 2 − ηA ) 2 f˜(d) = η d/2 A 2 (4π ) (1 + ηA /2)

(9.53)

Such a mean-field procedure has been consistently used with success in the two-dimensional case, and the origin of the success lies in the long range of

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

267

the ln-interaction. In higher dimensions, such a procedure will work even better since the logarithmic potential is felt over even longer distances due to extra volume factors. Let us introduce a logarithmic length scale l = ln(r/r0 ) along with the new variables τ (l) =

ε(r0 exp l) 4π 2 K

x(l) = 4π 2 KU (r0 exp l)

(9.54)

Here, x(l) is determined selfconsistently by integrating the effective field E(r). Then we get from Eqs 9.50 and 9.51

d ζ 2 l τ (l) = τ (0) + d−2 dv e(d+2)v−x(v) (9.55) dr0 0 and x(l) = x(0) + f˜(d)

ρ

l

dv 0

r0 eρv τ (v)

(9.56)

From Eqs 9.55 and 9.56 we may derive coupled renormalization group equations for τ (l) and x(l). However, in order to obtain equations that have a form more similar to equations that have appeared in the literature on the d-dimensional Coulomb gas, we introduce a new variable K(l) representing a scale dependent stiffness constant, as follows K −1 (l) ≡

τ (l) ρ r0 eρl

(9.57)

Thus, we see that the effect of a non-zero ρ on the stiffness amounts to a scaling change K(l) → eρl K(l). Using Eq. 9.56, we have ∂x(l) = 4π 2 f˜(d)K(l) ∂l

(9.58)

Differentiating K −1 (l) with respect to l and using Eq. 9.55, we obtain 2d ζ 2 ∂K −1 (l) = −ρK −1 (l) + d−2+ρ e[(d+2−ρ)l−x(l)] ∂l dr0

(9.59)

From this expression, we define a scale-dependent fugacity y(l) given by √ 2d ζ e[(d+2−ρ)l−x(l)]/2 (9.60) y(l) ≡ √ (d−2+ρ)/2 dr0

268

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Thus, we see explicitly that the renormalization of K(l) in principle influences the flow equation for y(l), which is obtained by differentiating with respect to l and using Eq. 9.58. We thus get the two coupled equations dK −1 (l) = y 2 − ρK −1 (l) dl dy(l) = [d − ηy − 2π 2 f˜(d)K(l)]y(l) dl

(9.61)

where ηy = (d − 2 + ρ)/2, and ρ is given by Eq. 9.52. It has a physical interpretation as an anomalous scaling dimension of the fugacity. Let us set ηA = 0, i.e. we consider the standard Coulomb-case (our starting point!), but in arbitrary dimensions. This means that ηy = 0 as well. We then get the following set of equations for the scale-dependent stiffness parameter K(l), or inverse dielectric constant, and fugacity y(l) dK −1 = y 2 − (2 − d)K −1 dl dy = [d − 2π 2 f (d)K]y dl

(9.62) (9.63)

where f (d) = (d − 2) [(d − 2)/2]/(4π )d/2 . These equations describe the flows of the stiffness parameter and the fugacity of the d-dimensional Coulomb gas. Precisely the same results were first obtained by Kosterlitz by a method completely different from the one we have used above, a good sign [136]. Finally, if we now set d = 2 we arrive at the celebrated Kosterlitz–Thouless flow equations for the dielectric constant and the fugacity of the two-dimensional Coulomb gas, namely dK −1 = y2 dl dy = [2 − π K] y dl

(9.64) (9.65)

Notice how the second term on the right-hand side of Eq. 9.62 vanishes when d = 2. This is of crucial importance. Eqs 9.64 and 9.65 describe how the dielectric constant and the effective fugacity of the Coulomb gas change when the length scale l they are viewed on, varies. These are therefore not standard renormalization group (RG) equations in the sense of Wilson-RG. Rather, they have the status of selfconsistency equations for scale-dependent electrostatics. Let us now consider what these equations predict. The result of the flows for K(l) and y(l) will depend on what the values of the bare parameter for the dielectric constant and the fugacity are. The bare values in this context refer to what the value of these quantities are at short length scales. Suppose that

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

269

the bare value of K is larger than 2/π . Then the right-hand side of Eq. 9.65 is negative, and y(l) is reduced as l increases. Consider now Eq. 9.64 under these circumstances. Since y(l) decreases with l, it means that K(l) increases. But then the right-hand side of Eq. 9.65 gets even more negative, thus accelerating the reduction of y(l). Thus, the system flows to a regime where liml→∞ y(l) → 0. Consider now the case where K is smaller than 2/π . Then y(l) increases with increasing l, and K is reduced further, thus accelerating the increase in y(l). Thus, in this case, liml→∞ y(l) → ∞. Hence, the value K ∗ = 2/π is a particular value of the stiffness which separates the regime where liml→∞ y(l) → 0 from the regime where liml→∞ y(l) → ∞. What does all of this mean, physically? The case liml→∞ y(l) → 0 simply means that in an appropriate temperature regime, there are no free charges in the two-dimensional Coulomb gas, all charges are bound into tight dipoles. Such a system of tightly bound dipolar pairs is incapable of carrying an electric current when it is subjected to an electric field, and is therefore an insulator. The case liml→∞ y(l) → ∞ corresponds to proliferation of free charges in the system, and such a system is capable of carrying a current when subjected to an electric field. This is therefore a metallic phase. Hence, we reach the conclusion that the sort of phase transition the two-dimensional Coulomb gas undergoes when it passes through the point K ∗ = 2/π , is a metal-insulator transition. Note how all of this fails when d = 2. For d = 1, the second term on the right-hand side of Eq. 9.62 is finite and negative. This means that no matter how large we initially make the fugacity (for instance by making K initially very large), K −1 (l) will decrease, hence increasing K(l) and thus reducing y(l). For all bare values of K, we always end up in a situation where liml→∞ y(l) → 0. Conversely, when d = 3 the second term on the right-hand side of Eq. 9.62 is finite and positive. By a similar type of argument as for d = 1, we always end up in the situation where liml→∞ y(l) → ∞. The d = 1 result is a statement that the one-dimensional Coulomb gas is always in the dielectric phase, never in the metallic phase, whereas the three-dimensional Coulomb gas is never in the dielectric phase, but always in the metallic phase. It is now very appropriate to go back to the two-dimensional superfluid, and ask ourselves what all of this means in that system. In other words, the metal–insulator transition of the two-dimensional Coulomb gas maps onto precisely what in the two-dimensional superfluid? We have already established in the previous section, that the charges in the two-dimensional Coulomb gas are to be identified with vortices in the phase-field of the superfluid/superconducting ordering field. Thus the metal–insulator transition corresponds to a phase transition in the superfluid from a low-temperature phase with only tightly bound vortex–antivortex pairs into a high-temperature phase where one has dissociated vortex–antivortex pairs. These vortices are the topological defects in the phasetexture of the superfluid. When they proliferate as a result of the dominance of the entropic contribution to the free energy, they convert the powerlaw decay of

270

TWO-DIMENSIONAL SUPERCONDUCTIVITY

the phase–phase correlator, (Eq. 9.19), into an exponential decay characteristic of short-range order. The phase-stiffness of the system, which is non-zero in the critical low-temperature regime, has been lost at the phase transition as a result of the appearance of vortices. Now, the phase-stiffness of the XY model is the energy cost of introducing twists in the phase of the superconducting order parameter, i.e. the energy cost of introducing gradients ∇θ . Superconductivity is a macroscopic quantum phenomenon associated with phase-coherence. The phase stiffness, often called the helicity modulus ϒ of the XY model, is defined as the cost in free energy of an initial twist θ in the phase of the order parameter across the system, ϒ∼

∂ 2F |θ =0 ∂θ 2

(9.66)

Going back to the partition function for the XY model, we have (upon normalizing ϒ to its value at zero temperature) 2 ϒ 1 J = cos(µ θ ) − cos(µ θ ) J N r kB T N r

(9.67)

This quantity probes the global phase-coherence of the system and can be directly identified with the superfluid density ρs of the system. This is a consequence of the London equation J=−

1 A µ0 λ2

(9.68)

as follows. The twist in the phase θ may be viewed as adding a vector potential A to the argument of the cosine-potential in the XY model (by minimal coupling). This alters the free energy. Now, by standard quantum mechanics, the current given above may be viewed as a linear-response expression for the derivative of the free energy with respect to the added vector potential. The second derivative of the free energy with respect to an added vector potential, evaluated at A = 0, is therefore the (negative of the) derivative of the current with respect to the vector potential, which is nothing but 1/λ2 ∼ ρs . Hence, we have a major result, namely ϒ ∼ ρs

(9.69)

Vortices are responsible for destroying the phase stiffness, i.e. ϒ, of the XY model, and they are therefore also responsible for destroying the superfluid density in the 2D superfluid/superconductor. To put this into perspective, it is worthwhile reminding ourselves that for the two-dimensional Ising model, we are able to consider the magnetization as a useful order parameter. The Ising model for d = 2 is capable of sustaining a lowtemperature phase with true long range spin–spin correlations because the spins

JUMP IN SUPERFLUID DENSITY

271

can only point in two directions. The model has a discrete symmetry, unlike the XY model, and therefore does not sustain gapless spin wave modes that can be excited at arbitrary low temperatures. However, if we preferred, we could detect the phase transition in the two-dimensional Ising model, not by monitoring the magnetization (a local order parameter), but by monitoring the proliferation of lines of overturned spins. These constitute two-dimensional domain walls and are the topological objects responsible for destroying the spin-stiffness (a global order parameter) in the two-dimensional Ising model. The Ising-analogue of the spin stiffness is the free-energy cost of forcing a domain wall into the system (since the minimal twist of boundary conditions is an angle π in the Ising case). The free energy of the domain line per unit length is the line tension of the domain-line. When domain-lines proliferate, they do so because their line tension vanishes, and it can be demonstrated that in fact this quantity vanishes precisely at Tc . It was, as a matter of fact, computed exactly for the two-dimensional Ising model in 1942 by Onsager [137], in his stellar paper on the exact solution to the two-dimensional Ising model. The line-tension of domain-lines may therefore also serve as a candidate generalized stiffness in this case. The spirit of the domain-line approach for the two-dimensional Ising model is similar in spirit to monitoring the proliferation of vortices in the two-dimensional XY model. The difference is that in the Ising-case, we have the luxury of being able to use a local order parameter, if we so wish, to detect the transition, whereas in the case of the XY case in two dimensions, we do not. We are forced to the (conceptually quite charitable!) conclusion that in the two-dimensional XY model, the general scheme of identifying topological objects and asking when their proliferation annihilates a generalized stiffness is the method of detecting the phase transition. This is basically a by now well accepted realization of Anderson’s quite general concept that a phase transition may be viewed as the proliferation of topological defects in some ordering field with an associated breakdown of a generalized rigidity [138].

9.7 Jump in superfluid density Let us consider in some detail the solution to the flow equations Eqs 9.64 and 9.65. We are primarily interested in solving the equations for low fugacity, since the equations themselves are based on the notion that the density of charge (free vortices) is small. What happens for high densities is beyond the current approach, and will not concern us here. We rewrite Eq. 9.65 slightly as follows using K −1 (l) = τ (l) 2 τ (l) − 1 dy(l) y(l) =2 π 2 dl π τ (l) ≡ 2T (l)y(l)

(9.70)

272

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Multiplying on each side by y(l) this may be recast into the form dy 2 (l) = 4T (l)y 2 (l) dl

(9.71)

We will now look for solutions consistent with a low fugacity, and consider therefore the regime close to the point where the scaling of y(l) changes, which as we have argued above happens when τ = π/2. In this case, we have 2 τ (l) − 1 π dT (l) 2 ≈ y 2 (l) dl π T (l) ≈

dT 2 (l) 4 ≈ T (l)y 2 (l) dl π

(9.72)

√ We may now combine Eqs 9.71 and 9.72, upon redefining y(l) →= y/ π , as follows d[y 2 (l)] − d[T 2 (l)] =0 dl

(9.73)

y 2 (l) − T 2 (l) = ±ω2

(9.74)

or equivalently

where ω is taken to be some positive integration constant, and we have deliberately written it in such a way as to distinguish two cases, namely that where it is negative and that where it is positive. We consider the former case first, and for this case, it is furthermore necessary to distinguish between two cases, namely that where T (l) < 0 and that where T (l) > 0. We consider therefore first the case where y 2 − T 2 < 0, T < 0. From Eq. 9.72 it follows that 2 2 dT (l) =− ω − T 2 (l) (9.75) dl π Upon introducing l˜ = (2ωl)/π and T˜ (l) = T (l)/ω, Eq. 9.75 takes the simpler form

or equivalently

dT˜ (l) = T˜ 2 − 1 ˜ dl

(9.76)

dT˜ (l) = dl˜ T˜ 2 − 1

(9.77)

JUMP IN SUPERFLUID DENSITY

273

which immediately may be integrated to yield coth−1 (T˜ (l)) = −(l˜ + θ )

(9.78)

where θ > 0 is yet another integration constant, and the choice of sign guarantees that T (l) < 0, since this is the case we now consider. Thus, we finally get T (l) = −ω coth(u) 2 u = ωl + θ π

(9.79)

Moreover, using Eq. 9.74 and the fact that the fugacity is positive, we also obtain y(l) =

ω sinh(u)

(9.80)

Now, consider the limit l → ∞, i.e. the long distance physics of the problem. It is immediately clear that both liml→∞ y(l) = 0 and liml→∞ T (l) = 0. Thus, for all initial values such that y 2 < T 2 , we end up in a dielectric insulating phase of the Coulomb gas. This corresponds to the low-temperature phase of the superfluid, where only spin waves, but no vortices, are thermally excited. The above also implies that in this regime, liml→∞ τ (l) = π/2, or equivalently, K ∗ ≡ lim K(l) = l→∞

2 π

(9.81)

Next consider the regime where y 2 − T 2 < 0, T > 0. We proceed by integrating the equations precisely as above, but we need to make another choice of sign in the integration constant θ appearing in Eq. 9.78 in order to guarantee the correct sign of T , and we get ˜ coth−1 (T˜ (l)) = (θ − l)

(9.82)

where θ > 0, whence T (l) = ω coth(u) 2 u = θ − ωl π Consequently, we have y(l) =

ω sinh(u)

(9.83)

(9.84)

where the argument u is given by that in Eq. 9.83. It is clear from the above that the solutions for y 2 − T 2 < 0, T > 0 cannot be trusted as l is increased indefinitely, since y(l) in fact diverges, contradicting the assumption that y(l) should

274

TWO-DIMENSIONAL SUPERCONDUCTIVITY

be small. However, we can say the following. As l increases, starting from an arbitrary, but small value of y(l), the solutions predict that y(l) increases. Thus, instead of y(l) flowing to zero, as in the case T (l) < 0, we have an unambiguous indication that tightly bound dipoles dissociate, resulting in a proliferation of free charges, or equivalently a proliferation of free vortices. The consequence of an increasing y(l) for K(l) is obvious, it decreases, thus accelerating the increase of y(l), further reducing K(l). In the regime y 2 − T 2 < 0, T > 0 we therefore obtain K ∗ ≡ lim K(l) = 0 l→∞

(9.85)

Based on Eqs 9.81 and 9.85, we are now ready to state a major result of the whole formalism we have presented in this section and the preceding one. It says that as we go through the metal–insulator transition, the renormalized stiffness parameter liml→∞ K(l) of the system (equivalently the inverse dielectric constant of the Coulomb gas), exhibits a discontinuity of universal magnitude, given by 2/π . In a moment, we shall translate this into the language of superfluidity. First, however, we complete our analysis of the flow equations by considering also the regime y 2 − T 2 > 0. In this case, the differential equation corresponding to Eq. 9.75 reads dT (l) 2 2 = ω + T 2 (l) dl π

(9.86)

which is straightforwardly solved, much as above, to yield the solutions T (l) = ω cot(u) ω y(l) = | sin(u)| 2ω l u=θ− π

(9.87)

where again θ > 0 is an integration constant. Since cot(u) does not have a definite sign, this solution encompasses both cases T > 0 and T < 0. The above three cases of the solutions to the flow equations may be summarized in the flowdiagram for y(l), T (l) in Figure 9.4 (which any student of statistical physics and superconductivity should know!), where the arrows indicate in which direction the quantities flow as l is increased We close the discussion of the flow equations by remarking that to the extent that they exhibit fixed points (it turns out to be an entire line of fixed points), this occurs at zero fugacity, i.e. y ∗ = liml→∞ y(l) = 0. This is a very fortunate circumstance, since the basic starting point for deriving the flow equations was Eq. 9.50 which is a low-density approximation to the dielectric constant. The fact that the fixed point occurs at zero fugacity means that the assumption of low

JUMP IN SUPERFLUID DENSITY

275

y

Metallic state

Insulating phase (dielectric) 1−p/2 K

Figure 9.4 Flowdiagram showing variation in renormalized fugacity y(l) and stiffness parameter K(l). Note how liml→∞ y(l) → 0 for all T < 0. The entire line Y = 0, T < 0 is therefore a fixed line, in contrast to a fixed point, for the flow equations. The two straight lines are given by y = −T , T < 0 and y = T , T > 0, and the thick line y = −T is the separatrix separating the two scaling regimes liml→∞ y(l) = 0 and liml→∞ y(l) = ∞. The thick solid line y = 0, T < 0 is a line of fixed points.

densities is selfconsistently shown to be correct. Had we encountered a finitefugacity fixed point, the entire calculation would have been uncontrolled and we would have, at the very least, been forced to include higher order fugacity terms. As it turns out, this need not concern us. Let us now translate the statement about the jump of 2/π in K ∗ at the phase transition into the language of superfluidity. To do this, we need to establish a connection between the superfluid density of the two-dimensional superfluid, and the the scale-dependent inverse dielectric constant (K(l)) of the two-dimensional Coulomb-gas. The rather tedious, but straightforward details of this may for instance be found in the textbook of Huang [139], Appendix A. The result is very straightforward, namely that the superfluid density, normalized to its zerotemperature value, may be expressed in terms of the density–density correlation function for vortices as follows 1 nk n−k ρs = lim 1 − k→0 kB T V k 2

(9.88)

where nk is the Fourier transform of the vortex density, or equivalently the charge density, and V is the volume of the system. The k → 0 limit of this is nothing but the spatial integral of the pair-distribution function. Hence Eq. 9.88 is nothing but the inverse of the dielectric constant as given in Eq. 9.46, in the low-density limit. Hence, the superfluid density and the stiffness parameter are

276

TWO-DIMENSIONAL SUPERCONDUCTIVITY

related as follows, K(T ) =

2 ρs (T ) m2 kB T

(9.89)

where m is the mass of the bosons constituting the superfluid, and we have reinstated Planck’s constant . (Converting from natural units back to physical units, a density acquires the dimension (/m)2 ). Therefore, if we measure ρs (T ) in a two-dimensional superfluid as a function of temperature approaching Tc from below, we have the quite remarkable prediction that at T = Tc , we will observe a discontinuity in ρs (T ) as a function of temperature as we cross the transition. It is finite up to Tc and vanishes at and above Tc in such a way that lim

T →Tc−

2 2 ρs (T ) = 2 π m kB T

(9.90)

exhibits a universal jump. This is a very powerful prediction of the theory, first made by Nelson and Kosterlitz [140], ranking on par with the prediction of BCS of a universal ratio between the zero-temperature gap and the critical temperature, as we discussed in Chapter 4. The prediction was quickly verified in experiments on superfluid thin He4 films by Bishop and Reppy [141], and effectively removed any serious skepticism that might have existed about the existence of the Kosterlitz–Thouless transition. A qualitative sketch of the superfluid density as a function of temperature is given in Figure 9.5. A comment is certainly in order here. Note how the global order parameter ρs of the superfluid vanishes discontinuously at the phase-transition. This is reminiscent of a first order phase transition. On the other hand, the correlation length of the superfluid is finite in the high-temperature phase but infinite in the low-temperature phase. This is a situation which is reminiscent of a second order transition. In fact, the Kosterlitz–Thouless transition is neither first nor second order. The above is an indication of the fact that the classification scheme of first and second order phase transitions is not entirely adequate. The Kosterlitz–Thouless transition is in fact an infinite order phase-transition. rs

Tc

T

Figure 9.5 Superfluid density ρs (T ) of a two-dimensional superfluid as a function of temperature. Note the discontinuity at the critical temperature. The jump in ρs at Tc , normalized to the critical temperature, is universal, limT →Tc− 2 ρs (T )/(mkB T ) = 2/π.

JUMP IN SUPERFLUID DENSITY

277

Let us now proceed to see what happens when we apply the duality technology to the three-dimensional case. As we will see in the next chapter, the topological defects of the superfluid/superconductor in three dimensions are vortex lines and not point-vortices. This precludes the possibility of a Kosterlitz–Thouless type of RG approach to this problem.

10 Dual Description of the Superconducting Phase Transition 10.1 Introduction In this chapter, we will utilize the three-dimensional analogue of the duality transformation introduced in the previous chapter to gain further insight into the character of the superconductor-normal metal transition. Recall that in Chapter 4, where we established and solved the BCS gap equation, it was emphasized that this was a mean-field approach which neglected fluctuations in the critical regime. The BCS approach works extremely well in superconductors like Al and Sn, even at the quantitative level. This is due to the fact that these superconductors are deep into the type I regime and fluctuation effects are tiny. In this chapter, we turn to the case of extreme type II superconductors like the high-Tc cuprates and uncharged superfluids like He4 . The latter can be seen as a limit of the extreme type II case, by letting the Ginzburg–Landau parameter κ → ∞. Fluctuation effects are now much more prominent, especially for the high-Tc cuprates. The reason is twofold. First, because of the large values of critical temperatures, thermal fluctuation effects are expected to be larger than for superconductors with low Tc . Another way of saying this is that a high Tc reflects the fact that Cooper-pairs are tightly bound, and hence the correlation length ξ , which is a measure of the spatial extent of a Cooperpair, i.e. over what distances in real-space two electrons are correlated into opposite-momentum and opposite-spin states, is small compared to its value in unconventional low-temperature superconductors. Hence, the van der Waals type of argument involving large ξ that leads to a justification of the meanfield approach, is no longer expected to work as well. Secondly, extreme type √ II superconductivity involves κ = λ/ξ 1. Now, ξ ∼ 1/Tc and λ ∼ 1/ ρs . √ Hence, κ ∼ Tc / ρs . In high-Tc cuprates, κ is large not only because Tc is Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

280

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

large, but also because high-Tc cuprate superconductivity arises out of very poor metals involving low charge carrier density ρn . This carrier density is an upper limit on the superfluid density ρs , which is therefore also low. This has important physical ramifications with respect to fluctuation effects. Recall from Chapter 10 that we established a relation between the phase stiffness (helicity modulus ϒ) of the superconducting condensate, and ρs as follows, ϒ∼

∂ 2F |θ =0 ∼ ρs ∂θ 2

(10.1)

where F is the free energy and θ is a phase-twist in the complex scalar superconducting order parameter across the system. This means that a low superfluid density implies the existence of large phase-fluctuations in the system. In superconductors arising out of good metals like Al, ρs and hence the phase stiffness, is much larger and these phase fluctuations may usually be ignored except in an immeasurably narrow temperature range around the critical temperature. We emphasize that the approach to be detailed here is not in contradiction to the BCS theory. Rather, it complements it in the situations where the critical fluctuation effects that are left out in the BCS mean-field approach need to be taken into account. We will base our discussion on the Ginzburg–Landau theory, just as in Chapter 10. The strength of such an approach is that the Ginzburg–Landau theory simply postulates the existence of superconducting order without asking how it has established itself. Therefore, what we shall have to say in this chapter is general and entirely model independent, applying in principle to extreme type II and even moderate type II superconductors with a complex scalar order parameter (spin-singlet superconductivity). We shall be interested in studying the critical properties of the superconductor and for this purpose the Ginzburg–Landau theory, which is a theory of a bosonic matter field coupled to a fluctuating gauge field, will suffice both for s-wave superconductors and d-wave superconductors. The two differ in one important respect, namely in that the former has no gapless fermionic excitations on the Fermi-surface, whereas the latter does. The nodal fermions in the d-wave superconductors in principle need to be taken into account in the superconducting state, but at Tc we may assume them to be fully thermalized and decoupled from the superconducting condensate. Were we, however, to study quantum fluctuations in the superconducting order parameter at very low temperatures, then we would need to consider the nodal fermions seriously, and a d-wave superconductor in this temperature regime has a quite different behavior than an s-wave superconductor. This is a quite involved situation which we will not deal with here, and where much work remains to be done. We take as our starting point the Ginzburg–Landau theory of the system, introduced in Chapter 4, which when written in dimensionful form is defined by the partition function of the system written as a functional integral over the

281

INTRODUCTION

fluctuating condensate order field ψ and the fluctuating gauge field A as follows Z = DψDAe−βH (ψ,A) u 4 2 1 2 ∗ 2 2 H (ψ, A) = dr α(T )|ψ| + |ψ| + |(∇ − ie A)ψ| + (∇ × A) 2 2m∗ 2µ0 (10.2) Here, m∗ and e∗ are effective masses and charges for the bosonic condensate constituents, A is a fluctuating gauge field related to a local induction B via the equation B = ∇ × A, and µ0 is the vacuum permeability. Next, we scale the quantities appearing in Eq. 10.2 as follows m∗ α(T ) β4 µ0 β ∗ 2m∗ ∗ 2 A→ A, e → e ,ψ → ψ, → m , u → u β µ0 β2 2β2 2(m∗ )2 (10.3) 2 Note the parameter m appearing in the above. As α(T ) becomes negative for low enough temperatures, we must think of m2 as some mass parameter, not a physical mass. Then, Eq. 10.2 may be written on the form Z = DψDAe−S(ψ,A) S(ψ, A) = dr m2 |ψ|2 + u|ψ|4 + |(∇ − ieA)ψ|2 + 12 (∇ × A)2 (10.4)

where there now appears a dimensionless action S in the exponent of the Boltzmann weight. Since S is dimensionless, all terms under the integral in S carry dimension L−d . Hence, we have the naive scaling dimensions of the quantities appearing in Eq. 10.4 1−d 2

[e] = L 2 −1 (10.5) If we now express all dimensionful quantities as dimensionless via the coupling constant e as follows [ψ] = L

,

ψ → ψe−1 ,

d

[A] = L1− 2 ,

A → Ae−1 ,

[u] = Ld−2 ,

r → re2 ,

[m2 ] = L−1 ,

m2 → ye4 ,

u → xe2

d

(10.6)

we may write the action in a form which we will use explicitly at the end of this chapter, namely S(ψ, A) = dr y|ψ|2 + x|ψ|4 + |(∇ − iA)ψ|2 + 12 (∇ × A)2 (10.7) Here, y appears as a temperature-like parameter, while whereas x essentially is like κ 2 , such that a large x corresponds to extreme type II, small x corresponds

282

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

to type I, and the mean-field demarcation line between type I and type II is given by x = 1/2. We shall come back to this point in Section 10.8. Most of this chapter will be concerned with the situation for large x 1. Consider for the moment the situation with x → ∞. This means that for a fixed |ψ|4 -coupling u, the theory corresponds to that of an uncharged superfluid, and we may simply drop the gauge field A from the description. It will live its own uneventful life as a free Maxwell field decoupled from the matter field ψ. We now make an approximation that is expected to be excellent in the type II regime, but which we will later show fails in the type I regime. In the type II regime, we will ignore amplitude fluctuations in ψ = |ψ|eiθ , at least for the purposes of studying the critical properties of the system. We simply set the magnitude of ψ equal to unity. Thus, as in the two-dimensional case all we are left with are phase-fluctuations in ψ, and as always they come in two varieties, longitudinal and transverse.

10.2 Lattice formulation of the Ginzburg–Landau theory Our starting point is the continuum Ginzburg–Landau model. In quantum field theory, the GL model is also referred as the scalar QED or the U (1)+Higgs model or the Abelian Higgs model. For completeness, we also take anisotropy into account, i.e. the effect that the electron transport exhibits uniaxial anisotropy such that motion in the [x, y)-plane is easier than motion along z-axis. The effective Hamiltonian for the Ginzburg–Landau model in an anisotropic system is given by HGL =

2 g d r α(T )|ψ| + |ψ|4 + 2 2mµ µ=x,y,z 1 + (∇ × A)2 2µ0 3

2

2 ∇µ − i 2π Aµ ψ

0

(10.8)

Here, ψ(r) = |ψ(r)|eiθ (r) is a complex order field representing the superconducting condensate. In superconductors, the amplitude |ψ(r)|2 should be interpreted as the local Cooper-pair density. Furthermore, mµ is the effective mass for one Cooper-pair when moving along the µ-direction, 0 = h/2e is the flux quantum, and µ0 is the vacuum permeability. In Eq. 10.8, the gauge field A is related to the local magnetic induction, b(r) = ∇ × A(r). Finally, the Ginzburg–Landau parameter g is assumed to be temperature independent, while α = α(T ) changes sign at a mean field critical temperature TMF (B), where Cooper-pairs start to form. B is the spatial average of the magnetic induction.

LATTICE FORMULATION OF THE GINZBURG–LANDAU THEORY

283

The critical temperature Tc where phase-coherence develops, is in principle always smaller than TMF . Hence, the existence a finite Cooper-pair density does not in itself imply that the system is in a superconducting state. Later on, we shall recast the Ginzburg–Landau theory in a quite different form that also exhibits a U (1)-symmetry, but where the field conjugate to the relevant phase is the number operator for the topological excitations destroying the order of the Ginzburg–Landau theory itself. Although this may seem like an unnecessary complication, it has the advantage of facilitating a detailed discussion of the vortex-liquid phase of the Ginzburg–Landau theory in terms of the ordering of some local field, namely the complex scalar field φ(r) to be introduced below. This is not possible using the Ginzburg–Landau function, ψ(r), since ψ(r) is always zero in the vortex liquid phase. In the zero-field low-temperature ordered phase, the system spontaneously chooses a preferred phase angle , and explicitly breaks the U (1) symmetry. The vortex-sector of the Ginzburg–Landau theory also exhibits a U (1)-symmetry breaking, but where U (1)-symmetry is broken in the high-temperature phase, and restored in the low-temperature phase. Eq. 10.8 has two intrinsic length scales, the mean-field coherence length ξµ2 (T ) =

2 2mµ |α(T )|

(10.9)

and the magnetic penetration depth λ2µ =

mµ β 4µ0 e2 |α(T )|

(10.10)

ξµ is the characteristic length of the variation of |ψ(r)| along the µ-direction, and λµ is the characteristic length of the variation of the current flowing along the µ-direction. In order to carry out Monte Carlo simulations of the Ginzburg–Landau model, the model is discretized by replacing the covariant derivative in the continuum Ginzburg–Landau Hamiltonian (Eq. 10.8), with a covariant lattice derivative,

2π Dµ ψ = ∇µ − i Aµ ψ

0

2π 1 −i aµ Aµ (r) 0 − ψ(r) ψ(r + µ)e ˆ →− Dµψ = aµ

(10.11)

The resulting model has all three spatial directions discretized. The effective Hamiltonian for the lattice Ginzburg–Landau model is given by,

284

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

g HLGL = ax ay az α|ψ|2 + |ψ|4 2 r 2 2π 2 −i aµ Aµ (r) 0 ψ(r + µ)e ˆ + − ψ(r) 2 2mµ aµ µ=x,y,z 1 2 + ( × A)µ 2µ0 aµ2 µ=x,y,z

(10.12)

Here, aµ and µˆ is a lattice constant and a unit vector along the µ-axis, respectively. Furthermore, the lattice derivative is defined as µ ψ(r) = ψ(r + µ) ˆ − ψ(r) Taking the continuum limit aµ → 0, the effective Hamiltonian for the lattice Ginzburg–Landau model Eq. 10.12 reduces correctly to the Ginzburg–Landau effective Hamiltonian in the continuum (Eq. 10.8). As defined in Eq. 10.12, the lattice Ginzburg–Landau model does not contain vortices. To reintroduce the vortices in the model, we must compactify the gauge-theory by requiring that the gauge invariant phase differences satisfy 2π θ (x + µ) ˆ − θ (x) − aµ Aµ (x) ∈ [−π, π

0

(10.13)

Whenever this constraint is used to bring the gauge invariant phase differences back to its primary interval, we automatically introduce a unit closed vortex loop, and the net vorticity of the system is guaranteed to be conserved at every stage of the Monte-Carlo simulation. From the renormalization group point of view the continuum Ginzburg–Landau model and the lattice Ginzburg–Landau model belong to the same universality class. We therefore expect the lattice Ginzburg–Landau model and the continuum Ginzburg–Landau model to give, qualitatively, the same results.

10.2.1

Lattice Ginzburg–Landau model in a frozen gauge approximation

In extreme type II superconductors, the zero temperature mean-field penetration depth is much greater than the zero temperature coherence length, λµ (T = 0) ξµ (T = 0). Thus, fluctuations of the gauge field represented by the last term in Eq. 10.8, around the extremal field configuration are strongly suppressed and can therefore be neglected. The effective Hamiltonian for the frozen gauge (FG)

LATTICE FORMULATION OF THE GINZBURG–LANDAU THEORY

285

model can be written as HFG =

α(T ) |α(0)|2 1 ax ay az |ψ |2 + |ψ |4 g α(0) 2 r +

|ψ (r + µ)||ψ ˆ (r)| 2−2 cos(µ θ − Aµ ) (10.14) 2

ξµ2

a µ=x,y,z µ

Here, we have defined a dimensionless order field and vector potential ψ =

Aµ =

ψ |α(0)| g

→ |ψ | ∼ [0, 1]

2π aµ Aµ

0

The natural energy scale along the µ-direction is, Jµ = 2

ξµ2 |α(0)|2 ax ay az 2 g aµ

Assuming a uniaxial anisotropy along the z-axis, the natural energy scale for the FG model is J0 = Jx =

20 d 2|α(0)|2 2 ξab az = g 4π 2 µ0 λ2ab

(10.15)

Here, we have put our coordinates (x, y, z)-axis parallel to the crystals (a, b, c)axis. Furthermore, ξx = ξy = ξab and ξz = ξc is the coherence length in the CuO-planes and along the crystal’s c-axis, respectively. Furthermore, λx = λy = λab and λz = λc is the penetration depth in the CuO-planes and along the crystals’ c-axis, respectively. In Eq. 10.15, d is the distance between two CuO superconducting planes in adjacent unit cells. The energy scale J0 is roughly the energy scale of exciting a unit vortex loop. The ratio between the energy scales Jx and Jz serves as an anisotropy parameter, ξab az λc az Jx = = (10.16) = Jz ξc ax λab ax In this model, the lattice constant aµ should be defined as aµ = max(dµ , C0 ξµ )

286

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Here, dµ is an intrinsic length along the µ-direction in the underlying superconductor to be modelled. Examples of such an intrinsic length are the distance between CuO-planes in adjacent unit cells, the (a, b)-dimension of the unit cell. To be consistent, the constant C0 should be larger than ∼4. This requirement aµ /ξµ > 4 ensures that the amplitude of the order field does not overlap [142]. Such overlap will give rise to a domain wall term (∇|ψ|), which is absent in the lattice Ginzburg–Landau model. Within the frozen gauge approximation, the gauge field serves only as a constraint, fixing the value of the uniform induction. In terms of magnetic induction this approximation is valid when B Bc1 (T ), where the field distribution from individual flux lines overlap strongly, giving uniform induction. Note that Bc1 (T ) also vanishes when the temperature approaches Tc . In zero field, this approximation is valid for all temperatures except an inaccessibly narrow temperature region around Tc .

10.3 Preliminary results Before we proceed, let us make a few remarks on the neglect of amplitude fluctuations in the type II regime. Is the neglect of such fluctuations in ψ in the above theory defined by Eq. 10.7 really a good approximation? It is well established to be correct in two dimensions. However, as is well known, in four dimensions mean field theory is exact, and in this case amplitude fluctuations alone suffice to correctly describe the phase transition. Three dimensions is between two and four, but is it, in some sense, closer to two dimensions than to four dimensions or vice versa? To answer this, consider the results of largescale Monte Carlo simulations performed directly on the lattice version of the theory defined by Eq. 10.14 in the absence of a gauge field [29]. All phase fluctuations as well as amplitude fluctuations are taken into account, and we now ask ourselves what these various fluctuations do close to the critical point where the superfluid density vanishes. This is shown in Figure 10.1. The Cooper-pair density |ψ|2 behaves quite differently from the superfluid density ϒ and the superconducting order parameter | ψ |2 , in that the former still is quite sizeable at and slightly above Tc , whereas the superfluid density vanishes. We thus conclude that if amplitude fluctuations alone had been capable of describing the phase transition from superfluid to normal fluid or from superconductor to metal, then the Cooper-pair density would have vanished at Tc . It does not, and the superfluid density is brought to zero at Tc by phasefluctuations [29, 31, 32, 143]. We shall now investigate the effect of longitudinal phase-fluctuations first, following the same path as in Chapter 9. As we shall see, longitudinal phase-fluctuations are even more innocuous in three dimensions than in two, whence it follows that the destruction of superfluid density is caused by transverse phase fluctuations.

PRELIMINARY RESULTS

287

0.8

D q (q)

1

ϒz

0.6

0.45 0.4 0.35 0.3 0.25 0.2 0.15 0.1 0.05 0

T′ = 0.1 T′ = 0.2 T′ = 0.3 T′ = 0.4 T′ = 0.5 T′ = 0.56

0

0.4 FG f=0 0.2 Γ=1 T ′MF = 1 0 0

2p

p

q

| < y′ > |2

< |y′|2 >

0.2

0.4

0.6

0.8

1

T′ 1 0.8 ϒz

D q (q)

0.4

0.6

T′= 0.10 T′= 0.14 T′= 0.18 T′= 0.21 T′= 0.22 T′= 0.23

0.3 0.2 0.1 0 0

0.4 FG f=0 Γ=1 T′MF = 0.3

0.2 0 0

| < y′ > |2

2p

p

q

< |y′|2 > 0.1

0.2

0.3

0.4

T′

Figure 10.1 Superfluid density ϒ, superconducting order parameter | ψ |2 (often called condensate fraction in the He4 literature, and Cooper-pair density |ψ|2 . Note how ϒ and | ψ |2 , both of which contain phase-fluctuations, are brought to zero at Tc , while | ψ |2 which does not contain phase-fluctuations, is still finite at Tc . This demonstrates that amplitude fluctuations are not critical at Tc . (adapted from Fig. 1 in Ref. [29]).

As in the two-dimensional case, we may write the effective action when only smooth phase-fluctuations are taken into account, in the form ρ0 S= 2

d3 r (∇θ )2

(10.17)

where ρ0 formally appears as same bare phase stiffness in the problem (analogous to J in the XY -model) which in the above units is given by ρ0 = 1. However, we will retain it in the following in order to remind ourselves of the presence of this bare stiffness in the problem. In the above, it is assumed that ∇θ is non-singular, which means that we ignore the angular (compact) nature of the phase-field θ .

288

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

The following discussion closely parallels that of the low-temperature discussion of the two-dimensional XY -model in Chapter 9. Consider the effect of the longitudinal phase fluctuations in computing the correlation function probing superconducting off-diagonal long-range order (ODLRO), 2 (r) = ψ ∗ (r)ψ(0) = ei[θ (r)−θ (0)]

= e [θ (r)−θ (0)]θ (0) = eG(r)

(10.18)

when only spin-wave fluctuations are included in the Hamiltonian, and where G(r) = [θ (r) − θ (0)]θ (0)

(10.19)

just as in Chapter 9. By using the equipartition theorem precisely in the same way as in Chapter 9, we obtain in the present units kB T G(r) = ρ0

d3 q eiqr − 1 (2π )3 q 2

(10.20)

Of interest for the purposes of establishing ODLRO, is the asymptotic longdistance behaviour of G(r). Compute the above integral by introducing a large momentum cutoff in the problem. It is straightforward to see that G(r) has the following form, r0 r kB T Si() r0 = 2π 2 ρ0 kB T K= 2π 2 ρ0

G(r) = −K +

(10.21)

where r0 is some characteristic length, and Si() = 0 du sin(u)/u is the sineintegral. Note how G(r) again vanishes as T → 0. Now we insert this into 2 (r) to obtain the long-distance behaviour r0

2 (r) = e−K+ r

(10.22)

where the expression for 2 (r) basically applies for r ≥ −1 . It is seen that 2 (r) decreases with r, but it is finite when r → ∞. Moreover, since the entire exponent in 2 (r) is negative, this implies that the correlation function is suppressed with increasing T at fixed r. Eq. 10.22 is drastically different from the two-dimensional case in that the spinwaves are not capable of

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

289

destroying ODLRO at all in three dimensions, whereas they are capable of reducing ODLRO to quasi-long range (but not short-range) order in two dimensions. Hence, as in the two-dimensional case, the fluctuations ultimately responsible for producing short-range order and a transition to a normal fluid/metal, are transverse phase fluctuations. Let us now incorporate them in the description, in much the same way as was done in Chapter 9. There will, however, be crucial differences, since transverse phase fluctuations in three dimensions give rise, not to point-like vortices as in two dimensions, but rather closed vortexloops, considered recently in great detail in the context of high-temperature superconductors by Tesanovic and Sudbø and co-workers [29, 32].

10.4 Vortex-loops as topological defects of the order parameter We will proceed as in the two-dimensional case by regularizing the Ginzburg– Landau theory (Eq. 10.4) on a lattice, ignoring amplitude fluctuations, as follows Z = dθ dAe−S(θ,A) S(θ, A) =

βJ x

J=

1 |( − ieA)e | + ( × A)2 2 2

iθ 2

a|ψ0 |2 m∗

(10.23)

where is a lattice derivative, a is a lattice constant of the numerical lattice, and ψ0 is the amplitude of the ψ-field, which we take to be uniform throughout the system. Finally, we expand the kinetic energy operator as follows

ˆ µ (x) 2 | = 2 1 − cos(µ θ (x) − eAµ (x)) |(µ − ieAµ )eiθ |2 → |eiθ (x+a µ)−iaA (10.24) We ignore the constant term, and set J = 1, thus getting Z = dθ dAe−S S=

−β cos(µ θ (x) − eAµ (x)) + 12 ( × A)2

(10.25)

x

We now follow steps similar to those in Chapter 9, and replace this cosinepotential by a periodic Gaussian one, thus obtaining the partition function

290

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Z=

dθ dAe−S(ψ,A)

n

S=

β x

2

(θ − eA + 2π n)2 + 12 ( × A)2

(10.26)

which is now the Villain-approximation to the three-dimensional lattice London model (i.e. three dimensional XY model coupled minimally to a fluctuating gauge field). Here, we have introduced an integer valued velocity field n, which we may view as the integer part of the gauge-invariant phase-difference θ − ieA. The field n will figure prominently in our discussion below. The kinetic term is linearized, as in Chapter 9, by introducing the Hubbard–Stratonovic decoupling 2 β 2 − v +ivu (10.27) e− 2 u = dv e 2β which allows us to write the partition function of the form Z= dθ dA dv e−S n

1 1 2 2 S= v + iv(θ − eA + 2π n) + ( × A) 2β 2 x

(10.28)

Now, we proceed by performing the θ -integrations. This yields the constraint µ vµi = 0

(10.29)

which is solved by introducing the new vector field hµi satisfying vµi = εµνλ ν hλi

(10.30)

where εµνλ is the three-dimensional Levi–Civita tensor. Now the partition function is given by Z= dA dh e−S n

1 1 2 2 S= ( × h) − i × h(eA − 2π n) + ( × A) (10.31) 2β 2 x By a partial integration of the second and third term in this action, it may be written as 1 1 2 2 S= ( × h) + ieh( × A) − i2π h( × n) + ( × A) 2β 2 x (10.32)

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

291

Next, we perform the sum over n in Eq. 10.31. By the Poisson summation formula, this converts the v-field into an integer valued field, equivalently h becomes integer valued. We will come back in a moment to exactly what the physical interpretation of this new vector field is. As a result of the above, we may write the partition function as Z= dA e−S {h}

1 1 2 2 ( × h) − ie × hA + ( × A) S= 2β 2 x

(10.33)

Now, it is a somewhat awkward fact that while the gauge field A is real valued, the vector field h is integer valued. This may be remedied by again using the Poisson summation formula to lift the field h from Z to R by introducing another integer valued field m in the partition function, thus writing it on the form Z= dh dAe−S {m}

1 1 2 2 ( × h) − ie × hA + ( × A) − i2π mh (10.34) S= 2β 2 x By comparing the action in Eq. 10.34 with the action Eq. 10.32, we arrive at the following physical interpretation of the new vector field m. We see that m=×n

(10.35)

Since n is the integer part of the gauge-invariant phase difference we started with, it is a current. Since m is the curl of this, it is the vorticity of this phase difference. In other words, the fields m are segments of vortex excitations in the superconducting ordering field. Finally, from Eq. 10.35, we see that µ mµi = 0

(10.36)

This means that the vortex segments are divergence free fields, and form closed loops. Thus, we have identified the topological defects in the Ginzburg–Landau model, they are precisely these vortex loops. (Note how the use of the phrase vortex ring is meticulously avoided!) The analogue of the Kosterlitz–Thouless vortex-pair unbinding taking place in the two-dimensional case will now be a vortex-loop unbinding characterized by a low-temperature phase of vortex loops with finite linetension and finite perimeter into a high-temperature phase characterized by vortex tangle with no line tension of the vortex loops, which therefore exist on all length scales up to and including the system size.

292

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Note how there is one feature which distinguishes the three-dimensional situation from the two-dimensional. Vortex–antivortex pairs have one characteristic feature, and that is the separation between the vortex and the antivortex. A vortex loop is an infinitely more complicated object, in that it also has shape. This is the basic feature which precludes the possibility of constructing, in a consistent manner, a Kosterlitz–Thouless style of renormalization group approach to the problem in three dimensions. Next, let us integrate out the electromagnetic gauge field A. We rewrite the action introducing Fourier-modes of the field A as follows 1 ie µ S= |Qq |2 + iπ(mq h−q + m−q hq ) − Aq (Qq × h−q )µ 2β 2 q 1 µ µ + A−q (Q−q × hq )µ + |Q−q A−q |2 (10.37) 2 Completion of squares is accomplished by introducing the auxiliary quantities 1 A+ q = (Aq + A−q ) 2 1 A+ (Aq − A−q ) q = 2i

(10.38)

and ie (Qq × h−q + Qq × h−q ) 2 e 0− = (Q−q × hq − Q−q × hq ) 2 0+ =

(10.39)

As a result of this, the A-part of the action may be written in the form

1 1 + 2 − 2 + 2 − 2 ˜ ˜ [( Q |[( A ) + ( A ) ] − ) + ( ) ] S= |Q q −q 0 0 2 q |Qq Q−q | e2 hq h−q

(10.40) The integrals over the shifted gauge-fields A˜ ± in the partition function are Gaussian and may be performed. Hence, the net result of integrating out these fields is to produce a term in the remaining part of the action which is simply a mass-term for the h-field. Note how the presence of the mass term depends on the existence of a charge e in the problem. In order to interpret this mass, we

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

293

proceed by integrating out the h-field. The remaining part of the action prior to integrating out the h-field now reads 1 e2 Qq Q−q hq h−q + hq h−q (10.41) S= π i(mq h−q + m−q hq ) + 2β 2 q We introduce 1 h+ q = (hq + h−q ) 2 1 h+ (hq − h−q ) q = 2i

(10.42)

along with iπ (m−q + m−q ) 2 e − 0 = 2 (mq − m−q )

1 2 Qq Q−q e + ξ2 = 2 β + 0 =

(10.43)

Introducing these variables into the action and completing squares, we get + 2 − 2 0 0 1 1 − 2 2 ξ 2 h+ S= + h− − 2 ((+ (10.44) q 2 q 2 0 ) + (0 ) ) 2 q ξ ξ ξ The shifted h field may now be integrated over, to give the final form of the action in terms of an interacting gas of closed vortex loops as follows mq m−q (10.45) S=β 2 e β + Qq Q−q q This may be written in term of real-space vortex segments interacting with a potential in terms of the following Hamiltonian, to be used in the partition function H = −2π 2 J0 m(x1 )V (x1 − x2 )m(x1 ) x1 ,x2

V (x) =

q

4

µ

where λ−2 = e2 β.

e−iqr sin2 (qµ /2) + λ−2

(10.46)

294

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

We now see that the mass e2 of the gauge-field h shows up as a screening length in the interaction between vortex segments. The charge in the original problem, i.e. the charge of the superconducting condensate, leads to short-range interactions between the vortex-loop segments. Setting the charge equal to zero in the above, we obtain an equivalent description of a neutral superfluid, such as He4 . The gauge field decouples from the order parameter in Eq. 10.25, and can simply be ignored as it gives rise to an additive analytic contribution to the free energy. The remaining model is the three-dimensional XY model. It may be written in terms of vortex-loop segments following the steps we have just gone through, and the result is Eq. 10.46 with screening length set to infinity. This means that the potential V (x) is the unscreened Coulomb potential in three dimension. Note that such a potential satisfies the Laplace equation −∂ 2 V (xx) = δ(x) in the continuum. Let us rederive the above result for the neutral case in an alternative manner following what we did in Chapter 9. In the continuum limit the threedimensional XY model may be written as J0 d3 r(∂θ )2 H= 2 J0 d3 r (∂θL )2 + (∂θT )2 = (10.47) 2 Again, we have split the gradient of the phase into a regular spin-wave part ∂θL and a part ∂θT giving rise to vortex segments. The latter part satisfies the equation εµνλ ∂ν (∂λ θT ) = 2π nµ where nµ (r) is a local vorticity in the µ-direction, and εµνλ is the threedimensional Levi–Civita tensor. A representation of (∂µ θT ) that satisfies this equation is the following (∂µ θT ) = −2π εµνλ ∂ν d3 r G(r − r )nλ (r ) (10.48) where G(r) is a solution to the three-dimensional Laplace equation, −∂ 2 G(r) = δ(r). The verification of this follows the lines given for the two-dimensional case in Chapter 9. If we now insert this representation into Eq. 10.47, using the Laplace equation for G(r) and the fact that ενλρ ενησ = δλη δρσ − δλσ δρη , we find J0 3 2 2 3 d r(∂θL ) + 2π J0 d r d3 r nµ (r)G(r − r )nµ (r ) (10.49) H = 2 Here, we have used a partial integration in the second term along with the fact that ∂µ nµ (r) = 0. The above describes a system of spin waves decoupled from

SUPERCONDUCTOR–SUPERFLUID DUALITY IN d = 3

295

a system of vortex segments forming closed loops and interacting with a threedimensional unscreened Coulomb potential (anti Biot–Savart law). Eq. 10.49 is therefore the continuum version of Eq. 10.46 with no screening, λ = ∞, when the spin-wave part is ignored. Coupling between spin waves and vortices are seen to be higher-order gradient terms and are therefore, as in the two-dimensional case, irrelevant in renormalization group sense.

10.5 Superconductor–superfluid duality in d = 3 In this section, we will formulate a Ginzburg–Landau theory for the above action for the system of interacting vortex segments forming closed loops. This Ginzburg–Landau theory is therefore a field theory of the ensemble of topological defects of the original Ginzburg–Landau theory of the superconductor, and hence a dual theory to the original system. Incidentally, we note in passing that we can also describe superfluidity in He4 simply by setting the charge e = 0. We shall now demonstrate that the dual theory to the Ginzburg–Landau theory of a superconductor is the Ginzburg–Landau theory of a charge-neutral superfluid, and vice versa. The details are as follows. The key point is to compare two equations derived above from the original Ginzburg–Landau theory. The two equations we compare are Eqs 10.28 and 10.32, written out in real space as follows

DA

Z(β) =

v

Z(β) =

Dh

m

exp − exp −

v2 x

1 − ivA + (∇ × A)2 2β 2

m2 x

2

e2 1 + 2π imh + h2 + (∇ × h)2 2 2β

(10.50) The first of these is Eq. 10.28 after having performed the θ -integrations and nsum. The second equation is Eq. 10.32 written in real space, with a term h2 /2 added by hand. The crucial observation now is that Eq. 10.28 is basically a version of the original Ginzburg–Landau model! Eq. 10.32 on the other hand, is a version of the vortex-loop gas formulation of the model. The point to note is that the action in these two partition functions are basically identical, provided we make the identification 1 2 v → h2 2β 2 1 1 (∇ × A)2 → (∇ × h)2 2 2β −bA → 2π mh

(10.51)

296

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Adding the extra term h2 /2 in the second of Eq. 10.50 is like adding a short-range interaction between vortex segments. This is an irrelevant perturbation, in renormalization group sense, to the already existing short-range piece of the interaction between vortex segments, and is not expected to alter the long-distance physics. Now, since we know that the first of the two equations Eq. 10.50 corresponds to a Ginzburg–Landau theory, it follows that the second one also does so. In the continuum limit, the field theory description of the second of Eq. 10.50 is therefore of a form [29, 32, 144, 145]

S(h, φ) =

d3 x

1 e2 (∇ × h)2 + h2 + m2φ |φ|2 + uφ |φ|4 + |(∇ − ied )φ|2 2β 2

(10.52) The field φ is a complex matter field describing the vortex segments of the theory, in the same way that the field in the original Ginzburg–Landau theory was a a matter field describing Cooper-pairs giving rise to segments of supercurrents. Moreover, ed = 2π in the units we are working with here. It has the interpretation of being a dual charge coupling the vortex segments, or equivalently the matter field φ, to the gauge-field h which mediates the (anti) Biot–Savart interaction between vortex segments. Finally, the term m2π |φ|2 is a local chemical potential term for the vortex segments, while the term uφ |φ|4 represents a steric repulsion between vortex segments. Eq. 10.52 is of the same form as Eq. 10.4 except for the mass term e2 h2 /2 of the gauge-field h. Note that if we had started out with a neutral theory in Eq. 10.4, e = 0, we would have ended up with a dual theory Eq. 10.52 of the same form as Eq. 10.4 with finite charge e. Hence, the dual theory of a superfluid in d = 3 is immediately seen to be the Ginzburg–Landau theory of a superconductor. To see the converse, namely that the dual of a superconductor is a neutral superfluid, is only slightly more involved. A physically intuitive argument proceeds as follows (more involved arguments involving renormalization group calculations merely confirm the correctness of the physical picture we shall give). In the presence of a finite charge in Eq. 10.4, the gauge field h in Eq. 10.52 is massive. This means (in complete analogy with, for instance, the massive meson-field mediating short-range nuclear interactions) that when e2 = 0, the gauge field mediates a short-range interaction between vortex segments, with range given by e−1 . Now, by the dimensional analysis leading to Eq. 10.5, charge has a positive scaling dimension when d = 3, whence ∂e2 >0 ∂l

(10.53)

Thus, for the purposes of describing the long-distance physics, we may set the renormalized effective charge liml→∞ e2 (l) = ∞ once the bare charge is non-zero. This means that on long length scales the gauge-field is suppressed

SUPERCONDUCTOR–SUPERFLUID DUALITY IN d = 3

297

completely in the action and may be discarded. The physics of this is that the short-range Biot–Savart interaction is an irrelevant perturbation to the steric repulsion represented by the term uφ |φ|4 . Hence, the long-wavelength physics is described correctly by Eq. 10.52, but with h removed from the action, namely S(φ) =

d3 x m2φ |φ|2 + uφ |φ|4 + |∇φ|2

(10.54)

This is nothing but the Ginzburg–Landau theory of a neutral superfluid. Thus, the dual of a three-dimensional superconductor is a three dimensional superfluid. Another point to note here, as a consistency check, is the following. Suppose we start out with a superconductor and dualize it once. The resulting dual action is that of a neutral superfluid. Suppose now that we dualize once more. This means that we are out to obtain the dual of the dual of a superconductor, which is the dual of a neutral superfluid. This, as we have seen, is just a superconductor. Hence, dualizing twice brings us, quite correctly, back to the starting point, Dˆ 2 = 1, where Dˆ is the duality operator. Based on the above, we can immediately infer that a vortex-loop tangle consisting of non-interacting vortex segments (a very peculiar case, admittedly, but as we shall see not entirely academic), is simply described by the Gaussian field theory S(φ) =

d3 x m2φ |φ|2 + |∇φ|2

(10.55)

The essential content of the above is shown in Figure 10.2. Observe the isomorphism along both the diagonals. Of course what is dual, and what is original theory eventually becomes a relative notion.

Duality transformation Original charged S(y, A)

Dual neutral S(f)

Original neutral S(y)

Dual charged S (f, h)

Figure 10.2 The relations between charged and neutral versions of the original and dual theory. The dashed lines indicate isomorphism.

298

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

10.6 Zero-field vortex-loop blowout Consider now for the moment the case of zero magnetic field. The main advantage of the above formulation is that the probability of finding a connected path of vortex segments, starting at x and ending at y, G(x, y), is given by the two-point correlation function of the φ-field [145] G(x, y) = φ ∗ (x)φ(y)

(10.56)

A vortex-loop unbinding will lead to a finite G(x, y) when |x − y| → ∞, because infinitely large loops will connect opposite sides of the vortex system. On the other hand, if lim|x−y|→∞ G(x, y) = 0, this implies that φ ∗ (x) = 0, corresponding to a broken U (1)-symmetry. Therefore, the dual field φ(r) is an order parameter of a vortex-loop unbinding transition. The broken U (1)-symmetry is associated with the loss of number conservation of connected vortex-paths threading the system in any direction (including direction perpendicular to an applied magnetic field, if that is present). This limit of the two-point correlation function is closely related to a quantity OL we will introduce below, which probes the connectivity of the vortex tangle in an extreme type II superconductor. The above connection makes it at the very least plausible that an abrupt change in this connectivity, as probed by the change in OL , is associated with breaking a U (1)-symmetry of the vortexsector of the GL-theory, equivalently an onset φ ∗ or φ . Since this only happens above a critical temperature, we may view φ as a disorder-field, in contrast to the order-parameter field ψ of the original GL-theory. We will make explicit use of this connection later on. In zero magnetic field, we will show that the loss of superfluid density, specific heat anomaly, change in vortex-loop distribution, loss of long-wavelength vortex-line tension, and abrupt change in vortex tangle connectivity abruptly occurs precisely at the same temperature both for the three-dimensional XY model, also when amplitude fluctuations are included. Thus we may associate the the phase transition from superconductor to normal metal or neutral superfluid to normal fluid (such as the λ-transition in H e4 ) as a vortex-loop blowout. The idea of a vortex-loop blowout being responsible for the λ-transition in He4 (also denoted helium II) must be credited to Onsager [146]. Ref. [146] is a discussion remark from as early as 1949, and the two last sentences of the remark are well worth quoting: ‘Finally, we can have vortex rings in the liquid, and the thermal excitation of Helium II, apart from the phonons, is presumably due to vortex rings of molecular size. As a possible interpretation of the λtransition, we can understand that when the concentration of vortices reaches the point where they form a connected tangle throughout the liquid, then the liquid becomes normal’. This is qualitatively the right idea. Note, however, how we have meticulously avoided the use of the phrase ‘vortex rings’ in our treatment, and used the phrase ‘vortex-loops’ instead. Vortex rings are precisely

299

ZERO-FIELD VORTEX-LOOP BLOWOUT

that, namely rings, while vortex-loops can have much more complicated shapes, being crinkled to a degree that one cannot speak even crudely of ring-like shapes, the hole in the doughnut is in fact completely filled in. This is an essential feature, since it endows the vortex loops with enough configurational entropy to be able to overcome the internal energy such that the line tension of the vortices, which is the free energy per unit length, may be driven to zero. An object that on large length scales looks like a ring, will have a Hausdorff dimension of 1. As we shall see in this chapter, however, the vortex-loop tangle arising out of a neutral superfluid has Hausdorff dimension larger than 2. For a superconductor, the Hausdorff dimension of the vortex-loop tangle is slightly smaller than 2. In any case, it is clear that one cannot speak of ring-like objects. The truly remarkable thing about Onsager’s vision from 1949, is that he correctly identified the nature of the topological defects in the order parameter which are responsible for driving the phase transition. The idea (as so many of Onsager’s ideas) was far ahead of its time, and there was no hope of putting them on a quantitative level back in 1949. Only with the advent of the Kosterlitz–Thouless theory in 1973 [130, 131] was the much simpler problem of vortex–antivortex unbinding tackled in two dimensions! Note that if one takes a vortex loop and slices through it with a plane, the loop cuts the plane in two places, which are the locations of a vortex and an antivortex. Hence, the two-dimensional counterpart of Onsager’s vortex-loop blowout is the vortex-antivortex unbinding of Kosterlitz and Thouless.

10.6.1

Definitions

Specific heat C To calculate the specific heat per site C, we use the fluctuation formula, 1 H 2 − H 2 C = . kB V (kB T )2

(10.57)

Here, the dimensionless volume V = Lx Ly Lz , and Lµ is the dimensionless linear dimension of the system along the µ-direction. Lµ is measured in units of the lattice constant aµ . As a check of consistency, we may also calculate the specific heat per site using the numerical derivation of the internal energy U , CU =

1 ∂U V ∂T

(10.58)

Note that for the FG model, where the effective Hamiltonian depends explicitly on the temperature, there strictly speaking is an additional term in the expression

300

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

for the internal energy,

∂ ln Z ∂H U =− = H − T ∂β ∂T

∼ For the three-dimensional XY model, if the simulations are properly done, C = CU . For the FG model, where the effective Hamiltonian explicitly depends on the temperature, C = CU . Note however that ∂H /∂T arises out of introducing a temperature dependence of the coefficients of the Ginzburg–Landau theory. The temperature dependence of these coefficients always has a temperature dependence set by the mean-field critical temperature. Thus, close to the true Tc these corrections, arising from integrating out the fermions of the underlying microscopic description of the superconductor, are always negligible compared to the contribution coming from the true critical fluctuations of the order parameter, i.e. the transverse phase-fluctuations. In terms of Eq. 10.15 the term −T ∂H /∂T

originates from the temperature dependence of the amplitude of the orderparameter. Were this to actually vanish at T = Tc , substantial corrections to the specific heat and entropy would result. As we will see later, at T = Tc , the ensemble average of the amplitude of the order parameter is far from renormalized to zero by vortex-loop fluctuations. Hence, at the critical point the correction term −T ∂H /∂T in the internal energy, with its resulting corrections to entropy, is negligible. There is now ample experimental evidence from the group of Ong at Princeton [147], that critical fluctuations are indeed important over a sizeable temperature window in the high-Tc cuprates of order several Kelvin below Tc a window which is consistent with a coherence length of order 10 ˚A, about two orders of magnitude shorter than in conventional superconductors. Local Cooper-pair density |ψ |2 As a probe for the local Cooper-pair density, we calculate |ψ |2 ≡

1 |ψ (r)|2

V r

(10.59)

We see in Eq.√10.59 that |ψ |2 involves both thermal and space average. Recall that ψ ≡ ψ/ |α(0)|/g. At the mean field level, we expect |ψ |2 to develop an expectation value below the mean field critical temperature TMF (B). Superfluid condensate density |ψ |2 As a probe for the local condensate density (density of Cooper-pairs participating in the superconducting condensate), we calculate | ψ |2 ≡

1 | ψ (r) |2 V r

(10.60)

ZERO-FIELD VORTEX-LOOP BLOWOUT

301

Note the difference between |ψ |2 and | ψ |2 . The former describes local Cooper-pair density, while the latter describes what is commonly known as the condensate density in 4 He-physics. In zero field, we expect | ψ |2 to develop an expectation value below the critical temperature Tc . Distribution of the order field phase angle To probe the distribution of the phase angle in ψ (r) = |ψ (r)|eiθ (r) , we define the distribution function ! 1 (10.61) δθ (r),θ Dθ (θ ) = V r Here, δi,j is the Kronecker delta function. In the simulations, we have chosen to work with a discrete set of phase angles, θ , θ (r) = 2π n/Nθ . Here, n ∈ [0, Nθ ] is an integer, and Nθ is the number of allowed discrete phase angles. In our > experience, the simulation results do not depend on Nθ , provided Nθ ∼ 16. In zero field, when the phase is disordered, we expect Dθ (θ ) to be uniformly distributed, D(θ ) = 1/Nθ . In the ordered phase, we expect Dθ (θ ) to show a peak around a preferred phase angle. Helicity modulus ϒµ To probe the global superconducting phase coherence across the system, we consider the helicity modulus ϒµ , defined as the second derivate of the free energy with respect to an infinitesimal phase twist in the µ-direction. Finite ϒµ means that the system can carry a supercurrent along the µ-direction. Within the three-dimensional XY-model, the helicity modulus along the µ-direction becomes, ! ϒµ 1 = cos[µ θ − Aµ ] Jµ V r 2 ! Jµ . sin[µ θ − Aµ ] − kB T V r For the FG case, ! ϒµ 1 = |ψ (r)||ψ (r + µ)| ˆ cos[µ θ − Aµ ] Jµ V r 2 ! Jµ . − × |ψ (r)||ψ (r + µ)| ˆ sin[µ θ − Aµ ] kB T V r

302

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Note the difference between | ψ |2 and ϒµ , they are not identical. The former quantity probes the superfluid condensate density, which is a locally defined quantity, while the latter quantity probes a global phase coherence along a given direction µ. Since ψ is the order parameter of the Ginzburg–Landau theory, close to the critical point we have | ψ |2 ∼ |τ |2β

(10.62)

where τ = (T − Tc )/Tc . On the other hand, ϒµ ∝ ρsµ , where ρsµ is the superfluid density in the µ-direction. Using the Josephson scaling relation ρsµ ∼ ξ 2−d ∼ |τ |ν(d−2) along with the scaling laws γ = ν(2 − η) and 2β = 2 − α − γ , we find ϒµ ∼ |τ |2β−ην

(10.63)

Here, d is the dimensionality of the system, ν is the correlation length exponent of the system, β is the order parameter exponent, γ is the order parameter susceptibility exponent, and η is the anomalous dimension of the order parameter two-point correlation function at the critical point. Therefore, although | ψ |2 and ϒµ are in principle different, they may appear to be very close if the anomalous dimension η of the ψ-field is small, as indeed is the case for the Ginzburg–Landau theory, where η ≈ 0.04. Note that for η > 0, the curve for ϒµ should bend more sharply towards zero at the critical point than | ψ |2 . We will explicitly show by direct calculations within the Ginzburg–Landau theory that | ψ |2 is very close to ϒµ both in zero field and finite magnetic field. In zero magnetic field this is precisely what one would expect based on the above, when η 1. For the special case of d = 3, we have 2β − ην = ν < 2β. To high precision, we have for the three-dimensional XY -model, that ν = 0.673 and η = 0.038. Vortex loop distribution D(p) To probe the typical perimeter L0 (T ) and the effective long-wavelength vortexline tension ε(T ) (not to be confused with the flux-line tension, which is always zero when gauge-fluctuations are completely suppressed due to the absence of tubes of confined magnetic flux), we define a vortex-loop distribution function D(p), which measures the ensemble-averaged number of vortex-loops in the system having a perimeter p. In order to compare results from different system sizes, we normalize D(p) with respect to the system size. We search for a vortex-loop using the following procedure. Given a vortex configuration, we start with a randomly chosen unit cell with vortex segments penetrating its plaquettes. We follow the directed vortex path and record the trace. When the directed vortex path encounters a unit cell containing more than one outgoing direction, we choose the outgoing direction randomly. When

ZERO-FIELD VORTEX-LOOP BLOWOUT

303

the vortex path encounters a previously visited unit cell, i.e. when it crosses its own trace, we have a closed vortex loop, its perimeter being p. We now delete the vortex-loop from the vortex configuration, to prevent double counting, and continue the search. The search is continued until all vortex segments are deleted from the system. Using a three-dimensional non-interacting boson analogy to the vortex system, it can be shown that the distribution function D(p) can be fitted to the form ε(T )p D(p) = Ap−α exp − (10.64) kB T Here, A is a temperature-independent constant, and the exponent α ≈ 5/2 to a first approximation. When ε(T ) is finite, there exists a typical length scale L0 = kB T /ε for the thermally excited vortex loops. The probability of finding vortex loops with much larger perimeter than L0 is exponentially suppressed, according to Eq. 10.64. When ε = 0, D(p) decays algebraically, and the length scale of the problem L0 = kB T /ε(T ), has diverged. As a consequence, configurational entropy associated with topological phase-fluctuations is gained without penalty in free energy. In zero field, there is only one critical point, and in this case L0 must be some power of the superconducting coherence length ξ(T ). Probe of vortex-connectivity, OL For probing the connectivity of a vortex tangle in a type II superconductor, in zero as well as finite magnetic field, we introduce a quantity OL , defined in zero magnetic field as the probability of finding a vortex configuration that can have at least one connected vortex path threading the entire system in any direction. In the presence of a finite magnetic field, OL is defined as the probability of finding a similarly connected vortex path in a direction transverse to the field direction, without using the PBC along the field direction. In zero field, we use the same procedure as in the finite-field, namely searching for connected vortex paths perpendicular to the z-direction, although in this case we could just as well have used any direction. Note that OL is very different from the winding number W in the two-dimensional boson analogy. There, W is proportional to the number of vortex paths percolating the system transverse to the field direction. However, in the calculation of W , the PBC along the field direction is used many times. This is entirely consistent with a number of other Monte Carlo simulation results on the three-dimensional XY -model which all show the loss of longitudinal phase-coherence and onset of longitudinal dissipation precisely at the vortex lattice melting transition. This is measured simply by the helicity modulus ϒz , which is quite different from OL . To the contrary, in our calculation of OL , we do not allow for the use of periodic boundary conditions in the z-direction to

304

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

measure vortex-tangle connectivity in the x- or y-directions. We have OL =

Nc Ntotal

(10.65)

Ntotal is the total number of independent vortex configurations provided by the Monte Carlo simulation. Furthermore, Nc is the number of vortex configurations containing at least one directed vortex path that traverses the entire system perpendicular to the direction, without using the PBC along the field direction. For convenience, we treat the zero field case as the limit limB→0 keeping the ‘field direction’ intact. We search for the possibility of finding a vortex path such as described above by using the following procedure. Assume that the magnetic induction points along the z-axis. We follow all paths of directed vortex segments starting from all four boundary surfaces with surface normal perpendicular to zˆ , and check whether at least one of these vortex paths percolates the system and reaches the opposite surface, without applying the PBC in the z-direction. Note that when crossing vortex segments are encountered, the procedure is to attempt to continue in a direction that will bring the path closer to the opposite side of the system, rather than randomly resolving the intersection. OL is therefore a necessary, but not sufficient condition for finding an actual vortex path crossing the system. However, in zero field this procedure does not make a difference to that of resolving the intersections randomly. This is demonstrated by the correlations of the change in OL and D(p), to be detailed in the next section. If a vortex path is actually found crossing the system in any direction in zero field, or without using PBC in the field-direction when a field is present, one may safely conclude that the vortex-line tension has vanished. If it were finite, it would not be possible to find such a path at all, either because all vortex-lines form closed confined loops in zero field, or because the vortex-line fluctuations along the field direction would be diffusive in finite field. In zerofield, this is clear by the above mentioned correlation between the change in OL and D(p), cf. the results of the next section. In this paper, we also investigate this in detail for the finite-field case, by considering the position of the lowest temperature TL where we have OL = 1 both as a function of system size and aspect ratio Lx /Lz = Ly /Lz . If vortex-line physics remains intact, TL should move monotonically up with system size, and should scale with Lx /Lz . Instead, we will find that TL moves down slightly, and saturates with increasing system size at fixed aspect ratio. In addition, we find that TL is virtually independent of aspect ratio for large enough systems. In the VLL phase OL = 0, since the field induced flux lines are well defined and do not ‘touch’ each other, and the thermally excited vortex-loops are confined to sizes smaller than the magnetic length. OL = 1 in the normal phase

ZERO-FIELD VORTEX-LOOP BLOWOUT

305

above the crossover region where the remnant of the zero field vortex-loop blowout takes place. Needless to say, it is a matter of interest to investigate precisely where OL changes value from zero to one. Note that OL itself is not a genuine thermodynamic order parameter, although it may be said to probe an order-disorder transition [29]. However, by the transcription of the vortex-content of the Ginzburg–Landau theory to the form of Eq. 10.52, it is brought out that probing the vortex-tangle connectivity by considering OL is closely connected to probing the two-point correlator of a local complex field φ(r), the dual field of the local vorticity-field mµ (r) of the Villain approximation and London approximation to the Ginzburg–Landau theory (Eq. 10.26). The two-point correlator φ ∗ (r)φ(r ) is ultimately the probe of whether or not the φ-theory (Eq. 10.52) exhibits off-diagonal long-range order and a broken U (1)-symmetry. An entirely equivalent interpretation of the change in OL does not involve a local field φ(r), but rather number conservation of vortex-lines threading the entire superconductor. This number is conjugate to the phase-field of the local complex field φ(r). An advantage of the present formulation involving Eq. 10.52 is that it directly relates he change in OL to the long-distance part of a correlation for a local field, and hence to a local order parameter φ(r) . This connection makes it at least plausible that the change in vortex-tangle connectivity, i.e. a change in the geometry of the vortextangle, may be related to a thermodynamic phase-transition. This is illustrated in Figure 10.3, where it is shown that the anomaly in the specific heat, the loss of superfluidity and the change in OL all occur at the same temperature. 3.5 3DXY f=0 Γ=7

3.0 2.5 2.0

C/k B

1.5 ϒz

1.0 0.5

OL 0 0

0.5

1.0

1.5

2.0

2.5

T′

Figure 10.3 Specific heat capacity C, helicity modulus ϒz and vortex-connectivity probe OL as functions of temperature. Note how the the anomaly in C, the vanishing of ϒz , and the onset of OL all occur at the same temperature.

306

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

10.7 Fractal dimension of a vortex-loop tangle One great advantage of the dual field theory formulation of the previous section is that it allows us to obtain information about critical exponents of the (dual) field theory by investigating geometric properties of the vortex-loop tangle. To see this, we first introduce the quantity P (x, y, N ) which is the probability of being able to perform a walk from the point x to the point y via a connected path of vortex segments in precisely N steps. Now, from this we can can derive several useful quantities. The one we shall focus on here is the probability distribution D(N ) of finding vortex loops of perimeter N . This is nothing but the probability of starting in point x and ending up in the same point in N steps, summed over all possible starting points x along the closed loop, normalizing to the number of starting points along the loop, which is just N . That is, we have D(N ) ∝

1 P (x, x, N ) ∝ N −α N x

(10.66)

This relation defines the geometric exponent α describing the vortex-loop tangle. (It should not be confused with the specific heat exponent.) Note also that all contributions in the above sum are equal, by translational invariance. Hence, we may pick out an arbitrary contribution to the sum, and invert to obtain P (x, x, N ) ∝ N 1−α

(10.67)

Note also that we have so far been careful to denote the configurations of vortex segments closing on themselves as vortex-loops, not vortex-rings. In fact the loops we are describing turn out to be highly crinkled line-objects which do not resemble rings at all. They are instead fractal objects with a Hausdorff dimension DH that can be computed from α. Not only that, but we may compute the anomalous scaling dimension ηφ for the dual matter field φ, from α. Let us demonstrate explicitly how this close connection between geometry and criticality in superconductors and superfluids can be found. Let us start with the simplest case, that of a tangle of non-interacting vortex segments. Then an analytic exact expression for P (x, x, N ) would be given by

1 (x − y)2 P (x, y, N ) ∝ d exp − (10.68) N N 2 with = 1/2. In analogy with this, we write down a scaling Ansatz for P (x, y, N ) for the general case of interacting loops as follows

|x − y| 1 (10.69) P (x, y, N ) ∝ d F N N 2

307

FRACTAL DIMENSION OF A VORTEX-LOOP TANGLE

where F is some scaling function and is some exponent, often called the wandering exponent, to be determined. This exponent is defined via the relation between the linear extent L of a walk and the number of steps N in the same walk, namely L ∼ N (10.70) Conversely, the number of links in a path of linear extent L is given by N ∼ L1/ ∼ LDH

(10.71)

where DH is the so-called Hausdorff dimension, or fractal dimension, of the vortex-loop tangle in the thermodynamic limit. For the non-interacting case, it can be shown that DH = 2. This follows immediately from what we have stated above, DH = 1/ = 2. If we merely add a steric repulsion to this, passing from Eq. 10.55 to Eq. 10.54, the effect must surely be to push vortex segments apart, thus reducing the Hausdorff-dimension, hence for this case we have DH < 2. Physically, this corresponds to the dual case of a charged three-dimensional superconductor. On the other hand, if we start out with a neutral superfluid, then the correct dual description is given by Eq. 10.52 with e2 = 0. In this case, in addition to having a steric repulsion between vortex segments we also have a long-range anti-Biot–Savart interaction between vortex segments. This latter interaction tends to produce a long-range attraction between vortex segments that are oppositely directed. This interaction will tend to compress the vortex tangle compared to the case with only steric repulsion. Moreover, we expect the long-range interaction to overcompensate the dilution of the tangle produced by the local steric repulsion such that in fact the tangle is even more compact than the non-interacting case. Thus, we expect that for the dual of a three-dimensional neutral superfluid, DH > 2. The various cases described above are illustrated in Figure 10.4.

Charged condensate

Gaussian loops

Neutral condensate

Figure 10.4 A schematic illustration of vortex loops in three cases. The three fractal dimenG < D (e = 0), where D G is the fractal sions are ordered according to: DH (e = 0) < DH H H dimension corresponding to a Gaussian field theory, i.e. random loops. Qualitively the three loops are self-avoiding, random and self-seeking.

308

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

We will be interested in the scaling function for |x − y| = 0. By combining Eqs 10.67 and 10.69 we find by simple inspection the scaling relation d = 1 − α

(10.72)

Let us now connect these geometrical properties of the vortex-loop tangle to statistical physics and critical properties. To do this, we consider the two-point correlation function for the dual field φ(x). We have G(x, y) = φ(x)φ ∗ (y)

(10.73)

This correlation function (propagator) is nothing but the probability amplitude of going from the point x to the point y via any connected vortex path. Hence, we have P (x, y, N ) (10.74) G(x, y) ∝ N

The sum over N in Eq. 10.74 cannot be performed exactly; however we will now focus on long loops such that the discrete character of the excursions of the vortex segments on the lattice can be neglected. We therefore replace the sum by an integral such that

1 (|x − y|) 1 G(x, y) ∼ dN d F (10.75) = N N 2 |x − y|d−1/ Close to criticality, on the other hand, we have the standard scaling Ansatz for the two-point correlation function G(x, y) ∼

1 |x − y|d−2+ηφ

(10.76)

which defines the anomalous scaling dimension ηφ . By comparing Eqs 10.72, 10.71, 10.75, and 10.76 we obtain the following scaling relations connecting geometric exponents of the vortex tangle to critical exponents of the dual field theory d =α−1 DH ηφ + DH = 2

(10.77)

For computational purposes it is most convenient to compute the geometric exponent α in simulations. The reason is that this quantity appears to have less finite-size effects than for instance those observed in direct computations of DH . However, once α is determined, DH and ηφ follow.

309

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

Table 10.1 Value of the loop-size distribution exponent, as determined from simulations Exponent

Gaussian

e=0

e = 0

α DH ηφ

5/2 2 1/2 0

2.312 ± 0.003 2.287 ± 0.004 0.437 ± 0.001 −0.287 ± 0.004

2.56 ± 0.03 1.92 ± 0.04 0.52 ± 0.01 0.08 ± 0.04

Limit α>2 DH < 3 > 1/3 ηφ > −1

The remaining exponents have been calculated using scaling relations Eq. 10.77. Gaussian results are exact, and confirmed for the different exponents independently.

In Table 10.1 we show results of large-scale Monte Carlo simulations [148] where the vortex-loop distribution exponent α has been computed, and scaling relations used to derive DH and ηφ . The qualitative picture described is Eq. 10.71 is confirmed by the results shown in Table 10.1. For the original charged case e = 0, corresponding to a dual theory which only features a steric repulsion, we indeed find DH 2, ηφ 0, while for the original neutral case corresponding to the dual charged case, we find DH 2, ηφ 0.

10.8 Type I versus type II, briefly revisited In this section, we will revisit the issue of type I versus type II superconductivity [45, 149]. As we have noted earlier, the distinction between the two is given in terms of the Ginzburg–Landau parameter κ = λ/ξ . At the mean-field level, the value of κ separating type I from type II behaviour is given by 1 κ=√ 2

(10.78)

Note also that when we speak of stable vortices as excitations in a superconductor, we are implicitly talking about type II superconductors. The reason is that in type I superconductors, vortices are not stable. This is due to the fact that for too small values of κ, the vortex-attraction of range ξ , overwhelms the vortexrepulsion due to circulating currents around each individual vortex, a repulsion of range λ. Alternatively, therefore, type I and type II superconductors can be viewed as superconductors where vortices interact attractively and repulsively, respectively. In this section, we start out with the Ginzburg–Landau model once again, but unlike the type II case studied in previous sections of this chapter, we do not ignore amplitude fluctuations of the superconducting order parameter. What we shall find is that the value of κ that separates type I from type II behaviour

310

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

is not precisely given by the mean-field estimate, but rather by [45, 149] κ=

0.76 ± 0.04 √ 2

(10.79)

This may be seen by reasoning as follows. We start out by performing large-scale Monte Carlo simulations on the full Ginzburg–Landau model, including amplitude fluctuations and phase-fluctuations in , as well as gauge-field fluctuations. As the system is warmed up, it passes from a low-temperature superconducting state to a high-temperature disordered state with no Meissner effect, which we obviously identify as the normal state. Now, we may compute the latent heat of this phase-transition as a function of κ. A first order phase transition has a non-zero latent heat, i.e. a jump in the entropy of the systems across the transition, whereas a second order phase transition does not. What is found is that the latent heat is finite deep in the type I regime, κ 1. The latent heat is zero deep in the type II regime, κ 1. The latent heat is found to vanish at a critical value of κ κ = κtri

(10.80)

where the numerical value is given in Eq. 10.79. We have denoted this critical value of κ by κtri , since it is the value that separates a first order phase transition from a second order one. A critical endpoint terminating a first order phasetransition line and where a second order phase-transition line commences, is a tricritical point. The above numerical result is in rather remarkable agreement with an early analytical calculation [144], which gave √ 3 3 4 " π #4 0.798 (10.81) κtri = 1− = √ 2π 9 3 2 Now, let us use the results of the previous sections to connect this change in character of the phase transition, from a first order to a second order on the one hand, to the notion of type I and type II superconductivity on the other. We will follow the discussions of Refs. [45, 149]. Because the critical fluctuations in a superconductor are vortex-loops, criticality at the phase transition from the superconducting state to the normal metallic state requires stable vortices to exist. I. e. they must interact repulsively. By the previous discussion, this requires the vortex tangle to have Hausdorff dimension DH ≤ 3 [148, 45]. A Hausdorff dimension equal to 3 would imply that the vortex tangle fills space in a compact manner, which is just another way of stating that the vortex system has collapsed on itself. Hence, if we were to monitor the vortex-loop distribution function in the first order regime, we would find DH = 3. By the scaling relation DH + ηφ = 2, we would conclude that ηφ = −1. Now, we may use the well-known Rushbrooke scaling law

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

311

2β = ν(d − 2 + ηφ ) to conclude that the order parameter exponent β = 0. That is, the order parameter vanishes discontinuously, the hallmark of a first order phase transition. On the other hand, for repulsive vortex interactions and a stable vortex tangle, DH < 3, ηφ < 1, and β > 0. This means that the superconducting order parameter vanishes in a continuous fashion, which is the hallmark of a second-order phase transition. Thus, via the connection between geometry and criticality, we find a first-order phase transition when vortices attract each other, and a second-order phase transition when vortices repel each other. However, as noted above, attractive and repulsive vortex interactions are precisely the characteristics of type I and type II superconductivity, respectively. Hence, we conclude that the distinction between type I and type II superconductivity is conceptually the same as the distinction between superconductors undergoing first order and second order phase transitions, respectively. The transition from one type of behaviour to the√ other happens at κtri , which is slightly renormalized from the mean field value 1/ 2. It should be noted that the latent heat even deep in the type II regime is tiny, and hence extremely precise measurements close to the critical temperature would be necessary in order to see the first order character. However, liquid crystals are described by a similar Ginzburg–Landau theory, as Eq. 10.7. In that case the Ginzburg–Landau parameter κ can be varied by varying the chemical compositions of the liquid crystal compounds and the latent heat involved in the smectic-A to nematic phase transition is sizeable. For such systems it has indeed been found experimentally that both first and second order phase transitions take place, depending on the value of κ [150]. We may summarize the discussion on effects of fluctuations in the Ginzburg– Landau model as follows. If we perform a mean-field analysis of the Ginzburg– Landau model, we arrive at the conclusion that the superconductor-normal metal transition is a second order phase transition with classical critical exponents. We may include effects of fluctuations both in the order parameter and the gaugefield A, arriving at different conclusions depending on what fluctuations we take into account. Historically, the first attempt at seriously considering fluctuation effects in the Ginzburg–Landau model were made by Halperin and co-workers who froze the superconducting order parameter ψ and considered only gauge-field fluctuations [43]. This is a procedure valid for extreme type I superconductors. The result is that this generates a term |ψ|3 in the free energy, with a negative coefficient. Since this now contains a cubic invariant, a first order phase-transition is inevitable. For the superconductors present at the beginning 1980s the critical region is extremely narrow, however the predicted jump in the entropy across the first order transition is found to be small, of order 0.01k per degree of freedom, where k is Boltzmann’s constant. Consequently the question was difficult to settle experimentally. However there is an isomorphism between superconductors and liquid crystals first discussed by Halperin and co-workers [151, 152], and on this system experiments can be done [153, 150].

312

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Table 10.2 A schematic view of some important results regarding the order of the phase transition in the GL model Description 1 At the mean field level the model reduces to the |ψ|4 theory, i.e. the effect of the gauge field vanishes completely. 2 |ψ|4 theory is a well known theory, which is much studied [154]. 3 To study the effect of the gauge field Halperin, Lubensky and Ma integrated out the gauge field exactly, this gives a cubic term in the remaining effective φ theory. This is a sound approach in the κ 1, i.e. strongly type I regime. 4 Dasgupta and Halperin studied the combined effects of phase and gauge field fluctuations, excluding amplitude fluctuations [155]. Various duality relations were derived, and the concept of an inverted XY transition was introduced. Excluding amplitude fluctuations is a valid approximation in the κ 1, i.e. strongly type II regime. 5 For the superconductors present at the beginning 1980s the critical region is extremely narrow, and the predicted jump across the first order transition very small. Consequently the question was difficult to settle experimentally. However there is an isomorphism between superconductors and liquid crystals [151, 152], and on this system experiments can be done [153, 150].

Fluctuations

Order

None

2.

|ψ|, arg ψ

2.

A

1.

arg ψ, A

2.

|ψ|, arg ψ, A (Experiment)

1. and 2.

Especially from cases 3 and 4 one can conclude that there must be a κtri separating first order and second order transitions. It is also important to realize that a correct description of this feature of the GL model requires a full description, including fluctuations in |ψ|, arg ψ and A. Adapted from Ref. [156].

The next serious step at considering fluctuation effects in superconductors was taken by Dasgupta and Halperin [155]. Here, they took the opposite approach, and ignored the gauge-field fluctuations altogether, focusing on the fluctuations in ψ of a specific type, namely phase fluctuations. As we have seen, this is a sensible procedure in extreme type II superconductors. A second order phase transition in the inverted three-dimensional XY universality class is found, i.e. a three-dimensional XY phase transition with inverted temperature axis (and a negative anomalous scaling exponent). In fact, we may also include the gaugefield fluctuations with the phase fluctuations, and the result is always a secondorder phase transition, as we have seen above [45, 149, 148]. Moreover, we may include amplitude fluctuations with phase fluctuations only, the result is still a permanent second order phase transition [154]. Thus, as long as we

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

313

y Normal state Tricritical point ytri

y c(x)

Type-I superconductor

Type-II superconductor x c(y)

xtri

0.5

x

Figure 10.5 Phase diagram of the Ginzburg–Landau model in the (x, y) plane (parameters as in Eq. 10.7). The value xtri = 0.295 ± 0.025, corresponding to a tricritical value of the √ . The solid line is the phase transition Ginzburg–Landau parameter given by κtri = 0.76±0.04 2 line from superconducting to normal state. The dashed line xc (y) is a line separating type I from type II superconductivity. The tricritical point separates a first-order phase transition (thick solid line) from a second-order phase transition (thin solid line), and also separates type I from type II superconductivity. The mean field value separating type I from type II superconductivity is given by x = 1/2. Note how it is possible to cross over from type I to type II behaviour in one and the same compound, for moderate values of κ, as the temperature is increased!.

ignore amplitude fluctuations in the order parameter ψ, a second-order phase transition always is obtained, either in the three-dimensional XY universality class (gauge-field fluctuations not included) or in the inverted three-dimensional XY universality class (gauge-field fluctuations included). Kleinert [135] then considered an attempt at combining gauge-field fluctuations and phase fluctuations with amplitude fluctuations by mimicking the amplitude fluctuations using a fluctuating temperature in the Ginzburg–Landau model. He then found that the superconductor–normal metal phase transition changes from first to second order as κ passes through the tricritical value given by Eq. 10.81. The next step was taken by Bartholomew who considered the Ginzburg–Landau model in Monte Carlo simulations, including all fluctuations in phase, amplitude, and gauge fields, finding a second √ order phase transition when κ is larger than some tricritical value κtri = 0.4/ 2 [44]. This value was improved on in Refs [45, 149] using very large scale Monte Carlo simulations in conjunction with sophisticated finite-size scaling techniques, finding a first order phase transi√ tion below κ = 0.76/ 2 and a second order phase transition above it. This is in rather remarkable agreement with Eq. 10.81.

314

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

All of the above may be put into a table showing various descriptions of the Ginzburg–Landau theory, including which fluctuations are taken into account at the superconductor–normal metal transition, and what the character of the resulting phase-transition is. This is shown in Table 10.2. In terms of the parameters used in Eq. 10.7, the phase diagram of the Ginzburg–Landau model is given in Figure 10.5.

PART III

Selected Applications

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

11 Small Scale Applications As a common introductory for the two chapters on applications we should motivate the contents as follows: Superconductor technology divides naturally into two main categories: small scale, usually electronic components or devices, and large scale where magnets and energy applications are of most importance. The applied part of this book intends to review some selected examples of superconductor applications. The entire spectrum of implemented and potential applications is so great today, that a comprehensive review is far beyond the scope of any physics text. However, there is a need to see the physics of superconductivity in the context of applications which is a major driving force in research on superconductors today. To this end, some examples of applications are given, and in important cases the underlying theory is worked out in some detail. A characteristic for superconductor-based technology is often that it is either superior to alternative methods, or only possible using superconductors. It should be emphasized that the potential for future applications other than those discussed in Chapters 11 and 12, or for improvements of existing ones, is enormous. Usually the question whether a demonstrated new superconductor technology is finally brought to the market is one of economy. This is always the case when alternative technologies are available, for instance in electric energy transport and storage, and in magnet technology. Long-term reliability and safety is another important consideration. The situation is somewhat different in areas where superconductor technology is unique, i.e. when no real comparable alternative exists. This is clearly the case with regard to some of the technologies based the Josephson junction. Although only a few examples have been chosen here, they suffice to demonstrate existing and future superconductor technology on scales ranging from micrometres in the Josephson junction to tens of kilometres in electric energy transport and maglev passenger movement.

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

318

SMALL SCALE APPLICATIONS

11.1

More JJ-junction and SQUID basics

11.1.1

Introductory remarks

In the present chapter we will discuss some further basic properties and how these are important for applications of superconductivity on a small scale, as well as giving outstanding examples of present day use.1 The most important small scale electronic device applications so far are based on Josephson junctions, a topic we already encountered in Chapter 5. Among these, the squid has reached by far the widest range of useful implementations due to its unique property as the most sensitive and versatile device for detection and measurement of magnetic flux. The SQUID has been under continuous development and improvements during several decades. It owes its sensitivity to the properties of the superconducting wavefunction phase which provides the basis for both flux quantization and Josephson tunnelling. The broad versatility is due to the possibility it offers for high resolution measurements of any physical quantity which can be converted into magnetic flux. This is the case with quantities like magnetic field, magnetic susceptibility, magnetic field gradient, electric current, voltage, and displacement. Therefore, a wide range of uses are open to the use of SQUID technology. A better understanding of the SQUID can only be reached through a good understanding of the Josephson effect. We therefore proceed to discuss the Josephson junction further, and then again turn to the SQUID and other applications.

11.1.2

RSJ – the resistively shunted Josephson junction

We showed in Chapter 5 that the current trough an unbiased Josephson junction can be expressed as I = I0 sin γ ,

(11.1)

where I0 is the maximum supercurrent the junction can sustain, usually referred to as the critical current, and γ = φ1 − φ2 is the difference in superconducting phase across the junction. We also discovered that while the current I could be expected to flow at zero voltage, another new phenomenon would appear when the current was forced to exceed I0 : A voltage V developed across the junction, and the phase γ became time dependent, giving an AC current with so-called Josephson frequency ωJ according to ωJ = ∂γ /∂t = (2e/)V = 2π V /0 . The current across the junction should now be written I = I0 sin[γ0 − (2eV /)t]

(11.2)

1 Suggested additional reading: S¨ app¨a H, Ryh¨anen T, Ilmoniemi R and Knuutila J, in Fossheim K., (ed) Superconducting Technology. 10 case studies, World Scientific Publishing, 1991.

MORE JJ-JUNCTION AND SQUID BASICS

319

where γ0 in the phase across the junction without the voltage V present. In junctions of high structural perfection the I –V characteristic is often found to be hysteretic as shown in graphs (b) and (c) of Figure 11.1. We will return to the details of this figure later on. For a junction to be practical in a squid it cannot be allowed to have such characteristics. Experience and theoretical analysis have taught us that the problem can be solved by shunting the junction, i.e. by adding an external resistance in parallel. This modification is commonly referred to as the RSJ-model (resistively shunted junction), as shown in Figure 11.2. One identifies from left to right: The current source, the resistive shunt R, the Josephson junction, the self-capacitance C bound to be present in the layered SIS junction structure, and finally the voltage V . We take the current source to be in a current controlled mode. This forces the phase γ in the equation I = I0 sin γ to adjust itself accordingly. The current now determines the phase difference across the junction, and not vice versa. We might further take into account the possibility that there is a fluctuating noise current In (t) associated with the components of the circuit, as is commonly true. The equation of motion for the circuit is then C

dV V + I0 sin γ + = I + In (t) dt R

(11.3)

Current i

1.5

1.0

0.5

0

0

0.5

bc = 3.0 Γ=0 Γ = 0.05

bc = 1.6

bc = 0.7

1.0

0

0.5

(a)

1.0

0

0.5

1.0 (c)

(b) Voltage v

Figure 11.1 Numerically calculated current-voltage characteristics of Josephson junctions with βc = 0.7, 1.6 and 3.0 at zero temperature, i.e. = 0 (solid lines), and with = 0.05 (dashed lines). (For reference, see the footnote at the foot of the opposite page). Parameters βc and are defined below.

I

I

R

I0

C

V

Figure 11.2 The RSJ model for a Josephson junction.

320

SMALL SCALE APPLICATIONS

an equation first studied by Stewart [157] and McCumber [158]. We choose first to analyze the differential equation (Eq. 11.3) under the assumption that In (t) can be neglected. We use the previously found relationship ∂γ /∂t = (2e/)V and write Eq. 11.1 as C γ¨ + γ˙ = I − I0 sin γ . 2e 2eR

(11.4)

Upon defining the quantity 0 (I γ + I0 cos γ ) 2π

(11.5)

C 2e ∂U γ¨ + γ˙ = − 2e 2eR ∂γ

(11.6)

U =− Eq. 11.4 may be written as

This is recognized as the equation of motion for a mass point moving down a corrugated surface, often referred to as a ‘washboard potential’, where U is a function of γ . Two characteristic situations are illustrated in Figure 11.3, I < I0 , and I > I0 respectively. In the first case the point mass gets trapped in one of the potential minima, and oscillates locally there. In the other case it goes on sliding. The first of these situations corresponds to zero time average phase difference, i.e. γ˙ = 0. This corresponds to the average voltage across the junction being zero. The second type of motion arises when the tilt is increased to make I > I0 . In this case the time average is γ˙ > 0, in other words, the point mass keeps sliding down the washboard. It is helpful also to note that in the mechanical analogue the capacitance C represents the particle mass, and 1/R is proportional to the friction coefficient, or damping of the motion.

U(g)

I > I0

I < I0

g

Figure 11.3 The washboard potential with a sliding point mass. Here I represents the tilt of the washboard as can be seen from Eq. 11.5.

MORE JJ-JUNCTION AND SQUID BASICS

321

Numerical analysis of Eqs 11.3–11.6 shows that hysteresis is controlled by the parameter βc , called the Stewart–McCumber parameter βc =

2π I0 R 2 C 0

(11.7)

Hysteresis is found for βc > 1. Calculations of current versus voltage is shown in Figure 11.1 for different values of βc . Distinct hysteresis appears for βc > 1. Further properties of Figure 11.1 will be discussed later. It requires highly qualified laboratory expertise to create junctions which meet the particular requirement βc < 1 for hysteresis-free junctions. Until now we neglected the current noise In (t). For a better understanding of the Josephson contact and SQUID physics the In (t) term should be reintroduced, and its consequences analysed. The full equation of motion is now: C γ¨ + γ˙ + I0 sin γ = I + In (t) 2e 2eR

(11.8)

The effects of noise are usually discussed in terms of noise spectral density SI (f ) of In (t). The meaning of SI (f ) is ‘noise power per bandwidth due to current noise In (t)’. Theoretical analysis shows that the noise spectral density of In (t) is given by the Nyquist result: SI (f ) = 4kB T /R

(11.9)

Since the current I represents the tilt of the washboard potential, the physical effect of In (t) is to cause fluctuations in that tilt. If these fluctuations become large enough they will cause the particle to escape from is local trapping site. This creates a condition for γ˙ to differ from zero, which again means that a voltage will appear, in this case corresponding to the appearance of voltage noise with increasing temperature. This will cause a rounding of the I –V curve before the steeper onset of current driven by the external voltage V . The noise corresponds to an additional voltage dVn and a total effective voltage V + dVn , causing the precursor “noise- rounding” effect in the I –V characteristic observed in the calculations of Figure 11.1. This current noise has an additional effect of lowering the effective critical current value, a potentially harmful consequence of noise since the critical current I0 must be above a certain value for proper operation of the junction. A criterion for I0 to be large enough to maintain a coherent supercurrent or ‘coupling of the junction’ is that the coupling energy exceeds the available thermal energy, expressed by the relation I0 0 /2π kT

(11.10)

322

SMALL SCALE APPLICATIONS

The quantity I0 0 /2π is what we referred to as the coupling energy of the junction. It is a measure of the energy associated with the current pattern for each flux quantum in the junction. A typical value of I0 is in the µA range at low temperatures, a small but easily measured current.

11.1.3

Further modelling of the Josephson junction

Having discussed the Josephson junction in rather simple terms above, let us examine it a little further. Before we rewrite the equation of motion, we remark first on the presence of the resistance R. Going back to the Josephson result for the current, we should, to be accurate, add a term coming from quasiparticle current in the presence of a voltage. The total current is now: I = I0 sin γ + V /Rq

(11.11)

Rq is a voltage dependent quasiparticle resistance. The term I0 sin γ still determines the main properties of the junction. Next, we rewrite the equation of motion by defining new, normalized variables: t ∗ = (2π I0 R/0 )t;

in (t ∗ ) = In (t)/I0

(11.12)

We assume further that the total resistance R, which is formed by Rq in parallel with the shunt resistance, satisfies the condition R Rq . For such cases the equation of motion (Eq. 11.8) describes the junction accurately. The thermal noise current In is the current in the resistance R. Its autocorrelation function is In (t + τ )In (t) = 2kT δ(τ )/R, where δ(τ ) is the Dirac delta function. With a little effort one finds the following reduced form of the equation of motion: βc

dγ d d2γ + ∗ = − (−iγ − cos γ ) + in (t ∗ ) ∗2 dt dγ dt

(11.13)

The current in (t ∗ ) = In /I0 is expressed as a Langevin function describing the thermal noise, and according to standard treatment obeys the relation in (t ∗ + τ ∗ )in (t ∗ ) = 2δ(τ ∗ )

(11.14)

where = 2π kT /I0 0 is the normalized thermal energy. The parameter βc is now analogous to mass, and inversely proportional to the damping of the system. Numerical analysis of Eq. 11.13 yields further insight into the current–voltage characteristics, as seen in Figure 11.1. What was computed there were the quantities i = I /I0 , and corresponding values of v¯ = v = V¯ /RI0 , resulting in the function v(i). ¯ V¯ is the time averaged voltage over the current-biased SQUID.

MORE JJ-JUNCTION AND SQUID BASICS

323

The graphs demonstrate the dependence of the I –V characteristics, here expressed as i versus v, ¯ on the two parameters and βc . First, we observe that embodies the rounding effect at finite temperatures mentioned above. It is therefore referred to as the noise rounding parameter, and the phenomenon itself as noise rounding. Second, as pointed out before, at βc ≤ 1 the characteristics is hysteresis free when = 0, but at higher values of βc there is distinct hysteresis even when = 0. This result defines one of the main technical challenges in applications of the Josephson effect: To control the parameter βc and thereby the characteristics of the junction. The use of Josephson contacts in the SQUID, requires that hysteresis is absent, as mentioned. This provides the important design criterion 2π I0 R 2 C/0 < 1. Fortunately, this nontrivial requirement on the I0 R 2 C product can be met in practice.

11.1.4

The autonomous DC SQUID

Next, we proceed to describe the structure, properties, and operational principles of the double junction DC SQUID, consisting of a superconducting loop interrupted by two identical junctions, both resistively shunted to avoid hysteresis. In the absence of hysteresis the state of the junctions and the DC SQUID are unambiguously determined by the applied voltage. Furthermore, since the flow patterns of supercurrent are characteristically different when the ring encloses an integral number n of flux quanta as opposed to (n + 12 ) quanta, the corresponding two I –V characteristics are also distinctly different. This fact provides the basis for practical use of the DC SQUID. We will now analyse the double-junction DC SQUID by extending the RSJ model to this case. This procedure neglects some technical aspects. But the DC SQUID is in reality such a complex device that one should make some initial simplifications to gain insight into the basic properties. Next, further aspects can be discussed on that basis. For instance, when it comes to practical implementation one cannot avoid considering the coupling of the SQUID to the external world in order to fully understand and control the properties. But it is not a good idea to include all such problems in the first basic analysis. Hence we start the analysis by using the RSJ model equation for both junctions simultaneously. First we note that in each junction, hereafter numbered i = 1, 2, the current Ii is Ii =

d2 γi dγi C + I0 sin γi + In,i + 2e dt 2 2eR dt

(11.15)

This provides us with two equations. First we observe that the total current through the DC SQUID is I = I1 + I2 , and next that the total magnetic flux

324

SMALL SCALE APPLICATIONS

threading the ring is =

0 (γ1 − γ2 ) = a + L(I1 − I2 )/2 2π

(11.16)

In other words, the flux in the ring it is the sum of the applied flux and the flux generated by the (difference of) currents I1 and I2 . a is as before, the external applied flux. The quantities C, R and I0 take on the same meaning as discussed in the RSJ model discussed before. L is the inductance of the ring, and In,i is the thermal noise current in the shunt resistance Ri . The junctions are characterized by the phase differences γi . For further analysis we combine the equations of motion for the two junctions by once adding them, and once subtracting one from the other. This allows us to study the behaviour of the quantities γ1 + γ2 and γ1 − γ2 , which turns out to be a useful procedure. To this end we define the quantities ν = (γ1 + γ2 )/2; φ = (γ1 − γ2 )/2

(11.17)

The instantaneous voltage across the two junctions is now V = RI0 dν/dt ∗ , using the previously defined rescaled, dimensionless time variable t ∗ = 2π RI0 t/ 0 , and the total flux is = 0 φ/π . Using the previously defined parameter βc , and introducing a new parameter βL = 2π LI0 /0

(11.18)

we combine the equations as described, to obtain two new equations of motion. Looking at the case where we add the equations for junction 1 and junction 2 we find d2 d C 2 (γ1 + γ2 ) + (γ1 + γ2 ) 2e dt 2eR dt + I0 (sin γ1 + sin γ2 ) + In,1 + In,2 .

I = I1 + I2 =

Upon introducing ν = (γ1 + γ2 )/2 and φ = (γ1 − γ2 )/2 we find d2 ν dν γ1 + γ2 I= C 2 + + 2I0 sin e dt eR dt 2 γ1 − γ2 × cos + In,1 + In,2 2 I d2 ν dν ≡i = C 2 + + sin ν cos φ + in,ν 2I0 2eI0 dt 2eRI0 dt

(11.19)

(11.20) (11.21)

with in,ν = (In,1 + In,2 )/2I0 . By rescaling the time variable and introducing t ∗ as explained we finally obtain βc

dν d2 ν + ∗ + sin ν cos φ = i + in,ν (t ∗ ) ∗2 dt dt

(11.22)

MORE JJ-JUNCTION AND SQUID BASICS

325

(The change of sign for in,ν (t ∗ ) is unimportant since this is a quantity which fluctuates around zero.) Proceeding in a similar manner when taking the difference I1 − I2 we find βc

dφ 2 d2 φ + ∗ + cos ν sin φ + (φ − φa ) = in,φ (t ∗ ) ∗2 dt βL dt

(11.23)

where we introduced the quantity φa = π(/0 ). The Langevin functions for in,ν , and in,φ represent uncorrelated thermal noise sources, and each of them are characterized by the correlation property in,ν (t ∗ + τ )in,ν (t ∗ ) = in,φ (t ∗ + τ )in,φ (t ∗ ) = δ(τ ). is again the noise rounding parameter defined previously. The equations developed here describe what is called the ‘autonomous DC SQUID’, i.e. one that is operating in a magnetic field with an external current I applied, but without other coupling to external devices, like a signal coil or control circuit, feedback circuit etc.

11.1.5

Simplified model of the DC SQUID

Numerical analysis of Eqs 11.22 and 11.23 has given much insight into the properties of the DC SQUID. For instance, under the assumption that the loop inductance L is very small, corresponding to βc 0, the equations can be expanded as a series, from which the voltage, the circulating current, and the transfer function ∂ V¯ /∂a can be estimated. Under the condition that L is negligible so that βL 1 and βc ≈ 0, the total flux in the ring is ≈ a . According to Eq. 11.22 the voltage can now be written as V ≈ RI0 (i − cos φa sin ν)

(11.24)

By integration of V over the period T of the Josephson oscillation, the average voltage across the current-biased DC SQUID is found [53], 1 V¯ = T

0

T

RI V dt ≈ 2

1−

2I0 π a cos I 0

2 12 (11.25)

In this limit the double junction DC SQUID behaves like a single Josephson junction with resistance R/2, and with an effective critical current Ic,eff = 2I0 cos(π a /0 ), in other words a flux-dependent critical current, with a modulation depth I0,eff = 2I0 when βL 1 and βL ≈ 0. This is seen by comparison with the I–V characteristics found for a single junction.

326

SMALL SCALE APPLICATIONS

The transfer function ∂ V¯ /∂a can be estimated on the basis of the above analysis by differentiation of Eq. 11.25 at a = 0 /2 and I = 2I0 which approximates the usual point of operation in a feedback circuit. To obtain realistic estimates one needs to relax the condition βL 1. RSJ model simulations indicate that at βL = π the modulation depth of critical current is approximately equal to I0 . This leads to the conclusion that ∂ V¯ /∂a ∝ I0,eff is reduced by approximately a factor of 2 for βL = π . The result is that the transfer function can be approximated as R ∂ V¯ ≈ ∂a 2L

(11.26)

√ Similarly, the dynamic resistance can be estimated as Rdyn = ∂ V¯ /∂I ≈ R/ 2 Operational properties The most important aspects of the DC SQUID with regard to operational properties are sketched in Figure 11.4. From left to right is shown the resistive shunting of each junction, and with a capacitance C associated with each, followed by a sketch of the two typical I –V characteristics, once with a flux a = n0 and once with a = (n + 12 )0 applied. This leads to a periodically varying voltage vs. applied flux, with a period 0 as shown in the right figure. These insights can be gained through numerical calculations, using the equations of motion discussed above. Looking through the mathematics of these equations, it is not easy to see from them why the I–V characteristics behave as shown in Figure 11.4. Clarke [159] has given a ‘simplistic’ analysis with a minimum amount of mathematics. We refer here to Figure 11.5, and also to Figure 11.4: we take the two junctions in the SQUID to be arranged symmetrically, one on each side of the loop, as is always done in a DC SQUID. The bias current I is then divided equally I

I

Φ

R I0

C

R V C

V Φ = n Φ0

IB

I0 Φ = (n + 1/2)Φ0 V

(a)

(b)

0

1 Φ/Φ0

2

(c)

Figure 11.4 (a) The DC SQUID; (b) I –V characteristics; (c) V vs. /0 at constant bias current IB . After Clarke [159].

327

MORE JJ-JUNCTION AND SQUID BASICS I

J I 2

Φ0 2L

−J

Φ0 /L

J I 2

+J

V

Im 1

2

Φ/Φ0 (a)

(b)

0

1 Φ/Φ0

2

(c)

Figure 11.5 Simplistic view of the DC SQUID: (a) a magnetic flux generates a circulating current J that is periodic in as shown in (b); as a result (c), the maximum supercurrent Im is also periodic in . After Clarke [159].

between the two paths, with I /2 in each. As long as the current in a junction is below the critical current I0 , a supercurrent tunnels through the junction at zero potential difference. If we allow an arbitrary amount of flux a to be applied to the ring, an additional supercurrent Icirc is set up, creating a self-generated flux LIcirc in the ring. Recalling that the total flux in a superconducting ring or loop is quantized as n0 , the following relation now applies: = a + LIcirc = n0

(11.27)

Taking the starting values of the applied flux as a = 0 or a = n0 , the circulating current according to Eq. 11.27 is initially zero. On increasing the applied flux, a finite circulating current JI circ = (a − n0 )/L develops in order to keep the total flux through the loop at its starting, quantized value. This internally generated, circulating current adds to the externally applied bias current I /2 in junction 1, and subtracts in the other, junction 2. The individual junction currents are related as I1 = I2 + 2Icirc and I2 = I1 − 2Icirc . Since the circulating current flows in opposite sense relative to the bias current in the two junctions, the junctions will respond differently to the same amount of externally applied flux. Junction 1 switches to the voltage state, i.e. a voltage develops across it, when it carries a total current equal to the critical current (see Figure 11.1). This happens when I1 = I /2 + Icirc = I0 . At this point the device current is I = 2I0 − 2Icirc . This is to be regarded as the device critical current at this applied flux. The maximum value clearly is 2I0 . What is important for use of the device is how it further responds to applied flux: At the same time as a increases from zero to 0 /2, Icirc increases from zero to 0 /2L according to Eq. 11.27, and the device critical current diminishes to 2I0 − 0 /L. We see from this that the critical current of the device as a whole has decreased by the amount 0 /L. Next, as we increase the applied flux beyond 0 /2 the SQUID makes a transition from the flux state n = 0 to n = 1, with reversal of the sign of Icirc . As a is increased to 0 , the critical current again increases

328

SMALL SCALE APPLICATIONS

to its maximum value 2I0 . The sequence discussed is depicted in Figure 11.5. It repeats periodically with increasing flux, and thereby results in the behavior of the DC SQUID illustrated in Figure 11.4. As Figure 11.4 also indicates, a practical device is biased at a constant current IB . This bias is above the critical current and therefore puts the entire DC SQUID in the voltage state, which is what we need in order to make it a flux to voltage transformer. It is the resulting voltage response to applied flux, shown in the right figure, which is so extensively exploited in practical applications of the device. An important question is how this device which is so sensitive, can be used both in low and high magnetic fields. The answer is that a combination of several factors make this possible: The sensitivity of the the transfer function ∂ V¯ /∂ at the bias current IB , combined with compensating feedback circuitry, as well as the use of a flux transformer that amplifies the flux detected at the observation point and transfers it to the SQUID, usually located some distance away. The DC SQUID is typically operated in socalled flux-locked loop. A simplified example is shown in Figure 11.6. The operating point of the SQUID is chosen at the steepest point on one of the periodic oscillations of the V –curve seen in Figure 11.4. In this design the SQUID is coupled to an external compensation inductor controlled by feedback from the SQUID output, thus causing the flux felt by the SQUID to be constant during operation even in a strongly varying external field. The feedback circuit also produces a voltage proportional to the flux that the circuit compensates. When calibrated, this voltage then measures the field detected by the device. In many uses of the SQUID other types of detector coils are used, such as first-order or second-order gradiometers. Gradiometers are used to eliminate spatially homogeneous external noise superimposed on the signal, like electromagnetic noise in the environment. A simplified but realistic and detailed sketch of a DC SQUID with signal coil attached is shown in Figure 11.7. The development of the SQUID has been a long battle against noise of many kinds. Noise may be environmental type, it may come from the components of the SQUID itself, and from the detecting circuitry and amplifier. Since the SQUID is a non-linear device, thermal noise has a dramatic effect on the dynamics. Figure 11.1 already gave some IB

Amplifier

Lock-in detector

Integrator

SQUID V 100 kHz oscillator

Figure 11.6

Modulation and feedback circuit for the DC SQUID. After Clarke [159].

SQUID APPLICATIONS Current nodes

329

I DC SQUID

Signal coil

High frequencies Low frequencies Parasite capacitance Base electrode I

Josephson junctions Counter electrode

Figure 11.7 Simplified structure of a planar DC SQUID together with a signal coil. The sites for the current nodes of the microstrip resonance and for the effective capacitance coupling are indicated. The directions of the current in the different signal-coil turns at frequencies lower and higher than the microstrip line resonance frequency are shown. After S¨app¨a et al. [160].

information on the influence of noise through the parameter as an example. According to careful studies [160] the autonomous DC SQUID discussed above √ has an optimal energy resolution ≈ 12kB T LC at βc ≈ 0.7. This expression can be interpreted as the ratio of thermal energy 12 kB T divided by the so-called effective noise bandwidth of the SQUID, 14 R/L. We conclude that a low-noise DC SQUID should have small junction capacitance, small loop inductance, and proper damping of the junctions. Examples of typical values are: C = 1 pF and L = 20–40 pH. In Figure 11.7 it is seen that the design attempts to meet these requirements. Obviously, the junction capacitance is made very small. DC SQUIDS may be shunted in several ways. We have only discussed one of these, the resistively shunted DC SQUID. In addition both capacitive and inductive shunting are possible, and have been well characterized.

11.2 SQUID applications 11.2.1

Biomagnetism: neuromagnetic applications

Introductory remarks2 Magnetic fields produced by living organisms has become one of the most wide-spread applications of the SQUID. Especially important is magnetoencephalography (MEG) which is a method for studying brain functions by mapping of the magnetic field produced by neural currents in the human brain. 2 Suggested additional reading: Ahonen A.I, et al., in Fossheim, K. ed. Superconducting Technology. 10 case studies, World Scientific Publishing, 1991 [161].

330

SMALL SCALE APPLICATIONS Action potential

Postsynaptic potential

Propagation

Synapse

Figure 11.8 Schematic illustration of an action potential, essentially consisting of two nearby opposite current dipoles propagating towards a synapse and the resulting postsynaptic potential corresponding to a single stationary current dipole. After Ahonen et al. [161].

Such magnetism is referred to as neuromagnetism. The function of the brain involves activity on the millisecond timescale. For such study there are two main windows: Electroencephalography (EEG) and magnetoencephalography (MEG). In EEG the potential distribution over the head is measured by electrodes attached to the scalp. In MEG the weak electromagnetic fields of typical amplitude 50–500 fT generated by the human brain are measured in order to locate the current sources generating the magnetic fields associated with cortical activity. Magnetoencephalography is a noninvasive tool for such study, offering spatial resolution on the millimetre scale and time resolution on the millisecond scale. A particular advantage of the MEG is its ability to locate cortical activity at deeper levels and spatially more accurately than EEG. The EEG is strongly influenced by currents in the scalp, which the MEG is not. Hence MEG offers superior quality with regard to locating accuracy. There are two types of signals from the brain: spontaneous activity, and evoked response to external stimuli. The principle of neuromagnetism The basis for MEG lies in concepts of action potential and postsynaptic potential. Information is carried from one neuron to another by the action potential via the synapse, mediated by the release of transmitter molecules which increase the permeability of the postsynaptic membrane as illustrated in Figure 11.8. Due to an interaction between chemical and electrical gradients there is a net current flow through the membrane and a change in voltage, called the postsynaptic potential (PSP). To a first approximation PSP is an intracellular current dipole oriented along the neuron, while the action potential may be described as a current quadrupole. In order for a resulting magnetic field to be detectable outside the head, a large

SQUID APPLICATIONS

331

number of neurons need to be activated, and to act in unison. The strength of a PSP current dipole is only 10−14 A. The observed magnetic field is believed to be mostly due to PSP cells which are perpendicular to the cortex. The field due to the action potential is very short range due to its quadrupolar nature. In addition, the dipolar PSP lasts an order of magnitude longer. The observed equivalent dipole is of the order of 10−8 A, which means that tens of thousands of neurons are activated at the same time. Dipoles which are observed in spontaneous activity, like in elliptic foci, may be an order of magnitude larger still. In order to calculate the field outside the head, resulting from cortical activity, some model assumptions have to be made. The head is often described as spherical symmetric, filled by a conductive medium with conductivity σ (r). The magnetic field outside such a body has important simplifying properties: (1) radial dipoles and their volume currents cancel each other and thus do not generate a magnetic field outside the body, (2) the radial component of magnetic field is produced by the primary current density only, and (3) both radial and tangential field components are independent of the conductivity profile. During measurement, the evoked response signal is usually assumed to be composed of the true source signal plus gaussian noise. By repeated sampling, say N = 100 times, the signal part is integrated up proportional to√N , the total number of samples, while the noise integrates up proportional to N . Thus an acceptable signal to noise ratio can be achieved. Instrumentation The SQUID is the only instrument with sufficient sensitivity to perform neuromagnetic studies. Usually, the external field is coupled into the SQUID by a a superconducting flux transformer, i.e. a pickup loop coil and a signal coil in series, shown in principle in Figure 11.9. Normally the signal is orders of magnitude smaller than the environmental noise. Therefore, the transformer usually has a gradiometer coil on the detecting side, sensitive only to the derivative of the magnetic field, ∂Bz /∂z, and insensitive to environmental noise with electromagnetic wavelength much longer than the size of the coil. An illustration of such a coil is shown in Figure 11.10. It consist of two identical coils in series, but oppositely wound. The first part may be regarded as the signal detector, and the second part as a compensator coil. In a case when spatially homogeneous noise is detected by the first coil, it is compensated by the second one, and the resulting signal picked up by the gradiometer is zero. If on the other hand an inhomogeneous field is present, the gradiometer coil detects a signal proportional to the spatial derivative along the coil axis. Depending on the design one may choose to make gradiometers that measure tangential derivatives ∂Bz /∂x and ∂Bz /∂y. Usually the whole device is placed in a magnetically shielded room. However, more and more sophisticated designs have made it possible to operate the

332

SMALL SCALE APPLICATIONS Pickup coil

Signal coil

→ Bext

→ Bcoupled

SQUID

Figure 11.9 Transformer. After Ahonen et al. [161]. Li Mi

L

Js Flux-locked SQUID

Li Mi

L

z Js Flux-locked SQUID y x

Li Mi

L

Js Flux-locked SQUID

Figure 11.10 Examples of gradiometers coupled to flux-locked SQUID. After Clarke [159].

SQUID in unshielded environment. For a more widespread use of SQUIDs in diagnostics, it is essential to avoid the use of shielded rooms for the sake of cost reduction. A potentially interesting area for the future is in cardiology. The capability to obtain high quality signals from the heart cycle is well established even using high-Tc superconductor SQUIDs. However, sensitivity to the positioning of the device is one of the problems with this method. During the 1990s a new development took place. Multichannel SQUID systems, containing well over 100 SQUIDs were built to be placed over the head, and

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

333

Figure 11.11 Multichannel SQUID system for neuromagnetic studies of the brain. With permission from Neuromag.

allowing a very detailed recording of brain activity in the entire brain. These systems are commercially available, and becoming increasingly important as a tool for brain diagnostics, and as a research tool for the study of brain function more generally. Figure 11.11 shows an example of multichannel squid system for neuromagnetic studies of the brain. Determining the precise location of epileptic foci before surgical treatment is an established clinical application of such systems.3

11.3 Superconducting electrodynamics in the two-fluid model 11.3.1

Frequency dependent conductivity in the two fluid model

Electrical current in the Meissner phase is confined to the penetration depth λ. This obviously is the DC limit of response to an electromagnetic field. Therefore, any theory for the low frequency response must have Meissner screening 3 Recommended further reading: See two review articles by Clarke J. (1) In Weinstock, H. ed. SQUID Sensors: Fundamentals, Fabrication and Applications. NATO ASI Series. Kluwer Academic Publishers, Dordrecht, The Netherlands 1996, and (2) In Weinstock, H. ed. Applications of Superconductivity. NATO ASI Series. Kluwer Academic Publishers, Dordrecht, The Netherlands 2000. These reference treat the rf SQUID.

334

SMALL SCALE APPLICATIONS

as its limiting low frequency behaviour. We will now treat electrodynamics in the situation where a superconductor surface is exposed to an AC electromagnetic field. Relevant cases may be electromagnetic radiation incident on the superconductor surface, for instance at normal incidence, or an electromagnetic wave traveling along the superconductor surface. This latter case will correspond to the situation in the technologically very important planar wave-guides and filters used in high frequency communications. We treat a superconducting half-space first as the basic entity. In the course of this treatment penetration depths for electromagnetic field in both normal and superconducting materials will be introduced. Furthermore, we need a model description of the superconducting electron gas. It turns out that the so-called two-fluid model is adequate for this purpose over a wide frequency range. The two-fluid model was historically introduced by Gorter and Casimir in 1934 [67]. It proposes to divide the mobile charges in the superconducting state of a metal into two distinct entities: A normal component of concentration nn with properties like those of the electron in the normal state, and a superfluid component of concentration ns whose properties are responsible for the observed screening of a static magnetic field in the Meissner phase. The total concentration of mobile charge is then (11.28) n = nn + ns where both nn and ns have to be temperature dependent in order to account for the temperature dependence of the penetration depth λ. Corresponding to this division one also foresees that currents are composed of two parts, a normal part Jn associated with nn , and a superconducting part, Js , associated with ns . For the total current then J = Jn + Js

(11.29)

Experimentally one finds in low-Tc superconductors that the London penetration depth λL obeys the following simple relation for its temperature dependence − 1 2 λL (T ) = λL (0) 1 − (T /Tc )4

(11.30)

This can be interpreted as a consequence of a density of normal component nn /n = (T /Tc )4 , and a corresponding density of superfluid component ns /n = 1 − (T /Tc )4

(11.31)

1 Since λL = ms /µ0 ns (T )qs2 2 , substituting ns from Eq. 11.31 reproduces Eq. 11.30. We define λL (0), the London penetration depth at 0 K, as 1

λL (0) = (ms /µ0 ns (0)qs2 ) 2

(11.32)

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

335

How does this relate to conductivity? Using Newton’s second equation for the case of zero friction we have ms

dv = qs E dt

(11.33)

The current density Js may be expressed as J s = ns qs v

(11.34)

Hence we can rewrite Eq. 11.33 as

dJ s −E =0 dt

(11.35)

which is the first London equation where = ms /ns qs 2 . In case of a sinusoidal field of frequency ω we expect a resulting sinusoidal current. After performing the derivation in Eq. 11.35 we obtain Js =

1 E = σs E iω

(11.36)

where we have defined a conductivity σs : σs =

1 1 = iω iµ0 ωλ2L

(11.37)

Since σs is expressed for a condition of zero loss (without a damping term in Newton’s equation of motion) it is a purely imaginary quantity. Also, if we assume low frequency, as when ωτ 1, we can take the usual DC expression for the normal state conductivity to apply for the normal component of the electron gas, with the normal current being in phase with the driving field: Jn = σn E = and the total current

J = Jn + Js =

nn qn2 τ E mn

nn qn2 τ 1 −i mn µ0 ωλ2L

(11.38) E

(11.39)

The conductivity is now a complex expression: σ = σ1 − iσ2 =

nn qn2 τ 1 −i mn µ0 ωλ2L

(11.40)

The response to an AC field in a superconductor clearly is out of phase with the applied E-field.

336

SMALL SCALE APPLICATIONS

11.3.2

Surface impedance and AC loss

Because of the altered screening effects resulting from the foregoing analysis there is a need to apply a different concept, adequate for this situation, in addition to Meissner screening. This is the concept of a (complex) surface impedance Z, measured in units of , defined by Z=

E|| J dz

(11.41)

where E|| is the electric field in the surface, driving the current J along the surface, and integration is from the surface (z = 0) to (in principle) infinity inside the conductor. Using Maxwell’s equation one derives for a normal metal, as we will show later, Zn = Rn + iXn 1 Rn = Xn = (µ0 ω/2σn ) 2

(11.42)

Consequently, the resistive and reactive parts of the surface impedance in a normal conductor are equal, and, since σ is frequency independent in the range we are considering, both go like ω1/2 . These results have been well verified experimentally. In the superconducting state matters are different due to the difference in AC conductivity discussed in the previous section. Since we already used London’s first equation to establish an expression for σ in the superconducting state, and in addition invoked the two-fluid model, superconductivity is built into the σs we derived above. We therefore now only need to use Maxwell’s equations, and the surface impedance takes the same form both in the superconducting and normal states when expressed in terms of σs . We have for the superconductor: Zs = Rs + iXs = We will show later that

iµ0 ω σs

1 Rs = µ20 ω2 λ2L σn 2 Xs = µ0 ωλL

1 2

(11.43)

(11.44) (11.45)

where we used the symbol σn for the conductivity of the superconductor in its normal state, corresponding to nn = n. We also note that the reactive part Xs of the surface impedance Zs is purely inductive. The usual expression for such impedance is X = ωL. In the present case therefore, we can conclude that Ls = µ0 λL , usually called the equivalent inductance, known also as the kinetic inductance. We now proceed to deduce the results briefly mentioned above, first

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

337

for the normal state. We want to find the intrinsic impedance Z. This quantity may be defined from Maxwell’s equations ∇ × H sn = Jns + iωεE sn

(11.46)

where the second term on the right-hand side is the displacement current due to bound charges, or

and by use of

∇ × H sn = (σn + iωε)E sn

(11.47)

∇ × E sn = −iωµ0 H sn

(11.48)

In all cases the superscript s here refers to ‘surface’ rather than ‘superconducting’ while subscript n refers to the normal state. Combining Eqs 11.47 and 11.48 by taking the curl of the second one and inserting the result in the first, and further s e−(α+iβ)z = E s e−γ z one finds writing Ens = En,o n,o γn2 = (σn + iωε) iωµ0

(11.49)

which can be written in the form

1 σn 12 γn = iω (µ0 ε) 2 1 − i ωε

(11.50)

In a good metal the displacement current density is very small compared to that caused by free charges. Numerically, therefore, one finds even for normal metals that σn /ωε 1. Hence, the general expression for γn can be approximated by

σ 1 1 1 n 2 γn = iω (µ0 ε) 2 −i = i (−iωµ0 σn ) 2 ωε 1

= (1 + i) (ωµ0 σn /2) 2 = (1 + i) /δn

(11.51)

where δn is the classical normal state skin depth, defined here as δn =

2 ωµ0 σn

1 2

(11.52)

We also note that under this approximation, since γn = αn + iβn is a complex quantity, we have for αn and βn αn = β n =

1 ωµ0 σn 2

1 2

=

1 δn

(11.53)

338

SMALL SCALE APPLICATIONS

These quantities are again closely related to the intrinsic impedance, a quantity we will deduce next. The complex surface impedance Z ≡ R + iX defined as indicated previously (Eq. 11.41), or alternatively by the relation Z≡

s e−γ z Ex,o s Hyz

(11.54)

here specifically referring to an electromagnetic AC field applied at normal incidence to the surface whose normal is along z. Using ∇ × E s = −iωµ0 H s one finds 1

Z=

(iωµ0 ) 2 1

(σ + iωε) 2

=

µ 1

1

ε

(1 − i (σ/ωε)) 2

0

2

1

=

µ ω1 2 0 (1 + i) 2σ

(11.55)

We can at this point easily distinguish between the normal and superconducting states. In the normal state the conductivity is a real quantity σn , and we find in this case for Zn = Rn + iXn , the corresponding terms in Zn =

ωµ0 2σn

1 2

+i

ωµ0 2σn

1 2

(11.56)

Next, introduce σ in the superconducting state as a complex quantity σs = σ1 − iσ2 as we did before. Inserting this, we have: Zs = Rs + iXs =

iωµ0 σ1 − iσ2

1 2

(11.57)

Since in the superconductor σ1 σ2 we can expand the root, and find, using the expressions for σ1 and σ2 from Eq. 11.40 Zs = Rs + iXs = 1 Rs = µ20 ω2 σn λ3L 2 Xs = µ0 ωλL

µ20 ω2 λ3L nn qn2 τ + iµ0 ωλL 2mn

(11.58) (11.59) (11.60)

We notice in particular that the surface resistance predicted by this model increases as the square of the frequency, compared to the square root dependence in the normal case. Observations confirm these predictions with good accuracy in, respectively, normal metals, and in high quality LTS superconductors. In HTS the frequency dependence is sometimes influenced by non-ideal structures. The agreement with predictions is therefore not as good in such cases. Examples of observations are given in Figure 11.12.

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

11.3.3

339

Surface resistance measurement

The most crucial information needed in order to evaluate the quality of superconducting surfaces or thin films for use in high frequency communication systems is the surface resistance Rs . This quantity will determine the loss properties, and this is the essential information to obtain. Several methods have been established for such purposes. As far as high-Tc materials are concerned, due to the anisotropic structure of these materials, measurements must be done on planar surfaces. This is contrary to well-established methods for low-Tc materials, which are often measured in cylindrical cavities including the walls. Since the planar sample can very well be used in both cases we describe briefly the so-called endwall replacement method. Figure 11.13 shows a sketch of a vertical cut through a cylindrical TE011 mode cavity with input and output signal attached as indicated. The short centre lead sticking into the cylinder are antennas for the excitation of the electromagnetic cavity, and for measurement of the response on the ‘out’ side. While the cylindrical walls and the bottom part are made of high quality copper, the top flange can be exchanged, placing here in one case a copper plate, and in the other case a high-Tc film deposited on some appropriate substrate. By sweeping across a certain frequency range around the resonance frequency f0 of the cavity, the detecting antenna will register a varying field response due 102

K Optical waveguide

Waveguide 77 K WR-15 u C eline Strip l cable a i x a Waveguide 9 Co RGWR-28

1

K

)

10−1

K

)

77

2 4.

Optical fiber (Silica)

3S

n

eY

(N b K 27 O eY

BC

10−5

in

10−4

BC

Sa w

O

(×

10−3

K

3. 7

×

(N

b

10 −

4. 2

)

5

10−2

St rip el

Attenuation (dB/cm)

u 300

line C

Stripe

10

Atmospheric propagation at sea level

St

rip

el in

10−6 10−7 0.1

1 10 Frequency (GHz)

100

Figure 11.12 Loss per meter as a function of frequency for various transmission media. (The surface acoustic wave propagation losses on LiNbO3 have been scaled to make a realistic comparison and represent dB/µs of delay for an equivalent electromagnetic wave in a media with εr = 10). After Lyons and Withers [162].

340

SMALL SCALE APPLICATIONS HTS sample TE011 cavity

In

Out

Absorber

Figure 11.13 Cross-section of a TE011 mode cylindrical cavity for measurements of surface resistance. After Shen [163].

to the finite width f of the resonance. This width is a measure of the quality of the cavity as a resonator, called its Q-value, defined by ω0 f0 2πf0 W ω0 W = ≡Q= = ω f P P

(11.61)

We can regard this as a measure of how much energy is dissipated per second (P ) relative to how much energy is put into the cavity per second. Here W is the stored energy, which, after multiplication by frequency essentially measures the rate of energy put into the cavity. Therefore, a measurement of the Q-value defined here is an appropriate way to characterize the quality of the cavity. These aspects are determined fully by the loss properties of the material. The next question is now how a measurement of the Q-value as described above gives access to the surface resistance Rs . First we have to replace the upper Cu flange by the superconductor. The change of Q will tell us how the materials differ. A relative measure of the surface resistance r of the superconductor compared to that of copper is often expressed as r=

Rs (Cu) k = Rs (SC) k + Q0 (Cu)/Q0 (SC) − 1

(11.62)

Here, k is a geometrical constant of the cavity. k=

1 2 + PSw (Cu)/Pew (Cu)

(11.63)

where PSw (Cu) is the power lost in the sidewall of the copper cavity while Pew (Cu) is the power lost in the end wall when the Cu end wall is in place. We did not prove these results. They are referred to here only to show that the analysis can be completed. The important relation is that expressed by r. Clearly, if all that is needed to determine the surface resistance of the superconductor, relative to that of copper, is a measurement of quality factors as explained, with the

HIGH-FREQUENCY RADIO TECHNOLOGY

341

10−1

Surface resistance (Ω)

10−2

10−3

10−4

10−5 0 10

1.2 cm substrate 5.1 cm substrate Rs a f 2 Cu 101 102 Frequency (GHz)

103

Figure 11.14 Relationship between surface resistance Rs at 77 K and frequency in a Tl2 Ba2 CaCu2 O8 film and in Cu. After Holstein et al. [164].

upper wall in place, once as a superconductor and once as a copper wall. Since copper is the standard by which metallic resistance is gauged, this does the job. What is found, is that although copper is a very good conductor, with low resistance, a superconductor is often 1000 or more times better, i.e. Rs is 103 to 104 times lower than that of copper at room temperature. This is a drawback for the method described, making it one of relatively low sensitivity. Other techniques have been devised to allow the superconductor to play a larger role in determining the total Q of the cavity. We refer to more specialized literature on this subject. Figure 11.14 shows results of measurement of surface resistance carried out on Tl2 Ba2 CaCu2 O8 film. We notice in particular that the square law for surface resistance discussed before is verified, even using different substrates. The validity of the result of the two-fluid theory is confirmed even in this high frequency range.

11.4 High-frequency radio technology 11.4.1

Microstrip filters and delay lines

Introduction Superconductors can have a dramatic impact on selected passive microwave device applications because of two properties that differ greatly from those of

342

SMALL SCALE APPLICATIONS

normal metals at high frequencies. First, much lower surface resistances is available using superconductors, a fact that transforms into much lower loss and much higher Q-values in superconducting microwave system components. Second, superconductors have a practically frequency independent penetration depth in the microwave frequency range. This has the important consequence that superconductors introduce no dispersion into a microwave device up 1 THz frequency in low-Tc superconductors, and well above this in high-Tc superconductors due to their larger gap frequency. The improvement over normal conducting performance is substantial. Superconductor passive devices may work quite well in cases where normal conductor devices would function very poorly or not at all. A normal metal component would, in many cases, have several orders of magnitude higher conductor loss than the superconducting ones. Important passive microwave device components are bandpass filters, which are becoming essential components in mobile phone base stations. Other uses are in chirp filters which can provide improved resolution in radar images, and delay lines used in various contexts. As we discussed previously in this chapter, the two-fluid model is adequate for an engineering representation of the physical properties of superconductors in the present context. Figure 11.15 shows how the surface impedance can be represented graphically in a circuit analysis. The surface resistance, which we previously found in Eq. 11.59, can be expressed as follows: 4 − 32 4 T 1 2 2 3 T Rs = µ0 ω λL (0)σn 1− 2 Tc Tc

(11.64)

where the temperature dependencies of nn /n and λL , respectively, have been inserted in the two parentheses. According to this expression the surface resistance goes to zero at T = 0. In reality this does not happen. Instead a limiting value is reached at low temperatures, independent of temperature but dependent on frequency. This effect is typically caused by small inclusions of normal phase. For niobium the residual resistance falls below 10−8 in the GHz range at about 1.2 K. High-Tc superconductors have a much shorter coherence length than low-Tc ones. The residual resistance is therefore a more serious problem Normal current path Surface impedance Ln

Rn Lsurf

Rsurf

Lsc Supercurrent path

Figure 11.15 Two-fluid model for the bulk impedance of superconductors and its equivalent surface impedance.

HIGH-FREQUENCY RADIO TECHNOLOGY

343

in high-Tc superconductors. We refer again to Figure 11.12 for examples of the improved surface resistance properties in superconductors compared to copper, in particular in high-Tc , in the 1–100 GHz range. For YBCO film the calculated curves are based on the two-fluid model. The potential improvement compared to Cu at 77 K is enormous. Although part of the improvement is lost when patterning is performed, compared to the unpatterened continuous film, a substantial advantage remains. Another important aspect is the loss per meter during signal transmission. Figure 11.12 leaves no doubt about the advantage of superconducting transmission media over surface acoustic wave signal transport, normal coaxial cable, and Cu stripline. This figure does not take into account dielectric losses, nor does it take into account transducer and conversion losses in the SAW device. Comparison to Nb and Nb3 Sn at 4.2 K is made. Implementation: filters and delay lines Figure 11.16 shows the design of a 4-pole so-called Chebyshev bandpass filter with 3% bandwidth, 0.05 dB passband ripple, and 4 GHz centre frequency. The filter was made by deposition of YBCO film on 425 µm thick LaAlO3 substrate. Data in Figure 11.17 shows a passband insertion loss of only 0.3 dB at 77 K and 0.1 dB at 13 K. Nb filters showed similarly 0.1 dB insertion loss at 4.2 K. Gold filters had an insertion loss of 2.8 dB at 77 K. The superconductor filters have far steeper skirts than gold filters, a very important feature to prevent cross-talk between channels, in particular when used as filters for mobile phone communication. Another important application of superconductor passive devices is in analogue signal processing where the high frequencies and wide bandwidths required place a premium on conductor loss. The tapped delay line architecture developed at Lincoln Laboratory is illustrated in Figure 11.18. A tapped delay line provides temporary storage and sampling of the input signal at intervals τi . The samples are multiplied by weights wi and coherently combined by spatial summation or time integration. Such delay lines are used to implement chirp 66 µm

165 µm

0.100”

Figure 11.16 Four-pole superconductive microstrip filter layout. The filters were fabricated on LaAlO3 substrates using gold, niobium and YBCO signal lines. After Lyons and Withers [162].

344

SMALL SCALE APPLICATIONS

Transmission (dB)

0

T = 77 K

−10 −20 −30 −40 −50

4.0

4.2 4.4 Frequency (GHz)

4.6

Figure 11.17 Measured transmission response at 77 K of a filter fabricated with a postannealed YBCO signal line and ground plane on a 425 µm thick LaAlO3 substrate. Passband insertion loss is 0.3 dB. After Lyons and Withers [162].

Input

t1

t2 w1

t3 w2

t4 w3

t5 w4

w5

Figure 11.18 Architecture of a transverse filter, where τi are time delays and wi are fixed or programmable tap weights. After Lyons and Withers [162].

Signal line conductor

Dielectric

Figure 11.19 Various transmission line geometries considered for the implementation of YBCO delay lines. After Lyons and Withers [162].

filters, matched filtering, correlation and Fourier transformation. The number of information cycles of the waveform gathered coherently in the filter determines the signal processing gain, i.e. the time-bandwidth product. Delay line transmission geometries are illustrated in Figure 11.19, in various combinations of signal line, dielectric and ground. Generally, the various structures perform very much in agreement with predictions.

HIGH-FREQUENCY RADIO TECHNOLOGY

11.4.2

345

Superconducting high-frequency devices

Introductory remarks Superconducting tunnel junctions are well suited for use in low-noise high frequency detectors. The noise level in the these quantum mechanical based detectors can be well below those of competing state-of-the-art detectors. The most demanding applications for mm- and sub-mm observations in radio astronomy already take advantage of these low-noise receivers. According to Dicke’s famous radiometer formula [165], the signal to noise ratio for a given bandwidth ( f ) and a given integration time ( t) is S Ts = f t N TR

(11.65)

where Ts is the equivalent blackbody temperature of the signal, and TR is the receiver noise temperature. From this formula we observe that for a given signal to noise ratio the integration time needed to observe a particular source is reduced by a factor of 4 if the receiver noise temperature is reduced by a factor of 2. Since the integration time sets the time scale of the telescope observation time, this transforms into far more efficient use of an expensive satellite telescope with moderate improvement of the detector. Superconducting device components are therefore of great interest. It turns out that the greatest advantage is obtained at several hundred GHz, i.e. in the mm and sub-mm wavelength regime, an interesting range for radio astronomy in space or on the ground. Phase sensitive heterodyne detectors normally use a mixer to down-convert a high frequency signal to an intermediate frequency (if) range where low noise semiconductor amplifiers are available. To perform the down-conversion a high frequency local oscillator (lo) is needed. For semiconductor mixers which need about 1 mW power above 200 GHz, these oscillators are rather heavy equipment. In contrast, a superconducting detector needs only low lo power. Furthermore, a large number of receivers can use the same lo. It is therefore possible to construct an array of detectors for radio astronomy used in satellite telescopes, that can scan the sky simultaneously in several directions. This gives another factor of 10 in efficiency. Lightweight low power lo solutions are also available for SIS mixers. For space use the ideal technology will be to build integrated all superconductor receivers, i.e. local oscillator, mixer and preamplifier on the same chip. The particular property of SIS junctions which makes them useful in the context outlined above, is their extremely sharp non-linear I –V characteristics. According to the physical properties we have discussed in Chapters 4 and 5, there are two distinct possibilities, either the quasiparticle tunnelling I –V characteristic near the gap Vg , or the Josephson effect pair tunneling characteristic at zero voltage, V = 0. Both may be used.

346

SMALL SCALE APPLICATIONS

Mixer principle It is the lack of broadband low-noise amplifiers for signals above ≈100 GHz that drives the need for superconductor technology in the mm to sub-mm range of radiowaves. When a local oscillator voltage is applied to a nonlinear element, in our case an SIS tunnel junction, a periodic variation of the small signal conductance dI /dV is produced, giving rise to a number of current components at the fundamental and harmonic frequencies of the lo. Combining the received signal voltage at frequency fs with the lo signal at flo the non-linear characteristic of the detector gives a product response at Fourier component frequencies fm = |mflo + fif | where fif = |fs − flo | is the so-called intermediate frequency signal, or if signal for short. This means that power is transferred to sum and difference frequencies of the two signals that are mixed in the SIS non-linear device. The situation is illustrated in Figure 11.20. From this new spectrum of frequencies the important signal is the one whose frequency has been downconverted to the range accessible to conventional low-noise amplifiers, the last stage before viewing the resulting telescope output. We will briefly outline a simplified mathematical description of the mixing process. The current through the nonlinear element can be written as a power expansion in the voltage V : I (V ) = a1 V + a2 V 2 + a3 V 3 + · · ·

(11.66)

The input signal consist of three parts: (1) the DC bias voltage V0 , which places the device at the correct operating point on the I –V curve, here the gap voltage Vg , (2) the lo-voltage vlo = Vlo cos (ωlo t), and (3) the weak signal we want to retrieve, vs = Vs cos (ωs t) where ω = 2πf . When these voltages are inserted into the expansion, Eq. 11.66, the resulting terms can be gathered according to their common coefficients ai . The sum of terms with the coefficient a1 is a scaled replica of the sum of all inputs. This is not what we are searching. Rather, the term we are interested in is found in the sum with the a2 coefficient: 2Vlo Vs cos ωlo t cos ωs t = Vlo Vs {cos(ωlo − ωs )t + cos(ωlo + ω)t}

2flo

Power

flo fif = |fs − flo|

0

fi

−1

(11.67)

fs

+1 Frequency

|3flo − fs|

−2

|flo + fs|

+2

Figure 11.20 Power spectrum for a mixer with the local oscillator (lo) and the signal frequencies applied. Note also the intermediate and image frequencies.

HIGH-FREQUENCY RADIO TECHNOLOGY

347

Here, the down-converted if voltage at fif = |fs − flo | is present, as well as a correspondingly up-converted one. By adjusting the local oscillator frequency ωlo various received signals can now all be converted to the same if frequency and amplified at the same frequency. The point is here that a single state-of-the art if amplifier optimized just for one frequency can handle a wide range of signal frequencies. A sweep of lo frequencies will give access to a range of received signal frequencies. The SIS junction has a pronounced microwave response, as illustrated in Figure 11.21, where the characteristics are shown both with and without lopower applied. At low-frequency radiation, the I –V curve is smeared at the gap singularity, the current increases at sub-gap voltages, and the DC Josephson current is depressed. Photon induced steps appear as the rf frequency is increased. These are of two kinds. Figure 11.21 (b) indicates photon-induced steps in the quasiparticle current at voltages 2 /e ± mhflo /e. They occur as photons are absorbed (or emitted) in the tunnelling process, thus allowing electrons to tunnel into the high density of states above the energy gap. The photon-induced structure increases in strength with microwave power until superconductivity is quenched. The other kind of steps (Figure 11.21(d)), is due to Josephson mixing products falling at zero intermediate frequency for bias voltages corresponding to multiples of the applied frequency (2eVk / h = fJ = kflo ). The amplitude of

(f) C RSJ

R SH 40 (e)

Current (µA)

Ic 20

h f lo e

(b)

(d)

(a)

0

2∆ e

−20 −40

(c) hf lo e

dVg

−4

−2

0

2

4

−2

0

2

4

Voltage (mV)

Figure 11.21 Typical I –V curves for SIS tunnel junctions. For a low critical current junction (or with an applied magnetic field) the left-hand curves show the I –V curve without (a) and with (b) lo applied (∼240 GHz). The right hand curves show how the Josephson effect changes the I –V curves without (c) and with (d) lo applied (∼240 GHz). Outlined in the figure is the I –V curve of a resistively shunted tunnel junction (RSJ), and the corresponding electrical circuit (e resp. f ). A Josephson mixer could also be biased at the open circle. After Winkler et al. [166].

348

SMALL SCALE APPLICATIONS

these Shapiro steps vary as Bessel functions, Jn (α1 ), with normalized microwave amplitude α1 = 2eVlo / hflo . Josephson junctions can be used in a number of applications, based on the effects that relate current and voltage via the phase difference across the junction. Some prominent examples are high frequency oscillators, voltage standards, parametric amplifiers, Josephson video detectors and mixers.4

4 Further

recommended reading may be found in the review by Winkler et al. [166].

12 Superconducting Wire and Cable Technology 12.1

Low-Tc wire and cable

12.1.1

Introductory remarks

Technical superconductors for energy and magnet applications1 consist of composite wires of superconducting and normal conducting material, both in high-Tc (HTS) or low-Tc (LTS) applications. To stabilize the superconducting state the superconductor is subdivided into a multi-filamentary structure embedded in low resistivity normal conducting matrix. As far as LTS applications is concerned, only the intermetallic stoichiometric compound Nb3 Sn and the alloy NbTi are important. In both of these the matrix consists of low resistance Cu matrix. Filament diameters range from a few µm to about 100 µm, and the filament number can be as high as 100 000. Wire diameters are between 0.1 mm and 2 mm, and the current capacity range is from a few ampere to 1000 A in fields up to 20 T in the liquid helium range at or below 4.2 K. The fabrication process includes bundling of components into a billet, with subsequent extrusion and drawing. Conductors for high current use are produced in the form of fully transposed cables. Depending on the design, additional stabilizer material of copper and aluminium, as well as strengthening members and cooling channels may be added. Wires of ceramic high-Tc cuprates are mostly manufactured by the powderin-tube method. Here the leading first generation technology is based on the development and use of BiSrCaCuO/Ag wires. These can tolerate magnetic 1 Based largely on the review by Krauth in Fossheim: Superconducting Technology. 10 case studies. [167] For further reading we recommend Buckel: Supraleitung [168], Wilson Superconducting magnets [169], R. P. Reed and Clark Materials at Low Temperature [170], Collings Applied Superconductivity, Metallurgy and Physics of Titanium Alloys [171] and Foner and Schwartz: Superconductor Material Science [172].

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

350

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

fields up to more than 20 T at 4.2 K. Even at 77 K the quality of these conductors is becoming interesting for some applications, as we will give examples of in the following. A second generation of superconductor tapes, manufactured by film deposition on a suitable substrate is emerging, and should be expected to take over the market.

12.1.2

General design considerations

The primary characteristics in the design and fabrication of technical superconductors may be broken down into three groups: 1. Superconductor properties

Critical temperature Tc Upper critical field Bc2 Critical current density Jc

2. Design of composite wire: Superconductor filaments in normal matrix

Stability against transition to normal state (quenching) AC losses Mechanical characteristics

3. Fabrication technology

Fabrication of multi-filamentary composites Fabrication of high current conductor cables with additional stabilization, mechanical reinforcement and cooling channels Compatibility of conductor properties with magnet fabrication technologies.

In the following we will discuss these three areas of wire and cable technology in turn, and give examples of results obtained.

12.1.3

Basic superconductor properties

The transition from normal-conducting to superconducting state is determined by three critical parameters, the critical temperature Tc , the upper critical field Bc2 , and the critical current density Jc . The first two are determined by the electronic properties, including the pairing mechanism for Cooper pair formation. In typical low-Tc materials of technical importance these parameters cannot be manipulated to any important extent. In high-Tc cuprate materials they can be manipulated first by choice of material composition, of which there are now a great number, and next by doping of the chosen material. However, in reality only optimally

LOW-Tc WIRE AND CABLE

351

Table 12.1 Development of the highest known Tc as a function of time. Tc and Bc2 values of some prominent materials Superconductor Nb NbZr NbTi V3 Ga Nb3 Sn (Nb, Ta)3 Sn Nb3 Ge PbMo6 S8 Y1 Ba2 Cu3 O7 Bi2 Sr2 Ca1 Cu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 Ca2 Cu3 O10

Tc 9.2 K 10.8 K 10.2 K 16.5 K 18 K 18 K 23 K 14 K 90 K 90 K 110 K 125 K

Bc2 (4.2 K) 0.27 T 11 T 11 T 22 T 22 T 25 T 30 T 45 T Highly anisotropic ≥50 T, BCu-O-layers ≥200 T, B ⊥Cu-O-layers

doped materials, to the highest achievable Tc are technically interesting. For values of Tc and Bc2 in important materials, we refer to Table 12.1. The critical current density Jc is strongly dependent on temperature and magnetic field in all classes of materials. In high-Tc materials Jc is in addition, strongly anisotropic, and depends critically on grain boundary alignment (texturing) and on successful introduction of pinning centres. Clearly, these aspects bring processing technology to the forefront as the key to achieving successful material control during manufacture of wires and cables. Optimization of Jc is a demanding task in all bulk superconductor applications, but specially so in the high-Tc cuprates. The great potential advantages of high-Tc materials are their high critical temperature and high upper critical fields. These advantages are easily lost unless extremely careful processing methods are developed to meet the challenges mentioned. In recent years much progress has been made in making multi-filamentary wires even of high-Tc superconductors, especially Bi2223 and Bi2212, by the powder-in-tube method. A new generation of highTc wires and cables is under development by superconductor film deposition on non-superconducting substrates with matching lattice constant. The ultimate success of high-Tc applications in the area of wires and cables will depend crucially on the outcome of this extremely demanding processing development. Only the solid solution alloy NbTi- and the Nb3 Sn-based binary intermetallic compound have so far reached the stage of an industrially produced commercial superconductor. The optimum composition of NbTi contains about 47 to 50 wt. per cent Ti. The exact critical parameters of Nb3 Sn depend on the composition and the perfection of the superconducting A15 phase. In ternary compounds like (NbTa)3 Sn or (NbTi)3 Sn Bc2 can be enhanced without sacrificing too much in Tc and workability. Adding 7.5 wt. per cent Ta to the Nb results in a Bc2 shift of about 3 T. According to the Bc2 values NbTi conductors can be used up to field levels of 10 T and Nb3 Sn-based conductors up to about 20 T. Possible candidates

352

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

for applications beyond 20 T are Chevrel phases, like PbMo6 S8 , or HTS like Bi2 Sr2 Ca2 Cu3 O10 and Bi2 Sr2 Ca1 Cu2 O8 when operated at low temperature. Due to their crystal structure with the superconductivity mainly in the CuO2 planes, the behaviour of HTS in a magnetic field is highly anisotropic, leading to much higher Bc2 values when the magnetic field is parallel to the CuO2 planes as compared with the field perpendicular to these planes. A high critical current density Jc at operational field is a precondition for most applications. Usually Jc values of 105 to 106 A/cm2 are desirable. A lower limit is 104 A/cm2 . A type II superconductor is penetrated by the magnetic field in form of quantized flux lines. Only the volume outside the flux line remains superconducting. Bc2 is reached when the flux lines fill up the total volume. An ideal type II superconductor can not carry a superconducting current because the flux lines move by the Lorentz force. This movements leads to electric fields and therefore to losses. The superconductor must therefore be hardened by microstructural features acting as pinning centres for flux lines. Effective pinnings centers can be for instance precipitates of normal conducting phase, like in NbTi, or grain boundaries as in Nb3 Sn. But grain boundaries may at the same time act as weak links, thus impeding the current flow from one grain to its neighbour. Thus it is possible to have high intragrain Jc , yet at the same time low intergrain Jc in the same material, giving low overall transport critical current density. High-Tc materials are well known for such problems, among them YBCO. As we have discussed in Chapter 8 the critical current density Jc is defined at the point where the Lorenz force begins to exceed the pinning force, i.e. at the onset of flux flow . In this regime, above Jc , current transport is no longer lossless. But even at low current density another loss mechanism is active. This is the flux creep process. The presence of such effects is seen in the decay of magnetization with time. The creep effect is usually very small in the liquid helium range, but becomes more and more significant as the temperature is increased. This is a well-known problem in all high-Tc materials operating at elevated temperatures up to 77 K or higher. We refer to the Topical Contribution by Muralidhar and Murakami (Section 13.4) showing how a sophisticated interplay between composition and processing can improve pinning up to 77 K in YBCO-type high-Tc materials. Another important phenomenon related to flux penetration and flux pinning is so-called flux jump. This phenomenon, which can lead to severe instabilities, may be suppressed by appropriate design. Due to inhomogeneities of the material the onset of flux flow is not a sharp criterion for determination of critical current. A practical criterion is therefore used: Jc is defined as the current density at the point where a 1 µV/cm electric field is observed across the sample in the transport direction. In small laboratory scale experiments the criterion is often set simply as 1 µV. A corresponding criterion using resistivity measurements is to identify the current where the resistivity reaches 10−14 to 10−13 m. Often the transition from superconducting to

LOW-Tc WIRE AND CABLE

353

107 0.1 µV/cm

Nb3Sn

(NbTa)3Sn

Jc non Cu [A/cm2]

106

10−14 Ωm

NbTi

4.2 K 2K 4.2 K 2K 4.2 K 2K

105

104

103

102 0

2

4

6

8 10 12 14 16 18 20 22 24 26 B [T]

Figure 12.1 Critical current density as a function of magnetic field and temperature for metallic superconductors: NbTi, Nb3 Sn, (NbTa)3 Sn at 4.2 K and 1.8 K, respectively. In case of Nb3 Sn-based conductors the bronze area is included in the calculation of Jc .

normal transport can be described by a power law, as discussed in Chapter 8, i.e. E ∝ I n . The higher the exponent n, the higher quality of a technical superconductor. A high value of the exponent n reflects uniform pinning and generally uniform material conditions. In Figure 12.1 Jc values of commercial grade NbTi, Nb3 Sn, and (NbTa)3 Sn are shown as a function of magnetic field at 4.2 K and 1.8 K. In Nb3 Sn the conductors were produced by the bronze route, as will be explained below. In this case the bronze area is included in the calculation of Jc . An estimate of Jc in the superconductor is obtained by multiplying the Jc value by a factor of 3.

12.1.4

Design of technical superconductors

The starting point for the mechanical design of a technical superconductor is its behaviour in a magnetic field. This field may be of external or of internal origin

354

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(self-field). According to the Bean model the full penetration field Bp , which is the maximum field that can be shielded is, as shown in Chapter 8 Bp = 2µ0 Jc a

(12.1)

in a slab of thickness 2a. We have referred to this condition as the critical state. Figure 12.2 and the discussion of the Bean model in Chapter 8 should be consulted for a better understanding of how this model describes flux penetration under different external fields Bm . In the Bean model, as we have

Bext

Jc

Jc

B T2

Bext Bp

Bext

T1

2

−a

+a

Bm

(1)

2a (b)

(a)

(c)

Bp

Bm

(2)

(a)

(b)

(c)

(d)

Figure 12.2 Field pattern in a superconducting slab according to the Bean model. Upper: field and current directions and field patterns for two temperatures T2 > T1 , (Jc (T2 ) < J (T1 )). Lower: Field pattern for a time varying field with amplitude Bm /2: (1) Bm < Bp , (2) Bm > Bp .

355

LOW-Tc WIRE AND CABLE

seen, Jc is defined by the field gradient, which is taken to be constant, i.e. dB = µ0 Jc dx

12.1.5

(12.2)

Stabilization

The Bean model does not say anything about stability. In reality there is always a decay of currents. This means that the field profile will flatten out, or ‘thermalize’, given sufficient time. The time taken for this process can vary by many orders of magnitude depending on the controlling factors for flux creep: temperature and pinning barriers. In addition, strong external disturbances can cause flux jumps with large energy dissipation, which can lead to quench of the superconductor. Such severe disturbances can be of magnetic, thermal, or mechanical nature leading to a positive feedback. Functional breakdown events due to such effects may be avoided by appropriate prevention measures. (i) Reduction of available magnetic energy by fine subdivision of the superconductor volume so that the heat capacity of the superconductor and its nearest surrounding matrix is high enough to limit the temperature increase T following the flux jump event. The technical term for this is adiabatic stabilization. (ii) Damping of the rate of flux change by highly conducting surrounding normal conducting matrix, Cu or Al. This ensures both a reduced heat generation and efficient heat removal to the coolant. The technical term for this is dynamic stabilization. The subdivision required to achieve these goals can be calculated by accounting for both energy and power balance, respectively. In case a magnetic field is perpendicular to the wire axis, the adiabatic stabilization requirement on the superconducting filament diameter d is 2 d< Jc

CT µ0

1 2

(12.3)

c where C is the volumetric specific heat, and T = dJ−J . Usually Jc decreases c /dT linearly with temperature so that T = Tc (Bop ) − Top , where Bop and Top are operational field and temperature, respectively. For typical parameter values of NbTi at 4.2 K this results in d < 100 µm filament diameter. When this criterion is used at 77 K for HTS systems one finds that much larger diameters are allowed due to the far higher heat capacity of both the superconductor and the matrix. Obviously, such thin filaments have a quite low current carrying capacity. Therefore a large number of them may be needed, bundled together and embedded in a normal conducting matrix. If this matrix is electrically and thermally highly conductive, one can achieve dynamic stabilization according to the above analysis. To avoid an unacceptable temperature increase inside a

356

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

filament, the following criterion must be fulfilled to prevent flux jumps: d

1 the result is B2 Qh = m 2µ0

For

Bm Bp

Bp 2 − Bm 3

Bp Bm

2 (12.9)

1 this gives, when combined with the Bean equation (Eq. 12.1) Qh = Bm Jc an

(12.10)

The demagnetization factor n has been included here. For circular filaments in a transverse field configuration n = 2. As can be seen from Eq. 12.10 magnetization and hysteresis losses can only be kept small by using fine filaments. For most applications d = 5–10 µm is sufficient, but for 50 Hz applications sub-micrometre filaments are required. The coupling losses Qc can be estimated for slow field changes, i.e. for Tm τ , according to B 2 8τ (12.11) Qc = m 2µ0 Tm

LOW-Tc WIRE AND CABLE

359

where Tm is the field rise time and τ is the conductor time constant given by τ=

2 µ0 lp 8π 2 ρtr

(12.12)

Here lp is the twist pitch (or transposition length lt ) as before, and ρtr is the effective transverse resistivity of the matrix (or of the cable or braid). Since lp typically is limited to values larger than about 10 times the respective diameter if each stage (strand or cable stage), the only means to reduce the coupling losses further is by introduction of resistive barriers, for instance CuNi, into the composite.

12.1.7

Mechanical characteristics

Important design criteria are related to mechanical loads that a superconductor has to accommodate during building and operation, i.e. during coil winding, cool-down, operation, and warm-up. The stresses during operation are dominated by magnetic forces. Typically the stress level is given by σ = JBR

(12.13)

where J is the overall current density, B is the magnetic field, and R is the coil radius. The conductor must withstand these stresses without mechanical damage and without degradation of the critical current density. NbTi conductors show little degradation of Jc as a function of stress and strain. Nb3 Sn-based conductors are much more sensitive to strain, especially in high magnetic fields. Also, Nb3 Sn conductors are very brittle after reaction (discussed below) and allow only strain levels below 0.3% for safe operation.

12.1.8

Fabrication technology

As described above, a technical superconductor consists of a composite of superconducting filaments and a stabilizing matrix, with additional optional components. A suitable fabrication process must be capable of producing long length of composite conductors in a reliable and economic way. The process must allow to optimize the superconducting properties, especially the current carrying capacity. The completed composite wire must be processable into more complex conductor geometries, like cables and magnet coils. In spite of the fact that many superconducting materials are known, the complexity of all these requirements has so far resulted in only two low-Tc materials of technical importance for bulk applications. These are the ductile alloy NbTi and the brittle intermetallic compound Nb3 Sn. Due to its difficult handling Nb3 Sn is only used at high fields

360

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(greater than 10 T) where the current carrying capacity of NbTi decreases very strongly. The fabrication of a multi-filamentary wire is shown schematically in Figure 12.5. In the case of NbTi/Cu composite, prefabricated NbTi and Cu parts are bundled inside a Cu-tube to form a billet with an outer diameter of typically 100–200 mm. The billet is evacuated and warm extruded to a rod of 20–70 mm diameter. Further area reduction is achieved by cold working on drawing benches, bull blocs, and multiple drawing machines. Twisting of the wire is performed close to final dimension. The number of NbTi filaments and the copper to superconductor ratio is chosen according to the application. The composite wire can be further processed into rectangular and other profiles and cables required for special applications. Co-processing of NbTi and Cu is possible because both materials are quite ductile and are similar with respect to hardness and resistance to deformation. With other, less favourable materials combinations other solutions had to be found. In some cases stabilization with ultrapure aluminum is desirable due to very low residual resistance. A process to achieve Al-stabilized conductor is by co-extrusion of Al onto a prefabricated NbTi/Cu composite wire or cable as shown in Figure 12.6. In Figure 12.7 some examples of NbTi conductors may be seen. The brittle Nb3 Sn compound cannot be processed by either coldworking or warmworking. The solution is to use a composite of ductile precursor materials and to develop the superconducting phase after the deformation process. The most reliable method is by the bronze route where Nb rods are embedded in a CuSn bronze, and the Nb3 Sn is formed by solid sate diffusion and reaction

Billet

Extrusion

Drawing

Twisting

Figure 12.5 Fabrication of a multifilamentary conductor. Conductors with a very large number of filaments (>10 000) are produced by a two stage bundling and extrusion.

Aluminium

Conductor

Profiling

Cabling

Co-extrusion

Figure 12.6 Examples of processing of multifilamentary wires for special applications (rectangular profiling, cabling, co-extrusion with aluminium).

LOW-Tc WIRE AND CABLE

(a)

(b)

(c)

(d)

361

Figure 12.7 Configuration of NbTi conductors. (a) Standard conductor with 54 filaments and a Cu:NbTi ratio α = 1.35 for Nuclear Magnetic Resonance (NMR) and laboratory magnets. Typical wire diameter 0.7 mm. (b) Conductor with 24 filaments and α = 6.5 for whole body magnetic resonance imaging (MRI) magnets. Typical wire diameter 1 to 2 mm. (c) Conductor with 6000 filaments with 5 µm diameter at a wire diameter of 0.65 mm for accelerators with low magnetization requirements for the filaments. (d) Conductor with 1200 filaments with 10 µm diameter and mixed Cu/CuNi matrix with low hysteresis and coupling losses e.g. for pulsed field applications. After Krauth in Fossheim [167].

process at about 700 ◦ C. This is the reason why the Nb3 Sn configuration differs from that of the NbTi conductor. To allow effective transformation of the Nb into Nb3 Sn within a reasonable time, in practice a few days, the filament diameter is limited to about 3 to 5 µm. Consequently, a very high number of filaments is required, typically 10 000, such that the bundling and deformation process has to be performed twice. In addition, the CuSn matrix does not stabilize and protect the conductor, so that additional copper has to be added, preferentially in the second bundling process. The pure Cu has to be protected from poisoning by Sn during the reaction heat treatment by means of a diffusion barrier, for instance of Ta. Figure 12.8 shows examples of resulting multi-filamentary wires. Optimization of critical current density is part of the conductor fabrication process. It is determined by the microstructure, and can therefore be controlled during the fabrication process. Optimization of Jc is achieved by introduction of finely dispersed microstructural features acting as pinning centres. In the case of NbTi normal conducting α-Ti precipitates in the superconducting β-phase are

362

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(a)

(b)

(c)

(d)

Figure 12.8 Configuration of Nb3 Sn conductors with Ta diffusion barriers. (a) Standard conductor with 6000 filaments in a bronze matrix and internal Cu stabilization. (b) Conductor with 20 000 filaments and external Cu stabilization. Fully transposed flat (keystoned) cables for accelerator magnets (dipoles and quadrupoles). (c) 23 NbTi strands with 0.84 mm diameter. (d) 36 Nb3 Sn strands with 0.92 mm diameter. After Krauth in Fossheim [167].

known as the most effective pinning centres. In the case of Nb3 Sn the grain boundaries act as pinning centres. A microstructure with fine grains is therefore required to get high Jc -values. This is achieved by performing the reaction heat treatment at about 700 ◦ C for three days. The reaction treatment can be performed either before the coil winding (react-and-wind) or after coil winding (wind-and-react). The latter is mostly used for small magnets, and the former for large magnets with low bending strain during coil winding.

12.2 High-Tc wire and cable 12.2.1

High-Tc wire and tape

Successful development of high-Tc wire as a basis for high current transport was so far achieved by use of Bi2223, and to some extent using Bi2212 material. The dominating methodology is to produce wires by the powder-in-tube (PIT)

HIGH-Tc WIRE AND CABLE

363

technique. This is done by filling the pre-reacted powder into silver a tube. Its dimension will determine how long length can eventually be produced. The resulting filled tube is extruded and drawn to several times its original length. Continued drawing leads to a single filamentary wire which may be rolled to the dimension of about 3 mm width and 0.3 mm thickness. After processing at temperatures approaching 900 ◦ C in oxygen atmosphere, and subsequent cooling to room temperatures at varying rates, a superconducting wire results. In the next stage multi-filamentary wires of 100-odd superconducting tape wires of kilometre lengths is produced. Production of such wires involves a repetition of the drawing stage in which the first extruded and partially drawn tube is cut into short lengths of metre size, and packed into a second Ag tube. The drawing and rolling process is now repeated, resulting in a multi-filamentary tape shaped wire. Thermal processing is similar to the single filament case. To illustrate the sophistication required to develop second generation of conductors of the quality required on a large scale, we refer to the Topical Contribution, by Thompson and Christen (Section 13.9).

12.2.2

Full-scale high-Tc cable

The technology for high-Tc cable manufacturing is maturing gradually. Several projects are under way. Full scale cables have so far been manufactured from Bi2223 tapes only. The next generation of tapes based on deposition of YBCO film is expected to provide great improvements in the long run. The speed of the manufacturing process is still far too low for this next generation of tapes to be applicable in cables. A good example of high-Tc cable implementation using Bi2223 tapes is the Danish HTS power cable project [173], the first HTS cable operated in a public network. In 2001 installation of a 30-m, 30 kVrms , and 2000 A three-phase HTS cable was carried out in a substation of the Copenhagen utility network. One year later, the operating experiences were deemed satisfactory. The cable supplied electric energy corresponding to the average consumption of about 25 000 households, over 100 000 MWh of energy. The advantages seen for a HTS power cable may be listed as follows • High current and power rating • Compact cable dimensions and low weight (about 1/3 of conventional cable) • Low losses • No thermal or magnetic interaction with surroundings. HTS power cables have a potential for reduced cost per transferred unit of energy compared to conventional technology due to low material consumption and potentially lower installment cost. The cables may be used as short internal

364

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

Figure 12.9 The Danish HTS cable design [173]. Reproduced with the authors’ permission.

substation connections and retrofits (replacement) of low capacity conventional cables in existing ducts. They may further be applied for urban feeder cables, bulk power transmission, low-voltage high-current cables, DC power, etc. The design of the Danish HTS cable is shown in Figure 12.9. The superconducting tapes are wound in a helical pattern on the inner corrugated flexible steel tube. The superconductor is cooled by liquid nitrogen flowing through the steel tube at a rate of 700 kg/hour at 4 bar. The HTS tapes are nowhere in direct contact with liquid nitrogen. The main structure from inner to outer layers is briefly characterized by the following sequence: The inner tube, called the ‘former’, on which the superconducting tapes are wound, has an outer diameter of 30 mm. Then follow first the superconductor tape layers, next a thermal insulation layer, an electrical insulation layer, an electrical Cu-screen, and finally a polyethylene sheath of ID/OD dimensions 95/105 mm. The critical current Ic was measured as 2770 A at 79 K, and 5000 A at 66 K. No degradation was detected during one year of operation.

12.2.3

HTS induction heater

Electromagnetic induction heating is commonly used for industrial heating of metals. Figure 12.10 illustrates the principle involved in induction heating [174]. A metal workpiece is placed inside a solenoidal coil, and when an AC current is passed through the windings, the time-varying magnetic field generated by the coil induces electric currents in the metal, causing resistive dissipation and

HIGH-Tc WIRE AND CABLE

365

Figure 12.10 Principles of billet heating using a superconducting coil [174]. Reproduced with the authors’ permission.

heating of the workpiece. For aluminum extrusion the typical billets used for extrusion are of about 20 cm diameter and 1–2 m length. The billet is heated to temperatures of around 500 ◦ C in about 2 min to soften the metal just before extrusion takes place. Runde and coworkers [174] have introduced a new concept in induction heating by use of high-temperature superconductor (HTS) windings in the induction coil. The great advantage is that the losses in the coil can be reduced to a small fraction of those in conventional coils. A simple analysis shows that the overall electrical efficiency η may be expressed as 1

η= 1+

ρc ρw µw

(12.14)

where ρc and ρw are the resistivities of the coil and the workpiece, respectively, and µw is the permeability of the workpiece. From Eq. 12.14 we observe that if the resistivities of the workpiece and the coil are similar, the efficiency approaches 1/2. However, if the resistivity in the coil is eliminated, the efficiency approaches 1, or 100%. These are of course ideal values, but the effect is in any case very significant. A demonstrator HTS induction heater has been shown to work as expected. The coils were of so-called stacked pancake design made of stainless steel reinforced multi-filamentary Bi-2223/Ag tape with a self-field

366

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY Epoxy cryostat

Superinsulation

Flux diverters HTS coils

LN2

Al billet

Thermal insulation

Figure 12.11 Cross-sectional view of the induction heater. The heater is concentrically built up around the dash-dotted symmetry line. The current leads and various structural parts made in fibreglass reinforced epoxy are not included in the drawing [174]. Reproduced with the authors’ permission.

critical current of 115 A. Figure 12.11 shows the design used. The reduced scale demonstrator prototype reached 500 ◦ C in about 5 minutes. In the original tests, DC HTS tapes were used. With AC tapes one would expect to be able to apply higher currents, and reduce the heating period substantially. An important feature of the design is the insertion of iron rings at each end of the coil. These are placed there to prevent solenoidal stray field from taking a short route through the coil near its ends. This would have allowed some field to cross the pancake coil windings normal to the tape, a field configuration which has a strongly detrimental effect on the critical current in Bi2223 tapes.

12.3

Magnet technology

Superconducting magnet technology is a mature field today, and well described in textbooks. In the present context we have found it interesting to present two outstanding unconventional examples of recent development in superconductor

MAGNET TECHNOLOGY

367

magnet applications. The frist one is a description of a fullscale complex magnet system, the worlds strongest, 45 T, stationary field hybrid magnet, built and operated by the National High Magnetic Field Laboratory at Florida Sate University in Tallahassee, Florida. For this outstanding example of magnet technology we refer to the Topical Contribution by Schneider-Muntau in Section 13.5. The second example is a pure materials development which has been carried out at the Superconductivity Research Laboratory at ISTEC in Tokyo. Murakami has led the efforts to tailor the pinning properties of YBCO-type cuprate superconductors for storage of truly high magnetic field. We refer to the topical contribution in by Muralidhar and Murakami (Section 13.4) on this subject.

PART IV

Topical Contributions

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

13 Topical Contributions This Chapter contains nine invited contributions written for this book by particularly outstanding scientists from Europe, Japan and USA in various fields of superconductor research. The authors have been asked to write their contributions in as short form as seemed pedagogically possible. These examples highlight specific subjects at the forefront of research and development at the time of writing this textbook. Scientific references belonging to this chapter are given at the end of the chapter.

13.1

Spin-Triplet superconductivity by Y. Maeno

What is the spin triplet superconductivity? When two electrons form a pair in the superconducting state, the total spin of the pair is either S = 0 (spin singlet) or 1 (spin triplet). Because of the symmetry relation for the permutation of electrons as Fermions, the state vector of a Cooper pair | = χ (k 1 , k 2 )|σ1 , σ2 must be antisymmetric with respect to the exchange of the two electrons involved. Here k i and σi are the momentum and spin of an electron and χ is the orbital wave function. For spin-singlet state with antisymmetric spin part, | ↑↓ − | ↓↑, the orbital wave function has to be symmetric so that the allowed orbital angular momentum L of a pair contains even-number components only: L = 0 is called the s-wave, L = 2 the d-wave, etc. It is in principle possible to form spin-triplet pairs. In this case the spin state is symmetric, | ↑↑, | ↑↓ − | ↓↑, or | ↓↓, corresponding to Sz = 1, 0, or −1, respectively. Thus the orbital wave function has to be antisymmetric with the orbital angular momentum L = odd number: L = 1 is called the p-wave, L = 3 the f-wave, etc. Conventional superconductors are in the spin-singlet s-wave state. However, a number of unconventional non-s-wave superconductors have been found. For Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

372

TOPICAL CONTRIBUTIONS

example, it has been shown that even the high-transition temperature copperoxide (high-Tc cuprate) superconductors have spin-singlet electron pairs, but the pairing is in the d-wave symmetry.

Which superconductors are spin triplet? Investigation of spin-triplet superconductivity started soon after the birth of the BCS theory [1]. It has been well established that superfluidity of 3 He is carried by Cooper pairs of 3 He atoms with their nuclear spins forming spin-triplet states [2]. However, it has not been easy to prove whether a candidate superconductor is in fact spin triplet, mainly because the Meissner effect masks the magnetic susceptibility of the electron spins. Nevertheless, there are a number of superconductors for which the spin-triplet pairing is strongly suggested [3]. An earlier example is the heavy Fermion superconductor UPt3 , for which there are three superconducting phases when the magnetic field and temperature are varied. Recently, a new class of superconductors have been found in which superconductivity occurs below the transition temperature of ferromagnetic ordering and coexists with the ferromagnetism. A good example of this class of superconductors is UGe2 . A layered ruthenate Sr2 RuO4 [4] is a unique example because it is probably the only oxide for which spin-triplet nature has been confirmed so far. As shown in Figure 13.1, its crystal structure is common to the first high-Tc cuprate superconductor discovered by Bednorz and M¨uller, La2−x Bax CuO4 , but the Tc of Sr2 RuO4 is 1.5 K, much lower than the corresponding high-Tc cuprate. Since the electronic properties of its normal state is characterized in detail, it is arguably the most extensively and quantitatively characterized spin-triplet superconductor [3]. From the nuclear magnetic resonance (NMR) Knight shift, the spin susceptibility for the magnetic field parallel to the RuO2 layer was found to be unchanged on entering the superconducting state, marking the definitive evidence for the spin-triplet pair formation with Sz = 0 [5]. In addition, from the muon-spin relaxation measurements, spontaneous internal magnetic field was found to emerge below Tc [6]. This suggests that the time-reversal symmetry (TRS) is broken in the superconducting state. The origin of the broken TRS is attributed to the unquenched orbital angular momentum of the pairs; thus Lz = +1 or −1. Taking into consideration of consistencies with a number of other experimental results, as well as with theoretical requirements, it is believed that the pairing state is described as S = 1, Sz = 0; L = 1, Lz = +1 or −1. Such spin and orbital state for this p-wave superconductivity is schematically represented in Figure 13.2. The mechanism of the spin-triplet formation has not been fully understood, but it is believed by many that the strong electron correlations due to Coulomb interactions among the 4d electrons of ruthenium ions play the essential role in the pairing, rather than the conventional electron-phonon interactions.

SPIN-TRIPLET SUPERCONDUCTIVITY BY Y. MAENO

Sr2RuO4

La2-cBacCuO4

Sr

La (Ba)

Ru

Cu

O

373

O

C

a a

Figure 13.1 The layered crystal structure common to the spin-triplet ruthenate superconductor and high-Tc cuprate superconductor. Image is by K. Deguchi.

Orbital angular momentum

Electron

Spin

c (z) b a

Figure 13.2 The representation of the spin triplet electron pairs in Sr2 RuO4 . Small arrows depict the spins of an electron pair, while the large arrow represents the orbital angular momentum. Image is by K. Deguchi.

New physics expected with spin-triplet superconductivity For spin-triplet superconductors, not only the charge degree of freedom, but also the spin degree of freedom exhibits “superfluidity”. Thus a variety of phenomena not present in spin-singlet superconductors are expected. Because of the internal degree of freedom of the triplet pairs, multiple superconducting phases are excepted to emerge and they are in fact observed in Sr2 RuO4 , as well as in UPt3 [3]. Although not reported in any superconductor so far, induction of collective motions of spin or orbital moments without breaking the pairs is also expected. For Sr2 RuO4 the phase of the wave function should vary with the

374

TOPICAL CONTRIBUTIONS

azimuthal angle and effects sensitive to this phase are also expected in the tunneling. Furthermore, the TRS broken state is characterized by “chirality”, with all the Cooper pairs within a single superconducting domain having a common sign of their orbital moments (plus or minus). If the chirality can be externally controlled, it may be used as a quantum bit, a nanoscale unit for future quantum devices.

13.2 π -SQUIDs – realization and properties by J. Mannhart The predominantly dx 2 −y 2 -pairing symmetry of the high-Tc superconductors influences fundamental properties of Josephson junctions and Josephson junction-based devices, such as Superconducting Quantum Interference Devices (SQUIDs). Notably, it offers the possibility to fabricate Josephson junctions which in equilibrium are biased by a phase shift of π , and dc π -SQUIDs which consist of such a π -Josephson junction and a conventional junction connected in a loop [7]. The electrical characteristics of these devices provide detailed insight into the symmetry of the superconducting order parameter, tracing for example possible admixtures of sub-dominant symmetry components. Furthermore, the devices present novel building blocks for superconducting quantum electronics [8]. All-high-Tc dc π -SQUIDs have been fabricated according to the design illustrated in Figure 13.3. A detailed description has been provided in [7]. Exploiting the bicrystal technology [9], the devices are based on two ∼10 µm wide, symmetric 45◦ [001]-tilt grain boundaries formed by ∼100 nm thick, c-axis oriented YBa2 Cu3 O7−δ -films grown on SrTiO3 -tetracrystals. Due to the orientation of the grain boundaries, across one of the junctions order parameter lobes with opposite signs face each other. This π -phase difference defines the π -junction. In practice the π -junction is the junction with the smaller critical current, because it has the smaller Josephson coupling energy. The current-voltage, I (V )-characteristics of the π -SQUIDs follow the behavior expected according to the resistively shunted junction model, with additional self-induced resonances which disappear for small applied magnetic fields, as shown in Figure 13.4 [10]. The magnetic field dependencies of the π -SQUIDs critical currents Ic (H ) (see Figure 13.5) are characterized by a minimum at small fields, exactly opposite to the behavior of the standard SQUIDs’ critical currents, which for vanishing applied fields are maximal. This characteristic effect is expected for superconductors with a pure dx 2 −y 2 -symmetry. The Ic (H )dependencies for larger applied magnetic fields are highly symmetric, proving that the measurements are not influenced by spurious trapped magnetic flux [7]. The self-induced resonances shown by the π -SQUIDs’ I (V )-characteristics reveal that in the voltage state the dx 2 −y 2 -wave symmetry induces circulating

π -SQUIDS – REALIZATION AND PROPERTIES BY J. MANNHART

375

Figure 13.3 Sketch of a π-SQUID fabricated by using the bicrystal technology (after [7]).

200

p- SQUID 4.2 K 0 µT

100

V (µV)

2.55 µT 0

−100

−200 −30

−20

−10

0 I (µA)

10

20

30

Figure 13.4 Current-voltage characteristics of a π-SQUID measured at 4.2 K at zero field and at the smallest magnetic field that causes a maximum of Ic (from [10]).

ac-currents, which oscillate with the Josephson frequency in the π -ring configuration. This provides evidence that the π -shift as well as the order parameter symmetry are maintained for Josephson frequencies up to several tens of GHz [10]. The technology to fabricate π -Josephson junctions and π -SQUIDs is extendable to the design of circuits with larger numbers of π -type junctions. Well operating π -SQUIDs have now also been fabricated by using the ramp-type Josephson junction technology [11].

376

TOPICAL CONTRIBUTIONS 0 - SQUID 15

0.4

10

0.2

5 Ic (µA)

Ic (µA)

p- SQUID 0.6

0.0

0

−0.2

−5

−0.4

−10

−0.6

−6

−4

−2 0 2 m0H (µT)

4

6

−15

−6

−4

−2 0 2 m0H (µT)

4

6

Figure 13.5 Dependencies of the critical current on applied magnetic field of a π-SQUID and of a standard SQUID at 77 K (from [7]).

This work was performed together with H. Bielefeldt, B. Chesca, B. Goetz, H. Hilgenkamp, A. Schmehl, C.W. Schneider, and R.R. Schulz. Support by the BMBF (project EKM 13N6918) and by the ESF (Pishift-Project) is gratefully acknowledged.

13.3 Doppler effect and the thermal Hall conductivity of quasiparticles in d-wave superconductors by N.P. Ong At temperatures very close to absolute zero, all the electrons in a superconductor are paired. The collection of Cooper pairs constitutes the condensate or superfluid. At finite temperatures T , however, a few of the Cooper pairs break up to form a gas of ‘singles’ called Bogolyubov quasiparticles (the entropy of the quasiparticle gas lowers the sample’s free energy). With increasing T , the quasiparticle population nqp (T ) increases rapidly until all the pairs become singles at the critical transition temperature Tc . The thermal conductivity κ has proved to be a fruitful way to study the transport properties of quasiparticles. In a temperature gradient −∇T , the flow of quasiparticles towards the cooler end generates a thermal current Je (as the condensate itself has zero entropy, it does not contribute to the thermal conductivity). However, the gradient also produces a parallel phonon current Jph which greatly complicates the interpretation of measurements of κ. First, let us consider the normal state of a conventional metal such as Pb. κ is the sum of the electronic term κe and the phonon term κph , viz. κ = κe + κph (κe is about 100 times larger than κph in Pb, but κe is 5-8 times smaller than κph in the cuprates). As T falls below Tc in Pb, the rapid (exponential) decrease of

DOPPLER EFFECT AND THE THERMAL HALL CONDUCTIVITY

377

50

κ (W/mK)

40 0.5 40 K

30 20 10

0.4 0 0

κxy (W/mK)

50

100 50 T(K)

150

0.3

60

0.2

70 0.1 75 K 0.0

0

2

4

6 8 m0 H(T)

10

12

14

Figure 13.6 (Main Panel) Curves of κxy versus the applied field H at selected temperatures in high-purity YBa2 Cu3 O7 . At high T , κxy is linear in H , but as T decreases, its field profile displays a prominent peak. The initial slope limH →0 κxy /H increases by a factor of 1000 between 85 and 40 K. The inset shows the zero-field thermal conductivity κ versus T . A prominent peak appears below Tc = 93 K [adapted from 13].

nqp leads to a sharp decrease in κe . However, this is partially compensated by an increase in κph because the decreasing nqp results in a marked decrease in the scattering of phonons. Hence the total κ in a typical s-wave superconductor decreases rather gradually below Tc . If the sample is of exceptional purity, this gradual decrease is interrupted by a resurgent κ ∼ κph which rises to a prominent peak below ∼ 12 Tc . The phonons, now largely free of any scattering by quasiparticles, develop exceedingly long mean-free-paths (mfp) limited only by the size of the crystal. Eventually, at very low T , κph vanishes as T 3 , reflecting the specific heat of the phonon gas. A major puzzle in the high-Tc cuprates became apparent shortly after the 1987 discovery of the ‘90-K’ superconductor YBa2 Cu3 O7 . Instead of decreasing below Tc , κ is observed to rise sharply, reaching a peak value 2–3 times larger than the value just above Tc = 93 K (inset of Figure 13.6). The origin of the giant anomaly in κ has been a source of debate. Recalling κ in Pb, many investigators initially identified the giant anomaly with a strong enhancement of the mfp of phonons. However, this identification was unconvincing because the quasiparticle population in the cuprates falls quite slowly below Tc (in contrast

378

TOPICAL CONTRIBUTIONS

with Pb). How can we distinguish the phonon and quasiparticle currents in the cuprates? Let us consider applying a magnetic field B normal to the plane of the crystal. The field pierces the condensate as an array of vortices. Quasiparticles do not ‘see’ the applied magnetic field, but they scatter from the vortices (which act like impurities in the otherwise uniform condensate). A quasiparticle incident on a vortex line strongly scatters from the steep decrease in the pair potential at the core. More germane to our discussion, it interacts with the intense azimuthal supercurrent surrounding the core. Generally, the energy of a quasiparticle is shifted in the presence of a superflow. If the quasiparticle moves in a direction parallel to that of the local superfluid velocity (co-moving), its velocity relative to the lattice is increased (this so-called Doppler effect is analogous to viewing a pedestrian walking on a moving ramp). Conversely, a quasiparticle moving against the superfluid has its velocity lowered. The difference in kinetic energies implies that quasiparticles prefer to go around a vortex in the direction against the azimuthal superfluid velocity. If the superflow is clockwise (viewed from above), the incident quasiparticle is preferentially scattered to the left, whereas it is scattered to the right when the flow is counterclockwise. The resulting ‘skew’ scattering produces a net ‘Hall entropy current’ (if −∇T is applied along x with H z, the Hall current is along y and given by Jy = κyx (−∇T ), where κxy is called the thermal Hall conductivity). Phonons, which are charge-neutral, do not experience this asymmetric scattering. Hence the thermal Hall effect acts very much like a selective filter that ignores the phonon current. The thermal Hall effect was detected in high-purity crystals of YBa2 Cu3 O7 and investigated in detail from ∼12 K to temperatures slightly above Tc [12, 13]. In weak fields, κxy increases linearly with H (main panel of Figure 13.6). In high-purity crystals, this linear field dependence evolves into a profile with a prominent peak. The profile is consistent with a very long quasiparticle meanfree-path when the field is absent. If we plot the initial slope κxy /H (H → 0) against T , we find that it displays a remarkable thousand-fold increase [13] between Tc and 30 K that dwarfs the corresponding increase in κ. This is consistent with an increase in of over 100 within this temperature interval. The steep increase is sufficient to produce a giant peak in κe that matches the observed giant anomaly. The thermal Hall effect presents the strongest evidence to date that the giant anomaly derives entirely from the quasiparticles.

13.4 Nanometer-sized defects responsible for strong flux pinning in NEG123 superconductor at 77 K by M. Muralidhar and M. Murakami The bulk superconductor composite of (Nd0.33 Eu0.38 Gd0.28 )Ba2 Cu3 Oy with 5 mol% (Nd0.33 Eu0.33 Gd0.33 )2 BaCuO5 , 0.5 mol% Pt, and 10 wt% Ag2 O exhibits

NANOMETER-SIZED DEFECTS RESPONSIBLE FOR STRONG FLUX PINNING

379

80

Jc (kA cm−2)

2000

60

T = 77K, Hc-axis

1500 1000

Jc (kA cm−2)

500 0

13

40

13.4 13.8 m0Ha (T)

16

Birr (T)

12

20

8 4 0

80

85 90 Ι (Κ)

95

0 0

2

4

6 8 m0Ha (T)

10

12

14

Figure 13.7 Field dependence of the critical current density (Jc ) for the (Nd0.33 Eu0.38 Gd0.28 )Ba2 Cu3 Oy sample with 5 mol% NEG-211, 0.5 mol% Pt, and 10 wt% Ag2 O at 77 K and H ||c-axis. The bottom inset shows the extrapolation of Birr (T).

the irreversibility field (Birr ) over 14 T for B//c axis at 77 K [14]. The critical current density reached 70, 49, and 22 kA/cm2 at 4.5, 7, and 10 T, respectively (see Figure 13.7). The extrapolation of temperature dependence of irreversibility field between 79 K and 94 K measured with a vibrating sample magnetometer indicated the actual Birr value at 77 K about 15 T (bottom inset of Figure 13.7). Structural analyses made by transmission electron microscopy (TEM) revealed a nanometer-scale modulation structure, which had a lamellar structure with spacing of a few nanometers. Similar nano-structures were observed in the NEG123/NEG211 composite samples with 3-7 mol% NEG-211. All the samples exhibited very high irreversibility fields over 12T at 77K [15]. Chemical analysis of the matrix showed that there is a chemical fluctuation in the (Nd+Eu+Gd)/Ba ratio on a nanometer scale. Scanning tunneling microscopy (STM) also confirmed the presence of nano-scale structure as shown in Figure 13.8a. Here its average spacing is around 3.5 nm, which is close to the coherence length of YBCO at 77K (ξab (77 K) ≈ 4.5 nm) [16]. The observation with higher magnification showed that the structure consisted of rows of aligned clusters of slightly off stoichiometric composition of 3–4 nm in size (see Figure 13.8b). These clusters were identified by EDX analysis as (NEG)1.015 Ba1.985 Cu3 Oy . Tunneling current spectra taken on the RE-rich clusters, and the regular matrix showed similar conductivity of both regions. This shows that the composition of the clusters is not much different from that of the 123 matrix.

380

TOPICAL CONTRIBUTIONS

(a)

(b)

Figure 13.8 STM images of the sample with 5 mol% NEG-211 [(a)-(b)]. The image was recorded with bias voltage Vs = 1 V and tunneling current It = 0.3 nA. The black arrows in (a) mark some nanolamellas. Note the presence of arrays of clusters around 3 to 4 nm in diameter dispersed in an organized manner in the NEG-123 matrix.

Thus superior flux pinning of NEG123/NEG211 composites at higher fields and temperatures is ascribed to the formation of new type of nanometer-scale lamellar array of RE-rich clusters. These new pinning medium led to an increase of Birr up to 15 T at 77 K and thus will make it possible to construct a superconducting magnet generating >10 T at liquid nitrogen temperature.

13.5 Hybrid Magnets by H. Schneider-Muntau A hybrid magnet is a combination of a powered resistive magnet (insert) with a surrounding superconducting magnet (outsert). Hybrid magnets are built with the goal to produce the highest continuous magnetic fields possible [17–21]. Design and construction of hybrid magnets are a considerable technological and logistical challenge. Besides the sheer size of the magnet, the interaction of the subsystems, the magnitude of the forces within and between the resistive and the superconducting magnet, the cryogenic requirements, and safe and reliable operation of such a complex system require detailed attention and very specific capabilities in several disciplines. The essential components of a hybrid magnet are: superconducting magnet, the cryostat, the resistive insert, and the quench detection and protection system (see Figure 13.9). The superconducting magnet (Figure 13.10, 13.11) surrounds the resistive magnet. Because of its bore size of 360 mm (Sendai, Nijmegen), 610 mm (Tallahassee) and 800 mm (Grenoble), the magnet becomes impressive in size,

HYBRID MAGNETS BY H. SCHNEIDER-MUNTAU

381

Cryostat housing 80 K shield Resistive coils Superconducting coil (NbTi) Superconducting coils (Nb3Sn) Support column Connection to vacuum pump

Mounting flange

20 K shield

Superfluid helium cunduit

Connection to supply cryostat Superconductor joint box

Access tube Resistive housing

Burst disk

Current connection Helium exhaust Cooling water connection

Figure 13.9 Cross-sectional view of the hybrid magnet at NHMFL. It generates the highest continuous field of 45 T in a bore of 32 mm since June 2000 and has since then provided more than 2000 h per year of measuring time to the international science community.

Figure 13.10 The outsert in construction. It generates 15 T in 615 mm.

382

TOPICAL CONTRIBUTIONS

Figure 13.11 The outsert being put on the central bore tube.

especially if the field contribution is above 8 T. Even more dramatic is the increasing stored energy (in round numbers): from 10 MJ (Nijmegen) to 60 MJ (Tsukuba and future Grenoble hybrid) to 110 MJ (Tallahassee). The energy content and, even more important, the coupling between the two magnet systems make a hybrid outsert much more challenging than a stand-alone, large-bore superconducting magnet. The most important design issues for the outsert are: (a) Changes of the field of the resistive insert result in induced currents. Field changes also induce eddy current heating and coupling losses between the filaments in the superconductor. They are proportional to (dB/dt)2 and define specific requirements for the coupling time constant between filaments. The worst case is an insert trip from full field which can result into an energy deposition of over 20 kJ. (b) The ramp time of the outsert should not be more than approximately one hour in view of its operation in a user facility. The hysteresis losses are proportional to the maximum field and are independent of the ramp rate and define a requirement for the maximum admissible energy deposition as a

HYBRID MAGNETS BY H. SCHNEIDER-MUNTAU

383

function of its evacuation time. These losses can reach values of up to 100 kJ for a high field magnet. Wires with a small effective diameter have lower hysteresis losses. (c) To limit the magnet size, the conductor should operate as closely as possible to its critical current. A high index number will reduce the heating from current sharing. (d) The stability of a magnet against quench depends, among other things, on the amount of stabilizer and the available enthalpy. The presence of helium, especially superfluid helium, within or beside the conductor, increases the margin considerably. (e) In case of a quench, the energy must be extracted from the magnet and discharged into an outer resistor. An alternative solution is to dissipate the energy equally over the volume by firing heaters to quench the magnet uniformly. It is obvious from above that the worst case scenario, for which the outsert magnet must be designed, is an insert trip after a ramp to full field, plus heating through current sharing. The heat must be absorbed and transported out of the conductor with only modest excursion in the local temperature. Therefore, important design criteria are, (a) the operating temperature, and (b) the temperature gradients between current carrying filaments, conductor matrix, surrounding helium, main helium buffer and refrigerator. Three different approaches have been developed for the design of the outsert in response to the requirements listed above. They can be distinguished by the superconductor they employ: the solid, cable-in-conduit and Rutherford cable conductor. The cryostat, together with the cryogenic system, must provide the environment for safe and reliable operation of the superconducting magnet. The operating temperature of the magnet has an important impact on the design of the cryostat and magnet performance. A bath-cooled, ventilated magnet wound from solid conductor and operated at about 4.2 K represents the standard technique and has the great advantage of simplicity. However, operation of the magnet at superfluid helium with its extremely high thermal conductivity and low viscosity, increases magnet performance considerably. The heat transfer between conductor and liquid and, therefore, conductor stability and margin to external disturbances is essentially improved. Also, the critical current density in the superconductor is much higher at lower temperatures. A subcooled 1.8 K superfluid helium bath, including magnet, at atmospheric pressure can be achieved if a 1.8 K heat exchanger is introduced into the main bath. Such a cryostat system consists of a 1.8 K vessel housing the magnet, a 1.8 K heat exchanger, and two radiation shields which are at intermediate temperatures between 4.2 and 100 K, optimized for minimum losses. The magnet is kept at 1.8 K by a thermal exchange loop through expansion of 4.2 K helium in a JouleThomson valve using a vacuum pump. The forces between and within the two magnet systems, the superconducting magnet and the resistive insert, must be considered in the case of axial and radial misalignment of any of the magnetic coil centers. These forces are generated between the current carrying conductors of all coils, and are transmitted through the coil winding and support structure

384

TOPICAL CONTRIBUTIONS

and the cryostat. In case of a major failure, they can reach alarming magnitudes of several MN, which is many times the weight of the superconducting magnet system. The resistive insert magnets have lower efficiency than do stand-alone magnets without background fields (Figure 13.12). The major difficulties are: (a) The reduced volume in which the electric power must be dissipated. For economic

Figure 13.12 The hybrid magnet with view on the support and cooling water connections of the resistive insert. It consumes 30 MW, 300l/s of cooling water are needed. The superconducting magnet is located in the top vessel.

MAGNETO-OPTICAL IMAGING OF VORTEX MATTER BY T.H. JOHANSEN

385

reasons, the magnet engineer has to choose the bore of the superconducting magnet as small as possible and, therefore, the resistive magnet must be very compact and efficiently cooled. (b) The additional field from the outer magnet. The background (booster) field from the superconducting magnet increases the Lorentz forces as the insert experiences the sum of its own and the outer field. Therefore, special high-strength conductors, a multi-coil design and an adequate support structure are required. (c) The high alignment forces between the coils. Impressive forces are generated within the insert and, to a lesser extent, between the insert and the outsert. (d) The forces resulting from the termination of the winding. These endforces are extremely large, resulting from the high fields and the high operating currents. They impact strongly on the design because of their magnitude and the limited space available. An early detection of a quench is important to avoid uncontrolled growth of the resistive zone and destruction through excessive heating. Detecting a quench is difficult because the small resistive voltages must be separated from the large inductive voltages induced when either magnet is swept. The inductive voltages are up to a factor of 1000 higher. Inductive voltages can be cancelled if the magnet is divided into zones of equal inductance and the voltages are compared in bridge fashion, for instance, between taps connected to the winding. In the event of a quench, the protection system must be capable of extracting enough energy from the system that high stresses from differential thermal expansion or even overheating/melting are precluded. This is done by discharging the magnet with a defined time constant into an external resistor. Limiting the maximum or hot-spot temperature to about 150 K and the discharge voltage for fully impregnated coils to 5 kV and for ventilated coils to 3 kV results in time constants of between 3 and 20 seconds, depending on the coil energy. The quench detection and control system of a superconducting outsert is best done with several industrial quality computers. As part of the total control system and its reliability, the safety devices such as the power supply, discharge resistor, breakers, and computers, must be checked continuously for their operational conditions.

13.6 Magneto-Optical Imaging of Vortex Matter by T.H. Johansen Space-resolved magnetic measurements have during the last decades proved increasingly useful in revealing micro-structural features and physical phenomena that control the overall electromagnetic behavior of superconductors. Among the various methods, scanning probe magnetometry, Bitter decoration etc., the technique of magneto-optical (MO) imaging has two major advantages, namely it allows easy zoom from cm-scale field-of-view down to micron resolution, and secondly, the time response is very quick (

Kristian Fossheim and Asle Sudbø The Norwegian University of Science and Technology Trondheim, Norway

c 2004 Copyright

John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex PO19 8SQ, England Telephone (+44) 1243 779777

Email (for orders and customer service enquiries): [email protected] Visit our Home Page on www.wileyeurope.com or www.wiley.com All Rights Reserved. No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning or otherwise, except under the terms of the Copyright, Designs and Patents Act 1988 or under the terms of a licence issued by the Copyright Licensing Agency Ltd, 90 Tottenham Court Road, London W1T 4LP, UK, without the permission in writing of the Publisher. Requests to the Publisher should be addressed to the Permissions Department, John Wiley & Sons Ltd, The Atrium, Southern Gate, Chichester, West Sussex PO19 8SQ, England, or emailed to [email protected], or faxed to (+44) 1243 770620. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the Publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. Other Wiley Editorial Offices John Wiley & Sons Inc., 111 River Street, Hoboken, NJ 07030, USA Jossey-Bass, 989 Market Street, San Francisco, CA 94103-1741, USA Wiley-VCH Verlag GmbH, Boschstr. 12, D-69469 Weinheim, Germany John Wiley & Sons Australia Ltd, 33 Park Road, Milton, Queensland 4064, Australia John Wiley & Sons (Asia) Pte Ltd, 2 Clementi Loop #02-01, Jin Xing Distripark, Singapore 129809 John Wiley & Sons Canada Ltd, 22 Worcester Road, Etobicoke, Ontario, Canada M9W 1L1 Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Library of Congress Cataloging-in-Publication Data Fossheim, K. (Kristian) Superconductivity : physics and applications / Kristian Fossheim and Asle Sudbo. p. cm. Includes bibliographical references and index. ISBN 0-470-84452-3 (alk. paper) 1. Superconductivity. I. Sudbo, Asle. II. Title. QC611.92.F67 2004 537.6 23 – dc22 2004002271 British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library ISBN 0-470-84452-3 Typeset in 10.5/13pt Times by Laserwords Private Limited, Chennai, India Printed and bound in Great Britain by Biddles Ltd, King’s Lynn This book is printed on acid-free paper responsibly manufactured from sustainable forestry in which at least two trees are planted for each one used for paper production.

Contents Preface

xi

Acknowledgements

I 1

BASIC TOPICS

1

What is superconductivity? A brief overview

3

1.1 1.2 1.3 1.4 1.5 1.6 1.7 2

xiii

Some introductory, historical remarks Resistivity The Meissner effect: perfect diamagnetism Type I and type II superconductors Vortex lines and flux lines Thermodynamics of the superconducting state Demagnetization factors and screening

3 6 10 13 17 18 23

Superconducting materials

27

2.1 2.2

27 27 27 29 31 31 34 35 35 37 37 40 41 42

2.3

2.4 2.5 2.6

Introductory remarks Low-Tc superconductors 2.2.1 Superconducting elements 2.2.2 Binary alloys and stoichiometric compounds Organic superconductors 2.3.1 Polymer and stacked molecular type 2.3.2 Fullerene superconductors Chevrel phase materials Oxide superconductors before the cuprates High-Tc cuprate superconductors 2.6.1 The discovery of cuprate superconductors 2.6.2 Composition and structure 2.6.3 Making high Tc materials 2.6.4 Phase diagrams and doping 2.6.5 Some remarks on the original idea which led to the discovery of cuprate superconductors 2.6.6 Thermal fluctuations of the superconducting condensate. A preliminary discussion

47 48

vi

CONTENTS

2.7 2.8 2.9 3

4

52 53 55

Fermi-liquids and attractive interactions

57

3.1 3.2 3.3 3.4

57 59 61 66 66 71 75

Introduction The non-interacting electron gas Interacting electrons, quasiparticles and Fermi-liquids Instability due to attractive interactions 3.4.1 Two electrons with attractive interaction 3.4.2 Phonon-mediated attractive interactions 3.4.3 Reduction of the effective Hamiltonian

The superconducting state – an electronic condensate 4.1 4.2 4.3 4.4 4.5

4.6

4.7

5

Heavy fermion superconductors MgB2 superconductor Summarizing remarks

BCS theory: a magnetic analogue Derivation of the BCS gap equation Transition temperature Tc and the energy gap Generalized gap equation, s-wave and d-wave gaps Quasi-particle tunnelling and the gap 4.5.1 Introductory remarks 4.5.2 The tunnelling principle 4.5.3 Single-particle NIN tunnelling 4.5.4 NIS quasiparticle tunnelling 4.5.5 SIS quasiparticle tunnelling BCS coherence factors versus quasiparticle-effects: ultrasound and NMR 4.6.1 Introductory remarks 4.6.2 Transition rates in ultrasound propagation and NMR 4.6.3 Longitudinal ultrasonic attenuation 4.6.4 Transverse ultrasound 4.6.5 Nuclear magnetic resonance relaxation below Tc The Ginzburg–Landau theory 4.7.1 Some remarks on Landau theory 4.7.2 Ginzburg–Landau theory for superconductors 4.7.3 Flux quantization

79 79 81 87 89 94 94 95 97 99 102 103 103 104 105 108 113 115 115 117 121

Weak Links and Josephson Effects

123

5.1

123 123 125 128 129 131

5.2 5.3

Weak links, pair tunnelling, and Josephson effects 5.1.1 Introductory remarks 5.1.2 DC Josephson effect: the Feynman approach AC Josephson effect 5.2.1 Alternative derivation of the AC Josephson effect Josephson current in a magnetic field

CONTENTS

5.4 5.5 5.6 5.7 5.8 6

London Approximation to Ginzburg–Landau Theory (|ψ| constant) 6.1

6.2

6.3 6.4 6.5 6.6 6.7

7

The London equation and the penetration depth λL 6.1.1 Early electrodynamics and the London hypothesis 6.1.2 Derivation of the London equation from the free energy The energy of a single flux line 6.2.1 Energy of a flux line: alternative derivation. An exercise Interacting flux lines: the energy of an arbitrary flux line lattice Self energy of a single straight flux line in the London approximation Interaction between two parallel flux lines Interaction between two flux lines at angle α General flux-line lattice elastic matrix in the London approximation

Applications of Ginzburg–Landau Theory (|ψ| spatially varying) 7.1 7.2 7.3 7.4 7.5

7.6 7.7 8

The SQUID principle The Ferrell–Prange equation The critical field Hc1 of a Josephson junction Josephson vortex dynamics Josephson plasma in cuprate high-Tc superconductors

The temperature-dependent order parameter |ψ(T )| The coherence length ξ 7.2.1 Relations between λ, ξ and Hc Two types of superconductors The structure of the vortex core The length ξ and the upper critical field Bc2 7.5.1 Isotropic systems 7.5.2 Bc2 , ξ , and λ in anisotropic superconductors Ginzburg–Landau–Abrikosov (GLA) predictions for Bc2 /Bc1 Surface superconductivity and Bc3

vii 134 136 138 139 140

141 141 141 146 148 151 154 160 162 164 166

171 171 172 174 175 180 182 182 184 188 190

More on the Flux-line System

199

8.1

199 199 200 201

8.2

Elementary pinning forces and simple models 8.1.1 The concept of a pinning force 8.1.2 Pinning force and flux gradient Critical state and the Bean model

viii

CONTENTS

8.3

8.4 8.5

8.6

8.7

II 9

Flux-line dynamics, thermal effects, depinning, creep and flow 8.3.1 TAFF, flow and creep: Definitions 8.3.2 Flux flow 8.3.3 Thermally activated flux creep: Anderson model Single particle TAFF FLL elasticity and pinning 8.5.1 Collective effects 8.5.2 Collective creep: inverse power law U (J ) 8.5.3 Logarithmic U (J ) 8.5.4 The vortex solid–liquid transition 8.5.5 Lindemann criterion and melting of a clean flux-line system 8.5.6 Modelling non-linear vortex diffusion Flux-line entry at Bc1 : thermodynamic and geometric restrictions 8.6.1 The critical field Bc1 8.6.2 The Bean–Livingston barrier 8.6.3 Geometric barriers Critical current issues 8.7.1 Critical current in the Meissner state 8.7.2 Depairing critical current 8.7.3 Reduction of Jc at grain boundaries 8.7.4 Relaxation of magnetic moment and the irreversibility line 8.7.5 How can Jc be increased?

204 204 205 206 207 208 208 212 213 215 218 224 228 228 229 232 233 233 234 235 236 242

ADVANCED TOPICS

247

Two-dimensional superconductivity. Vortex-pair unbinding

249

9.1 9.2 9.3 9.4 9.5 9.6 9.7

249 250 251 255 257 264 271

Introduction Ginzburg–Landau description Critical fluctuations in two-dimensional superfluids Vortex–antivortex pairs Mapping to the 2D Coulomb gas Vortex-pair unbinding and Kosterlitz–Thouless transition Jump in superfluid density

10 Dual description of the superconducting phase transition 10.1 10.2

Introduction Lattice formulation of the Ginzburg–Landau theory 10.2.1 Lattice Ginzburg–Landau model in a frozen gauge approximation

279 279 282 284

CONTENTS

10.3 10.4 10.5 10.6 10.7 10.8

Preliminary results Vortex-loops as topological defects of the order parameter Superconductor–superfluid duality in d = 3 Zero-field vortex-loop blowout 10.6.1 Definitions Fractal dimension of a vortex-loop tangle Type I versus type II, briefly revisited

III SELECTED APPLICATIONS

ix 286 289 295 298 299 306 309

315

11 Small scale applications 11.1 More JJ-junction and SQUID basics 11.1.1 Introductory remarks 11.1.2 RSJ – the resistively shunted Josephson junction 11.1.3 Further modelling of the Josephson junction 11.1.4 The autonomous DC SQUID 11.1.5 Simplified model of the DC SQUID 11.2 SQUID applications 11.2.1 Biomagnetism: neuromagnetic applications 11.3 Superconducting electrodynamics in the two-fluid model 11.3.1 Frequency dependent conductivity in the two fluid model 11.3.2 Surface impedance and AC loss 11.3.3 Surface resistance measurement 11.4 High-frequency radio technology 11.4.1 Microstrip filters and delay lines 11.4.2 Superconducting high-frequency devices

317 318 318 318 322 323 325 329 329 333 333 336 339 341 341 345

12 Superconducting Wire and Cable Technology 12.1 Low-Tc wire and cable 12.1.1 Introductory remarks 12.1.2 General design considerations 12.1.3 Basic superconductor properties 12.1.4 Design of technical superconductors 12.1.5 Stabilization 12.1.6 AC losses 12.1.7 Mechanical characteristics 12.1.8 Fabrication technology 12.2 High-Tc wire and cable 12.2.1 High-Tc wire and tape 12.2.2 Full-scale high-Tc cable 12.2.3 HTS induction heater 12.3 Magnet technology

349 349 349 350 350 353 355 358 359 359 362 362 363 364 366

x

CONTENTS

IV TOPICAL CONTRIBUTIONS 13 Topical Contributions 13.1 Spin-Triplet superconductivity, by Y. Maeno 13.2 π -SQUIDs – realization and properties, by J. Mannhart 13.3 Doppler effect and the thermal Hall conductivity of quasiparticles in d-wave superconductors, by N.P. Ong 13.4 Nanometer-sized defects responsible for strong flux pinning in NEG123 superconductor at 77 K, by M. Muralidhar and M. Murakami 13.5 Hybrid Magnets, by H. Schneider-Muntau 13.6 Magneto-Optical Imaging of Vortex Matter, by T.H. Johansen 13.7 Vortices seen by scanning tunneling spectroscopy, by Oystein Fischer 13.8 Resistivity in Vortex State in High-Tc Superconductors, by K. Kadowaki 13.9 Coated conductors: a developing application of high temperature superconductivity, by James R. Thompson, and David K. Christen References Chapter 13

V

HISTORICAL NOTES

369 371 371 374 376

378 380 385 388 392

395 397

399

14 Historical notes on superconductivity: the Nobel laureates Heike Kamerlingh Onnes John Bardeen Leon N. Cooper J. Robert Schrieffer Ivar Giaever Brian D. Josephson J. George Bednorz K. Alex M¨uller Alexei A. Abrikosov Vitaly L. Ginzburg Pierre-Gilles de Gennes Philip W. Anderson

401 401 402 403 404 405 407 408 410 411 413 414 415

References

417

Author index

423

Subject index

425

Preface Writing this textbook was motivated by the opinion of the authors that the time has come for an updated look at the basics of superconductivity in the aftermath of progress during the last couple of decades, both through the discoveries of new superconductors, and the ensuing theoretical development. High-Tc superconductor research since 1986 represents an almost unlimited source of information about superconductivity. This is an advantage in the sense that there is ample material with which to fill new books, but a disadvantage in the sense that only a very small fraction of all the efforts that were made, and the results that came out, can be discussed here. In this sense the situation is entirely new: The older texts, like those of de Gennes and Tinkham could discuss or refer to almost all aspects of superconductivity of importance in the 1960s and 1970s. With tens of thousands of papers published after 1986, there is no possibility to take such an approach any more. We apologize to the numerous researchers in the field whose work we could not mention. This situation leaves it even more to the taste of the authors to choose. First and foremost we have wanted to review the basics of superconductivity to new students in the field. Secondly, we wanted to allow those who take a serious interest in the subject at the PhD level, to follow the ideas to old heights like in the BCS theory, or to new heights like in the theory of the vortex system in high-Tc cuprates. Superconductivity is now a far richer subject thanks to the discovery of high-Tc cuprates by Bednorz and M¨uller. Suddenly, superconductivity became an arena for the study of critical behaviour in three-dimensional superconductors, an unthinkable situation in the low-Tc era. Our book seeks, among other things, to clarify this new aspect of superconductivity. In addition, we wanted to respect the wish of students to learn where physics meets the real life of applications. We have concentrated the material here to the central topics, basically how to describe and exploit the properties of Josephson junctions on the small scale, and on the large scale to give some insight into the makings of wires and cables. A special feature of this book is the inclusion of a chapter containing Topical Contributions from distinguished scientists in various areas of superconductivity research and development, from the smallest to the largest scale. Each of these scientists were invited to contribute their leading edge knowledge to give a clear idea of

xii

PREFACE

the state of the art in several important sub-fields as of September 2003 when the writing of this book came to a conclusion. Kristian Fossheim National High Magnetic Field Laboratory, Tallahassee, Florida and The Norwegian University of Science and Technology Trondheim, Norway Asle Sudbø The Norwegian University of Science and Technology Trondheim, Norway

Acknowledgements From Kristian Fossheim: My part of the writing was done in about equal parts during a sabbatical at the National High Magnetic Field Laboratory (NHMFL) at Florida State University, in Tallahassee, Florida during the academic year 2000/2001, and upon my return to Trondheim, Norway, at the Physics Department of the Norwegian University of Science and Technology (NTNU). I greatfully acknowledge the warm hospitality of the NHMFL, and in particular Jack Crow, Director, and Hans Schneider-Muntau, Deputy Director of the NHMFL. I also wish to express my thanks to my wife Elsa for her patience and her willingness to type, from day to day, my handwritten notes during our stay in Tallahassee. I also thank the Physics Department of NTNU, Trondheim for relieving me of some of my teaching duties during one semester of writing. In this book we also wanted to make Nobel laureates in the field more visible to the students, as human beings, and not just as scientific references. I therefore visited ten laureates, videotaping interviews with them. I want to thank them for the friendliness with which they all met me. It gave me some of the best moments of my scientific life to meet these great scientists and fine individuals in their own settings, and hear their own story told. In the Historical Notes, Chapter 14 a few and brief references to these encounters are mentioned. The rest of the material will have to be presented elsewhere. I also want to thank Ulrik Thisted, my PhD student who undertook the task of weeding out the mistakes in my drafts, and Torbjørn Hergum for various assistance, in particular for drawing the major part of the figures. I dedicate this book to the memory of my parents, Nikolina and Øyvind Fossheim. From Asle Sudbø : I thank the Department of Physics at the California Institute of Technology, and in particular Professor Nai-Chang Yeh, for warm hospitality during the initial stages of this project in the autumn of 2000, which I had the privilege of spending at CalTech on sabbatical leave. It gave me an opportunity to try out part of the material in this textbook on some of the brightest students one can possibly have. I also thank Professor Hagen Kleinert and the Department of Theoretical Physics at the Freie Universit¨at Berlin for their hospitality during 4 months of 2001, where part of the writing was completed. I also want to thank Dr Anh Kiet Nguyen, Dr Joakim Hove, and Dr Sjur Mo for several helpful suggestions and for making some of the material in their PhD theses available to me for this book. Having them as graduate students was truly a pleasure and

xiv

ACKNOWLEDGEMENTS

a privilege. Finally, I want to express my sincere thanks to Professor Zlatko Tesanovic, for the innumerable and inspiring discussions I have had with him over the years on the physics of strongly correlated systems. I dedicate this book to the memory of my good friend Anthony Houghton. The authors would like to extend their special thanks to scientific colleagues in the US, Europe and Japan for their topical contributions in Chapter 13: D. K. Christen, Ø. Fischer, T.H. Johansen, K. Kadowaki, Y. Maeno, J. Mannhart, M. Murakami, M. Muralidhar, N. P. Ong, H. Schneider-Muntau and J. R. Thompson.

PART I

Basic Topics

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

1 What is Superconductivity? A Brief Overview 1.1 Some introductory, historical remarks Progress in science in general, and in physics in particular, is characterized by many great discoveries both in theory and experiment. On superficial observation these sudden advances may look like a series of accidental occurrences. But in most cases such an impression would be wrong, in many cases even totally misleading. Very often discoveries occur when the time is ripe, i.e. when certain preconditions have been met, such as adequate technical capability, or attainment of a necessary intellectual and theoretical level. The discovery of superconductivity – the property of certain conductors to display zero DC electrical resistance – by Heike Kamerlingh Onnes and co-workers in 1911 illustrates the point [1]. It was a true discovery, and indeed a remarkable one, because there were no valid arguments around to predict such a phenomenon. Yet, to draw the conclusion that it was accidental would be unjustified. The necessary technical basis and opportunity for the discovery had been solidly established in the same group by the liquefaction of the inert gas helium in 1908. And research, both experimental and theoretical, on the electrical conductivity of metals at temperatures approaching the absolute zero, was ongoing and considered an important issue by leading physicists. They were even puzzled by an apparent similarity between the temperature dependences of electrical conductivity and heat capacity in metals. On travelling down the infinite road towards zero degrees Kelvin, new discoveries could and should be expected, since temperature is the most universal variable by which the (equilibrium) state of matter is defined. In fact, the absence of discoveries along this route should have been the real surprise. Even the cryogen itself, liquid helium, was later to offer a number of opportunities for important discovery. And many more were to come in other condensed matter systems below ambient temperatures. Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

4

WHAT IS SUPERCONDUCTIVITY?

Even the choice by Onnes of the metal to study, mercury, while appearing perhaps surprising today, was a judicial and natural one at that time: It was the metal that offered the most ideal conditions for the study of intrinsic properties of metals at low temperatures due to the purity at which it could be obtained. Purity was indeed a valid consideration, and would be even today, when studying electrical conductivity versus temperature. Research in the Leiden laboratory was carried out by coworkers and students of Onnes in a strictly systematic manner. Metal upon metal was measured, and the results contemplated. Gold was found to have almost immeasurably low resistance in the liquid helium range; but mercury became the first substance found to be superconducting, at a temperature near 4 K. The distinctive feature was a sudden drop of resistance by several orders of magnitude on lowering the temperature below what appeared to be a sharply defined temperature. Lead and tin were soon added to the list. Onnes dismissed the prevailing idea that electrons would ‘freeze to the atom’, and surmised instead that ‘the free electrons would remain free’ while the ‘vibrators’ (atoms) would become ‘practically immovable’1 . The timeliness of their research is also illustrated by the fact that thermal properties were much in focus, thanks to the blackbody problem, the early quantum theory of Planck, and the attempts by Einstein and others to explain low-temperature heat capacity, as well as by ongoing research on thermal and electrical conductivity of solids at lowtemperatures. The electron, a relatively recent discovery, had brought electrical phenomena to the forefront of research. The fact that the atomic nucleus was discovered that same year, 1911, makes this a truly remarkable year in the history of scientific discovery. The Leiden group attached considerable hope to the technological potential of superconducting coils for generation of magnetic field, foreseeing fields as high as 10 T. But they soon found an unexpected obstacle: An upper limit for current that would flow at zero resistance in lead or tin superconductors in the self field of the coil, what we today call the critical current Ic . This difficulty could not be circumvented until decades later, when it was realized, first through theoretical work, that a different kind of superconductor was needed. This new class of superconductors was to be labeled ‘type II’ as opposed to type I for Sn and Pb and similar conductors which had been studied in Leiden. Only upon discovering, understanding, and further developing type II materials could critical current density be raised to much higher, practical values. From the 1960s on a gradual development of superconductor technology has taken place, until today when superconducting magnets are commonplace in laboratories and hospitals all over the industrialized world. And the remarkable SQUID technology developed for measurement of small magnetic fields, has taken on a wide range of applications, and is showing promise in ever new fields by use of both old and new superconductors. 1 For

an account of early work on superconductivity, see Dahl [2].

SOME INTRODUCTORY, HISTORICAL REMARKS

5

Other great discoveries were to follow. The magnetic properties of superconductors attracted considerable attention through the 1920s and 1930s. A breakthrough came in 1933 when Meissner and Ochsenfeld [3] showed that in magnetic fields below a certain threshold value the flux inside the superconductor was expelled, and that this defined a new thermodynamic state and was not a consequence of infinite conductivity. The phenomenon became known as the Meissner effect, and laid the foundation for a thermodynamic treatment of superconductivity, later to be expanded when Abrikosov [4, 5] was finally permitted to report his theory of the magnetic properties of superconductors at a meeting in Moscow in 1957. That same year Schubnikow’s [6] important experimental work from the 1930s could also finally be recognized publicly and posthumously in the Soviet Union. This work had already established important magnetic properties of type II superconductors two decades earlier, and had shown promise for superconductors to carry larger current densities than materials previously studied by Onnes, and by Meissner and others. 1957 was also the year when the beautiful quantum theory, known as the BCS theory, was published by Bardeen, Cooper and Schrieffer [7], finally explaining the fascinating properties of superconductors from first principles. It had taken 46 years from the time of the discovery. A few years later Josephson’s [8] astonishing predictions regarding the physical properties of inhomogeneous superconductors were announced, soon followed by experimental verifications, and by a variety of applications as well as further theoretical development. It would take another 25 years before superconductivity made the transition from being mainly an exotic laboratory phenomenon, known mostly to physicists, to become almost a household word. That development was to take place by the discovery of a new class of superconductors, known as high-Tc cuprates, by Bednorz and M¨uller [9] at the IBM laboratory in R¨uschlikon near Z¨urich in 1986. This is an example of a great discovery made on the basis of systematic, goal oriented research. From then on the world outside of physics became fully aware of the almost magical properties of superconductors. The discovery started a race towards applications that is still ongoing, with great economic prospects. Equally intense was the desire to understand the mechanism. At the time of writing this book, that goal has not yet been reached. In the meantime, research has benefited greatly from the famous semi-phenomenological theories of the London brothers from the 1930s, and of Ginzburg and Landau [10] published in 1950, in particular. It has been estimated that well over 50 000 scientific papers have been published on superconductivity since the high-Tc discovery in 1986. A single book can only give a modest insight into this vast amount of knowledge and results. The present one aims to shed light on what the authors regard as the most central issues, with special emphasis on developments taken place during the last 15–20 years.

6

1.2

WHAT IS SUPERCONDUCTIVITY?

Resistivity

Two fundamentally important and intuitively startling properties are associated with superconductivity: • The transition from finite resistivity, ρn in the normal state above a superconducting transition temperature Tc , to ρ = 0, i.e. perfect DC conductivity, σ = ∞, below Tc . • The simultaneous change of magnetic susceptibility χ from a small positive paramagnetic value above Tc to χ = −1, i.e. perfect diamagnetism below Tc . These aspects are qualitatively illustrated in Figure 1.1. Actual measurements of resistivity as a function of temperature in a high-temperature superconducting material are shown in Figure 1.2. We shall return to the second of the above statements in Section 1.3. Let us now discuss the implications of the first statement. The traditional way to measure resistance is by balancing a Wheatstone bridge, using the sample as the fourth and unknown resistance. When balanced, the precision of the measurement is as good as that of the resistors used in the circuit, or possibly limited by the zero-readout accuracy of the galvanometer used in balancing the bridge. There is a limit to how low resistance one can claim to measure: Zero resistance is not accessible to direct measurement. By standard methods we can measure a reduction in resistance by many orders of magnitude, but we can never measure zero resistance in a strict sense. If we try to measure the inverse quantity, i.e. conductivity σ = 1/ρ, the impossibility

Superconductor r=0

0

Tc Temperature T

Susceptibility c(T)

Resistivity r(T )

Non-superconductor 0

−1

0

Tc Temperature T

Figure 1.1 Sketches of the two basic characteristics of a superconductor: The left figure shows the drop to zero resistivity, ρ = 0, at a temperature Tc , compared to a nonsuperconducting behavior. The right hand figure shows the corresponding drop in susceptibility to the ideal diamagnetic value of χ = −1 below Tc . The onset of the diamagnetic response corresponds quite closely to the point where ρ → 0 on the temperature axis. The figure also indicates that χ is positive but quite small above Tc .

RESISTIVITY

7

800

Resistance R(mΩ)

Tl-Ba-Ca-Cu-O 600 Superconducting phase

400

Normal phase

200 r=0 0

0

100

200

300

Tc Temperature T(K)

Figure 1.2 Experimental data on the resistance of a Tl-Ba-Ca-Cu-O ceramic sample from the early days (1988) of high-Tc discovery (unpublished data from the Trondheim group). As was often the case during the early days the material was not of precisely determined composition. The value of Tc indicates that the material was close to Tl2 Ba2 Ca2 Cu3 O10 composition.

remains. No method is available to measure an infinite quantity. For the discoverers of superconductivity this was a real dilemma. Kamerlingh Onnes held on to the belief that a ‘micro-resistance’ remained below Tc . It is, however, still possible to arrive at the reasonable conclusion ρ → 0, or equivalently σ → ∞, by inference from real measurements. Experiments have been devised for this purpose. In such experiments the magnetic field associated with an induced current has been found to remain constant during a time span as long as 1 year. This allows an estimate to be made of the lower bound of the decay constant, and of the upper bound of the resistance. The resulting analysis of such a measurement leads to the conclusion that the lower bound on the decay constant τ for the current in the superconductor is of the order of 100 000 years, implying that the total time for the current to die out completely would be millions of years. Let us see how such an estimate can be made. To be specific, we assume that a current I0 is set up by induction in a superconducting closed loop at time t = 0, at a temperature below Tc . Next, the associated magnetic field is monitored over a very long period of time over some area in the loop, as illustrated in Figure 1.3. As long as a resistance R exists in the superconducting loop, with inductance L in the presence of a current I = I (t), conservation of energy requires d 1 2 LI + RI 2 = 0 (1.1) dt 2 with the well-known solution

I (t) = I0 e−(R/L)t

(1.2)

8

WHAT IS SUPERCONDUCTIVITY?

a

B r

I(t)

V

I

R, L

Figure 1.3 Sketch of a simple setup to monitor the possible decay of current I (t) via its associated magnetic induction B(t) in a closed loop of inductance L and resistance R. The wire has a diameter a and a loop radius r. The field B is normal to the loop area. The magnetic sensor is a Hall probe.

where I0 was the initial current at time t = 0. The decay time of the current, as well as of the corresponding magnetic induction B, is τ = L/R. Now, if the B-field surrounding the loop is measured to be the same after a time t1 , say 1 year later, it appears to mean that I (t1 = 1 year) = I (t = 0) = I0 , and similarly for the corresponding B-field. However, this statement is not an exact one. The B-field we measure, resulting from the current I (t), can only be measured with a certain accuracy, determined by the instruments used. If we assume that the change of B-field can be detected with a relative instrumental resolution δB/B0 = 10−5 , an observation of ‘no change’ in reality only sets an upper bound on the possible decay δI of current and of field δB that may have occurred. What the measurement can determine is therefore only the maximum amounts by which the current I and the field B may have decayed. In reality the decay may have been much lower. Hence we can estimate

and

δI > I0 − I (t1 ) = I 0 (1 − e−(R/L)t1 )

(1.3)

δB > B0 − B(t1 ) = B0 (1 − e−(R/L)t1 ).

(1.4)

From this it follows that δI δB = > 1 − e−(R/L)t1 I0 B0 Solving for R, we find its upper bound δB δI L L = − ln 1 − R < − ln 1 − t1 B0 t1 I0 where all quantities on the right can be determined from the experiment.

(1.5)

(1.6)

RESISTIVITY

9

If we assume that we have used a single-loop inductor with a diameter a and loop radius r, and use the inductance formula for a single loop which applies for r a: L ≈ µ0 r ln(r/a), we find the expression for the upper bound on R as µ0 r ln(r/a) δB R 5.8 × 1013 s. Because 1 year is close to 3 × 107 s, the lower bound on the decay time is about 2 million years. This is a factor of 10 longer than the observations referred to above, so we were a bit generous. But we have to remember that the real observation was of no change. The instruments are the limitation, and we may not have overestimated the actual decay time at all. On the contrary, it might have been found to be much longer had instruments with higher resolution been used. The quest for an even better experimental verification of ρ = 0 in the superconducting state could be continued. If we had used a SQUID superconducting detector of the magnetic field (see Chapters 5 and 11), the detection limit for the small changes in magnetic field would be lowered by several orders of magnitude more, and the upper bound on resistance and resistivity might have been lowered correspondingly. The lower bound on the decay time τ = L/R would then be raised by many orders of magnitude above 1013 s that we have found so far. τ might even approach the lifetime of the Universe. This would be in accordance

10

WHAT IS SUPERCONDUCTIVITY?

with theoretical arguments in ideal situations. What better measure could we ask for to conclude that zero resistivity is physically possible? Having satisfied ourselves that ρ = 0 is an appropriate statement about the electrical resistivity in a superconductor, we must immediately caution against one particular misinterpretation: We have to keep in mind that this state of affairs only applies to DC resistivity. An applied AC electric field accelerates charge. We cannot avoid continually transferring energy to the electron system as long as we keep accelerating it, i.e. as long as we expose it to an AC electric field. We shall return to this question in detail in Chapter 11, and find that the resistance increases with the square of the frequency, but with a very small prefactor. Consequently, there is no abrupt change from DC to the AC resistivity in the superconducting state as we start increasing the frequency from zero. This loss becomes important only at very high frequencies. Still, because of the fact that in the actual technical construction of superconducting cables, normal metals unavoidably have to be used as part of the whole structure, there are losses, so-called coupling losses in the normal metal surrounding the superconductor even at standard electric grid frequencies, i.e. at 50 Hz or 60 Hz. In addition, losses caused by displacement of supercurrent vortices in a magnetic field are important in such cases, even in DC situations. These questions are treated in Chapters 8 and 12. That supercurrents in ideal situations can run without observable loss for years, indeed perhaps much more than 106 years as we found previously, is one of Nature’s most fascinating phenomena. It contradicts all experiences we have from physical systems in the macroscopic world, because it implies frictionless or lossless motion of matter, in this case charged matter, which is displaced relative to the ions. A classic analogue to electronic supercurrent transport in an electrical circuit could be that of sliding a pebble along a flat, icy surface. The pebble soon comes to rest because it spends all its energy working against friction. However, in the superconducting circuit the charged particles (current) continue to run, hence there is no friction. It is precisely because this situation is so contrary to all our experience with other real systems that superconductivity is such a startling and counterintuitive phenomenon. In fact, as we shall see, superconductivity is a pure quantum physics phenomenon on a macroscopic scale. Superconductivity has an additional property compared to the lossless motion of charged particles in atoms, namely phase coherence of the manybody wavefunction. Indeed one of the most remarkable feats of science was the development of a manybody quantum theory that finally explained superconductivity, and with predictive power.

1.3

The Meissner effect: perfect diamagnetism

From the discovery of zero electrical resistivity by Onnes in 1911, 22 years would pass until the next important discovery by Meissner and Ochsenfeld.

THE MEISSNER EFFECT: PERFECT DIAMAGNETISM

11

They found that the superconducting state possesses a second characteristic, defining property – perfect diamagnetism. Prior to this discovery there had been considerable debate regarding the magnetic properties, and the discussion had been based on an interpretation of the superconducting state with perfect conductivity as the (only) basic characteristic. Meissner and Ochsenfeld managed to escape this conceptual trap by observing that a magnetic field, which was applied above Tc would be expelled from the body of the superconductor on cooling below Tc , leading to B = 0 inside. Using the constitutive equation for a magnetic body we therefore have to write, in the superconducting state: B = µ0 (H + M) = 0

(1.9)

which means that in the superconductor M = −H.

(1.10)

Therefore, the susceptibility takes on the ideal value for a perfect diamagnet: χ=

dM = −1. dH

(1.11)

Because permeability is κ = 1 + χ we also have κ = 0 below Tc . These two ways of expressing the Meissner effect are of course equivalent, but the diamagnetic statement χ = −1 is perhaps physically more ‘descriptive’ and appealing. What happens is that shielding currents arise in the superconductor surface. These currents create a field both inside and outside the superconductor such that on the inside the applied and the induced fields exactly cancel, while outside they add. The result is that we observe expulsion of the B-field: zero B-field inside, and an increased field near the sample, on the outside. This is illustrated in Figure 1.4. While in the normal state Faraday lines would pass straight through the metal, practically as if there was only vacuum, in the superconducting Meissner state all lines are forced to pass on the outside. The highest H

B≠0

T > Tc c 0; k≈1 NORMAL

H

Cooling

B=0

T < Tc c = −1; k = 0 SUPERCONDUCTING

Figure 1.4 The Meissner effect in a superconductor.

12

WHAT IS SUPERCONDUCTIVITY?

density of flux lines is found near the equator, while near the poles there is a lower flux density than before the flux expulsion. That this situation represents a thermodynamic state is demonstrated by the experimental observation that the state is uniquely defined by the values of the thermodynamic variables, temperature T and applied field H , independent of how that state was reached. It is important in this context to observe that this is not possible if perfect conductivity was the only special property that the superconductor attained on passing below Tc . This can be confirmed by a simple thought experiment, as in the two sequences illustrated in Figure 1.5. Imagine (i) that a specimen which is originally at room temperature, is cooled in zero applied field to below a temperature Tc where it acquires zero resistance, ρ = 0. Now turn on an external magnetic field. Lenz’ law requires currents to arise in the specimen so as to screen out the applied field. As ρ = 0 this situation will persist forever, and no field will penetrate. Let us call this state I. Next, remove the field. Because the prevailing requirement from Lenz’ law is to allow no change of flux in the specimen, the currents in the sample will diminish to zero as the field is turned off. At the end of the sequence the sample is still free of magnetic flux inside. Call this state II. In the next sequence, (ii), start the experiment at room temperature, this time in an applied external field. This field penetrates the sample completely and almost totally undistorted due to the low paramagnetism of nonmagnetic metals. Now cool the specimen in the magnetic field to below the same temperature Tc as before. Although the sample, by assumption, acquired ρ = 0 on

Cooling

(a) Ha = 0; T > Tc

(b) Ha = 0; T < Tc

(d) Ha = 0; T < Tc (c) Ha > 0; T < Tc

Cooling

(e) Ha > 0; T > Tc

(f) Ha > 0; T < Tc

(g) Ha = 0; T < Tc

Figure 1.5 Cooling a hypothetical normal conductor with infinite conductivity in zero external field, and in a finite field, and comparing the resulting states of the material. The figure is explained in the text, and important conclusions are drawn from that discussion.

TYPE I AND TYPE II SUPERCONDUCTORS

13

passing through Tc , Lenz’ law requires the flux inside to remain perfectly constant. Call this state III. Next, remove the external field. Again Lenz’ law requires the flux to stay constant. This can indeed be implemented by a spontaneous current arising on the surface. Since by assumption ρ = 0, the situation will persist forever. Call this state IV. Now compare, in particular, state II and state IV. The thermodynamic variables T and H are the same, but the states are quite different as just described. The difference was unavoidable due to the assumption that the only new property that the specimen acquired on passing below Tc was perfect conductivity. However, on exposing real superconductors to precisely the same sequences the superconductor ends up in exactly the same state, namely one of total flux expulsion in both cases, and again the situation is persistent. We have two important conclusions to draw from these observations: • Superconductivity is more than just ρ = 0. • Superconductivity is a thermodynamic state, contrary to a state characterized by just ρ = 0. What happens in the Meissner effect is that spontaneous currents arise in the surface to exactly cancel the B-field inside. Diamagnetism is well known to exist in all matter, but usually the corresponding susceptibility is very small, typically χ = −10−6 in atomic and molecular diamagnetism. Perfect diamagnetism clearly is a totally different phenomenon. The reason for the large negative value is precisely the fact that currents encompass the entire body, and are not broken up into tiny currents circulating individual atoms. We might add that diamagnetism exists in metals in the normal state too, due to surface currents in a magnetic field. But this effect is more than overcome by the paramagnetism of the conduction electrons. In the discussions of the superconducting state we have so far assumed that currents and fields employed were below the threshold where superconductivity breaks down. In Chapter 8 we discuss the limits as to how large currents and fields a superconductor can tolerate before being forced to allow magnetic flux to penetrate. As long as the superconductor is at a field below such values, and χ = −1 is maintained, we say that the superconductor is in the Meissner state, or Meissner phase, as shown in Figure 1.6. These remarks point to the need of defining more precisely the thermodynamic range of superconductivity in the (H, T )-plane. This has been well established for a great number of metals and alloys, as well as high-Tc and other classes of superconductors. We return to this problem in the next section.

1.4 Type I and type II superconductors Superconducting materials have the ability, as we have seen, to exist either in the normal state or the superconducting state, depending on the external

14

WHAT IS SUPERCONDUCTIVITY? H Hc(0) NORMAL

Meissner phase SUPERCONDUCTING Tc

T

Figure 1.6 The Meissner phase of a superconductor. Under the curve, in the shaded area, the material is perfectly screened against an external magnetic field.

magnetic field they experience. It turns out that if we increase the magnetic field beyond a certain critical value Hc or Hc1 , which is different for different materials, the Meissner effect breaks down. That is to say, flux penetrates into the material. A sketch is shown in Figure 1.7. This figure shows the negative of the magnetization along the positive vertical axis. The slope of the line from the origin is then exactly 1 as long as the sample is in the Meissner state, corresponding to χ = −1. Let us here first discuss the ideal case which best brings out the underlying physics: Imagine we study a long, thin needlelike specimen, with the applied field parallel to its axis, in which case the demagnetization factor n = 0.2 A pickup coil can be used to measure the amount H Type I

Type II

Magnetization – M

I n≈0 ∆I ∝ ∆M

SM 0

N Hc (a)

SV

SM 0 Applied field H

Hc1

N Hc2

(b)

Figure 1.7 (a) shows the typical behaviour of a type I superconductor which switches abruptly from the Meissner state SM to the normal state N at Hc . (b) shows a different behaviour in a type II superconductor: At a lower critical field Hc1 the superconductor changes state from the Meissner state with complete screening, SM , to a state of vortex line penetration SV , and finally, at Hc2 , to the normal state N. The insert indicates that the magnetization development can be monitored by a coil around the rod-like sample (demagnetization factor n ≈ 0) such that the change of current I is proportional to the change of magnetization M. 2 We

refer to Section 1.7 for a discussion of demagnetization factors.

TYPE I AND TYPE II SUPERCONDUCTORS

15

of flux which penetrates the sample. Now turn on a magnetic field. At low fields the Meissner state, corresponding to complete screening, is found. But as the field increases further we will discover two distinctly different outcomes, depending on the materials we investigate. This will allow us to sort all known superconductors into two categories as follows: • Type I: The superconductor switches abruptly over from the Meissner state to one of full penetration of magnetic flux, the normal state, at a well-defined critical field, Hc . Examples of such materials are Hg, Al, Sn, In. Figure 1.7a shows a sketch of this behaviour. The ideal behaviour is only observed when n = 0. • Type II: The superconductor switches from the Meissner state to a state of partial penetration of magnetic flux, the mixed state, at a critical field Hc1 . Thereafter it crosses over continuously to full flux penetration, the normal state, at an upper field Hc2 . Examples: Nb3 Sn, NbTi, and all high-Tc cuprates. Figures 1.7b and Figure 1.8b illustrate this behaviour. The distinction between type I and type II turns out to be so important that hereafter we shall think of every superconductor we encounter as belonging to one class or the other. Several chapters of this book are occupied with aspects

Type II n ≠ 0: FILM

Type I n ≠ 0: DISC

a(H)

H

H

n=0

−M

Φ0 =

h 2e

−M

n≠0 Hc (a)

H

Hc1

Hc2

H

(b)

Figure 1.8 Illustration of flux penetration in cases when the demagnetization factor n = 0. In the (a) upper part, normal lamina penetrate the disc from the periphery when n = h arrange 0. In (b) vortices with flux lines carrying an elementary amount of flux 0 = 2e themselves in a hexagonal pattern in a field normal to a type II film. In the case of type I the laminar penetration is seen only when n = 0. When n = 0 the transition from the Meissner state to the normal state is abrupt, no lamina appear. In the case of type II superconductor the observed mixed state behaviour is inherent to the material, irrespective of the value of n.

16

WHAT IS SUPERCONDUCTIVITY?

related to their distinction, which turns out to be essential from a practical as well as a theoretical point of view. At this point we will limit the discussion to the descriptive level, and refer the more advanced discussion to later chapters. In order to see another difference between the two types of superconductors, let us relax the requirement on the demagnetization factor, and allow n to be non-zero. This forces flux to penetrate inhomogeneously even into a type I superconductor. Using various techniques to decorate and picture the flux distribution the following facts emerge, as illustrated in Figure 1.8a and b. In type I materials the flux penetrates in the form of continuous lamina, flat or meandering. The lamina are alternating normal and superconducting layers, parallel to the field, whose relative thicknesses depend on both temperature and applied field. The following constraints have been found to apply to these structures: Superconducting lamina are flux-free in a Meissner-like state, while the normal ones contain a magnetic flux density corresponding to the critical field, i.e. Bc = µ0 Hc . The relative thickness of normal and superconducting lamina is fixed by a combination of this fact, and by flux conservation. We refer to Section 7.3 for a further discussion. In type II materials, on the contrary, flux penetrates in tiny, precisely quanh tized units of flux 0 = 2e where h is Planck’s constant, and e is the magnitude of electronic charge. We call these objects flux lines or vortex lines, a distinction in terminology which will be made clear in the next Section. The density of such flux lines increases with increasing applied magnetic field, as is reflected in the M versus H diagram (Figure 1.8b). The magnetic energy density Hc2 /2µ0 required to break down the Meissner state completely at Hc in the type I case, with n = 0, measures directly the stability of the superconducting phase against that of the normal one. Hence this crucial information is obtainable by relatively simple measurements. Hc , it turns out, differs from one material to another, not a surprising fact considering that all metals have different electronic properties, like Fermi surfaces and band structures. If we study flux penetration into specimens of other shapes by allowing n = 0, we will find that when the Meissner state breaks down, the details of how flux penetrates and the precise fields at which it first occurs, and where it is completed, depend on the shape of the specimen due to the demagnetization effects alluded to above. An important point regarding these shape dependent effects is that whenever the demagnetization factor for a chosen combination of geometry and field direction is nonzero, the external field varies along the surface of the specimen. This causes flux to penetrate inhomogeneously whenever n = 0, unlike the case when n = 0. In the former case the transition from the Meissner state to the fully penetrated state is gradual when M versus H is measured even in type I. We underscore again the importance of the fact that partial flux penetration in type I superconductors, often referred to as the intermediate state, is very different from that of the mixed

VORTEX LINES AND FLUX LINES Type I

Type II

Hc Applied field H

17

Hc2 N

N SV Hc1

SM

SM Tc

Tc Temperature T

Figure 1.9 Phase diagram of type I (left) and type II (right). S = superconducting, M = Meissner phase, V = vortex phase, N = normal phase.

phase of type II. It is precisely this difference that makes type II superconductors useful on a large scale, while type I are not. Figure 1.9 illustrates the complete phase diagram for type I and type II superconductors in the H, T − plane.

1.5 Vortex lines and flux lines We want to stress a very important conceptual difference between what we call vortex lines and flux lines. Often, these terms are used interchangeably. This is permissible in most conventional type II superconductors, where the ratio between the upper and lower critical fields Hc2 and Hc1 , is not very large. In the cuprate high-Tc superconductors, however, this ratio is enormous. It then turns out to become important to distinguish between the concepts of flux lines and vortex lines. As already mentioned, Abrikosov predicted the existence of the so-called mixed phase, in what has become known as type II superconductors. The distinguishing characteristic of these, as we have seen, is their ability to allow magnetic field penetration in the form of magnetic vortices of quantized circulation. This cannot happen in type I superconductors. In the centre of each magnetic vortex superconductivity is destroyed, i.e. the density of superconducting electrons is zero, while outside the centre, it is non-zero. Hence, far away from the centre of the vortex the associated magnetic field goes to zero. As we will see in later chapters, the ratio of the penetration depth λ to the length over which a magnetic field destroys superconductivity, ξ , determines the extent to which a superconductor is type I or type II. When the ratio λ/ξ is small it is type I, and when the ratio increases roughly beyond one, the superconductor becomes progressively more type II. This situation is illustrated in Figure 1.10.

18

WHAT IS SUPERCONDUCTIVITY?

B(r) x : |y| < |y0|

l3 r

l2

l1

0

r

Figure 1.10 The parameters ξ of the vortex line and λ of the flux line. As explained in the text, the distinction between the concepts of vortex lines and flux lines becomes increasingly important as λ becomes greater and greater compared to ξ . λ measures the radius of circulation of supercurrent around the vortex core. The wavefunction is severely depressed for r < ξ , and goes to zero on the axis.

Flux lines are tubes of confined magnetic flux. They have a diameter given by the distance with which a magnetic field can penetrate into the superconductor. On the other hand, a vortex line is a line with a diameter given by the distance over which a magnetic field suppresses superconductivity. This length is conceptually different from the magnetic penetration depth. It is then easy to imagine that a thick line with a large diameter has a typical bending length which is much longer than a very thin line. Moderate (conventional) type II superconductors are characterized by the fact that the two length scales described above are roughly equal. In extreme type II superconductors, such as the highTc cuprates, this is not at all the case. The magnetic penetration length, i.e. the diameter of the flux line, is typically 100 times larger than the diameter of the vortex line. Hence, the vortex line resides deep inside the flux line and moreover fluctuates on a vastly different length scale than the flux-line. In essence, they therefore represent different degrees of freedom of the system. This will turn out to be of crucial importance in the theoretical treatment presented in Chapters 9 and 10. In these contexts, therefore, the conceptual distinction between flux lines and vortex lines is essential. In the extreme type II case, where flux lines no longer can be defined, basically being treated as infinitely thick objects, a vortex line is still perfectly well defined.

1.6 Thermodynamics of the superconducting state We have already pointed out that the superconducting state has a limited stability against application of a magnetic field. This became apparent in the discussion of the magnetization diagrams, M(H ), in Section 1.4. The M(H ) diagrams can

THERMODYNAMICS OF THE SUPERCONDUCTING STATE

19

be read as phase diagrams, and hence may be subjected to thermodynamic analysis. A very useful aspect of thermodynamics is as a tool to derive relationships between measurable quantities by analysis of free energies. We will now look into this possibility for superconductors. Let us first recall the so-called thermodynamic square, Figure 1.11, a useful mnemonic device from which one can quickly read out the basic relationships, in this case with respect to magnetic properties, of completely general validity. The starting point is the following square: −m0M

A

G

U S

Figure 1.11

T

E

H

Thermodynamic square.

Here M is magnetization, T is absolute temperature, A is Helmholtz free energy, U is internal energy, G is Gibbs’ energy, S is entropy, E is enthalpy, and H is the applied magnetic field. The idea here is that each free energy should be considered as depending on the two variables next to it. Following the suggestion of the arrows it may be used to read out thermodynamic derivatives. Going in the direction of the arrows generates a positive sign, going in the opposite direction generates a negative sign. Some examples: ∂G = −µ0 M ∂H T ∂G = −S (1.12) ∂T H ∂U =T ∂S M When discussing the superconducting state in an external magnetic field H , and the resulting magnetization, we should use the Gibbs’ energy G, and consider it dependent on T and H . We rewrite the first relation in Eq. 1.12 as dG = −µ0 MdH

(1.13)

This relation applies both in the normal and superconducting state. Next, integrate from zero to Hc at constant T in the superconducting state: 0

Hc

dGs = −µ0

Hc

Ms (T , H ) dH 0

(1.14)

20

WHAT IS SUPERCONDUCTIVITY?

Here M = M(T , H ), but varies only with H as T is constant during the integration. We now consider a type I superconductor. The Meissner state, in which we now carry out the integration, was found in Section 1.3 to be characterized by M = −H . Using this, Eq. 1.14 yields

Hc (T )

dGs = −µ0

0

Hc (T )

(−H )dH =

0

µ0 2 H (T ) 2 c

(1.15)

On the left-hand side we have

Hc

dGs = Gs (T , Hc ) − Gs (T , 0)

(1.16)

µ0 2 H (T ) 2 c

(1.17)

0

The result is: Gs (T , Hc ) − Gs (T , 0) =

We want to calculate the energy difference between the normal and the superconducting states, which addresses the question of stability of the superconducting state. To do that we recall first that χ for a normal metal is small, χ 1. This implies that a normal metal in a field Hc has practically the same Gibbs energy as in zero field. Hence we write Gn (T , Hc ) = Gn (T , 0)

(1.18)

This corresponds to saying that the integral

Hc

dGn = −µ0

0

Hc

Mn dH

(1.19)

0

taken in the normal state can be treated as zero. From the fact that the two phases coexist in the intermediate state of type I, with a field Hc in the normal lamina and zero in the superconducting ones, we conclude that Gn (T , Hc ) = Gs (T , Hc )

(1.20)

Comparing Eqs 1.18 and 1.20 we see that Gn (T , 0) = Gs (T , Hc )

(1.21)

THERMODYNAMICS OF THE SUPERCONDUCTING STATE

21

Putting this back into Eq. 1.17 gives: Gn (T , 0) − Gs (T , 0) =

µ0 2 H (T ) 2 c

(1.22)

The interesting aspect of this relation is that the difference in energy density between the (Gibbs’) energy in normal and superconducting states without a field present can be expressed by the characteristic energy µ20 Hc2 in the simple fashion of Eq. 1.22. From this relationship it becomes clear that Hc2 is in a deeper sense a measure of the ‘condensation energy’ of the Meissner state, or the stability of the Meissner state with respect to the normal one. The energy density is lower in the superconducting state by the amount µ20 Hc2 (T ). Alternatively we can write it as 2µ1 0 Bc2 (T ). We will later discover (Chapter 8) that the condensation energy can be found on a microscopic basis, leading to a relationship between Hc and the superconducting energy gap. It is useful at this point to calculate other thermodynamic aspects of the Meissner phase. Analytically this can be done if we can find an expression for Hc (T ). It turns out that experiments, to a good approximation, give a unanimous 2 answer, which we can use in the further analysis: Hc (T ) = Hc (0) 1 − TTc . This is a simple parabolic shape with the top of the parabola at Hc (0) on the vertical H-axis, and an approximately linear shape where it meets the Taxis. With the important result for the condensation energy and the functional expression for Hc in hand, we choose a relationship from the thermodynamic square, that for entropy: ∂Gs Ss = − (1.23) ∂T H We can now find the entropy change at the phase boundary by taking the temperature derivative of Eq. 1.22 directly and obtain: Sn (T , 0) − Ss (T , 0) = −µ0 Hc

dHc dT

(1.24)

We note here that the quantity −µ0 Hc dHc /dT is always positive, meaning that the entropy in the superconducting state is always lower than in the normal state. Hence, the superconducting state is characterized by greater order than the normal state. An entropy drop at (Tc , Hc ) accompanies the superconducting transition. The exception is when T = Tc , where Hc = 0. We see that in this case Sn = Ss , and there is no entropy drop. At this particular point the entropy is therefore continuous, characteristic of a 2nd order transition. There are two aspects of the superconducting state that show the increased order below Tc indicated by the thermodynamic analysis: Formation of Cooper pairs represent a partial ordering of the electron gas, and the superconducting wavefunction

22

WHAT IS SUPERCONDUCTIVITY?

shows an ordered phase of the wavefunction, or phase coherence. These facts are of course related. Another quantity closely related to entropy is the latent heat. Here we find L = T (Sn − Ss ) = −T µ0 Hc

∂Hc ≥0 ∂T

(1.25)

Again, this is a positive quantity as long as we are considering finite Hc . At Tc , where Hc = 0 we get L = 0, again characteristic of a second order or continuous transition. Finally, let us look at the heat capacity, which from thermodynamics is found by differentiation of the entropy CH ≡ T Taking the 2nd derivative of

µ0 2 2 Hc

∂S ∂T

(1.26) H

we find:

Cs (T ) − Cn (T ) = µ0 T

dHc dT

2

d2 Hc + Hc dT 2

(1.27)

which, at Tc becomes Cs (Tc ) − Cn (Tc ) = µ0 Tc

dHc dT

2 >0

(1.28)

T =Tc

We find a discontinuity at Tc , an upward jump on lowering the temperature through Tc as all quantities in the right-hand side are positive. Experiments have verified this aspect in every case it was measured in the low-Tc superconductors. In high-Tc materials the story is more complicated. There, fluctuations play a dominant role near Tc , and a different description altogether is necessary, as will be discussed in several chapters of this book. The discontinuity found in Eq. 1.28 is characteristic of mean-field theories and mean-field systems. The BCS theory, which eventually explained superconductivity in low-Tc materials, belongs to that class, and reproduces the experimental results nearly perfectly. Figure 1.12 illustrates examples of two different phase transitions. The left figure illustrates the BCS mean-field like behaviour, measured on a low-Tc material. The right figure illustrates the situation in a high-Tc material and shows a completely different form, with no jump, and with fluctuation contributions on both sides of Tc . We shall return to these questions which are of major importance in high-Tc materials, with a ratio λ/ξ 1, the so-called high-κ materials.

DEMAGNETIZATION FACTORS AND SCREENING

High Tc

Specific heat Cp

Low Tc

23

Tc

Tc Temperature T

Figure 1.12 Sketch of typical forms of specific heat curves measured from above the superconducting transition in a mean-field low-Tc metallic superconductor like Al (left), and in a substance with strong superconductivity phase fluctuations like the high-Tc compound YBCO (right).

1.7

Demagnetization factors and screening

When a specimen of ellipsoidal shape is subject to a homogeneous external field along one of its principal axes, it is well-known from magnetostatics (see for instance Jackson, 1975 [11]) that the internal fields B i and H i are both parallel to the applied field B a . The constitutive relation is B i = µH i = µ0 (H i + M) = (1 + χ )µ0 H i

(1.29)

As already discussed, in the Meissner state χ = −1, which leads to B i = 0. These two statements are equivalent, and consistent. For the applied fields we have similarly Ba = µ0 Ha (1.30) provided no magnetized matter is surrounding the magnetized body under study. These relations apply separately inside, and outside the measured body, and do not answer the question: what is the relationship between the applied field H a and the internal field H i ? This is not a trivial question. What complicates the relationship between the applied fields and the internal fields Bi , Hi , Ba , Ha is the so-called demagnetizing field. We refer to standard books on magnetostatics for a discussion of the theory of demagnetization effects. Here we will use the results without derivation. The word ‘demagnetization’ was originally coined for use in ferromagnets. It applies with opposite consequences in superconductors as compared to ferromagnets, but is equally important to consider here due to the fact that magnetization effects and demagnetization are very strong in

24

WHAT IS SUPERCONDUCTIVITY?

superconductors. The reason for this is that in superconductors the susceptibility χ = −1, the ideal and complete diamagnetism. Briefly stated, when a magnetic field H a is applied to a superconductor, the screening currents which appear near the surface, create an additional field in the specimen. This is called the demagnetizing field H D . We now have: Hi = Ha − HD

(1.31)

We will only address situations where the internal field is homogeneous, i.e. cases like those we mentioned in the introductory statement above. With this restriction we can still treat all ellipsoidal shapes. These all have a uniform field inside the body when exposed to a uniform external field. We may then write H D = nM

(1.32)

where n is the (scalar) demagnetizing factor, and M is the uniform magnetization of the body. We now have the relationship H i = H a − nM

(1.33)

In a superconductor M = −H i ; which, upon insertion in Eq. 1.33 leads to the important relationship Hi =

1 Ha 1−n

(1.34)

precisely the relationship which we pointed out was missing previously. To take a concrete example, let us examine the situation when a compact ellipsoidal body of superconductor is placed in an external magnetic field applied along one of the principal axes. At the surface of the superconductor the tangential component of H is continuous. The internal field is now parallel to the applied field which exists everywhere on the circumference of the extremal cross-section of the sample as viewed along the field direction. In case of a spherical body this circumference corresponds to the equatorial circle. This makes the field H a just outside the circumference equal to the field H i just inside. Eq. 1.34 now allows us to calculate the field just inside, and because this equals the field just outside, the field just outside is equal to Ha /(1 − n). We learn from this that a demagnetization factor n < 1 makes the field at the maximum circumference larger than the applied field Ha . Some important examples are the following, illustrated in Figure 1.13: • For a sphere, n = 13 , always giving a tangential field of 32 Ha at the equator. • In case the field is applied normal to a long rod of circular cross-section, n = 12 , and the tangential field is 2Ha .

DEMAGNETIZATION FACTORS AND SCREENING Ha

Ha

Ha

n = 1/3 3 H 2 a

(a)

25

n = 1/2

n=0

2 Ha

(b)

Ha

(c)

Figure 1.13 Demagnetization factors for different geometries with n given for each case. Horizontal arrows indicate the value of applied field at the surface in each case.

• With the field applied along the axis of the long rod, n = 0; no demagnetization occurs. The field along the entire surface of the rod is tangential to the (extremal) crossection, and equal to the applied field Ha . Demagnetization effects are very important in superconductors, where χ = −1 in contrast to normal metals where χ ≈ 10−4 or less. In practical cases, when the body under study is not ellipsoidal, one approximates the real geometry with an inscribed ellipsoidal surface which gives a best possible description of the real body, and uses the demagnetizing factor which applies to that ellipsoidal shape. This gives quite good results. A paradox : Having just proven that the field just outside the superconductor (usually) exceeds the applied field, one needs to consider what will happen when the applied field approaches Hc , the critical field of a type I superconductor. If we let the applied field Ha take the value (1 − n)Hc , then the internal field Hi becomes everywhere precisely equal to the critical field Hc . This looks like we now should expect the entire sphere to be driven into the normal state. However, this would cause M to become zero, since in the normal state this is the case with good approximation. This gives Hi = Ha < Hc , and we should conclude that we have a body driven into the normal state by a field H < Hc . This situation is an impossible paradox. Solution: What happens, is that the specimen allows some field to penetrate parts of the superconductor with normal lamina (type I), or vortices (type II). We have a coexistence of alternating normal and superconducting lamina in one case and vortices in the other. Such a thermodynamic coexistence of two phases is commonly found in nature. The situation is therefore normal, in agreement with the thermodynamic laws. The existence of such mixed normal and superconducting volumes is well documented in the scientific literature. Because of the effects discussed here, one finds in real situations that the transition from superconducting to normal state does not occur abruptly and

26

WHAT IS SUPERCONDUCTIVITY?

completely at the thermodynamic field, Hc , but rather over a certain range of fields, the width of which is determined by the demagnetization factor. We refer again to Figure 1.8 for an illustration of these points. With n = 0, as it is with the field along the axis of a long thin rod, the transition in a type I superconductor occurs abruptly at Hc , as we are led to expect from the foregoing, otherwise not.

2 Superconducting Materials 2.1 Introductory remarks After the initial discovery of superconductivity in an element of the periodic table, Hg, almost 20 years went by before research was undertaken in alloys. Another 40 years would pass before organic superconductors were synthesized in the 1970s. Then, another decade would pass before superconducting cuprates were discovered in 1986, followed by fullerenes shortly after. There is a line of progression of structures from the very simple to the quite complex. At the same time, Tc has increased by a factor of 40 from the beginning in mercury to the record Tc in cuprate perovskite; and there is a time span of 90 years between their discoveries. This seemingly slow development is governed by the general development of physics in a broader sense. Theoretical physics could not handle the manybody quantum theory necessary until the mid-1950s when the BCS theory was worked out. And the mechanism developed there was the only one to be relied upon until the superconducting cuprates were found 30 years later. Even today, 90 years after the initial discovery, there is a fierce debate about the mechanism for the high Tc cuprate superconductors. Superconductivity is still a subtle and very complex phenomenon.

2.2 Low-Tc superconductors 2.2.1

Superconducting elements

After superconductivity in Hg had been found, Sn and Pb followed suit. This brought Tc up from 4 K to 7 K. By the time the Meissner effect was discovered, several more elements of the periodic table had been added to the list. Meissner, among others, undertook studies of the transition elements with high melting point, called ‘hard’ metals. Discovery of superconductivity was announced in Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

28

SUPERCONDUCTING MATERIALS

Table 2.1 Ref. [12] Li F

Superconductors in the periodic table, including thin films. Adapted from

Be 0.03

Cs FP

Ba P

1

2

Tc = Superconducting transition F = Film P = Pressure applied Sc Ti 0.01 0.4

V 5.4

Cr F

Y P

Zr 0.6

Nb 9.3

Mo Tc 0.9 7.8

Ru 0.5

La Hi 4.9a 0.1 6.3b 3 4

Ta 4.4

W Re 0.02 1.7

Os 0.7

Ir 0.1

8

9

5

6

Eu F

Ce P Th 1.4

7

Pa 1.4

U P

10

11

Al Si 1.2 FP

P P

Zn 0.9

Ga 1.1

Ge FP

As P

Se P

Cd 0.5

In 3.4

Sn 3.7

Sb P

Te P

Hg 4.2

Tl 2.4

Pb 7.2

Bi FP

12

3

4

5

6

7

8

Lu 0.1

Am 1.0

tantalum in 1928 with Tc = 4.4 K, thorium in 1929, with Tc = 1.4 K, and Nb in 1930 with Tc = 9.2 K. The latter remains the highest Tc found in any element. Table 2.1 shows the elements with known superconducting Tc , a total of over 40 when observations of superconductivity under high pressure and in thin films are included. We notice in particular that superconductivity is neither found in the magnetic compounds, nor in the noble metals or copper. This indicates that superconductivity is incompatible with magnetism, and absent in metals with the highest electrical conductivity. Both of these rules will turn out to be understandable in light of the BCS theory; magnetism breaks up the Cooper-pairs, and is therefore a destructive influence; and excellent electrical conductivity is a signature of weak electron–phonon interaction, a property that reduces the effect of the electron–phonon mechanism for superconductivity in the BCS theory. In pure form the elements of the periodic table have provided excellent materials for scientific research in superconductivity. None of these pure elements have, however, contributed to applications of superconductivity on a large scale, like wires and cables for magnets. However, on a small scale Pb and Nb have been used for advanced development of Josephson technology. For SQUIDs (superconducting quantum interference device) niobium has been the best material overall, and is widely preferred in those particular low-Tc applications, to be discussed in Chapters 5 and 11.

LOW-Tc SUPERCONDUCTORS

2.2.2

29

Binary alloys and stoichiometric compounds

The earliest work on binary alloys has been largely forgotten, partly due to the overwhelming number of compounds that have been made and tested in later years. One person alone, Bernd T. Matthias, is said to have made some 3000 different alloys in his heroic attempt to achieve high-Tc superconductivity during the 1950s and 1960s. These efforts never succeeded, a fact which in itself gave strong impetus to go in totally new directions in more recent years. The history of the development of Tc is shown in Figure 2.1. The record shows [2] that research on binary alloys was started already in 1928 in Leiden by de Haas and Voogd. They found superconductivity in

180

160

* *

HgBaCaCuO 1993

Liq. CF4 140

TlBaCaCuO

120

BiSrCaCuO 1988 100 Tc(K)

YBCO (LBCO) 1987

80

60

Liq. N2

* = under pressure * LaBaCuO 1986

40

20

Liq H2

NbN NbC

Nb3Sn

Nb3Ge

V3Si Nb-Al-Ge Hg Pb Nb 0 Liq. He 1900 1920 1960 1980 1940 Year

Figure 2.1

*

History of Tc .

2000

30

SUPERCONDUCTING MATERIALS

A B

Figure 2.2

The A15-structure, A3 B.

SbSn, Sb2 Sn, Cu3 Sn, and Bi5 Tl3 . They noticed that the combination of a superconducting element with a non-superconducting one was successful. In Bi5 Tl3 , Tc was raised by a factor of 2–3 compared to pure Tl. What was even more interesting, was that the magnetic threshold for destruction of superconductivity in this material was much higher than in any of the elements known to be superconducting at the time. The material would remain superconducting up to 0.5 T at 3.4 K, and by extrapolation it was predicted to tolerate 0.9 T at 1.3 K. But soon they found an even more promising material; a Pb–Bi eutectic alloy with a critical field Bc = 2.3 T at 1.9 K. Unfortunately, the substance was so difficult to make and to handle that it never was to fulfill its promise as a material for wires, which might otherwise have made it an important material for superconducting electromagnets. After an intense period of research on binary alloys around 1930, not much happened in the materials area until Bernd T. Mattias and John K. Hulm started a new programme in the US in the early 1950s. Their ‘materials approach’ to superconductivity would bear rich fruit. A number of new compounds were made, with impressively high Tc and high critical fields. Throughout the 1950s the materials that were developed for use as superconductors included: solid solutions of NbN and NbC with Tc = 17.8 K; V3 Si with Tc = 17 K; Nb3 Sn with Tc = 18 K; NbTi with Tc = 9 K. Later (1973) Nb3 Ge was added to this list with the highest Tc of all, at 23.2 K, a record that lasted until 1986. We refer to Table 2.2 for some additional facts. The intermetallic compounds, just mentioned, belonging to the A3 B type of materials are classified as A15 compounds (Figure 2.2). They share a special feature, namely a softening of an elastic mode above Tc , a property which suggests relating their high transition temperatures to enhanced electron–phonon interaction caused by the softening. The two materials that have led to successful industrial production of low-temperature superconducting magnets are Nb3 Sn and NbTi. The first one is a stoichiometric, intermetallic compound, the second an alloy. These have paved the way for superconducting technology to

ORGANIC SUPERCONDUCTORS

31

Table 2.2 Some binary alloys and stoichiometric compounds. Values of Tc and Bc2 (0) may vary somewhat depending on precise composition Compound V3 Si Nb3 Sn Nb3 Ge V3 Ga NbTi VTi

Tc [K]

Bc2 (0) [T]

17 18 23.2 14 9 7

25 24 38 21 15 11

B

A e−

a

b e−

d+

d−

c

d

Figure 2.3 Predicted model substance for organic superconductor (Adapted from Little, 1964 [14]).

conquer the market for large laboratory magnets and magnetic resonance imaging magnets over the entire industrialized world. Behind this development lay great efforts in processing and materials science, as well as daring ventures into science-driven technological developments. Among the technical achievements were processing methods to make wires consisting of a large number of very thin filaments, a necessary procedure in order to stabilize the superconductor in a normal matrix.

2.3 Organic superconductors 2.3.1

Polymer and stacked molecular type

Research on electronically conductive organic materials dates back to the 1940s. High electrical conductivity was first discovered in 1954, in perylene bromine complex. Much later the discovery of a pronounced conductivity peak in (TTF)(TCNQ) near 60 K in 1973 [13] stimulated a lot of effort in the direction of low-dimensional systems, so-called charge transfer salts. Superconductivity in a polymer material was first found in (Sn)x in 1975. This was followed by the discovery in 1979 of superconductivity in a molecular salt,

32

SUPERCONDUCTING MATERIALS

Table 2.3 Some selected organic superconductors Material

Symmetry of counter molecule

(TMTSF)2 PF6 (TMTSF)2 ClO4 βL − (ET)2 I3 κ − (ET)2 Cu(NCS)2 κ − (ET)2 Cu[N(CN)2 ]Br α − (ET)2 RbHg(SCN)4 κH − (ET)2 Ag(CF3 )4 · TCE κL − (ET)2 Ag(CF3 )4 · 112DCBE κH − (ET)2 Au(CF3 )4 · TCE λ − (BETS)2 GaCl4

Octahedral Tetrahedral Linear Polymeric Polymeric Polymeric Planar Planar Planar Tetrahedral

TCE: 112DCBE:

1,1,2-trichloroethane 1,1-dichloro-2-bromoethane

H3C C

Se

Se C

C H3C

CH3 H2C

C

Se

Se

0.9 1.4 1.5 10.4 11.8 0.5 11.1 4.1 10.5 8

S

C C

H2C

CH3

Tc [K]

S

C

S C

C

S

S

TMTSF

S C

CH2

C S

C S

CH2

ET (BEDT-TTF) S H2C H2C

C

Se

Se C

C S

Se

S C

CH2

C Se

C S

CH2

BETS (BEDT-TSF)

(TMTSF)2 FF6 under 1.2 Gpa pressure, and with a Tc of 0.9 K [15]. Since then, a long list of organic superconductors have been synthesized, some of which are seen in Table 2.3. Tc remains low, although it has increased by a factor of more than 10 since the first discovery. In this sense progress has been remarkable. In another sense it has been disappointing, since predictions had been made for roomtemperature superconductivity in stacked organic structures. This prediction was set forth in 1964 by Little [14] in a paper where he suggested the possible existence of superconductivity in an organic substance consisting of a long unsaturated polyene chain, called the ‘spine’, with an array of side chain molecules attached at regular intervals (see Figure 2.3). He showed that even if the spine was initially an insulator because the valence bond was full and the conduction bond was empty, the addition of side chains could increase the effective electron–electron attraction to the point where it became energetically favourable to enter the superconducting state by mixing in states of the conduction band. It was concluded that superconductivity at room temperature could result. This paper in particular stimulated a worldwide effort to discover superconductivity in substances of appropriately stacked organic structures. The mechanism proposed by Little has later become known as the polaron mechanism. It is

ORGANIC SUPERCONDUCTORS

33

an alternative to the phonon mechanism, which was the one worked out in detail in the BCS-paper. Due to the higher energies involved in this new mechanism, Tc was expected to be much higher in the polaronic superconductors than in those with phonon-mediated pairing. Some of the organic superconductors are best described as a stack of twodimensional superconducting sheets with Josephson coupling between them. A good example is the so-called κ-type BEDT-TTF salts. They have different zero-degree coherence length ξ0 and ξ0⊥ in the stacking plane and normal to it, respectively. Table 2.4 shows Tc and coherence lengths for four different ET compounds, as determined by analysis of magnetic measurements. One finds the remarkable result that the interplanar coherence length ξ0⊥ is shorter than the interplanar distance by a factor of about 5. Supercurrent in the direction normal to the stacking planes must therefore be carried by Cooper pair tunnelling, so-called Josephson tunnelling. We refer to Chapter 5 for a discussion of the physics of Josephson tunnelling. What determines the important coherence length? Disregarding anisotropy for the moment, let us call this length ξ0 . A simple argument by means of the uncertainty principle leads to the following expression: ξ0 ≈

vF kTc

(2.1)

where is Planck‘s constant divided by 2π , vF is the Fermi velocity, and k is the Boltzmann constant. This indicates an inverse relationship between Tc and ξ0 , and proportionality between ξ0 and vF . Ideally we would want both ξ0 and Tc to be high, Tc for obvious reasons, ξ0 because a higher value provides better stability of the superconducting state. But clearly, a compromise is the best one can hope for. We see from the values in Table 2.4 that ξ0 in the 2D-plane is much longer than in the direction normal to the plains. This gives an indication for a ‘design-criterion’ for stacked superconductors. We shall encounter a similar situation in the inorganic high-Tc compounds in Section 2.5.

Table 2.4 Tc , and coherence lengths normal to the stacking plane ξ0⊥ , and parallel, ξ0 , for some ‘ET ’-compounds Material

Tc [K]

ξ0⊥ [nm]

ξ0 [nm]

κ − (ET)2 Cu(NCS)2

8.7 ± 0.2

0.31 ± 0.05

2.9 ± 0.5

κ − (d8 − ET)2 Cu(NCS)2

9.0 ± 0.2

0.32 ± 0.05

2.9 ± 0.5

κ − (ET)2 Cu[N(CN)2 ]Br

10.9 ± 0.2

0.58 ± 0.1

2.3 ± 0.4

κ − (d8 − ET)2 Cu[N(CN)2 ]Br

10.6 ± 0.2

0.57 ± 0.1

2.3 ± 0.4

After Ishiguro et al. [13].

34

SUPERCONDUCTING MATERIALS

2.3.2

Fullerene superconductors

The Buckminster fullerene C60 is a carbon molecule containing 60 atoms located at the vertices formed by the intersections of 12 pentagonal and 20 hexagonal faces, altogether forming a closed cage, as shown in Figure 2.4. We note that all atoms are in equivalent positions, where each is surrounded by one pentagon and two hexagons. One π electron and three σ electrons form a sp2 hybrid orbital. C60 condenses into an fcc structure, leaving room for introduction of small interstitial dopants like K and Rb. Other structures are bct K4 C60 and bcc K6 C60 . A significant transfer of electrons from K 4s orbitals to the C60 conducting band takes place. The electrical conductivity increases with dopant concentration, with a maximum for K3 C60 . The resulting substances have a well-defined Fermi surface. Superconductivity has been observed in a number of fullerene-based materials. The initial discovery was made in K3 C60 [16]. As shown in Table 2.5, transition temperatures go as high as 40 K. In Table 2.8 in the last section of this chapter a Tc as high as 45 K is indicated. Critical fields Hc2 are quite high, 28 T in K3 C60 and 38 T in Rb3 C60 . The fullerenes have been carefully studied with respect to isotope effects in Tc -values. The presence of significant Tc -dependence on atomic masses indicates electron–phonon mediated superconductivity. The presence of the Hebel–Slichter peak in nuclear magnetic resonance (NMR) (see Chapter 4) is considered definite proof that the BCS mechanism discussed in Chapter 3 is active.

Figure 2.4

Structure of C60-molecule (Buckminster ball).

OXIDE SUPERCONDUCTORS BEFORE THE CUPRATES

35

Table 2.5 Structure and Tc ’s of some fullerene type superconductors Material

Symmetry of the salts

Tc [K]

K3 C60 Cs2 RbC60 (NH3 )4 Na2 CsC60 Cs3 C60 NH3 K3 C60 Rbx (OMTTF)C60 (benzene)

fcc fcc fcc bct/bcc Orthorhombic

19.3 33 29.6 40 28 26

fcc = face-centered cubic, bct = body-centered tetragonal, bcc = body-centered cubic, OMTTF = octamethylenetetrathiafulvalene.

2.4

Chevrel phase materials

Superconductors referred to as Chevrel phase materials were discovered in 1971 (Figure 2.5) [17]. These are ternary molybdenum chalcogenides of composition MMo6 X8 , where X is one of the chalcogenes S, Se, or Te. M can be one of many different metals or rare earths. A most remarkable property of these compounds is the high critical magnetic field of some of them, as listed in Table 2.6. Figure 2.6 shows the temperature dependence of Bc2 (T ) for a number of low-Tc superconductors.

2.5 Oxide superconductors before the cuprates Superconductivity was found in 1964 in the perovskite oxide SrTiO3 [18], whose structure is shown in Figure 2.7. The following oxide compounds were found to exhibit superconductivity: doped SrTiO3−δ , NbO, and TiO. They had Tc ’s X = S, Se, Te Mo M

Figure 2.5

Structure of the Chevrel phase.

36

SUPERCONDUCTING MATERIALS

Table 2.6 Critical temperatures Tc , and critical fields Bc2 in some Chevrel phase materials Compound

Tc (K)

Bc2 (T)

SnMo6 S8 PbMo6 S8 LaMo6 S8

12 15 7

34 60 45

1) Nb3Ge 2) Nb79(AlGe)21 3) PbGd0.2Mo6S8 4) PbMo6S8 5) Nb0.3Ti0.7 6) Ti0.5V0.5 7) TaS1Se1 8) TaS2 (pyridin)

60 MxMo6S8

m0Hc2 (T)

50

40

30

20

Schicht

A-15

5) Nb-Ti 10

6)

V-Ti

8) 7) 0

2

4

6

1)

3) 4)

2)

8 10 12 14 16 18 20 22 T (K)

Figure 2.6 Upper critical field µ0 Hc2 versus temperature in various superconductors. After Fischer [19].

O Sr Ti

Figure 2.7

The cubic ABX3 structure. A prominent example is SrTiO3 .

HIGH-Tc CUPRATE SUPERCONDUCTORS

37

in the range 0.7 K to 2 K. In the years after 1964, bronzes were found to be superconductors: Kx WO3 , Kx MoO3 , Kx ReO3 . These had Tc ’s in the 4–6 K range. The 1970s brought discoveries of LiTi2 O4 and Ba(PbBi)O3 , both with Tc = 13 K. Naturally, they all had low carrier density. By now the results were encouraging, and the development pointed to oxide perovskites as a possibly promising class of materials. Some groups therefore pursued such a course.

2.6 High-Tc cuprate superconductors 2.6.1

The discovery of cuprate superconductors

The breakthrough to a new era in higher superconducting transition temperatures came in 1986 by the discovery of superconductivity in the La2−x (Ba,Sr)x CuO compounds by two scientists at the IBM Zurich laboratory, J. George Bednorz and K. Alex M¨uller [9]. Figure 2.8 shows the corresponding undoped mother perovskite La2 CuO4 . In their article in Zeitschrift f¨ur Physik they cautiously announced: ‘Possible high Tc superconductivity in the Ba-La-Cu-O system.’ Their material showed onset of superconductivity at about 30 K, well above previous records (see Figure 2.9). Initially the reaction from the scientific community was somewhat reluctant, but this changed to intense interest and competition, as soon as their results were confirmed by other groups, in Japan, in the US and China. The next important development occurred when the Houston group lead by Chu showed that external pressure could raise Tc substantially, going above 40 K under 13 kbar pressure [20]. An effect which is equivalent to application of

O La Cu

Figure 2.8 La2 CuO4 tetragonal crystallographic unit cell.

38

SUPERCONDUCTING MATERIALS

0.05

Resistivity r(Ω cm)

0.04

0.03

0.02

I = 0.50A/cm2

0.01

0

0

100 200 Temperature (K)

300

Figure 2.9 Resistivity versus temperature in La2−x Bax CuO. After the original publication by Bednorz and M¨uller, 1986 [9].

high pressure is achieved by replacing some of the ions with smaller ones having the same chemical properties. Thus, replacing Ba with the smaller ion Sr led to a Tc of 38 K. Naturally, one would think that a similar procedure ought to be tried at the La-site. The Huntsville group led by Wu proceeded in collaboration with the Houston group to replace both La and Ba, with Y and Sr, respectively. This suddenly brought Tc above 90 K [21].The news spread quickly all over the world. Soon the successful new compound turned out to be YBa2 Cu3 O7 (Figure 2.10). The discovery was made more or less simultaneously in several laboratories, in Tokyo, Beijing and at Bell Labs in the US. This breakthrough was of historic proportions. Tc had now moved well above the boiling point of liquid N2 at 77 K. The best values of Tc turned out to be in the range 91–93 K in YBa2 Cu3 O7−δ , depending on the value of δ (see Figure 2.11). The ensuing response from the scientific community was without parallel in the history of science. Suddenly, the efforts were joined by thousands of scientists and students around the world, trying to understand YBa2 Cu3 O7−δ and the other newly discovered compounds, and to push Tc even higher. Several new compounds with higher Tc were soon synthesized. With one exception, Ba1−x Kx BiO3 , all had one common feature: a quasi-2D network of CuO2 – i.e. they were all cuprate perovskites. The new materials are very different from traditional metals, being doped oxides. Their normal state properties are different from metals, and they are so strongly anisotropic that they could be shown in some cases to possess metallic-like conductivity in directions parallel to the CuO2 planes – although not free-electron like – while behaving

HIGH-Tc CUPRATE SUPERCONDUCTORS

39

Charge reservoir layer

Conduction layer

Cu O Charge reservoir layer

Y Ba

Figure 2.10 Structure of orthorhombic YBa2 Cu3 O7 . 100

Tc(K)

80 60 40 20 Normal 0 0.0

Superconductor 0.5 Oxygen content x

1.0

Figure 2.11 Tc versus x in YBa2 Cu3 O6+x . Data from Cava et al. (circles) [21] and from Jorgensen et al. (triangles) [22].

like semiconductors along the c-axis, normal to CuO2 planes. This profound anisotropy affects essentially all physical properties [23]. In the ensuing years huge efforts were spent on achieving superconductivity at still higher temperatures, even with the hope of reaching room temperature. This did not happen, but the efforts resulted in a long list of new superconducting compounds with complex structures and intriguing properties. A superconducting transition temperature as high as 163 K was eventually reported in the Hg-based HgBa2 Ca2 Cu3 O8 compound at a high external pressure. We refer again to Figure 2.1 which summarizes the main historical development of Tc

40

SUPERCONDUCTING MATERIALS

versus time. For further details about the historical record we refer the reader to Dahl [2].

2.6.2

Composition and structure

Referring now to Figure 2.10 showing the YBCO structure, one clearly sees the connection to the simple cubic perovskites. Essentially, YBCO is a stack of three perovskite unit cells where, compared to the basic model ABX3 (Figure 2.7), with atoms removed in some places and substituted in other places. The typical oxygen octahedra, so familiar in the ABX3 compounds like SrTiO3 have been split in two by a middle layer, and Ba replaces Y as the central atom in two out of three layers. We notice also that YBa2 Cu3 O7 is a modification of the structurally simpler compound YBa2 Cu3 O6 . Processing of high-Tc superconductors to single-phase material requires elaborate processes, which we will not go in details about here. Let us just remark that as far as YBCO is concerned the processing route usually goes via making the non-superconducting YBa2 Cu3 O6 first. This materials may be obtained under appropriate conditions in an oxygen atmosphere from a mixture of Y2 O3 + BaO + CuOx , heated to over 900 ◦ C. The resulting material is of tetragonal structure, with a lot of oxygen vacancies. On lowering the temperature to somewhere between 400 ◦ C and 500 ◦ C more oxygen is absorbed by the structure and a different oxygen ordering takes place, with Cu-O chains, as shown in Figure 2.10. The chain formation

Figure 2.12 Permanent magnet levitating above a chunk of high-Tc superconducting Y1 Ba2 Cu3 O7 .

HIGH-Tc CUPRATE SUPERCONDUCTORS

41

breaks the tetragonal structure with different lattice parameters along the a- and b-directions. A subsequent quenching of the material traps the oxygen in the structure. When all available oxygen sites are filled in this structure we have the YBa2 Cu3 O7 compound shown. Doping of SrTiO3 had been demonstrated to lead to superconductivity due to a reduction process, whereby oxygen was removed. The situation in YBCO is related, but more complicated, as can be seen in Figure 2.11. Starting with the YBa2 Cu3 O6+x structure at x = 0 and increasing the oxygen content via external oxygen supply at high temperatures the compound at first is an insulator, but becomes a superconductor at x-values grater than 0.4. From there on Tc increases until it goes through a maximum at x ≈ 0.93, and diminishes slightly until x = 1 is reached. Optimal doping (corresponding to the highest Tc ) of YBCO therefore is achieved in Y1 Ba2 Cu3 O7−δ with δ ≈ 0.07. On inspecting the resulting structure, one plane at a time, one finds that the orthorhombic YBCO structure consists of layers as do all high-Tc compounds. Beginning at the bottom and proceeding upwards they are: CuO, BaO, CuO2 , Y, CuO2 , BaO, CuO. The CuO2 layers are superconducting in YBCO like in all other high-Tc materials. But YBCO possesses the additional CuO chains, as mentioned. These can also be superconducting, depending on the degree of filling. In this respect YBCO is unique among high-Tc materials. Another aspect of this structure is that the oxygens are not in equivalent positions in the lattice, contrary to ABO3 type structures. There are four inequivalent O sites and two inequivalent Cu sites.

2.6.3

Making high Tc materials

High-Tc materials, being doped oxides, are made by heating a mixture of appropriate amounts of metal oxides in powder form to temperatures in the range 850–950 ◦ C. Materials that contain some percentage of superconductor are then easily obtained. But making materials of good quality, whether polycrystalline or single crystals is quite a different and highly non-trivial matter. Only quite elaborate procedures with attention paid to every detail of composition, temperature, pressure and atmosphere will bring out high quality materials. Regrinding, compressing and sintering repeatedly, is usually necessary. The resulting bulk material is then a fine-grained ceramic, brittle, and with high density of defects and grain boundaries. Making the big step towards single crystals is an even greater challenge. Growing large crystals of high quality has turned out to be extremely difficult. The main reason for this is to be found in the layered structure, which permits easy diffusion and growth along the (a, b)-planes, but allows only very slow diffusion and growth along the c-direction. Some of these materials end up quite ‘flaky’, like in the Bi-based materials where layer by layer may be peeled off quite easily. This is an intrinsic property of the material

42

SUPERCONDUCTING MATERIALS CuO

BaCuO2 Ba2CuO3

YBa2Cu3O7−d

Y2Cu2O5

YBa4Cu3O8.5 Y2BaCuO5−d

BaO

Y2BaO4

YO1.5

Figure 2.13 Isothermal phase diagram for the Y2 O3 -BaO-CuOx system at 900 ◦ C in 1 atm oxygen. Calculations by Rian [24]. Lines connect phases which exist in equilibrium at this temperature.

itself, reflecting the great anisotropy. Much of the difficulty in crystal growth and processing lies also in the fact that even the simplest of them are quaternary compounds. When 3 oxides are mixed, several different phases may result. Figure 2.13 shows a chemical equilibrium phase diagram relevant to YBCO. Matters grew even more complex when it turned out that the road to higher Tc went through compounds like Bi2 Sr2 Ca2 Cu3 O10+δ or Bi2 Sr2 Ca1 Cu2 O8+δ , with four metal ions, as can be seen in Figure 2.14, and several similar ones with Tl or Hg replacing Bi. In the process of making such substances a number of unwanted phases will normally be created. In this case perfection is practically impossible in bulk production, but single crystals may be grown. In order to study the intrinsic properties of new materials, access to single crystals is a necessity. Table 2.7 shows a list of high-Tc compounds, with corresponding Tc -values.

2.6.4

Phase diagrams and doping

Superconductivity in high Tc materials depends on appropriate doping; and the phase diagrams show a remarkable similarity: as a function of the appropriate doping parameter they all have an antiferromagnetic phase near zero doping, followed by an insulating phase, then the superconducting phase underneath a sort of metallic phase in a certain doping range, and finally Tc goes to 0 again. The typical situation is sketched in Figure 2.15, where the various phases

HIGH-Tc CUPRATE SUPERCONDUCTORS

43

BiO

BiO SrO CuO2 Ca CuO2 SrO BiO

BiO

SrO

Figure 2.14

Structure of Bi2 Sr2 CaCu2 O8 crystal.

are indicated. One finds the peculiar property that in every substance there exists a range of x-values, where superconductivity is observed, with optimal doping corresponding to the highest Tc , somewhere near the middle of that range. Above this dome-shaped curve is the ‘normal’ state, a kind of unconventional metallic region. To the left of the dotted line in Figure 2.15 is a region which is often referred to as that of a ‘strange’ metal, while to the right of the same line one finds more normal metallic properties. Much of the secret of highTc compounds may be found in these peculiar normal state properties. Often the question is asked: how can we understand high-Tc superconductivity if we don’t even understand the normal state? Anderson is the scientist who most relentlessly has pursued this question [25].

44

SUPERCONDUCTING MATERIALS

Table 2.7 Some representative examples of high-Tc cuprate superconductors and their Tc ’s. The reported values of Tc will vary somewhat, depending on the processing conditions and resulting oxygen content and other deviations from stoichiometry Compound

Tc [K]

Nicknames

39 92 84 110 90 110 125 91 116 122 95 122 133 25

LCCO or LaSCCO Y123 or YBCO Bi2212 or BiSCCO Bi2223 or BiSCCO

La1.85 Sr0.15 CuO4 YBa2 Cu3 O7 Bi2 Sr2 CaCu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 CuO6 Tl2 Ba2 CaCu2 O8 Tl2 Ba2 Ca2 Cu3 O10 TlBa2 CaCu2 O7 TlBa2 Ca2 Cu3 O9 TlBa2 Ca3 Cu4 O11 HgBa2 CuO4 HgBa2 CaCu2 O6 HgBa2 Ca2 Cu3 O8 Nd1.85 Ce0.15CuO4−y

Tl2223 or TBCCO

Hg1223 or HBCCO NCCO

300

T* TN

T (K)

200

Optimally doped metal (non-Fermi-liquid)

Pseudogap Underdoped insulator

100

Overdoped metal (Fermi-liquid)

AFM Tc Insulator Superconducting 0 0

0.10

0.20

0.30

x

Figure 2.15 Typical overall phase diagram with doping in high-Tc cuprate superconductors (AFM = antiferromagnetic phase).

HIGH-Tc CUPRATE SUPERCONDUCTORS

45

40

10 0

0.05

0.10

0.15 0.20 Doping x

Tetragonal

20

Orthorhombic

Tc(K)

30

0.25

0.30

Figure 2.16 Tc versus doping in La1−x Srx CuO4 . Data from Radelli et al. [26].

How doping is achieved, i.e. how the parameter x on the horizontal axis of Figure 2.15 is controlled, depends on the compound. In the case of the La-based, original high-Tc materials, the key is to replace trivalent La with divalent Ba or Sr (Figure 2.16). Because the basic compound La2 CuO4 is charge neutral, replacing La3+ with Ba2+ and still demanding charge neutrality results in a freed positive charge, donated to the valence band. On the other hand, in the case of oxygen depletion, removing an oxygen atom leaves behind two incomplete bonds, which upon completion free two positive charges, or holes. The charge structure of the cuprates can be described in a very simple block form by separating the superconducting atomic layers from the non-conducting ones, as shown in Figure 2.10 for the case of YBa2 Cu3 O7 . This case is special due to the existence of CuO chains. But the general charge structure scheme for all cuprate superconductors is as follows: A stack of alternating layers of charge reservoirs (like BaO or CuO) and conducting CuO2 layers that receive the mobile charges (usually holes) from the charge reservoirs. This internal redistribution of charge occurs in a fine tuned balance between the valences (affinities) of participating atoms. The undoped YBa2 Cu3 O6 has an insulating CuO2 layer where the d9 electrons of Cu2+ ions are antiferromagnetically bound. On admitting oxygen to YBa2 Cu3 O6 the chains are formed at the expense of taking away the necessary two electrons per atom from the CuO2 -plane. This is equivalent to doping the CuO2 plane with positive mobile charges, or holes. The result is a hole-like superconductor. The process is different in La2−x Bax CuO4 , where Ba2+ replaces La3+ , but the result is similar. When Ba is brought into the insulating La2 CuO4 unit cells, it delivers two negative charges to the bonds, but it needs one more to make up for three electrons donated by La, so an extra electron is taken from CuO2 to complete all bonds, and thereby a hole is released in the CuO2 plane, to give conduction. Although hole- doping is the rule in highTc superconductors there are some cases where the mobile charges are electrons. Figure 2.17 shows these possibilities for both types of carriers where the aspect

46

SUPERCONDUCTING MATERIALS Metallic

Insulating

Temperature T(K)

Electron-doped Nd2−xCexCuO4−y

Metallic

Hole-doped La2−xSrxCuO4−y

200

N-type

P-type 100

P-type

N-type

AFM SC

AFM

SG SC

0.3

0 Concentration x in Ln2−xMxCuO4−y

0.4

Detector output 1.0 mV

Figure 2.17 Comparison of electron-doped and hole-doped superconductor. The assignment SG refers to the possible existence of a spin glass phase.

0

100

200 Time (s)

300

400

Figure 2.18 These measurements of flux jumps in a superconducting ring gave the first verification of the flux quantisation according to 0 = 2e h in high-Tc superconductors. Adapted from [27].

of electron-hole symmetry is emphasized. Upon learning that these materials are dominated by hole carriers, one might ask: What about the pairing of carriers, is it still as we know it from the low-Tc metallic superconductors? The answer was found quite early by the Birmingham group [27] who demonstrated that flux quantization was intact in the new materials, and that the flux quantum was h 0 = 2e as before. In this sense it did not matter what the sign of the charge is. The measurements which provided proof of pairing in high-Tc superconductors are shown in Figure 2.18.

HIGH-Tc CUPRATE SUPERCONDUCTORS

2.6.5

47

Some remarks on the original idea which led to the discovery of cuprate superconductors

In spite of all efforts which have been spent on establishing a theoretical understanding of superconductivity in cuprate perovskites, a final conclusion on this matter has not yet been reached. It is nevertheless quite interesting to follow the reasoning which led Bednorz and M¨uller on the right track. We quote here a section taken directly from a paper given by M¨uller on the occasion of the celebration of the first 10 years of high-Tc superconductivity in 1996 [28]. (for simplicity we omit here the numerous references given): Strong electron-phonon interactions can occur in oxides, owing to polaron formation as well as mixed-valence states. This can go beyond the standard BCS theory. A phase diagram with a superconducting to bipolaronic insulator transition was proposed early by Chakraverty. A mechanism for polaron formation is the Jahn–Teller (JT) effect as studied by H¨ock et al. in a linear chain model. From it, one expects heavy polaron masses if the JT stabilization energy becomes comparable to or larger than the bandwidth of the degenerate orbitals, and thus localization. Intermediate polarons are expected if the JT energy is not too large compared to the bandwidth. We recall that the JT theorem states the following: A nonlinear molecule or a defect in a crystal lattice exhibiting an electron degeneracy will spontaneously distort in lowering its symmetry, thereby removing its degeneracy. Isolated Fe4+ , Mn3+ , Ni3+ and Cu2+ in an octahedral oxygen environment show strong JT effects because their incompletely occupied eg orbitals, transforming as 3z2 − r 2 and x 2 − y 2 , point towards the negatively charged oxygen ligands. Although SrFe4+ O3 is a distorted perovskite insulator, LaNiO3 is a JT undistorted metal in which the transfer energy bπ of the eg electrons of the Ni3+ is large enough to quench the JT distortion. On the other hand, LaCuO3 is a metal containing only the non-JT Cu3+ . Therefore, it was decided to investigate and ‘engineer’ nickel- and copper-containing oxides, with reduced bandwidth bπ , partially containing Ni3+ or Cu2+ states. The JT polaron proposed in 1983 was one envisaged to lead to a heavy mass of the particle; and intermediate, mobile polaron suited for superconductivity was not considered. However, in the ferromagnetic conductor La1−x Cax MnO3 , a giant oxygen isotope effect has been discovered most recently and ascribed to the presence of intermediate JT polarons due to the Mn3+ ions in the oxide. This important and new evidence for the existence of intermediate JT polarons is quite in favor of the new original concept. In R¨usclikon, there was a tradition of more than two decades of research in insulating oxides that undergo structural and ferroelectric transitions, which was a strong motivation to pursue the program. Furthermore, in 1979 the present author had started to work in the field of granular superconductors in which small Al grains are surrounded by amorphous Al2 O3 . In these systems Tc ’s have been reported to be as high as 5 K, compared to pure Al with a Tc of 1.1 K. In our laboratory, the search for superconductivity was initiated together with J. G. Bednorz in mid-summer of 1983. our efforts first concentrated on Ni3+ -containing perovskites, such as mixed crystals of LaNiO3 and LaAlO3 . In these unpublished efforts, the metallic behavior of the various synthesized double and triple oxides was measured, and at low temperatures

48

SUPERCONDUCTING MATERIALS

they exhibited localization upon cooling. This indicated the possible existence of JT polarons, however, without any signs of superconductivity. In Figure 2.9, results of these efforts are reproduced. In late summer of 1985, the efforts were shifted to copper-containing compounds, such as LaCuO3 . Because Cu3+ has two electrons in the eg subshell, the latter is half-filled. Thus, its ground state is not degenerate. It was clear that an oxide with mixed Cu2+ /Cu3+ or Cu3+ /Cu4+ had to be tried. At this stage, Bednorz became aware of a paper by Michael, Er-Rakho and Raveau on the mixed perovskite BaLa4 Cu5 O13.4 , exactly meeting the requirements of mixed valence. The French authors had shown that this mixed oxide, a metal at room temperature and above, contained Cu2+ and Cu3+ . Thus, we tried to reproduce it, at the same time continuously varying the Cu2+ /Cu3+ ratio by changing the Ba concentration on Bax La5−x Cu5 O5(3−y) , and we looked for superconductivity. A representative and concise account of the discovery of superconductivity in Bax La5−x Cu5 O5(3−y) and the relevant superconducting phase present appeared in the September 4, 1987, issue of Science and, in more detail, in the first of the two Nobel lectures in 1987, and would exceed the scope of this contribution.

2.6.6

Thermal fluctuations of the superconducting condensate. A preliminary discussion

Already in 1988 two more significant series of high-Tc superconductors were synthesized: one Bi-based, and one Tl-based. Later, a Hg-based series was also found. These series gave Tc ’s higher than the 93 K of YBCO, as could already be seen from Table 2.7. At the same time, however, their anisotropy was found to be much stronger than in YBCO, and the coherence length is very short, both a disadvantage and a challenge for their practical use. Why the coherence length is so short can be seen from Eq. 2.1, which can be obtained from the BCS theory, and may be assumed to hold approximately even in high-Tc . Equation 2.1 predicts a very short coherence length in high-Tc due to the combination of small Fermi surfaces with low vF , caused by the low concentration of holes, and the high Tc . The expression used here may also be derived from the uncertainty relation, and is not sensitive to the pairing mechanism. This prediction for ξ0 is approximately followed in real systems. While ξ0 = 1600 nm in Al, it is only of the order of 1 nm in the high-Tc compounds. This gives the thermal energy of kT a chance to create fluctuations of large spatial extent in the order parameter since they will occur in a typical volume ξ 3 . This volume is of the order of (1/1600)3 = 2.4 × 10−10 times smaller in high Tc materials than in aluminium. The energy barrier E against the creation of a fluctuation in the order parameter is proportional to the respective volumes ξ 3 in each case, and also proportional to the square of the thermodynamic field, i.e.

HIGH-Tc CUPRATE SUPERCONDUCTORS

E ≈

1 3 2 ξ Bc 2µ0

49 (2.2)

The ratio of condensation energies in a volume of ξ¯ 3 in the two materials is therefore

EYBCO (ξ¯ 3 Bc2 )YBCO =

EAl (ξ¯ 3 Bc2 )Al

(2.3)

where we have written ξ¯ 3 to indicate a geometric average of ξ1 ξ2 ξ3 for the anisotropic cases. A numerical estimate of the barrier ratio expressed by Eq. 2.3 gives 1.3 × 10−6 , favouring fluctuations enormously in YBCO as compared to Al. The ratio of probabilities for thermal fluctuations at a temperature T can be written as −

E kT YBCO

p1 e PYBCO = PAl − E kT Al p2 e

−

=

p1 e

ξ¯ 3 Bc2 2µ0 kT

−

p2 e

ξ¯ 3 Bc2 2µ0 kT

YBCO

(2.4)

Al

Let us try to gain some insight into the consequences of Eq. 2.4. Here the exponents are far more important than the unknown coefficients p1 and p2 . From measurement, Bc in aluminium is 0.02 T, and Bc in YBCO may be taken to be about 1.5 T. The ξ0 -values for YBCO and Al, can be estimated from Eq. 2.1. For Al, vF = 2.03 × 106 and Tc = 1.17 K which gives the estimate ξ0 = 2.2 × 103 nm. This is not too far away from the measured value, ξ0 = 1.6 × 103 nm. For YBCO, vF is about 100 times lower than in Al. This tells us that the ratio of coherence lengths ξAl /ξ¯YBCO should be about 104 , which is of the correct magnitude compared to measured values. Furthermore, the ratio between fluctuating volumes (ξAl )3 /(ξ¯YBCO )3 is about 1012 . So, not only is the fluctuating volume in YBCO a factor 10−12 smaller than in Al, but since the fluctuations take place at temperatures near 100 K in YBCO, versus 1 K in Al, the available energy to drive the fluctuations in YBCO is ≈102 greater. The effect of thermal fluctuations should therefore be expected to be hugely greater in YBCO than in Al. We can now estimate the exponents in Eq. 2.4 to gain an impression of the difference in probabilities for thermal fluctuations in the respective superconducting volumes of size ξ¯ 3 . For Al we find near Tc : ¯3 2 ξ Bc

E ≈ ≈ 4.0 × 107 (2.5) kT Al 2µ0 kTc Al

50

SUPERCONDUCTING MATERIALS

Clearly, this is an impossible barrier to overcome. Hence, thermally driven fluctuations in the density of Cooper pairs in a volume ξ¯ 3 in Al occur with practically vanishing probability. Let us now compare this with the situation on YBCO. We find

E kT

≈ YBCO

ξ¯ 3 Bc2 2µ0 kTc

≈1

(2.6)

YBCO

2 × ξ , and taken a rough average of In this estimate, we have written ξ¯ 3 = ξab c 3 −9 tabulated values to find ξ¯ = (1.5 × 10 m)2 × 0.5 × 10−9 m ≈ 2 × 10−27 m3 . With a resulting probability PYBCO ∝ e−1 the conclusion is that thermally driven fluctuations that suppress superconductivity in a ξ¯ 3 -volume must occur profusely. Conversely, the same argument says that in the normal state above Tc , fluctuations will occur with similar likelihood, in this case creating superconducting ξ¯ 3 -volumes in the normal matrix. In conclusion, the superconducting transitions in YBCO and other high-Tc materials, occur with such violent fluctuation of the superconducting wavefunction near Tc that the behaviour is bound to be non-classical, non-mean-field like, quite different from low-Tc physics. At this point one may even wonder how a substance with such violent fluctuations can sustain superconductivity at all near Tc . This is a very valid question indeed that will be dealt with in Chapters 9 and 10. Clearly, the superconducting phase transition in YBCO and other high-Tc superconductors is fundamentally different from low-Tc materials. The important question is how it is different. At this stage, let us also ask: What topological form will the fluctuations discussed above have? Will they always be in the shape of a ξ¯ 3 -volume as defined above? Not necessarily. There is sufficient thermal energy that the volume could be extended in one coordinate, for instance in a tubular shape, and still have a very good chance for the fluctuation to occur. As is now well established by computer-simulation there is firm prediction for a high rate of generation of thermally induced vortex loops. According to the prediction, this behaviour is accompanied by a vortex ‘blow-out’ phase transition within a vortex liquid phase [29, 30]. Figure 2.19 attempts to sketch such possibilities. These issues are discussed more precisely in Advanced Topics. It should be kept in mind for comparison, that on lowering the temperature of a high-Tc compound to liquid helium temperatures, fluctuations even in these compounds would occur with a low probability. It is the combination of high temperature, short coherence length and anisotropy which make the high-Tc compounds so different in terms of fluctuation properties at elevated temperatures. Figure 2.20 shows a highly unusual phenomenon in a high-Tc superconductor. The characteristic rule of superconductivity, that diamagnetic response is found only below Tc , is broken; diamagnetism is observed above Tc . The effect is explained by the presence of Cooper-pairs already formed above Tc .

HIGH-Tc CUPRATE SUPERCONDUCTORS

51

Figure 2.19 Sketch of possible configurations of thermally generated flux loops in high-Tc superconductors in the ordered phase as discussed by Tesanovic [31, 32], and Nguyen and Sudbø [29, 30].

1G 0

180 µG

c (emu/g)

−0.05

−0.1

−0.15

−0.2

−0.25 36

37

38

39 T (K)

40

41

42

Figure 2.20 Magnetic susceptibility in the superconductor La1.85 Sr0.15 CuO4 showing the presence of diamagnetic response (upper curves) even above Tc due to the presence of significant concentration of Cooper pairs above the superconducting phase transition. Tc is known to be 38 K from other independent measurements. The numbers given in the figure, 1 G and 180 µG, refer to the ac-field used in the measurements. Only of the lowest field did the weak superconducting resparse show up above Tc . After Thisted et al. [33].

52

SUPERCONDUCTING MATERIALS

2.7 Heavy fermion superconductors The term ‘heavy fermion superconductors’ refers to a class of superconductors characterized by very high effective electron mass, m∗ , 2-3 orders of magnitude larger than the free electron mass. The first discovery of such superconductors was made by Steglich and coworkers in 1979 [34]. The compound was CeCu2 Si2 . This discovery was later followed by UBe13 and UPt3 . The main characteristics of some of these superconductors are given in Table 2.8. Figure 2.21 shows the structure of the material where superconductivity was first discovered. Typical for these superconductors is that they contain elements like the rare earth Ce with two 4f electrons, and the actinide U with 5f electrons. When these f electrons mix or hybridize with conduction electrons a sharp band with high density of states D(E) arises at the Fermi energy. Since D(E) ∝ (m∗ )3/2 Table 2.8

Heavy fermion superconductor properties.

Superconductor

Tc (K)

Hc1 (mT)†

Hc2 (T)

λ(µm)

ξ (nm)

κ

m∗ /m0

UPt3

0.48

0.7

1.8//c 2.3//a, b 10.2 2.5//c 10.5//a 2.1//a 2.5//c

1

12//a, b 14//c 9.5 7.5//a 13//c

90

180

UBe13

0.87

6.7

URu2 Si2

1.2

0.2

CeCu2 Si2

∼1

∼2.5

∼1 ∼1 0.5

9

55

260

260

140 380

Reproduced from the website of Zbigniew Koziol http://www.iyp.org/vp/super/heavy/reference.html. † the value is estimated.

c = 9.94 Å

Si Cu Ce a = 4.10 Å

Figure 2.21

Structure of CeCuSi.

MgB2 SUPERCONDUCTOR

53

one ascribes the high density of states to the high effective mass. Hence the name referred to above. Clearly, this property carries over to other physical characteristics as well. The electronic specific heat is directly proportional to the effective mass. Hence the electronic specific heat is hugely increased compared to that of usual metals. In the superconducting state the penetration depth λ is proportional to (m∗ )1/2 . Hence this quantity is also very large, as seen in Table 2.8. Other heavy fermion superconducting compounds not included in the table are Ce3 Bi4 Pt3 , CeNi2 Ge2 , UPd2 Al3 and YBiPt. Recent research in heavy fermion superconductors indicate that they are a quite diverse group, showing distinctly non-universal behaviour. Some, like UPd2 Al3 exhibit coexistence of long-range antiferromagnetic order and a Landau Fermi-liquid phase in a range Tc < T < TN . Another group, like CeCu2 Si2 (see Figure 2.21), are intermetallics that show pronounced deviations from Landau Fermi-liquid behaviour, due to fluctuations in the local magnetization. For these and other reasons heavy fermion superconductors are still an active area of research. It is still not clear whether a generalized Fermi-liquid theory can be found to describe all superconductors in this class.

2.8

MgB2 superconductor

Magnesium diboride, MgB2 , is a metallic compound known since the 1950s. It is a hard and brittle material with a hexagonal structure, as seen in Figure 2.22, with magnesium located in the external corners and in the face centre positions of the upper and lower hexagon, and with boron located in the inner hexagon, rotated by 60◦ with respect to the Mg hexagons. Superconductivity in MgB2 was discovered as late as 2001 [35, 36], with Tc at 39 K, a record by far in an ordinary metallic compound. This value of Tc is close to what has been considered the maximum possible by pairing caused by electron–phonon interaction. MgB2 has several interesting physical properties.

B Mg

Figure 2.22 Structure of MgB2 superconductor.

A15-phase

Nb3 Ge Nb3 Sn V3 Si

Charge transfer salt Bechgaard salts, spin density wave

Non-cuprate perovskite

κ − (BEDT − TTF)2 Cu(NCS)2 (TMTSF)2 X X = ClO4 , PF6 , ReO4

Ba1−x KBiO3 ; x = 0.4

Perovskite high-Tc cuprate superconductors

Fullerene based

K3 C60 Rb3 C60 Pb2.7 Tl2.2 C60

La2−x Bax CuO4 ; x = 0.2 YBa2 Cu3 O7−δ Bi2 Sr2 Ca2 Cu3 O10 TbBa2 Ca2 Cu3 O9 HgBa2 Ca2 Cu3 O8+δ

Heavy fermion compounds

UPd2 Al3 CeCu2 Si2 UPt3

LaMo6 Se8

Chevrel phase: Mo-based chalcogenides

Layered non-cuprate

MgB2

PbMo6 S8

Category

Superconductor

30 93 110 123 133

Tc (K)

3.3 2.5 2.9 1.3

190

ξab

17–32 38

∼40 ∼2 1.9

5

60

39 24 23

19–40

Bc2 (T)

115 198

Bc2 (T)

30

8.7–10.5 0.9–1.4

19.3 29.6 45

0.46

2.0

11

15.2

23.2 17.9 17.0

39

Tc (K)

0.5 0.09

ξc

λab

500 480 3500

290 150 173 130

λc

980

240

∼3 ∼2 ∼1–10

600

215

90 65 60

85–180

λ(nm)

12–14

2.2

3 3 3

2–5

ξ (nm)

Table 2.9 Special properties of some superconductor categories

High Tc , high Bc2 , extreme Type II, anisotropic layered

Special properties

Record Tc for non-cuprate perovskite

Organic, quasi-2D Organic, quasi-1D

Organic, high Tc , molecular based

High carrier mass: m ∼ 102 me

High Tc , high Bc2

High Tc , lattice instability

Record Tc for BCS-type metal

Special properties

54 SUPERCONDUCTING MATERIALS

SUMMARIZING REMARKS

55

In addition to the high Tc -value, it has been found to have two quite distinct energy gaps caused by pairing involving electrons from different parts of the Fermi surface. The high Tc value is a compromise between the two gap values. The high Tc is favoured both by the light element boron and by strong covalent binding. The isotope effect reflected in the dependence of Tc on isotope mass is a strong indication of BCS type electron–phonon pairing mechanism. The most important phonon modes involved in the pairing are in the B-planes. The upper critical magnetic field Bc2 has not been determined with any accuracy yet. Values as high as 32 T have been reported, but much lower values have also been found. MgB2 shows promise for several applications including transport of high currents and Josephson junctions. Several other compounds of related composition have been found, but all with lower Tc than MgB2 .

2.9 Summarizing remarks In this chapter we have attempted to review some basic facts about the most important materials in superconductivity research and applications today. Necessarily such a review will be sketchy, considering the vast literature available on these subjects. Essentially, this chapter can only be an appetizer for a deeper look into this immensely rich area. Still, it is hoped that it may be sufficient for those students who want to get a broad overview, but who do not necessarily intend to pursue the subjects at a much deeper level. Finally, in Table 2.9 we summarize some special properties associated with different categories of superconductors, so that the reader can in one glance get an idea about how they differ in some important respects.

3 Fermi-Liquids and Attractive Interactions 3.1 Introduction In solid state physics, The Theory of Everything is given by a Hamiltonian of electrons moving more or less freely through a lattice of ions. Electrons and ions have a kinetic energy, and they interact with each other via the Coulomb interaction. This Hamiltonian is in some sense trivial, it is simply the sum of potential and kinetic energies. However, as we know, the amazing number of different phenomena taking place in condensed matter physics goes to show that trivial Hamiltonians need not exhibit trivial ground states. Superconductivity is an example of this. Another notable example is the fractional quantum Hall effect. The main difficulty is to be able to identify correctly the manybody renormalized low-energy excitations in various circumstances. This is what is non-trivial, and the excitations vary enormously, ranging from bosonic spinwaves in Mott–Hubbard insulators and quantum Heisenberg antiferromagnets to fermionic bogoliubons in superconductors via anyonic excitations with fractional charge in the fractional quantum Hall effect. These systems all have the same underlying microscopic Hamiltonian, and the diversity of the possible low-energy excitations basically reflect that they are emergent long-wavelength properties whose basic characteristics to some extent are a result of the initial conditions in which we have prepared the underlying electron-ion system. The grand unified theory of solid state physics is given by the Hamiltonian H = He−e + Hion−ion + He−ion

(3.1)

where He−e is the Hamiltonian for electrons moving through the solid, Hion−ion is the Hamiltonian for the ions in the solid, and He−ion is the Hamiltonian describing the coupling between the electrons and the ions. For electrons with Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

58

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

mass m and ions with mass M, we have He−e =

p2 e−e i + VCoulomb (ri − rj ) 2m i

Hion−ion =

i

He−ion =

i,j

Pi2 2M

+

e−ion VCoulomb (ri

ion−ion VCoulomb (Ri − Rj )

i,j

− Rj )

(3.2)

Here ri denotes an electron-position, while Ri denotes an ion-position. The dominant effect of the Coulomb interactions between the ions is to freeze them into a lattice. Once we have assumed the existence of this ion-lattice ion−ion ground state, VCoulomb (Ri − Rj ) has performed its principle task and we no longer need to consider it. In a perfect solid with no lattice defects and no lattice vibrations, the electrons may be considered as moving in an external periodic potential set up by the ions. Ignoring electron–electron interactions, this is basically a one-body problem of an electron moving in a periodic external potential. The exact eigenstates are Bloch-states. These states are adjusted to the perfect lattice and are not scattered at all, a perfect crystal is transparent to Bloch-electrons. Including lattice vibrations around equilibrium positions of the ions, but still no lattice defects, the Bloch-states will couple to the lattice vibrations, whose quantized excitations are bosonic phonons. We then need to include coupling of Bloch-electrons to phonons. Finally, we should include Coulomb-interactions between electrons. Hence, a sensible way of viewing the above Hamiltonian in the absence of lattice defects (we shall ignore such site-disorder) is that of Bloch-electrons with Coulomb-interactions coupled to phonons. This is the situation we shall consider. We start by describing electrons ignoring interaction effects altogether, then modify the description in the nece−e essary fashion when VCoulomb (ri − rj ), and finally include the electron-phonon interaction. In this chapter, we will give a brief introduction to the concept of Landau Fermi-liquid theory, which forms the cornerstone of our current understanding of ordinary metals. We will also present the effective Hamiltonian for phonon-mediated superconductivity, which forms the basis for the celebrated BCS theory of conventional low-temperature superconductivity arising out of good metals. The Fermi-liquid theory is a spectacularly successful framework which transforms the daunting problem of interacting electron systems into a theory which conceptually is almost as simple as the non-interacting electron gas. We will also give a brief review of why such a drastic simplification of the problem actually works, even in extreme cases like the heavy fermion compounds. The accepted theory of conventional phonon-mediated superconductivity we have available today for superconductivity (namely the BCS theory,

THE NON-INTERACTING ELECTRON GAS

59

named after the originators of the theory, Bardeen, Cooper, and Schrieffer [7]), basically assumes that the interacting electron gas forming the metal that ultimately becomes a superconductor, exhibits well defined electron-like excitations that can form Cooper-pairs. Theories for superconductivity based on metallic states which do not exhibit such electron-like excitations have been proposed, notably in the context of attempting to explain high-temperature superconductivity in copper oxides. None of them have so far achieved what the Fermiliquid-based BCS theory did in such a brilliant manner–to make predictions for a complicated many-body problem, with right numbers. The Fermi-liquid theory, and the BCS theory, which we will introduce the reader to in this chapter, are certainly two of the most successful theories in condensed matter physics ever.

3.2 The non-interacting electron gas The language we will use to formally describe manybody systems in this book, is second quantization, mainly due to its convenience in the context of manybody systems with non-definite number of particles. This is precisely the situation which is forced upon us for superconductors. The basic building blocks of this formalism, are the annihilation- and creation-operators for electrons with linear † momentum k and spin σ . The operator ck,σ creates a state of an electron in a plane-wave (or Bloch-state) and spin state with quantum numbers (k, σ ), while ck,σ destroys such a state. The fact that electrons are fermions obeying the Pauli principle is is taken into account by postulating anticommutation relations for these operators, namely † † ck ,σ + ck ,σ ck,σ = δk,k δσ,σ ck,σ

(3.3)

where the δ-symbols are Kronecker-deltas, δα,β = 1 if β = α, and δα,β = 0 otherwise. In this language, the operator that counts the number of electrons in a given state defined by the quantum numbers (k, σ ) is given by the operator † nk,σ = ck,σ ck,σ . The Hamiltonian of a non-interacting electron system of states (k, σ ) where the energy of such states is given by εk,σ , is simply the energy per state multiplied by the number operator of such states, and finally summed over all states. Normally, we assume that the energies are independent of σ , i.e. we have εk . Then, the Hamiltonian is given by H =

† εk ck,σ ck,σ

(3.4)

k,σ

The ground state of this system is given by filled states (k, σ ) up to the Fermimomentum kF , where we denote the energy of the uppermost filled state by εF .

60

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

This Fermi-sea is completely inert in the absence of interactions, and we will denote this ground state by |φ0 . It has the important property that nk,σ |φ0 = (εF − εk )

(3.5)

where the Heaviside step function has the property (x) = 1, x > 0, (x) = 0, x < 0. Physically, the above is simply a statement that in the ground state of the non-interacting electron gas, all levels below the Fermi-level are occupied with (maximal) occupation number equal to 1 per spin state in accordance with the Pauli principle, all states above the Fermi-level are unoccupied. An extremely important quantity in a many-particle system is the probability amplitude of finding a particle in a state (k , σ ) at time t , given that it was in state (k, σ ) at time t. This quantity is the so-called single-particle propagator, or Green’s function, of the system. For the non-interacting case we will denote it by G0 (k, k , t − t ) = G0 (k, t − t )δk,k

(3.6)

It plays a central role in describing the electronic structure of any manybody electron system. The right hand side of the relation above follows from the fact that in a non-interacting system, a particle cannot be scattered out of a planewave state defined by a wavenumber k. Note also that G0 only depends on t and t only via the combination t − t when H is time-independent. Mostly, it is convenient to work with the Fourier-transform of the above quantity, namely ∞ dteiωt G0 (k, ω) G0 (k, ω) = −∞

=

1 ω − εk + iδk

(3.7)

where δk = δsign(εk − εF ), and δ is an infinitesimal positive quantity. The pole in the propagator is given by ω = εk − iδk , which defines the spectrum of the single-particle excitations of the system. The imaginary part plays the role of a damping term for the excitations, i.e. an inverse lifetime. In the freeelectron case, this damping term is infinitesimal in the free-electron gas, i.e. the excitations of energy εk are infinitely long lived. The imaginary part of G0 (k, ω) gives the single-particle spectral weight 1 δk 1 A(k, ω) = − [G0 (k, ω)] = = δ(ω − εk ) π π (ω − εk )2 + δk2

(3.8)

which provides direct information on the occupation of a plane-wave state |k of energy ω. Hence, the momentum distribution n(k) of the free electron gas is given by A(k, ω) integrated over all frequencies ω, while the k-space sum of

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

61

A(k, ω) gives the density of states D(ω). At zero temperature n(k) is given by the Fermi-Dirac distribution function n(k) = (εF − εk ) Note that the magnitude of the step-discontinuity in this momentum distribution function is 1 at the Fermi-level. Going back to Eq. 3.7, we see that this value of the discontinuity happens to be the same as the value of the residue at the pole of the free-electron propagator. As we shall see below, this is not a coincidence.

3.3 Interacting electrons, quasiparticles and Fermi-liquids When spin-independent pairwise-interactions between electrons are taken into account (we ignore multibody interactions, as usual), the Hamiltonian includes a two-particle scattering term where two incoming electrons in states k, σ and k , σ are scattered to states k + q, σ and k − q, σ with a matrix element V which in principle depends on the initial scattering states and the momentum transfer q in the process. We assume that the two-particle scattering is elastic. Thus, we may under quite general conditions write the total Hamiltonian as follows † † H = εk ck,σ ck,σ + Vk,k ,q ck+q,σ ck† −q,σ ck,σ ck ,σ (3.9) k,k ,q,σ,σ

k,σ

A typical term in the interaction term of the Hamiltonian is illustrated in Figure 3.1. For such an interacting system, a rather remarkable fact is that we can again write down an exact expression for the single-particle propagator, denoted by G(k, t), i.e. the probability amplitude that if a particle is found in state |k, σ at time 0, it will still be found in this state at time t. This expression is known k + q, s

k′ − q, s′

q

k, s

k′, s ′

Figure 3.1 A typical two-body scattering event contributing to the interaction part of the Hamiltonian, Eq. 3.9. The dashed line connecting the electrons is an illustration of Vk,k ,q denoting some effective interaction, such as Coulomb-interaction, phonon-mediated electronelectron interaction, and soforth.

62

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

as Dysons equation, and is given by, when expressed in terms of the Fouriertransform of G(k, t) G−1 (k, ω) = G−1 0 (k, ω) − (k, ω)

(3.10)

where (k, ω) is the so-called one-particle irreducible self-energy. In general, this is a complex quantity. It has the following physical interpretation: The real part of (k, ω), R = ( (k, ω)), gives a reactive shift of the excitation spectrum of the interacting electrons, such that this spectrum is given by ε˜k = εk + R . The imaginary part, I = ( (k, ω)) essentially gives the inverse lifetime of the interacting electron in the plane-wave state k, σ , i.e. I ∼ τk−1 , where τk−1 is the lifetime of the electron in the state |k, σ . Let us work this out in more detail. Inverting Eq. 3.10, we have G0 (k, ω) 1 − G0 (k, ω) (k, ω) 1 = ω − εk − (k, ω)

G(k, ω) =

(3.11)

where we have ignored δk in the free electron propagator compared to the imaginary part of , which we anticipate to be finite. We now want to bring this onto a form such that it resembles, as much as possible, Eq. 3.4 for the free-electron propagator. We imagine that, in some sense, the interactions are not ‘too strong’, and write the complex self-energy on the form = R + i I , and assume that the imaginary part (the damping-piece) is small compared to the real part (the reactive-shift piece), | I |/| R | 1. The pole in G(k, ω) determines the exact single-particle excitation spectrum of the interacting system. This spectrum is therefore determined from the equation ω − εk − R (k, ω) − i I (k, ω) = 0

(3.12)

To zeroth order, we ignore the imaginary part of . This gives the self-consistency equation for the reactively shifted single-particle spectrum ω = ε˜k = εk + R (k, ε˜k )

(3.13)

Taking into account a small imaginary part of means that the frequency giving the pole in the propagator is shifted, and this in turn implies that we have to Taylor expand the real part of around the frequency ω = ε˜k , as is evident from Eq. 3.13. Thus, we consider the real part of Taylor-expanded to first order around ω = ε˜k , as follows

R (k, ω) = R (k, ε˜k ) + (ω − ε˜k )

∂ R |ω=ε˜k ∂ω

(3.14)

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

63

On the other hand, since we are computing to first order in I , we consider the imaginary part of evaluated at ω = ε˜k . Let us now insert these expressions into Eq. 3.12. We obtain ∂ R |ω=ε˜k − i I (k, ε˜k ) = 0 ω − [εk + R (k, ε˜k )] −(ω − ε˜k ) ∂ω =ε˜k

∂ R (ω − ε˜k ) 1 − |ω=ε˜k − i I (k, ε˜k ) = 0 ∂ω

(3.15)

We now define the lifetime τk of the interacting electrons in state |k, σ , as well as the quantity zk by the following equations

(k, ε˜k ) 1 =− R τk 1 − ∂

∂ω |ω=ε˜k zk =

1 1−

(3.16)

∂ R ∂ω |ω=ε˜k

Inserting all of this in the exact expression for G, we find G(k, ω) =

zk ω − ε˜k +

i τk

(3.17)

If we compare Eq. 3.17 with Eq. 3.7, we see that the main effects of interactions between electrons are to produce a shift of the single-particle spectrum as well as a finite lifetime for the interacting electrons in a given plane-wave state. In addition, the residue of the propagator, the quantity zk , is reduced from the value 1 which it had in the non-interacting case. This is seen directly from Eq. 3.16, as

R on physical grounds is expected to be a decreasing function of frequency: At high energies, the effect of interactions is expected to be smaller than at low energies, because rapidly moving electrons have less time to interact with their surroundings than slow electrons. Hence, ∂ R /∂ω < 0, and thus zk < 1. Roughly speaking, it is as if the electrons in the non-interacting case have been degraded in the interacting case, only a remainder (a residue) less than one remains. What we are particularly interested in, is if this residue is non-zero on the Fermi-surface, i.e. if there is anything left at all of the single-particle excitations we had in the free case. More precisely, are there any remnants at all left of the non-interacting electrons, at low energies close to the Fermisurface, once interactions have been turned on? If there is, i.e. if zkF > 0, then we have some amount of well-defined low-energy single-particle excitations similar to the ones that are exact eigenstates in the non-interacting case. Such free-electron-like excitations are called quasiparticles. An interacting fermionic system with such quasiparticles is called a Fermi-liquid. Such single-particle

64

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS nk

1

zkF

kF

k

Figure 3.2 The zero-temperature momentum distribution nk of an interacting electron system. The magnitude of the discontinuity on the Fermi surface is precisely the quasiparticle residue. The dashed line is the momentum distribution of the non-interacting system, which has a discontinuity of magnitude 1 on the Fermi-surface.

like excitations are no longer exact eigenstates of the system, since interaction terms permit scattering in and out of Bloch-states. However, in a Fermi-liquid the quasiparticles are nevertheless defined well enough at low energies, at least, to enable us to consider them as bona fide electron-like excitations of the system. The momentum distribution which we in principle may obtain from the quasiparticle propagator given in Eq. 3.17 is illustrated in Figure 3.2. The important feature to note is the discontinuity of magnitude zkF on the Fermi-surface, the hallmark of a Fermi-liquid. The concept of quasiparticles in interacting fermion systems was first introduced by Landau in 1950. It has proven to be an enormously successful and important paradigm, basically forming the cornerstone of our understanding of metallic systems. The basic idea which underlies the Landau Fermi-liquid picture is that there is a one-to-one correspondence between the quantum numbers of non-interacting electrons and those of interacting electrons. This means that we may imagine that we start out with some simple Hamiltonian like Eq. 3.4, of which we know the eigenstates and eigenexcitations, and then perturbatively introduce interactions in the problem. When this is done, the resulting quasiparticles of the theory are obtained adiabatically from the excitations of the non-interacting system, and in particular the quantum numbers of the excitations in the interacting and non-interacting case are in one-to-one correspondence with each other. Although this may naively seem like a hopeless approach, it turns out to be a surprisingly robust framework when considering metals. Even in heavy fermion compounds, where interaction effects are so strong that one gets a renormalization of the bare electron mass by factors of order 1000, one still has not obliterated completely the residue of the electrons that exist in the noninteracting case. Examples of systems that do not conform to the Fermi-liquid paradigm exist, however. Notably, quasi-one dimensional organic conductors are not Fermiliquids. This is because interactions in one-dimensional systems constitute a

INTERACTING ELECTRONS, QUASIPARTICLES AND FERMI-LIQUIDS

65

singular perturbation to the free-electron case as a consequence of severely restricted Fermi-surface kinematics. As a result, forward scattering, which is innocuous in higher dimensions, is singular in one dimension and all vestiges of free-electron systems are destroyed as soon as interactions are switched on. The long-lived low-energy excitations in this case turn out to be bosonic in character, and are collective excitations in terms of the constituent electrons of the underlying system. Under such circumstances, there can be no one-to-one correspondence between the quantum numbers of the interacting case and of the non-interacting case. How can it be that an approximation that has all the appearances of a nonstarter, works so spectacularly well in most cases? Understanding the microscopics of the Fermi-liquid theory is not the main purpose of this book, so we mention it only briefly. It is however an important problem to understand, and for more details the reader is referred to the vast literature on the subject. What is absolutely crucial when one does any sort of perturbation theory, is to start with the right reference system. Why, then, is the non-interacting electron system a good and sensible starting point to perturb about, when the goal is to describe an interacting electron system? The reason is embedded in the Pauli principle. The number of states that an added particle to the system can scatter into, is severely limited by the Pauli principle, and this effectively suppresses the effect of switching on interactions. As a result, the free case is a good stable system to perturb around. It has the feature of having a finite compressibility in the ground state, and therefore collective modes, such as zero-sound, as well as thermodynamic quantities will change in a smooth manner when interactions are introduced. In contrast, this is not true for a bosonic system. For instance, noninteracting bosons do not support zero-sound, whereas the interacting system does. Hence, quantities do not evolve in a smooth manner as some interaction parameter is varied. Quite the contrary, the limit of zero interactions is a singular limit. So, the non-interacting boson system is not a good starting point to perturb around. The principal reason for why Fermi-liquid theory works is the kinematic restrictions imposed on the interacting system through the Pauli principle. This is all we shall have to say about this, for a more detailed exposition the reader may for instance consult the very nice review article by Varma et al. [37]. It should be emphasized here that in all of the above, we have assumed interactions to mean a repulsive interaction between electrons. This is very natural, in that the dominant interaction between electrons in condensed matter systems is the Coulomb interaction, whose Fourier-transform is given by a matrix element V of the type we considered in connection with Eq. 3.9, namely Vk,k ,q =

1 2π e2 4π ε0 q 2

(3.18)

In this case, V only depends on the momentum transfer q in the scattering process, not on the initial scattering states. However, as we shall see in the

66

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

next section, this is not the only source of interaction between electrons in a solid. For instance, electrons obviously interact with the ions of a solid as they move through it causing scattering of electrons and ions. These scattered ions may in turn interact with other electrons, thus mediating an effective electron–electron interaction. This phonon-mediated interaction turns out to be of a quite different nature than the photon-mediated Coulomb-interaction above. In particular, it has the property that in a thin energy-shell around the Fermi-surface, it is attractive. This feature alone suffices to produce an instability of the Fermiliquid. Attractive electron–electron interactions are singular perturbations to the non-interacting case.

3.4 Instability due to attractive interactions In the previous section, we established that the Fermi-liquid picture of interacting electrons is stable to repulsive interactions. In this section, we will start by investigating what happens to the Fermi liquid when an effective attractive interaction between two electrons is introduced as a perturbation to the noninteracting system. Later, we will show how a weak phonon-mediated interaction between electrons may produce a net attraction, even when the a priori dominant repulsive Coulomb interaction is accounted for.

3.4.1

Two electrons with attractive interaction

In this subsection, we will consider a rather artificial, but nonetheless extremely instructive problem, first considered by Leon Cooper. It exhibits in a lucid manner the dramatic effect an arbitrarily weak attractive interaction between electrons has, in stark contrast to a repulsive interaction. The Cooper problem is defined as follows. Consider the situation where we have an inert Fermi-sea, in which the electrons are treated as non-interacting. To this Fermi-sea we add two electrons above the Fermi-surface (by necessity). These two extra electrons do not interact with the inert Fermi-sea. They do however interact with each other, but in a very peculiar manner. The interaction is such that the two electrons attract if they both are within a small energy ω0 from the Fermi-surface, and on opposite sides of the Fermi-surface, otherwise they do not interact at all. In the absence of interactions, one electron occupies a plane-wave state |k, the other occupies the plane-wave state |−k. Let us denote the two-particle state of the two extra electrons in the absence of such a peculiar interaction by |k, −k, and in the presence of the interaction by |1, 2. Denoting the Hamiltonian of the system by H = H0 + Veff

(3.19)

H0 |k, −k = 2εk |k, −k

(3.20)

then we have

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

67

where εk is the single-particle excitation energy of the non-interacting fermion system (see Eq. 3.4). Note that due to the Pauli principle, we must have 2εk > 2εF in the presence of the inert Fermi-sea. This sea plays the role of providing blocking-factors for added states. Adding interactions, the exact Schr¨odinger equation for the (admittedly peculiar) two-particle problem defined above is given by H |1, 2 = E|1, 2

(3.21)

where E is the exact two-particle energy of the two electrons above the Fermisurface, in the presence of an attractive interaction. We assume that the states |k, −k form a complete set such that the exact two-particle eigenstate can be expanded in this basis, thus |1, 2 =

ak |k, −k

(3.22)

k

Our task is to obtain the expansion coefficients ak and finding the value of E. This will solve the Schr¨odinger-equation for the problem. Let us insert Eq. 3.22 into Eq. 3.21, obtaining (H0 + Veff )

ak |k, −k = E

k

ak |k, −k

(3.23)

k

We next project the resulting equation down on the adjoint states < k , −k |, where we have k , −k |k, −k = δk,k , in order to obtain a Schr¨odinger equation for the coefficients ak . Using the above orthogonality relation, we thus find ak [2εk − E] = −

ak k , −k |Veff |k, −k

(3.24)

k

The quantity k , −k |Veff |k, −k is basically a two-particle scattering matrix element for particles on opposite sides of the Fermi surface, from a two-particle state |k, −k to a two-particle state |k , −k . This scattering process is illustrated in Figure 3.3. So far, this is quite general, and we now specialize to the case where this scattering matrix element is of the somewhat peculiar nature described above, namely attractive in a thin shell around the Fermi-surface, and zero elsewhere. That is, we have k , −k |Veff |k, −k = −V ; |εk − εF | < ω0 = 0; otherwise

(3.25)

68

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

k

k′

−k′

−k

Figure 3.3 Scattering event of two particles maintained on opposite sides of the Fermisurface, scattered by the matrix element k , −k |Veff |k, −k which is operative in the thin shell around the Fermi-surface indicated by the dashed circles.

Then Eq. 3.24 takes the form ak [2εk − E] = V

ak (εk − εF )(ω0 − |εk − εF |)

(3.26)

k

The first -function ensures that the single-particle energies ε are above the Fermi-surface, the second one ensures that the effective attraction only is operative in a thin shell around the Fermi-surface. At this stage it is more convenient to go over to energy integrals instead of k-space integrals, by introducing the density of states D(ε), and viewing the expansion coefficients as functions of energy ε. Introducing the density of states D(ε) (the k-space sum of the spectral weight A(k, ε) obtained from G0 (k, ε) (see Eq. 3.8), as follows 1 δk 1 [G0 (k, ε)] = π π (ε − εk )2 + δk2 k k = δ(ε − εk )

D(ε) = −

(3.27)

k

where δ(ε − εk ) is a Dirac delta function, and we have used that limη→0 η/(x 2 + η2 ) = π δ(x). Noting that ak only depends on k via εk , we may write Eq. 3.26 as follows ∞ dε a(ε)δ(ε − εk )(ε − εF )(ω0 − |ε − εF |) a(εk )[2εk − E] = V =V

−∞ ∞ −∞

k

dεD(ε)(ε − εF )(ω0 − |ε − εF |)

(3.28)

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

69

We then obtain, upon renaming variables

εF +ω0

a(ε)[2ε − E] = V

dε D(ε )a(ε )

(3.29)

εF

The right hand side of Eq. 3.29 is seen to be independent of ε, and hence we immediately conclude that a(ε) must have the form a(ε) =

C 2ε − E

(3.30)

where C is some normalization constant. Its precise value will not be important, and we do not specify it further. Inserting the Ansatz Eq. 3.30 for a(ε) into Eq. 3.29, we find the self-consistent equation for the eigenvalue E 1=V

εF +ω0

εF

D(ε )dε 2ε − E

(3.31)

Utilizing the fact that we are considering a thin shell around the Fermi-surface, and assuming that the density of state D(ε) varies slowly, we may simply replace it by its value on the Fermi surface, D(εF ). Introducing the dimensionless coupling constant λ ≡ V D(εF ), we obtain 1=λ

εF +ω0

εF

dε 2ε − E

2(εF + ω0 ) − E = λ ln 2εF − E

(3.32)

We then introduce the energy difference between the states of two non-interacting particles on the Fermi-surface, and the exact energy eigenvalue E, i.e. = 2εF − E. In terms of this variable, Eq. 3.32 may be written 1 2ω0 = ln 1 + (3.33) λ Note that the way V is defined in Eq. 3.25, it is a positive quantity, hence λ is a positive quantity. Thus we see that in order for Eq. 3.33 to have a solution, > 0 is required. This means that E < 2εF ! This is a a quite dramatic result, since the basic starting supposition was that the inert Fermi-sea was completely filled up to the Fermi-level, and the two extra electrons lived above the Fermi-surface. Now, we have just reached the rather startling conclusion that an arbitrary weak attractive interaction leads to an exact two-particle state with a total energy lower than twice the Fermi-energy. What this indicates, is that the inert Fermi-sea is suffering some sort of collapse such that energy

70

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

states below the top of the Fermi-sea become accessible. At this stage, such an interpretation of the above result is merely a plausible conjecture. Confirmation of its physical soundness will have to await the analysis in the next chapter, where the full self-consistent treatment of all electrons in a thin shell around the Fermi-surface will be completed. Let us solve Eq. 3.33 for . We find =

2ω0 ≈ 2ω0 e−1/λ e1/λ − 1

(3.34)

where the last approximation follows if λ 1, i.e. if the effective electron– electron attraction is in some sense weak. Several remarks are now in order. First, we see that has an essential singularity as λ → 0. This means that the above result for could never have been obtained to any finite order in perturbation theory in λ. Hence, an arbitrarily weak attraction is a singular perturbation to a free electron gas. It destabilizes a Fermi-liquid. Secondly, we see that λ > 0 only if D(εF ) > √ 0. For a parabolic 2 2 band εk = k /2m in three dimensions, we have D(ε) ∼ ε. Hence, if the Fermi sea vanishes by draining electrons out of the system, λ → 0 and → 0. In other words, the tendency to pairing of electrons that we see above vanishes when the Fermi-sea vanishes. We should not expect a two-electron bound state for arbitrarily weak attraction in vacuum. Thirdly, if we were to reinstate in the problem, we would find = 2ω0 e−1/λ

(3.35)

This shows that the pairing is also a quantum effect, since the bound state energy gap vanishes when → 0, i.e. it vanishes in the classical limit. Last, but by no means least, we note that to the extent we choose to take the above results seriously (and we should), the fact that the two-electron bound state resides at an energy which apparently is prohibited by the Pauli principle, in a vague way hints at the fact that perhaps bound pairs of electrons are not as much slaves to the Pauli principle as are individual electrons. In fact, this is precisely true, as we will come back to in Chapter 4. By forming Cooperpairs, electrons can shed their fermion statistics. The resulting quantum fluid of Cooper-pairs is not as protected from interactions as are the Pauli principle loyal fermionic fluids. This is basically the root cause of why attractive interactions are able to destabilize the Fermi-liquid while repulsive interactions are virtually incapable of doing so in metallic states. Recall that when we briefly analyzed the microscopic foundations of Landau Fermi-liquid theory, we stated that the Pauli principle severely suppressed the effects of (repulsive) interactions, thus saving the electron-like quasi-particles from obliteration. For attractive interactions, the Pauli principle is essentially sidelined and no longer acts as a suppressor of interaction effects. This opens up the possibility of ground states qualitatively different from the free electron gas.

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

71

The resulting electron pair that we have described the genesis of in the above, is referred to as a Cooper-pair, named after Leon Cooper who had the audacity to consider the then outrageous problem of two electrons interacting attractively in the peculiar manner described above. Cooper’s calculation is truly remarkable in that when he performed it, there was no known mechanism by which electrons could interact attractively in solid states physics. As it turns out, the phenomenon of Cooper-pairing of electrons is at the heart of the phenomenon of superconductivity.

3.4.2

Phonon-mediated attractive interactions

In this section we will start with the Hamiltonian for electrons interacting with each other through the Coulomb interaction and add the coupling of electrons to phonons. A canonical transformation reduces this to an effective Hamiltonian with a modified electron-electron interaction that under certain circumstances could be attractive, despite the apparent complete dominance of the Coulomb-interaction compared to the weak electron–phonon couling. It is very much like David’s triumph over Goliath–intelligence and a sit of luck wins over brute force. Let us, before we start with formalities, give an intuitive picture of what is going on. The crucial point which facilitates the above rather remarkable result, is that heavy lattice ions are slow movers around their equilibrium positions compared to fast and light electrons. Hence, dynamic local lattice distortions arising from electron-ion collisions, remain long after the electron that caused them have passed. This phenomenon will be called retardation. A local lattice distortion gives rise to a small dipole moment that can interact with electrons. As a result, another electron in the vicinity of the local lattice distortion can be drawn towards it long after the initial electron has left the scene. As the electrons are far removed from each other, the repulsive Coulomb interaction is reduced. It is this ‘wait a little and see’ tactics that allows the electron–phonon coupling to circumvent the apparent insurmountable obstacles of the Coulombrepulsion. On the other hand, the second electron is not allowed to wait for a too long time before taking advantage of the local lattice distortion, since the latter eventually will decay as the ion settles around its equilibrium again. Hence the second electron has a limited amount of time at its disposal before moving in on the lattice distortion caused by the first electron. It therefore stands to reason that in order to reduce as much as possible the (for pairing purposes) adverse effects of the Coulomb-repulsion, the two electrons should put as much distance as possible between themselves per unit time. The best two-particle state for such purposes is a state where the two electrons occupy plane-wave states of opposite wavenumbers, i.e. they move in opposite directions. (Anybody who has ever been on an airliner between two major central European cities has experienced this by looking out the window of the aircraft and seeing another

72

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

airliner whizzing past in the opposite direction. They are out of sight in seconds, in contrast to those that fly in more or less the same direction, which can be followed for minutes.) This crude real-space picture already gives us a hint that Cooper’s calculation discussed in the previous subsection, while appearing quite artificial, in fact is precisely the right problem to consider. We now proceed to derive an effective electron–electron interaction, mediated by photons and phonons, which gives rise to the physics discussed above. The starting point is the second-quantized version of the interacting electron gas coupled to quantized lattice vibrations, or phonons. It is given by H=

† εk ck,σ ck,σ +

k,σ

Ve−ph =

k,k ,q,σ,σ

1 2π e2 † ck+q,σ ck† −q,σ ck,σ ck ,σ + Ve−ph 2 4π ε0 q

† † Mq (a−q + aq )ck+q ck

(3.36)

k,q,σ

where Mq is the matrix element for electron–phonon coupling. The operators (aq† , aq ) are creation and destruction operator for phonons, and satisfy the following commutation relations reflecting that phonons are bosons aq† aq − aq aq† = δq,q

(3.37)

Phonons are not material particles, and their number is not conserved in a solid. A typical electron-phonon scattering event is shown in Figure 3.4. In Eq. 3.36, we have assumed that one particular phonon-mode dominates the coupling to the electrons. Had we had several phonon-modes of equal coupling strength, we would have had to include a sum over phonon modes λ as well, in Ve−ph . The matrix element Mq may be expressed in terms of the eigenfrequencies ωq,λ of harmonic lattice vibrations and the Fourier-transform V˜e−ion (q) of k + q, s

q

k − q, s

Mq

M−q

k, σ

q

k, σ

Figure 3.4 Scattering events between electrons and phonons. In the left process, a phonon is absorbed by an electron causing recoil. In the right process, an electron emits a phonon causing recoil. In the latter case, the electron sets up a local dynamic lattice distortion. The vertex is denoted by a black dot and its strength is given by Mq .

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

73

the electrostatic electron-ion interaction as follows (when also a phonon-mode index λ is included) Mq,λ = i(q · ξ λ ) (3.38) V˜e−ion (q) 2Mion ωq,λ where Mion is the ion-mass and ξ λ is a unit vector giving the direction of the lattice-vibration mode λ. It is difficult to compute Mq,λ with any precision from first principles, and we will simply take this matrix element as some parameter. This coupling is much weaker than electron–photon coupling. Note also that limq→0 Mq,λ = 0. The fact that Mq,λ ∼ q reflects the fact that the electron-phonon coupling is a coupling between a point charge and a dipole moment. Let us see how we can transform the electron-phonon coupling into an effective electron-electron interaction in a fairly simple manner. Note that the interaction in Figure 3.1, when viewed as a Coulomb-interaction, may be considered as obtained from two scattering events as those depicted in Figure 3.4, but where the dashed lines are photons and not phonons, and where the scattering vertex has strength e, the electron charge, and not strength Mq . In Figure 3.1, we then interpret the dashed line between the electrons as a free-photon propagator. Since electrons are virtually at a standstill compared to photons, this interaction is non-retarded and we may ignore the frequency dependence of the photon-propagator. Under such circumstances, the photon propagator is nothing but the static Coulomb-interaction. We may proceed precisely along the same lines when phonons are involved. We obtain an effective electron–electron interaction by taking the two scattering events in Figure 3.4 and forming a two-particle scattering term as in Figure 3.1. We then interpret the dashed line connecting the electrons as a free phononpropagator. Free phonons have the Hamiltonian H = ωq aq† aq (3.39) q

where ωq is the eigenvalue of a phonon in a plane-wave state |q. The explicit expression for the free phonon-propagator D0 (q, ω), which has the same interpretation as the propagator for electrons, is given by D0 (q, ω) =

ω2

2ωq − ωq2 + iη

(3.40)

where η is a positive infinitesimal quantity. Using this, we obtain the phononmediated part of the electron–electron interaction Veff (q, ω) =

2|Mq |2 ωq ω2 − ωq2

(3.41)

74

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

In the above, q is the momentum transfer in the electron-electron scattering process, while ω is the energy transfer. Electrons are by no means at a standstill in solids compared to the velocity of sound waves. Thus, we cannot ignore the frequency dependence of this part of the electron–electron interaction. The result of all of the above is that Eq. 3.36 may be written on the form of a purely electronic system where the trace of the phonons is manifest in the additive contribution they give rise to in the electron-electron interaction, as follows H=

k,σ

V˜eff (q, ω) =

† εk ck,σ ck,σ +

k,k ,q,σ,σ

2|Mq |2 ωq 1 2π e2 + 4π ε0 q 2 ω2 − ωq2

† ck† −q,σ ck,σ ck ,σ V˜eff (q, ω)ck+q,σ

(3.42)

Note that when ω2 < ωq2 , the phonon-mediated piece of the electron–electron interaction is negative, i.e. it is attractive. This in itself does not mean all that much, the issue is if this attractive piece can overcome the manifestly repulsive piece originating in the Coulomb-interaction. In fact, it is easy to see that it can, at least for some momentum transfer and energy transfer. We note that as ω2 approaches ωq2 from below, the phonon-mediated piece of the interaction formally diverges! Hence, it does not matter how small |Mq |2 is, the phononpiece will always be able to overcome the Coulomb-piece. The physics of this is precisely what was alluded to in the introduction to the section. Namely, by waiting for a time which is of order the time-scale of the lattice vibrations, an electron may come in and be dragged towards a local lattice distortion caused by an electron passing the site at some earlier time. This minimum waiting time corresponds to the upper frequency cutoff. In Figure 3.5, a sketch of V˜eff (q, ω) is given as a function of frequency ω at fixed finite momentum q, the figure on the left. Note that when ω is close enough to typical phonon-frequencies ωq the total effective interaction is positive. For all ω2 > ωq2 it is repulsive, and this is also the case for too small ω2 . This latter fact is what we alluded to in the introduction to this subsection, namely that the electron can not wait for too long a time before taking advantage of the local lattice distortion. Thus, the effective attraction we see for not too small and not too large frequencies, is basically the Fourier-spacetime version of the “wait and see” tactics described at the start of the section. The figure on the right in Figure 3.5 is an idealized and simplified version of V˜eff (q, ω). We ignore entirely the repulsive part of the interaction, since we expect the effect of repulsive terms to be suppressed by the Pauli principle as discussed in the previous section. The attractive part is extended to all frequencies ω2 < ωq2 , and is moreover taken to be a constant independent of ω in this range. This simplification is the one that was originally considered by Bardeen,

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS Veff

Veff

w

−wq

75

wq

w

−wq

wq

Figure 3.5 The left figure shows V˜eff (q, ω) at fixed q as a function of ω. The right figure shows a much simplified version of it.

Cooper, and Schrieffer in their seminal 1957 work on phonon-mediated superconductivity [7]. It is an extreme simplification, but nonetheless yields results that are in spectacular agreement with experiments. While the agreement with experiments (to within a few percent for studiously chosen quantities) may have been a source of some surprise at the time, given the crudeness of the approximation of V˜eff (q, ω), we now understand why this is so. The point is that the simplified interaction contains the essential feature of the more realistic V˜eff (q, ω), namely attraction in a certain frequency range close to typical phonon-frequencies. What other details are left out are not all that important, the validity of the results obtained is virtually guaranteed by the principle of universality: Certain physical properties do not depend on tiny details of the microscopic Hamiltonian. All we need to do is to derive some effective description and compute properties from this, and we get the right results (if we focus on the right properties!). In the next chapter, we shall compute some results that come out right due to universality, and we shall also compute one notable quantity which definitely does not.

3.4.3

Reduction of the effective Hamiltonian

Let us next proceed to further simplifying the Hamiltonian Eq. 3.42. The simplifications we will make are expected to be sensible provided that the frequency range where V˜eff (q, ω) is attractive in a tiny energy range compared to the Fermi-energy, i.e. the shell around the Fermi-surface in Figure 3.3 is exceedingly thin compared to the radius of the Fermi-sphere. The implication of this is that when the frequency range of attraction is narrow, the phase-space for scattering such that the attractive interaction is felt, is maximized by having both the initial and final two-particle states within the thin shell. The energy transfer in the scattering process caused by V˜eff (q, ω) is ω = εk − εk+q = εk − εk −q . All energies (εk , εk , εk+q , εk −q ) must lie within a thin energy shell around the Fermi-surface if the initial and final two-particle states are to contain electrons that attract each other. What values of (k, k , q) in Eq. 3.42 will ensure

76

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

q

q k1 k2

k1 −q

k2

−q

Figure 3.6 Phase-space of two-particle scattering within a thin shell of the Fermi-surface. There is only one situation where both the initial and scattered states are within the thin shell, provided one of the initial and one of the scattered states are, and that is if the initial momenta are on opposite sides of the Fermi-surface.

this? The interaction term describes scattering of initial state |k, σ to state |k + q, σ > and scattering of the state |k , σ to state |k − q, σ . What relation between (k, k ) ensures that if |k + q, σ is a state within the energy shell, then so is |k − q, σ for all q? The answer is that this occurs if k = −k (see Figure 3.3), and this maximizes the phase-space for scattering of attractively interacting states. Hence, we will keep only such terms in Eq 3.42. The situation is also illustrated in Figure 3.6. Consider two electrons in momentum states k1 and k2 , both within a thin energy shell around the Fermisurface. Suppose one electron is scattered into momentum state k1 + q and the other into k2 − q. If the total momentum of the initial and scattered states is k1 + k2 = Q, then we see from the left figure that in general, one of the scattered states will not be within the thin shell even if the other is. There is only one situation that guarantees that both the scattered states are within the thin shell if one of them are, and that is if k1 + k2 = 0. This situation will tend to dominate the contribution to the scattering phase space, given that the twoparticle scattering matrix element is operative only if both of the initial and final states are within this thin shell. This domination becomes progressively more pronounced the thinner the shell is. If we dispensed with retardation altogether, and considered the scattering matrix element to be operative over the whole electronic band, then the above reduction into opposite momentum states is more questionable. Nonetheless, with the recent renaissance of purely electronic pairing mechanisms invoked in attempts of explaining such phenomena as superconductivity in high-Tc cuprates, the reduction is often used. Mostly out of old habit and with little or no justification. In the case of phonon-mediated attraction, the approximation is however on quite firm ground. Moreover, we expect the attractive interaction mediated by phonons to be of short range. Thus, electrons should be allowed to approach each other closely in space (although they avoid each other in time). Due to the Pauli principle, it is therefore plausible to suggest that the electrons that can approach each other in space most easily are such electrons that are in opposite spin states. Therefore, we also set σ = −σ . Setting k = −k, σ = −σ , and redefining k + q → k, k → k in the interaction term of the effective Hamiltonian, Eq. 3.42 may be

INSTABILITY DUE TO ATTRACTIVE INTERACTIONS

written on the form † † † H = εk ck,σ ck,σ + Vk,k ck,σ c−k,−σ c−k ,−σ ck ,σ k,σ

77

(3.43)

k,k ,σ

where Vk,k is an attractive two-particle scattering matrix element which is operative if both k and k are within a thin shell around the Fermi-surface. Eq. 3.43 is the celebrated BCS-reduced Hamiltonian forming the starting point for discussing phonon-mediated superconductivity. In Figure 3.7, we also provide a real-space illustration of a Cooper-pair of two electrons moving in a lattice, where we have in mind a phonon-assisted pairing mechanism (the only really known pairing mechanism to date). The electrons move approximately linearly in opposite directions and in opposite spin-states. Each electron leaves behind a trail of lattice distortions as it moves through the lattice, which the other electron can feel and be attracted towards via the matrix element Eq. 3.38. In order to maximize the attraction, it is advantageous for the electrons to move co-linearly, since this maximizes the time the electrons spend close to lattice distortions while at the same time being mobile. Moreover, moving in precisely opposite directions puts maximum distance between the two electrons per unit time, thus minimizing the adverse effects, for pairing-purposes, of the repulsive Coulomb-interaction. The above is a rough real-space version of the k-space arguments given in the previous paragraph. It clearly illustrates that Cooper-pairing is a k-space phenomenon, not a pairing phenomenon in real-space.

Electrons

Figure 3.7 Real-space representation of a Cooper-pair with phonon-mediated superconductivity. The black dots are lattice ions unperturbed by the motion of the electron through the lattice. The hatched dots are lattice ions that have been displaced slightly by the electrons passing close by. Since the ions are heavy and slow, the local lattice distortions remain long after the electrons have passed. An electron moving in precisely the opposite direction can now take full advantage of the extended line of distortions, more so than an electron crossing this line. Thus, phonon-mediated electron–electron attraction is maximized for electrons in opposite linear momentum states. Moreover, such states also minimize the adverse effects of Coulomb-repulsion, since the two electrons then put a maximum amount of distance between themselves in a minimum amount of time.

78

FERMI-LIQUIDS AND ATTRACTIVE INTERACTIONS

In metals, electrical resistivity has many sources, among them electron–phonon coupling, but also scattering of electrons off impurities. In very clean metals with low density of lattice defects or other sources of point-like or extended impurities, one might expect the electron–phonon coupling to dominate the contribution to the scattering. Provided the pairing mechanism we have described in previous sections is the source of superconductivity, the source of resistivity and superconductivity is basically one and the same scattering mechanism. This immediately gives some insight into a fact which seems to be borne out in most cases, namely that good metals become superconductors only at low temperatures. While mercury has a room temperature resistivity of 98 × 10−8 m and critical temperature of about 4.2 K, copper, the archetypical good metal, has a room temperature resistivity of 1.7 × 10−8 m and critical temperature which is in the millikelvin range. There really is no theory available to us that allows us to compute Tc from known experimentally accessible normal state properties with any great precisions. What we have, as we shall see in the next chapter, are rough estimates in terms of an electron–phonon coupling constant for which one has some crude estimate. It will turn out, however, that the critical temperature is exponentially sensitive to this couling constant, and hence great variation in Tc are expected. Paradoxically, therefore, we would expect the largest superconducting critical temperature in a poor metal! This goes to show that superconductivity is much more than just perfect conductivity. We already know this, of course, because the Meissner effect is a defining property of a superconductor which obviously has no counterpart in a perfect free electron gas with zero resistivity. The physical consequences of the Meissner effect have been mentioned, and will be elaborated on in much more detail in the chapters to follow.

5:48 pm, 6/26/05

4 The Superconducting State – an Electronic Condensate 4.1 BCS theory: a magnetic analogue We have seen in Chapter 3 that the effective Hamiltonian for electrons interacting attractively (by some mechanism) when two electrons are in opposite spin-states and states of opposite linear momentum, is given by the BCS reduced Hamiltonian † † † H = εk ck,σ ck,σ + Vk,k ck,σ c−k,−σ c−k ,−σ ck ,σ (4.1) k,σ

k,k ,σ

It is possible to recast the effective BCS Hamiltonian into a language reminiscent of what we are acquainted with for the Heisenberg model for magnetic insulators, using the so-called Anderson pseudospin formalism. Such pseudospin formalisms have subsequently been used extensively in the context of a number of physical phenomena, such as the bi-layer quantum Hall effect, to mention one example. We have seen in the previous chapter, that the effective Hamiltonian capturing the essentials of conventional phonon-assisted low-Tc superconductivity, is given by H =

k,σ

† εk ck,σ ck,σ +

k,k

† † Vk,k ck,↑ c−k,↓ c−k ,↓ ck ,↑

(4.2)

where the interaction term represents scattering of two-particle spin-singlet states on opposite sides of the Fermi-surface. We now recast this into the form of a (pseudo)spin-Hamiltonian, where it will become evident that superconducting off-diagonal long-range order is equivalent to pseudo-magnetic ordering, which is more familiar to us in that it at least has a classical counterpart. (Throughout Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

80

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

this chapter, we work with units such that = 1). We introduce the standard Pauli matrices τ1 , τ2 , τ3 , as well as the spin-lowering and raising operators τ ± = τ1 ± iτ2 . Next, we introduce the operators τk1 , τk2 , τk3 , as follows † † τk3 = ck,↑ ck,↑ − c−k,↓ c−k,↓ † † τk+ = 2ck,↑ c−k,↓

(4.3)

Inserting this into the effective Hamiltonian (Eq. 4.2), we obtain H =

k

εk (τk3 + 1) +

1 Vk,k (τk1 τk1 + τk2 τk2 ) 4

(4.4)

k,k

Note that this has the form of an XY-Heisenberg Hamiltonian of spins in an external magnetic field in the z-direction. However, it should be noted that the usual labels for spin-sites on a real-space lattice is replaced by indices in Fourier-space. This just underscores that point that Cooper-pairing is a k-space phenomenon. The point that enormously simplifies the treatment of the above pseudo-spin Hamiltonian is that the original effective interaction matrix element Vk,k is essentially a contact interaction in real-space, and hence a long-range potential in k-space. Thus, van der Waals type mean-field arguments can be brought to bear on the problem, and we expect that a mean-field decomposition of the pseudo-spin Hamiltonian will yield excellent results. With longer range interaction in real-space, and hence shorter range interactions in k-space, fluctuation effects are expected to become more prominent. Moreover, we have tacitly assumed that the majority of the two-particle scattering events take place between electron pairs of zero total linear momentum, an approximation that is expected to be excellent as long as the phase-space for attraction is limited to a thin shell around the Fermi-surface. Hence, Eq. 4.4 is expected to be an effective Hamiltonian which is reasonable for the case where the interaction responsible for Cooper-pairing is retarded. Spontaneous symmetry breaking in this pseudomagnet occurs for the case where the pseudomagnetic field vanishes, i.e. for the case where we ignore the kinetic energy term. This magnetic analog leads us to choose the magnetization to be oriented in the 1–2-plane, and thus define an order parameter as follows † † τk1 = ck,↑ c−k,↓ + c−k,↓ ck,↑

(4.5)

The task now will be to derive a self-consistent mean-field equation for this pseudomagnetic order parameter. Before doing this, let us make a few general remarks. Note that if the order parameter exists, it implies that the particle number is not conserved in the ground state of the system. Global conservation of particle number is reflected

DERIVATION OF THE BCS GAP EQUATION

81

by a global U (1)-symmetry of the original effective Hamiltonian. Thus, we see that superconductivity really amounts to breaking a global U (1)-symmetry in the ground state of the interacting electron gas. In physical terms, this means that the superconducting ground state is a coherent superposition of states with different number of particles, however with a majority of the states containing a number of particles which is close to the number of particles one would have in the U (1)-symmetric normal metallic state. Going back to the magnetic analogue, we see that superconductivity is equivalent to obtaining spontaneous pseudomagnetization in the 1–2-plane. It is as if an XY-magnet has ordered. For this reason, and since the symmetry group U (1) essentially is isomorphic to the symmetry group O(2), it is often said that the normal metal-superconductor transition is in the universality class of the XY-model. As we shall see later, while this statement is correct for the superfluid to normal fluid transition in H e4 , it is strictly speaking not correct in the case of a superconductor, which has a charged condensate. If the condensate has a charge, it means that it couples to an electromagnetic vector potential, a gauge-field. This elevates the symmetry of the system to a local U (1) symmetry, as opposed to the global U (1) symmetry of the XY model describing a superfluid. The presence of a gaugefield in the problem in principle alters the interactions, and hence also some critical properties. In many cases, the differences are, however, unobservably small. Not only is the normal metal–superconductor transition strictly speaking not in the XY-universality class, but depending on the value of the Ginzurg–Landau order parameter, the transition may not even be a critical phenomenon, but a first order phase transition! What will transpire is that the demarcation between first order phase transition and second order phase transition√is given by the tricritical value of the Ginzburg–Landau parameter κtri = 0.79/ 2. It also turns out that this value is the fluctuation-corrected demarcation between type-I and type-II superconductivity!

4.2 Derivation of the BCS gap equation In this section, we compute the free energy of the superconductor in the mean-field approximation. The superconducting gap is found by minimizing the expression for the free energy as a function of the gap-parameter. We first proceed by reducing the effective Hamiltonian to a self-consistent one-body problem by first introducing expectation values of the creation- and annihilation operators for Cooper-pairs. We have justified this mean-field procedure above, in the context of the pseudo-spin formalism. We first define the c-numbers bk = c−k,↓ ck,↑ † † c−k,↓ bk† = ck,↑

(4.6)

82

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

such that we have c−k,↓ ck,↑ = bk + c−k,↓ ck,↑ − bk .

(4.7)

δbk

We next insert this into the effective Hamiltonian and retain terms up to linear in δbk , ignoring terms of order O(δbk2 ). This gives † † † H = εk ck,σ ck,σ + Vk,k [bk† c−k ,↓ ck ,↑ + bk ck,↑ c−k,↓ − bk† bk ] (4.8) k,k

k,σ

This Hamiltonian is immediately simplified by introducing the superconducting gap-parameter, defined as follows Vk,k bk† †k ≡ − k

k ≡ −

Vk,k bk .

(4.9)

k

We the obtain an effective one-body Hamiltonian on the following form † † † † H = εk ck,σ ck,σ − [k c−k,↓ ck,↑ + k ck,↑ c−k,↓ − bk† k ] (4.10) k,σ

k

Note that because of presence of pair-production and pair-annihilation terms, Eq. 4.10 is not yet on the standard form of an effective non-interacting electron gas, and hence we cannot at this stage read off what the quasiparticle spectrum of Eq. 4.10 is. In order to achieve this, we perform a rotation of the basis to a set of new fermion operators that diagonalize this Hamiltonian, as follows. We introduce two new species of fermion annihilation operators (ηk , γk ) along with their corresponding creation operators, which are related to the original electron operators via the unitary transformation ck,↑ = cos(θ )ηk − sin(θ )γk † c−k,↓ = sin(θ )ηk + cos(θ )γk

(4.11)

and their corresponding adjoint operators. Inserting this into the Hamiltonian we obtain [εk + k bk† ] H= k,σ

+

[εk cos(2θ ) − sin(θ ) cos(θ )(k + †k )]ηk† ηk

k

−

k

[εk cos(2θ ) − sin(θ ) cos(θ )(k + †k )]γk† γk

DERIVATION OF THE BCS GAP EQUATION

−

83

[k cos2 (θ ) − †k sin2 (θ ) − 2εk sin(θ ) cos(θ )]ηk† γk k

† − [k cos2 (θ ) − k sin2 (θ ) − 2εk sin(θ ) cos(θ )]γk† ηk

(4.12)

k

We next proceed by choosing the value θ in such a way as to precisely diagonalize the Hamiltonian, i.e. such that only terms like ηk† ηk and γk† γk appear. This is achieved by choosing the following value of θ , upon ignoring phase-fluctuations in the complex order parameter entirely and setting k = †k tan(2θ ) = −

k εk

(4.13)

For such values of θ , we have 1 1− 2 1 cos2 (θ ) ≡ u2k = 1+ 2 sin2 (θ ) ≡ vk2 =

where Ek ≡

εk2 + |k |2

εk Ek εk Ek

(4.14)

(4.15)

Before we go further, it is appropriate to mention the factors vk2 and u2k which were introduced in Eq. 4.14. These are normally referred to as coherence factors. They play an extremely important role in the following sections where we will study ultrasound attenuation and nuclear magnetic resonance (NMR). Their existence was a prediction that came out of the BCS theory. It turns out that observed results for NMR and ultrasound attenuation in superconductors depend sensitively on these coherence factors, since in these two cases they conspire subtly and in entirely different ways. An even more subtle point is that, as we shall see, they conspire in different ways in transverse and longitudinal ultrasound attenuation! Bardeen, Cooper and Schrieffer [7] came up with predictions with correct numbers for these effects in a complicated manybody problem. This is undoubtedly one of the major triumphs of condensed matter physics of the 20th century. Using Eqs 4.14 in 4.12, we finally obtain the simple fermionic Hamiltonian which formally has the form of a free fermion quasiparticle gas H = [εk + k bk† ] + Ek [ηk† ηk − γk† γk ] (4.16) k,σ

k

The above Hamiltonian now has the form of a constant (mean-field) term H0 ≡ † k [εk + k bk ] plus the Hamiltonian for a spinless fermion system with two species of fermions, described by the operators (ηk† , ηk ) and (γk† , γk ), where

84

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

we can identify the quasiparticle excitation energies as (Ek , −Ek ) for the two species of fermions. Note that the two species of quasiparticle fermions are spinless since they are linear combinations of electrons and holes with opposite spins. Rather than having ↑-spin electrons and ↓-spin electrons as our degrees of freedom as in the metallic phase, we have two distinct linear combinations of particle-hole spin-singlets as our relevant degrees of freedom. Thus, the total number of degrees of freedom is conserved. The expression in Eq. 4.15 immediately provides a physical interpretation of k defined in Eq. 4.9. It appears as a gap in the quasiparticle spectrum on the Fermi-surface (where εk = 0), a gap which is present because the expectation value < c−k,↓ ck,↑ > is non-zero. This expectation value is essentially the order parameter of the superconducting state, as was made clear from the pseudo-magnet analog above, and hence we will refer to the gap k as the superconducting gap. Note that the gap strictly speaking is not precisely the same as the superconducting order parameter, by the definition (Eq. 4.9)! For one thing, the k-space structure of the two objects are different. However, they are both non-zero or zero simultaneously, and for this reason the gap in the quasiparticle spectrum may effectively serve as a bona fide order parameter, and in most cases this is in fact what is done. Since this now has the form of a free fermion gas, plus a constant term which does not contain fermionic degrees of freedom (the first term), it is elementary to write down the grand canonical partition function for the problem, which is given by

Zg = e−βH0 (1 + e−βEk )(1 + eβEk ) = e−βF k

H0 ≡ [εk + k bk† ].

(4.17)

k

This implies that the free energy F of the system is given by 1 F = H0 − [ln(1 + e−βEk ) + ln(1 + eβEk )] β

(4.18)

k

which has the form of a pure mean-field term plus the contribution to the free energy from a two-component effective non-interacting fermion gas. At zero temperature (β → ∞), the entropic contribution to the free energy vanishes, and Eq. 4.18 takes the form [Ek (−Ek ) + Ek (Ek )] F = H0 + k

= H0 +

[Ek (1 − (Ek )) − Ek (Ek )]

k

[εk + k bk† − Ek ] = k

(4.19)

DERIVATION OF THE BCS GAP EQUATION

85

where we have used the Heaviside step-function (x) = 1 − (−x), (x) = 0, x < 0, (x) = 1, x > 0. The gap k , which at this stage has the status of a variational parameter, is self-consistently determined by minimizing the free energy with respect to variations in k . We therefore demand that the following (equivalent) sets of equations be satisfied for the superconducting gap ∂F =0 ∂k ∂F =0 ∂†k

(4.20)

This mean-field requirement on the gap applies regardless of what the details of the k-space structure of the attractive interaction Vk,k is. One must remember that the above is a functional derivation such that only one term in the k-space sums are picked out when the derivation is performed. Applying the first of Eqs 4.20 to 4.18, we obtain bk†

∂Ek + ∂k

eβEk e−βEk − 1 + e−βEk 1 + eβEk

=0

(4.21)

or equivalently bk† = k

tanh(βEk /2) 2Ek

(4.22)

≡χ (k)

where χ (k) may be interpreted as a pair-susceptibility, i.e. the ability the system has to form Cooper-pairs. Using this explicit self-consistent relation between the order parameter bk and the gap parameter k in the definition (Eq. 4.9), we finally arrive at a self-consistent equation for k , namely the celebrated BCS gap-equation k = −

k

Vk,k k

tanh(βEk /2) 2Ek

(4.23)

As it is written here, it applies at the mean-field level to any superconductor, and as long as we do not specify the origin of the attraction, it is not limited to phonon-mediated superconductivity. Physically, we expect that in reality the detailed frequency spectrum of the ‘glue’-bosons does play some role in the phenomenon, but such details are left out of the above treatment. If we were to take such details into account, then we would arrive at a description which would be quite specific to the precise pairing mechanism we have in mind. The

86

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

lack of such details in the above mean-field theory is usually referred to as a weak-coupling approximation. The more sophisticated (but still mean-field!) description where the details of the specific spectra of the ‘glue’-bosons are taken into account, is usually referred to as Eliashberg theory, or strong coupling theory. We will not go into the details of this theory here, but simply state that the above picture of the superconductor as an electronic condensate is the basic picture in weak-coupling as well as strong-coupling theory. One remark is appropriate here. The phenomenon of Bose–Einstein condensation is well known, both in the context of cold dilute inert gases, as well as in the superfluid transition of H e4 . The basis for Bose–Einstein condensation even in ideal quantum gases is very much dependent on the fact that the basic constituents which condense are bosons that experience a statistical bosonic symmetry attraction. Electrons, on the other hand, obey the Pauli principle, which roughly may be viewed as a very brutal hard-core repulsion, rendering the pressure of even the ideal fermionic quantum gas finite at zero temperature, P = (4π 2 /3m)(3/8π )2/3 ρ 5/3 , where ρ is the particle density. How can electrons then condense? The answer lies in the fact that by first forming Cooper-pairs, which roughly may be considered to be bosons, the electrons effectively shed the shackles of the Pauli principle, and subsequently undergo a condensation into a superconducting condensate. Therefore, we reach the important conclusion that in principle, superconductivity arises as a result of some sort of condensation in a quantum fluid of Cooper-pairs. We will return to a more detailed description of precisely what this means, but it is important to understand that the formation of Cooper pairs occurs, in principle, at a temperature which is above the true superconducting transition temperature. It is only as a result of a mean-field approximation that we find that the temperature at which we get Cooper-pairs is the same as the temperature where superconductivity occurs. In three dimensional systems of good metals, fluctuation effects that lead to a separation of the Cooper-pair formation temperature and the superconductivity, are tiny and almost immeasurably low. However, in systems like high-Tc superconductors, which first of all are quasi-two-dimensional and secondly arise out of metals with very low carrier density, but nonetheless have very respectable transition temperatures, fluctuation effects are much more prominent, and ignoring them therefore becomes a much more dubious endeavour. The important fluctuations that destroy superconductivity, but do not dissociate Cooper-pairs, are transverse phase-fluctuations of the complex two-component superconducting gap function k . The stiffness of the phase of this gap-function, which is a measure of how difficult it is to excite transverse phase-fluctuations, is given by the superfluid density of the system, which is limited by the carrier density. Poor metals thus are expected to give rise to superconductivity where phase-fluctuations play a prominent role. Good metals are expected to give superconductivity where mean-field theory should work very well. In

TRANSITION TEMPERATURE Tc AND THE ENERGY GAP

87

superconductors, the Ginzburg–Landau parameter κ is determined by the super√ fluid density and the critical temperature, κ = λ/ξ ∼ Tc / ρs . Hence, in type-I and moderate type-II superconductors, we can ignore fluctuation effects. In extreme type-II superconductor, like the high-Tc compounds, they cannot be ignored. We will give a detailed description of phase-fluctuations of the superconducting order parameter in Chapters 9 and 10.

4.3 Transition temperature Tc and the energy gap The minimum of the free energy is determined self-consistently by having the gap-parameter satisfy the equation k = −

Vk,k k

k

tanh(βEk /2) 2Ek

(4.24)

At this stage, this is a mean-field equation with a quite general interaction matrix element Vk,k . Assuming that the potential is separable, i.e. Vk,k =

λη gη (k)gη (k )

(4.25)

η

where gη (k) are basis functions for the irreducible representations of the crystal symmetry group of the lattice which the electrons move through, then the gap can be written on the general form k (T ) =

η (T )gη (k)

(4.26)

η

The indices η denote symmetry channels that are represented in the total gapfunction. We will take a particularly simple form of this matrix element, namely Vk,k = −V

(4.27)

for such pairs of wavenumbers k, k that lie in a thin shell around the Fermisurface of thickness ω0 , and zero otherwise. The physical interpretation of ω0 is that it is an upper frequency cutoff on the spectrum of the bosons that provide the ‘glue’ between the electrons forming the Cooper-pairs. For phonon-assisted superconductivity, we have ω0 = ωD , where ωD is the Debye-frequency. Inserting this into the gap equation (Eq. 4.24), we conclude that the gap k is

88

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

k-independent, i.e. it is the simplest case of a gap which transforms as the identity under the allowed symmetry operations of the crystal which the electrons move through. Hence, the gap-equation can be written in the form

1=V

tanh(βEk /2) k

(4.28)

2Ek

There are two cases where this equation is easy to solve, namely T = Tc and T = 0, and we consider the former first. Letting T → Tc− , i.e. in the limit of a vanishing gap, the above equation simplifies in that we ignore the gap in the quasiparticle spectrum Ek . Moreover, we replace the k-sum by an energy integral by introducing the normal-state density of states Dn (ε). The k-space sum is by assumption limited to a narrow region around the Fermi-surface. We therefore need to consider the density of states near the Fermi-surface. Assuming that the Fermi-level is not located close to energies where Dn (ε) has a rapid variation, e.g. not located close to van Hove singularities, we may then simply replace Dn (ε) with Dn (0), i.e. the density of states at the Fermi-level when all energies are measured relative to the Fermi-surface. Finally, upon introducing the dimensionless coupling constant λ ≡ V Dn (0), we get the following equation determining Tc

1=λ

ωD

dε 0

tanh(βε/2) ε

= λ tanh(βωD /2) ln(βωD /2) −

βωD /2

dx 0

ln(x) cosh2 (x)

,

(4.29)

where we have performed a partial integration to isolate the logarithmic singularity in the integral. For phonon-assisted superconductivity (more generally, for weak-coupling superconductivity), λ 1. This means that in order to satisfy the above equation, we require that βωD /2 1. Hence, since the second integral above is rapidly convergent, the above simplifies to ∞ ln(x) βωD − dx 1 = λ ln 2 cosh2 (x) 0 π βωD − ln = λ ln 2 4eγ γ 2e βωD = λ ln π

(4.30)

89

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

m where γ ≡ limm→∞ l=1 1/ l − ln(m) = 0.5772156649 . . . is the Euler– Mascheroni constant. This equation may be solved to give kB Tc =

1 1 2eγ ωD e− λ ≈ 1.13ωD e− λ π

(4.31)

On the other hand, at T = 0, the gap-equation (Eq. 4.28) takes the form

ωD 1 dε 1=V =λ √ 2 2Ek ε + 2 0 k

ωD / ω dx D = λ sinh−1 =λ (4.32) √ 2 x +1 0 Again, when λ 1, this requires ωD / 1 for solution of the equation to exist, and hence sinh−1 (ωD /) ≈ ln(2ωD /). Thus we obtain 1

(T = 0) = 2ωD e− λ

(4.33)

Note that both Tc and (T = 0) depend sensitively on the coupling constant λ, and that both are functions of λ with an essential singularity as λ → 0. This reflects the fact that an attractive interaction is a singular perturbation to the free electron gas, in contrast to the repulsive Coulomb-interaction. There is no way we can obtain the above results for Tc and (T = 0) to any finite order in perturbation theory in the dimensionless coupling constant λ. Moreover, since the dimensionless coupling constant λ is not easy to compute reliably from first principles even in simple metals like aluminum, it is extremely hard to compute values of Tc and (T = 0) reliably. This reflects the fact that these quantities depend on all details of the system, and really should not be the focus of any computations, when the goal is to gain some qualitative understanding of the problem. This is actually a lesson that applies to all types of phase transitions. However, what was noted by Bardeen, Cooper and Schrieffer was the following remarkable fact. If we form the ratio of (T = 0) and kB Tc , then we obtain 2(T = 0) 2π = γ ≈ 3.52. kB Tc e

(4.34)

This is a universal amplitude ratio, all materials-dependent quantities precisely cancel out!

4.4 Generalized gap equation, s-wave and d-wave gaps As the BCS Hamiltonian is formulated in Eq. 4.1, it does not make specific references to any particular pairing mechanism, although originally the founders of

90

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the theory definitely had in mind a phonon-assisted pairing mechanism. What is central, is the idea that the basic physical phenomenon underlying superconductivity is pairing of electrons into Cooper-pairs, followed by a condensation of the electron system into a macroscopically phase-coherent matter wave. In a sense, superconductivity is the matter-wave counterpart of laser-light, which is basically a phase-coherent lightwave. The electron-pairing picture will be maintained. However, as a slight generalization of the above approach, we may ignore the issue of the origin of some attractive effective interaction between electron, leaving open even the possibility that it may not be phononic in origin, but could also be purely electronic. Thus, we may generalize the interaction to the case where it is not limited to be operative in a thin shell around the Fermi-surface, i.e. we include the possibility of a non-retarded attractive interaction. We also propose a slightly more complicated form of the matrix element Vk,k than what we suggested in the previous section, based on the physics of phonon-mediated attractive interactions between electrons. Assume that an electron moves through a crystal with some symmetry. Any physical quantity will ultimately reflect the symmetry of the crystal in some way. It can therefore be expanded in a complete set of functions that all reflect the particular crystal symmetry that the electrons experience. For instance, if the system is approximately isotropic we can expand any physical quantity in the complete set of the well-known spherical harmonics, if the crystal has simple cubic symmetry we can expand in the complete set of cubic harmonics, and so on. Let us denote the set of such complete basis functions by {gη (k)}, where η is an index that denotes which particular one of the basis functions is meant. Now, let us assume further that the matrix element Vk,k is factorizable. By this we mean that it can be factorized into two factors, where one factor only depends on k and the other one only depends on k. Now, since the set {gη (k)} is complete, by assumption, we may write λη gη (k)gη (k ) (4.35) Vk,k = η

where λη is the strength of the interaction in the η-channel. To be specific, consider an example. Assume that the lattice is square (twodimensional, with lattice constant set to unity) and that the electron-electron interactions are such that when two electrons are on the same site, on nearestneighbor sites (horizontal and vertical bonds), and on next-nearest-neighbour sites (diagonal bonds) they experience interactions U/2, 2V , and 4W , respectively. Fourier-transforming this to obtain Vk,k we find Vk,k =

U + 2V [cos(kx ) cos(kx ) + sin(kx ) sin(kx ) 2 + cos(ky ) cos(ky ) + sin(ky ) sin(ky )]

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

91

+ 4W [cos(kx ) cos(kx ) + sin(kx ) sin(kx )] × [cos(ky ) cos(ky ) + sin(ky ) sin(ky )]

(4.36)

Now, we would like to re-express this as a sum of factorized terms using the complete set of square lattice harmonics. As the interaction given above is of finite range, Vk,k has a finite number of terms and thus a finite number of square lattice harmonics will suffice to completely express the matrix element. It turns out that the five lowest order square lattice harmonics will do the job. They are given by 1 g1 (k) = 2π 1 g2 (k) = [cos(kx ) + cos(ky )] 2π 1 g3 (k) = cos(kx ) cos(ky ) 2π 1 g4 (k) = [cos(kx ) − cos(ky )] 2π 1 g5 (k) = sin(kx ) sin(ky ) (4.37) 2π Re-expressing Eq. 4.36 in terms of the above basis functions, we find an expression of the form of Eq. 4.35, with λ1 = 2U π 2 , λ2 = λ4 = 4V π 2 , λ3 = λ5 = 4W π 2 , and λη = 0, η ≥ 6. We note in passing the following fact, which will figure prominently in what follows. The symmetry group of the square lattice is C4v . What is important to note about the five basis functions listed above, is that the first two transform as the identity under all symmetry operations included in C4v . The latter three change sign under π/2 rotations. In this respect, they have common properties with l = 0 and l = 2 spherical harmonics functions that are the basis functions for the isotropic case. l = 0 spherical harmonics are commonly referred to as s-wave functions, while l = 2 spherical harmonics are referred to as d-wave functions. Hence, the first two basis functions above are s-wave basis function, g2 (k) is often called an extended s-wave function. The latter three are d-wave functions. Of these, g4 (k) is the most well-known one in the context of high-Tc superconductivity, since the gap in the cuprate superconductors to a very good approximation appears to be of the form k = 0 (T )g4 (k). Note that l = 1 square lattice harmonics do not enter in the above. The reason is that in all of the above, we have implicitly considered only such cases where we have spinsinglet pairing. This means that the spin-part of the Cooper-pair wave functions is antisymmetric so the space-part of it must be symmetric. This requires even-l basis functions. Spin-triplet pairing would be required in order to make use of odd-l basis functions.

92

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

Returning now to the general case, as far as the superconducting gap is concerned, it is clear that when Vk,k takes the form of Eq. 4.35, we obtain the gap-equation k = −

Vk,k k χk = −

k

=

5

5

λη gη (k)

η=1

k

gη (k )k χk

≡−η /λη

(4.38)

η gη (k)

η=1

which shows that the gap itself is also expressible as a linear combination of basis functions, as it should be, being a physical quantity. The coefficients η are not k-dependent, but do of course depend on temperature. Using the expansion of the gap in terms of basis function on both sides of the gap-equation, we find the set of coupled self-consistent equations for that gap in the different channels η η =

5 η =1

Mη,η = −λη

η Mη,η

gη (k)gη (k)χk

(4.39)

k

In general, these equations require numerical efforts in order to be solved. Considering, once again, the above square lattice example, and setting U > 0, V < 0, and W = 0, we find that there is no attraction in the λ1 -channel, and attraction in the λ2 -channel (extended s-wave) and the λ4 -channel (d-wave). Hence, we see that the gap function, which is closely related to the Fouriertransform of the Cooper-pair wave function, adjusts itself so as to be zero in channels where the wavefunction is non-zero for zero separation between the electrons. By choosing extended s-wave or d-wave, the electrons in the Cooper-pair avoid the onsite Coulomb interaction. Recall that in phonon-assisted Cooper-pairing, the electrons did not avoid each other in space, but used retardation to eliminate the adverse effects of Coulomb-interactions. I.e. they avoided each other in time. In the present non-retarded example, the electrons avoid each other in space, but not in time. Avoiding each other in space (higher-angular momentum pairing) or in time (retardation) are the basic two ways electrons can avoid the repulsive Coulomb-interaction. In the BCS gap-equation, the presence or lack of retardation effects is manifest in the presence or lack of an energy cutoff around the Fermi-surface. In the absence of such a cutoff, i.e. in the absence of retardation, the entire Brillouinzone contributes to the gap. Since (r) = k k eik·r , this means that (0) = k k . Hence, k must be chosen so as to obtain (0) = 0 in order to avoid

GENERALIZED GAP EQUATION, s-WAVE AND d-WAVE GAPS

93

Coulomb-repulsion. Gaps of the form k = 0 (T )g2 (k), and in particular k = 0 (T )g4 (k), have this property. The latter gap-function has a form which is believed to be very close to the form of the gap-function in high-Tc cuprates. As an important application and in preparation for later sections, let us obtain the superconducting density of states Ds (E), which may now be found as follows. Imagine that we have some function g(k) that depends on k only through

Ek =

εk2 + 2k , and assume k to be independent of k. Then we have

g(k) =

k

dεDn (ε)g( ε2 + 2 )

=

dEDn (ε)

=

dε g(E) dE

dEDs (E)g(E)

(4.40)

√ dε , where Dn (ε) where we have introduced E = ε2 + 2 and Ds (E) = Dn (ε) dE is the normal state density of states. The above is exact provided we have Dn (ε) =

1 δ(ε − εk ) N

(4.41)

k

Here, N is the number of Fourier modes of the wave-number, equivalently the number of lattice sites in the problem. The normal state density of states is now assumed to be a slowly varying function of ε around the Fermi surface such that we approximate it by Dn (ε) ≈ Dn (0) when we measure energies relative to the Fermi surface energy. Implicit in this assumption is that sharp features in Dn (ε) are absent near the Fermi surface, i.e. there are no van Hove singularities near the Fermi surface. Then we have E Ds (E) =√ (E − ||) 2 Dn (0) E − 2

(4.42)

where (x) is the Heaviside step-function (x) = 1, x > 0, (x) = 0, x < 0. When the gap function k is not a constant in k-space, we derive a density of states more formally from the spectral weight A(k, ω) introduced in Section 3.2, as follows. Introduce, in analogy to Eq. 3.6, the Green’s function G(k, t) for the superconducting condensate. Formally, this Green’s function is given by + G(k, t; σ ) = −i0|ck,σ (t)ck,σ (0)|0

(4.43)

where |0 is the BCS superconducting groundstate. It is an eigenstate of the Hamiltonian Eq. 4.16. Moreover, we have

1 G(k, ω; σ ) = dteiωt G(k, t; σ ) (4.44) 2π

94

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

Without loss of generality we choose one spin direction, σ =↑ say, and find G(k, t; ↑) = −i0|(cos(θ )ηk+ (t) − sin(θ )γk+ (t))(cos(θ )ηk (0) − sin(θ )γk (0))|0

(4.45)

Now, using the fact that (ηk , γk ) diagonalize the BCS Hamiltonian, we have that 0|ηk+ γk+ |0 = 0 0|ηk γk |0 = 0

(4.46)

Hence, we obtain G(k, t; ↑) = −i cos2 (θ )0|ηk+ (t)ηk (0)|0 − i sin2 (θ )0|γk+ (t)γk (0)|0

(4.47)

Each bracket is now a free fermion propagator in the superconducting state, hence upon Fourier-transforming we find, introducing the coherence factors in Eq. 4.14, u2k vk2 + (4.48) ω − Ek + iδk ω + Ek + iδk where δk is infinitesimal. The spectral weight is therefore given by, using Eq. 3.8 G(k, ω; ↑) =

A(k, ω; ↑) = u2k δ(ω − Ek ) + vk2 δ(ω + Ek )

(4.49)

which should be compared to Eq. 3.8, and which is seen to be spin-independent. Due to the fact that we are considering spin-singlet pairing, we obtain the same result for σ =↓. Thus, we finally obtain the superconducting density of states per spin channel as 1 Ds (ω) = A(k, ω) N k

1 2 [uk δ(ω − Ek ) + vk2 δ(ω + Ek )] = N

(4.50)

k

which again is seen to be independent of the spin index σ due to the fact that we are here considering spin-singlet pairing.

4.5 Quasi-particle tunnelling and the gap 4.5.1

Introductory remarks

The field of superconductivity made two important steps forward at the experimental discovery of tunneling of single charge carriers (‘quasiparticles’) by Giaever in 1960 [38], and the subsequent predictions of tunnelling of Cooper pairs by Josephson in 1962 [8]. These discoveries set the stage for a new era in superconductivity on the small scale. Structures in which the thickness dimension was as small as a few nanometers could be manufactured in laboratories, and their properties controlled reproducibly. Avenues were opened for

QUASI-PARTICLE TUNNELLING AND THE GAP

95

entirely new research and insights, and for electronic devices of a kind that could not even in principle be achieved by conventional methods, all due to the unique properties of the superconducting state, and its wave-function. At the time of the discovery of these new phenomena quantum mechanical tunnelling was a well-established concept in atomic and nuclear matter, and had recently been demonstrated by Esaki to occur between semiconductors separated by a thin barrier. It took the curiosity of two young and independent student minds to divert from conventional thinking, and venture into the new landscapes: The scientific world was startled at the simplicity and profoundness of their discoveries. Giaever pointedly describes his discovery as a method of ‘measuring the superconducting energy gap with a voltmeter’. This apparent simplicity, and the importance of the results led to immediate acceptance. Josephson’s theory, on the other hand, met some initial skepticism. But within a year, experimental evidence began to accumulate in favour of Josephson‘s ideas, and further theoretical work by many groups expanded our understanding of the physics involved, and contributed to the foundation of present-day sophisticated devices, leading on to what we call today ‘Josephson technology’. Here again initial discoveries in pure physics found their way to applications in electrical engineering sciences and technical products.

4.5.2

The tunnelling principle

The tunnelling of a small particle through a barrier in vacuum is a standard problem in atomic physics books, and solvable by relatively simple mathematics using the Schr¨odinger equation, on requiring continuity of the wave-function through the barrier. Usually, the height of the barrier is an unknown parameter, which may eventually be determined by comparison of experiment and theory. When tunnelling is to take place between two conductors, separated by an insulating barrier, several possibilities arise. If we let N symbolize a normal metal, and S a superconductor, and have the substances separated by a thin insulator I, then we may combine these substances in various configurations: NIN, SIS, NIS, N1 IN2 , S1 IS2 etc. Some of these possible structures are illustrated schematically in Figure 4.1. The symbols φ, φl , φr in superconductors indicate the phases of the wavefunctions. In each case the tunnelling particle leaves the substance to the left, say,

N1

I (a)

N2

N

I (b)

S, f

S1, fl

I

S2, fr

(c)

Figure 4.1 Schematic illustration of various possible configurations for tunneling between two normal metals (a), between normal metal and superconductor (b), and between two superconductors (c).

96

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE E

f(E)D(E) EF

E

f (E)D(E)

f (E)D(E) EF

1

∆

2

EF

EF

N

S

f(E)D(E)

D(E)

D(E)

N1IN2 T ≠ 0, V = 0

NIS T ≠ 0, V = 0

(a)

(b)

I

I T>0 T=0 V (c)

∆ e (d)

V

Figure 4.2 (a) and (c) Illustrate tunnelling between two normal metals N1 and N2 through a thin insulating barrier I as seen in a density of states versus energy diagram, with the Fermi–Dirac function factored in. In (a) T = 0 and applied voltage V = 0. In (c) the I − V characteristic is shown as linear, as a consequence of displacing the electron distributions in (a) along the vertical axis by application of an increasing voltage. The right hand figures illustrate similarly the situation for tunneling between a normal metal and a superconductor with an energy gap , at T = 0 and V = 0 in (b), and that of varying voltage applied, in (d). The consequence of varying T is indicated in (d). Note the onset of tunnelling at V = /e.

where it occupies an allowed state in the conduction band of free carriers, and, after tunnelling enters into an allowed state in a band on the right side of the insulating barrier. These processes are restricted by the energy spectra and the statistics governing the bands from which they tunnel, and into which they arrive. Normal metals are well understood so that the appropriate mathematical description of the process between normal metals is straightforward. Furthermore, the BCS theory for superconductivity gave an accurate description of the energy bands in typical low-Tc metallic superconductors. Because this theory already existed by the time of the experimental work by Giaever and coworkers, the appropriate integrals could be written down. Figure 4.2 shows sketches of bands for two of the interesting cases. Figure 4.2a shows the N1 IN2 case, while Figure 4.2b illustrates the NIS case with no external voltage applied. Figure 4.2c and d illustrate the corresponding current–voltage characteristics for the NIN case (c), and the NIS case (d), respectively. None of these represent the Josephson case, however. In the Josephson effect the phase properties of

QUASI-PARTICLE TUNNELLING AND THE GAP

97

the wavefunction come into full play. This requires a different approach, as will be discussed later. The Giaever case is a simpler one. Let us look at the terms that contribute to the tunneling of single carriers, beginning with the NIN case where only normal electrons are involved.

4.5.3

Single-particle NIN tunnelling

For this discussion we refer to Figure 4.2a. The total number of electrons travelling across the barrier from left to right is proportional to the number of filled electron states on the left-hand side (l) and to the number of states that are unoccupied on the right-hand side (r). The tunnelling current il→r at a particular energy level E and in an interval dE is then il→r = Cn Dl (E)fl (E) × Dr (E)fr,h (E)dE

(4.51)

where fl and fr,h are the probabilities that the energy level E to the left is occupied, and that states at the same level to the right are unoccupied, respectively. According to quantum theory, when the transitions take place from left to right, i.e. when the transitions are completed as il→r , the unknown constant Cn may be written as Cn =

2π |Tn |2

(4.52)

where |Tn |2 is the tunnelling probability, given by the squared matrix element for the transition of an electron from the left electrode to the right electrode. We have, in addition, to factor in the number of available states (holes, h) to the right in the same energy interval by use of the relation fr,h (E) = 1 − fr (E)

(4.53)

The total tunnelling current, when adding processes taking place at all energy levels is then

∞ 2π ∞ |Tn |2 Dl (E)fl (E)Dr (E)(1 − fr (E)) dE Il→r = il→r (E)dE = −∞ −∞ (4.54) In equilibrium, of course, a similar integral applies to transitions from right to left. These transitions have to be subtracted to get the net current across the barrier. Finally, therefore: The net current ININ between two normal metals found upon subtraction of Ir→l from Il→r becomes:

2π ∞ |Tn |2 Dl (E)Dr (E)(fl(E) − fr (E)) dE (4.55) ININ = Il→r − Ir→l = −∞ In both equations above we have allowed integration from −∞ to +∞. This is permissible due to the difference term (fl (E) − fr (E)). The properties of these

98

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

functions makes the integrand extremely small outside a narrow energy window of order kT . Now, without a voltage applied, the difference (fl (E) − fr (E)) is simply zero, as may be seen from Figure 4.2a and b: No net charge transport can occur without an applied voltage. The claim that fl (E) − fr (E) = 0 may seem like an oversimplification if we consider two metals with different Fermi energies to the left and to the right. A very important condition has to be fulfilled for this equality to hold: The two electron gases must constitute one thermodynamic system. This requires particle exchange across the barrier, in fact vigorous tunneling must take place. It is a basic result of thermodynamics that two systems which come into equilibrium due to exchange of particles, will do so by spilling over particles until they have adjusted their chemical potentials to the same level. In the present context we will approximate the chemical potential µ by the Fermi-energy EF . So EF,l and EF,r become exactly equal at equilibrium. Now clearly fl (E) − fr (E) becomes zero since what really goes into the Fermi-functions is always the difference E − EF . This argument also points to the fact that initially there must be a current to establish equilibrium. But this process is fast, and happens during deposition of the films. We need not worry about such transient properties. We can break this symmetry by applying a voltage V , raising the electron band on one side with respect to the other side. Now current will flow since we have to put E + eV or E − eV as the argument in one or the other of the f -functions, and fl (E) − fr (E + eV ) becomes non-zero. The current is now ININ =

2π |Tn |2

∞

−∞

Dl (E)Dr (E + eV )(fl (E) − fr (E + eV ) dE

(4.56)

We may if eV Ef , to a very good approximation, make the following simplification for calculation of the integral for ININ : (f (E) − f (E + eV )) dE ≈ −

∂f eV dE ∂E

(4.57)

∂f Under the integral − ∂E acts like a δ-function; hence we obtain

ININ =

2π 1 |Tn |2 Dl (EF )Dr (EF )eV ≡ GNIN V = V RNIN

(4.58)

where GNIN is the normal conductance, or the inverse of the resistance RNIN of the entire NIN contact. We have taken Dl and Dr outside the integration, replacing them by the constants Dl (EF ) and Dr (EF ) since under normal circumstances E will be near EF where D(E) varies slowly with E. This result is shown in Figure 4.2c where the simple linear characteristic of one NIN contact is illustrated.

QUASI-PARTICLE TUNNELLING AND THE GAP

4.5.4

99

NIS quasiparticle tunnelling

The analysis given above proves that the NIN tunneling contact acts as an ohmic element in a circuit, a fact worth noting, but as such not particularly exciting or useful since for most purposes we have more practical ways of making resistors. However, the situation is substantially altered once we allow one, or both, of the metals to become superconducting. This can in many cases be achieved simply by cooling the contact. If the two metals were, for instance, Nb with a superconducting transition temperature Tc = 9 K and Pb with Tc = 7 K, we could implement the following contacts by lowering the temperature: N1 IN2 at all T > 9 K; NIS between 7 K and 9 K; and S1 IS2 below 7 K. What makes the NIS or SIS configurations so interesting, and useful, is (i) that they provide us with radically different, nonlinear current-voltage I–V characteristic both for single electron tunneling and for Cooper pair tunnelling, and (ii) that entirely new phenomena arise in SIS contacts in particular, reflecting deeper aspects of the superconducting wavefunction. These aspects are exceedingly interesting from a physics point of view, and harbor the promise for a multitude of important applications. On changing our system under investigation to an NIS-contact, as long as we are discussing single-particle tunnelling, the integrals introduced above do not change in principle, only the density of states Ds in the superconductor replaces one of Dn functions in the normal state. The Fermi–Dirac functions remain unaltered. Again we have to apply a voltage to set up a net current in one of the two directions (see Figure 4.3.) In Section 4.4 we have shown that the density of states of quasiparticles in the superconductor Ds (E) is related to the one in the normal metal Dn (0) near E N

E S

N

S

E FS + ∆ E FN

E FN

E FS E FS

E FS − ∆

V = 0; T ≠ 0; I = 0 (a)

∆ V = e ; T ≠ 0; I ≠ 0 (b)

Figure 4.3 (a) T = 0. Almost no electrons available for tunneling leads to very low tunnel current. (b) Bands displaced by eV . Optimal condition for quasiparticle tunnelling from N to S. In both cases EFN and EFS refer to Fermi energies of normal and superconducting metals, respectively.

100

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the Fermi energy by E ; |E| ≥ Ds (E) 2 = (E − 2 )1/2 Dn (0) 0; |E| <

(4.59)

where energy E is now measured from the Fermi-level EFS . On insertion of Ds (E) the current can be expressed as

∞ |E| 2π q 2 |Tn | Dl (0)Dr (EF ) INIS = 1 (f (E) − f (E + eV )) dE −∞,|E|> E 2 − 2 2 (4.60) where the superscript q reminds us that only quasiparticles (single electrons) are to be counted. The notation |E| > under the integral sign indicates that integration over the interval |E| > is excluded. On comparison with the NIN-case we discover q that INIS can be simplified to q

INIS =

GNIN e

∞

−∞

|E| 1 (f (E) − f (E + eV )) dE E 2 − 2 2

(4.61)

This integral can only be solved analytically in the T = 0 limit, giving 0; |eV | < q 1 (4.62) INIS = GNIN 2 (eV )2 − 2 ) ; |eV | ≥ e The quasiparticle current increases sharply from zero at V < e like the square root of the voltage in excess of e when V > e . A crucial point, which was eloquently exploited by Giaever and coworkers, is the ensuing relation for the differential conductance, defined as GdNIS = dINIS /dV (rather than GNIS = INIS /V used before). One quickly verifies that

∞ dINIS Ds (E) ∂f (E + eV ) = GNIN dE (4.63) GdNIS ≡ dV D ∂(eV ) −∞ n (EF ) Here the derivative of f approaches a δ-function when kT → 0. At finite values it assumes a form similar to a Gaussian distribution, and with a width of the order of kT . In the T = 0 limit the result is then exactly GdNIS = GNIN

eV (eV )2 − 2

1 = GNIN DS (E = eV ) 2

(4.64)

QUASI-PARTICLE TUNNELLING AND THE GAP

101

4

Relative conductance

(dI/dV)NIS (dI/dV)NIN

Pb/MgO/Mg ∆ = 1.34 × 10−3eV

3

T = 0.33 K

2

1

0

0∆

4∆ 8∆ 12∆ Voltage bias eV in units of ∆

16∆

Figure 4.4 Relative conductance of Pb/MgO/Mg contact in the NIS configuration relative to that of the corresponding NIN contact. The structure above the gap is caused by phonon processes during tunnelling. Adapted from Giaever et al. [39].

This means that a measurement of dINIS /dV , indeed a measurable quantity, probes the superconducting quasiparticle density of states function directly. Most clearly we see this in the experimentally accessible quantity GdNIS /GNIN = Ds (E = eV )

(4.65)

An example of an early manifestation of this relationship is seen in Figure 4.4, except for some additional phonon structure. The expected property that the relative conductance diverges like Ds at eV = , is therefore confirmed. A physical measurement can of course never truly measure a divergence in the strict mathematical sense. Neither should one take such a prediction literally in the real world. After all, we are talking about a model, the BCS theory, which has built into it certain idealizations that are not to be regarded as exact. Still, the model predicts a remarkably sharp onset of quasiparticle current vs. V that has been confirmed by experiments, even at temperatures well above T = 0, and the overall behaviour is very close to the BCS prediction. In the so-called excitation representation electron-like and hole-like excitations are depicted in a positive energy continuum above the superconductor gap energy . This is illustrated in Figure 4.5. The superconducting energy gap is introduced by joining the hole-like branch and the electron-like branch at a finite gap energy , and with consequences for the density of states, proportional to |∇E(k)|−1 .

102

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE E = |E′ − EF|

E′

E = |E′ − EF|

EF h

kF

k

0

(a)

e

kF (b)

h

k

0

e

kF

k

∆ (c)

Figure 4.5 (a) Usual free-electron gas representation of T = 0 in a normal metal; holes ◦ below EF , electrons • above. (b) Excitation representation of a normal electron gas at T = 0. Hole branch: ◦h, electron branch •e. (c) Excitation representation in a superconductor with −1 a gap . The two branches join at , and the density of states proportional to ∂E near ∂k the minimum point is strongly modified from that of the normal state in (b).

4.5.5

SIS quasiparticle tunnelling

With the construction of an a SIS contact the possibility arises to establish both a quasiparticle current and a Cooper-pair current between the two superconductors. Both of these can be treated fully by quantum theory, on a similar footing to that used in NIN and NIS contacts above. However, only the SIS-case is reasonably straightforward in the established language of single particle transitions. When Cooper-pairs tunnel the addition of matrix elements for the two constituent particles requires heavier formalism which belongs in a more advanced treatment. The familiar problem in quantum mechanics of adding before squaring comes in. We will attack this case with a different and simpler method in the next section. And, having established a method for calculation of NIS -quasiparticle current, one needs only extend that procedure to the S1 IS2 case directly. The resulting integral can be guessed on the basis of the earlier discussion: q ISIS

GNIN = e

∞

−∞

|E| |E + eV | ((f (E) − f (E + eV )) dE 2 2 E 2 − ((E + eV )2 − 2 ) 12 2 1 (4.66)

Again, it is understood that integration is not to be carried out in the gaps. This current can only be calculated numerically. Instead of working out this problem we resort to simple physical argument. In four successive sketches, Figure 4.6, a qualitative picture is developed for quasiparticle tunneling between two superconductors with different gaps, 1 and 2.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS E S1

103

E S2

∆1

∆2

S1

S2

eV = ∆2 − ∆1

∆1

∆2

EF1

EF2

V=0

V=

(a)

∆2 − ∆1 e (b)

E ∆1 EF

S1

I

S2 ∆2

1

EF

V=

∆1 + ∆2 e (c)

1 V Rnn

2

∆2 − ∆1 e

∆2 + ∆1 e

V

(d)

Figure 4.6 Qualitative illustration of quasiparticle tunneling between two superconductors with different gaps, (a), (b) and (c) at different values of bias field, (d) showing the resulting overall I–V characteristic to be expected.

4.6 4.6.1

BCS coherence factors versus quasiparticle-effects: ultrasound and NMR Introductory remarks

As we have seen in Section 4.2 the BCS theory predicts an energy gap (T ) = o (Tc − T )1/2 associated with the superconducting state due to an effectively attractive electron-electron interaction in the presence of an ionic lattice. This picture needs experimental confirmation. In the preceding section we already discussed a possible method, quasi-particle tunnelling. There are several other methods as well. In fact, specific heat measurements and infrared absorption had already shown, even before the BCS theory was worked out, that a gap had to be present. This was particularly evident well below Tc . In this sense the BCS theory explained already existing results. However, a more complete and satisfactory confirmation of the BCS theory requires measurement of both the gap size, the temperature dependence of the gap, the density of states, and

104

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

confirmation of more subtle effects like the so-called coherence factors. In this section we will illustrate both some theoretical approaches, and some experimental procedures that confirm central aspects of the BCS theory for metallic, low-temperature superconductors.

4.6.2

Transition rates in ultrasound propagation and NMR

Ultrasonic attenuation and NMR have turned out to be excellent tools for testing of the predictions from the BCS theory. Some experimental results for ultrasound appeared already in the BCS paper, and lent immediate support to this important work. Longitudinal phonons interact with the quasi-particles in the same way as with electrons in the normal state. The BCS theory for the attenuation of longitudinal phonons gives a very simple expression to test, as will be outlined below, with (T ) as the only unknown quantity. Early measurements at Brown University [40] showed overall consistency with the predictions of BCS, although the experimental data had low precision near Tc . We will now investigate how ultrasonic attenuation may be used to gain insight, possibly verifying more fully the BCS result. Let us follow the main line of reasoning leading to a prediction for ultrasonic attenuation and NMR relaxation rate. Up to a certain point these physical effects can be described by the same formalism. In quantum mechanical terms we need to calculate transition rates αs . These are the net transition rates between energy levels E and E + ω, in fact quite similar to tunnelling which we discussed previously, in Section 4.5. In the present context the energy ω refers to the exchange of a phonon in the case of ultrasound, and to the exchange of a quantum of electromagnetic radiation in the case of NMR. With the tunnelling effect as a reference, the expression for the desired quasiparticle transition rate in the superconducting state may be logically constructed as

αs = |M|2 C(, E, E + ω)Ds (E)Ds (E + ω) f (E) − f (E + ω) dE (4.67) Here, M is a matrix element for the appropriate electronic transition, the same one as in the normal state due to the close correspondence between quasiparticles and normal state electrons. The Ds -factors are the same density of states we used under the discussion of tunnelling in Section 4.5. However, there is a fundamental difference between the normal state and the superconducting state: In the latter case there is coherence between occupied one-electron states, making scattering events interdependent. This is an interference effect which is expressed by the coherence factors contained in the function C(, E, E + ω)1 . 1 See for instance de Gennes: Superconductivity of metals and alloys, Chapter 4. W. A. Benjamin, Inc. New York, 1966, for a thorough discussion of coherence factors in superconductivity.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

105

The choice of sign in the coherence factor is essential, and distinguishes two important cases. We quote here the form valid at low frequencies, ω . 1 E(E + ω) ∓ 2 2 1 = C(, E, E + ω) = 1 ∓ (4.68) 2 E(E + ω) 2 E(E + ω) Using previously developed expressions for Ds we now obtain the following integral for the transition rate in the superconducting state

∞ E(E + ω) ∓ 2 f (E) − f (E + ω) 2 2 αs = |M| Dn (0) dE (4.69) 1/2 −∞ (E 2 − 2 )1/2 (E + ω)2 − 2 The upper sign here refers to so-called case I processes, and the lower one to case II. The first of these involves a scalar potential as in longitudinal ultrasound, the second one corresponds to the presence of a vector potential A as in transverse ultrasound and in NMR. The notation for the integration limits has been simplified. It is understood that no integration is to be carried out in the range |E| < , since no quasiparticles are present there. Next, to normalize the superconducting scattering rate (Eq. 4.69), against the rate in the normal state we set = 0 to obtain αn corresponding to the normal state transitions rate. Integration of (4.69) gives αn = |M|2 Dn2 (0)ω.

(4.70)

Performing the normalization αs /αn we find an integral which subsequently may be worked out for different cases:

∞ E(E + ω) ∓ 2 f (E) − f (E + ω) 1 αs /αn = dE (4.71) 1/2 ω −∞ (E 2 − 2 )1/2 (E + ω)2 − 2 By calculating and measuring the ratio αs /αn the matrix element |M|2 drops out of the problem, as it did here, and we need not be concerned with its actual value; similarly for Dn2 (0).We are now in a position to discuss two distinct cases: ultrasound and NMR.

4.6.3

Longitudinal ultrasonic attenuation

The attenuation coefficient for ultrasound, α u , is the exponent by which the intensity of an ultrasonic wave at frequency ω decays with distance. Its value is measured in dB/m or in Nepers/m. The quantity α u is also closely related to the mechanical quality factor, the Q-factor, of the sample under study when treated as an acoustic resonator. It represents the ratio of dissipated energy to supplied energy. For this reason the normalized transition rate also corresponds to the normalized ultrasound attenuation, i.e. αsu /αnu = αs /αn . These relative rates can for instance be evaluated in the limit when ω approaches zero, an

106

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

approach which applies in the usual ultrasonic phonon energy range – typically at 100 MHz – where ω is very small, on the scale of the energy gap as well as on the scale of kT in most cases. Upon cancellation of the coherence factors against a density of states factor in Eq. 4.71 one finds an integral which can be simplified as follows in the low ω limit (ω → 0).

1 f (E) − f (E + ω) dE = − ω

∂f dE ∂E

(4.72)

Integration in the allowed range, i.e. excluding the range − to + by integration from −∞ to −, and from to ∞, one finds directly for longitudinal attenuation 2 αsl /αnl = 2f () = , (4.73) (T 1 + e )/kT a remarkably simple result, in form very similar to the Fermi–Dirac function. This result should not come as a complete surprise: Rather, the transition rate and therefore also the attenuation, should be expected to depend on the gap in this manner, since the Fermi–Dirac function determines the rate at which quasiparticles are created above the gap, and hence also the relative attenuation. In spite of this, the result (Eq. 4.73) is not entirely obvious. Without the accidental cancellation of a factor in the function C against a density of states factor in Ds , this simplicity would have been lost. Figure 4.7 shows data obtained on indium and analysed to give the limiting value of at low temperatures, (0) [41]. The early measurements quoted above, gave a good overall confirmation of the theory, but did not test this result fully, especially not near Tc where the temperature dependence is very strong, with a vertical tangent at Tc . Because this is also the region where the difference between the two-fluid model and the BCS model could be expected to be most distinct, ultrasound provides an important testing ground for the predictions of the combined effects of the energy gap and the coherence factors. In the case just discussed, only the gap remains as the controlling factor. This is quite different for transverse ultrasound, as will be discussed below. The BCS prediction for attenuation (Eq. 4.73), was tested by careful measurements using longitudinal ultrasound at 210 MHz very close to Tc in superconducting aluminium [42], (Figure 4.8). The agreement with BCS theory is seen to be remarkably good. We note the almost vertical slope in ultrasonic attenuation at Tc , and the fact that the attenuation drops by 25% over only 40 mK, all of this in full agreement with the BCS prediction. We conclude, that in the case of aluminium the BCS predictions for the temperature exponent of the gap, i.e. the exponent 1/2 in (Tc − T )1/2 , as well as its zero degree value, 0 = 3.52 kT , are in agreement with the experiment. Recalling that BCS is a mean field theory, this constitutes a demonstration that the BCS approach is good in typical low Tc superconductors even in the close vicinity of Tc . No traces of fluctuation effects are seen, in accord with the arguments given in Section 2.6.6.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

107

60 In

Attenuation [dB/cm]

50

an

q||e, q|| [001] 40

f = 270 MHz BCS theory, 2∆(0) = 3.1kT c

30

Datapoints as

20 10 0

1.0

1.5

2.0

2.5

3.0

3.5

4.0

Temperature (K) (a)

0.4

q||e, q|| [110] f = 150 MHz

0.2

In

2a n −1 as

−1

0.3

Slope → ∆(0) = 3.1 kTc 0.1

0

0

0.5

1.0

1.5

2.0

Temperature (K) (b)

Figure 4.7 (a) Measurements of attenuation of longitudinal ultrasound in indium in the normal and superconducting states. The normal state data were obtained by application of a magnetic field H > Hc . (b) Analysis of data at 150 MHz using the function (Eq. 4.73), leads to determination of (0)[41].

However, theoretical work by Halperin and colleagues [43], and later work by Bartholomew [44] and by Mo and co-workers [45], has shown that when κ = λ/ξ 1 the superconducting phase transition is expected to be first order. Aluminium is extreme Type I with a κ-value of order 10−2 , so the theory should apply in this case. Evidently the experiment quoted above would have to be carried out with even much higher than mK temperature resolution to reveal the predicted effect. Judging by the data presented here, the predicted first order jump has to be very small in Al, but its existence even here cannot be excluded on the basis of the presented data.

108

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE 1.00 q||e, q||[110] 0.95

Relative attenuation

210 MHz BCS theory

0.90

Error bars

0.85

a ls /a ln

Experiment

0.80 0.75

40

30 20 Temperature(T c − T ) (mK)

10

0

0.70

Figure 4.8 Measurements of the attenuation of longitudinal polarized ultrasound in superconducting Al, compared to BCS prediction in Eq. 4.73. Notice the temperature scale in mK. Adapted from Fossheim et al. [42].

4.6.4

Transverse ultrasound

The physics of scattering of transverse phonons in superconductors, as observed in experiments using transversely polarized ultrasonic waves, is distinctly different from the longitudinal case. This interesting fact has been largely overlooked in textbooks in superconductivity until now, in spite of the fact that the physics has been well described and understood. In early experiments [46] the attenuation of transverse acoustic waves in very pure metals was found to drop precipitously just below Tc . This effect became known as the ‘rapid fall’. It was somewhat erroneously considered to be due purely to Meissner screening of the fields associated with the transverse wave. It turns out, rather, that this difference offers an interesting possibility to test no less than a hallmark of the BCS physics, namely the coherence factors [47], cf. Eqs 4.14. With transverse waves these factors do not drop out of the transition rates as they did in the longitudinal case just discussed. An experimental test to reveal their possible presence is therefore a highly worthwhile enterprise. The difference referred to, is due to the different electronic responses to the ionic displacements of longitudinal and transverse acoustic waves in a conducting medium. In the presence of a longitudinal wave the electron gas is driven by the electrostatic fields created by the ‘piling up’ and ‘thinning out’ of positive ionic charge as the wave propagates through the lattice. This essentially electrostatic response is very fast, limited only by the plasma frequency, and therefore occurs completely in phase with the ionic motion. The interaction between the primary ionic wave and the electron gas is of a scalar nature, and independent of the direction of both electron spin σ and momentum k. The response of the electron gas is often described as that of maintaining (approximate) charge neutrality.

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

109

The case of transverse waves is wholly different; there is no piling up or thinning out of charge in the transverse motion of the lattice. Charge neutrality, preexisting before injection of the acoustic wave, is preserved in the electronic response as well. In this case the transverse ionic current generates a time varying magnetic field, which in its turn drives an electronic current. The coupling between the ionic motion and the electron gas is therefore of electromagnetic nature and much slower than in the longitudinal case, involving the electronic skin depth δ. The presence of the induced magnetic field as an intermediary between ionic and electronic currents becomes extremely important when entering into the superconducting state. This necessarily leads to Meissner screening of electronic currents below Tc , an effect which is not present in the longitudinal case. Screening occurs in the entire range of the acoustic wave, in the bulk, contrary to how we previously encountered the Meissner effect, as a response occurring in a thin layer λ near the surface. As transverse wave propagation is easily generated at a single wavevector q at a time, this opens up for a determination of the superconducting penetration depth λ versus q in the bulk of the material. As was mentioned earlier, the coherence factors now appear in a different way: The interaction between a free charge and a magnetic field occurs via the product p × A = k × A, where A is the vector potential. This term is independent of spin, but changes sign on replacing k by −k. When evaluating the integrals discussed above this property turns out to require the opposite sign in the coherence factor function C introduced in Eq. 4.68. Although the coherence factors dropped out against a density of states factor in the longitudinal case, this clearly cannot happen here, and the coherence factors remain in the problem. Furthermore, screening has to be taken care of, and finite frequency electrodynamics enters in an important way. We now outline the approach which has been followed by Fossheim [42, 47]. The attenuation coefficient α for ultrasonic waves propagating in a conducting medium can be expressed as the energy dissipated per second divided by the energy input per second, both calculated per unit area of the wavefront. In the presence of induced current densities and fields this leads to the expression α=

1/2Re(j ∗ E) 1/2ρvi2 vs

(4.74)

Here we need an expression for the electronic current density j whose complex conjugate appears in Eq. 4.74, and the electric field E within the superconductor, which is by no means zero in this electrodynamic problem. Other factors in the above expression are the density of the material ρ, the ionic velocity vi and the velocity of sound vs . The quantity we have to express is primarily the field E, since the current density can always be written as j = σ E ≡ (σ1 + iσ2 )E. Here we have defined the complex frequency dependent conductivity σ as consisting

110

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

of a real part σ1 and an imaginary part σ2 . Next we express the electric field by these conductivities. For this purpose we combine Maxwell‘s equations ∂B ∂t ∇ × B = µ0 (j s + j i ) = µ0 (σ E + j i ). ∇×E =−

(4.75) (4.76)

Here we have introduced the magnetic induction B created by the ionic current density j i of the transverse acoustic wave, and the associated self-consistent electric field E generated by the time-dependent magnetic induction. We will assume the waveform to be exp i(qx − ωt) for all fields and currents in Eqs 4.75 and 4.76. To solve these equations for E we assume that the wave is traveling in the positive x-direction, generating the transverse ionic currents along the y-axis, and consequently the induction B is along the z-direction. In this plane wave scheme the spatial derivatives are nonzero only when taken with respect to x. We combine the two Maxwell equations by taking the curl of Eq. 4.75 and the time derivative of Eq. 4.76, and find ∇×

∂B ∂ = µ0 (σ E + j i ) ∂t ∂t

(4.77)

which is to be combined with ∇ × ∇ × E = −∇ ×

∂B ∂t

(4.78)

Recalling that for transverse waves there is no net charge accumulation, we have ∇ × E = 0 in the second of these equations. Using this to simplify Eq. 4.78, and after equating the right-hand side of Eq. 4.77 with the left-hand side of Eq. 4.78, we arrive at E=

iµ0 ω j q 2 − iµ0 ω(σ1 + iσ2 ) i

(4.79)

and eventually to

−σ1 + i E=

q2 µ0 ω

q2 + σ2 µ0 ω ji 2 + σ2 + σ12

(4.80)

This expression is fully valid in both the normal and the superconducting states. Referring to Eq. 4.74 we now normalize the attenuation coefficient in the superconducting state against that in the normal state, in both cases taking

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

111

the expression for the electric field from Eq. 4.80. The procedure is now to carry out σ1s |E s |2 Re(j s × E s ) αst = = αnt Re(j n × E n ) σ1n |E n |2

(4.81)

We have attached the suffixes s and n to the respective fields in the superconducting and normal states. To further develop Eq. 4.80 we introduce one simplifying aspect: the imaginary part of the normal state conductivity can be shown to be negligible in comparison with the real part at usual ultrasonic frequencies up to several hundred megahertz, hence σ2n is omitted hereafter. Note, however, that σ2s can by no means be neglected. After some algebra the final, normalized attenuation was found by Fossheim as [47] αst αnt

σ1s (qδ)4 + 1 σ1n = 2 2 σ2s σ1s 2 + + (qδ) σ1n σ1n

(4.82)

We leave it as an exercise to carry out the manipulations required to obtain this result from Eq. 4.81. In Eq. 4.82√we have introduced the parameter δ = (1/µ0 ωσ1n )1/2 . Except for a factor 2 this is the usual normal state skin depth for electromagnetic fields. We note from the way the skin depth appears together with the imaginary conductivity in the denominator of Eq. 4.82, that normal state screening plays a role. The product of skin depth δ and wavevector q – essentially the ratio of skin depth to acoustic wavelength – measures the effectiveness of the normal state screening since the term (qδ)2 adds to the term σ2s /σ1n which represents superconducting screening. The latter contains the Meissner effect. Thus in a subtle way Eq. 4.82 describes a continuous crossover between normal state screening and superconducting screening. What is being screened, of course, are the induced currents j , and B-fields that provide the coupling between the transverse lattice waves and the electron gas. And, as these are screened out, so is the electric field E. Therefore the whole coupling mechanism breaks down in a narrow temperature range below Tc . This eliminates a dissipation channel, and the acoustic attenuation drops dramatically, as mentioned above, the so-called ‘rapid fall’ which was referred to before. It is a phenomenon full of essential superconductor physics, as we demonstrate in more detail, next. Importantly, the coherence factors did not drop out of the problem, but are present in the conductivities. We proceed to discuss these aspects, making use of the transition rates again, i.e. Eq. 4.71, as was done originally by Mattis and Bardeen [48]. It is appropriate to associate the transition rate with the processes that determine σ1s since this is the loss part of the complex conductivity. The

112

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

resulting integral, still with the coherence factors intact, cannot be solved analytically, but an approximate analytic form was found by Cullen and Ferrell [49] 2 8 1 σ1s 2 ln − 8.42/π =1+ σ1n 2 kT eω kT

(4.83)

Mattis and Bardeen also gave σ2s /σ1n in integral form, but an analytic solution was only given under conditions which are outside of the accessible range in the experiments we are discussing here. The work of Fossheim [47] introduced instead a nonlocal modification of the London expression for σ2s /σ1n , as follows: σ2s 1 =2 λ−2 L (0) × T × K(qξ0 ) σ1n µ0 ωσ1n 2 δ =2 × T × K(qξ0 ) λL (0)

(4.84)

Here λL (0) is the zero degree London penetration depth, T = (Tc − T ), and K(qξ0 ) is the nonlocal Pippard kernel (see [47]). Since this term Eq. 4.84 appears not as a factor in the expression for αst /αnt , but added to the term (qδ)2 this approximation is not as essential to have in the correct BCS form as is the case with σ1s /σ1n , which contains the dominating effect of the coherence factors. That aspect is essential very close to Tc as it turns out that the presence of the coherence factors in σ1s /α1n dominate the behavior of the attenuation αst /αnt in the first few mK below Tc , below which it is overlapped and followed by the Meissner screening. And while at the transition the attenuation would have zero slope if the Meissner screening was the dominant effect, on the contrary, with the coherence factors present a sharp break occurs, with vertical slope. Perhaps no other phenomenon defines Tc as sharply as this in superconductivity. The issue is therefore whether experiments can confirm the latter prediction. Experiments in indium [47] and in aluminium [42] shown in Figure 4.9 provide substantial verification of the presence of the coherence factors, showing the predicted sharp break on the sub-millikelvin scale. In fact, in Ref. [47], Tc was resolved with ±2/10000 K resolution! In the aluminium results, there appeared a correction factor in the parameter λL (0) which was interpreted as an effect of electronic effective mass enhancement by about 1.5 due to electron–phonon interaction, also in accord with cyclotron resonance experiments. Again, evidence for the predicted first order transition [50] was not found. Evidently, even the already very high resolution of this experiment was not sufficient to see it. Calculations of the attenuation of transverse waves in several metals were carried out by [51], covering a wide range of frequencies. At frequencies of the order of 1 GHz, depending on the metal, it was found that the presence of the qδ-factor alters the sign of the initial slope of αst /αnt from a sharp downward break to an equally sharp upward break. This latter effect resembles very closely

1.0

147 MHz 206 MHz 245 MHz 285 MHz 305 MHz

0.8

Relative attenuation

q|| [110], e||[010]

0.6

113

ats /a tn

BCS COHERENCE FACTORS VERSUS QUASIPARTICLE-EFFECTS

Theoretical curve, m = 1.4 0.4

0.2

30

25

20

15

10

5

0

0

Temperature T c − T (mK)

Figure 4.9 Attenuation of transversely polarized ultrasound in superconducting Al near Tc . Measurements by Fossheim et al. [42]. The continuous curve is a calculation based on theory by Fossheim [47]. µ is the mass enhancement factor mentioned in the text.

the behavior of the NMR relaxation rate at the superconducting transition. In essence, transverse ultrasonic experiments and NMR experiments contain the same information regarding the presence of BCS coherence factors, whether the ultrasonic frequency is high or low. It should be mentioned that the ultrasonic experiments referred to were carried out on ultra-pure 6N metals, where the electronic mean free path at low temperatures is of the order of millimetre length, making the product q 1, being the electronic mean free path. In this case the electronic attenuation in the normal state is temperature independent and proportional to q, and the rapid fall or rapid rise below Tc is a very strong and sharp effect.

4.6.5

Nuclear magnetic resonance relaxation below Tc

One of the earliest and most successful confirmations of the BCS theory was provided by the nuclear magnetic resonance measurements of the longitudinal relaxation rate 1/T1 in a superconductor by Hebel and Slichter [52]. The observed rise of the relaxation rate just below Tc , to a level above that in the normal state, confirmed a crucial aspect of the theory. A good idea of the expected behavior is obtained by use of the scattering rate already given in Eq. 4.71. By again introducing the derivative of the Fermi–Dirac function like before, and adding symmetric contributions from the ranges E ≥ and E ≤ − after allowing ω → 0, one finds the following integral expressing the relative NMR relaxation rate αs /αn in the superconducting state normalized against that in the

114

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

normal state as αs = −2 αn

∞

E 2 + 2 E 2 − 2

∂f ∂E

dE.

(4.85)

This integral diverges logarithmically. If ω had been allowed to retain a finite value, the divergence would be avoided, and the result would be of the order of ln(/ω), as discussed by Tinkham [53], of the order of 10 for typical cases. This is far larger than what is measured. Various schemes have been discussed in the literature to reduce this discrepancy. The main ones have been to take account of anisotropy of the energy gap, and to assume nonuniform lifetimes of quasiparticles over the Fermi-surface. What has become quite clear after the discovery of high-Tc superconductors is that the rise in relaxation rate below Tc is tied to the symmetry of the wavefunction. The relaxation peak is present in s-wave superconductors, as was worked out by BCS, but not in d-wave superconductors like the high-Tc cuprates. An example of a low-temperature measurement Superconductivity research during the first 75 years since 1911, was always a domain of low temperature physics, and a large part still is, in spite of highTc superconductivity. Figure 4.10 shows an example of an experimental setup which led to the ultrasonic data near Tc quoted previously in this section [42]. The measurements in aluminium required careful temperature control and measurements down to 1.1 K. This is just within the temperature range accessible by pumping away the evaporating gas from liquid helium 4 He, whose boiling point is 4.2 K at STP. The cylindrical chamber shown in the figure is immersed in helium, which at these temperatures (T < 2.2 K) is a superfluid, in a cryogenic glass Dewar and filled with superfluid through the tube indicated in the figure as the pumping line. Inside the chamber shown here, the sample is mounted onto the lower end of a quartz crystal acting as an acoustic delay line, centrally located in solid copper block for temperature stabilization. The use of superfluid helium in addition, offers excellent conditions for temperature stabilization since it is well known to sustain zero temperature gradients. This is ideal for the present purpose which requires a temperature stability better than 1/1000th of a degree. Other details of the physical attachments are shown in the figure. Note in particular the pumping outlet. It has a narrow constriction, 0.65 mm in diameter. While this arrangement still allows efficient pumping of gas from the chamber due to the short length of the hole, and the low density of the gas, it reduces substantially the flow of superfluid He film out of the chamber. If the superfluid is allowed to flow up along the inner wall of the pumping line over its full diameter, a phenomenon which is well known to occur, it will reach high enough temperatures to evaporate, thereby reducing the pumping efficiency sufficiently to prevent the lowest temperatures to be reached. The

THE GINZBURG–LANDAU THEORY

115

Pump Leads Signal

Spring Electrode Transoucer Delay rod Solid cu cylinder Cu chamber Ge S H

Sample Transoucer Electrode Spring

Figure 4.10 Experimental arrangement used to reach 1.1 K by pumping in liquid helium.

constriction reduced the film flow substantially, and the system worked exactly as planned, allowing 1.1 K to be reached. This as a good example of the type of know-how which is sometimes needed to perform good low-temperature measurements. The insert in the chamber is also equipped with a temperature sensor and heater for control of the temperature to submillikelvin level.

4.7 The Ginzburg–Landau theory 4.7.1

Some remarks on Landau theory

The Ginzburg–Landau theory [10] for superconductivity represents one of the most useful tools available for the theoretical description of superconductivity. It starts with a free energy expansion, completely in line with the general Landau theory [54] for condensed matter, with particular attention being paid to the term representing the gradient of the ordering quantity. In Section 4.1 we have referred to magnetic analogies to superconductivity for an intuitively simplified discussion of the quantum mechanical wavefunction. We begin here similarly with a brief discussion of the Landau free energy for a ferromagnet, where the ordering quantity is the spin. When spins, or the corresponding magnetic moments µi , are summed up and averaged over the volume they occupy, the magnetization may be expressed as M = i µi /V . M may take different orientations depending on symmetry, in order to minimize the total energy. Examples of such behaviour are commonly found in magnetic

116

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

domains in ferromagnets, where neighbouring domains may have the magnetization pointing in orthogonally different directions due to anisotropy. The domain walls between these small volumes are a kind of topological defects where the spins gradually change direction form one domain to the neighboring one, a configuration called Bloch wall, that costs extra energy to produce. This energy appears in the free energy expansion as the square of the gradient of M. This arrangement is still energetically favorable due to the resulting reduced field energy outside the material. Apart from this, the Landau expansion is permissible when assuming that we perform the calculation of the free energy relatively close to Tc , although not too close in case fluctuations might become important. The point here is that we can define a small parameter in this range, namely m = M(T )/M(0), which is the ratio between the actual magnetization M(T ), and the saturation value M(0) at T = 0. This quantity m(T ) may be used as an expansion parameter to whatever order is necessary. We have still one more aspect to take care of: There is always a background energy F0 (r, T ), which is independent of m. This can most easily be thought of as the entire free energy of the system at m = 0, for instance just above the magnetic ordering temperature Tc . The Landau free energy density is then: 1 1 F (r, T ) = F0 (r, T ) + αm2 + βm4 + c |∇m|2 (4.86) 2 4 Notice here that there are no terms of odd power in the m-expansion. Physically this is due to the obvious fact that the free energy in a ferromagnet must be independent of whether the spins point up or down. This constraint applies to most systems, whether magnetic or not, and is always caused by symmetry. We will now for simplicity confine the analysis to the interior of one domain where M and m are constant, and disregard the remaining terms. Minimizing the remaining free energy, requires

We find The solutions are:

∂F =0 ∂m

(4.87)

2αm + 2βm3 = m(α + βm2 ) = 0

(4.88)

m=0

and

m2 = −

α β

(4.89)

Generally, both α and β are themselves functions of temperature and are to be thought of here as the lowest order term in a temperature dependent expansion of the coefficients of Eq. 4.86. By studying the minimization conditions in more detail one finds that the expansion of α must have a zero’th order term equal to zero, so to lowest order α = α1 (T − Tc )

(4.90)

THE GINZBURG–LANDAU THEORY

117

where α1 is a constant. For β we find that the zero-order term β0 is finite, and we stop the expansion there. This adds up to α1 (Tc − T ) β0 1 1 α1 2 m= (Tc − T ) 2 β0

m2 =

(4.91)

So, the magnetization grows from 0 at Tc , like the square root of Tc − T . Above Tc its value is m = 0 in accordance with the first solution in Eq. 4.89. Both aspects are illustrated in Figure 4.11. What happens physically is that above Tc spins are totally disordered, producing m = 0. Below Tc , however, ordering increases gradually like the square root of temperature measured relative to Tc . Because of the gradual associated ordering taking place in the magnetic spins when T is lowered below Tc , the quantity m is called the ‘order parameter’ of the ferromagnetic transition. We also see that m is indeed suitable as a small quantity to expand in. The above gives an idea of the basic content of Landau theory, applicable to a wide range of systems where ordering takes place below a certain temperature. We have so far neglected the gradient term. This will often not be permissible, as we will see in superconductors.

4.7.2

Ginzburg–Landau theory for superconductors

Magnetization m(T )

The Landau approach works specially well in systems with long correlation length, called coherence length ξ in superconductors. We should measure this length on an atomic scale. Because ξ in low-Tc superconductors can be as long as thousands of interatomic distances (recall for instance Al, with ξ(0) = 1600 nm) superconductors offer a particularly suitable arena for the application of Landau theory, in that case called Ginzburg–Landau theory. As, on the other hand, ξ in high-Tc materials is only of the order of one, or a few, unit cell distances, one

1

(Tc − T ) 2

Tc Temperature T

Figure 4.11 Magnetization m(T ) versus temperature according to standard Landau theory described in the text.

118

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

should rightly be concerned about the validity of Ginzburg–Landau theory in such systems. Experience has shown that for many purposes it works quite well even there, when discussing equilibrium properties. However, one has to exercise great caution. For instance, as we have shown in Section 2.6 one should expect very vigorous thermal fluctuation in the order parameter, the superconducting wavefunction ψ, on approaching Tc . Indeed this causes immense complications in high-Tc as compared to low-Tc superconductors. Leaving those problems aside for now we proceed to develop the Ginzburg–Landau theory of superconductivity. We emphasize the following: The superconducting wavefunction ψ does possess the property required for an order parameter: Its equilibrium value is zero above Tc and increases gradually below Tc when written as 1

ψ = n 2 eiϕ = |ψ|eiϕ

(4.92)

where n is the density of Cooper pairs. Whether we refer to the BCS theory or use the language of the two-fluid model we know that the appearance of the factor n ensures that ψ has the required property. The phase ϑ is another quantity of great importance, and one that we shall dwell considerably on in later chapters. The next important step is to write the gradient term in the free energy expansion in a quantum mechanically appropriate manner. We have to define the momentum operator in a magnetic field, writing p = (−i∇ − 2eA)

(4.93)

where the symbols have their usual meaning in quantum mechanics, and we have introduced the charge −2e of a Cooper pair; and below we introduce its mass m. We are now ready to sum up the terms in the Ginzburg–Landau free energy density for a superconductor: β 1 1 2 |ψ|4 + |(−i∇ − 2eA)ψ|2 + B 2 2m 2µ0 (4.94) We remark here that since all the terms in Eq. 4.94 represent energy densities, the total free energy of the system is

d3 rFs (r, T ) (4.95) Fs (T ) = Fs (r, T ) = Fn (r, T ) + α |ψ|2 +

V

For the ensuing calculations we will define a vector G ≡ (−i∇ − 2eA), and we remind ourselves that the vector potential A is related to the magnetic induction B by B = ∇ × A. Next we carry out the minimization procedure for the free energy by making variations in ψ and ψ ∗ , i.e. by letting ψ → ψ + δψ, and ψ ∗ → ψ ∗ + δψ ∗ . The equilibrium condition δFs (T ) = 0 will then give us the Ginzburg–Landau

THE GINZBURG–LANDAU THEORY

119

equations, two equations of paramount importance in superconductivity. We can immediately write δFs (r, T ) = α(ψ + δψ)(ψ ∗ + δψ ∗ ) − αψψ ∗ β (ψ + δψ)2 (ψ ∗ + δψ ∗ )2 − ψ 2 ψ ∗2 + 2 1 G(ψ + δψ)G∗ (ψ ∗ + δψ ∗ ) − GψG∗ ψ ∗ + 2m

(4.96)

with G as defined above. Next we simplify: δFs (r, T ) = α(ψδψ ∗ + ψ ∗ δψ) + β(ψ |ψ|2 δψ ∗ + ψ ∗ |ψ|2 δψ) 1 + (GψG∗ δψ ∗ + GδψG∗ ψ ∗ ) (4.97) 2m The last parenthesis is GψG∗ δψ ∗ + GδψG∗ ψ ∗ = (−i∇ − 2eA)ψ(i∇ − 2eA) δψ ∗ + (−i∇ − 2eA) δψ(i∇ − 2eA)ψ ∗ (4.98) Summing up:

δFs (T ) =

d3 r (αψδψ ∗ + βψ |ψ|2 δψ ∗

V

1 (−i∇ − 2eA)ψ(i∇ − 2eA) δψ ∗ + c.c.) + 2m

(4.99)

After a partial integration we obtain, using ∇A = 0

1 3 2 2 ∗ δFs (T ) = (−i∇ − 2eA) ψ)]δψ + c.c. d r [(αψ + β |ψ| ψ + 2m V (4.100) Requiring δFs (T ) = 0 demands that the functions in front of δψ ∗ and δψ are zero, which means that we have GL-I:

αψ + β |ψ|2 ψ +

1 (−i∇ − 2eA)2 ψ = 0 2m

(4.101)

This is the first of the two Ginzburg–Landau equations, hereafter referred to as GL-I. Next, as a preparation for the derivation of the second Ginzburg–Landau equation, GL-II, we introduce Maxwell‘s equation ∇ × H = J which we use in the form ∇ × B = µ0 J . We write it out as µ0 J = ∇ × B = ∇ × (∇ × A) = ∇(∇ × A) − ∇ 2 A = −∇ 2 A

(4.102)

in the London gauge where ∇ × A = 0. When we later encounter the term − µ10 ∇ 2 A we will recognize this as the supercurrent J .

120

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

The procedure by which GL-II is obtained is to vary A in the free energy Fs (r, t), i.e. we let A → A + δA and find the corresponding variation in Fs (r, t). For this minimization of the free energy density Fs (T ) with respect to the vector potential A we need only retain the A-dependent parts of Fs (r, t). We write this as Fs (r, t, A). Next we take the variation δFs (r, t, A) = Fs (r, t, A + δA) − Fs (r, t, A)

(4.103)

In writing out the expression here we temporarily introduce the symbol p for −i∇ to simplify the mathematics. The proper operator is immediately reintroduced in the next step. We find 1 (p − 2e(A + δA))ψ (p∗ − 2e(A + δA))ψ ∗ 2m 1 (p − 2eA)ψ (p∗ − 2eA)ψ ∗ − 2m 1 + (∇ × (A + δA))2 − (∇ × A)2 2µ0 e iψ ∗ ∇ψ + iψ∇ψ ∗ + 4e |ψ|2 A δA =− m 1 + (∇ × δA)(∇ × A) (4.104) µ0

δFs (r, t, A) =

Now δFs (r, t, A) is to be integrated over the superconductor volume. We do the last term first:

1 1 3 (4.105) d r(∇ × δA)(∇ × A) = − d3 r∇ 2 A × δA µ0 µ0 Therefore, the entire δFs (T ) becomes

ie 4e2 1 2 3 ∗ ∗ 2 |ψ| A − δFs (T ) = d r (ψ∇ψ − ψ ∇ψ) + ∇ A δA = 0 m m µ0 (4.106) This requires the square bracketed term to be zero. Using the result from Eq. 4.102 the equation for the supercurrent is obtained: e 1 (4.107) (iψ ∗ ∇ψ − iψ∇ψ ∗ ) + 4e |ψ|2 A J = − ∇2A = µ0 m or GL-II:

J =

e ∗ ψ (−i∇ − 2eA)ψ + c.c. m

This is the second Ginzburg–Landau equation.

(4.108)

THE GINZBURG–LANDAU THEORY

121

c

B

Figure 4.12 Flux quantization. The larger area is the superconductor. The small hatched area illustrates a normal domain inside the superconductor where a magnetic flux penetrates a cross section of the sample. The contour c encloses this area completely.

To be precise, in deriving the GL equations so far we have omitted a surface integral:

(4.109) dψ ∗ (−i∇ − 2eA)ψdσ + c.c. This is correct to do if (−i∇ − 2eA)⊥ ψ = 0, i.e. when the normal component of the operator as applied at the surface gives zero. On inserting this condition into GL-II we find that it expresses the condition that no current is entering through the surface, J⊥ = 0. This is physically sound when the surface is a boundary to vacuum or an insulating material. We could turn the question around and ask what boundary condition on ψ would in general make J⊥ = 0. To answer this question, we apply the operator (−i∇ − 2eA)⊥ in GL-II and require J ⊥ = 0, i.e.: J⊥ =

e ∗ ψ (−i∇ψ − 2eA)⊥ ψ + c.c. = 0 m

(4.110)

We continue the discussion of this problem in Chapter 5.

4.7.3

Flux quantization

Imagine that some region of a superconductor is in the normal state due to magnetic flux penetrating it, as illustrated in Figure 4.12. Thus, we may think of the superconductor as a multiply connected domain described by a surface of genus one. In this case, given the order parameter ψ = |ψ|eiϕ the line integral of the gradient ∇ϕ around a closed contour encircling the normal domain has to be given by 2π N , where N ∈ Z. This follows since the order parameter must 2 be singled valued at any given point, and 1 dl∇ϕ = ϕ1 − ϕ2 independent of

122

THE SUPERCONDUCTING STATE – AN ELECTRONIC CONDENSATE

the path connecting the start-and endpoint. Thus we have ! dl · ∇ϕ = 2π N

(4.111)

Now, in the presence of a magnetic field, this is only slightly modified. The magnetic field couples to the superconducting order parameter via the vector potential A in such a way as to modify the phase of the superconducting order parameter by the usual minimal coupling scheme. The gauge invariant phase of the order parameter now has the gradient ∇ϕGI (r) = ∇ϕ(r) −

2e A

(4.112)

where we have used the fact that the charge of the Cooper pair is 2e. Such a modification is necessary in order to preserve gauge-invariance of the supercurrent, a physical observable. We have 2e/ = 2π/(h/2e) = 2π/0 , where the 0 = h/2e = 2.0679 × 10−15 T m2 . It is this gauge-invariant order parameter which now is subjected to the constraint ! (4.113) dl∇ϕGI = 2π N as the requirement of singled-valuedness must still hold. Hence, we obtain ! 2π dl × A = 2π N (4.114) 0 By using this in conjunction with Stokes’ theorem we have

! dl × A = dS∇ × A = dSB ≡ = N 0 C

S

(4.115)

S

where B = ∇ × A and is the magnetic flux through the surface S enclosed by the contour C. This flux is thus seen to be quantized in units of 0 . Note that the only place where any information about the superconducting state enters into this is in the statement that the charge of the superconducting condensate is 2e. Had we had a normal metal, we could apply precisely the same reasoning to the phases of the single-electron wavefunction which couples to a vector potential with the charge e instead of 2e. In that case, we would again get flux-quantization, but with twice the periodicity in magnetic field.

5 Weak Links and Josephson Effects 5.1 Weak links, pair tunnelling, and Josephson effects 5.1.1

Introductory remarks

When two superconductors are brought into contact in such a way that the critical current in the contact region is much lower than that of the individual constituents, the contact is called a ‘weak link’. Before contact is established the two superconducting constituents have independent wavefunctions, and therefore arbitrary and independent phases ϕ. Each superconductor wavefunction is characterized by its amplitude |ψ| and phase ϕ: = |ψ|eiϕ

(5.1)

After establishment of the weak link, coherence is established across the barrier, with a phase difference ϕ causing interference between the previously independent wavefunctions. When a Cooper-pair tunnels from the left side to the right of the junction, say, it probes successively the phases of both wavefunctions, the ‘left’ one with phase ϕl and the ‘right’ one with phase ϕr . More precisely, the system can be described as having one wavefunction as a whole. A typical realization of a weak link is a SIS tunnel junction, consisting of two superconducting films, separated by a very thin oxide layer, typically 1–2 nm thick. For low-Tc junctions the most commonly used superconductors are Nb and Pb. Niobium has turned out to be the best one overall. The critical current density of these junctions may be in the range 103 –104 A/cm2 , far below the typical critical current density of bulk superconductors. Transport across the barrier is a tunnel process, and this explains the low current. Tunnelling of Cooper-pairs naturally occurs with a probability far below that which could be expected for single particles. Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

124

WEAK LINKS AND JOSEPHSON EFFECTS

Josephson predicted in 1962 [8] that such a junction would have entirely new and unexpected properties: It should be able to sustain a supercurrent without application of a voltage; and if driven by an external current source to exceed its critical current, radiation of high frequency electromagnetic waves would appear. These predictions were soon confirmed experimentally, and moved superconductivity into a new era. A weak link system can be established in several ways (Figure 5.1). Instead of a thin oxide layer which was mentioned, other materials may be used, for instance a normal metal, corresponding to an SNS junction, in which case the metal layer can be much thicker. Another well established method is to create the whole system from a single superconductor, by splitting for example a continuous film into two regions, leaving just a narrow constriction between, of typical dimensions like the coherence length ξ . This latter construction is referred to as a Dayem bridge. In this case the critical current density is the same in the bridge and the bulk, but the overall critical current of the device is much lower than in the two parts. This is sufficient to make it a weak link. A recently developed method, specially suited for high-Tc superconductors, takes advantage of their very short, nanometre size coherence length ξ . In these superconductors a very narrow interruption of superconducting properties can be achieved by depositing a high-Tc film across a naturally occurring grain boundary in a substrate like SrTiO3 . The grain boundary forces the superconductor to develop a chain of defects along the length of the grain boundary. Above the grain boundary, therefore, there is a weak link between the two parts of the superconductor film. Such contacts are commonly referred to as grain boundary junctions or bi-crystal junctions. So-called break junctions and step junctions are variations on this method, where the topology of the substrate plays a role in creating the weak link. The observation already made, that the phase difference ϕ between the two sides of the junction provides the driving force for the transport of Cooper-pairs, is something we already could have seen from the Ginzburg–Landau equations. The two driving fields for a supercurrent were found to be the vector potential A ~x

I,N

GBJ Sl Sl

Sr

S

S

Sr

~x GB

(a)

(b)

(c)

Figure 5.1 Different types of weak links, (a) between superconductors Sl and Sr with normal (N) or insulating (I) barrier between; (b) narrow constriction; (c) grain boundary junction GBJ in a superconductor deposited in top of a substrate with a grain boundary (GB).

WEAK LINKS, PAIR TUNNELLING, AND JOSEPHSON EFFECTS

125

and the superconductor phase gradient ∇ϕ. In the case of a Josephson junction between two homogeneous superconductors the phase gradient becomes discretized, i.e ∇ϕr → (ϕl − ϕr )/d where d is the barrier thickness. So, already based on the GL-equations the physics community should not have been too surprised in 1962 by the prediction of a phase difference driven, voltage independent supercurrent across a thin barrier between two superconductors. Once the idea has been put forward one realizes the effect should be expected, provided Cooper-pair tunnelling can take place.

5.1.2

DC Josephson effect: the Feynman approach

The basic equation used in analysing the Josephson effect is the time dependent Schr¨odinger equation i

∂ = E ∂t

(5.2)

1

In a superconductor = ||eiϕ = ρs2 eiϕ , ϕ being the macroscopic superconducting phase and ρs the density of Cooper-pairs. However, when a coupling with overlap exists between the wavefunction to the left, l , and to the right, r , a term must be added to account for the ‘leakage’ of wavefunction so that l changes with time at a rate which is proportional to the amount of leakage from r into the left side. And similarly, a symmetric equation must exist for the rate of change of r . This results in the following modification of Eq. 5.2. ∂l = El l + Kr ∂t ∂r i = Er r + Kl ∂t i

(5.3) (5.4)

Here El and Er are the ground state energies of the unperturbed system when K = 0, i.e. with no transfer of charge. We do not need to know El and Er , but remark that the difference El − Er = −2eV is fixed by the potential difference V . We will take El = Er when K = 0, i.e. for a thick barrier. If we further choose the zero of energy to be midway between El and Er , we can share the potential energy difference between the two states symmetrically [55] by writing: ∂l = eV l + Kr ∂t ∂r i = −eV r + Kl ∂t i

(5.5) (5.6)

126

WEAK LINKS AND JOSEPHSON EFFECTS

The functions l and r may be written 1

1

l = ρl2 eiϕl ;

r = ρr2 eiϕr

(5.7)

i.e. each function is assumed to have a well-defined macroscopic phase, constant in space, and a well defined Cooper-pair density. This first limitation will have to be lifted later, but for the moment we can limit the discussion to a contact area that is very small, so that no spatial variation of ϕ is possible. We can now insert the wave functions with timedependent ρl and ρr into the differential equations (Eqs 5.5 and 5.6) and equate real and imaginary parts separately, a procedure which immediately leads to the following four relations, with γ ≡ ϕr − ϕl : K ∂ϕr =− ∂t ∂ϕl K =− ∂t

ρl ρr ρr ρl

1 2

cos γ +

eV

(5.8)

cos γ −

eV

(5.9)

1 2

1 2K ∂ρr =− (ρl ρr ) 2 sin γ ; ∂t

1 2K ∂ρl = (ρl ρr ) 2 sin γ ∂t

(5.10)

We note that variations of phase ϕ is due to the combined effects of the phase difference γ across the contact, and the potential difference V . Variations in pair density, on the other hand, are solely due to phase difference γ . The supercurrent across the contact is straightforwardly calculated by use of J = −2e

∂ρl ; ∂t

or

J = −2e

∂ρr ∂t

(5.11)

The time derivatives are already given above, so that we have: J =

1 4Ke (ρl ρr ) 2 sin γ

(5.12)

J = J0 sin γ

(5.13)

which we often rewrite as

a major result in the Josephson theory. It tells us that a supercurrent is driven across the thin barrier separating two superconductors simply by the superconducting phase difference across the barrier. The predictions from the theory outlined above have been extensively confirmed experimentally. An example of an IV-characteristic showing the DC Josephson current is seen in Figure 5.2. The data are from an S1 IS2 structure,

WEAK LINKS, PAIR TUNNELLING, AND JOSEPHSON EFFECTS

127

Figure 5.2 The I-V curve of a 0.7-µm square Nb/AlOx /Nb Josephson junction. The vertical scale is 20 µ A/div and the horizontal scale is 1 mV/div.[56]

with S1 = Nb and S2 = Pb. It shows the Josephson DC current at finite voltage which was discussed previously. Note that these measurements show the I-V curve for both positive and negative bias. The fact that a voltage is not needed to drive a supercurrent is something we already know well from the Meissner effect. In Chapter 6 we will find that the vector potential provides the driving mechanism. The Josephson effects established the phase of the wavefunction as a driving mechanism on equal footing with the vector potential, or magnetic field. The superconducting phase thereby took on a more firm and real existence. Observations of the corresponding physical effects followed, first few in numbers, then in abundance in the years after Josephson’s prediction. Superconductivity

Normalized current i

1.5

1

0.5

0

Figure 5.3

0

0.5 1 Normalized voltage, v

1.5

Quasiparticle current in intrinsic junction in Bi2 Sr2 CaCu2 O8 crystal [57].

128

WEAK LINKS AND JOSEPHSON EFFECTS 60

Current I (mA)

T = 68 K

0

−60 −0.15

0

0.15

Voltage (V)

Figure 5.4 I-V characteristic of (Pb0.2 Bi0.8 )2 Sr2 CaCu2 O8 crystal at T = 68 K showing intrinsic Josephson effect. After Kleiner et al. [58].

broadened its territory enormously by these discoveries, as mentioned before. In particular a range of unprecedented possibilities opened up in the area of electronic applications. An unusual realization of the Josephson effect was observed in a single crystal high-Tc superconductor Bi2 Sr2 Cu2 Cu3 O10 . This strongly anisotropic, layered structure consists of alternating superconducting CuO2 -layers separated by nonsuperconducting ones. The material can behave like a stack of SIN- and SISstructures. Hence, currents flowing along the c-axis normal to the layers have been observed, corresponding to either quasiparticle current or supercurrent, as seen in Figures 5.3 and 5.4 [57, 58].

5.2

AC Josephson effect

Josephson’s discovery included, however, another effect, one which even in hindsight may be seen as a surprising phenomenon an applied voltage across an junction would bring about an oscillatory variation of phase difference. We can find this fact from analysis of the time dependence of the phase difference by taking the difference between Eq. 5.8 and Eq. 5.9. This gives the Josephson frequency ωJ , when ρl = ρr , by ∂γ ∂ 2e = (ϕr − ϕl ) = ωJ = V ∂t ∂t

(5.14)

which is in an observable range, since V = 1 µV leads to fJ ≡ ωJ /2π = 483.6 MHz. We are speaking here of electromagnetic phenomena related to the movement of charge at elevated frequency: The Josephson contact emits electromagnetic radiation at the frequency ωJ .

AC JOSEPHSON EFFECT

129

Equation 5.14 for the Josephson frequency can be integrated to give the time dependence of the phase difference in zero magnetic field: γ = γ0 +

2e V t = γ 0 + ωJ t

(5.15)

Clearly then, as the Josephson current depends on sin γ , it will now be modified to J = J0 sin(γ0 + ωJ t)

(5.16)

It is this oscillatory Cooper-pair current which generates the microwave electromagnetic radiation. In the opposite case, when microwave radiation is incident )ωJ on the I-V curve. on the junction, steps appear at regular intervals Vn = n( 2e These steps, caused by absorption of n quanta of electromagnetic radiation at the Josephson frequency, are called Shapiro-steps after their discoverer. Figure 5.5 illustrates the I-V characteristic during illumination by electromagnetic radiation at ω = ωJ .

5.2.1

Alternative derivation of the AC Josephson effect

The simplified derivation of the AC Josephson effect did not explicitly bring out the role of the vector potential A, related to the B-field by ∇ × A = B. We therefore rederive the AC Josephson current in a manner which makes the role of A explicit. In so doing we have to use a gauge invariant form of the phase difference across the barrier. The necessity of doing this is seen in the PRF = 0

Voltage (µV)

600 300 0

PRF > 0

Increasing

4 Step number

3 2

2∆ In

1

−300 −600 I (arbitrary units)

Figure 5.5 Microwave-induced Shapiro steps in I-V curves of a Nb point contact Josephson junction at 4.2 K at different microwave power levels irradiating the junction at 72 GHz. I-V curves are shifted for clarity [59].

130

WEAK LINKS AND JOSEPHSON EFFECTS

GL-equations where the correct quantity to consider is ∇ϕ −

2e A

(5.17)

To bring out the phase difference between the two sides we integrate from left to right and get: γl→r

r r 2e 2π = A dl ∇ϕ − A dl = ∇ϕ − 0 l l

(5.18)

where it is understood that the integration starts on the left-hand side of the junction (see Figure 5.1a), at a point which is deeper than the penetration of magnetic field, and ends similarly on the right side. We have also inserted 0 for h/2e. Taking the vector potential Az (x) to be parallel to the direction of integration z, normal to the contact, corresponds to placing the B-field parallel to the contact plane, and pointing along the y-axis, with By (x) = ∂Az /∂x. On integrating we obtain γl→r

2π = (ϕr − ϕl ) − 0

r

Az dz

(5.19)

l

The phases ϕr and ϕl may be taken here to be fixed phases which exist in the absence of any AC current. Even though ϕ may not be well defined in the junctions, we may write the integral of the gradient as the difference between the endpoints and neglect a 2π × n contribution. When we take the time derivative z of this last relation we find, using Ez = − ∂A ∂t , r ∂Az ∂γ −1 −1 = −2π 0 dz = 2π 0 Ez dz = 2π −1 0 V ∂t ∂t l ∂γ 2e = V = ωJ as before. ∂t

(5.20) (5.21)

This derivation brings out explicitly the point that the AC Cooper-pair supercurrent across the contact is driven by a time-dependent vector potential, which again is created by a static electric field by the voltage V . A relevant question is now whether this current, being a Cooper-pair supercurrent, is lossless. A DC super-current can run forever as long as it is truly DC. But here, we are discussing time-dependent currents, i.e. accelerated mass and charge, and the process can only be sustained as long as we feed energy into the circuit. This will be the case in any super-current charge transport. In addition to this loss, observation shows that energy is radiated from the contact as a microwave electromagnetic field. Thus the Josephson effects are quite complex phenomena. The Shapiro steps (see Figure 5.5) in the I-V diagram

JOSEPHSON CURRENT IN A MAGNETIC FIELD

131

resulting from feeding microwave power into the contact is another manifestation of the energy exchange involving Cooper-pair super-current. More precisely, transfer of a Cooper-pair across the barrier costs an energy 2eV = ωJ , exactly the photon energy. Some of this energy is radiated, as mentioned.

5.3

Josephson current in a magnetic field

One of the truly remarkable and useful aspects of the Josephson contact comes about when its sensitivity to magnetic field is considered. Let the planar junction be placed in the xy-plane, with the magnetic field parallel to the y-axis. The GL-equations tells us that the DC supercurrent will be established according to ρe Js = (5.22) (∇ϕ − 2eA) m This current is the equivalent of the Meissner-effect according to London theory, but with the addition of a ∇ϕ driving term. Eq. 5.22 is easily rewritten as 2e m ∇ϕ = Js + A (5.23) 2e2 ρ Now choose an integration contour as shown in Figure 5.6, where the film thickness direction is along the z-axis, and the B-field along the + y-axis. We define the sum of length parameters λL + λR + δ = dJ . The length of the junction is L. Next, we perform an integration of Eq. 5.23 along the contours CL and CR in the superconductors, resulting in 2e m ϕRa (x) − ϕRb (x + δx) = A + 2 Js δl (5.24) CR 2e ρ 2e m A + 2 Js δl (5.25) ϕLb (x + δx) − ϕLa (x) = CL 2e ρ lR

lL CL

La

CR

Ra ∆x

L

By

x

Lb

z

Rb d dJ

Figure 5.6 A good choice of integration path.

132

WEAK LINKS AND JOSEPHSON EFFECTS

Now we exploit the following possibility: (i) The integration parallel to the junction may be performed so deep in the superconductor that screening current density is zero on both sides; (ii) that part of the integration which is done within the penetration depth of field and screening currents may be performed at right angles to that current. Figure 5.6 illustrates these two points. Forming now the phase difference ϕ(x + x) − ϕ(x) this can be achieved by manipulation of Eqs 5.24 and 5.25: ϕ(x + δx) − ϕ(x) ≡ ϕLb (x + δx) − ϕRb (x + δx) − ϕLa (x) − ϕRa (x) (5.26) 2e 2e ϕ(x + δx) − ϕ(x) = A · dl (5.27) A · dl + A · dl ≈ CL CR when we have taken λL + λR δ, which is a good approximation in most cases. Also the contribution from the two gaps will tend to be of opposite sign and equal size. Integration across the thickness δ can therefore be neglected. The result is that the phase difference across the barrier depends on x, as we get 2e ϕ(x + δx) − ϕ(x) = A · dl 2e = By (λR + λL + δ)δx = 2π −1 0 By dJ δx

(5.28)

which in integrated form becomes ϕ(x) = 2π −1 0 By dJ x + ϕ0

(5.29)

The shielding supercurrent density can now be written down using the standard Josephson relation Eq. 5.13. J = J0 sin(2π −1 0 By dJ x + ϕ0 ) 2π = J0 sin x + ϕ0 λϕ with λϕ =

(5.30)

0 By dJ

The interesting result is that the Josephson current across the barrier is a sinefunction, in other words varying in sign and amplitude along the direction perpendicular to the magnetic field, as illustrated in Figure 5.7. Looking at the whole pattern of super-currents in a Josephson junction in the presence of a magnetic field one recognizes the similarity with vortices

JOSEPHSON CURRENT IN A MAGNETIC FIELD

133

lj

Figure 5.7

A periodic pattern of supercurrent circulation in a Josephson junction.

penetrating a type II superconductor. In addition to the current crossing the barrier, charge conservation requires currents to flow along the contact in the direction transverse to tunnelling currents. This establishes a periodic pattern of supercurrent circulation, with the period λϕ defined previously (see Figure 5.7). The associated vortex patterns are called Josephson vortices. We note here that although similar to the usual vortices in type II superconductors, they are of a different nature since they have no normal core. Consequently, no upper critical field Hc2 is associated with the Josephson vortices. From Figure 5.7 one can immediately conclude (neglecting end effects) that a rectangular junction will obey a simple rule that the current is zero every time the relation L = nλϕ = n

0 By dJ

(5.31)

is satisfied, or at values of the magnetic field which obey: By = n

0 ; LdJ

n = 1, 2, 3 . . .

(5.32)

in other words every time an integral number of flux quanta is located in the junction. In case ϕ0 = 0 maximum current will appear at every field corresponding to the condition L = (n + 12 )λϕ

or

0 By = (n + 12 ) Ld ; J

n = 0, 1, 2 . . .

(5.33) (5.34)

The total current is found by integration of Eq. 5.30. Assuming we have a rectangular contact of area S = LW the current is found by integrating over the area S:

i λ2πϕ x−ϕ0 I = J0 sin ϕ(x)dS = e iJ0 e dS (5.35) S

S

where J0 is assumed to be constant, and dS = W dL

134

WEAK LINKS AND JOSEPHSON EFFECTS Ic

0

1

2

3

4

5

Φ Φ0

Figure 5.8 DC Josephson effect in magnetic field. Maximum zero-voltage current as a function of the magnetic flux.

The integration gives the following Josephson diffraction current: sin(π B /0 ) Imax = I0 (0) π B /0

(5.36)

Here we have removed a factor sin ϕ0 whose maximum is 1. Figure 5.8 shows a graph of I (B). Based on these results one can conclude that the principle for a sensitive detector of magnetic field has been established due to the sensitivity of the current in a Josephson junction to magnetic field. But the possible device described above is easily surpassed by a different design, which is far more sensitive. This is the SQUID, which we discuss next.

5.4

The SQUID principle

The SQUID (an acronym for superconducting quantum interference device), employs a design with two current paths in a loop-like structure. Current is fed into the loop on one side and collected on the other, in principle as sketched in Figure 5.9. In reality, the structure is usually made of flat layers of thin films, in a superconductor-insulating-superconductor sequence. Figure 5.9 can be thought of as a cross-section through such a structure. A complete contour is drawn inside the two superconductor branches, deep enough that we can regard the current as 2eA vanishingly small. In other words we assume: Js = ρe m (∇ϕ − ) = 0 which requires ∇ϕ = 2e A along the dashed contour C. We integrate this relation along C, and add also to this the integration across both junctions to make a complete closed contour, to obtain 2e (ϕr (a) − ϕl (a)) − (ϕr (b) − ϕl (b)) =

A · dl

(5.37a)

THE SQUID PRINCIPLE

135

a

I

l

r

I

Φ C

b

Figure 5.9

A double Josephson junction structure.

or 2e γa − γb =

A · dl =

2π 0

(5.37b)

where γa = ϕr (a) − ϕl (a); γb = ϕr (b) − ϕl (b). The total lumped current I can now be written as a sum of the currents across junction a and junction b:

resulting in

I = I0 sin(ϕr (a) − ϕl (a)) + I0 sin(ϕr (b) − ϕl (b))

(5.38a)

I = I0 sin γa + I0 sin γb

(5.38b)

π π sin γb + I = 2I0 cos 0 0

(5.38c)

by use of standard trigonometric relations for the addition of sine functions. The maximum current which the device can carry without dissipation is Imax = 2I0 | cos(π /0 )|

(5.39)

With this device a flux change B 0 can be detected. And since the area where the flux is felt by the SQUID (i.e. the whole loop) is much larger than the Josephson contact discussed previously, this shows that the SQUID can be many orders of magnitude more sensitive than a single contact in magnetic field measurements. This result is the basis for most applications of the SQUID. We shall return to that issue in Chapter 11. Calculation based on Eq. 5.39 for the resulting current through a two-point contact is illustrated in Figure 5.10. The flux introduced in the analysis above consists of two parts; the external flux e due to the applied magnetic field, and the flux LIscr due to screening currents Iscr in the loop with inductance L. In other words = e − LIscr

(5.40)

136

WEAK LINKS AND JOSEPHSON EFFECTS

Imax 2I0

1

0.5

0

1

2 Φ/Φ0

3

Figure 5.10 Maximum current which is possible to pass through a SQUID, as a function of the flux through it, measured in units of 0 .

Clearly, the maximum current Imax referred to previously is influenced by the presence of flux generated by screening currents, and the simple result given in Eq. 5.39 is strictly valid only when LIscr is negligible. In Chapter 11 we discuss the equations of motion for the DC SQUID in greater detail, and give references to extensive literature. A new and interesting development in SQUID physics and technology has taken place by the discovery of d-wave pairing in high-Tc cuprate superconductors. We recommend reading about the outstanding work described by Mannhart in the a topical contribution to this book, in Chapter 13.

5.5

The Ferrell–Prange equation

What happens to screening currents in a Josephson junction exposed to an external magnetic field? We now address this question, referring to Figure 5.11, a sketch of the situation we discuss. We recognize the main structure as that of a Josephson junction of length L in the x-direction and with an external field applied along the y-axis. In the presence of the applied B-field screening currents are generated. In the superconductor these penetrate to a usual depth λ. However, where the screening current crosses the insulator barrier, the density of Cooper-pairs is much lower than in the superconductor bulk or film. Hence the screening length is much larger in the junction. This length is usually called the Josephson penetration depth λJ . The previously defined lengths dJ and δ are also indicated in the figure. Our task is now to express λJ in terms of other known parameters. We can now repeat the procedure previously adopted, i.e. integrating the relation ∇ϕ = 2e A along a closed contour crossing the junction at distances dx like before. 2e γ (x + dx) − γ (x) = A · dl (5.41)

THE FERRELL–PRANGE EQUATION λ

137

dJ

λJ

B

δ

L

x

z

Figure 5.11 Illustration of geometries relevant to derivation of the Ferrel–Prange equation.

The right-hand side becomes 2e d 2e A · dl = d = 2π 0

(5.42)

where d is the flux enclosed within the contour, between the contour crossings at x and x + dx. The integration on the left side of Eq. 5.41 at x and x + dx leads to dγ = γ (x + dx) − γ (x) = 2π

d 0

(5.43)

in the same notation and by the same argument as before. We can write this as dγ 2π d = dx 0 dx

(5.44)

We can now introduce the magnetic field instead of the flux by observing that B=

d dJ dx

(5.45)

Introducing this into Eq. 5.44 gives us 2π dj d 2π dJ dγ = = B dx 0 dJ dx 0 0 dγ B= 2π dJ dx

(5.46)

138

WEAK LINKS AND JOSEPHSON EFFECTS

From Maxwell‘s equations we get the supercurrent density Js = ∇ × H = µ0 ∇ × B = µ0 dB dx along the z-axis. When this is inserted into Eq. 5.46 together with J = J0 sin γ we find: 2π J0 µ0 dJ d2 γ = sin γ 2 0 dx

(5.47)

1 d2 γ = 2 sin γ 2 dx λJ

(5.48)

which is usually written

This is the Ferrell–Prange equation [60] which predicts how the screening field penetrates into and parallel to the Josephson junction, with λJ =

0 2π dJ µ0 J0

1 2

(5.49)

When the phase difference γ is very small sin γ can be approximated by γ . In this case we get 1 d2 γ = 2γ 2 dx λJ

(5.50)

γ (x) = γ (0)e−x/λJ

(5.51)

which is easily solved as

Using this in the previously found relation for B, Eq. 5.46, we obtain B(x) = B(0)e−x/λJ

(5.52)

The Josephson penetration depth can be estimated on the basis of typical values for the parameters entering in Eq. 5.49. With J0 ∼ 102 A/cm2 and dJ ∼ 10−5 cm, one finds λJ ∼ 0.1 mm. The result is that λJ is much larger than λ, as we argued from the outset.

5.6

The critical field Hc1 of a Josephson junction

What field could we guess is required to force Josephson vortices into a Josephson junction using an external field? For this question we already have a relevant reference: The argument leading to an expression for Hc1 in bulk superconductors. In the bulk we expect Hc1 to be determined by distributing one quantum

JOSEPHSON VORTEX DYNAMICS

139

of flux 0 over the characteristic area for penetration of flux in the presence of the Meissner effect, i.e. π λ2 . This leads to the approximate expression Hc1 ≈ 0 /π λ2 in bulk superconductors. In the case of a Josephson junction there are two characteristic lengths, one along the junction, λJ , and one transverse to it, dJ , as introduced before. We should therefore expect Hc1 in the junction to be approximately given by Hc1 ≈

0 dJ λJ

(5.53)

which is indeed correct to within a numerical factor of order unity. The precise expression turns out to be Hc1 =

5.7

2 0 . π 2 dJ λJ

(5.54)

Josephson vortex dynamics

We have only discussed static vortices above. A lot of interesting physics is connected with dynamic phenomena, i.e. Josephson vortices in motion. Because of the fact that these do not have a normal core, as mentioned, they can move extremely rapidly and with minute losses within the junction. Vortex dynamics is described by the Sine–Gordon equation. In deriving the Josephson penetration depth λJ via the Ferrell–Prange equation we came close to this problem. One only needs to add a dynamic term to the equation, namely the acceleration 2 term ∂∂tγ2 to change the validity from that of a static to a dynamic description, resulting in ∂ 2γ ∂ 2γ 1 + = 2 sin γ ∂x 2 ∂t 2 λJ

(5.55)

The solution of this equation is solitary-like, i.e. representing the Josephson vortex as a solitary wave in a non-linear medium. Figure 5.12a shows the location of the vortex in the junction, and Figure 5.12b shows a representation of the solitary wave in more detail. This solitary wave moves along the junction with a speed close to that of the speed of light due to its low dissipation in the absence of a normal core. Moreover, high frequency radiation is generated from the junction as the solitons reach the surface in rapid succession. The solitary waves can be driven by a current source or a voltage source applied to the junction.

140

WEAK LINKS AND JOSEPHSON EFFECTS Φ0

ity

c Velo

x

z

By magnetic field

J supercurrent

y (a)

Figure 5.12

(b)

The Josephson vortex as a solitary wave. After Pedersen [61].

A practical problem arises in the use of these junctions as high-frequency radiation sources due to the great mismatch of impedance between the junction and the surrounding vacuum. This mismatch is caused by the difference in wave velocities. In the case of solitary wave analysis it is necessary to consider an extended or long junction, with a length L λJ . In a long junction one includes the effects of the self field in addition to the externally applied magnetic field. This corresponds to taking into account the screening currents in the SQUID, a possibility we already pointed out. For a general introduction to soliton physics in Josephson junctions, see reference [61].

5.8 Josephson plasma in cuprate high-Tc superconductors An interesting development related to the Josephson effects was the prediction [62] and observation by numerous groups, among them Matsuda and coworkers [63], of plasma effects in Bi2 Sr2 CaCu2 O8+δ . Neighbouring superconducting CuO2 layers are coupled by the Josephson effect through the block layers between the CuO2 layers, and the Josephson plasma is generated by the coupling between the Josephson current flowing along the c-axis and the electromagnetic field, leading to current oscillations at frequencies well below the superconducting gap frequency, in the GHz to THz range. Longitudinal and transverse plasma waves propagating along the c-axis and in the ab-plane are of quite different nature. These phenomena have already been developed to an advanced stage, and it has become possible to make devices that emit electromagnetic waves in the THz range. Another, related phenomenon is the interaction between the plasma and vortices. This leads to strong dependencies of the plasma frequencies on the state of the vortex matter created by an external magnetic field. Furthermore, the static interaction between pancake vortices and Josephson vortices has led to new insight into so-called crossing lattices of vortex matter.

6 London Approximation to Ginzburg–Landau Theory (|ψ| constant) 6.1 The London equation and the penetration depth λL 6.1.1

Early electrodynamics and the London hypothesis

Figure 6.1 describes an essential property of Meissner screening: The interior of a superconductor is shielded against a static magnetic field, a phenomenon we already discussed briefly in Chapter 1. We will now discuss the physics of this effect and its history. Already years before the discovery of Meissner screening, speculations had been made by Onnes among others, that the current in a superconductor might involve surface currents. The discovery made by Meissner and Ochsenfeld [3] in 1933 proved that this was correct, in the case of diamagnetic response to an external magnetic field. Logically the magnetic field could be expelled from the interior only by setting up a surface current. But the current could not exist only in the surface. It would have to penetrate to a certain depth called λ. If this were not so, a finite current should exist in a layer of zero thickness, which would imply an infinite density of free charge. Since there is of the order of one free charge pr metal atom, the penetration depth must be finite, and its length must be controlled by the free electron number density ne . The more electrons are present per volume, the more effective is the screening, and the shorter must λ be. The prediction for an electrodynamic screening length λ had already been made by de Haas Lorentz [64] in 1925. In modern SI units it reads 1 λ = (mq /µ0 ns q 2 ) 2 (6.1) where q is the charge of the carriers in the superconducting state, mq their mass, and ns their number density. This is the same formula that we use for screening Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

LONDON APPROXIMATION TO G–L THEORY

Penetrating field B(x)

142

Ba Bae−x/l l ~ 100−1000 nm

l Distance from surface, x

Figure 6.1

Meissner screening.

of a static magnetic field today. The prediction would give a penetration depth of about 50 nm in typical metals, a value which later has turned out to be in good agreement with observation. The derivation of the result for λ goes as follows: Near the surface of a superconductor an electric field can exist, accelerating the superconducting electrons frictionlessly according to mq v˙ = −qE

(6.2)

where, v is the carrier velocity and E the electric field. Time derivative is indicated by the dot. Since current density can be written as J = −ns qv this gives an expression for E: E=−

mq v˙ µ0 mq J˙ = = µ0 λ2 J˙ q µ0 ns q 2

(6.3)

Taking the curl on both sides we obtain ∇ × E − µ0 λ2 ∇ × J˙ = 0

(6.4)

Using ∇ × E = −B˙ we find µ0 λ2 ∇ × J˙ + B˙ = 0

(6.5)

Applying Maxwell’s equation ∇ × B = µ0 J leads to λ2 ∇ × ∇ × B˙ + B˙ = 0

(6.6)

˙ hence The first term is equal to −∇ 2 B, ∇ 2 B˙ =

1 ˙ B λ2

(6.7)

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

143

˙ from the surface towards the interior, The solution is an exponential decay of B over the characteristic distance λ Note that this is proposed as the electrodynamics of a superconductor. It is fundamentally different from the skin depth of a metal since we assumed frictionless motion of charge. Heinz and Fritz London [65] observed that on performing the time integration of Eq. 6.7 one is left with an equation between a static magnetic field B and a stationary current J , with an additional unknown integration constant. Setting the constant of integration equal to zero, they obtained B = −µ0 λ2L ∇ × J

(6.8)

Here we have renamed the parameter λ as λL . Equation 6.8 is the famous (second) London equation, which correctly describes the Meissner effect mathematically. Furthermore, on introducing the vector potential A via ∇ × A = B, we obtain the profound relationship between the vector potential and the supercurrent J =−

1 µ0 λ2L

A = −A

(6.9)

Notice that this equation is analogous to Ohm‘s law: J = σ E. Hence, in a superconductor exposed to a static magnetic field it is the vector potential A that drives a stationary supercurrent J . The factor is a response function, analogous to the conductivity σ in a normal metal. Although this equation seemed to express the Meissner effect correctly, and as such was a major achievement, its justification on microscopic grounds remained unknown since the London treatment is purely phenomenological. To justify the result from first principles remained a challenge for more than 20 years, until the famous BCS paper of 1957 [7]. In any case, the phenomenological basis for the important length parameter λL , the London penetration depth, had now been established and a prediction made for the screening length of a static B-field. It is mathematically the same parameter as was originally found by de Haas Lorentz, a fact which has gone largely unnoticed in the scientific literature. For completeness we repeat the simple steps leading to the Meissner effect as a consequence of the finite screening length λL for static magnetic fields. Our starting point is now the London Eq. 6.8, which we rewrite as B + λ2L ∇ × ∇ × B = 0

(6.10)

The simplest situation is the 1-dimensional case with the field applied parallel to the z-axis along the surface of a superconductor of long length along y, and with the x-axis measuring the distance from the surface into the superconductor, as already depicted in Figure 6.1. Equation 6.10 may be reformulated into B = λ2L ∇ 2 B

(6.11)

144

LONDON APPROXIMATION TO G–L THEORY

with the solution in the 1-dimensional case − λx

B(x) = Ba e

(6.12)

L

Ba is the externally applied induction field related to the applied field Ha by Ba = µ0 Ha . The solution of the London equation shows the significance of the parameter λL as the screening length over which the applied field is reduced to Ba /e. The length λL is mainly controlled by the superfluid density ns . BCS theory showed later that due to pairing of electrons the mass mq and charge q are twice that of the normal electron gas, and the full value of ns is half of the density n in the normal state. We could introduce factors of 2 in the mass, charge and particle density, but the end result is the same for λL . These factors cancel out, and the zero degree value of λL acquires the same value by either choice. In the case of pure metals the main variations in ns from one metal to another come from different valency. The typical values of the calculated λL lie in the range 40–50 nm in metallic superconductors such as Al, Sn and Pb. Because there is an effective mass involved, as well as different band structures, deviations from the ideal values are to be expected. In doped superconductors on the other hand, ns is of course determined by the doping level rather than by band structure effects. The solution (Eq. 6.12) precisely describes the Meissner effect: when an external static magnetic field is applied to a superconductor, supercurrents arise spontaneously in the surface layer to a characteristic depth λL so as to create an opposing field in the sample, exactly cancelling the applied field inside. It depends on the shape of the superconducting sample how the currents run, and whether the screening is complete or not (Figure 6.2). A partial deeper penetration of field will often occur, depending on the demagnetization factor of the sample with respect to the direction of the applied field. We refer back to Section 1.7 for a brief discussion of this point. Experimental values for the relative penetration depth λ were determined in Ref. [66] which reported on the temperature dependence of the quantity λ/λ0 where λ0 is the value near 0 K. It showed a steep descent of λ/λ0 below and

Js

Js

Js Ha Ha

Figure 6.2 field.

Ha

Some examples of sample shapes and screening currents in an external magnetic

145

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

away from the transition temperature Tc . This corresponded well with the two 2 fluid model of Gorter and Casimir [67], which would give λλ0 = 1−[T1/T ]4 . c These authors had introduced the idea that the electron gas in the superconducting state consists of a uniform mixture of two electron fluids, one being the normal component and having properties like in the normal state, the other one being the superfluid component observed only below Tc , and being responsible for the superconducting properties. In the two-fluid model they argued that a fraction w of superconducting electrons would condense into an ordered state, and vary from zero at T = Tc to unity at T = 0 according to 1 − (T /Tc )4 . When this was put into the expression for λ the experimentally observed behavior would result. Figure 6.3 shows data by Schawlow [68] confirming that this form even agrees well with BCS theory. After World War II, Pippard [69] performed measurement of the surface impedance of metals at radio-frequencies up to 1200 MHz. In the normal state the penetration is the familiar classical skin depth δ, which, upon passing below Tc becomes λ. The wave-vector dependence had not yet been sorted out; the possibility remained therefore that the measured λ could be different from the λL which had been predicted for the DC case. Even so, the data seemed in harmony with the predictions of the two-fluid model. Further measurements of λ in the presence of a static magnetic field led Pippard to propose the existence of a new length parameter, the superconducting coherence length ξ , which would cause the observed entropy change in pure tin at the superconducting transition to be distributed to a depth as much as 20 times the penetration depth λ. 1400 1200

− BCS theory Experimental data

dy

dl ˚ (A)

1000 800 600 400 200 0

1

2

3

4

5

1 y= √1 − t4

Figure 6.3 Early results on the temperature dependence of λ in a type I superconductor [68].

146

LONDON APPROXIMATION TO G–L THEORY

A decisive step was taken when Pippard showed that, contrary to the prediction of the London theory, λ depended very sensitively on impurity scattering. With the addition of only 3% indium to tin λ changed by a factor of 2, while at the same time the changes in Tc and Hc were insignificant. In the London theory λ depended only on m/n, offering no hint at an explanation. Figure 6.4 shows data demonstrating the effect of the mean free path l on penetration depth λ. Pippard realized that the key point was a breakdown of the underlying assumption of local response in the London theory. We shall return to Pippard’s analysis in Section 7.3.

6.1.2

Derivation of the London equation from the free energy

The London equation applies in the presence of a magnetic field, giving rise to both a kinetic energy density Fk and a magnetic energy density Fm . The superconductor is already at a temperature T < Tc when the London equation takes effect, so the total energy includes also the condensation energy density Fs . The total energy density F for the problem is found by integrating the three densities over the volume V : 3 3 F = Fs (r)d r + Fk (r)d r + Fm (r) d3 r (6.13) V

V

V

We may regard the condensation energy density as unaffected by the application of a magnetic field. Then Fs (r) d3 r = Fs may be regarded as a constant

106 l (cm)

10

5

10

20

30

40 106l (cm)

50

Figure 6.4 Pippard non-local behaviour as evidenced by mean free path dependent penetration depth. After J. Waldram, thesis 1961 [70] and Lynton, 1962 [71].

THE LONDON EQUATION AND THE PENETRATION DEPTH λL

147

background term. The kinetic energy is

1 2 mv (r)ns d3 r Fk (r)d r = 2 s µ0 λ2L J 2 (r) d3 r = 2

Fk =

3

(6.14) (6.15)

which is obtained on writing J = −ns ev s . The magnetic energy is Fm =

Fm (r) d3 r =

1 2 b (r) d3 r 2µ0

(6.16)

In Eq. 6.16 we have introduced the vector b allowing it to represent local induction on a scale smaller than λL . For later treatment of the physics of the flux lines this allows a distinction between induction on scales larger than λL represented by B and on scales smaller than λL . Hereafter we write λ for λL . After combining all three terms, introducing b, and using the Maxwell equation µ0 J = ∇ × b we find F = Fs +

1 2µ0

λ2 (∇ × b(r))2 + b2 (r) d3 r

(6.17)

We want to vary b(r) an amount δb(r) and find the corresponding δF , i.e. we replace b(r) with b(r) + δb(r) and take the difference in F before and after the operation. The resulting δF to lowest order in δb is found to be 1 δF = 2µ0

2bδb + 2λ2 (∇ × b)(∇ × δb) d3 r

(6.18)

To obtain the condition under which the free energy is minimized we set δF = 0. We find that this requires b(r) + λ2 ∇ × ∇ × b(r) = 0

(6.19)

Here we have recovered the London equation. The physical meaning of the London equation is therefore to express the minimization condition for the free energy of the superconductor in the presence of a magnetic field. This is a result worth contemplating. It takes some of the mystery out of the London equation. There is a good, understandable reason for this equation, which was originally postulated without proof.

148

LONDON APPROXIMATION TO G–L THEORY

6.2 The energy of a single flux line Upon subjecting a type II superconductor to a field higher than Hc1 the Meissner screening breaks down, and individual flux quanta penetrate the superconductor. An important problem with regard to the physics of the vortex state, referred to as the mixed state between Bc1 and Bc2 , is the determination of the energy contents of a flux line. We will calculate this quantity as the energy per unit of length. We begin by deriving an expression for b(r), and then integrate the energy density associated with the field and currents in a flux line. The aim of the calculation will be to find, in the London approximation, the sum of kinetic and magnetic energies whose densities were already given in Eqs 6.15 and 6.16, respectively. The background energy Fs is of no interest in this context. We find F =

1 2µ0

b2 (r) + λ2 (∇ × b(r))2 d3 r

(6.20)

r>ξ

The limit of integration is a reminder that we cannot include the vortex core, of radius ξ , in this derivation because the London equation does not apply when ns varies in space. The justification for this approximation is that ξ λ in most type II superconductors, notably in all high-Tc materials. The energy associated with the vortex core is therefore quite small. The energy F is also often referred to as the line tension. It tells us how much energy is required to create extra length of flux line. Flux lines are not like rubber bands, there is no elastic energy associated with stretching a straight flux line. However, it does require extra length to bend a flux line in a superconductor, either uniformly or locally, and the energy per unit length required to achieve this elongation is the line tension. A practical way of approaching this problem was discovered by the Russian physicist Abrikosov1 (1957) [4, 5]. We replace the singularity inside r < ξ when we let ξ → 0 by a 2D delta-function δ2 (r). Let us first discuss that aspect. The London equation now takes the form: b + λ2 ∇ × ∇ × b = 0 δ2 (r)

(6.21)

Notice that higher order terms in δb in Eq. 6.18 are neglected. The deltafunction represents a solution where b(r) is not smooth. In Eq. 6.21 0 is a vector along the direction of the induction normal to the surface, where 0 is the flux associated with an area of radius |r| ∼ λ. 1 It was not immediately obvious that the approach of Abrikosov was correct. It is known that Landau rejected it when Abrikosov first presented it to him. This delayed the publication of Abrikosov’s theory by years. The consequences of Abrikosov’s idea were far-reaching, however, leading to the prediction of a flux line lattice, a truly remarkable result which was later to be confirmed experimentally.

THE ENERGY OF A SINGLE FLUX LINE

Integrating Eq. 6.21 immediately gives 2 b + λ ∇ × ∇ × b dσ = 0 × δ2 (r) dσ = 0

149

(6.22)

where dσ is a surface element, and we integrate over the plane perpendicular to the flux line. The last relation is obtained since 0 and dσ are parallel, and by the properties of the 2D delta-function. Next we carry out λ2 [∇ × (∇ × b)]dσ = λ2 (∇ × b)dl = λ2 µ0 J dl ≈ 0 (6.23) r=R

r=R

The last form approximates zero because we take the line integral at such large distance, R λ, that the current associated with the flux line vanishes. From Eq. 6.22 we are now left with a relation which determines the total flux associated with a single flux line: (6.24) bdσ = 0 We have proved that 0 is the flux associated with the local field b of a single flux line when ξ can be regarded as vanishingly small compared to λ. This corresponds to insisting that δ |ψ| = 0, which is the overall approximation made in the present chapter. We can now go back to solving (6.22) for the region ξ < r λ. We first rewrite it approximately as 2 bdσ + λ (∇ × b)dl = 0 (6.25) ξ ξ . This corresponds to a cut-off k⊥ < 1/ξ . The integration over kx and ky is simplified by transforming to polar coordinates. 2 1 F = 0 Lz 2µ0 2π

1 ξ

dk

0

2 1 = 0 2µ0 (2π )2

0

2π k 1 + λ2 k 2

λ2 ξ2

du 2π k 2λ2 k 1 + u

where

u = λ2 k 2

(6.99)

162

LONDON APPROXIMATION TO G–L THEORY

The final result is 20 F = ln κ Lz 4π µ0 λ2

κ=

λ ξ

(6.100)

The problem is now solved for the free energy per length of a straight flux line in the London approximation for the isotropic case.

6.5

Interaction between two parallel flux lines

We discuss next a simple application of the expression for the interaction energy between flux lines, specified to two parallel, straight flux lines along the z-axis, with flux line no 1 at r 1 = (x1 , y1, z1 ), and no 2 at r 2 = (x2 , y2 , z2 ), as shown in Figure 6.7. This is an important example, as it can be viewed as the beginning stage of studying the forces at work in the flux line lattice. We already derived the general energy expression we have to start from; which we now specify for two parallel flux lines: 2 U12 = 0 (6.101) dr 1 dr 2 V (r 1 − r 2 ) µ0 d3 k ei k (r 1 −r 2 ) (6.102) V (r 1 − r 2 ) = (2π )3 1 + λ2 k 2 V (r 1 − r 2 ) is the potential energy between two arbitrary line elements dr 1 and dr 2 , and is valid whatever configuration the two flux lines assume. Carrying out the integral (Eq. 6.102) gives V (r 1 − r 2 ) =

1 e−|r 1 −r 2 |/λ 1 e−r/λ = 2π λ2 r 2π λ2 |r 1 − r 2 |

(6.103)

FL2 FL1 dr2 r2 z (r2 − r1) r1

dr1

x

y

Figure 6.7 Coordinates used in calculating the interaction energy between two parallel, straight flux lines.

INTERACTION BETWEEN TWO PARALLEL FLUX LINES

163

This is essentially the well-known Yukawa potential. Since the vortices are ˆ dr 2 = dz2 kˆ where kˆ is a unit vector parallel to the z-axis, we have dr 1 = dz1 k; along the positive z-axis. We introduce for the distance |r 1 − r 2 | : 1 2 |r 1 − r 2 | = (x1 − x2 )2 + (y1 − y2 )2 + (z1 − z2 )2 1 1 2 2 2 = ρ 2 + (z1 − z2 )2 ≡ ρ 2 + z2

(6.104)

where z2 = z2 − z1 , and ρ 2 = (x1 + x2 )2 + (y1 − y2 )2 . Inserting this expression into the integrand of Eq. 6.101 results in

U12

2 = 0 µ0

∞ −∞

20 = 2π µ0 λ2

dz1

1 2 2

1 e−(ρ +z2 ) /λ dz2 × 2π λ2 (ρ 2 + z 2 ) −∞ ∞

2

2

∞

−∞

dz1

∞

−∞

dz2

1 −(ρ 2 +z 2 ) 2 /λ

e

(ρ 2 + z2 2 )

(6.105)

The integral over dz1 gives the length of vortex line no 1. We divide it over to the left-hand side and get the energy pr unit length U12 . The integral over z2 gives U12 =

ρ 20 K 0 λ 2π µ0 λ2

(6.106)

where ρ is the distance between the flux lines in the (x,y) plane, and K0 ( ρλ ) is a modified Bessel function. We find that the result can be written as the product of the flux 0 times the field h(ρ) at distance ρ. U12 = 0 h(ρ);

h(ρ) =

1 b(ρ) µ0

(6.107)

The total energy of two interacting, parallel flux lines is therefore: tot U12 = 2F + 0 h(ρ)

(6.108)

We can now find the force between the two filaments in the x-direction: f2,x = −

∂U12 ∂(2F ) ∂h(ρ) − = −0 ∂x2 ∂x2 ∂ρ

(6.109)

164

LONDON APPROXIMATION TO G–L THEORY

The interaction force is repulsive. If we introduce the current jy , by Maxwell‘s ∂ h, where jˆ is the unit vector along y, we find equation; j y = −jˆ ∂ρ f2,x = jy 0

(6.110)

We notice in particular that the force in the x-direction on a flux line is zero only when the superfluid current (and velocity) at that point is jˆy = 0. This corresponds well with the Lorentz force on a charge e, F = ev × B. The whole situation of two interacting vortices can be easily illustrated by letting the currents and fields of the two overlap. One finds repulsive interaction when the vortices are parallel, and attractive when they are anti-parallel as is also implied by the mathematical analysis. Interestingly, when two flux lines of opposite rotation are made to coincide, they annihilate, since the sum of all currents must everywhere be zero. Clearly, the situation of anti-parallel flux lines is an extremely unstable one. See also Chapter 8, Figure 8.1.

6.6

Interaction between two flux lines at angle α

In high-Tc materials the consensus is that a flux line liquid exists above a certain flux line lattice (FLL) melting temperature Tm . A situation, which has been predicted to exist between Tm and Tc (H ) is that of an entangled flux line fluid. The behaviour of this fluid will be quite dependent on whether the flux lines are stuck in their entanglement, or are able to disentangle and straighten out. The answer to this question should be sought in the flux-line–flux-line interaction energy. In the case of parallel flux lines there is distinct repulsion, as we have seen in Section 6.5. But in a liquid state we can envisage flux lines which are softly bending and interwoven between each other, as shown in Figure 6.8. The flux lines at positions of closest spatial approach interact at some angle α, which is different from one place to another. One interesting question which arises here

Figure 6.8 Flux lines in a rigid Abrikosov vortex lattice (left), and a putative entangled flux-line system in the molten phase (right).

INTERACTION BETWEEN TWO FLUX LINES AT ANGLE α FL1

165

FL2 z

d y

x

a

Figure 6.9 Coordinates for calculation of interaction between two flux lines at an angle α. Both flux lines are located in the (y, z)-plane, one displaced a distance d along the x-axis from the other. Hence the distance of closest approach is d. The angle they are splayed is denoted by α, in the present case the splaying is symmetric around the z-axis.

is the following: What is the energy cost of moving two nearly intersecting flux lines across each other to disentangle? This situation may be closely modeled by letting two flux lines be placed at a crossing angle α, like in Figure 6.9. To calculate the interaction energy we can again revert to the general formalism employed before. The difference between this case and the one treated in Section 6.5, is that the interacting line elements are at an angle α, and at a distance d, which means that the line elements dr 1 and dr 2 are at such angle, wherever their location is on line 1 and line 2. The integral to work out is now: dr 1 dr 2 V (r 1 − r 2 ) (6.111) U1,2 (α) = F L1

F L2

The integration over the variables in parallel position was carried out in Section 6.5. Taking advantage of that integration result, and inserting the cos α for the vector product of dr 1 × dr 2 , where |dr 2 | = dy/ sin α, and after dividing by the length of line 1 on both sides, we get 20 U1,2 (α, d) = 8π 2 λ2

∞

−∞

dy cos αK0 sin α

1

(d 2 + y 2 ) 2 λ

(6.112)

where K0 is again the same Bessel function encountered in Section 6.5. We find U1,2 (α, d) =

20 cot αe−|d|/λ 8π λ2

(6.113)

In fact, if we consider the fact that the systems also may be uniaxially anisotropic, then we may parametrize this in the London model by introducing two penetration

166

LONDON APPROXIMATION TO G–L THEORY

lengths, namely λab which is the penetration length in the (a, b)-plane ((x, y)plane) for a magnetic field oriented along the c-axis (z-axis), and λc which is the penetration length along the (a, b)-plane for a screening current along the c-axis. Eq. 6.112 then generalizes to U1,2 (α, d) =

20 −|d|/λab −|d|/λc − tan(α/2)e cot(α/2)e 4π λ2

(6.114)

as was shown by Sudbø and Brandt [77]. This is seen to reduce to Eq. 6.113 when λab = λc . Note how the angle at which flux lines do not interact (electromagnetically) in fact increases when the anisotropy ratio λc /λab increases. For the isotropic case, the interaction changes sign at α = π/2. When λc /λab → ∞, the interaction never changes sign, but approaches zero as α → π . The neutrality angle where the electromagnetic interaction between two rigid flux lines vanishes therefore increases with anisotropy.

6.7 General flux-line lattice elastic matrix in the London approximation As a final application of Eqs 6.83 and 6.91, let us use them to derive an expression for the general elastic fluctuation matrix of a flux-line lattice in an arbitrarily tilted external magnetic field, valid beyond the continuum approximation for the flux-line system. This means that we explicitly take into account the underlying Abrikosov lattice structure when deriving the fluctuation Hamiltonian for flux lines around their ground state configuration. The continuum approximation is a special case of the result we will derive, and as a byproduct we will obtain expression for the flux-line liquid elastic moduli in this limit when the external magnetic field is tilted an arbitrary angle with respect to the crystal c-axis. ˆ The exposition here closely follows that of Sardella [78] and Nguyen and Sudbø [76]. The starting point is Eq. 6.83 20 F = dr αi dr βj Vαβ (r i − r j ) 2µ0

(6.115)

ij

We now rewrite this by being slightly more explicit in writing the line integrals that are involved. The line integrals are along directed flux lines, the average direction of the flux lines is the z-axis, and hence we have dr αi = dz(dr αi /dz). We now insert this into Eq. 6.115 and obtain 20 drβj drαi F = Vαβ (r i (z) − r j (z )) dz dz 2µ0 dz dz ij

(6.116)

GENERAL FLUX-LINE LATTICE ELASTIC MATRIX

167

where the information on the shape of the flux lines is encoded in drβj /dz. We now imagine that the ground state of this system is the Abrikosov fluxline lattice, and expand the free energy in fluctuations around this ground state, keeping terms up to quadratic order in the displacements sj (z) around the ground state, where we have ri (z) = Rj + sj (z)

(6.117)

where Rj denotes the positions of flux lines in the ground state Abrikosov vortex lattice, and sj (z) denotes the fluctuations around these positions. The first thing to notice is that drβj (z)/dz = 1 if β = z, and drβj (z)/dz = dsj (z)/dz if β = (x, y). Let us now expand the tensor Vαβ (ri (z) − rj (z )) up to quadratic order in the displacements sj (z), obtaining Vαβ (ri (z) − rj (z )) = Vαβ (Ri − Rj ) + [si (z) − sj (z )]∇Vαβ (r)r=Ri −Rj 1 + [si (z) − sj (z )]n [si (z) − sj (z )]m 2 × ∇n ∇m Vαβ (r)r=Ri −Rj + . . .

(6.118)

Inserting this back into the expression for the energy, Eq. 6.116, we obtain, upon collecting terms up to quadratic order and noticing that terms that are linear by necessity must vanish since we are expanding around a minimum, we have for the elastic energy F = F − F0 , where F0 is the total energy of the ground state Abrikosov flux-line lattice (NB We must keep terms that are linear in displacements when expanding the tensor Vαβ (ri (z) − rj (z ))!) 20 dsαi dsβj F = Vαβ (Ri − R) dz dz 2µ0 dz dz ij

1 + [si (z) − sj (z )]n [si (z) − sj (z )]m ∇n ∇m Vαβ (r)r=Ri −Rj 2 dsαi [si (z) − sj (z )]β ∇β Vzα (r)r=Ri −Rj +2 (6.119) dz where (α, β) ∈ (x, y). The next step is to express this in terms of the Fouriermodes of the displacement vectors si (z). Now, because we are assuming an underlying Abrikosov lattice which gives rise to a Brillouin zone, the wavevectors of the displacement vectors are only defined up to an arbitrary reciprocal lattice vector Q. Hence, when we Fourier-expand the displacement vectors sj (z), we express the Fourier transform through a sum over reciprocal lattice vectors

168

LONDON APPROXIMATION TO G–L THEORY

Q of the Abrikosov vortex lattice and an integral over the wavevector k that runs over the first Brillouin zone. This means that we can write F =

1 sα (−k)αβ (k)sβ (k) 2

(6.120)

k

which defines the elastic matrix αβ (k). In the above expression, k runs over the first Brillouin zone. Such an expression is arrived at by partial integrations in Eq. 6.119, and then introducing the Fourier transforms of sj (z) as follows si (z) =

d3 k sβ (k) eikRi (2π )3

(6.121)

Moreover, because of the underlying Abrikosov flux-line lattice we must take into account that the wavevectors k are only defined up to reciprocal lattice vectors of the Abrikosov lattice, whence

eikRi = (2π )2

B δ2 (k − Q)eikz z 0

(6.122)

Q

i

where δ2 (k − Q) is a two-dimensional Dirac δ-function. Inserting all of this into Eq. 6.119, we find Eq. 6.120 with αβ (k) =

B2 fαβ (K) − fαβ (Q) 2µ0

(6.123)

Q

where we have introduced the function fαβ (k) = kz2 V˜αβ (k) + kα kβ V˜zz (k) − kz kβ V˜zα (k) − kz kα V˜zβ (k) (6.124) and where V˜αβ (k) is the Fourier transform of Eq. 6.91, namely V˜αβ (k) =

2 qα qβ 1 δαβ − 1 + 1 k 2 1 + 1 k 2 + 2 q 2

(6.125)

In Eq. 6.123, we introduced K = Q + k and moreover symmetrized the tensor fαβ (k). From Eq. 6.119, as it stands, we would have obtained fαβ (k) = kz2 V˜αβ (k) + kα kβ V˜zz (k) − 2kz kβ V˜zα (k)

(6.126)

However, for numerical purposes, when computing elastic modes of the flux-line lattice, it is often convenient to use the symmetrized form since it guarantees positive definite eigenvalues of the elastic matrix. The expression Eq. 6.123 is very useful, among other things it directly lends itself to a computation of the

GENERAL FLUX-LINE LATTICE ELASTIC MATRIX

169

elastic shear moduli of the Abrikosov flux-line lattice, of which there are several when the magnetic field is tilted away from the c-axis. ˆ The continuum limit of the elastic description of the Abrikosov flux-line lattice is obtained by omitting all terms in the sum over Q except Q = 0. Since the underlying lattice is not taken into account, this is basically an elastic description of a flux-line liquid, so the shear moduli are not accessible in this approximation. The bulk and tilt moduli are, however. Let us see how we can extract them from what we have derived above. In the flux-line liquid limit, taking only the Q = 0 terms and using that fαβ (k = 0) = 0, from Eqs 6.120 and 6.123 we simply have the elastic free energy given by F =

B2 sα (−k)fαβ (k)sβ (k) 2µ0

(6.127)

k

When the external magnetic field is tilted away from the c-axis ˆ by an angle θ we have four distinct elastic moduli of the flux-line liquid, such that the elastic description on symmetry grounds is given by the expression F =

1 ⊥ (k)(kz sx )2 + c44 (k)(kz sy )2 c11 (k)(ks)2 + c44 2 k +2c14 (k)(kz sx )(ks)

(6.128)

The elastic moduli that enter her can be obtained by comparing Eq. 6.128 with Eq. 6.127, and they are found to be given by Refs [73, 76, 78] ⊥ c44 (k) =

1 + [λ2ab + (λ2c − λ2ab ) sin2 θ ]k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

c44 (k) =

B2 1 2 2 4µ0 1 + λab k + (λ2c − λ2ab )q 2

c11 (k) =

1 + [λ2ab + (λ2c − λ2ab ) cos2 θ ]k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

c14 (k) =

(λ2c − λ2ab ) sin θ cos θ k 2 B2 4µ0 [1 + λ2ab k 2 ][1 + λ2ab k 2 + (λ2c − λ2ab )q 2 ]

(6.129)

⊥ (k) and c (k) are known as tilting moduli. Here, the set of moduli given by c44 44 When the flux lines on average are directed away from the symmetry c-axis, ˆ there appear two tilting moduli in the problem. The reason is that when the system is layered and the z-axis is tilted an angle θ away from the c-axis, ˆ we have a hard and a soft tilting mode depending on whether the tilting away from the z-axis is parallel to the crystal ab-plane, or out of the crystal ab-plane.

170

LONDON APPROXIMATION TO G–L THEORY

(Similar effects are present in the shear moduli of the flux-line lattice, which do not concern us here since we are considering the flux-line limit). Notice that for ⊥ (k) = c (k). The third of the four elastic moduli c (k) is θ = 0, we have c44 11 44 the bulk modulus, or compressional modulus, of the flux line liquid. The fourth of the elastic moduli, namely c14 (k) does not have a counterpart in an isotropic superconductor, nor in an anisotropic superconductor when the magnetic field is parallel to the c-axis. ˆ The new elastic modulus appearing is a mixed tiltand bulk-modulus, suggesting that in a tilted magnetic field, the elastic tilting and compressional modes of the flux-line liquid interact with each other. These mixed elastic moduli vanish in the limit when k → 0. (For the shear moduli, we have a similar situation. We get a hard and a soft shear mode, as well as a mixed shear-tilt mode). Note how all of the other elastic moduli, bulk as well as tilting moduli, take the value B 2 /µ0 when k = 0. Mass anisotropy is not seen at all in this socalled local limit. Moreover, the elastic properties of the flux-line liquid are oblivious to the value of λ (or κ) in the local limit. At finite k-vectors, the flux-line liquid softens considerably as the degree to which a superconductor is type II, increases. But the effect of mass anisotropy and the hardness of the superconductor (degree of type II) only influence the elastic properties of the flux-line lattice provided a non-local elastic theory is used. We shall come back to this point in Chapter 8, when we consider the Lindemann criterion for melting of the flux-line lattice.

7 Applications of Ginzburg–Landau Theory (|ψ| spatially varying) 7.1 The temperature-dependent order parameter |ψ(T )| As a first application of the Ginzburg–Landau (GL)-equations we derive the temperature dependence of the order parameter ψ. This can be done under the simplest possible conditions, with B = 0, and under homogeneous conditions ∇ψ = 0. The free energy now reduces to F (T ) = F0 (T ) + α |ψ|2 +

β |ψ|4 + · · · 2

(7.1)

Taking the derivative leads to the equilibrium condition δF = 0 ⇒ (α + β |ψ|2 ) |ψ| = 0 δ |ψ|

(7.2)

One solution is that |ψ| = 0, which is correct for the superconducting wavefunction above Tc . The other alternative is α + β|ψ|2 = 0. This gives α |ψ|2 = − (7.3) β Since α = α1 (T − Tc ) where α1 is a constant ,we find to a useful approximation, like in the magnetic case |ψ|2 =

α1 (Tc − T ) β

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

172

APPLICATIONS OF GL-THEORY 1 2

|Ψ|

|Ψ| ~ (Tc − T )

|Ψ| = 0

Tc

T

Figure 7.1 Temperature dependence of the order parameter |ψ|.

or |ψ| =

α1 β

1 2

1

(Tc − T ) 2

(7.4)

as sketched in Figure 7.1. Since the interpretation of |ψ|2 is that it represents the superfluid density ns , we have ns ∝ (Tc − T )

(7.5)

Some important remarks on the limitation of GL-theory are in order here. The last two results are both typical mean-field-like, a consequence of the tacit assumption of the GL-approach that fluctuations of ψ are to be neglected. In real cases, the temperature exponent 1/2 is good in the low-Tc materials, but not expected to hold in high-Tc materials. The difference comes from the properties we discussed in Section 2.6, that the coherence length is quite long in lowTc and quite short in high-Tc materials, making fluctuations important in the latter case. According to the results above, the superfluid density ns – corresponding to the density of Cooper-pairs – vanishes at Tc . Again, this mean-field like prediction is correct for long ξ , low Tc materials. In these the Cooper-pairs do start to condense at Tc , and the superfluid density ns and wavefunction ψ build up as the temperature is lowered below Tc . The lower the temperature, the more Cooper-pairs are created. However, again the situation does not prevail in high-Tc materials. It turns out that in those materials the wavefunction amplitude |ψ| is not zero above Tc . We return to these profound problems in Chapter 10.

7.2

The coherence length ξ

The coherence length ξ is a temperature-dependent as well as a materialdependent quantity. We will now demonstrate how it may be derived from

THE COHERENCE LENGTH ξ

173

the GL-theory, even without a magnetic field present. In this case the GL-I equation immediately becomes α(T )ψ + β |ψ|2 ψ +

1 (−i∇)2 ψ = 0. 2m

(7.6)

This is a differential equation for spatial variations of the order parameter. In geometries where 1D calculation may be used for simplicity, it reads −

2 d2 ψ + α(T )ψ + β |ψ|2 ψ = 0. 2m dx 2

(7.7)

On dividing through by the parameter α we observe that an operator defined 2 d2 in the first term of Eq. 7.7 must be dimensionless. Therefore, the as 2mα dx 2 quantity ξ defined by ξ≡

2 2mα(T )

12 (7.8)

must have the dimension of a length. Such a finding is significant, and suggests that this is to be understood as a characteristic length of the system. Indeed, this is the temperature-dependent GL coherence length ξ . Its temperature dependence is predicted to have the classical exponent ν = 1/2, according to 1 (T /Tc − 1)− 2 ; T > Tc (7.9) ξ(T ) = ξ0 1 (1 − T /Tc )− 2 ; T < Tc 1

where the length ξ0 is /(2mα1 Tc ) 2 . The length ξ(T ) is of fundamental importance in superconductivity, representing the coherence length of the wavefunction. We may regard this as the shortest distance over which the wavefunction is allowed to vary without generating pair breaking kinetic energy. We notice in particular the important aspect that ξ(T ) diverges towards Tc , from below as well as from above. This means that when the wavefunction is perturbed by for instance a magnetic field, or by normal inclusions in the superconductor, the length ξ(T ) is the healing length over which ψ recovers its full value. Clearly, this situation also exists when flux lines or vortices penetrate a type II superconductor, where, as we know, ψ → 0 at the centre. ξ(T ) is then the effective radius within which the Cooper-pair density is suppressed, a fact which allows the calculation of the energy cost of breaking the Cooper-pairs in a radius ξ around the vortex centre. A similar role is played by ξ(T ) at a superconducting to normal interface in the laminar structure of type I superconductors. Here ξ defines the wall thickness, quite analogous to domain walls in systems like ferromagnets, ferroelectrics, etc. All results of the GL-theory are purely phenomenological. The coefficients of the energy expansion, α1 ,β and c are unknown. However, they can be determined

174

APPLICATIONS OF GL-THEORY

by relating them to measurable quantities, like ξ , λ and Hc . The consistency of data taken by independent methods may then be checked, with the prospect of asserting the overall picture, as well as imposing a quantitative control on the expressed relations between experimentally determined quantities. The penetration depth λ is the other length parameter of particular importance in superconductivity. How can it be expressed by use of the GL-equations? Since λ is a measure of the depth of supercurrent response to a magnetic field, this suggests looking at the second GL-equation. In situations where the Cooper-pair density remains unperturbed, like when a magnetic field penetrates to depth λ in the Meissner state, we can simply neglect the gradient of ψ in GL-II. What remains is J =

e ∗ ψ (−2eA)ψ + c.c. m

=−

4e2 |ψ|2 A m

(7.10) (7.11)

From the London equation we have J = −(1/µ0 λ2 )A. This gives the relation 4e2 |ψ|2 = µ 1λ2 . Here we must have |ψ|2 = ns for consistency of these indepenm 0 dent derivations. The result clearly is in accord with the BCS-picture since it leads to the conclusion that λ2 =

m (2e)2 µ0 |ψ|2

(7.12)

This offers a somewhat more precise definition of the length λ, where 2e corresponds to the magnitude of the charge of a Cooper-pair, and m is the corresponding mass. By now we have obtained results for ξ and λ, and can also express the quantity κ = λ/ξ , which is of fundamental importance in superconductivity.

7.2.1

Relations between λ, ξ and Hc

So far we have used the GL free energy expansion and the GL-equations to gain insight into the characteristic lengths of the superconductor. Next, we look for relations between these and the important thermodynamic quantity Hc . We consider again a homogeneous superconductor in the absence of a magnetic field. The free energy is Fs (T ) = Fn (T ) + α |ψ|2 +

β |ψ|4 + · · · 2

(7.13)

TWO TYPES OF SUPERCONDUCTORS

175

Using |ψ|2 = − βα we find Fs (T ) = Fn (T ) −

α2 2β

(7.14)

This must agree with the difference in Gibbs’s energy between the normal and superconducting states derived in Chapter 1, hence µ0 2 α2 = H 2β 2 c

(7.15)

We can also find expressions for α and β from the preceding relations. Using µ0 Hc2 = −α |ψ|2 ;

α |ψ|2 = − ; β

and

−4e2 µ20 Hc2 1 = αm λ2

(7.16)

we find −4e2 µ20 Hc2 λ2 m

(7.17)

(4e2 )2 µ30 Hc2 λ4 α2 = µ0 Hc2 m2

(7.18)

α= and β=

By combining the equations containing Hc , ξ and λ we obtain the interesting result that Hc λξ =

0 √ 2π 2µ0

(7.19)

Since the right-hand side is a constant, we see that on varying the temperature, the three quantities Hc , λ and ξ are predicted to vary in such a way that their product remains fixed. Equally interesting and useful is the combination λ(T )ξ(T ) =

7.3

0 2π 2µ0 Hc (T ) √

(7.20)

Two types of superconductors

In complete analogy with Ohm’s law, J = σ E, which we pointed out is formally equivalent to the London equation, Pippard [69] adopted the corresponding

176

APPLICATIONS OF GL-THEORY

non-local version of Ohm’s law from Reuther and Sondheimer [79] for the so-called anomalous skin-effect, 3σ J = 4π l

r(r · E)e−r/ l 3 d r r4

(7.21)

Non-locality enters the problem when the response to a field can only be determined correctly by integrating over a volume of the size of l 3 (3D case), where l is comparable to or longer than the distance δ, the depth over which the E-field varies. Consequently, in the London equation ξ would have to be introduced whenever the coherence length ξ is greater than λ, since λ is the penetration distance of B whose vector potential drives the current. From experience in studies of the anomalous skin-effect in pure, normal metals Pippard saw the analogy for the superconductor in the simplest case to be J =−

ξ(l) A ξ0

(7.22)

where ξ0 is the value of ξ(l) in the limit of large l, i.e. for the pure case, and = (µ0 λ2L )−1 . Clearly, this equation predicts a reduced response when ξ(l) is reduced by impurities. Because experimentally λ is found to increase with decreasing l, ξ(l) must decrease as l decreases, as can be seen from Eq. 7.20. Eq. 7.22 can be viewed as one which applies when ξ λ, which we may call the London limit. It is also a limiting form of the general Pippard non-local relation, which he constructed on the basis of the combined insight from Eq. 7.22 and the Reuther–Sondheimer integral. The whole chain of arguments led Pippard to propose for superconductors, in complete analogy with the non-local response to an electric field in a normal metal 3 r(r · A)e−r/ξ 3 J =− d r (7.23) 4π ξ0 r4 where ξ(l)−1 = ξ0−1 + l −1 . Limiting cases which can be worked out are: λ = (ξ0 /ξ )λL √ 1 3 3 λ= ξ0 λ2L 2π

for

ξ λ

(London limit)

for

ξ λ

(Pippard limit)

where we used the symbol λL for the original London value of λ. These expressions have been verified experimentally. It is remarkable that the microscopic BCS theory [7] later confirmed the essential correctness of Pippard’s bold adaptation of non-local electrodynamics

TWO TYPES OF SUPERCONDUCTORS

177

from normal metals to superconductors. The BCS theory also gave an expression for the ξ0 -parameter: ξ0 = 0.18vF /kTc , where vF is the Fermi velocity, and k = 1.38 × 10−23 J /K is Boltzmann’s constant. Essentially the same answer is obtained using the uncertainty principle. In that case the idea is to relate the coherence length to the energy gap. The introduction of the coherence length lead to the extremely important distinction between two types of superconductors, i.e. those with ξ > λ versus those with ξ < λ, called type I and type II superconductors, respectively. A precise expression for this distinction is derived later in this chapter. At this point a semiquantitative, less stringent argument, proves the main point (see Figure 7.2). In both the parts of Figure 7.2 we are faced with a situation where a change takes place between a point at the origin, r = 0, where the normal state with B = Bc ends, followed by a region where superconductivity recovers over a distance ξ , while screening extends over the distance λ. We refer first to the left figure, where the situation is sketched from the NS-interface into the superconducting region. Here B(r) falls off from r = 0 according to B(r) = Bc e−r/λ . Next, the superconducting wavefunction is suppressed over a much wider range, i.e. over the coherence length ξ . The energy argument now goes as follows: To expel the magnetic field from the volume of the superconductor costs the energy 2µ1 0 Bc2 per volume. However, a volume equal to the product Aλ of laminar interface area A and penetration depth λ, is not screened against Ba , amounting to a total energy E1 = λA

1 2 B 2µ0 c

(7.24)

saved in setting up the laminar structure, compared to what it would cost to have a totally sharp boundary between normal and superconducting volumes, i.e. if λ = 0. On the other hand, the density of Cooper-pairs ns is suppressed since the proximity to the normal interface forces the superconducting wave-function ψ Type I

Type II B (r)

B (r)

l

NS interface

|y(r)|2

|y (r)|2

x

l x

Vortex center

Figure 7.2 Variations of magnetic field B and wavefunction ψ at the normal-superconducting interface.

178

APPLICATIONS OF GL-THEORY

to go to zero at the normal boundary where B = Bc . The distance over which ψ is suppressed from full equilibrium value ψ0 to zero, is precisely the length ξ that we introduced in Eq. 7.8. In the volume defined by the total laminar wall area times ξ , superconductivity is essentially destroyed. This costs an amount of energy corresponding to breaking the majority of Cooper-pairs in this volume, E2 = ξ A

1 2 B . 2µ0 c

(7.25)

So the net energy E gained by setting up the laminar walls is given by the difference E = E1 − E2 . For the situation to be stable E must be positive:

E = ξ A

1 2 1 1 2 Bc − λA Bc = ABc2 (ξ − λ) > 0 2µ0 2µ0 2µ0

(7.26)

We can regard this condition as the defining one for type I superconductivity, and note that it corresponds to the√simple statement that ξ > λ, not very different from the exact condition: κ < 1/ 2 to be shown later. The fact that the interface energy is positive in type I, makes the system want to establish as small an interface area as possible. It does so by setting up the laminar structure shown in Figure 7.3. We note from the picture that the lamina are not flat, but show a meandering structure as long as the field is directed normal to the flat sample surface. Experiments have shown that the laminar structure can be straightened out and stabilized by a magnetic field tilted in the plane of the laminar direction [80, 81], as sketched in Figure 7.4. With a flat geometry and a tilted field, as shown in Figure 7.4, the laminar structure acquires a thickness period where normal lamina thickness dn and superconducting lamina thickness ds add up to a total thickness d = ds + dn . In the normal lamina B is everywhere Bc , and in the superconducting lamina we take B = 0. Furthermore, if we assume that the lamina extend across a length L of a plate-like rectangular slab structure, there is a simple flux-conserving relationship between the laminar geometry, the thermodynamic field Bc and the applied field Ba . Conservation of total flux a applied to the specimen requires that a = Ba Ld = 0 × Lds + Bc Ldn ⇒ dn =

Ba a = d Bc L Bc

(7.27)

Here we have disregarded the small tilt of B a with respect to the surface normal. Since dn + ds = d we find also Ba Ba d + ds = d ⇒ ds = 1 − d (7.28) Bc Bc

TWO TYPES OF SUPERCONDUCTORS

179

Figure 7.3 Meandering laminar structure with alternating normal and superconducting regions, typical for type I superconductors with the magnetic field applied normal to a flat slab. From [82]. Reproduced with permission of the Royal Society.

Ba

dn

ds

d

L

Figure 7.4 Sketch of laminar structure in type I superconductor, straightened by tilting the applied magnetic field Ba [80].

180

APPLICATIONS OF GL-THEORY

This shows how the laminar thicknesses dn and ds vary with applied field and temperature through the dependences of ds and dn on Ba and Bc (T ). This result applies as long as the total d is a constant. Original work in this area was done by Landau [83, 84]. Next we discuss the second alternative, κ > 1. The energy argument we used before, pertaining to the interface energy, applies again, but due to the condition ξ < λ the energy E required to create the interface is now negative: 1 2 B A(ξ − λ) < 0 2µ0 c

(7.29)

√ So, to within a factor 1/ 2 as before, λ > ξ is the condition for type II superconductivity. Therefore now, the larger the interface area can be made, the more energy is gained. Can this go on without limit? Clearly no, because, as we have seen, flux is quantized in elementary units 0 = h/2e. This is how far the division of flux can and will go. These flux quanta are established by circulating superfluid currents, vortices of Cooper-pair flow that will go on forever once created, provided the temperature is held below Tc . Because of the smallness of the flux quantum, there will be a huge number of these in a finite field. A field of 1 T in a sample with 1 cm2 cross-section will cause the sample to be penetrated by more than 1011 vortices! We shall later study the physics of these in greater detail. As a consequence of ∇B = 0 we can immediately conclude that any such quantized vortex, once created, must extend continuously all the way through a homogeneous superconductor or form closed loops. The physics of vortices constitutes the central issue in the science of superconductivity in type II superconductors. We return to this subject in several later chapters of this book.

7.4 The structure of the vortex core In Chapter 6 we derived, as a byproduct of finding the line energy, the radial dependence of the local field from a vortex: 0 λ b= + b0 ln (7.30) r 2π λ2 This was obtained as an approximation when integrating curl b × dl for ξ < r λ. The rigorous result is r 0 b(r) = (7.31) K 0 λ 2π λ2 where K0 ( λr ) is a zero’th order Bessel function [72]. This form flattens the dependence on r within a radius ξ , the ‘hard core’. For convenience we repeat

181

THE STRUCTURE OF THE VORTEX CORE

the limiting forms: 0 λ b(r) = ln ; rλ 2 r 2π λ 1 0 π λ 2 −r/λ b(r) = e ; r λ 2 2r 2π λ

(7.32)

(7.33)

The structure of the vortex, therefore, is an inner volume of radius ξ where the field locally is high enough to destroy superconductivity by breaking most of the Cooper-pairs, i.e. ns approaches zero. This means also that the wavefunction ψ must likewise approach zero. It is equal to zero only at the centre. How can we prove that ns is so suppressed? Physically the upper critical field where the superconductor crosses over to the normal state, can be estimated by Bc2 ≈

0 πξ2

(7.34)

This implies that superconductivity is destroyed when the cores start to overlap. The reason why this leads to a normal state, is that at Bc2 cores with ns ≈ 0, overlap. This argument is also bears on ψ, since |ψ|2 = ns . Figure 7.5 shows a sketch of a cut through the vortices, represented by ns and b(x). Figure 7.6 b (x) ns = |y|2

x

Figure 7.5

Cut through the centre of neighbouring vortices, showing b(x) and |ψ|2 (x).

|y|2

Bc1 < B Bc . κ >

√1 2

2 . 2mξ 2

(7.42) √1 2

we have

is the exact condition for the appearance of a vortex phase

in type II superconductors. When κ < √1 we get Bc2 < Bc . In that case, as we 2 lower the field from above, we meet the Bc field before Bc2 . Here the Meissner effect sets in, and the mixed phase will not appear. We have type I behaviour. The importance of the value of κ = λ/ξ is apparent. We have two types of superconductors: κ

Bc when n = 0.

κ>

√1 : 2

type II with vortex state at Bc1 < B < Bc2

The laminar structure of field penetration in type I is amply documented. It occurs when an inhomogeneous field surrounds a sample with demagnetization factor n = 0. The field may then exceed Bc in some areas, and some flux is allowed to penetrate the sample in order to lower the total energy. On penetration, the laminar structure appears as the device by which the sample avoids being exposed to a field B > Bc anywhere. At this point it may be interesting to ask for an exact expression for Bc1 too. A rigorous argument, which avoids use of thermodynamics, and only relies on geometric consideration, disregarding any finite core effects, is the following. Bc1 is defined as the field at which the first vortex enters the

184

APPLICATIONS OF GL-THEORY

superconductor. That being so, let one flux quantum be in the superconductor at the field Bc1 . Let us for this purpose work in the London approximation where the normal core radius is set equal to zero. The flux quantum 0 is now allowed to occupy the whole specimen, the field being distributed according to the function e−r/λ . The critical field Bc1 at which one flux quantum has entered can then be computed by weighting each area dA = 2π r dr by the distribution function e−r/λ . The field is the total flux divided by effective area as follows: Bc1 =

∞

0 − λr

e

2π r dr

=

0 2π λ2

(7.43)

0

which is the exact answer in the London approximation with |ψ| constant.

7.5.2

Bc2 , ξ , and λ in anisotropic superconductors

So far we have discussed superconductivity in isotropic systems. However, for layered, highly anisotropic high-Tc compounds there is a need to develop methods to treat such cases. This is achieved by the Lawrence–Doniach (LD) theory [85, 86]. In a simple model picture, let us assume that the superconductor can be described by a state of alternating superconducting and insulating layers, of type SISISI, where S = superconductor and I = insulator, or SNSNSN, where N is a normal layer. In such systems, if the contact between S-layers is poor, the main charge transport between S-layers may take place by tunnelling, both for normal carriers and for Cooper-pairs. Among high-Tc materials the Bi-based compounds are good examples of such behaviour. In such a layered structure, let the x, y axes lie in the ab-plane, and the z-axis along the normal to the ab-plane. We will assume for simplicity that a- and b-axes are equivalent, corresponding to a tetragonal symmetry. In the high-Tc cuprates the orthorhombic structure is usually realized, but the distinction between a and b is far less significant than the difference between c and a, b. An immediate consequence is that the effective mass along a, b, called mab may be quite different than mc . In this situation the inverse mass appears as a tensor quantity in transport problems and in summing up energy terms. The free energy for a stack of superconducting planes with restricted contact between layers can be written down as

F =

n

1 d2 r α |ψn |2 + β |ψn |4 2 2 ∂ψn 2 ∂ψn 2 2 + + + ∂y 2mab ∂x 2mc

∂ψn 2 ∂z

(7.44)

THE LENGTH ξ AND THE UPPER CRITICAL FIELD Bc2

185

The summation is over all planes, and integration is in each plane, in two dimensions. The distinction between the ab- and c-directions is most manifest in the coherence length, which is often much shorter in the c-direction than in the ab-plane, even shorter than the S-S-plane distance s in high-Tc cuprates. Here one may choose to discretize the last derivative in extreme cases of layeredness. This term would take the form 2 |ψn − ψn−1 |2 2mc s 2

(7.45)

and by the summation, each layer n will be found to interact with one nearest neighbour on each side. On writing ψn = |ψn |eiϕn , and ψn−1 = |ψn |eiϕn−1 assuming identical layers, one finds by insertion in Eq. 7.44 that the energy for two adjacent planes is 2 |ψn |2 (1 − cos(ϕn − ϕn−1 )) mc s 2

(7.46)

This expression bears a striking resemblance to the Josephson coupling energy1 , as it ought to since the physics is the same when charge transport between layers takes place by tunnelling. On the other hand, in case we stick with the continuum version of derivation even along z, within some distance from Tc , due to the divergence of ξ(T ) we can instead use the continuum GL-equation found before, ↔−1 but with the modification that inverse mass is now a tensor expressed as m ; i = a, b, c. The only change from the isotropic case, is that we have to write the product of the kinetic operator and the inverse mass tensor in a new form. ↔−1 As the kinetic operator is squared, the way to write the product is to place m between the two operators. The GL-equation for the anisotropic, continuous case is called the LD-equation and now reads 2 αψ + β |ψ| ψ − 2 2

2e 2e ↔−1 ∇−i A · m · ∇−i A ψ =0

(7.47)

The inverse mass tensor has principal values: m1ab , m1ab , m1c . The anisotropy encountered here is extremely important in the high-Tc cuprates, and its consequences must be dealt with realistically in any serious approach. We immediately come upon this fundamental issue in the description of the coherence length, ξ . Clearly, we now have to write the relationship 1 The Josephson coupling energy expresses the energy stored in the junction, and can be determined by

up the electrical work which the current source does in changing the phase ϕ, i.e. by

integrating Is V dt = Is (/2e)d( ϕ).

186

APPLICATIONS OF GL-THEORY

between ξ and the parameter α in a new form, with corresponding labels i on ξ and m: 2 ξi2 = (7.48) 2mi α(T ) And since ξi is anisotropic, so is λi as expressed by 0 ξab λab = ξc λc = ξi λi = √ 2 2π Bc

(7.49)

Thermodynamic quantities like Bc , of course, should have no anisotropy label. The inverse relationship between ξi and λi is noteworthy. Remembering that the index i on ξi represents the direction of the corresponding axis and the direction of movement of the mass mi , the index i on λi takes a different meaning: It refers to supercurrent shielding by currents flowing in the plane normal to the i-th axis. The anisotropy was introduced above through the masses mi , and these are different by a factor of the order of 10 in high-Tc compounds. The lattice anisotropy has a direct influence on masses mi , and via the mass it propagates to all other directionally distinguishable quantities. One other notable consequence is in the critical fields, where we now have c

Bc2 =

0 2 2π ξab

;

ab

Bc2 =

0 2π ξab ξc

(7.50)

The reason why we have to divide by the product ξab ξc in the second case is that the currents defining the vortices and flux lines flow around the axis lying in the ab-plane and therefore flow both in the ab-plane and in the c-direction. c ab Since ξab ξc we get Bc2 < Bc2 . To summarize, the anisotropy factor γ can be written as 1 ab Bc2 ξab λc mc 2 = = = c (7.51) γ ≡ mab ξc λab B c2

An illustration of the definitions of the length parameters λ and ξ in anisotropic superconductors of the type discussed above is given in Figure 7.7. In Figure 7.8 we have illustrated how the vortices created in a layered superconductor are broken up into a stack of ‘pancakes’. When the field is tilted, the pancakes are connected by horizontal Josephson vortices, shown in the figure only as horizontal lines. An important distinction is the fact that pancakes have a normal core, while the Josephson vortices have no such core. To study Hc2 , or Bc2 in the strongly anisotropic case we return to the discretised version Eq. 7.45, but with appropriate terms included to allow a magnetic field through a vector potential A. We choose to let Az = Bx, where B is along the y-axis, in the ab-plane.

THE LENGTH ξ AND THE UPPER CRITICAL FIELD Bc2

187

z

lb xc y

xb

lc

Figure 7.7 Sketch of a vortex of elliptical cross section aligned parallel to the a axis in an anisotropic superconductor described by the anisotropic Ginzburg–Landau theory.

(a)

(b)

(c)

Figure 7.8 Stacks of 2D pancake vortices: (a) straight stack, the configuration of lowest energy at zero temperature, and (b) disordered stack, which occurs at higher temperatures. (c) Sketch of a tilted stack of pancake vortices in successive superconducting layers, connected by interlayer Josephson strings.

We will now express the contribution to the LD-equation in the n’th superconducting plane by the continuous model as 2 αψn + β |ψn | ψn − 2mab 2

2 2e ∇ − i A ψn

(7.52)

A contribution must be added here to include the effect of coupling to planes n − 1 and n + 1. Since ψn has neighbours ψn−1 and ψn+1 the phases relative to these with respect to the phase of ψn must be expressed explicitly. The three terms in the summation over three planes ψn+1 , ψn , ψn−1 must be modified to take account of the phase contribution from the vector potential A. The phase difference to look for is indicated by the second term in the operator (∇ − i 2e A). 2e Here i A is equivalent to the derivative of the phase difference, so it must be multiplied by the distances between planes to give the phase difference.

188

APPLICATIONS OF GL-THEORY

And finally, the difference between wave functions on the corresponding two neighbouring planes has to be divided by s 2 to give the discretized second derivative. Upon adding these terms to those written down before, recalling also the direction of the field we have chosen, we find αψn + β |ψn |2 ψn − −

2 ∇ 2 ψn 2mab x,y

2ieA s 2ieAz s 2 − z e − 2ψ − ψ e ψ =0 n+1 n n−1 2mc s 2

(7.53)

This equation can be simplified enormously by linearization, i.e. by removing β |ψn |2z ψn , and by having A = (0, 0, Az ), and finally by writing the last parenthesis in the form of a coupling energy. Also, here again we make the perfectly reasonable assumption that all superconducting planes are physically equivalent. We can now omit the index n on the various ψ-functions. We find 2 ∂ 2 ψ 2 2eAz s αψ − − ψ =0 (7.54) 1 − cos 2mab ∂x 2 2mc s 2 Inserting the expression α =

2 2 mab ξab

and Az = Bx, and expanding the cos-func-

tion for small argument, corresponding to small s we find the equation d2 ψ mab 2π Bx 2 1 + − 2 ψ =0 (7.55) mc 0 dx 2 ξab (T ) Using a trial solution of the form ψ = eiky y eikz z f (x) one finds Bc2 =

0 2π ξab ξc

(7.56)

7.6 Ginzburg–Landau–Abrikosov (GLA) predictions for Bc2 /Bc1 The most important parameters to be determined by measurements in type II superconductors are the lower and upper critical fields, Bc1 and Bc2 , and the ratio κ = λ/ξ . Difficulties were always connected with the determination of the lower critical field Bc1 , because of the presence of pinning, which can mask completely the predicted sharp drop in the magnetization at Bc1 . Therefore, experimental data on Bc1 are often quite uncertain. The test of consistency with GLA theory is usually to compare data according to the relation (Bc1 Bc2 )1/2 /Bc = ln κ. Due to the ln κ factor, this is a quite insensitive test of the consistency of data on

GINZBURG–LANDAU–ABRIKOSOV (GLA) PREDICTIONS FOR Bc2 /Bc1

189

critical fields and κ. A much more sensitive test can be made by taking the ratio of critical fields Bc1 and Bc2 rather than their product, as we will now show. By deriving the well-known formula for Bc1 Bc1 =

0 (ln κ + ε) 4π λ2

(7.57)

one has in reality derived the κ-dependence of the ratio Bc2 /Bc1 , or the inverse thereof. This is easily shown by writing Bc1 in the form Bc1 =

0 (ln(λ/ξ ) + ε) 2 2π ξ 2λ2 /ξ 2

=

0 (ln κ + ε) (ln κ + ε) = Bc2 (7.58) 2 2 2π ξ 2κ 2κ 2

We define the function K(κ) by the relation 2κ 2 Bc2 ≡ K(κ) = Bc1 (ln κ + ε)

(7.59)

Taking the first and second derivatives of K(κ) one finds this function to have a minimum, occurring at a κ-value κe1/2−ε . In order to carry out a test procedure, we need to distinguish between isotropic systems, where Eqs 7.57, 7.58 and 7.59 are the predictions, and layered structures as in the high-Tc cuprate materials. The results are remarkably simple [12]: The K(κ)-functions have precisely the same form as in Eqs 7.58 and 7.59. With the field along the c -axis one obtains c c Bc2 /Bc1 =

2κc2 ≡ K(κc ); (ln κc + ε)

κc = λab /ξab

(7.60)

With the field in the ab-plane we get ab ab Bc2 /Bc1

2 2κab ≡ K(κab ); = (ln κab + ε)

κab

λab λc = ξab ξc

12 (7.61)

We then have K(κ) = K(κc ) = K(κab ) = 2κ 2 /(ln κ + ε)

(7.62)

Therefore, in all these cases the same maximum of Bc2 /Bc1 is predicted to exist, given by the criterion κ = e1/2−ε . Data in the literature on independent measurements of all parameters Bc1 , Bc2 , λ, and ξ turn out to be rather scarce. It is common practice to use the GLArelations to calculate for instance the coherence length on the basis of a measurement of Bc2 , using the relation we have found in Section 7.5.1. Figure 7.9 shows a plot of the function K(κ) given in Eq. 7.62.

190

APPLICATIONS OF GL-THEORY

10−1

K −1 (k)

10−2

10−3

10−4

1

10

100

k

Figure 7.9 = 0.13.

The function K −1 (κ) = Bc1 /Bc2 derived in Eq. 7.62 from GLA theory, with

GLA theory has been an enormously powerful tool by which to work out the physics of the vortex state of superconductors, even well beyond the limits of expected applicability.

7.7 Surface superconductivity and Bc3 So far our treatment of the Ginzburg-Landau equations at the mean-field level has not taken into account the surface of the sample. It has been implicitly assumed that we are working in the bulk. At the surface of the superconductor, however, some additional boundary conditions need to be imposed on the solutions, since one can quite reasonably expect the presence of an interface between the superconductor an a non-superconducting material such as a normal metal or an insulating material, to affect the nucleation of superconductivity in the material. For the purposes of studying the nucleation (i.e. onset) of superconductivity, it suffices to consider the linearized version of the first Ginzburg-Landau equation, namely

or equivalently

1 (−i∇ − 2eA)2 ψ = −αψ 2m

(7.63)

2 2mα 1 2e −i∇ − A ψ = − 2 ψ ≡ 2 ψ ξ

(7.64)

SURFACE SUPERCONDUCTIVITY AND Bc3

191

where we have introduced the characteristic length ξ2 ≡ −

2 2mα

(7.65)

We now make a couple of simplifying assumptions. a) We consider ξ to be small compared to the bulk dimension of the sample. b) We assume that the surface is such that the local radii of curvature of the boundaries are large compared to ξ . This allows us to consider the problem of a plane boundary. We first take the external magnetic field to be parallel to the surface, which is located in the (y, z )-plane, with magnetic field B = B zˆ . The superconducting sample is located in the half-space x > 0, while we take the non-superconducting material to be located in the half-space x < 0. The latter material is here chosen to be either vacuum or an insulating material, we will only briefly consider the case of a metallic coating of the superconductor, where the boundary conditions to be imposed are different. Then, the boundary condition to be imposed is that the component of the gauge-invariant supercurrent normal to the surface is zero, i.e. ∂ −i − 2eAx ψ|x=0 = 0 (7.66) ∂x We choose to work in the gauge A = Bx yˆ and look for a solution to equation of the form ψ = f (x)eiky

(7.67)

Inserting this Ansatz into the GL-equation and the boundary condition we find −

2 d2 f 1 (k − 2eBx)2 f = −αf + 2 2m dx 2m

(7.68)

with the constraints that df/dx = 0 for x = 0 and x = ∞. The above equation is the Schr¨odinger equation for a harmonic oscillator with frequency ω=

2eB m

(7.69)

and with a minimum of the quadratic potential located at X0 =

k 2eB

(7.70)

The complication arises because the boundary condition states that the solution must be flat at a position x = 0 while the minimum of the potential is located at x = X0 . If X0 = ∞ or X0 = 0, this is simple, because when the minimum of

192

APPLICATIONS OF GL-THEORY

the potential is located very far from the surface (X0 = ∞) we can ignore the boundary condition, and when X0 = 0 the boundary condition is satisfied by the standard solution to the Schr¨odinger equation in terms of a Gaussian multiplied by Hermite polynomials with Eigenvalues 2eB 1 1 = n+ ; n = 0, 1, 2, . . . (7.71) −α = ω n + 2 m 2 The lowest Eigenvalue for these two cases (X0 = (0, ∞)) quite clearly corresponds to the case where nucleation of superconductivity is energetically most favourable (for X0 = (0, ∞)), and corresponds to 2eB 1 2 = −α = m 2 2mξ 2 (h/2e) 0 B= = = = Bc2 2eξ 2 2π ξ 2 2π ξ 2

(7.72)

Hence, we rederive the well-known result that when the surface of the boundary does not constitute a complicating factor in the GL equations (which happens deep in the specimen or right at the surface) then superconductivity is nucleated at the upper critical magnetic field Bc2 . (But note that this type of sharp onset of superconductivity at a sharply defined field is an artifact of mean-field theory! In reality, Bc2 is a crossover line). Hence, we reach the conclusion that the surface has consequences for the solution to the GL equations only at intermediate values of X0 . Let us first see precisely what we mean by this statement. We start by considering the lowest energy solution for X0 very large, which is given by the well-known harmonic oscillator function for n = 0, namely mω (x − X0 )2 f (x) = A exp − 2 x − X0 2 = A exp − (7.73) ξ Thus, we see that the solution is located within a distance ξ of the position X0 . Hence, we conclude that within a sheeth of thickness ξ of the surface of the sample, nucleation of superconductivity is altered by the presence of a surface. We must now think of the Schr¨odinger equation −

2 d2 f 1 (k − 2eBx)2 f = −α(X0 )f + 2 2m dx 2m

(7.74)

as en Eigenvalue problem where the Eigenvalue is X0 -dependent, and our task is to minimize this with respect to X0 subject to the boundary condition on f at the

SURFACE SUPERCONDUCTIVITY AND Bc3

193

surface. This may in principle be done by writing down the general solution to this equation in terms of a linear combination of two degenerate hypergeometric functions, finding the expansion coefficients from the boundary conditions at the surface and at infinity, thus determining the lowest eigenvalue. This requires numerical work. We proceed by a different analytical method which yields the correct answer to within 2%. We start by rewriting the equation as mω 2 d2 f 2mα(X0 ) + (x − X0 )2 f = − f (7.75) 2 dx 2 √ √ Introducing z = mω/x, z0 = mω/X0 , and β = −2α/ω, we find −

−

d2 f + (z − z0 )2 f = βf dz2

(7.76)

where the task now is to find the lowest possible value of β subject to the boundary conditions df/dz = 0 at z = (0, ∞). This problem may be phrased as the following variational problem of minimizing the functional ∞ 2 df 2 2 dx + (z − z0 ) f dz 0 ∞ β= (7.77) dxf 2 0

with respect to variations in f. The Euler-Lagrange equation for this variational problem is precisely the above scaled differential equation. To do the minimization, we use a trial wavefunction of a form similar to the lowest eigenvalue state of the harmonic oscillator, but now shifted with respect to the minimum of the oscillator potential 1 2 f = exp − bz (7.78) 2 which we note satisfies the correct boundary conditions. It is a simple matter to perform the necessary integrals, and we obtain β=

1 2z0 b + −√ + z02 2 2b πb

(7.79)

This is now to be minimized with respect to b, which yields b in terms of z0 . This particular value of b is then to be substituted back in the expression for β, which then is minimized with respect to z0 . One may just as well do the minimization in reverse order, first minimize with respect to z0 and then with respect to b. We choose the latter. 2 ∂β + 2z0 = 0 = −√ ∂z0 πb

(7.80)

194

APPLICATIONS OF GL-THEORY

√ yielding z0 = 1/ π b. Substituting this back in β and minimizing with respect to b, we find ∂β 1 1 1 = − 2+ =0 ∂b 2 2b π b2 which yields b =

√

1 − 2/π . Substituting this back into β yields 2 βmin = 1 − π

(7.81)

(7.82)

We now go back to the definition of β = −2α/(ω), and reintroduce the characteristic length 1/ξ 2 = −2mα/2 as well as the frequency ω = 2eB/m to find 2 h/2e Bc2 (7.83) = = βmin = 1 − = 2 2 π B 2eBξ 2π ξ B Hence, we find that in the presence of a surface, i.e. when nucleation of superconductivity occurs within a length ξ from the surface plane, the upper critical field at which it starts to nucleate as the field is lowered from above, is given by 1 B = Bc3 = √ Bc2 = 1.66Bc2 1 − 2/π

(7.84)

A more careful numerical analysis based on hypergeometric functions yields the slightly larger value for the surface nucleation field Bc3 = 1.69Bc2

(7.85)

We see that our analytical estimate is in excellent agreement with this, differing by less than 2%. It is straightforward, but a bit tedious, to obtain essentially perfect agreement with the numerical result if we use a slightly refined variational function f (x) = (1 + cz2 ) exp(−bz2 /2). Physically, the boundary condition df/dx = 0; x = 0 means that the order parameter ψ is enhanced at the surface, since the solution to the problem ignoring boundary conditions has a negative derivative. Thus, we may view this as pinning of Cooper-pairs to the surface of the sample. We should, however, be cautious about regarding Bc3 as some sort of critical field, it is after all a surface phenomena we are talking about, and superconductivity with long-range order in the superconducting order parameter does not exist at any finite temperature in two dimensions, as we shall see in Chapter 9. Moreover, as the above results show, Bc3 is tied to the notion of the bulk upper critical field Bc2 , which itself is not a critical field either, but rather defines a crossover line. Bc3 is therefore best thought of as a surface enhanced crossover line where one sees the first nucleations of locally superconducting islands in the system. The main point

SURFACE SUPERCONDUCTIVITY AND Bc3

195

about the above results, is that when superconductivity occurs in a system, it tends to nucleate at the surface of an ideal (defect-free) sample, not in the interior of it. Alternatively, if we have material defects in the interior of the system, superconductivity may nucleate in the vicinity of such defects as well. Let us also consider the case of an inclined magnetic field with respect to the sample surface. We imagine tilting the field in the (x, z ) plane and angle θ with respect to the sample surface located in the (y, z )-plane. hence we have B = B cos(θ )ˆz + B sin(θ )xˆ

(7.86)

We now work in a gauge such that the vector potential is given by A = B[x cos(θ ) − z sin(θ )]yˆ

(7.87)

The first Ginzburg-Landau equation now becomes 2 2 ∂ 2 ψ ∂ 2eB 2 ∂ 2 ψ 2 − i + [x cos(θ ) − y sin(θ )] ψ = −αψ − + 2m ∂x 2 2m ∂z2 2m ∂y (7.88) √ 2 2 Again, introducing √ √ 1/ξ = −2mα/ and new coordinates ζ = mω/x, η = mω/y, ρ = mω/z with ω = 2eB/m, and defining β = −2α/(ω) the equation may be written on the form 2 ∂ 2ψ ∂ 2ψ ∂ − 2 − + [ζ cos(θ ) − ρ sin(θ )] ψ = βψ + i ∂η ∂ζ ∂ρ 2

(7.89)

We now try a solution of the form ψ(ζ, η, ρ) = g(ζ, ρ) exp[iζ0 η]

(7.90)

and obtain the following differential equation −

∂ 2g ∂ 2g − 2 + [ζ cos(θ ) − ζ0 − ρ sin(θ )]2 g = βg ∂ζ 2 ∂ρ

(7.91)

This equation is the Euler-Lagrange equation for the variational problem of minimizing the following functional 2 2

∞ ∞ ∂g ∂g 2 2 + ∂ρ + (ζ cos(θ ) − ζ0 − ρ sin(θ )) g 0 dζ −∞ dρ ∂ζ

∞ ∞ β= 2 0 dζ −∞ dρg (7.92)

196

APPLICATIONS OF GL-THEORY

Here, we follow the strategy of the previous treatment and try a variational Ansatz of the form 1 2 1 2 g(ζ, ρ) = exp − aζ − bρ (7.93) 2 2 Performing the necessary Gaussian integrals, we find 1 1 1 2 1 2ζ0 2 2 2 β= b + cos (θ ) + a + sin (θ ) + cos (θ ) ζ0 − √ 2 b 2 a πb (7.94) Minimizing this with respect to a, b, and ζ , we find 2 β = cos(θ ) 1 − + sin(θ ) π 2 (7.95) b = cos(θ ) 1 − π √ with a = sin(θ ) and ζ0 = 1/ π b. Now, in analogy with the θ = 0 case, where we had Bc2 2 βmin = 1 − = (7.96) π Bc3 (0) we may define β=

Bc2 Bc3 (θ )

(7.97)

which leads to 1 1 1 sin(θ ) = cos(θ ) + Bc3 (θ ) Bc3 (0) Bc2

(7.98)

or equivalently Bc3 (θ ) =

Bc3 (0) cos(θ ) +

(7.99)

√sin(θ ) 1−2/π

Hence, we see that when the field is perpendicular to the surface, Bc3 = Bc2 , and the variation in Bc3 is smooth in between the limiting cases θ = 0 and θ = π/2. In particular 1 dBc3 Bc3 (0) 1 − |θ =0 = = = 1.66 (7.100) Bc3 dθ Bc2 1− 2 π

SURFACE SUPERCONDUCTIVITY AND Bc3

197

A more careful numerical analysis of the problem of tilted magnetic fields yields for the above slope the result 1.35, which is not too far away from our analytical estimate. A more accurate variational result may be obtained by refining the variational function, to a form like g(ζ, ρ) = (1 + cζ 2 + dρ 2 ) exp(−(aζ 2 + bρ 2 )/2). In the case of a metallic coating of the superconductor, a current can in principle go across the interface at x = 0, such that the boundary conditions are different. Consider again the case of a magnetic field parallel to the surface, with the vector potential given by A = Bx y. ˆ The boundary condition to be used is then given by, crudely dψ ψ |x=0 = − dx l

(7.101)

where l is some characteristic length that provides a proximity effect of superconductivity into the metal. This reduces the flatness of ψ at the surface, i.e. the pinning of Cooper pairs to the surface is reduced. Hence one can expect Cooper pairs at the surface to diffuse into the metal and be destroyed. A metallic overlayer thus acts as a pair-breaker and this will impede surface nucleation of superconductivity and suppress surface superconductivity above Bc2 . Finally, a cautionary remark is in order concerning hard superconductors, i.e. those with large bulk values of κ. The treatment in this section has been exclusively at the mean field level. As the surface of the superconductor is approached from within one must expect a continuous depletion of superfluid density. As we shall demonstrate in Chapters 9 and 10, the superfluid density is connected to the phase-stiffness of the order parameter. This will also reduce the correlation length ξ , since this is basically a measure of the length over which the local phases of the order parameter are correlated. A reduction in ξ would lead to an increased estimate for the upper critical field compared to the bulk value.

8 More on the Flux-line System 8.1 Elementary pinning forces and simple models 8.1.1

The concept of a pinning force

We have previously derived the force per unit length from one vortex, labelled as number 1, on another parallel vortex labelled as number 2, in Chapter 6. This situation is illustrated in Figure 8.1. We found in Chapter 6: f2,x = jy 0

(8.1)

f 2 = J 1 × 0

(8.2)

which we can rewrite as

where J 1 is the supercurrent density from vortex number 1 at the position of vortex number 2. If there is a current from other vortices, or an additional external current, giving a total current density J s , this will determine the total force per length, f on the reference vortex, i.e. f = J s × 0 .

(8.3)

f becomes a volume force, F , if we divide both sides by unit area, and we have F = Js × B

(8.4)

This force will, if acting alone, cause a continuous displacement of flux lines as long as the force F is acting upon the flux line lattice. This is a basic problem encountered when a type II superconductor is to be used for current and energy transport. The forced motion of the vortices against the friction of the electron gas, normal and superfluid, causes dissipation of energy, and the superconductor Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

200

MORE ON THE FLUX-LINE SYSTEM

2

1

Figure 8.1 Two interacting flux lines, repulsive forces shown.

behaves essentially like a normally conducting material. To stop or prevent this motion, a pinning force F p of magnitude at least equal to F is necessary. When |F | < Fp the flux-line lattice will be at rest; whereas the lattice will move if |F | > Fp . The precise value of F corresponding to the volume pinning force Fp is specially significant. When the applied force density is equal to Fp the corresponding current density is defined as the critical current density, Jc . We now have Fp = Jc B or Jc ≡ Fp /B

(8.5)

This is the conceptual definition of Jc . How it is to be determined is not obvious. Fp is not usually measured directly. Rather, by judicious choice of a criterion for determination of Jc , one can calculate the pinning force based on that definition.

8.1.2

Pinning force and flux gradient

Equation 8.4 could equally well be written by means of Maxwell‘s equation ∇ × H = J , as F = (∇ × H ) × B

(8.6)

This points to the significant fact that a current corresponds to the existence of a gradient of H . We have here the curl of H , ∇ × H , but in well defined cases

CRITICAL STATE AND THE BEAN MODEL

201

ˆ along the z-axis and this is just a negative gradient. Take for example H = kH ˆ ˆ ˆ the current along the y-axis. We get, using i, j , k as unit vectors J = ∇ × H = −jˆ

∂ H = Jy jˆ ∂x

(8.7)

The volume force acting on the flux lattice is now, on introducing the B-field |F | =

B ∂B µ0 ∂x

(8.8)

This relation provides a basis for a definition of critical current density Jc in the Bean model.

8.2 Critical state and the Bean model The critical current density Jc will in general depend on both r and B. This should be regarded not only as a possibility, but as a reality under usual conditions. This fact tends to complicate the analysis of the critical current condition substantially. Even so, simplified models are quite often useful. Bean [87] suggested to model Jc as a constant value corresponding to regarding Jc = µ−1 0 (dB/dx) as constant. Figure 8.2 shows sketches of the correspondence between Jc and the flux gradient ∂B/∂x in several situations, including the reversal of flux gradient on reducing the applied field Ba after it has been raised to a maximum value Bm , larger than B ∗ , which is the field where the flux first penetrates to the center. In all these sketches |Jc | is taken to be a constant value in space and time. This demonstrates the properties of the simplest form of Bean model. The situation where the flux front reaches the center, and the current density is Jc everywhere, is the Bean critical state. It allows a simple and often quite useful analysis of what is going on in the sample under varying external applied field. The Bean model, as shown in Figure 8.2, takes Jc to be independent of B. This is a condition which is never quite correct. In cases where the pinning force is independent of B, Jc will be proportional to B −1 . We have also to keep in mind that higher temperatures necessarily will influence Jc negatively, and that a spatial dependence of Jc is also present unless the material is perfectly homogeneous with regard to pinning force. Experience tells us that relatively simple modifications of the Bean model may be sufficient to account for more complicated situations. One modification, often referred to as the Kim–Anderson model [88], is described by the following expression for Jc Jc (T , B) =

J0 (T ) 1 + B/B0

(8.9)

202

MORE ON THE FLUX-LINE SYSTEM Bm

B(x)

B(x)

B*

(3) Ba

B(x)

(1)

Ba

(2) (2)

(1) x

−d/2

d/2

+Jc

x

−d/2

d/2

+Jc

x (1)

(1)

(1)

(2,3)

−Jc (a)

d/2

+Jc (2,3)

−Jc

x

−d/2

x

x −Jc

(b) +Jc (2)

−Jc (c)

Figure 8.2 Bean model. (a) Flux distribution (upper part) and corresponding current distribution (lower part) after application of an external field Ba which is subsequently kept constant. (b) Similar to situation (a), labelled as (1); then (2) after raising Ba to B ∗ where the flux front reaches the centre of the sample, the situation referred to as the critical state, and (3) after increasing Ba to Bm above B ∗ . (c) Shows the effect of lowering the applied field, case (1) and case (2), by different amounts.

which has been shown to agree well with experimental results in some cases. Here J0 (T ) is the critical current density at zero field and B is the local flux density. B0 is a model parameter to be determined by experiment. Next we derive a simple relationship between Jc and the magnetization, implied to exist in Figure 8.3. Imagine that we have measured a complete magnetization curve M(H ), looking like the one sketched in Figure 8.3a. In Figure 8.3b we indicate how the area A represents the difference in magnetisation of the sample at point (1) and point (2) in Figure 8.3a. The total magnetization difference at H1 is M = M↑ − M↓ = M(H1 ), where we have once arrived at H1 from lower field (1), and once from higher field (2), as illustrated in Figure 8.3b. The two approaches to H1 result in different magnetisations M↑ and M↓ , and with a difference M↑ − M↓ . This construction can also be made via graphical display of the Bean model. Now,

CRITICAL STATE AND THE BEAN MODEL

203

−M

(1) ∆M H1 (2)

Hc2

H

(a)

(2)

H

A ∝ ∆M × d (1)

(b)

− d2

d 2

x

Figure 8.3 (a) is a sketch of magnetization versus field H in a type II superconductor with pinning. Magnetization starts out from zero. Points (1) and (2) refer to the same magnetic field with different magnetization. The dotted line is the magnetization without pinning. In (b) we sketch how the magnetisation difference M is obtained.

since Jc =

M(x) x ,

we have M(x) = Jc x in the Bean model. We calculate 1 M↓ = − d/2

d/2

0

1 Jc x dx = − Jc d 4

(8.10)

Correspondingly we get M↑ = 14 Jc d. The difference is then M = M↑ − M↓ = 1 2 Jc d, or Jc = 2

M d

(8.11)

This allows an estimate of Jc from a half cycle measurements of M(H ), (‘Magnetization Jc ’). In other sample geometries, a numerical, geometry dependent factor of the order of unity will modify the right-hand side of Eq. 8.11.

204

MORE ON THE FLUX-LINE SYSTEM

The simple, and very useful rule we glance from this, is that the wider the magnetization loop is, the higher is Jc . This kind of data analysis is widely used to obtain Jc . Before computing the Jc -value, one should also attempt to remove the equilibrium part of the magnetization curve, i.e. the M(H ) curve which is obtained without pinning. This magnetisation method for measurement of Jc is often easier to use than the transport method.

8.3 Flux-line dynamics, thermal effects, depinning, creep and flow 8.3.1

TAFF, flow and creep: Definitions

Current transport measurement are always central in the study of superconductivity. In Figure 8.4 we have sketched measured voltage V versus current I , (alternatively electric field E versus current density J ) in the presence of an external magnetic field which has created a certain vortex density in the superconductor. The definitions which apply to the 3 different parts of the I–V curve are: ‘thermally assisted flux flow’ (TAFF) in the low current end, ‘flux flow’ in the high current region, and ‘flux creep’ in the transition region between the two. While the latter two terms were commonly used in low-Tc research, the new term, TAFF, was coined for this new aspect of high-Tc , I–V characteristics. The particularly important feature of this plot is the highly nonlinear region, where the critical current Ic is marked in the region crossing over between TAFF and flux flow. What has been agreed on as a practical measure is to define Ic at the point where V = 1 µV, or similarly, E = 1 µV/cm. The point is that

E, V

Flux flow

Flux creep 1 µV

TAFF Jc, Ic

J, I

Figure 8.4 A sketch for the definition of Ic or Jc by transport measurement. This curve has a linear V versus I at low I , followed by a highly nonlinear region at intermediate values of I , and finally a linear relation again. The effective resistance is quite different in the two regions where ohmic behaviour is found. The plot can be read either as an E –J characteristic or as an I –V characteristic.

FLUX-LINE DYNAMICS, THERMAL EFFECTS, DEPINNING, CREEP AND FLOW

205

there is no way to define sharply what Ic is. One has to agree on a criterion related directly to measurements. However, it should be noted that flux flow is a phenomenon which arises when the current is high enough to essentially tear loose the whole flux lattice, and set it in sliding motion. It is then quite reasonable and conceptually sound to define Ic and the corresponding Jc as the point where this flux motion is just about to begin. All of the above implies the presence of various kinds of flux line dynamics present during the measurement.

8.3.2

Flux flow

If the superconductor is pin-free, or if the Lorentz force is so strong that it exceeds the pinning force, the vortex velocity v is limited by the viscous drag exerted by the surrounding medium, through the force balance 0 J = ηv giving v=

1 0 J η

(8.12)

Multiplying the above equation with B gives the E-field E = Bv =

B 0 J = ρff J η

(8.13)

with a flux flow resistivity ρff =

1 B0 η

(8.14)

The most widely accepted theory of flux-flow was worked out by Bardeen and Stephen [89]. They considered a vortex core of radius ξ , which can be treated as if it were in the normal state. When a vortex is set into linear motion the moving flux pattern will generate an electric field in its surroundings, the vortex core included. The induced resistive currents in the vortex core creates a loss W = ρff J 2 , and thereby a flux-flow resistivity. The result is ρff = ρn

B Bc2

(8.15)

where ρn is the normal state resistivity. It is not difficult to guess such a relation: when B reaches Bc2 , ρff becomes ρn as it should. When B goes to zero, ρff goes to zero as it should, and in between the factor B/Bc2 is simply the fraction of the material occupied by the vortex cores. ρff is therefore equal to ρn times this fraction. The result is the same as if a uniformly distributed current were passed through the material and losses would appear from the fraction of the current which passed through the core regions.

206 8.3.3

MORE ON THE FLUX-LINE SYSTEM

Thermally activated flux creep: Anderson model

Random thermal forces may induce escape of a vortex from its potential minimum at the pinned position. Depinned vortices will move, or ‘creep’ in order to relax the critical state field gradient. We outline the theory of flux creep which was put forward by Anderson and Kim [88]. The escape rate R from pin sites is determined by the Boltzmann factor, R = ν0 e−U/kT

(8.16)

where U is the height of the activation barrier and ν0 is some microscopic attempt frequency, typically of order 10−8 − 10−10 s−1 . As indicated in Figure 8.5, the effective height of the barrier will be reduced with increasing current. We can model this by writing U = U0 (1 − J /Jc ). Here Jc is the critical current density, and is proportional to the maximum energy gradient dU/dx. The decay of a finite (non-equilibrium) magnetization as well as its associated current density J , proportional to R, for forward jumps is U0 dJ ∝ e− kT (1−J /Jc ) dt

(8.17)

J=0

J < Jc

J ~ Jc

Figure 8.5 force.

Energy landscape for a flux line in a pinning environment and a uniform external

SINGLE PARTICLE TAFF

207

with the long-time solution J (t) ∝ const. − ln(t).

(8.18)

Hence, at long times the magnetization current and therefore also the magnetic moment decay proportional to ln t. In a transport measurement the E –J characteristics will be exponential, since the force equation eE = ev × B can be written as U0

E = Blν0 e− kT (1−J /Jc )

(8.19)

where l is the effective jump distance. This equation is of course the equivalent of an I–V characteristic. It is highly non-linear as required by experimental observation sketched in Figure 8.4, and the model contains simple creep behaviour. The flux-creep theory described here is a single particle model, i.e. depinning events occur by escape of individual vortices, independently at individual pins. The simplest way of accounting for collective dynamics is to assume that bundles of correlated flux-lines move simultaneously. Anderson suggested that all fluxlines within a distance λ would constitute a correlated flux bundle. However, the bundle concept does not introduce truly new dynamics, as its effect can be shown to alter only phenomenological parameters like U , Jc , l etc. A more advanced approach to collective dynamics is the theory of collective creep, a subject we return to below.

8.4 Single particle TAFF The creep rate as given above has a finite value even for J = 0. This unphysical result occurs because we did not take into account the asymmetry of forward and backward flux jumps. If one subtracts jumps in the backwards direction from forward jumps in the rate equation, one obtains the E-field, U U − kT0 (1−J /Jc ) − kT0 (1+J /Jc ) E = Blν0 e −e −U0 /kT

= 2Blν0 e

U0 J sinh kT Jc

(8.20)

which gives the same result as earlier at large currents, J Jc kT /U0 , but at low current it gives a linear resistance, the so-called TAFF resistance (thermally assisted flux flow) E = 2Blν0

U0 J = ρTAFF J Jc kT

(8.21)

208

MORE ON THE FLUX-LINE SYSTEM

According to this analysis, magnetization current and magnetic moment will decay exponentially with time in a way analogous to skin effect in normal superconductors. Linear resistance has been found at low current densities in a large range of temperatures below the transition. The relevance of the TAFF diffusive dynamics for this regime was discussed by Kes and coworkers [90].

8.5 FLL elasticity and pinning 8.5.1

Collective effects

Among the more important recent developments is a deeper insight into the wavevector dispersion of the elastic constants, which is important for melting as well as for pinning of the flux line lattice. In this Section we give an elementary discussion of pinning effects based on the elasticity theory worked out before in Chapter 6. An elastic energy is always written as (1/2)cε2 , where c is an elastic constant, and ε is a corresponding elastic strain. This is the case whether the strain is applied to the crystal lattice as well as to the flux line lattice. What concerns us in the following is the flux line lattice. To visualize the meaning of typical strains and elastic constants in the FLL, we refer to Figure 8.6 which illustrates the three important strains, with corresponding elastic constants c11 for a strain ε1 , c44 for a strain ε4 , and c66 for a strain ε6 . Calculations in Section 6.7 show that an important k-vector dispersion occurs at high k due to non-local response. By high k we mean k-vectors that are comparable to the inverse screening length λ−1 . We have three lengths to com√ 1 pare: (i) The lattice constant of the FLL, a = [(2/ 3)0 /B] 2 , (ii) the screening length λ and (iii) the wavelength λε of the strain. Due to the high density of vortices giving a short length a at a typical magnetization, we usually have λ a except very close to Bc1 . What is important for the elastic response under such conditions is whether the applied strain has a k-vector which is of the order of λ−1 or greater. Under such conditions the flux line interactions are substantially weakened, since the denominator in the expression for cii typically goes like 1 + k 2 λ2 , with an exception for c66 . We refer to Chapter 6 regarding the elastic properties of the FLL. In the isotropic case the results are: c11 (k) ≈

B2 ; µ0 (1 + k 2 λ2 )

c44 (k) ≈ c11 (k) + 2c66 ln

c66 ≈

B 0 BBc1 · ≈ ; 2 8µ0 2π λ 8µ0

κ2 1 + kz2 λ2

(8.22)

We notice that c66 is non-dispersive and very small compared to the two others. In high-Tc superconductors where λ is very long (≈150 nm) the softening of the

FLL ELASTICITY AND PINNING

209

e1; c11

e4; c44

e6; c66

Figure 8.6 Elastic strains ε1 , ε4 , and ε6 of a flux line lattice under homogeneous strain, i.e. k = 0. Corresponding elastic moduli are indicated in each case.

FLL becomes important at k-vectors with wavelength even larger than 150 nm, and all shorter wavelengths. The lattice constant a at 0.2 T is about 100 nm. From there on up in field, screening currents from surrounding flux lines overlap more and more, with the gradual breakdown of net screening, and accompanied by softer and softer FLL. Let us estimate the effects on thermal phonons at the Brillouin zone boundary of the crystal lattice. These have a k-vector in the ab-plane of approximately π(nm)−1 . The product kλ is then about 300. This means that the elastic constants c44 and c11 for tilt and compression are two orders of magnitude softer as seen by Brillouin zone phonons than by zone centre, k = 0 modes. In other words, acoustic waves with low wavevector will propagate faster in the presence of a magnetic field, while at the zone boundary it makes almost no difference. (Recall here that the elastic constant of the FLL is to be added to that of the crystal lattice.) We note that at k = 0, c66 typically is weaker than c11 and c1 c44 by a factor 18 BBc1 as seen from the approximation c66 ≈ BB 8µ0 . The above discussion underscores the susceptibility of the FLL of high-Tc materials to thermal fluctuations.

210

MORE ON THE FLUX-LINE SYSTEM

We refer here for completeness the results for c44 and c66 in the anisotropic case with the field along the c-axis, from which c11 can also be found. c44 (k) ≈ c66 ≈

B2 κ 2 2 2c66 ln + 2 µ0 (1 + (kx2 + ky2 )λ2c + kz2 λ2ab ) 1 + kz2 λ2ab

(8.23)

B 0 × 8µ0 2π λ2ab

(8.24)

Here κ = λab /ξc and = λc /λab = ξab /ξc . Except for differences arising in symmetry properties, we recognize the results from the isotropic case: c66 remains low and non-dispersive, and its magnitude relative to c44 is still of the order of Bc1 /8B; more precisely (0 /2π λ2ab )/8B. The key idea in collective weak pinning is to describe the distortion of the vortex lattice in terms of a correlation volume, Vc = Rc2 Lc where Rc and Lc are the transverse and longitudinal correlation lengths, respectively. A correlated volume may be thought of as a volume Rc2 Lc , which appears approximately like a piece of regular flux-line lattice, but with an average lattice constant which may be slightly different from that of the unpinned lattice. The whole flux-line system may be thought of as a collection of such correlated volumes, and Rc and Lc are average lengths defining the typical correlation volume Vc . The underlying energy principle which determines the positions of flux lines, and hence the distortions in each correlation-volume, is the balance between the elastic energy cost of deforming the flux-line lattice locally within Vc versus. the energy gained by letting the flux lines pass through several point pins within Vc . The collective pinning theory was originally developed by Larkin and Ovchinnikov [91]. For a brief analysis of these effects on Jc , following Tinkham [53] we disregard the strain ε1 . To calculate the increased elastic energy connected with strains ε4 and ε6 we need to estimate δFe = 12 c44 ε42 + 12 c66 ε62

(8.25)

Here we can divide the range ξ of the pinning force by the corresponding correlation lengths to obtain the strains. ε4 =

ξ ; Lc

ε6 =

ξ Rc

(8.26)

This gives 2 2 1 1 ξ ξ δFe = c44 + c66 2 Lc 2 Rc

(8.27)

Next we consider the pinning energy δFp . When N elementary pinning forces 1 f are added randomly in a volume Vc , the total force is N 2 f . Here N = nVc ,

FLL ELASTICITY AND PINNING

211

where n is the number of forces f per volume, and Vc is the correlation volume. This force acts, on the average, over a distance ξ , after which it becomes random. The potential energy is force times distance: 1

1

1

1

1

δFp = ξ N 2 f/Vc = ξf n 2 /Vc2 = ξf n 2 /Lc2 Rc

(8.28)

The total energy δF = δFe + δFp is 1 δF = c44 2

ξ Lc

2

1 + c66 2

ξ Rc

2

1

−

ξf n 2 1

(8.29)

Lc2 Rc

By the minimisation of δF one finds approximate expressions for Lc , Rc , Vc , as functions of c44 , c66 , ξ, n, f . The minimum of δF is found [53] to be δFmin = −

n2 f 4

(8.30)

2 ξ2 8c44 c66 1

On equating the pinning force per unit volume f (n/Vc ) 2 with the maximum Lorenz force density Tinkham found for the critical current density: Jc =

n2 f 4 2 ξ 3B 2c44 c66

(8.31)

This expression has implications borne out by experiment: Jc increases with softening of the lattice, i.e. with smaller elastic moduli, because the flux line system can more easily adjust the positions of individual flux lines to fit the random position of pins. This is often observed near the melting temperature of the flux-line lattice. It is interesting to imagine the opposite extreme; that of a completely rigid FLL in a random arrangement of (weak) pins of high density. In this case the pinning force will be zero: The total pinning energy Vp is in this case necessarily independent of the position of the FLL. The force is given by the negative of the gradient of U , and since U does not vary with position, the force must be zero. This sends a message that the density of pins should be high enough to contain a wide k-spectrum in the Fourier expansion n(k) of the pin density n(r), to take advantage of the wide range of k-values where the elastic constants c11 and c44 are soft. A Fourier density peaking at the FLL Brillouin zone boundary wavevector might seem ideal. This corresponds to a pinpoint density with an average distance like the FLL lattice constant. However, this would be ideal for that particular field only. If pinning is to be effective over a wide range of fields, there has to be a broad variation in pin distance, even for the use of the Brillouin zone boundary matching criterion to be good. Hence we end up,

212

MORE ON THE FLUX-LINE SYSTEM

again, with a broad spectrum of Fourier density k-values as a good guideline. Only when optimizing pinning for a particular value of the magnetic field, i.e. a particular FL density, can a pin distance corresponding to the Brillouin zone wavelength or its vicinity, be the optimal solution.

8.5.2

Collective creep: inverse power law U (J )

From the previous discussion of collective pinning it becomes evident that a full description of creep phenomena needs to take into account collective effects. This has been attempted [91, 92], and has led to interesting new predictions for collective creep, i.e. for the behaviour of an elastic flux line lattice in the presence of random, weak point-pin sites. In this theory the collective creep regime is characterized by diverging time and length scales in the limit of zero driving force which is also the signature of so-called vortex glass behaviour. We review here only briefly some aspects of collective creep theory without full justification, and refer to the original literature for details. The correlated volume Vc = Rc2 Lc was defined in the previous subsection as the characteristic volume which maintains the quality of a regular flux-line lattice even in the presence of distortions due to the interaction with a high density of point pins. Theory predicts that the volume Vc grows with the displacement ω of flux lines, raised to the power D, the dimensionality of the correlated volume, divided by the so-called wandering exponents ξ . In other words Vc ∝ ωD/ξ . Here D = 0 for single pancake vortices, considered as point vortices, D = 1 for a single vortex line, D = 2 for a bundle of point vortices (pancakes), and D = 3 for a bundle of vortex lines. The wandering exponent ξ is determined by equating the energy of the elastic vortex lattice deformation to the fluctuation in pinning energy. The next requirement is that both these energies should be of the order of the energy gain due to the driving force j BVc ω, the Lorentz force density multiplied by volume and displacement. Through this requirement the correlated volume becomes current dependent, and results in a current-dependent flux creep activation barrier U = Uc

Jc J

µ (8.32)

with µ = (D + 2ξ − 2)/(2 − ξ ) > 0. It has the surprising and important consequence that as J → 0, the activation energy U → ∞. This leads to vanishing of both flux motion and linear resistance in that limit. In the single vortex regime in three spatial dimensions µ = 1/7, and the divergence of U is weak (near logarithmic). As the current density decreases one crosses over from single vortex regime to a regime of small bundles with µ = 5/2, then to larger bundles with µ = 1, and finally to large bundles with

FLL ELASTICITY AND PINNING

213

µ = 7/9. Other values of the exponent µ are obtained when a layered structure becomes dominant like in some high-Tc cuprates. The collective creep theory applies at current densities much lower than the critical one, i.e. J Jc . However, U is expected to go to zero at J = Jc (in the Anderson–Kim model as U0 (1 − J /Jc )). To incorporate this into the collective creep model one often rewrites Eq. 8.32 as U (J ) = Uc [(Jc /J )µ − 1], where Uc = U0 /µ [92]. This provides an interpolation between the low current (‘glassy’) phase and the high current (linear A-K) phase.

8.5.3

Logarithmic U (J )

The various models used for U (J ) have often turned out to be difficult to distinguish on the basis of experimental data. This situation is compounded by the discovery that in many cases a logarithmic U (J ) is found to give the most adequate interpretation of data, i.e. U (J ) = Uc ln

Jc J

(8.33)

Due to the short coherence length and the strong anisotropy of high-temperature superconductors, pinning energies are small, and thermally activated flux motion is a significant source of dissipation in the current carrying state, even when the Lorentz force on the vortices is less than the depinning force. The resulting decay of a screening current corresponds to a decay of the induced magnetic moment. For this reason, measurement of the magnetic relaxation serves as a powerful tool to investigate the dynamics of vortices in superconductors. In the thermally activated regime of flux creep the decay rate of the magnetisation current density is given by the rate equation, dJ U (T , B, J ) = −A × exp − dt T

(8.34)

Where A is a constant. In Figures 8.7, 8.8 and 8.9 [93], [94] we illustrate the procedures involved in analysing magnetization current decay data for possible logarithmic activation energy. The substance studied was HgBa2 CaCu2 O6+x (Hg-1212) with a Tc = 127 K. In Figure 8.7 the time dependence of magnetisation was measured over two decades in time in 1 T magnetic field parallel to the c-axis using a SQUID detector. The magnetic moment due to screening currents caused by the flux gradient set up by application of the external field is shown here. Notice the great differences observed at different temperatures. Data have been corrected for the equilibrium magnetisation which would be present without pinning.

214

MORE ON THE FLUX-LINE SYSTEM

5K

m − meq

0.06

10 K

0.04

15 K 20 K

0.02

0.00 0

100

1000

25 K 30 K 35 K 40 K 60 K 10000

Time (s)

Figure 8.7 Typical relaxation curves in Hg-1212 of the non-equilibrium magnetic moment in a field of 1 T, at different temperatures as indicated by the numbers. The magnetic field is along the c axis. After Gj¨olmesli et al. [94]. 2500

2000

U (K)

1500

1000

500

0

0.1 T 0.5 T 1T 2T 4T 1 × 10−3

1 × 10−2

1 × 10−1

J a mJ (emu)

Figure 8.8 The barrier energy of Hg-1212 as calculated from Eq. 8.35. Each curve consists of data sets obtained at the temperatures indicated in Figure 8.7. The numbers indicate the values of the external magnetic fields, in tesla. B parallel to the c-axis. After Gj¨olmesli et al. [94].

In Figure 8.8 data were analysed by the Maley method [95]. This consists first in inverting Eq. 8.34, to write it as dmJ U (T , B, mJ ) = T ln A − ln (8.35) dt

FLL ELASTICITY AND PINNING

215

1200

Uc (T )

800

400

0

0

1

2

3

4

B (T)

Figure 8.9 Resulting Uc versus T from the analysis of data in Figure 8.8.

after replacing current J in Eq. 8.34 with the associated magnetic moment mj = m − meq . Here, the quantity meq is determined from the experimental data by the asymmetry in the magnetization during increasing versus decreasing field. Next, all measurement taken at different temperatures in the same magnetic field are regarded as giving access to different segments of U (J ) since J associated with any magnetisation is proportional to that magnetisation. The data in Figure 8.8 immediately attests to a current-dependent activation energy close to logarithmic in its dependence on J , according to Eq. 8.33. The experiment also gives further information about the B-field dependence of the activation energy, while it was not necessary to assume T -dependence of U . A logarithmic U (J ) could possibly be expected from a model [96] in which a logarithmic spatial variation of pinning energy is involved. Alternatively, it can be a special case of collective creep for 2D pinning in the extreme lowcurrent limit [97]. Alternatively again, it may be viewed as a special case of the inverse power law Eq. 8.32 with vanishing µ. Furthermore, in the critical region near a vortex glass transition (see later), power law E–J curves are expected for intermediate currents, irrespective of the value of µ, often referred to as the vortex glass exponent. Such power-law E–J would suggest logarithmic U (J ) for intermediate currents, and could fill the gap between the low current limit and high current limit in the interpolation formula for the collective creep. We note finally, that the experiment just described gave indication of a different type of creep at very low temperatures, a temperature independent limit creep due to quantum mechanical tunnelling between pin sites.

8.5.4

The vortex solid–liquid transition

A much debated subject in the scientific literature on the properties of the vortex system in superconductors, and in high-Tc superconductors in particular,

216

MORE ON THE FLUX-LINE SYSTEM

is the question regarding the nature of the transition between a vortex liquid and a vortex solid, following the works of Gammel and Bishop [98], Nelson [99], and Fisher et al. [100]. Two views have been advocated, that the solid phase may be in the nature of a vortex glass, or that it may be a more regular vortex lattice. In the first case a continuous transition is expected, in the latter a first order discontinuous one. Over the years the conclusion has been reached that both are possible. Depending on the amount of pinning, at low pin density freezing of a regular lattice may occur. We refer here to the Topical contribution of Kadowaki (Section 13.8) showing in a convincing manner that a first order transition to a regular vortex solid can indeed take place. At high density of pins the “vortex matter” is sufficiently distorted from a regular lattice that it freezes into what has become known as a vortex glass state. The analysis of this state was made earlier than the first order transition, largely due to the difficulty of obtaining superconducting material with low pin density. The fact that the frozen vortex system may appear as a regular lattice has been amply demonstrated by various decoration and imaging techniques. We refer to Figure 8.10 for an example. The other alternative, the vortex glass, was concluded to exist from very detailed I–V (or E–J) characteristic measurements [102] in YBCO thin film (see Figure 8.11 [103]). The glass line (Tg -line) in the phase diagram may be determined by scaling of E–J data. Just at Tg the current–voltage characteristic is expected to show

Figure 8.10 Magnetic decoration techniques allows imaging of nearly perfect triangular vortex lattice. After Tr¨auble and Essmann [101].

FLL ELASTICITY AND PINNING

217

1

3

log E

0

−1

Tg 2

−2 1 −3

4

5

6

7 log J

8

9

10

Figure 8.11 Schematic I–V isotherms of an YBCO single crystal in a magnetic field applied parallel to the c-axis. The dashed line marks the glass transition temperature below which the curves decrease exponentially. The temperature decreases in equal steps from top to bottom or from left to right. Region 1 marks the linear I–V behaviour, region 2 indicates non-linear behavior above Tg and region 3 is when d(log E)/d(log I ) = 3 both above and below Tg . [103]. Simplified from Blatter et al. [97].

power law behaviour, E ∝ Jα

(8.36)

with α = (z + 1)/(D − 1), where z is the dynamic exponent with typical value 4–5, and D is the relevant spatial dimension. Above Tg the characteristic should change from ohmic ρ(T ) ∝ (T − Tg )ν(z+2−D)

(8.37)

at very low J where ν is the temperature exponent for the coherence length, to power law at high J . Below Tg a glass-type response at small current densities is expected as U0 Jc µ E ∝ exp − kT J

(8.38)

Again a power law critical behaviour is expected at high current densities. The crossover between the two regimes of power law at small scales and large current, and liquid/glassy state at small scales (probed by low current density) scale as Jx± ∝ |T − Tg |ν(D−1)

(8.39)

218 8.5.5

MORE ON THE FLUX-LINE SYSTEM

Lindemann criterion and melting of a clean flux-line system

In this subsection, we will present a calculation that determines the rough position of the line in the (B, T ) phase-diagram where the flux-line lattice may be expected to melt into a liquid state, i.e. the transition line from an Abrikosov flux-line lattice to a vortex state with zero shear stiffness. Crucial in our considerations will be the observation that conventional melting of a three-dimensional solid is expected to be a first order phase transition. This means that longwavelength fluctuations do not occur at the point of the transition, unlike in a second order phase transition. Under such circumstances, short-wavelength fluctuations are the ones responsible for inducing the transition from the solid to the liquid state. For our purposes this may be rephrased as follows. The Fourier modes of the fluctuations that dominate at the transition point are those that live at the boundary of the first Brillouin zone of the vortex lattice, i.e. those Fourier modes of fluctuations that have the largest wave vectors. Thus, it is reasonable to conjecture that when we want to estimate the position of the melting line using a description of the vortex lattice in terms of elasticity theory, we need to consider wave-vector dependent elastic moduli, i.e. non-local elastic moduli. In fact, as we shall see, this is absolutely crucial in order to obtain a reasonable estimate of the location of the melting line, since it will turn out that the elastic moduli of the flux-line lattice soften significantly as the wave vectors increase, and this dramatically enhances the susceptibility of the flux-line system to thermal fluctuations. Moreover, the variation of the position of the melting line with degree of layeredness of the material, can only be brought out through a non-local formulation. Before we go into the details, let us outline the structure of the the calculation that determines the position of the melting line, Tm (B). We consider a situation where we have an external magnetic field along the zˆ -direction, and we consider also the case where we have uniaxial anisotropy. This will make our results directly applicable to the study of the melting transition in the high-temperature cuprates, where the issue of flux-line lattice melting was first seriously considered as an experimental reality. (Many years earlier, Eilenberger had considered the melting of the flux-line lattice theoretically in moderate type II superconductors, and concluded that a melting line would be practically indistinguishable from the upper critical field line Hc2 (T )) [104]. The ground state of the system is the hexagonal Abrikosov vortex lattice, and we now consider the Hamiltonian that governs the elastic fluctuations around this ground state. Hence, we write the positions of the flux lines as rν = Rν + sν (z) Here, Rν is the position of flux line number ν, while sν (z) = (sxν (z), syν (z), 0) is the displacement of the νth flux line away from its position in the perfect

FLL ELASTICITY AND PINNING

219

Abrikosov flux-line lattice. Note how this displacement vector has two components, which vary with the distance along each flux line. In order to consider the fluctuations of the flux-line lattice in the continuum limit, we define an effective elastic Hamiltonian governing these fluctuations. For an ideal triangular lattice the Hamiltonian in the harmonic approximation takes the simple form

1 2 H = si (−k) cL (k)ki kj + δij c66 (k)k⊥ + c44 (k)kz2 sj (k) (8.40) 2 k

Here, cL , c66 and c44 are bulk-, shear-, and tilting elastic moduli, respectively, and si (k) are the Fourier modes of sν (z). Given the Hamiltonian Eq. 8.40, the elastic propagator can be written in the form

PT PL (8.41) + Gij (k) = kB T 2 + c (k)k 2 2 + c (k)k 2 c66 (k)k⊥ c11 (k)k⊥ 44 44 z z 2 is the transverse where c11 (k) ≡ cL (k) + c66 (k). Moreover, PT = δij − ki kj /k⊥ 2 is the longitudinal projection operator. projection operator, while PL = ki kj /k⊥ To examine the stability of the flux-line lattice against thermal fluctuations we will determine the mean square displacement of the flux lines from their equilibrium positions d2 (T ) = sν2 = TrGij (k) (8.42) ν

k

Here .. indicates a thermal average with respect to the Hamiltonian Eq. 8.40. Using Eq. 8.41 in Eq. 8.42

∞

d (T ) = kB T 2

×

0

dkz 2π

0

2

2 dk⊥ 2π

1 2 + c (k)k 2 c66 (k)k⊥ 44 z

+

1 2 + c (k)k 2 c11 (k)k⊥ 44 z

(8.43)

The Lindemann criterion now states that the flux-line lattice will melt when thermal fluctuations are such that the thermally induced root mean square displacements of each flux line is some fraction of the intervortex distance in the ground state of the Abrikosov vortex lattice, i.e. the melting criterion is given by d(T ) = cl, where l is the lattice parameter of the flux-line lattice, and c is some fraction typically of order c = 1/10. In the triangular Abrikosov vortex lattice, √ we have 3l 2 /2 = 0 /B, i.e. l is determined by a flux quantization condition. In the above expression, we have approximated the k-space integral over the first Brillouin-zone by assuming a circular Brillouin-zone of radius , where 2 , and b = H /H . Here H is the spatial average of the field, 2 = 2b/ξab sp c2 sp

220

MORE ON THE FLUX-LINE SYSTEM

averaged over the sample, and Hc2 is the upper critical field. Moreover, ξ⊥ is the ab-plane coherence length. The k-dependant elastic moduli can only be obtained from the full Ginzburg– Landau theory after a very arduous and lengthy calculation, there really appears to be no easy way of obtaining them. However, a detailed derivation may be found in the paper by Houghton and colleagues , [105], and the interested reader is referred to this paper, see also the work of Sardella [106]. The expressions for the elastic moduli, despite their involved derivations, are relatively simple and given by

B 2 mab 1 1 c44 (k) = (8.44a) ω0 2 + µ0 mc k⊥ + (mab /mc )(kz2 + ω0 ) 2bκ 2 B2 k 2 + (mab /mc )ω0 c11 (k) = ω0 2 + (m /m )(k 2 + ω )) µ0 (k 2 + ω0 )(k⊥ ab c 0 z

1 (8.44b) − 2 k⊥ + (mab /mc )kz2 + kψ2 2 . Compare these expression with those given in where kψ2 = 2(1 − b)/ξab Eq. 6.129 in Chapter 6, for the case where the magnetic field is parallel to the c-axis. ˆ These expressions are a bit more precise than those given there and in Subsection 8.5.1, in that they explicitly also incorporate the core-contribution to the elastic moduli. Generalization of the above Eqs 8.44a and 8.44b for parallel flux lines (kz = 0) for the case where the magnetic field is tilted away from the c-axis ˆ was given by Sardella [106]. The corresponding generalization of Eqs 8.44a and 8.44b for the case kz = 0 has not yet been achieved. In the above, ω0 is the spatial average of the square of the Ginzburg–Landau function in the ground state of the Abrikosov flux-line lattice. Since we will not need an explicit expression for this quantity here, we do not specify it further. Moreover, the uniaxial anisotropy is manifest through the parameter mc /mab , where mc is the normal-state quasiparticle mass in the z-direction, while mab is the quasiparticle mass in the ab-plane. Another way of writing this is mc /mab = λ2c /λ2ab . The shear modulus of the Abrikosov flux-line lattice is for all practical purposes k-independent. In the present geometry, where the external magnetic field is directed along the axis of uniaxial anisotropy, the shear modulus will be that of an isotropic superconductor, since only shearing in the ab-plane makes any physical sense in this case. Thus, the shear modulus is given by

c66 =

Bc2 b(1 − b)2 µ0 8κ 2

(8.45)

FLL ELASTICITY AND PINNING

221

Several things are worth noting about these expressions. First of all, when k → 0, all effects of uniaxial anisotropy, manifest through the parameter mc /mab , vanishes. Note also that when k = 0, the maximum value of c44 and c11 occurs at the upper critical field, as a function of magnetic field. Using the dimensionless wavevector q = k/, the above expressions for c44 and c11 may be written

1 B 2 (1 − b) mab 1 c44 (q) = (8.46) + 2 + (m /m )(q 2 + m2 ) µ0 2bκ 2 mc q⊥ 2bκ 2 ab c z λ q 2 + (mab /mc )m2λ B 2 (1 − b) c11 (q) = 2 + (m /m )(q 2 + m2 )) µ0 2bκ 2 (q 2 + m2λ )(q⊥ ab c z λ

1 (8.47) − 2 q⊥ + (mab /mc )qz2 + m2ξ where we have introduced the ‘mass’-parameters m2ξ = (1 − b)/b and m2λ = (1 − b)/2bκ 2 . Now, another interesting feature of the wave-vector dependant moduli becomes evident. For finite k(q), they vanish at the upper critical field, in contrast to the k = 0 moduli, which acquire their maximum at that value of the magnetic field. This means that those Fourier modes that are most relevant for melting the flux-line lattice, become particularly soft as the magnetic field approaches the upper critical field limit. This is true for the case of uniaxial anisotropy, as well as for the isotropic case. It substantially contributes to melting the flux-line lattice well below the upper critical field line, and is a key feature which leads to a suppression of the melting line below the upper critical field even for moderately small Lindemann parameters c. To determine d2 (T ) from Eq. 8.42, we have to integrate over the entire circularized Brillouin-zone 0 < q⊥ < 1. Therefore, it is evident that a fully non-local theory, i.e. an elastic description with wave-vector dependant moduli, is essential. For arbitrary field and temperature, the necessary integrals in Eq. 8.42 can only be done numerically, however with some limitations (that turn out to be not very restrictive in strong type II superconductors), analytic results can be obtained that provide key insights into the main physical parameters controlling the position of the melting line. We proceed by writing d2 (T ) = d21 (T ) + d22 (T )

(8.48)

where d21 (T ) is the contribution to Eq. 8.42 containing the shear modulus, while d22 (T ) is the contribution to Eq. 8.42 containing the bulk modulus. For b > 1/2κ 2 we find

2 kB T mc 2bκ 2 √ d21 (T ) = ( 2 − 1) (8.49) 0 c0 4π c44 mab 1 − b 66

222

MORE ON THE FLUX-LINE SYSTEM

while under the condition b > 1/2κ 2 and (1 − b)/b 1 we find

kB T 2 mc bκ 2 2 d2 (T ) = 0 c0 4π c44 mab 1 − b 11

(8.50)

0 and c0 are the elastic moduli given above taken at k = 0. The factors Here, c44 11 in square brackets in each term is what we would have obtained had we used k-independent elastic moduli in the calculation. The other factors enter into the expressions only because the k-dependence of the elastic moduli is taken into account. Note that if we had ignored the k-dependence, the enhancement factors both coming from the large value of κ in extreme type II superconductors, as well as the enhancement factor coming from the mass anisotropy, would have been missed. Below, we shall identify a dimensionless parameter that explicitly shows how dramatic the effect of including non-local elastic moduli really is. 0 and c0 , thus finding To see this, we introduce explicit expressions for c44 11 √ √ 4( 1 m t b 2 − 1) c (8.51) d2 (T ) = + 1 l2 √ √ 2π mab 1 − t 1 − b 1−b

Hence, the Lindemann melting criterion is given by √ √ t 4( 2 − 1) b mab 2 c ≡α + 1 ≥ 2π √ √ mc 1−t 1−b 1−b Here, we have introduced the Ginzburg criterion parameter 2 kB Tc µ0 x 2 = 02 ξ 4π Bc2 ab and t = T /Tc . The dimensionless parameter α is given by 0 B c2 mab 1 α = 2 × 107 c2 mc κ 2 Tc2

(8.52)

(8.53)

(8.54)

This parameter essentially controls the position of the melting line in the (B, T ) phase diagram. In Eq. 8.54 we have again singled out in square brackets what we would have obtained for α had we only used local elastic moduli, the other two factors involving the mass ratio and the Ginzburg–Landau parameter κ appear exclusively due to non-locality in the elastic description of the flux-line lattice. If α is very large, it is clear from Eq. 8.52 that t and b need to be very close to unity for the melting criterion to be satisfied. A reduction in α facilitates a suppression of the melting line below the upper critical field line. In conventional supercon0 = 1 T, T = 10 K, and m /m ≈ 1. If ductors, typically we have κ ≈ 1, Bc2 c c ab

FLL ELASTICITY AND PINNING

223

we set c = 0.1, we have α ≈ 104 . In high-temperature superconductors, on the 0 = 100 T, T = 100 K, and m /m ≈ 100. other hand, we have κ ≈ 100, Bc2 c c ab −1 This gives α ≈ 10 , which is a reduction of nothing less than five orders of magnitude. Notice that the factor in square brackets in the expression for α is about the same in conventional moderate type II superconductors and extreme type II high-temperature superconductors, namely of order 107 c2 . The reduction in α originates exclusively in mass anisotropy and large value of κ. It is therefore an intriguing fact that the enhancement of Tc in high-temperature superconductors compared to conventional low-temperature superconductors in itself does not contribute substantially to suppressing the melting line below the Bc2 line, since the enhancement of Tc is cancelled by the enhancement of 0 . Bc2 However, once non-locality is included and mass anisotropy and large values of κ explicitly come into play, then the melting line is suppressed well below the upper critical field line, and the liquid phase of the flux-line system should be easily experimentally accessible. The one dominant feature which makes this possible, is not first and foremost the mass anisotropy, but rather the large value of the Ginzburg–Landau parameter κ, notice how it is the square root of the mass anisotropy that enters in the melting criterion while it is the square of the Ginzburg–Landau parameter which is relevant. Once more, it is the use of a nonlocal elastic theory of the flux-line lattice which brings out the dependence of both the mass anisotropy and the Ginzburg–Landau parameter. It is in particular the factor 1/κ 2 which brings the melting criterion above in reasonable agreement with experiments [98] for a sensible Lindemann parameter c ≈ 0.4, and the √ factor mab /mc which distinguishes between flux-line lattice melting in YBCO and BSCCO in a manner consistent with experiments [98]. In a deep sense, the sensitivity of the melting criterion to κ reflects the softness of phase-fluctuations of the superconducting order parameter in strong type II superconductors. This is because large values of κ are due to small values of the superfluid density in these compounds. On the other hand, the superfluid density is nothing but a measure of the stiffness of phase fluctuations. We shall have much more to say about such fluctuations in Chapters 9 and 10. In closing this subsection, we emphasize that the above is not a theory of melting of the flux-line lattice, the Lindemann criterion is after all just that, a criterion. It does however provide useful insight into what parameters that determine the position of the melting line, provided the assumption of a first order melting transition is correct. In fact, numerous Monte Carlo simulations and experiments now strongly indicate that this is indeed so. See for instance the work of Hetzel and co-workers [107] for the first demonstration through large-scale Monte Carlo simulations that the Abrikosov vortex lattice melts in a first order melting transition, and the contemporary experimental work of Safar and colleagues [108], showing pronounced hysteresis in resistivity data at what was interpreted as a melting transition of the flux-line lattice.

224 8.5.6

MORE ON THE FLUX-LINE SYSTEM

Modelling non-linear vortex diffusion

The voltage–current characteristics in many high-Tc superconductors are well described by a power-law over many orders of magnitude in the electric field. This has been found directly from transport measurements, and indirectly from the magnetic relaxation. It seems to be the general behaviour for YBCO- and BISCCO-based compounds, as well as for the Hg-based cuprate superconductors. As pointed out before, the power-law E–J-characteristics is most commonly interpreted as a result of thermally activated flux creep with a pinning barrier diverging slowly as the current vanishes, i.e. U (J ) ∝ log(Jc /J ) or U (J ) ∝ (Jc /J )µ , with µ small. Although there is evidence for some curvature in log(E) versus log(J ), the power-law may still serve as a first order approximation and as a model description of the voltage–current characteristic of high temperature superconductors. An analysis of the magnetic relaxation due to a power-law, with static boundary conditions, has been given by Vinokur and Feigel’man [109] and by Gilchrist and van der Beek [110]. Analysis of the AC-losses due to a power-law has been given by Rhyner [111] who considered an AC magnetic field at the surface of a superconducting semi-space. Such a configuration would apply to a real sample when the characteristic penetration depth of the field is small compared to the sample thickness or radius. In the following we consider the situation from zero to full penetration of a cylindrical sample, infinite in the axial direction. The boundary condition is a sinusoidally time-varying magnetic field applied at the surface, and the AC-susceptibility is calculated for different n-values. The numerical results are compared to experimental susceptibility data on a YBCO single crystal. The power-law can be written in dimensionless units as n E J = (8.55) E0 J0 By letting n vary from n = 1 to n = ∞, one covers a full class of cases ranging from ohmic with ρ = E0 /J0 , to the ideal critical state superconductor with a well-defined critical current density Jc = J0 , as illustrated in Figure 8.12. In terms of vortices and vortex dynamics, the limit n = ∞ represents the static critical state in which the vortex density gradient is balanced by the pinning force Fp = J0 B. When n has some finite value, this is equivalent to a relaxation of the critical state, e.g. by thermally activated creep. Now consider an infinitely long cylindrical sample of radius a in an axial magnetic field B = Bac sin(ωt). Maxwell’s equations for the field in the sample in cylindrical coordinates read ∂B 1 ∂ (rE) = − r ∂r ∂t ∂ B = −µ0 J ∂r

(8.56) (8.57)

FLL ELASTICITY AND PINNING

225

1.0

0.8

E/ E0

0.6 n=1 0.4 n=4 0.2 n = 20 0.0 0.0

Figure 8.12

0.2

0.4

0.6 J / J0

0.8

n=∞ 1.0

1.2

Power-law curves for different n-values from Eq. 8.55.

where E and J are azimuthal field and currents, while the B-field is in the axial direction. Next we introduce the dimensionless variables b = B/Bac , ζ = r/a and τ = ωt/2, and aualyze the above equations with respect to the reduced magnetic field b, obtaining n

∂b a n+1 ∂b ∂b 1 ∂ ζ = × sgn ζ ∂ζ ∂ζ δ ∂τ ∂ζ

(8.58)

Here sgn denotes the sign function, and the characteristic length-scale δ represents a generalized penetration depth which can be written as (n−1)

2

(n+1) δ = δcl(n+1) × δBean

(8.59)

where δcl = 2E0 /µ0 ωJ0 is the classical skin depth in the linear limit (n = 1) and δBean = Bac /µ0 J0 is the Bean penetration depth in the critical state (static) limit (n = ∞). The combined depth δ reduces to its appropriate limits δ = δcl and δ = δBean when n = 1 and n = ∞ respectively. The total magnetic flux in a cylindrical sample of radius a is (t) = 2π

a

B(r)r dr,

(8.60)

0

and the complex susceptibility, χ = χ + iχ , is a measure of the first harmonic Fourier components of the spatially averaged flux density,

226

MORE ON THE FLUX-LINE SYSTEM

χ + 1 = χ =

1 2 π a Bac 1 π a 2 Bac

2π

(t) sin ωt d(ωt) ωt=0 2π

(t) cos ωt d(ωt).

(8.61)

ωt=0

The susceptibility can be calculated exactly in both the linear [112] and the critical state [113] limits. In the linear limit one finds 1 + χ = 1 + χ + iχ =

2J1 (ka) kaJ0 (ka)

(8.62)

with k = (1 + i)δcl and J0 (ka) and J1 (ka) denote Bessel functions of zero’th and first order respectively. (For a London superconductor k = 1/λ, which results in loss-free screening currents and χ = 0.) In the limit n = ∞ Eq. 8.58 reduces to the critical state equation, ∂B/∂r = ±µ0 J0 [111]. The susceptibility can then be found by calculating the critical state profiles for a cycle of the surface field and integrating over space and time. This has been done by Clem [113], and the solution reads χ = g1 (x) χ = g2 (x)

(8.63)

where x = Bac /B ∗ = Bac /µ0 J0 a, and g1 (x) and g2 (x) are known polynomials of x and sin−1 (x −1/2 ). In the linear case the susceptibility will depend on the frequency of the AC field, but not on the amplitude, while in the critical state limit the situation is the opposite, a behaviour which is also reflected in δ. Moreover, in the linear limit the response is purely harmonic while for n > 1 the response is anharmonic, resulting in an infinite set of higher order susceptibility terms. The AC susceptibility can be measured over a wide range of penetration, often by varying either the temperature or the static background magnetic field, or both. A maximum in the loss component χ is observed when the penetration depth is of the order of the sample radius, i.e. when 2

(n−1)

(n+1) ∼a δcl(n+1) δBean

(8.64)

or

2E0 µ0 J0 ω

1 (n+1)

Bac µ0 J0

(n−1) (n+1)

∼a

(8.65)

In the exact limits the conditions for a peak maximum in χ is δBean = a and δcl a/1.77, respectively. By taking the differential of Eq. 8.65 we find the

FLL ELASTICITY AND PINNING

227

relation d ln(ω)/d ln(Bac ) = n − 1. These differentials can be found experimentally by measuring the shift in the loss maxima (e.g. with temperature) as a function of both amplitude and frequency of the AC field. Such experiments may therefore be used to obtain the value of n directly. Numerical values of χ and χ were calculated [93] for different values of n by letting the ratio δ/a vary from zero to some large number 1. B(r, t) was found by solving Eq. 8.58 by means of finite differences, and χ and χ were found by integrating in space and time according to Eqs 8.60 and 8.61. A convenient way of plotting susceptibility results is the Cole–Cole plot, in which χ is plotted as a function of χ . We now make a comparison of the numerical results with experimental susceptibility data obtained on a single crystal YBCO. The data used here are only a small subset from a wider experimental study [114]. The crystal sample was cubic with sides 1 mm, and due to such a non-ideal sample shape, a comparison is only of a semi-quantitative nature. The susceptibility was measured as a function of temperature in different DC fields ranging from 1 to 8 T and with an AC field of amplitude 10−4 T, and frequency 121 Hz. The measured χ (T ) and χ (T ) are shown in Figure 8.13 and in a Cole–Cole plot in Figure 8.14. The data collapse in Figure 8.14 shows that the same process is governing the susceptibility behaviour for all curves, occurring at different temperatures 1.0

1 + c′

0.8 0.6 8T

7T

5T

4T

3T

2T

1T

0.4 0.2 0.0

)

c′′

0.2

0.1

0.0 70

75 Temperature (K)

80

85

Figure 8.13 AC susceptibility data on a single crystal YBCO, with Bc at 121 Hz. Applied fields have corresponding values in the upper and lower panel. After Gj¨olmesli [93] and Karkut et al. [103].

228

MORE ON THE FLUX-LINE SYSTEM

c′′

0.3

n=1

0.2 n→∞ 0.1 B||c Bac = 10−4 T DC fields 1, 2, 3, 4, 5, 7, 8 T

0.0 0.0

0.2

0.4

0.6

0.8

1.0

1 + c′

Figure 8.14 Cole–Cole plot of the susceptibility data shown in Figure 8.13. The plotted data follow the n = 1 curve at the highest values of 1 + χ , corresponding to the highest temperatures. But at some point they switch over to a non-linear domain with n 1. This is the freezing point of the lattice. Data Aualysis: Ref [93] from Karkut et al. [103].

determined by the DC field. In other words, the susceptibility can be written as a function of a single variable which changes monotonically with temperature and field. At large penetration, χ + 1 1 the data follow closely the linear curve n = 1. Then at some particular value 1 + χ 0.95 and χ 0.2, the curve makes a small jump into the non-linear region with n > 1. Moreover, the linearnonlinear jump is rather sharp, occurring over less than 0.2 K, indicative of a phase transition of the vortex state, possibly from a vortex liquid to a vortex glass [93]. We conclude that the non-linear diffusion due to a power-law E–J-characteristic gives a generalized penetration depth δ which reduces to the classic skindepth and to the Bean penetration depth in the appropriate limits. The peak shift in χ with respect to amplitude and frequency can be used to determine the value of the exponent n. The non-linear diffusion equation was solved numerically and the complex magnetic susceptibility was calculated, in order to be compared to experimental data. By plotting χ versus χ the experimental data collapse occurred, with indications of a sharp transition from a vortex liquid state with linear dynamics into a state of non-linear dynamics, possibly a vortex glass.

8.6 Flux-line entry at Bc1 : thermodynamic and geometric restrictions 8.6.1

The critical field Bc1

The mixed state of a superconductor is one where the superfluid phase coexists with the flux-line lattice, a vortex glass, or with the flux-line liquid. When

THERMODYNAMIC AND GEOMETRIC RESTRICTIONS

229

an applied magnetic field is increased from zero, the superconductor is first in the Meissner phase, with complete shielding. At a certain value of the applied field Hc1 = µ10 Bc1 it becomes energetically favourable to have flux-lines created near the surface, and for these to penetrate the body of the superconductor. A thermodynamic analysis to determine Hc1 starts by writing down the Gibbs free energy G when n vortices per area are inside and far apart so that their mutual interaction can be neglected. We now have: G = nF − BH

(8.66)

where F is the vortex line energy previously determined in Chapter 6. This is an excellent approximation very near Hc1 where in principle even a single flux-line can penetrate alone. Since the average field is B = n0 , we make this substitution, and find F −H (8.67) G=B 0 The lowest value for G as long as the expression in the parenthesis is positive, is G = 0, corresponding to B = 0, as expected for a system in the Meissner phase. A simultaneously positive value of the expression in parenthesis signifies stability against vortex entrance, consistent with Meissner screening. However, when the expression in the parenthesis is negative, i.e. when H > F /0 , G can be lowered below the Meissner-state value G = 0 by B = 0. A finite B means that flux has entered, and that the energy G is lower than in the Meissner state, which is consistent with instability towards flux penetration. The critical field at which the instability occurs clearly is F 0 λ Bc1 = +ε (8.68) = ln 0 ξ 4π λ2 as derived before.

8.6.2

The Bean–Livingston barrier

When a vortex is created near the surface of a superconductor in the Meissner state two opposing forces act on it. The screening currents create a Lorentz force normal to a flat surface, attempting to move the vortex into the material according to fx,L = 0 jy

(8.69)

230

MORE ON THE FLUX-LINE SYSTEM

as shown in Eq. 6.110. We can write this as fx,L = 0

H −x e λ λ

(8.70)

reflecting the decay of the screening current into the superconductor. The second force is the image force attracting the vortex to the surface. Using the result in Eq. 6.106 where the distance between the vortex and its image is 2x, the interaction energy which is now negative, becomes U12

20 2x =− K0 λ 2π µ0 λ2

Taking the derivative, and making use of the relation these Bessel functions the resulting image force is fx,im

(8.71) d dx K0 (x)

= −K1 (x) for

20 2x =− K1 3 λ 2π µ0 λ

(8.72)

We now evaluate the force at x = ξ , since this is as close as we can approach the surface using the vortex model. The sum of opposing forces is fx = fx,L + fx,im

20 H −ξ/λ 2ξ = 0 e − K1 3 λ λ 2π λ

(8.73)

The total force is zero at field ξ 0 2ξ eλ K1 Hsb = 2 λ 2π µ0 λ

(8.74)

which is called the surface barrier field for obvious reasons. Furthermore, using the property of the Bessel function lim K1 (x) =

x→0

1 x

(8.75)

for ξ λ one finds lim Hsb =

1 0 = √ Hc 4π µ0 ξ λ 2

(8.76)

This is the surface barrier field at which the net force against flux entry is zero. This barrier field has important implications. As an example, in microwave applications where flux entry would represent a loss factor it is important that Hc in type II superconductors like Nb is much greater than Hc1 . To take full advantage of this situation the surface should be smooth, at least on the scale of λ,

THERMODYNAMIC AND GEOMETRIC RESTRICTIONS

231

∆G

H > Hsb 0

x

(c)

Figure 8.15 Sketch of the Gibbs energy from which the two opposing forces active in the Bean–Livingston barrier are derived. At H = Hsb the slope of the curve at the origin will be zero, providing free entry of flux.

since the force found above is calculated under the assumption of a flat surface. Figure 8.15 shows how the Bean–Livingston barrier [115] can be viewed and understood to operate. In most real situations sample shapes and surface conditions will allow flux entry of static fields near Hc1 . Normally Hsb will be the entry field only when special precautions are taken.

232 8.6.3

MORE ON THE FLUX-LINE SYSTEM

Geometric barriers

The concept of a geometric barrier was introduced by Zeldov and coworkers [116] and discussed also extensively by Brandt [117]. This is a shape dependent barrier which can be explained qualitatively by reference to the sketch in Figure 8.16. A sample S of thickness d, with sharp corners is placed in a magnetic field. Near the sharp corners the local field is enhanced considerably compared to the applied field H , and therefore penetrates first at these points. This undermines the opposing forces due to the Bean–Livingston barrier. However, for the flux line to enter, the length of flux line Lf as seen in the figure, has to be considerably longer than just Ls = d, which would be the length corresponding to penetration along the flat outer surface. If we approximate the length Lf by a half circle at the point when it just leaves the surface we estimate that Lf ∼ π d2 . The flux line therefore was stretched by an amount L = Lf − Ls ≈ (π − 2)

d d ∼ 2 2

(8.77)

compared to the length it would have in the centre of the specimen. Notice also that Figure 8.16 indicates that a vortex line has jumped directly to the centre of the sample once it entered. This is because here again the length inside the sample is only equal to d. Alternatively we may say that the flux line was driven to the centre by the Meissner currents discussed before. Hence it is energetically advantageous to travel all the way to the centre in case of no pinning. The energy cost of creating the flux line near the surface is therefore raised by ∼50% due to sample geometry in this simple estimate. Consequently we may expect the flux entry field to be raised by an amount which is of the same order of magnitude as Hc1 itself. Obviously, the effect is strongly shape dependent, hence its name. In case of elliptical crossection it may be shown that there is no geometrical barrier.

d 2 S

Lf

d

d 2

Figure 8.16

Sketch illustrating flux entry in the presence of a geometrical barrier.

CRITICAL CURRENT ISSUES

233

This effect also has an associated hysteresis, since there is no corresponding barrier against flux exit. The geometric barrier therefore is recognized experimentally by hysteresis in magnetisation experiments even in the absence of pinning. The additional effect of pinning was discussed by Brandt [117].

8.7 Critical current issues 8.7.1

Critical current in the Meissner state

According to the London equation there is a relation between the supercurrent density and the magnetic field at any point in the superconductor. In the Meissner phase, due to screening, the current and field can only penetrate to a depth measured by λ. Due to the correspondence between J and H it does not matter whether J is the sum of a transport current and a screening current. Experiments show that there is a critical current density Jc above which screening and superconductivity break down. Due to the equivalence of transport current and screening current it is to be expected that superconductivity breaks down when the total current density–the sum of transport and screening current–exceeds the critical current density Jc . The famous Silsbee hypothesis states the converse: A superconductor looses its state of zero resistance when the total magnetic field strength due to transport current and the applied field exceeds the critical field strength Hc . Mainly because of large variations in charge density, λ may vary by an order of magnitude, from ≈15 nm in good polyvalent metals to 150 nm in YBCO. What we have then, in a surface layer of thickness 15–150 nm, is a decaying screening current and an associated magnetic field which are locally related in the London approximation. With a field H created by a current J along a cylindrical rod, the H -field is circular in the plane normal to the rod with radius ∂ a. We get ∂r Hθ (r) = J from Maxwell’s equations ∇ × H = J , leading to J =

Hθ (a) λ

(8.78)

where Hθ (a) is the value of Hθ at the surface. Now, if we allow J to reach Jc , this corresponds to Hθ (a) = Hc . In other words: Jc =

Hc λ

(8.79)

This is the relation which holds in the Meissner state, and therefore is valid in type I as well as type II superconductors. It is worth noting that this rule is very similar to the one we derived for Jc in the Bean critical state. In that case Jc was also given by a field divided by a length, namely M/d. Since H and

234

MORE ON THE FLUX-LINE SYSTEM

M are in the same units, what these expressions have in common, is that the gradient of the field gives the critical current. Does the relation Jc = Hc /λ reconcile with a calculation based on Ampere’s law? If the superconducting rod is of radius a, and the total current is I , the field at the surface, Hθ (a) is given by I = 2π aHθ (a)

(8.80)

or, if the current is strong enough to reach Hc : Ic = 2π aHc

(8.81)

Equation 8.81 looks different from Eq. 8.78. But for real comparison we have to introduce the current density, J = I /Aeff = I /2π aλ;

I = 2π aλJ

(8.82)

Here, the effective area was written as Aeff = 2π aλ, since a λ. We now find 2π aλJc = 2π aHc , which leads to Jc =

Hc λ

(8.83)

and we have recovered the answer we had before, in Eq. 8.79.

8.7.2

Depairing critical current

Calculations of critical current density can be carried out using Ginzburg–Landau as well as BCS theory. Except for a numerical factor they come out with essentially the same result: Jc ≈

Hc λ

In Ginzburg–Landau-theory the exact result is √ Hc 2 2 Hc Jc = √ 0.54 λ 3 3 λ

(8.84)

(8.85)

In BCS theory the kinetic energy added to the system by turning on a current J , has to be compared to the energy gained by forming the Cooper-pairs. When the kinetic energy equals the pair condensation energy we have the critical current

CRITICAL CURRENT ISSUES

235

density. The condensation energy can be expressed on the basis of thermodynamics as ( 12 µ0 )Hc2 , and from BCS theory as 12 N (0)2 , where N (0) is the normal density of states at the Fermi level, and is the BCS energy gap. This would give Hc2 = µ0 N (0)2 Using Jc = Hλc we find Jc = nomenology and BCS.

(8.86)

√

µ0 N (0)2 λ

as a mixed expression between phe-

Example Measurements in a 1-mm diameter wire have given critical current at 0 K: Ic = 75 A. With a = 0.5 mm, λ = 5.1 × 10−6 cm; Jc (0) = 2πIcaλ = 4.7 × 107 A/cm2 . A simple estimate of Jc based on the basic formula Jc = Hc /λ gives typically, with µ0 Hc ≈ 0.1 T and λ ≈ 100 nm: Jc =

Bc = 1012 A/m2 µ0 λ

Often such values are quoted in A/cm2 , in this case: Jc ≈ 108 A/cm2 . This is the maximum ideal current density the superconductor can sustain under any circumstance. There are many reasons why one does not reach this value in practical cases. The most important obstacles are typically flux motion and grain boundary problems, particularly in high-Tc cuprates. Yet, often one finds that real materials can come within a factor of 2–3 of this pair-breaking current.

8.7.3

Reduction of Jc at grain boundaries

So far we have discussed the idealized situation as far as critical current density Jc is concerned. These considerations give a good idea of what maximum of critical current density we can expect in a superconductor. However, there are many mechanisms by which Jc may be reduced, even substantially. Of course, if in a granular material the grains do not join together well, for instance due to a transition layer of different composition between the grains, this has a strongly derogative effect. High-Tc materials are known for their short coherence length ξ . In a transition layer the wavefunction ψ may be depressed over a distance ξ without bridging properly across the boundary, in which case little current can pass across the interface, except by tunnelling which may be very weak. In addition, due to the dx 2 −y 2 character of the wavefunction in high-Tc cuprates several misorientation effects at the microscopic level are possible, each representing an obstacle to current transport, and hence to reduction of Jc [118]. These mechanisms are illustrated in Figure 8.17. Referring to this figure

MORE ON THE FLUX-LINE SYSTEM

+

+

−

|∆|

x

x

+

−

−

+

+

−

(b)

+ −

Large Jc

j = ∆j

+

−

−

+

Small Jc

+ −

− +

I

+ −

j = ∆j + p

+

− +

+

− +

−

Position

−

(a)

(c)

+

−

− +

−

236

− +

Figure 8.17 Illustration of different mechanisms by which Jc may be reduced at grain boundaries in high-Tc dx 2 −y 2 type superconductors. After Hilgenkamp and Mannhart [118].

the mechanisms are from top down: In Figure 8.17a two adjoining grains are differently oriented, causing a depression of the wavefunction over a distance ξ due to frustration caused by misorientation of CuO2 -planes. In Figure 8.17b one sees a case of alignment of the lobes of the dx 2 −y 2 function allowing a high Jc , and a misalignment causing a small Jc . Finally in Figure 8.17c a faceted grain boundary facilitates the current in one channel, and opposes it in the other. The result is lower Jc .

8.7.4

Relaxation of magnetic moment and the irreversibility line

Soon after the discovery of high-Tc superconductors by Bednorz and M¨uller, the IBM team also found an important difference between low-Tc and high-Tc

CRITICAL CURRENT ISSUES

237

superconductors when exposed to a magnetic field [119]. Essentially the discovery was that in a broad temperature region below Tc (H ) the superconducting properties were reversible, corresponding to critical current Jc = 0. Only below a much lower temperature Tirr (H ) did the behaviour shift to irreversible, corresponding to Jc = 0. This created a dividing line in the (H, T )-plane, later called the irreversibility line. Furthermore, this line was not a fixed line, determined once and for all for a given material. Rather, in a given sample the experimentally determined location of the irreversibility line Tirr (H ) depended on the characteristic measuring time of the experiment, and in samples of the same nominal composition it would depend also on sample history. These effects are present to some extent in all superconductors, but to a far less degree in low-Tc than in the cuprate high-Tc materials. What is going on can briefly be described as follows: After a certain arrangement of vortices has been established, typically after application of a magnetic field, and subsequent removal of the field to observe the vortex dynamics, vortices will leak out of the sample, leaving the most shallow pinning sites first. As time passes, the depinning process goes slower since the vortices have to climb higher and higher barriers in order to leave their pinning sites. The process goes on indefinitely, all the time at a slower rate. This effect is most clearly demonstrated by observing the decay of the magnetic moment m(t) originally present as mi at a time ti when the field is switched off, and then monitoring the relaxation process over decades of time. The observed time-dependent magnetization is typically such that the magnetic moment, when plotted versus time on a double logarithmic scale, decays linearly, i.e. the functional dependence is a power law. Due to the relatively strong decay observed in high-Tc materials the behavior in these was termed ‘giant flux creep’ [120]. In Figure 8.18 we give an example of magnetization decay measurements at several temperatures in a wide range, observed in a thin film of Bi2223. The decay was monitored by a squid, located in a superconducting chamber, shielded against outside signals except for the signal picked up by a gardiometer coil surrounding the sample. Measurements started immediately after switching off a 10 mT field from a small solenoid surrounding the sample, starting the flux leakage from the sample [121]. Below 50 K the decay is seen to be quite linear in the double logarithmic plot over 4 decades in time, except for a small deviation in the long time limit (t ≥ 100 s) at the highest temperatures. The dominating decay behaviour may be expressed simply as −S t m = mi (8.87) ti where the exponent S is S = ∂(ln m)/∂(ln t). For temperatures T ≥ 50 K a crossover to faster dynamics is apparent, as would be expected in a crossover to vortex liquid. In this range the data are relatively noisy, due to the low magnetic moment.

238

MORE ON THE FLUX-LINE SYSTEM 10 20 K

m (a.u.)

1

10−1 47.5 K 55 K 10−2 50 K 60 K 10−3 10−1

1

102

10

103

104

t (s)

Figure 8.18 Relaxing irreversible magnetic moment in a Bi2223 film after a field step of −10 mT is applied at different temperatures. The flux is leaving the sample, and shielding currents decay proportionally to the decrease of the magnetic moment. The temperatures are from top to bottom: 20, 25, 30, 35, 37.5, 40, 42.5, 45, 47.5, 50, 55, and 60 K. The c-axis oriented thin film with Tc = 97 K was grown by metalorganic chemical vapor deposition (MOCVD) by Endo and coworkers at the Electrotechnical Laboratory in Japan. The measurements are by Tuset et al. [122].

The above experiment makes very clear why the so-called irreversibility line depends on the timescale of the experiment: The longer timescale is allowed in a given experiment, the more of the magnetization decay is integrated into the observation. To illustrate the consequences of this, we refer to Figure 8.19 where the position of the peak in the loss component of the dynamic susceptibility was measured as a function of temperature at different frequencies and field directions. The excitation field was parallel to the static magnetic field. Figure 8.19 shows the irreversibility line as measured by AC susceptibility in YBCO crystal at a range of frequencies. Here the line is determined as the locus of points where the loss peak in the imaginary part of the susceptibility χ appears in the (H, T )-plane. We clearly see the effect of changing the time-scale of the experiment: With increasing frequency the Tirr (H ) line moves up in temperature. The question is now how this line can be described quantitatively, or at least semiquantitatively. A crude argument which gives some insight, but without taking into account the collective effects we discussed before, goes as follows: Assuming that pinning occurs at pin points of volume Vc , the energy gained by having a flux line pass through this volume is equal to the condensation energy U = 12 µ0 Hc2 (T )Vc

(8.88)

CRITICAL CURRENT ISSUES

8

239

H⊥c H||c

m0 Hdc (T)

6

4

f (Hz)

2

12.1 121 1.21 k 12.1 k 121 k

0 70

75

(a)

80 T (K)

85

90

0T

90

0.4 T 1.5 T T (K)

85

4T

80

6T 75

8T

10 (b)

H||c 102

103 f (Hz)

104

105

Figure 8.19 Irreversibility line measurements (a) at various frequencies in YBCO with H c-axis and H ⊥c-axis. The bottom, (b), figure shows how the irreversibility line with H c is shifted to higher temperature with increasing frequency. After Karkut et al. [103].

Assume further that Vc may be written as a02 ξ(T ) where a02 is the correlation area in the transverse direction given by the flux-line lattice constant. The critical field has almost linear temperature dependence in the field range we are discussing 1 in high-Tc materials, i.e. Hc ∝ (1 − T /Tc )1 and ξ(T ) ∝ (1 − T /Tc )− 2 in the mean field approximation, as in Ginzburg–Landau theory. The result is, when inserting the expression for a0 = 1.075(0 /B)1/2 that

240

MORE ON THE FLUX-LINE SYSTEM

U=

U0 1 − B

T Tc

n ;

n = 1.5

(8.89)

In order to test this line of thinking, Sagdahl [123] analysed a relaxation model for the permeability, writing the two components on the usual Debye form 1 1 + (ωτ )2 ωτ µ = 1 + (ωτ )2 µ =

(8.90) (8.91)

The relaxation time is expected to be τ = a/Rl where l is the typical jump distance, R is the flux jump rate and a is a macroscopic distance describing the total depth of penetration of flux. We rewrite this as τ = (a/f0 l) exp(U/kB T )

(8.92)

Here f0 is an attempt frequency, and U is the pinning potential already introduced. The maximum in µ occurs at ωτ = 1, setting the criterion for B and T to be on the irreversibility line as B ∗ and T ∗ at a selected frequency and AC amplitude. Using this criterion we arrive at the following condition for the irreversibility line: U = − ln(ωτ0 ) kB T ∗

(8.93)

where τ0 = (a/f0 l). Next, inserting the expression for U arrived at previously we find that Eq. 8.93 converts to U0 (1 − T ∗ /Tc )n /kB T ∗ B ∗ = − ln(ωτ0 )

(8.94)

where Aj is a parameter which we leave undetermined. Finally, we rewrite Eq. 8.94 as B ∗ = C(ω)(1 − T ∗ /Tc )n /T ∗

(8.95)

where C(ω) = −(U0 /kB ) ln(ωτ0 ). This constitutes an expression for the irreversibility line in the present analysis. In [123] this expression was tested, and found to agree with experiments, with n = 1.5 at the fields above 1.5 T, while n = 1 below. Furthermore, in fitting the expression the parameter Tc had to be taken with a value well below the zero-field value Tc (0). This shows that the model does not apply in the vicinity of Tc (0). The irreversibility line was found

CRITICAL CURRENT ISSUES

241

to be almost flat over several degrees below Tc (0). In other words very weak irreversibility was found in that temperature interval. Clearly pinning very close to Tc (0) at very low fields is quite different from that at high fields. This can at least partly be argued to be caused by twin boundaries taking a more prominent role as pinning centres when the flux line density is low, in which case the flux line dynamics may be altered substantially. It turns out that Eq. 8.89 agrees surprisingly well with experiments, considering the simplicity of the model, and the complexity of the real problem. Figure 8.20 gives an example of such overall agreement. Part of the reason should be ascribed to the fact that point pinning is important in YBCO due to the presence of oxygen vacancies as pinning sites. In the vicinity of the melting line the softening of the FLL strengthens the role of individual pinning. The irreversibility lines of high-Tc compounds are located well below the Hc2 line, and the difference is larger the more 2D-character the material possesses. This has represented a great challenge in the search for material processing methods suitable for attainment of high-Jc at reasonably elevated temperatures and in high magnetic fields. It is natural to ask how the irreversibility line is related to the melting line. The answer is that these are of different origin and largely independent, but not unrelated. The irreversibility line is determined for the decay of magnetisation current, in other words governed by flux line dynamics, while the melting line is a thermodynamic line and as such an equilibrium phase boundary, fixed in the (H, T )-plane for a given piece of material. The position of the melting line should be expected to depend somewhat on pinning 8

B* (T)

6

4

2

0

65

70

75

80

85

90

T* (K)

Figure 8.20 The irreversibility line B ∗ (T∗ ) in the field range 0 to 7.5 T (H c) determined from AC permeability measurements on an YBCO single crystal with f = 121 Hz and Bac = 3 × 10−4 . The solid and dashed lines represent theoretical fits using Eq. 8.95, with exponents n = 1.5 for fields higher than 1.5 T and n = 1 for fields lower than 1.5 T. After Sagdahl [123].

242

MORE ON THE FLUX-LINE SYSTEM

properties of the material. However, melting can only be observed in materials with relatively low density of pins. In pin-free materials each superconductor should possess a unique melting line. The irreversibility line is highly anisotropy dependent, as is the melting line as was shown in Figure 8.19 in two directions in YBCO. Clearly, both flux line dynamics and melting properties should be expected to be different in the two cases: When flux lines are along the c-axis they are free to displace sideways in two directions, while in the ab-plane they are packed parallel between superconducting CuO2 sheets and can only move sideways parallel to the ab-plane. This means that a thermal energy kB T has much less influence on the configuration of flux lines when the field is in the ab-plane than when it is along the c-axis. Therefore it is much harder to melt the FLL with the field in the ab-plane than along the c-axis. The melting line for field in the ab-plane is therefore much higher than with field along the c-axis. The statement made above that the irreversibility lines are independent but not unrelated can now be given more content: We see from Figure 8.19 that the irreversibility line is much steeper and higher up in temperature with field in the ab-plane than when it is in the c-direction. In this sense they are clearly related. But the irreversibility lines move as a function of frequency of the AC field, in this sense they are independent. The relationship between the two types of lines is due to the fact that time constants near phase boundaries depend stronger on temperature relative to T (H ) and tend to diverge at the phase boundary. A wide range of time constants is therefore available in the vicinity of the Tm -line. As it turns out the experimentally accessible time constants are in that same range. Hence the irreversibility line will appear not too far away from the Tm -line. A sketch of this is given in Figure 8.21.

8.7.5

How can Jc be increased?

The irreversibility line problem in high-Tc materials has been a serious obstacle against the development of wires and cables for many kinds of superconductor B Tm

Tirr

Bc2

Reversible

Irreversible Tc

T

Figure 8.21 Sketch of the irreversibility line Tirr and the melting line Tm .

243

CRITICAL CURRENT ISSUES

applications. Huge research efforts have been made to overcome it. The improvements which have been achieved are very impressive. Compared to the critical current densities obtained in the early stages of high-Tc research these systematic efforts have led to increased critical current density by many orders of magnitude. For a good example we refer to the topical contribution by Muralidhar and Murakami (Section 13.4) on a modification of YBCO-type material, where extremely strong magnetic fields may be stored in bulk material. The highest fields reached are so strong as to challenge the physical strength of the material itself due to the strong forces that the pinned vortex lattice causes on the structure. In the following we give some some more examples of results where the improvements are substantial. The first example is from the work of Krusin-Elbaum and coworkers [124]. In this case the mercury-based superconductor HgBa2 Ca2 Cu2 O6+δ , also referred to as Hg-1212, was subjected to 0.8 GeV proton bombardment which induced fission processes in Hg, leaving tracks in the material. These tracks created what is often referred to as ‘columnar defects’ in a ‘pinning landscape’ which reduced the vortex motion (creep) substantially. Figure 8.22 shows the resulting improvements in critical current density, as well as a big shift of the irreversibility line,

1.0 0.8

−0.1 T −1.0 T −2.0 T

R/RN

10

5

1.52 × 1017 cm−2

4

mo H( T)

J (106 A/cm2)

Unirr

0.4 0.2

1

Hg-1212

0.6

mo H = 2 T Irr

0.0

3

80 ∆Tirr

2

100 T (K)

0T 120

Irradiated

0.1 Unirradiated

1 Unirradiated

Hg-1212 0.01

0 0

20

40

60 T(K)

80

100

60

70

80

90

100 110 120

T(K)

Figure 8.22 The effect of proton bombardment at 0.8 GeV, with resulting fission fragments creating columnar defects in superconducting HgBa2 CaCu2 O6+δ . On the left the improvement of critical current is shown at various fields, with open and closed symbols showing the results before and after irradiation, respectively. The proton fluence of the irradiation was 1.52 × 1017 cm−2 . The figure on the right shows the corresponding shift of the irreversibility line, with the insert giving simultaneous resistivity changes [124].

MORE ON THE FLUX-LINE SYSTEM

500 nm

244

5 4 3

0

1

2

2 3

1

4

(a)

5 −H4

−H3

−H2 −H1

0

µm H1

H2

H3

H4

3 Pb/Ge 2

With antidot lattice

M(10−4 emu)

1 Without antidot lattice 0

−1

−2 T=6K −3 (b)

−96

−72

−48

−24

0 H(G)

24

48

72

96

˚ film with a square lattice of subFigure 8.23 (a) An AFM picture of a single Pb (500 A) micron antidots (periods d = 1 µm, radius r = 0.2 µm. (b) Magnetization loop M(H ) at ˚ ˚ 2 multilayers with and without the triangular antiT = 6 K of a (Pb (100 A))/(Ge (50 A)) dot lattice (d = 1 µm). The solid line is a fit following the logarithmic dependence of the magnetization between the matching fields Hm and Hm+1 . The dashed line is demonstrating the validity of the linear behaviour of M(Hm ). The loops were measured for M > 0 and symmetrized for clarity for M < 0 [125].

CRITICAL CURRENT ISSUES

Jc (106A/m2)

1.0

245

TP

0.5

TP1 0

Figure 8.24

3.5

4.0 Temperature (K)

4.5

Tc

4.8

The ‘peak effect’ demonstrated in NbSe2 [126].

moving it up by about 20 K at the highest field employed [124]. Since the irreversibility line is a borderline between regions where Jc = 0 and Jc = 0 this means that a much larger area of the (H, T )-plane is potentially useful after the irradiation. A different strategy was followed by Fossheim and coworkers [127] who were able to embed carbon nanotubes into Bi2 Sr2 CaCu2 O8+x . Due to the small diameter of the nanotubes, in the 10 nm range, they are suitable as columnar defects and can provide strong pinning. The next example, Figure 8.23 is from a thin film superconductor by V. Moshchalkov and coworkers [125]. In this case a thin film superconductor was modified by making a large number of holes, “antidots”, in the films, creating a regular lattice of holes. Each hole is capable of pinning one or more vortices. The measurements shown are magnetization vs. applied field in both the positive and the negative directions. The narrow inner curve shows, for comparison, the magnetization before making the holes in the film. The magnetization is very low, corresponding to a very low critical current density. In the upper curve, corresponding to measurements in the film with pinning arrays, the situation has changed dramatically: As the magnetic field is turned on, one finds a magnetization which is orders of magnitude higher than in the intrinsic case. In addition, some structure appears. The first peak corresponds to a matching of the number of holes with the number of vortices available for pinning, at the so-called ‘matching field Bφ ’. On further increase of the applied field, new matching conditions are found, representing two, and three vortices per hole, etc. A number of different geometries and variations in pinning strategies have been investigated. An interesting effect which arises in many superconductors when the temperature approaches Tc from below, is the appearance of a sharp maximum in the critical current density just before it goes to zero at Tc . This is the so-called ‘peak effect’, and is ascribed to collective pinning. It arises because the flux

246

MORE ON THE FLUX-LINE SYSTEM

line system softens on approaching Tc , as can be seen from the analysis we have done of the elastic properties of the FLL previously in this chapter. Since a softer vortex lattice is able to adjust more easily to the random positions of pinning centra, the vortices are now better pinned. However, as Tc is approached further, the Cooper pair density and the wavefunction diminish even more, and pinning vanishes altogether. Jc then must go to zero. The example given in Figure 8.24 is from Kes and coworkers on NbSe2 [126], with Tc = 7.1 K. Three characteristic temperatures are indicated in the figure, representing the minimum of critical current density reached below the peak temperature, the position of the maximum, and finally Tc where Jc goes to zero.

PART II

Advanced Topics

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

9 Two-dimensional Superconductivity. Vortex-pair Unbinding 9.1 Introduction In this chapter, we will go through the case of how superfluidity is destroyed in thin film superconductors or thin films of superfluids with a scalar order parameter. The starting point is the Ginzburg–Landau theory, now applied to two-dimensional systems. In this case, the distinction between superconductors (charged condensates) and superfluids (neutral condensates) vanishes. The reason is that in the case of superconductors, the effective London penetration depth is given by the bulk penetration depth λ and the thickness of the film d as follows λ λeff = λ d mq λ= µ0 ns q 2

(9.1)

where q is the charge of the carriers in the superconducting state, mq their mass, and ns their number density. We may thus write the effective penetration depth in the form mq λeff = . (9.2) 2 µ0 ns qeff Thus, when d → 0, this is equivalent to letting qeff → 0, and we thus effectively have a neutral condensate in this case. The physics of this is simply that in the case of an infinitely thin film λeff → ∞, thus precluding gauge-field fluctuations in the interior of the film. We therefore can ignore the vector potential A as an independent fluctuating variable in the action. In the presence of an external Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

250

TWO-DIMENSIONAL SUPERCONDUCTIVITY

field inducing vortices in the thin film, this would simply enter as appropriately twisted, but non-fluctuating, boundary conditions on the sample. Here, we shall for the moment ignore an externally imposed magnetic field.

9.2 Ginzburg–Landau description The Ginzburg–Landau theory in the two-dimensional case, regardless of the charge of the condensate, takes the form Fs (r, T ) = Fn (r, T ) + α |ψ|2 +

β 2 |ψ|4 + |∇ψ|2 2 2m

(9.3)

where ψ(r) = |ψ(r)|eiθ (r) is the complex scalar order parameter of the condensate. For the subsequent discussion, we will find it convenient to regularize this continuum theory by placing it on a lattice, i.e. we introduce a short distance cutoff in the problem, which in physical terms is taken to be of the order of the coherence length ξ . Moreover, we ignore the normal state free energy, measuring free energies in the superconducting state relative to the normal state. Such a lattice regularization is tantamount to introducing finite differences instead of gradients everywhere. Also, the order parameter will now be defined on lattice sites with labels given by the set {i}, which runs through 1, . . . , N = L2 , where L is the length of the sample in each direction. Ultimately, the L → ∞ limit needs to be taken. Note that in the end, it is really the continuum version of the Ginzburg– Landau theory we will be interested in, more precisely the continuum version at the critical point of the theory. When a phase transition happens to be a critical phenomenon, this means that there is a diverging length scale (ξ ) in the problem. We shall identify this length in the present chapter. Under such circumstances, the physics we are interested in are critical fluctuations on a length scale set by the diverging length. Hence, the lattice constant in our regularized theory is an irrelevant variable and the physics at the critical point of the lattice superconductor is expected to capture the physics of the continuum theory. Lattice regularizations, however, do require a bit of caution whenever they are applied, since it is not in any way obvious that such discretizations of space are not singular perturbations. Moreover, even if the lattice constant ‘disappears’ from the problem in this case, it does not necessarily leave the scene quitely, but may endow the system with an exponent η. The lattice regularized Ginzburg–Landau theory for a two-dimensional lattice superconductor takes the form 2 β 2 Dµ ψ Fs = α |ψi |2 + |ψi |4 + 2 2m µ=x,y i

Dµ ψ = ψi+µ − ψi

(9.4)

CRITICAL FLUCTUATIONS IN TWO-DIMENSIONAL SUPERFLUIDS

251

where ψi+µ is the order parameter evaluated at a lattice site which is shifted one lattice constant (set equal to unity) in direction µ. Expressing the above in terms of the amplitude and phase of the order parameter we find 2α(T ) 2 4 ψ + ψ Fs = J1 i i α(0) i ξµ2 + |ψi+µ ||ψi |(1 − cos(µ θ )) (9.5) 2 a µ=x,y µ where µ θ = θi+µ − θi J1 = 2α(0)β ψi ψi = α(0) β

(9.6)

9.3 Critical fluctuations in two-dimensional superfluids In principle, this formulation allows for both amplitude and phase fluctuations. However, we will ignore the amplitude fluctuations in the following. We simply set the amplitudes |ψi | = 1. This is very much like what we do in spin models where the length of the spin is taken to be frozen, and only the direction of the spin is taken to be important in investigating whether the magnet orders or not. Although we will not go into the details here, it is by now very well established that phase-only approximation to the fluctuations in ψi is on solid ground. This means that we can write the energy for latticized two-dimensional superconductor/superfluid on the form 1 − cos(µ θ ) Fs = J0 i,µ

J0 = J1

ξµ2 aµ2

(9.7)

when all constant terms are ignored. This is the well-known two-dimensional XY-model. It may be recast slightly into the following form (in addition, we introduce H as the Hamiltonian instead of Fs ) 1 − cos(θi − θj ) (9.8) H = J0 i,j

Here, i, j denotes nearest neighbour coupling, which emerges naturally by putting gradient terms in the Ginzburg–Landau theory on the lattice, and i runs

252

TWO-DIMENSIONAL SUPERCONDUCTIVITY

over all lattice sites in the problem. The entire Ginzburg–Landau theory is now expressed solely in terms of the phase of the superconducting order parameter, and the resulting statistical mechanics is entirely governed by phase fluctuations. Phase differences between lattice points are expressed as lattice gradients of the phase. Let us for simplicity denote them by ∇θ , which is a vector. A vector may always be split into a transverse part and a longitudinal part. The transverse part is divergence free, the longitudinal part is curl-free, hence we have ∇ · (∇θ )T = 0, ∇ × (∇θ )L = 0

(9.9)

Consider first this model at low temperatures. We then expect that thermally generated fluctuations in θ are, in some sense, small. The situation we have in mind in this case is depicted in Figure (9.1). This means that we can expand the cosine-term to leading order in the phasegradients, arriving at H=

J0 (θi − θj )2 2

(9.10)

i,j

where J0 now can be identified as a bare spin-wave stiffness parameter. The correlation function that probes the phase-coherence in the system is (r) = eiθi e−iθj

(9.11)

Figure 9.1 Spin-wave configurations, or equivalently longitudinal phase-fluctuations, in the two-dimensional XY -model on a square lattice. The arrows indicate values of θi , analogous to an XY spin direction, on the lattice points where the order parameter is defined.

CRITICAL FLUCTUATIONS IN TWO-DIMENSIONAL SUPERFLUIDS

253

where r = i − j. At low temperatures, the statistical average can safely be computed using the Hamiltonian Eq. 9.10. Since this is quadratic in the phase fluctuations, the average may be evaluated exactly. First of all, this leads to the simplification that (r) = e−(θ (r−θ (0))

2 /2

= e−(θ (r)−θ (0))

θ (0)

(9.12)

Here, r is the lattice vector between points i and j . In the last equality above, we have used the fact that the system is assumed to be translationally invariant. This means that we are neglecting effects of disorder in what follows. Thus, we are faced with the task of computing the correlation function G(r) ≡ [θ (r) − θ (0)]θ (0)

(9.13)

The computation of this quantity is facilitated by the equipartition theorem applied to Eq. 9.10, expressed in terms of the Fourier-modes θq of the phasefluctuations as follows H=

J0 2 q θq θ−q 2 q

(9.14)

This is quadratic in each of the Fourier modes and thus we have, by the equipartition theorem kB T J0 2 q θq θ−q = 2 2

(9.15)

which implies that the Fourier transform of the correlation function φ(r)φ(0) is given by θq θ−q =

kB T 1 J0 q 2

(9.16)

d2 q eiq·r − 1 (2π )2 q2

(9.17)

Thus, we get kB T G(r) = J0

Note how the phase-fluctuations vanish when T → 0. This means that phasecorrelations become truly long-ranged when T = 0, so at least in this limit we have established long-range order. What happens as we switch on T ? The above Fourier-integral may be evaluated straightforwardly, to obtain G(r) = −

r kB T ln 2π J0 a

(9.18)

254

TWO-DIMENSIONAL SUPERCONDUCTIVITY

√ where a is some short-distance cutoff a = e−γ /2 2 and γ = 0.577 . . . is the Euler–Mascheroni constant. Inserting this back into Eq. 9.12, we get (r) =

r −η a

(9.19)

where η = kB T /2π J0 . Note how this correlation function fits in with a general Ansatz for the two-point correlator 2 (r) close to a critical point, which on general grounds may be written as 2 (r) =

1 r d−2+η

G(r/ξ )

(9.20)

where ξ is some correlation length of the problem, d is dimensionality, G is some scaling function, and η is a so-called anomalous scaling dimension of the superfluid matter field ψ. Eq. 9.20 is of the form of Eq. 9.19, provided we set d = 2 and ξ = ∞. The latter is the hallmark of a system which is critical. Thus, what we learn from this is that a two-dimensional superfluid/superconductor has an entire low-temperature phase, which is critical. This is also reflected in the anomalous scaling dimension η = kB T /2π J0 , which is non-universal. Critical exponents associated with critical points are universal. Non-universality of exponents means that we are dealing here with a critical line, not a critical point. An important feature of (r) is that limr→∞ (r) → 0 provided η = 0, i.e. as soon as T = 0. Hence, there is never true long-range order at finite temperature in a two-dimensional superfluid/superconductor. In other words, the U (1) symmetry that is spontaneously broken in the three-dimensional case is never broken at finite temperature in two dimensions. This is a specific example of a somewhat more general statement, namely the Hohenberg–Mermin–Wagner theorem that states that at finite T , no continuous symmetry can be spontaneously broken in dimensions d ≤ 2[128, 129]1 . What we at most can have is power-law decay (which is much slower than exponential decay characteristic of shortrange order). Power laws mean that there is no length scale in the problem any longer, ξ → ∞ in Eq. 9.20. The system is thus scale-invariant, which is exactly the hallmark of criticality. This is often referred to as quasi-long-range order. The above result is based on the presumption that we can define local order of the phase-fields, and expand in small fluctuations around local order. A minute or two of reflection reveals that this cannot possibly be correct at high temperatures. It is obvious that in the high-temperature limit, even short range order must break 1 Often just referred to as the Mermin–Wagner theorem. Both the papers of Hohenberg and of Mermin and Wagner demonstrate the absence of long-range order in low dimensions for systems with continuous symmetries. Hohenberg considers neutral superfluids, Mermin and Wagner consider ferromagnets. Ironically, the title of the paper by Hohenberg is nonetheless Existence of long range order in one and two dimensions! A humorous remark by Halperin at Hohenberg’s 60th birthday suggested that perhaps the title is the reason for the much more frequent reference to Mermin–Wagner, rather than Hohenberg–Mermin–Wagner! Let it be said at once that both papers arrive at correct conclusions.

VORTEX–ANTIVORTEX PAIRS

255

down, and the above analysis is invalid. What have we missed? The process of elimination reveals the answer. Our starting point only has phase-fluctuations to begin with. The smooth phase-fluctuations we have included so far correspond to longitudinal phase-fluctuations. What we have left out, are transverse phasefluctuations. Their inclusion in the description, and their physical consequences, will be the topic of the next sections. We conclude this section by emphasizing that what we have demonstrated here, is that smooth phase-fluctuations (analogues of spin-waves in magnetic systems) suffice to destroy long range order in two dimensions and render the system critical, at any finite temperature. Spin-waves are therefore critical fluctuations in two dimensions (spin waves are not critical in three dimensions). Nonetheless, this does not mean that it does not cost energy to ‘twist’ the phase of the superconducting order parameter at low temperatures. Even if the system does not exhibit true long-range phase order, it still has a phase stiffness associated with it. On the other hand, at very high temperatures, phases are randomly oriented relative to each other even on the shortest length scales, and a local twist is expected to come at no cost in the free energy. Hence, somewhere in between low and high temperatures some phenomenon must occur such that the phase stiffness vanishes. If this happens at a finite temperature, then this phenomenon must in fact be a phase-transition, not a crossover. This is because a finite phase stiffness cannot be brought to precisely zero on a finite temperature interval in an analytic manner. It must therefore vanish in a phase transition. That this putative phase transition must be a subtle one, is clear from the simple observation that it cannot be a phase transition from an ordered low-temperature state to a disordered high-temperature state. It must be a phase transition from a quasi-ordered state to a disordered state. Under such circumstances we do not have the luxury, as we have in three dimensions, of probing the phase transition by monitoring the expectation value of a local ordering field (a local order parameter) and asking when it vanishes. In fact, when we are dealing with systems with a continuous symmetry in two dimensions we are forced to invoke a much more general (but often unnecessary) method of detecting a phase transition: We must identify a generalized stiffness of the system, which is a global quantity, and investigate when this stiffness vanishes through a proliferation of topological defects facilitated by entropy production in the free energy. In fact, this is a method we can always use, also in three dimensions, to detect phase transitions. We shall rephrase the three-dimensional superconductor to normal metal transition in this language in the next chapter.

9.4

Vortex–antivortex pairs

Transverse phase fluctuations are more violent than the smooth longitudinal ones considered in the previous section. Consider the quantity ∇θ and imagine

256

TWO-DIMENSIONAL SUPERCONDUCTIVITY

integrating this around some arbitrary closed contour in the plane. The vorticity q of the phase-distribution is measured by the quantity

dl × ∇θ = 2π q

(9.21)

Here, q ∈ Z. It is impossible to continually deform a phase distribution with q = 0 where only longitudinal, smooth phase fluctuations are excited, into a distribution where q = 0. Those phase distributions where q = 0 and those where q = 0 are topologically distinct. A vortex with a vorticity q is a topological defect superimposed on the phase distribution where no vortices are present. It is obvious that for high enough temperatures, transverse phase fluctuations will be excited thermally, not only smooth longitudinal ones. Vortices will therefore be generated spontaneously at high enough temperatures since this will increase the configurational entropy of the system, thereby lowering the free energy. Vortices are topological defects of the superconducting ordering field eiθ (r) . When they proliferate, the phase stiffness of the system vanishes, and this defines the phase transition. In Figure 9.2, we illustrate a vortex configuration in the twodimensional XY -model on a square lattice, while in Figure 9.3 we illustrate a vortex–antivortex pair. Note that for a charged superfluid, ∇θ gives rise to an electric current. The curl of this current is a magnetic field, and by Eq. 9.21 we thus see that q

Vortex

Antivortex

Figure 9.2 Four examples of vortex configurations, or equivalently transverse phasefluctuations, in the two-dimensional XY -model on a square lattice. Notice how each vortex corresponds to a collective phase-mode. The black dot in the centre is meant to illustrate the core of the vortex in this particular configuration. Thermally excited transverse phase fluctuations always give a vortex and an antivortex. The arrows indicate values of θi , analogous to an XY spin direction, on the lattice points where the order parameter is defined.

MAPPING TO THE 2D COULOMB GAS

257

Figure 9.3 An example of a vortex–antivortex pair. If we encircle one of these vortices along one of the small paths, we pick up a phase-difference ±2π. The phase-difference along the large path is zero. The fluctuations outside of this path correspond to spin waves.

may be interpreted essentially as the quantum of a magnetic field penetrating through an area enclosed by a contour C which the integral in Eq. 9.21 is taken around. It is intuitively perhaps obvious that no net magnetic field can be generated throughout the system by thermal fluctuations. Hence, vortices must always be generated in pairs of opposite vorticity, a vortex–antivortex pair. At low temperatures where vortices are expected to be unimportant, the above statement of the existence of vortex–antivortex pairs translates into a statement that at low temperatures only very tightly bound pairs exist. The proliferation of free topological defects at high temperatures, responsible for destroying the phase stiffness of the system, is equivalent to saying that the vortex–antivortex pair has dissociated into two free vortices of opposite vorticity. As we shall see, the above may be precisely rephrased into the language of a metal-insulator transition in a two-dimensional Coulomb gas, where the low-temperature phase corresponds to an insulating dielectric phase and the high-temperature phase corresponds to a metallic plasma phase.

9.5

Mapping to the 2D Coulomb gas

When vortex configurations are thermally excited in the two-dimensional superfluid, this is equivalent to generating a set of fluctuating ‘charges’ {qi } with overall charge-neutrality imposed, i qi = 0. The loss of phase-stiffness in the system, which we have argued above to be the phase-transition, must be related somehow to the statistical mechanics of this ensemble of charges. This follows

258

TWO-DIMENSIONAL SUPERCONDUCTIVITY

from the fact that these charges are manifestations of transverse phase fluctuations in the superconducting ordering field, and that the longitudinal phase fluctuations are incapable of driving the system into the high-temperature phase. What we need to do, is to include explicity the feature that the phases of the order parameter are angular variables defined on the interval θi ∈ [0, 2π . For the purposes of studying the phase transition in the two-dimensional superfluid on a lattice, i.e. where we have introduced a short-distance cutoff in the problem, we will perform a number of standard steps essentially amounting to what is called a duality transformation. Such a transformation is basically the following. When we focus on studying the critical properties of a system exhibiting a critical phenomenon, we try to identify precisely the thermal excitations that are responsible for destroying order in this system. These excitations may be viewed in general as topological defects in some ordering field, in our case the superfluid/superconducting condensate wave function ψi . Next, we attempt to express the partition function, more precisely the part of the partition function giving a singular contribution to the free energy, in terms of these topological defects. When this has been done, we have effectively executed a duality transformation. Strictly speaking the final step in the duality transformation is to write down a field theory for the action appearing in the partition function when it is written in terms of the topological objects of the original system. This field theory is the dual to the original field theory we started from. In this context, let us make an important remark on duality before we start doing computations in earnest. Suppose we have arrived at some dual field theory starting from an original theory such as the Ginburg–Landau theory of the two-dimensional superfluid. This dual theory itself has topological defects in its (dual) ordering field, which in principle we may identify. The partition function for the dual model may thus also be written in terms of the topological defects of the dual ordering field, and a field theory can be written for the corresponding action. This field theory is the dual of the dual model, and must in fact correspond to the original starting model. Duality squared must be equal to one. This is a statement which holds for all systems with only one phase transition. It is much weaker than the statement of self-duality, which means that the dual model has an identical form as the original model (but with inverted coupling constants). For instance, the dual model of the two-dimensional XY model does not have the same form as the two-dimensional XY model. The dual of the dual of the two-dimensional XY model is the XY model itself. However, the two-dimensional Ising model is selfdual, while the dual of the three-dimensional Ising model is a three-dimensional Ising gauge-theory, i.e. a lattice model with a local Ising theory. This is probably the simplest example where two models with the same symmetry, but where one has a global symmetry and the other has a local one, are related by a duality transformation. As it turns out, a similar situation is true for three-dimensional systems with local and global U (1) symmetries, which we will consider in the next chapter.

MAPPING TO THE 2D COULOMB GAS

259

The model with a global U (1) symmetry is a description of a three-dimensional charge-neutral superfluid, while the model with a local symmetry is a model of a three-dimensional superconductor. Hence, three-dimensional superfluids and superconductors are duals of each other. The partition function for the system is a priori given by

ZXY = Dθ e−βHXY HXY = J

1 − cos(θi − θj )

(9.22)

i,j

We next ignore the constant term in the Hamiltonian, and introduce the Fourier expansion of eα cos(x) as follows ∞

eα cos(x) =

In (α)einx

(9.23)

n=−∞

where In (α) is a Bessel function of order n. Inserting this in Eq. 9.22, we get ZXY =

∞

Dθ exp

Inµj (β)

(inµj µ θj )

(9.24)

n=−∞

Carrying out the angular integrations yields a constraint on the integer-valued field n given by µ nµj = 0

(9.25)

This is solved by introducing the two-dimensional curl nµj = εµν ν φj

(9.26)

where εµν is the two-dimensional Levi–Civita tensor, and φj is some scalar integer-valued field, which constitutes the actual degrees of freedom of the system. Up to now, everything is exact. The partition may now be written in terms of our new degrees of freedom, {φj }, as follows Iφj (β) (9.27) Z= {φj }

This may be approximated, using standard properties of the Bessel functions, as follows 1 (9.28) exp − [µ φj ]2 Z= 2β {φj }

j,µ

260

TWO-DIMENSIONAL SUPERCONDUCTIVITY

which we now want to write in a form that explicitly exhibits the topological excitations of the theory. Strictly speaking, the approximation we have made in passing from Eq. 9.27 to Eq. 9.28 is quantitatively useful at large values of β, i.e. it is naively expected to be a good low-temperature approximation. However, it is also qualitatively useful outside of the low-temperature domain. First, the symmetries of the exact partition function Eq. 9.27 and the approximate partition Eq. 9.28 are the same. This means that that the topological excitations of these two objects are the same. Hence, we expect that for the purpose of studying the critical properties of the system, these two objects essentially produce results which are in the same universality class. Less important details, such as the exact value of the critical temperature, will of course differ. To proceed further, we first introduce the Poisson-summation formula ∞

f (n) =

n=−∞

∞

∞

k=−∞ −∞

dz f (z)ei2π kz

(9.29)

Thus, the partition function is written in the following form, when we introduce a scalar auxiliary field pi Z=

{pi }

1 2 D{φ} exp − [µ φj ] + i2πpj φj 2β

(9.30)

The next step is now to perform the φj integrations, which gives Z = Z0

exp −4π 2 β

{pi }

pi D(|i − j |)pj

i,j

−2µ D(|i − j |) = δij

(9.31)

where Z0 is the partition function for spin waves. Note how the partition function factorizes (in the approximation of Eq. 9.28) in the product of a spin-wave part and a part which is isomorphic to the partition function of a two-dimensional Coulomb gas. We will see below that the quantities pj may be thought of as vortices in the original phase fields θi . The above factorization shows that spin waves and vortices do not interact within the approximation made in Eq. 9.28. Explicitly, we have

D(|i − j |) =

π

−π

dqx 2π

π

−π

dqy eiq·(i−j) 2π 2 µ 1 − cos(qµ )

(9.32)

which is just the Coulomb-potential on the two-dimensional lattice. It has the asymptotic value D(|i − j |) ∝ ln(|i − j |) as |i − j | → ∞, moreover the only

MAPPING TO THE 2D COULOMB GAS

261

allowed vortex configurations are those where i pi = 0. This ‘charge-neutrality’ condition follows from the fact that the above describes a Coulomb system with no screening, and hence it is incompressible. This means that any finite charging of the system will cost an infinite amount of energy in the thermodynamic limit such that configurations with i pi = 0 are suppressed. Let us now see how the fields pi correspond to vortex configurations of the original phase fields. In order to interpret the pi -excitation in as easy a fashion as possible, it is convenient to retrace our above steps, using the following approximation for the exponential of the cosine-potential in the XY action eβ cos(x) ≈ eβ

β exp − (x + 2π n)2 2 n=−∞ ∞

(9.33)

where we allow x to vary on the interval −∞, ∞ on the right-hand side. This approximation is usually referred to as the Villain-approximation, and is extremely useful in the current context (as well as in higher dimensions, as we shall see in Chapter 10). Essentially, the partition function for the XY -model is approximated by the partition function for a 2π periodic Gaussian model as follows

β Z= (µ θj − 2π aµ,j )2 Dθ exp − (9.34) 2 {aµ }

µ,j

where aµ,j is an integer-valued field, and we are instructed to sum over all such integers. The next step is to introduce the Fourier transform for each of the exponentials appearing in the partition function using

∞ β 1 1 exp − (x + 2π n)2 = √ dy exp − y 2 + iy(x + 2π n) (9.35) 2 2β 2πβ −∞ Thus we get, up to multiplicative factors which do not contribute to singular parts of the free energy,

1

2 − vµj + ivµj (µ θj + 2π aµ,j ) (9.36) Dθ Dvµ exp Z= 2β {aµ }

µ,j

The next step is to carry out the integrations over the phase-field θj , thus producing the constraint µ vµ,j = 0 (9.37) which is satisfied provided vµ,j = εµν ν φj

(9.38)

262

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Let us insert this representation into the partition function Eq. 9.36. Upon a partial integration in the exponent of Eq. 9.36, it may be written on form

Z=

{aµ }

1 2 − vµj − 2π iεµν µ aν,j φj Dφ exp 2β

(9.39)

µ,j

Now, comparing this with Eq. 9.30, we see that it has an identical form to Eq. 9.39, but we can identify the p-fields, namely pj = εµν µ aν,j . If we now think of aµj as the integer part of the phase-difference µ θj , which we may think of as a current, then we see that pj represents the vorticity of the original fields. It is also useful to rederive all of the above in a continuum version using a particular representation of the gradients of the phase which also takes into account the singularities arising from the fact that the phase is an angular variable, i.e. is defined with compact support, θi ∈ [0, 2π . We write the gradient of the phase (a vector) as a longitudinal and transverse part, cf. Eq. 9.9. The longitudinal part, corresponding to spin waves, is non-singular, while the transverse part gives rise to vortices. Moreover, since they are orthogonal components of the phase gradient, we have (∂θ )2 = (∂θL )2 + (∂θT )2

(9.40)

Recall also the equation relating ∂θT to vorticity, namely Eq. 9.21, which we may also write, using Stoke’s theorem, as ∂ × (∂θT ) = 2π q or equivalently εµν ∂µ ∂ν θT = 2π q(r)

(9.41)

where q(r) is the local vortex density. This equation is satisfied if the following representation is used for (∂ν θ )T

(∂ν θ )T = −2π εµλ ∂λ

d2 r G(r − r )q(r )

provided that the function G(r − r ) satisfies the Laplace equation −∂ 2 G(r) = δ(r)

(9.42)

MAPPING TO THE 2D COULOMB GAS

263

From this, we obtain

d r1 d2 r2 ∂λ G(r − r1 )∂ρ G(r − r2 )q(r1 )q(r2 ) (∂ν θT ) = (2π ) ενλ ενρ

= (2π )2 δλρ d2 r1 d2 r2 ∂λ G(r − r1 )∂ρ G(r − r2 )q(r1 )q(r2 )

2 2 = −(2π ) d r1 d2 r2 G(r − r1 )[∂ 2 G(r − r2 )]q(r1 )q(r2 )

2 (9.43) = +(2π ) d2 r1 q(r1 )G(r − r1 )q(r) 2

2

2

Here, we have used a property of the two-dimensional Levi–Civita tensor, namely that ενλ ενρ = δλρ . If we now write the XY model in the continuum limit as follows

K H= d2 r(∂θ )2 2

K d2 r[(∂θL )2 + (∂θT )2 ] = 2

(9.44)

and then utilize Eq. 9.43, we obtain K H = 2

d r(∂θL ) + 2π K 2

2

2

2

d r

d2 r q(r)G(r − r )q(r )

(9.45)

which again describes a spin-wave system and a Coulomb gas in two dimensions, since G is the Green’s function for the electrostatic potential between point charges in two dimensions. Again, note how spin-waves and vortices decouple in Eq. 9.45, which in this derivation is a consequence of expanding the cosine of the gradient up to quadratic order only. Coupling between spin waves and vortices is seen to be an effect due to higher order gradient terms, and is therefore irrelevant in renormalization group sense. To summarize this section, we have shown that the physics of the twodimensional XY model, i.e. that of a two-dimensional superfluid or superconductor, corresponds to that of a spin wave system coupled to vortex configurations of the XY model. In one particular approximation the spin waves and vortices decouple. Since the spin waves render the system critical at any finite temperature, but do no suffice to induce short-range phase correlations, it follows that the phase-transition from quasi-long range order to short-range order must be encoded in the Coulomb-piece of the partition function. Precisely what sort of phase transition such a system is capable of sustaining, will be the topic of the next section.

264

TWO-DIMENSIONAL SUPERCONDUCTIVITY

9.6 Vortex-pair unbinding and Kosterlitz–Thouless transition In this section, we study the phase transition in the two-dimensional Coulomb gas. We emphasize that we will be using nomenclature appropriate for a system of charges, but want to stress that the connection between the two-dimensional Coulomb gas and the two-dimensional XY model presented in the previous section (i.e. phase-only approximation to the Ginzburg–Landau theory of a two-dimensional superfluid) must always be kept in mind. We will ignore the spin wave part of the partition function, Z0 , since it gives no singular contributions to the free energy. The two-dimensional Coulomb gas has the feature of having an internal energy which consists of contributions that are logarithmic in the separation between the charges of the system. This is a feature which will be of utmost importance in what follows, since it implies that the internal energy and the entropic contribution to the free energy will behave precisely in a similar manner as a function of separation of vortices in a vortex–antivortex pair. Since we have that F = U − T S, we tentatively conclude that due to the logarithmic interaction, the internal energy U and the entropic term T S compete on an equal footing such that at high enough temperatures T , the entropy wins. This means that in the Coulomb gas language, a low-temperature dielectric phase of a system of charges consisting of tightly bound dipoles is converted, at some temperature, into a plasma of dissociated dipoles. In other words, the twodimensional Coulomb gas is capable of sustaining a metal–insulator transition. This would not happen in the one-dimensional Coulomb gas, which is always in the dielectric phase because the internal energy is linear in separation of charges, while the entropy is logarithmic, and hence the former dominates for large separations. Nor would it happen in the three-dimensional Coulomb gas which is always in the metallic phase, due to the fact that the internal energy is inversely proportional to separation between charges, while the entropy is logarithmic, the latter always wins for large separations. So the two-dimensional case is quite special, and it is the logarithmic character of the Coulomb-interaction between charges which is the central point. Coulomb-potentials (in any dimension) also have the special property that they are not screened by dipoles. A cautionary remark to begin with is absolutely necessary. One-dimensional superfluids do not map onto the one-dimensional Coulomb gas, and threedimensional superfluids do not map onto the three-dimensional Coulomb gas! The three-dimensional case will be dealt with in Chapter 10 by similar techniques as in the two-dimensional case, but the result will not be a system of point charges interacting with a Coulombic potential in three dimensions. The topological defects of the three-dimensional superfluid turn out to be vortex-lines, not point-vortices. Therefore, although a three-dimensional Coulomb gas does not have a finite-temperature phase transition, a three-dimensional superfluid

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

265

certainly does! When the two-dimensional Coulomb gas transitions from a dielectric phase to a metallic phase, it is the screening properties of the system which are altered in a non-analytic fashion as a function of temperature. We now follow the pioneering work of Kosterlitz and Thouless [130, 131], with only slight modifications due to Young [132], and Jos´e and co-workers [133]. The approach basically amounts to setting up a self-consistent description of a charge-neutral system in terms of scale-dependent electrostatics. The interested reader may also find it useful to consult the excellent review article on the two-dimensional Coulomb gas by Minnhagen [134]. Imagine that we have a system with a low density of charges, such that an asymptotically exact low-density approximation to its dielectric constant is given by the following expression ε = 1 + 2π nd α

(9.46)

where α denotes the polarizability of the medium. In the following, we will work in arbitrary dimensions d, and specialize to the d = 2 case at the end. The following closely follows the treatment of the problem by Kleinert et al. [135], which again builds on the approach of Young to the problem. In arbitrary dimensions, we assume that the point-charges of the system interacts with an interaction of the following form d − 2 − ηA |x| 2−d+ηA 2 V (x) = −1 (9.47a) 2 + ηA a η d/2 A 2 (4π ) 2 where the -function is defined by

∞

(x) =

dt t x−1 e−t

(9.47b)

0

This is a generalized potential which will correspond to precisely a logarithmic interaction when 2 − d + ηA = 0. Here, ηA is some parameter that describes deviations from standard Coulomb interactions in d dimensions. The standard Coulomb case for arbitrary d corresponds to ηA = 0, and we thus get a logarithmic interaction for the Coulomb-case if and only if d = 2. In this section, we will derive to lowest order in the fugacity the recursion relations for a scale-dependent stiffness parameter K(l) and a scale-dependent fugacity y(l) for a d-dimensional plasma where the bare pair-potential is given by Eq. 9.47a. This potential reduces to a logarithmic interaction when d = 2, and ηA = 0. As will become clear below, the stiffness parameter is basically the inverse of a scale-dependent dielectric constant. The scale-dependent fugacity y(l) basically gives the density of free unbound charges in the system, provided the density is low. Thus, when liml→∞ y(l) → 0, we have no free charges in the

266

TWO-DIMENSIONAL SUPERCONDUCTIVITY

system, only tightly bound dipoles. On the other hand, when liml→∞(l) y(l) → ∞ this is an indication that vortex–antivortex pairs dissociate and free charges appear in the system. Hence, we will look for changes in the scaling of the fugacity as the hallmark of the phase transition in the system. The starting point will be a low-density approximation for a dielectric constant of this system. Introducing the solid angle in d dimensions d = 2π d/2 / (d/2) and the density of dipoles in the fluid by nd , a low-density approximation for the dielectric constant is given by ε = 1 + nd d α

(9.48)

where a standard linear-response analysis gives α = 4π 2 Ks 2 /d for the polarizability, and s 2 is the mean square of the dipole moment in the system. To compute this, we need the low-density limit of the pair-distribution function n± (r) of the plasma, which is readily obtained from the grand canonical partition function expanded to second order in the bare fugacity ζ , and replacing the thermal de Broglie wavelength by a short-distance cutoff r0 , as follows n± (r) =

ζ2 r02d

e−4π

2 KV

(9.49)

In this way, we may now go on to express a scale-dependent dielectric constant as follows

4π 2 d K r ds s d+1 n± (s) (9.50) ε(r) = 1 + d r0 Note, however, that in Eq. 9.50, a mean-field approximation is understood to be used by replacing the bare potential V in n± (r) by an effective potential U (r). This effective screened potential must be selfconsistently determined by demanding that it gives rise to an electric field in the problem given by ∂U K f˜(d) = E(r) = ∂r ε(r) r 1−ρ

(9.51)

ρ = 2 − d + ηA

(9.52)

where and f˜(d) is defined by

d − 2 − ηA (d − 2 − ηA ) 2 f˜(d) = η d/2 A 2 (4π ) (1 + ηA /2)

(9.53)

Such a mean-field procedure has been consistently used with success in the two-dimensional case, and the origin of the success lies in the long range of

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

267

the ln-interaction. In higher dimensions, such a procedure will work even better since the logarithmic potential is felt over even longer distances due to extra volume factors. Let us introduce a logarithmic length scale l = ln(r/r0 ) along with the new variables τ (l) =

ε(r0 exp l) 4π 2 K

x(l) = 4π 2 KU (r0 exp l)

(9.54)

Here, x(l) is determined selfconsistently by integrating the effective field E(r). Then we get from Eqs 9.50 and 9.51

d ζ 2 l τ (l) = τ (0) + d−2 dv e(d+2)v−x(v) (9.55) dr0 0 and x(l) = x(0) + f˜(d)

ρ

l

dv 0

r0 eρv τ (v)

(9.56)

From Eqs 9.55 and 9.56 we may derive coupled renormalization group equations for τ (l) and x(l). However, in order to obtain equations that have a form more similar to equations that have appeared in the literature on the d-dimensional Coulomb gas, we introduce a new variable K(l) representing a scale dependent stiffness constant, as follows K −1 (l) ≡

τ (l) ρ r0 eρl

(9.57)

Thus, we see that the effect of a non-zero ρ on the stiffness amounts to a scaling change K(l) → eρl K(l). Using Eq. 9.56, we have ∂x(l) = 4π 2 f˜(d)K(l) ∂l

(9.58)

Differentiating K −1 (l) with respect to l and using Eq. 9.55, we obtain 2d ζ 2 ∂K −1 (l) = −ρK −1 (l) + d−2+ρ e[(d+2−ρ)l−x(l)] ∂l dr0

(9.59)

From this expression, we define a scale-dependent fugacity y(l) given by √ 2d ζ e[(d+2−ρ)l−x(l)]/2 (9.60) y(l) ≡ √ (d−2+ρ)/2 dr0

268

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Thus, we see explicitly that the renormalization of K(l) in principle influences the flow equation for y(l), which is obtained by differentiating with respect to l and using Eq. 9.58. We thus get the two coupled equations dK −1 (l) = y 2 − ρK −1 (l) dl dy(l) = [d − ηy − 2π 2 f˜(d)K(l)]y(l) dl

(9.61)

where ηy = (d − 2 + ρ)/2, and ρ is given by Eq. 9.52. It has a physical interpretation as an anomalous scaling dimension of the fugacity. Let us set ηA = 0, i.e. we consider the standard Coulomb-case (our starting point!), but in arbitrary dimensions. This means that ηy = 0 as well. We then get the following set of equations for the scale-dependent stiffness parameter K(l), or inverse dielectric constant, and fugacity y(l) dK −1 = y 2 − (2 − d)K −1 dl dy = [d − 2π 2 f (d)K]y dl

(9.62) (9.63)

where f (d) = (d − 2) [(d − 2)/2]/(4π )d/2 . These equations describe the flows of the stiffness parameter and the fugacity of the d-dimensional Coulomb gas. Precisely the same results were first obtained by Kosterlitz by a method completely different from the one we have used above, a good sign [136]. Finally, if we now set d = 2 we arrive at the celebrated Kosterlitz–Thouless flow equations for the dielectric constant and the fugacity of the two-dimensional Coulomb gas, namely dK −1 = y2 dl dy = [2 − π K] y dl

(9.64) (9.65)

Notice how the second term on the right-hand side of Eq. 9.62 vanishes when d = 2. This is of crucial importance. Eqs 9.64 and 9.65 describe how the dielectric constant and the effective fugacity of the Coulomb gas change when the length scale l they are viewed on, varies. These are therefore not standard renormalization group (RG) equations in the sense of Wilson-RG. Rather, they have the status of selfconsistency equations for scale-dependent electrostatics. Let us now consider what these equations predict. The result of the flows for K(l) and y(l) will depend on what the values of the bare parameter for the dielectric constant and the fugacity are. The bare values in this context refer to what the value of these quantities are at short length scales. Suppose that

VORTEX-PAIR UNBINDING AND KOSTERLITZ–THOULESS TRANSITION

269

the bare value of K is larger than 2/π . Then the right-hand side of Eq. 9.65 is negative, and y(l) is reduced as l increases. Consider now Eq. 9.64 under these circumstances. Since y(l) decreases with l, it means that K(l) increases. But then the right-hand side of Eq. 9.65 gets even more negative, thus accelerating the reduction of y(l). Thus, the system flows to a regime where liml→∞ y(l) → 0. Consider now the case where K is smaller than 2/π . Then y(l) increases with increasing l, and K is reduced further, thus accelerating the increase in y(l). Thus, in this case, liml→∞ y(l) → ∞. Hence, the value K ∗ = 2/π is a particular value of the stiffness which separates the regime where liml→∞ y(l) → 0 from the regime where liml→∞ y(l) → ∞. What does all of this mean, physically? The case liml→∞ y(l) → 0 simply means that in an appropriate temperature regime, there are no free charges in the two-dimensional Coulomb gas, all charges are bound into tight dipoles. Such a system of tightly bound dipolar pairs is incapable of carrying an electric current when it is subjected to an electric field, and is therefore an insulator. The case liml→∞ y(l) → ∞ corresponds to proliferation of free charges in the system, and such a system is capable of carrying a current when subjected to an electric field. This is therefore a metallic phase. Hence, we reach the conclusion that the sort of phase transition the two-dimensional Coulomb gas undergoes when it passes through the point K ∗ = 2/π , is a metal-insulator transition. Note how all of this fails when d = 2. For d = 1, the second term on the right-hand side of Eq. 9.62 is finite and negative. This means that no matter how large we initially make the fugacity (for instance by making K initially very large), K −1 (l) will decrease, hence increasing K(l) and thus reducing y(l). For all bare values of K, we always end up in a situation where liml→∞ y(l) → 0. Conversely, when d = 3 the second term on the right-hand side of Eq. 9.62 is finite and positive. By a similar type of argument as for d = 1, we always end up in the situation where liml→∞ y(l) → ∞. The d = 1 result is a statement that the one-dimensional Coulomb gas is always in the dielectric phase, never in the metallic phase, whereas the three-dimensional Coulomb gas is never in the dielectric phase, but always in the metallic phase. It is now very appropriate to go back to the two-dimensional superfluid, and ask ourselves what all of this means in that system. In other words, the metal–insulator transition of the two-dimensional Coulomb gas maps onto precisely what in the two-dimensional superfluid? We have already established in the previous section, that the charges in the two-dimensional Coulomb gas are to be identified with vortices in the phase-field of the superfluid/superconducting ordering field. Thus the metal–insulator transition corresponds to a phase transition in the superfluid from a low-temperature phase with only tightly bound vortex–antivortex pairs into a high-temperature phase where one has dissociated vortex–antivortex pairs. These vortices are the topological defects in the phasetexture of the superfluid. When they proliferate as a result of the dominance of the entropic contribution to the free energy, they convert the powerlaw decay of

270

TWO-DIMENSIONAL SUPERCONDUCTIVITY

the phase–phase correlator, (Eq. 9.19), into an exponential decay characteristic of short-range order. The phase-stiffness of the system, which is non-zero in the critical low-temperature regime, has been lost at the phase transition as a result of the appearance of vortices. Now, the phase-stiffness of the XY model is the energy cost of introducing twists in the phase of the superconducting order parameter, i.e. the energy cost of introducing gradients ∇θ . Superconductivity is a macroscopic quantum phenomenon associated with phase-coherence. The phase stiffness, often called the helicity modulus ϒ of the XY model, is defined as the cost in free energy of an initial twist θ in the phase of the order parameter across the system, ϒ∼

∂ 2F |θ =0 ∂θ 2

(9.66)

Going back to the partition function for the XY model, we have (upon normalizing ϒ to its value at zero temperature) 2 ϒ 1 J = cos(µ θ ) − cos(µ θ ) J N r kB T N r

(9.67)

This quantity probes the global phase-coherence of the system and can be directly identified with the superfluid density ρs of the system. This is a consequence of the London equation J=−

1 A µ0 λ2

(9.68)

as follows. The twist in the phase θ may be viewed as adding a vector potential A to the argument of the cosine-potential in the XY model (by minimal coupling). This alters the free energy. Now, by standard quantum mechanics, the current given above may be viewed as a linear-response expression for the derivative of the free energy with respect to the added vector potential. The second derivative of the free energy with respect to an added vector potential, evaluated at A = 0, is therefore the (negative of the) derivative of the current with respect to the vector potential, which is nothing but 1/λ2 ∼ ρs . Hence, we have a major result, namely ϒ ∼ ρs

(9.69)

Vortices are responsible for destroying the phase stiffness, i.e. ϒ, of the XY model, and they are therefore also responsible for destroying the superfluid density in the 2D superfluid/superconductor. To put this into perspective, it is worthwhile reminding ourselves that for the two-dimensional Ising model, we are able to consider the magnetization as a useful order parameter. The Ising model for d = 2 is capable of sustaining a lowtemperature phase with true long range spin–spin correlations because the spins

JUMP IN SUPERFLUID DENSITY

271

can only point in two directions. The model has a discrete symmetry, unlike the XY model, and therefore does not sustain gapless spin wave modes that can be excited at arbitrary low temperatures. However, if we preferred, we could detect the phase transition in the two-dimensional Ising model, not by monitoring the magnetization (a local order parameter), but by monitoring the proliferation of lines of overturned spins. These constitute two-dimensional domain walls and are the topological objects responsible for destroying the spin-stiffness (a global order parameter) in the two-dimensional Ising model. The Ising-analogue of the spin stiffness is the free-energy cost of forcing a domain wall into the system (since the minimal twist of boundary conditions is an angle π in the Ising case). The free energy of the domain line per unit length is the line tension of the domain-line. When domain-lines proliferate, they do so because their line tension vanishes, and it can be demonstrated that in fact this quantity vanishes precisely at Tc . It was, as a matter of fact, computed exactly for the two-dimensional Ising model in 1942 by Onsager [137], in his stellar paper on the exact solution to the two-dimensional Ising model. The line-tension of domain-lines may therefore also serve as a candidate generalized stiffness in this case. The spirit of the domain-line approach for the two-dimensional Ising model is similar in spirit to monitoring the proliferation of vortices in the two-dimensional XY model. The difference is that in the Ising-case, we have the luxury of being able to use a local order parameter, if we so wish, to detect the transition, whereas in the case of the XY case in two dimensions, we do not. We are forced to the (conceptually quite charitable!) conclusion that in the two-dimensional XY model, the general scheme of identifying topological objects and asking when their proliferation annihilates a generalized stiffness is the method of detecting the phase transition. This is basically a by now well accepted realization of Anderson’s quite general concept that a phase transition may be viewed as the proliferation of topological defects in some ordering field with an associated breakdown of a generalized rigidity [138].

9.7 Jump in superfluid density Let us consider in some detail the solution to the flow equations Eqs 9.64 and 9.65. We are primarily interested in solving the equations for low fugacity, since the equations themselves are based on the notion that the density of charge (free vortices) is small. What happens for high densities is beyond the current approach, and will not concern us here. We rewrite Eq. 9.65 slightly as follows using K −1 (l) = τ (l) 2 τ (l) − 1 dy(l) y(l) =2 π 2 dl π τ (l) ≡ 2T (l)y(l)

(9.70)

272

TWO-DIMENSIONAL SUPERCONDUCTIVITY

Multiplying on each side by y(l) this may be recast into the form dy 2 (l) = 4T (l)y 2 (l) dl

(9.71)

We will now look for solutions consistent with a low fugacity, and consider therefore the regime close to the point where the scaling of y(l) changes, which as we have argued above happens when τ = π/2. In this case, we have 2 τ (l) − 1 π dT (l) 2 ≈ y 2 (l) dl π T (l) ≈

dT 2 (l) 4 ≈ T (l)y 2 (l) dl π

(9.72)

√ We may now combine Eqs 9.71 and 9.72, upon redefining y(l) →= y/ π , as follows d[y 2 (l)] − d[T 2 (l)] =0 dl

(9.73)

y 2 (l) − T 2 (l) = ±ω2

(9.74)

or equivalently

where ω is taken to be some positive integration constant, and we have deliberately written it in such a way as to distinguish two cases, namely that where it is negative and that where it is positive. We consider the former case first, and for this case, it is furthermore necessary to distinguish between two cases, namely that where T (l) < 0 and that where T (l) > 0. We consider therefore first the case where y 2 − T 2 < 0, T < 0. From Eq. 9.72 it follows that 2 2 dT (l) =− ω − T 2 (l) (9.75) dl π Upon introducing l˜ = (2ωl)/π and T˜ (l) = T (l)/ω, Eq. 9.75 takes the simpler form

or equivalently

dT˜ (l) = T˜ 2 − 1 ˜ dl

(9.76)

dT˜ (l) = dl˜ T˜ 2 − 1

(9.77)

JUMP IN SUPERFLUID DENSITY

273

which immediately may be integrated to yield coth−1 (T˜ (l)) = −(l˜ + θ )

(9.78)

where θ > 0 is yet another integration constant, and the choice of sign guarantees that T (l) < 0, since this is the case we now consider. Thus, we finally get T (l) = −ω coth(u) 2 u = ωl + θ π

(9.79)

Moreover, using Eq. 9.74 and the fact that the fugacity is positive, we also obtain y(l) =

ω sinh(u)

(9.80)

Now, consider the limit l → ∞, i.e. the long distance physics of the problem. It is immediately clear that both liml→∞ y(l) = 0 and liml→∞ T (l) = 0. Thus, for all initial values such that y 2 < T 2 , we end up in a dielectric insulating phase of the Coulomb gas. This corresponds to the low-temperature phase of the superfluid, where only spin waves, but no vortices, are thermally excited. The above also implies that in this regime, liml→∞ τ (l) = π/2, or equivalently, K ∗ ≡ lim K(l) = l→∞

2 π

(9.81)

Next consider the regime where y 2 − T 2 < 0, T > 0. We proceed by integrating the equations precisely as above, but we need to make another choice of sign in the integration constant θ appearing in Eq. 9.78 in order to guarantee the correct sign of T , and we get ˜ coth−1 (T˜ (l)) = (θ − l)

(9.82)

where θ > 0, whence T (l) = ω coth(u) 2 u = θ − ωl π Consequently, we have y(l) =

ω sinh(u)

(9.83)

(9.84)

where the argument u is given by that in Eq. 9.83. It is clear from the above that the solutions for y 2 − T 2 < 0, T > 0 cannot be trusted as l is increased indefinitely, since y(l) in fact diverges, contradicting the assumption that y(l) should

274

TWO-DIMENSIONAL SUPERCONDUCTIVITY

be small. However, we can say the following. As l increases, starting from an arbitrary, but small value of y(l), the solutions predict that y(l) increases. Thus, instead of y(l) flowing to zero, as in the case T (l) < 0, we have an unambiguous indication that tightly bound dipoles dissociate, resulting in a proliferation of free charges, or equivalently a proliferation of free vortices. The consequence of an increasing y(l) for K(l) is obvious, it decreases, thus accelerating the increase of y(l), further reducing K(l). In the regime y 2 − T 2 < 0, T > 0 we therefore obtain K ∗ ≡ lim K(l) = 0 l→∞

(9.85)

Based on Eqs 9.81 and 9.85, we are now ready to state a major result of the whole formalism we have presented in this section and the preceding one. It says that as we go through the metal–insulator transition, the renormalized stiffness parameter liml→∞ K(l) of the system (equivalently the inverse dielectric constant of the Coulomb gas), exhibits a discontinuity of universal magnitude, given by 2/π . In a moment, we shall translate this into the language of superfluidity. First, however, we complete our analysis of the flow equations by considering also the regime y 2 − T 2 > 0. In this case, the differential equation corresponding to Eq. 9.75 reads dT (l) 2 2 = ω + T 2 (l) dl π

(9.86)

which is straightforwardly solved, much as above, to yield the solutions T (l) = ω cot(u) ω y(l) = | sin(u)| 2ω l u=θ− π

(9.87)

where again θ > 0 is an integration constant. Since cot(u) does not have a definite sign, this solution encompasses both cases T > 0 and T < 0. The above three cases of the solutions to the flow equations may be summarized in the flowdiagram for y(l), T (l) in Figure 9.4 (which any student of statistical physics and superconductivity should know!), where the arrows indicate in which direction the quantities flow as l is increased We close the discussion of the flow equations by remarking that to the extent that they exhibit fixed points (it turns out to be an entire line of fixed points), this occurs at zero fugacity, i.e. y ∗ = liml→∞ y(l) = 0. This is a very fortunate circumstance, since the basic starting point for deriving the flow equations was Eq. 9.50 which is a low-density approximation to the dielectric constant. The fact that the fixed point occurs at zero fugacity means that the assumption of low

JUMP IN SUPERFLUID DENSITY

275

y

Metallic state

Insulating phase (dielectric) 1−p/2 K

Figure 9.4 Flowdiagram showing variation in renormalized fugacity y(l) and stiffness parameter K(l). Note how liml→∞ y(l) → 0 for all T < 0. The entire line Y = 0, T < 0 is therefore a fixed line, in contrast to a fixed point, for the flow equations. The two straight lines are given by y = −T , T < 0 and y = T , T > 0, and the thick line y = −T is the separatrix separating the two scaling regimes liml→∞ y(l) = 0 and liml→∞ y(l) = ∞. The thick solid line y = 0, T < 0 is a line of fixed points.

densities is selfconsistently shown to be correct. Had we encountered a finitefugacity fixed point, the entire calculation would have been uncontrolled and we would have, at the very least, been forced to include higher order fugacity terms. As it turns out, this need not concern us. Let us now translate the statement about the jump of 2/π in K ∗ at the phase transition into the language of superfluidity. To do this, we need to establish a connection between the superfluid density of the two-dimensional superfluid, and the the scale-dependent inverse dielectric constant (K(l)) of the two-dimensional Coulomb-gas. The rather tedious, but straightforward details of this may for instance be found in the textbook of Huang [139], Appendix A. The result is very straightforward, namely that the superfluid density, normalized to its zerotemperature value, may be expressed in terms of the density–density correlation function for vortices as follows 1 nk n−k ρs = lim 1 − k→0 kB T V k 2

(9.88)

where nk is the Fourier transform of the vortex density, or equivalently the charge density, and V is the volume of the system. The k → 0 limit of this is nothing but the spatial integral of the pair-distribution function. Hence Eq. 9.88 is nothing but the inverse of the dielectric constant as given in Eq. 9.46, in the low-density limit. Hence, the superfluid density and the stiffness parameter are

276

TWO-DIMENSIONAL SUPERCONDUCTIVITY

related as follows, K(T ) =

2 ρs (T ) m2 kB T

(9.89)

where m is the mass of the bosons constituting the superfluid, and we have reinstated Planck’s constant . (Converting from natural units back to physical units, a density acquires the dimension (/m)2 ). Therefore, if we measure ρs (T ) in a two-dimensional superfluid as a function of temperature approaching Tc from below, we have the quite remarkable prediction that at T = Tc , we will observe a discontinuity in ρs (T ) as a function of temperature as we cross the transition. It is finite up to Tc and vanishes at and above Tc in such a way that lim

T →Tc−

2 2 ρs (T ) = 2 π m kB T

(9.90)

exhibits a universal jump. This is a very powerful prediction of the theory, first made by Nelson and Kosterlitz [140], ranking on par with the prediction of BCS of a universal ratio between the zero-temperature gap and the critical temperature, as we discussed in Chapter 4. The prediction was quickly verified in experiments on superfluid thin He4 films by Bishop and Reppy [141], and effectively removed any serious skepticism that might have existed about the existence of the Kosterlitz–Thouless transition. A qualitative sketch of the superfluid density as a function of temperature is given in Figure 9.5. A comment is certainly in order here. Note how the global order parameter ρs of the superfluid vanishes discontinuously at the phase-transition. This is reminiscent of a first order phase transition. On the other hand, the correlation length of the superfluid is finite in the high-temperature phase but infinite in the low-temperature phase. This is a situation which is reminiscent of a second order transition. In fact, the Kosterlitz–Thouless transition is neither first nor second order. The above is an indication of the fact that the classification scheme of first and second order phase transitions is not entirely adequate. The Kosterlitz–Thouless transition is in fact an infinite order phase-transition. rs

Tc

T

Figure 9.5 Superfluid density ρs (T ) of a two-dimensional superfluid as a function of temperature. Note the discontinuity at the critical temperature. The jump in ρs at Tc , normalized to the critical temperature, is universal, limT →Tc− 2 ρs (T )/(mkB T ) = 2/π.

JUMP IN SUPERFLUID DENSITY

277

Let us now proceed to see what happens when we apply the duality technology to the three-dimensional case. As we will see in the next chapter, the topological defects of the superfluid/superconductor in three dimensions are vortex lines and not point-vortices. This precludes the possibility of a Kosterlitz–Thouless type of RG approach to this problem.

10 Dual Description of the Superconducting Phase Transition 10.1 Introduction In this chapter, we will utilize the three-dimensional analogue of the duality transformation introduced in the previous chapter to gain further insight into the character of the superconductor-normal metal transition. Recall that in Chapter 4, where we established and solved the BCS gap equation, it was emphasized that this was a mean-field approach which neglected fluctuations in the critical regime. The BCS approach works extremely well in superconductors like Al and Sn, even at the quantitative level. This is due to the fact that these superconductors are deep into the type I regime and fluctuation effects are tiny. In this chapter, we turn to the case of extreme type II superconductors like the high-Tc cuprates and uncharged superfluids like He4 . The latter can be seen as a limit of the extreme type II case, by letting the Ginzburg–Landau parameter κ → ∞. Fluctuation effects are now much more prominent, especially for the high-Tc cuprates. The reason is twofold. First, because of the large values of critical temperatures, thermal fluctuation effects are expected to be larger than for superconductors with low Tc . Another way of saying this is that a high Tc reflects the fact that Cooper-pairs are tightly bound, and hence the correlation length ξ , which is a measure of the spatial extent of a Cooperpair, i.e. over what distances in real-space two electrons are correlated into opposite-momentum and opposite-spin states, is small compared to its value in unconventional low-temperature superconductors. Hence, the van der Waals type of argument involving large ξ that leads to a justification of the meanfield approach, is no longer expected to work as well. Secondly, extreme type √ II superconductivity involves κ = λ/ξ 1. Now, ξ ∼ 1/Tc and λ ∼ 1/ ρs . √ Hence, κ ∼ Tc / ρs . In high-Tc cuprates, κ is large not only because Tc is Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

280

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

large, but also because high-Tc cuprate superconductivity arises out of very poor metals involving low charge carrier density ρn . This carrier density is an upper limit on the superfluid density ρs , which is therefore also low. This has important physical ramifications with respect to fluctuation effects. Recall from Chapter 10 that we established a relation between the phase stiffness (helicity modulus ϒ) of the superconducting condensate, and ρs as follows, ϒ∼

∂ 2F |θ =0 ∼ ρs ∂θ 2

(10.1)

where F is the free energy and θ is a phase-twist in the complex scalar superconducting order parameter across the system. This means that a low superfluid density implies the existence of large phase-fluctuations in the system. In superconductors arising out of good metals like Al, ρs and hence the phase stiffness, is much larger and these phase fluctuations may usually be ignored except in an immeasurably narrow temperature range around the critical temperature. We emphasize that the approach to be detailed here is not in contradiction to the BCS theory. Rather, it complements it in the situations where the critical fluctuation effects that are left out in the BCS mean-field approach need to be taken into account. We will base our discussion on the Ginzburg–Landau theory, just as in Chapter 10. The strength of such an approach is that the Ginzburg–Landau theory simply postulates the existence of superconducting order without asking how it has established itself. Therefore, what we shall have to say in this chapter is general and entirely model independent, applying in principle to extreme type II and even moderate type II superconductors with a complex scalar order parameter (spin-singlet superconductivity). We shall be interested in studying the critical properties of the superconductor and for this purpose the Ginzburg–Landau theory, which is a theory of a bosonic matter field coupled to a fluctuating gauge field, will suffice both for s-wave superconductors and d-wave superconductors. The two differ in one important respect, namely in that the former has no gapless fermionic excitations on the Fermi-surface, whereas the latter does. The nodal fermions in the d-wave superconductors in principle need to be taken into account in the superconducting state, but at Tc we may assume them to be fully thermalized and decoupled from the superconducting condensate. Were we, however, to study quantum fluctuations in the superconducting order parameter at very low temperatures, then we would need to consider the nodal fermions seriously, and a d-wave superconductor in this temperature regime has a quite different behavior than an s-wave superconductor. This is a quite involved situation which we will not deal with here, and where much work remains to be done. We take as our starting point the Ginzburg–Landau theory of the system, introduced in Chapter 4, which when written in dimensionful form is defined by the partition function of the system written as a functional integral over the

281

INTRODUCTION

fluctuating condensate order field ψ and the fluctuating gauge field A as follows Z = DψDAe−βH (ψ,A) u 4 2 1 2 ∗ 2 2 H (ψ, A) = dr α(T )|ψ| + |ψ| + |(∇ − ie A)ψ| + (∇ × A) 2 2m∗ 2µ0 (10.2) Here, m∗ and e∗ are effective masses and charges for the bosonic condensate constituents, A is a fluctuating gauge field related to a local induction B via the equation B = ∇ × A, and µ0 is the vacuum permeability. Next, we scale the quantities appearing in Eq. 10.2 as follows m∗ α(T ) β4 µ0 β ∗ 2m∗ ∗ 2 A→ A, e → e ,ψ → ψ, → m , u → u β µ0 β2 2β2 2(m∗ )2 (10.3) 2 Note the parameter m appearing in the above. As α(T ) becomes negative for low enough temperatures, we must think of m2 as some mass parameter, not a physical mass. Then, Eq. 10.2 may be written on the form Z = DψDAe−S(ψ,A) S(ψ, A) = dr m2 |ψ|2 + u|ψ|4 + |(∇ − ieA)ψ|2 + 12 (∇ × A)2 (10.4)

where there now appears a dimensionless action S in the exponent of the Boltzmann weight. Since S is dimensionless, all terms under the integral in S carry dimension L−d . Hence, we have the naive scaling dimensions of the quantities appearing in Eq. 10.4 1−d 2

[e] = L 2 −1 (10.5) If we now express all dimensionful quantities as dimensionless via the coupling constant e as follows [ψ] = L

,

ψ → ψe−1 ,

d

[A] = L1− 2 ,

A → Ae−1 ,

[u] = Ld−2 ,

r → re2 ,

[m2 ] = L−1 ,

m2 → ye4 ,

u → xe2

d

(10.6)

we may write the action in a form which we will use explicitly at the end of this chapter, namely S(ψ, A) = dr y|ψ|2 + x|ψ|4 + |(∇ − iA)ψ|2 + 12 (∇ × A)2 (10.7) Here, y appears as a temperature-like parameter, while whereas x essentially is like κ 2 , such that a large x corresponds to extreme type II, small x corresponds

282

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

to type I, and the mean-field demarcation line between type I and type II is given by x = 1/2. We shall come back to this point in Section 10.8. Most of this chapter will be concerned with the situation for large x 1. Consider for the moment the situation with x → ∞. This means that for a fixed |ψ|4 -coupling u, the theory corresponds to that of an uncharged superfluid, and we may simply drop the gauge field A from the description. It will live its own uneventful life as a free Maxwell field decoupled from the matter field ψ. We now make an approximation that is expected to be excellent in the type II regime, but which we will later show fails in the type I regime. In the type II regime, we will ignore amplitude fluctuations in ψ = |ψ|eiθ , at least for the purposes of studying the critical properties of the system. We simply set the magnitude of ψ equal to unity. Thus, as in the two-dimensional case all we are left with are phase-fluctuations in ψ, and as always they come in two varieties, longitudinal and transverse.

10.2 Lattice formulation of the Ginzburg–Landau theory Our starting point is the continuum Ginzburg–Landau model. In quantum field theory, the GL model is also referred as the scalar QED or the U (1)+Higgs model or the Abelian Higgs model. For completeness, we also take anisotropy into account, i.e. the effect that the electron transport exhibits uniaxial anisotropy such that motion in the [x, y)-plane is easier than motion along z-axis. The effective Hamiltonian for the Ginzburg–Landau model in an anisotropic system is given by HGL =

2 g d r α(T )|ψ| + |ψ|4 + 2 2mµ µ=x,y,z 1 + (∇ × A)2 2µ0 3

2

2 ∇µ − i 2π Aµ ψ

0

(10.8)

Here, ψ(r) = |ψ(r)|eiθ (r) is a complex order field representing the superconducting condensate. In superconductors, the amplitude |ψ(r)|2 should be interpreted as the local Cooper-pair density. Furthermore, mµ is the effective mass for one Cooper-pair when moving along the µ-direction, 0 = h/2e is the flux quantum, and µ0 is the vacuum permeability. In Eq. 10.8, the gauge field A is related to the local magnetic induction, b(r) = ∇ × A(r). Finally, the Ginzburg–Landau parameter g is assumed to be temperature independent, while α = α(T ) changes sign at a mean field critical temperature TMF (B), where Cooper-pairs start to form. B is the spatial average of the magnetic induction.

LATTICE FORMULATION OF THE GINZBURG–LANDAU THEORY

283

The critical temperature Tc where phase-coherence develops, is in principle always smaller than TMF . Hence, the existence a finite Cooper-pair density does not in itself imply that the system is in a superconducting state. Later on, we shall recast the Ginzburg–Landau theory in a quite different form that also exhibits a U (1)-symmetry, but where the field conjugate to the relevant phase is the number operator for the topological excitations destroying the order of the Ginzburg–Landau theory itself. Although this may seem like an unnecessary complication, it has the advantage of facilitating a detailed discussion of the vortex-liquid phase of the Ginzburg–Landau theory in terms of the ordering of some local field, namely the complex scalar field φ(r) to be introduced below. This is not possible using the Ginzburg–Landau function, ψ(r), since ψ(r) is always zero in the vortex liquid phase. In the zero-field low-temperature ordered phase, the system spontaneously chooses a preferred phase angle , and explicitly breaks the U (1) symmetry. The vortex-sector of the Ginzburg–Landau theory also exhibits a U (1)-symmetry breaking, but where U (1)-symmetry is broken in the high-temperature phase, and restored in the low-temperature phase. Eq. 10.8 has two intrinsic length scales, the mean-field coherence length ξµ2 (T ) =

2 2mµ |α(T )|

(10.9)

and the magnetic penetration depth λ2µ =

mµ β 4µ0 e2 |α(T )|

(10.10)

ξµ is the characteristic length of the variation of |ψ(r)| along the µ-direction, and λµ is the characteristic length of the variation of the current flowing along the µ-direction. In order to carry out Monte Carlo simulations of the Ginzburg–Landau model, the model is discretized by replacing the covariant derivative in the continuum Ginzburg–Landau Hamiltonian (Eq. 10.8), with a covariant lattice derivative,

2π Dµ ψ = ∇µ − i Aµ ψ

0

2π 1 −i aµ Aµ (r) 0 − ψ(r) ψ(r + µ)e ˆ →− Dµψ = aµ

(10.11)

The resulting model has all three spatial directions discretized. The effective Hamiltonian for the lattice Ginzburg–Landau model is given by,

284

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

g HLGL = ax ay az α|ψ|2 + |ψ|4 2 r 2 2π 2 −i aµ Aµ (r) 0 ψ(r + µ)e ˆ + − ψ(r) 2 2mµ aµ µ=x,y,z 1 2 + ( × A)µ 2µ0 aµ2 µ=x,y,z

(10.12)

Here, aµ and µˆ is a lattice constant and a unit vector along the µ-axis, respectively. Furthermore, the lattice derivative is defined as µ ψ(r) = ψ(r + µ) ˆ − ψ(r) Taking the continuum limit aµ → 0, the effective Hamiltonian for the lattice Ginzburg–Landau model Eq. 10.12 reduces correctly to the Ginzburg–Landau effective Hamiltonian in the continuum (Eq. 10.8). As defined in Eq. 10.12, the lattice Ginzburg–Landau model does not contain vortices. To reintroduce the vortices in the model, we must compactify the gauge-theory by requiring that the gauge invariant phase differences satisfy 2π θ (x + µ) ˆ − θ (x) − aµ Aµ (x) ∈ [−π, π

0

(10.13)

Whenever this constraint is used to bring the gauge invariant phase differences back to its primary interval, we automatically introduce a unit closed vortex loop, and the net vorticity of the system is guaranteed to be conserved at every stage of the Monte-Carlo simulation. From the renormalization group point of view the continuum Ginzburg–Landau model and the lattice Ginzburg–Landau model belong to the same universality class. We therefore expect the lattice Ginzburg–Landau model and the continuum Ginzburg–Landau model to give, qualitatively, the same results.

10.2.1

Lattice Ginzburg–Landau model in a frozen gauge approximation

In extreme type II superconductors, the zero temperature mean-field penetration depth is much greater than the zero temperature coherence length, λµ (T = 0) ξµ (T = 0). Thus, fluctuations of the gauge field represented by the last term in Eq. 10.8, around the extremal field configuration are strongly suppressed and can therefore be neglected. The effective Hamiltonian for the frozen gauge (FG)

LATTICE FORMULATION OF THE GINZBURG–LANDAU THEORY

285

model can be written as HFG =

α(T ) |α(0)|2 1 ax ay az |ψ |2 + |ψ |4 g α(0) 2 r +

|ψ (r + µ)||ψ ˆ (r)| 2−2 cos(µ θ − Aµ ) (10.14) 2

ξµ2

a µ=x,y,z µ

Here, we have defined a dimensionless order field and vector potential ψ =

Aµ =

ψ |α(0)| g

→ |ψ | ∼ [0, 1]

2π aµ Aµ

0

The natural energy scale along the µ-direction is, Jµ = 2

ξµ2 |α(0)|2 ax ay az 2 g aµ

Assuming a uniaxial anisotropy along the z-axis, the natural energy scale for the FG model is J0 = Jx =

20 d 2|α(0)|2 2 ξab az = g 4π 2 µ0 λ2ab

(10.15)

Here, we have put our coordinates (x, y, z)-axis parallel to the crystals (a, b, c)axis. Furthermore, ξx = ξy = ξab and ξz = ξc is the coherence length in the CuO-planes and along the crystal’s c-axis, respectively. Furthermore, λx = λy = λab and λz = λc is the penetration depth in the CuO-planes and along the crystals’ c-axis, respectively. In Eq. 10.15, d is the distance between two CuO superconducting planes in adjacent unit cells. The energy scale J0 is roughly the energy scale of exciting a unit vortex loop. The ratio between the energy scales Jx and Jz serves as an anisotropy parameter, ξab az λc az Jx = = (10.16) = Jz ξc ax λab ax In this model, the lattice constant aµ should be defined as aµ = max(dµ , C0 ξµ )

286

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Here, dµ is an intrinsic length along the µ-direction in the underlying superconductor to be modelled. Examples of such an intrinsic length are the distance between CuO-planes in adjacent unit cells, the (a, b)-dimension of the unit cell. To be consistent, the constant C0 should be larger than ∼4. This requirement aµ /ξµ > 4 ensures that the amplitude of the order field does not overlap [142]. Such overlap will give rise to a domain wall term (∇|ψ|), which is absent in the lattice Ginzburg–Landau model. Within the frozen gauge approximation, the gauge field serves only as a constraint, fixing the value of the uniform induction. In terms of magnetic induction this approximation is valid when B Bc1 (T ), where the field distribution from individual flux lines overlap strongly, giving uniform induction. Note that Bc1 (T ) also vanishes when the temperature approaches Tc . In zero field, this approximation is valid for all temperatures except an inaccessibly narrow temperature region around Tc .

10.3 Preliminary results Before we proceed, let us make a few remarks on the neglect of amplitude fluctuations in the type II regime. Is the neglect of such fluctuations in ψ in the above theory defined by Eq. 10.7 really a good approximation? It is well established to be correct in two dimensions. However, as is well known, in four dimensions mean field theory is exact, and in this case amplitude fluctuations alone suffice to correctly describe the phase transition. Three dimensions is between two and four, but is it, in some sense, closer to two dimensions than to four dimensions or vice versa? To answer this, consider the results of largescale Monte Carlo simulations performed directly on the lattice version of the theory defined by Eq. 10.14 in the absence of a gauge field [29]. All phase fluctuations as well as amplitude fluctuations are taken into account, and we now ask ourselves what these various fluctuations do close to the critical point where the superfluid density vanishes. This is shown in Figure 10.1. The Cooper-pair density |ψ|2 behaves quite differently from the superfluid density ϒ and the superconducting order parameter | ψ |2 , in that the former still is quite sizeable at and slightly above Tc , whereas the superfluid density vanishes. We thus conclude that if amplitude fluctuations alone had been capable of describing the phase transition from superfluid to normal fluid or from superconductor to metal, then the Cooper-pair density would have vanished at Tc . It does not, and the superfluid density is brought to zero at Tc by phasefluctuations [29, 31, 32, 143]. We shall now investigate the effect of longitudinal phase-fluctuations first, following the same path as in Chapter 9. As we shall see, longitudinal phase-fluctuations are even more innocuous in three dimensions than in two, whence it follows that the destruction of superfluid density is caused by transverse phase fluctuations.

PRELIMINARY RESULTS

287

0.8

D q (q)

1

ϒz

0.6

0.45 0.4 0.35 0.3 0.25 0.2 0.15 0.1 0.05 0

T′ = 0.1 T′ = 0.2 T′ = 0.3 T′ = 0.4 T′ = 0.5 T′ = 0.56

0

0.4 FG f=0 0.2 Γ=1 T ′MF = 1 0 0

2p

p

q

| < y′ > |2

< |y′|2 >

0.2

0.4

0.6

0.8

1

T′ 1 0.8 ϒz

D q (q)

0.4

0.6

T′= 0.10 T′= 0.14 T′= 0.18 T′= 0.21 T′= 0.22 T′= 0.23

0.3 0.2 0.1 0 0

0.4 FG f=0 Γ=1 T′MF = 0.3

0.2 0 0

| < y′ > |2

2p

p

q

< |y′|2 > 0.1

0.2

0.3

0.4

T′

Figure 10.1 Superfluid density ϒ, superconducting order parameter | ψ |2 (often called condensate fraction in the He4 literature, and Cooper-pair density |ψ|2 . Note how ϒ and | ψ |2 , both of which contain phase-fluctuations, are brought to zero at Tc , while | ψ |2 which does not contain phase-fluctuations, is still finite at Tc . This demonstrates that amplitude fluctuations are not critical at Tc . (adapted from Fig. 1 in Ref. [29]).

As in the two-dimensional case, we may write the effective action when only smooth phase-fluctuations are taken into account, in the form ρ0 S= 2

d3 r (∇θ )2

(10.17)

where ρ0 formally appears as same bare phase stiffness in the problem (analogous to J in the XY -model) which in the above units is given by ρ0 = 1. However, we will retain it in the following in order to remind ourselves of the presence of this bare stiffness in the problem. In the above, it is assumed that ∇θ is non-singular, which means that we ignore the angular (compact) nature of the phase-field θ .

288

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

The following discussion closely parallels that of the low-temperature discussion of the two-dimensional XY -model in Chapter 9. Consider the effect of the longitudinal phase fluctuations in computing the correlation function probing superconducting off-diagonal long-range order (ODLRO), 2 (r) = ψ ∗ (r)ψ(0) = ei[θ (r)−θ (0)]

= e [θ (r)−θ (0)]θ (0) = eG(r)

(10.18)

when only spin-wave fluctuations are included in the Hamiltonian, and where G(r) = [θ (r) − θ (0)]θ (0)

(10.19)

just as in Chapter 9. By using the equipartition theorem precisely in the same way as in Chapter 9, we obtain in the present units kB T G(r) = ρ0

d3 q eiqr − 1 (2π )3 q 2

(10.20)

Of interest for the purposes of establishing ODLRO, is the asymptotic longdistance behaviour of G(r). Compute the above integral by introducing a large momentum cutoff in the problem. It is straightforward to see that G(r) has the following form, r0 r kB T Si() r0 = 2π 2 ρ0 kB T K= 2π 2 ρ0

G(r) = −K +

(10.21)

where r0 is some characteristic length, and Si() = 0 du sin(u)/u is the sineintegral. Note how G(r) again vanishes as T → 0. Now we insert this into 2 (r) to obtain the long-distance behaviour r0

2 (r) = e−K+ r

(10.22)

where the expression for 2 (r) basically applies for r ≥ −1 . It is seen that 2 (r) decreases with r, but it is finite when r → ∞. Moreover, since the entire exponent in 2 (r) is negative, this implies that the correlation function is suppressed with increasing T at fixed r. Eq. 10.22 is drastically different from the two-dimensional case in that the spinwaves are not capable of

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

289

destroying ODLRO at all in three dimensions, whereas they are capable of reducing ODLRO to quasi-long range (but not short-range) order in two dimensions. Hence, as in the two-dimensional case, the fluctuations ultimately responsible for producing short-range order and a transition to a normal fluid/metal, are transverse phase fluctuations. Let us now incorporate them in the description, in much the same way as was done in Chapter 9. There will, however, be crucial differences, since transverse phase fluctuations in three dimensions give rise, not to point-like vortices as in two dimensions, but rather closed vortexloops, considered recently in great detail in the context of high-temperature superconductors by Tesanovic and Sudbø and co-workers [29, 32].

10.4 Vortex-loops as topological defects of the order parameter We will proceed as in the two-dimensional case by regularizing the Ginzburg– Landau theory (Eq. 10.4) on a lattice, ignoring amplitude fluctuations, as follows Z = dθ dAe−S(θ,A) S(θ, A) =

βJ x

J=

1 |( − ieA)e | + ( × A)2 2 2

iθ 2

a|ψ0 |2 m∗

(10.23)

where is a lattice derivative, a is a lattice constant of the numerical lattice, and ψ0 is the amplitude of the ψ-field, which we take to be uniform throughout the system. Finally, we expand the kinetic energy operator as follows

ˆ µ (x) 2 | = 2 1 − cos(µ θ (x) − eAµ (x)) |(µ − ieAµ )eiθ |2 → |eiθ (x+a µ)−iaA (10.24) We ignore the constant term, and set J = 1, thus getting Z = dθ dAe−S S=

−β cos(µ θ (x) − eAµ (x)) + 12 ( × A)2

(10.25)

x

We now follow steps similar to those in Chapter 9, and replace this cosinepotential by a periodic Gaussian one, thus obtaining the partition function

290

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Z=

dθ dAe−S(ψ,A)

n

S=

β x

2

(θ − eA + 2π n)2 + 12 ( × A)2

(10.26)

which is now the Villain-approximation to the three-dimensional lattice London model (i.e. three dimensional XY model coupled minimally to a fluctuating gauge field). Here, we have introduced an integer valued velocity field n, which we may view as the integer part of the gauge-invariant phase-difference θ − ieA. The field n will figure prominently in our discussion below. The kinetic term is linearized, as in Chapter 9, by introducing the Hubbard–Stratonovic decoupling 2 β 2 − v +ivu (10.27) e− 2 u = dv e 2β which allows us to write the partition function of the form Z= dθ dA dv e−S n

1 1 2 2 S= v + iv(θ − eA + 2π n) + ( × A) 2β 2 x

(10.28)

Now, we proceed by performing the θ -integrations. This yields the constraint µ vµi = 0

(10.29)

which is solved by introducing the new vector field hµi satisfying vµi = εµνλ ν hλi

(10.30)

where εµνλ is the three-dimensional Levi–Civita tensor. Now the partition function is given by Z= dA dh e−S n

1 1 2 2 S= ( × h) − i × h(eA − 2π n) + ( × A) (10.31) 2β 2 x By a partial integration of the second and third term in this action, it may be written as 1 1 2 2 S= ( × h) + ieh( × A) − i2π h( × n) + ( × A) 2β 2 x (10.32)

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

291

Next, we perform the sum over n in Eq. 10.31. By the Poisson summation formula, this converts the v-field into an integer valued field, equivalently h becomes integer valued. We will come back in a moment to exactly what the physical interpretation of this new vector field is. As a result of the above, we may write the partition function as Z= dA e−S {h}

1 1 2 2 ( × h) − ie × hA + ( × A) S= 2β 2 x

(10.33)

Now, it is a somewhat awkward fact that while the gauge field A is real valued, the vector field h is integer valued. This may be remedied by again using the Poisson summation formula to lift the field h from Z to R by introducing another integer valued field m in the partition function, thus writing it on the form Z= dh dAe−S {m}

1 1 2 2 ( × h) − ie × hA + ( × A) − i2π mh (10.34) S= 2β 2 x By comparing the action in Eq. 10.34 with the action Eq. 10.32, we arrive at the following physical interpretation of the new vector field m. We see that m=×n

(10.35)

Since n is the integer part of the gauge-invariant phase difference we started with, it is a current. Since m is the curl of this, it is the vorticity of this phase difference. In other words, the fields m are segments of vortex excitations in the superconducting ordering field. Finally, from Eq. 10.35, we see that µ mµi = 0

(10.36)

This means that the vortex segments are divergence free fields, and form closed loops. Thus, we have identified the topological defects in the Ginzburg–Landau model, they are precisely these vortex loops. (Note how the use of the phrase vortex ring is meticulously avoided!) The analogue of the Kosterlitz–Thouless vortex-pair unbinding taking place in the two-dimensional case will now be a vortex-loop unbinding characterized by a low-temperature phase of vortex loops with finite linetension and finite perimeter into a high-temperature phase characterized by vortex tangle with no line tension of the vortex loops, which therefore exist on all length scales up to and including the system size.

292

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Note how there is one feature which distinguishes the three-dimensional situation from the two-dimensional. Vortex–antivortex pairs have one characteristic feature, and that is the separation between the vortex and the antivortex. A vortex loop is an infinitely more complicated object, in that it also has shape. This is the basic feature which precludes the possibility of constructing, in a consistent manner, a Kosterlitz–Thouless style of renormalization group approach to the problem in three dimensions. Next, let us integrate out the electromagnetic gauge field A. We rewrite the action introducing Fourier-modes of the field A as follows 1 ie µ S= |Qq |2 + iπ(mq h−q + m−q hq ) − Aq (Qq × h−q )µ 2β 2 q 1 µ µ + A−q (Q−q × hq )µ + |Q−q A−q |2 (10.37) 2 Completion of squares is accomplished by introducing the auxiliary quantities 1 A+ q = (Aq + A−q ) 2 1 A+ (Aq − A−q ) q = 2i

(10.38)

and ie (Qq × h−q + Qq × h−q ) 2 e 0− = (Q−q × hq − Q−q × hq ) 2 0+ =

(10.39)

As a result of this, the A-part of the action may be written in the form

1 1 + 2 − 2 + 2 − 2 ˜ ˜ [( Q |[( A ) + ( A ) ] − ) + ( ) ] S= |Q q −q 0 0 2 q |Qq Q−q | e2 hq h−q

(10.40) The integrals over the shifted gauge-fields A˜ ± in the partition function are Gaussian and may be performed. Hence, the net result of integrating out these fields is to produce a term in the remaining part of the action which is simply a mass-term for the h-field. Note how the presence of the mass term depends on the existence of a charge e in the problem. In order to interpret this mass, we

VORTEX-LOOPS AS TOPOLOGICAL DEFECTS OF THE ORDER PARAMETER

293

proceed by integrating out the h-field. The remaining part of the action prior to integrating out the h-field now reads 1 e2 Qq Q−q hq h−q + hq h−q (10.41) S= π i(mq h−q + m−q hq ) + 2β 2 q We introduce 1 h+ q = (hq + h−q ) 2 1 h+ (hq − h−q ) q = 2i

(10.42)

along with iπ (m−q + m−q ) 2 e − 0 = 2 (mq − m−q )

1 2 Qq Q−q e + ξ2 = 2 β + 0 =

(10.43)

Introducing these variables into the action and completing squares, we get + 2 − 2 0 0 1 1 − 2 2 ξ 2 h+ S= + h− − 2 ((+ (10.44) q 2 q 2 0 ) + (0 ) ) 2 q ξ ξ ξ The shifted h field may now be integrated over, to give the final form of the action in terms of an interacting gas of closed vortex loops as follows mq m−q (10.45) S=β 2 e β + Qq Q−q q This may be written in term of real-space vortex segments interacting with a potential in terms of the following Hamiltonian, to be used in the partition function H = −2π 2 J0 m(x1 )V (x1 − x2 )m(x1 ) x1 ,x2

V (x) =

q

4

µ

where λ−2 = e2 β.

e−iqr sin2 (qµ /2) + λ−2

(10.46)

294

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

We now see that the mass e2 of the gauge-field h shows up as a screening length in the interaction between vortex segments. The charge in the original problem, i.e. the charge of the superconducting condensate, leads to short-range interactions between the vortex-loop segments. Setting the charge equal to zero in the above, we obtain an equivalent description of a neutral superfluid, such as He4 . The gauge field decouples from the order parameter in Eq. 10.25, and can simply be ignored as it gives rise to an additive analytic contribution to the free energy. The remaining model is the three-dimensional XY model. It may be written in terms of vortex-loop segments following the steps we have just gone through, and the result is Eq. 10.46 with screening length set to infinity. This means that the potential V (x) is the unscreened Coulomb potential in three dimension. Note that such a potential satisfies the Laplace equation −∂ 2 V (xx) = δ(x) in the continuum. Let us rederive the above result for the neutral case in an alternative manner following what we did in Chapter 9. In the continuum limit the threedimensional XY model may be written as J0 d3 r(∂θ )2 H= 2 J0 d3 r (∂θL )2 + (∂θT )2 = (10.47) 2 Again, we have split the gradient of the phase into a regular spin-wave part ∂θL and a part ∂θT giving rise to vortex segments. The latter part satisfies the equation εµνλ ∂ν (∂λ θT ) = 2π nµ where nµ (r) is a local vorticity in the µ-direction, and εµνλ is the threedimensional Levi–Civita tensor. A representation of (∂µ θT ) that satisfies this equation is the following (∂µ θT ) = −2π εµνλ ∂ν d3 r G(r − r )nλ (r ) (10.48) where G(r) is a solution to the three-dimensional Laplace equation, −∂ 2 G(r) = δ(r). The verification of this follows the lines given for the two-dimensional case in Chapter 9. If we now insert this representation into Eq. 10.47, using the Laplace equation for G(r) and the fact that ενλρ ενησ = δλη δρσ − δλσ δρη , we find J0 3 2 2 3 d r(∂θL ) + 2π J0 d r d3 r nµ (r)G(r − r )nµ (r ) (10.49) H = 2 Here, we have used a partial integration in the second term along with the fact that ∂µ nµ (r) = 0. The above describes a system of spin waves decoupled from

SUPERCONDUCTOR–SUPERFLUID DUALITY IN d = 3

295

a system of vortex segments forming closed loops and interacting with a threedimensional unscreened Coulomb potential (anti Biot–Savart law). Eq. 10.49 is therefore the continuum version of Eq. 10.46 with no screening, λ = ∞, when the spin-wave part is ignored. Coupling between spin waves and vortices are seen to be higher-order gradient terms and are therefore, as in the two-dimensional case, irrelevant in renormalization group sense.

10.5 Superconductor–superfluid duality in d = 3 In this section, we will formulate a Ginzburg–Landau theory for the above action for the system of interacting vortex segments forming closed loops. This Ginzburg–Landau theory is therefore a field theory of the ensemble of topological defects of the original Ginzburg–Landau theory of the superconductor, and hence a dual theory to the original system. Incidentally, we note in passing that we can also describe superfluidity in He4 simply by setting the charge e = 0. We shall now demonstrate that the dual theory to the Ginzburg–Landau theory of a superconductor is the Ginzburg–Landau theory of a charge-neutral superfluid, and vice versa. The details are as follows. The key point is to compare two equations derived above from the original Ginzburg–Landau theory. The two equations we compare are Eqs 10.28 and 10.32, written out in real space as follows

DA

Z(β) =

v

Z(β) =

Dh

m

exp − exp −

v2 x

1 − ivA + (∇ × A)2 2β 2

m2 x

2

e2 1 + 2π imh + h2 + (∇ × h)2 2 2β

(10.50) The first of these is Eq. 10.28 after having performed the θ -integrations and nsum. The second equation is Eq. 10.32 written in real space, with a term h2 /2 added by hand. The crucial observation now is that Eq. 10.28 is basically a version of the original Ginzburg–Landau model! Eq. 10.32 on the other hand, is a version of the vortex-loop gas formulation of the model. The point to note is that the action in these two partition functions are basically identical, provided we make the identification 1 2 v → h2 2β 2 1 1 (∇ × A)2 → (∇ × h)2 2 2β −bA → 2π mh

(10.51)

296

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Adding the extra term h2 /2 in the second of Eq. 10.50 is like adding a short-range interaction between vortex segments. This is an irrelevant perturbation, in renormalization group sense, to the already existing short-range piece of the interaction between vortex segments, and is not expected to alter the long-distance physics. Now, since we know that the first of the two equations Eq. 10.50 corresponds to a Ginzburg–Landau theory, it follows that the second one also does so. In the continuum limit, the field theory description of the second of Eq. 10.50 is therefore of a form [29, 32, 144, 145]

S(h, φ) =

d3 x

1 e2 (∇ × h)2 + h2 + m2φ |φ|2 + uφ |φ|4 + |(∇ − ied )φ|2 2β 2

(10.52) The field φ is a complex matter field describing the vortex segments of the theory, in the same way that the field in the original Ginzburg–Landau theory was a a matter field describing Cooper-pairs giving rise to segments of supercurrents. Moreover, ed = 2π in the units we are working with here. It has the interpretation of being a dual charge coupling the vortex segments, or equivalently the matter field φ, to the gauge-field h which mediates the (anti) Biot–Savart interaction between vortex segments. Finally, the term m2π |φ|2 is a local chemical potential term for the vortex segments, while the term uφ |φ|4 represents a steric repulsion between vortex segments. Eq. 10.52 is of the same form as Eq. 10.4 except for the mass term e2 h2 /2 of the gauge-field h. Note that if we had started out with a neutral theory in Eq. 10.4, e = 0, we would have ended up with a dual theory Eq. 10.52 of the same form as Eq. 10.4 with finite charge e. Hence, the dual theory of a superfluid in d = 3 is immediately seen to be the Ginzburg–Landau theory of a superconductor. To see the converse, namely that the dual of a superconductor is a neutral superfluid, is only slightly more involved. A physically intuitive argument proceeds as follows (more involved arguments involving renormalization group calculations merely confirm the correctness of the physical picture we shall give). In the presence of a finite charge in Eq. 10.4, the gauge field h in Eq. 10.52 is massive. This means (in complete analogy with, for instance, the massive meson-field mediating short-range nuclear interactions) that when e2 = 0, the gauge field mediates a short-range interaction between vortex segments, with range given by e−1 . Now, by the dimensional analysis leading to Eq. 10.5, charge has a positive scaling dimension when d = 3, whence ∂e2 >0 ∂l

(10.53)

Thus, for the purposes of describing the long-distance physics, we may set the renormalized effective charge liml→∞ e2 (l) = ∞ once the bare charge is non-zero. This means that on long length scales the gauge-field is suppressed

SUPERCONDUCTOR–SUPERFLUID DUALITY IN d = 3

297

completely in the action and may be discarded. The physics of this is that the short-range Biot–Savart interaction is an irrelevant perturbation to the steric repulsion represented by the term uφ |φ|4 . Hence, the long-wavelength physics is described correctly by Eq. 10.52, but with h removed from the action, namely S(φ) =

d3 x m2φ |φ|2 + uφ |φ|4 + |∇φ|2

(10.54)

This is nothing but the Ginzburg–Landau theory of a neutral superfluid. Thus, the dual of a three-dimensional superconductor is a three dimensional superfluid. Another point to note here, as a consistency check, is the following. Suppose we start out with a superconductor and dualize it once. The resulting dual action is that of a neutral superfluid. Suppose now that we dualize once more. This means that we are out to obtain the dual of the dual of a superconductor, which is the dual of a neutral superfluid. This, as we have seen, is just a superconductor. Hence, dualizing twice brings us, quite correctly, back to the starting point, Dˆ 2 = 1, where Dˆ is the duality operator. Based on the above, we can immediately infer that a vortex-loop tangle consisting of non-interacting vortex segments (a very peculiar case, admittedly, but as we shall see not entirely academic), is simply described by the Gaussian field theory S(φ) =

d3 x m2φ |φ|2 + |∇φ|2

(10.55)

The essential content of the above is shown in Figure 10.2. Observe the isomorphism along both the diagonals. Of course what is dual, and what is original theory eventually becomes a relative notion.

Duality transformation Original charged S(y, A)

Dual neutral S(f)

Original neutral S(y)

Dual charged S (f, h)

Figure 10.2 The relations between charged and neutral versions of the original and dual theory. The dashed lines indicate isomorphism.

298

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

10.6 Zero-field vortex-loop blowout Consider now for the moment the case of zero magnetic field. The main advantage of the above formulation is that the probability of finding a connected path of vortex segments, starting at x and ending at y, G(x, y), is given by the two-point correlation function of the φ-field [145] G(x, y) = φ ∗ (x)φ(y)

(10.56)

A vortex-loop unbinding will lead to a finite G(x, y) when |x − y| → ∞, because infinitely large loops will connect opposite sides of the vortex system. On the other hand, if lim|x−y|→∞ G(x, y) = 0, this implies that φ ∗ (x) = 0, corresponding to a broken U (1)-symmetry. Therefore, the dual field φ(r) is an order parameter of a vortex-loop unbinding transition. The broken U (1)-symmetry is associated with the loss of number conservation of connected vortex-paths threading the system in any direction (including direction perpendicular to an applied magnetic field, if that is present). This limit of the two-point correlation function is closely related to a quantity OL we will introduce below, which probes the connectivity of the vortex tangle in an extreme type II superconductor. The above connection makes it at the very least plausible that an abrupt change in this connectivity, as probed by the change in OL , is associated with breaking a U (1)-symmetry of the vortexsector of the GL-theory, equivalently an onset φ ∗ or φ . Since this only happens above a critical temperature, we may view φ as a disorder-field, in contrast to the order-parameter field ψ of the original GL-theory. We will make explicit use of this connection later on. In zero magnetic field, we will show that the loss of superfluid density, specific heat anomaly, change in vortex-loop distribution, loss of long-wavelength vortex-line tension, and abrupt change in vortex tangle connectivity abruptly occurs precisely at the same temperature both for the three-dimensional XY model, also when amplitude fluctuations are included. Thus we may associate the the phase transition from superconductor to normal metal or neutral superfluid to normal fluid (such as the λ-transition in H e4 ) as a vortex-loop blowout. The idea of a vortex-loop blowout being responsible for the λ-transition in He4 (also denoted helium II) must be credited to Onsager [146]. Ref. [146] is a discussion remark from as early as 1949, and the two last sentences of the remark are well worth quoting: ‘Finally, we can have vortex rings in the liquid, and the thermal excitation of Helium II, apart from the phonons, is presumably due to vortex rings of molecular size. As a possible interpretation of the λtransition, we can understand that when the concentration of vortices reaches the point where they form a connected tangle throughout the liquid, then the liquid becomes normal’. This is qualitatively the right idea. Note, however, how we have meticulously avoided the use of the phrase ‘vortex rings’ in our treatment, and used the phrase ‘vortex-loops’ instead. Vortex rings are precisely

299

ZERO-FIELD VORTEX-LOOP BLOWOUT

that, namely rings, while vortex-loops can have much more complicated shapes, being crinkled to a degree that one cannot speak even crudely of ring-like shapes, the hole in the doughnut is in fact completely filled in. This is an essential feature, since it endows the vortex loops with enough configurational entropy to be able to overcome the internal energy such that the line tension of the vortices, which is the free energy per unit length, may be driven to zero. An object that on large length scales looks like a ring, will have a Hausdorff dimension of 1. As we shall see in this chapter, however, the vortex-loop tangle arising out of a neutral superfluid has Hausdorff dimension larger than 2. For a superconductor, the Hausdorff dimension of the vortex-loop tangle is slightly smaller than 2. In any case, it is clear that one cannot speak of ring-like objects. The truly remarkable thing about Onsager’s vision from 1949, is that he correctly identified the nature of the topological defects in the order parameter which are responsible for driving the phase transition. The idea (as so many of Onsager’s ideas) was far ahead of its time, and there was no hope of putting them on a quantitative level back in 1949. Only with the advent of the Kosterlitz–Thouless theory in 1973 [130, 131] was the much simpler problem of vortex–antivortex unbinding tackled in two dimensions! Note that if one takes a vortex loop and slices through it with a plane, the loop cuts the plane in two places, which are the locations of a vortex and an antivortex. Hence, the two-dimensional counterpart of Onsager’s vortex-loop blowout is the vortex-antivortex unbinding of Kosterlitz and Thouless.

10.6.1

Definitions

Specific heat C To calculate the specific heat per site C, we use the fluctuation formula, 1 H 2 − H 2 C = . kB V (kB T )2

(10.57)

Here, the dimensionless volume V = Lx Ly Lz , and Lµ is the dimensionless linear dimension of the system along the µ-direction. Lµ is measured in units of the lattice constant aµ . As a check of consistency, we may also calculate the specific heat per site using the numerical derivation of the internal energy U , CU =

1 ∂U V ∂T

(10.58)

Note that for the FG model, where the effective Hamiltonian depends explicitly on the temperature, there strictly speaking is an additional term in the expression

300

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

for the internal energy,

∂ ln Z ∂H U =− = H − T ∂β ∂T

∼ For the three-dimensional XY model, if the simulations are properly done, C = CU . For the FG model, where the effective Hamiltonian explicitly depends on the temperature, C = CU . Note however that ∂H /∂T arises out of introducing a temperature dependence of the coefficients of the Ginzburg–Landau theory. The temperature dependence of these coefficients always has a temperature dependence set by the mean-field critical temperature. Thus, close to the true Tc these corrections, arising from integrating out the fermions of the underlying microscopic description of the superconductor, are always negligible compared to the contribution coming from the true critical fluctuations of the order parameter, i.e. the transverse phase-fluctuations. In terms of Eq. 10.15 the term −T ∂H /∂T

originates from the temperature dependence of the amplitude of the orderparameter. Were this to actually vanish at T = Tc , substantial corrections to the specific heat and entropy would result. As we will see later, at T = Tc , the ensemble average of the amplitude of the order parameter is far from renormalized to zero by vortex-loop fluctuations. Hence, at the critical point the correction term −T ∂H /∂T in the internal energy, with its resulting corrections to entropy, is negligible. There is now ample experimental evidence from the group of Ong at Princeton [147], that critical fluctuations are indeed important over a sizeable temperature window in the high-Tc cuprates of order several Kelvin below Tc a window which is consistent with a coherence length of order 10 ˚A, about two orders of magnitude shorter than in conventional superconductors. Local Cooper-pair density |ψ |2 As a probe for the local Cooper-pair density, we calculate |ψ |2 ≡

1 |ψ (r)|2

V r

(10.59)

We see in Eq.√10.59 that |ψ |2 involves both thermal and space average. Recall that ψ ≡ ψ/ |α(0)|/g. At the mean field level, we expect |ψ |2 to develop an expectation value below the mean field critical temperature TMF (B). Superfluid condensate density |ψ |2 As a probe for the local condensate density (density of Cooper-pairs participating in the superconducting condensate), we calculate | ψ |2 ≡

1 | ψ (r) |2 V r

(10.60)

ZERO-FIELD VORTEX-LOOP BLOWOUT

301

Note the difference between |ψ |2 and | ψ |2 . The former describes local Cooper-pair density, while the latter describes what is commonly known as the condensate density in 4 He-physics. In zero field, we expect | ψ |2 to develop an expectation value below the critical temperature Tc . Distribution of the order field phase angle To probe the distribution of the phase angle in ψ (r) = |ψ (r)|eiθ (r) , we define the distribution function ! 1 (10.61) δθ (r),θ Dθ (θ ) = V r Here, δi,j is the Kronecker delta function. In the simulations, we have chosen to work with a discrete set of phase angles, θ , θ (r) = 2π n/Nθ . Here, n ∈ [0, Nθ ] is an integer, and Nθ is the number of allowed discrete phase angles. In our > experience, the simulation results do not depend on Nθ , provided Nθ ∼ 16. In zero field, when the phase is disordered, we expect Dθ (θ ) to be uniformly distributed, D(θ ) = 1/Nθ . In the ordered phase, we expect Dθ (θ ) to show a peak around a preferred phase angle. Helicity modulus ϒµ To probe the global superconducting phase coherence across the system, we consider the helicity modulus ϒµ , defined as the second derivate of the free energy with respect to an infinitesimal phase twist in the µ-direction. Finite ϒµ means that the system can carry a supercurrent along the µ-direction. Within the three-dimensional XY-model, the helicity modulus along the µ-direction becomes, ! ϒµ 1 = cos[µ θ − Aµ ] Jµ V r 2 ! Jµ . sin[µ θ − Aµ ] − kB T V r For the FG case, ! ϒµ 1 = |ψ (r)||ψ (r + µ)| ˆ cos[µ θ − Aµ ] Jµ V r 2 ! Jµ . − × |ψ (r)||ψ (r + µ)| ˆ sin[µ θ − Aµ ] kB T V r

302

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Note the difference between | ψ |2 and ϒµ , they are not identical. The former quantity probes the superfluid condensate density, which is a locally defined quantity, while the latter quantity probes a global phase coherence along a given direction µ. Since ψ is the order parameter of the Ginzburg–Landau theory, close to the critical point we have | ψ |2 ∼ |τ |2β

(10.62)

where τ = (T − Tc )/Tc . On the other hand, ϒµ ∝ ρsµ , where ρsµ is the superfluid density in the µ-direction. Using the Josephson scaling relation ρsµ ∼ ξ 2−d ∼ |τ |ν(d−2) along with the scaling laws γ = ν(2 − η) and 2β = 2 − α − γ , we find ϒµ ∼ |τ |2β−ην

(10.63)

Here, d is the dimensionality of the system, ν is the correlation length exponent of the system, β is the order parameter exponent, γ is the order parameter susceptibility exponent, and η is the anomalous dimension of the order parameter two-point correlation function at the critical point. Therefore, although | ψ |2 and ϒµ are in principle different, they may appear to be very close if the anomalous dimension η of the ψ-field is small, as indeed is the case for the Ginzburg–Landau theory, where η ≈ 0.04. Note that for η > 0, the curve for ϒµ should bend more sharply towards zero at the critical point than | ψ |2 . We will explicitly show by direct calculations within the Ginzburg–Landau theory that | ψ |2 is very close to ϒµ both in zero field and finite magnetic field. In zero magnetic field this is precisely what one would expect based on the above, when η 1. For the special case of d = 3, we have 2β − ην = ν < 2β. To high precision, we have for the three-dimensional XY -model, that ν = 0.673 and η = 0.038. Vortex loop distribution D(p) To probe the typical perimeter L0 (T ) and the effective long-wavelength vortexline tension ε(T ) (not to be confused with the flux-line tension, which is always zero when gauge-fluctuations are completely suppressed due to the absence of tubes of confined magnetic flux), we define a vortex-loop distribution function D(p), which measures the ensemble-averaged number of vortex-loops in the system having a perimeter p. In order to compare results from different system sizes, we normalize D(p) with respect to the system size. We search for a vortex-loop using the following procedure. Given a vortex configuration, we start with a randomly chosen unit cell with vortex segments penetrating its plaquettes. We follow the directed vortex path and record the trace. When the directed vortex path encounters a unit cell containing more than one outgoing direction, we choose the outgoing direction randomly. When

ZERO-FIELD VORTEX-LOOP BLOWOUT

303

the vortex path encounters a previously visited unit cell, i.e. when it crosses its own trace, we have a closed vortex loop, its perimeter being p. We now delete the vortex-loop from the vortex configuration, to prevent double counting, and continue the search. The search is continued until all vortex segments are deleted from the system. Using a three-dimensional non-interacting boson analogy to the vortex system, it can be shown that the distribution function D(p) can be fitted to the form ε(T )p D(p) = Ap−α exp − (10.64) kB T Here, A is a temperature-independent constant, and the exponent α ≈ 5/2 to a first approximation. When ε(T ) is finite, there exists a typical length scale L0 = kB T /ε for the thermally excited vortex loops. The probability of finding vortex loops with much larger perimeter than L0 is exponentially suppressed, according to Eq. 10.64. When ε = 0, D(p) decays algebraically, and the length scale of the problem L0 = kB T /ε(T ), has diverged. As a consequence, configurational entropy associated with topological phase-fluctuations is gained without penalty in free energy. In zero field, there is only one critical point, and in this case L0 must be some power of the superconducting coherence length ξ(T ). Probe of vortex-connectivity, OL For probing the connectivity of a vortex tangle in a type II superconductor, in zero as well as finite magnetic field, we introduce a quantity OL , defined in zero magnetic field as the probability of finding a vortex configuration that can have at least one connected vortex path threading the entire system in any direction. In the presence of a finite magnetic field, OL is defined as the probability of finding a similarly connected vortex path in a direction transverse to the field direction, without using the PBC along the field direction. In zero field, we use the same procedure as in the finite-field, namely searching for connected vortex paths perpendicular to the z-direction, although in this case we could just as well have used any direction. Note that OL is very different from the winding number W in the two-dimensional boson analogy. There, W is proportional to the number of vortex paths percolating the system transverse to the field direction. However, in the calculation of W , the PBC along the field direction is used many times. This is entirely consistent with a number of other Monte Carlo simulation results on the three-dimensional XY -model which all show the loss of longitudinal phase-coherence and onset of longitudinal dissipation precisely at the vortex lattice melting transition. This is measured simply by the helicity modulus ϒz , which is quite different from OL . To the contrary, in our calculation of OL , we do not allow for the use of periodic boundary conditions in the z-direction to

304

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

measure vortex-tangle connectivity in the x- or y-directions. We have OL =

Nc Ntotal

(10.65)

Ntotal is the total number of independent vortex configurations provided by the Monte Carlo simulation. Furthermore, Nc is the number of vortex configurations containing at least one directed vortex path that traverses the entire system perpendicular to the direction, without using the PBC along the field direction. For convenience, we treat the zero field case as the limit limB→0 keeping the ‘field direction’ intact. We search for the possibility of finding a vortex path such as described above by using the following procedure. Assume that the magnetic induction points along the z-axis. We follow all paths of directed vortex segments starting from all four boundary surfaces with surface normal perpendicular to zˆ , and check whether at least one of these vortex paths percolates the system and reaches the opposite surface, without applying the PBC in the z-direction. Note that when crossing vortex segments are encountered, the procedure is to attempt to continue in a direction that will bring the path closer to the opposite side of the system, rather than randomly resolving the intersection. OL is therefore a necessary, but not sufficient condition for finding an actual vortex path crossing the system. However, in zero field this procedure does not make a difference to that of resolving the intersections randomly. This is demonstrated by the correlations of the change in OL and D(p), to be detailed in the next section. If a vortex path is actually found crossing the system in any direction in zero field, or without using PBC in the field-direction when a field is present, one may safely conclude that the vortex-line tension has vanished. If it were finite, it would not be possible to find such a path at all, either because all vortex-lines form closed confined loops in zero field, or because the vortex-line fluctuations along the field direction would be diffusive in finite field. In zerofield, this is clear by the above mentioned correlation between the change in OL and D(p), cf. the results of the next section. In this paper, we also investigate this in detail for the finite-field case, by considering the position of the lowest temperature TL where we have OL = 1 both as a function of system size and aspect ratio Lx /Lz = Ly /Lz . If vortex-line physics remains intact, TL should move monotonically up with system size, and should scale with Lx /Lz . Instead, we will find that TL moves down slightly, and saturates with increasing system size at fixed aspect ratio. In addition, we find that TL is virtually independent of aspect ratio for large enough systems. In the VLL phase OL = 0, since the field induced flux lines are well defined and do not ‘touch’ each other, and the thermally excited vortex-loops are confined to sizes smaller than the magnetic length. OL = 1 in the normal phase

ZERO-FIELD VORTEX-LOOP BLOWOUT

305

above the crossover region where the remnant of the zero field vortex-loop blowout takes place. Needless to say, it is a matter of interest to investigate precisely where OL changes value from zero to one. Note that OL itself is not a genuine thermodynamic order parameter, although it may be said to probe an order-disorder transition [29]. However, by the transcription of the vortex-content of the Ginzburg–Landau theory to the form of Eq. 10.52, it is brought out that probing the vortex-tangle connectivity by considering OL is closely connected to probing the two-point correlator of a local complex field φ(r), the dual field of the local vorticity-field mµ (r) of the Villain approximation and London approximation to the Ginzburg–Landau theory (Eq. 10.26). The two-point correlator φ ∗ (r)φ(r ) is ultimately the probe of whether or not the φ-theory (Eq. 10.52) exhibits off-diagonal long-range order and a broken U (1)-symmetry. An entirely equivalent interpretation of the change in OL does not involve a local field φ(r), but rather number conservation of vortex-lines threading the entire superconductor. This number is conjugate to the phase-field of the local complex field φ(r). An advantage of the present formulation involving Eq. 10.52 is that it directly relates he change in OL to the long-distance part of a correlation for a local field, and hence to a local order parameter φ(r) . This connection makes it at least plausible that the change in vortex-tangle connectivity, i.e. a change in the geometry of the vortextangle, may be related to a thermodynamic phase-transition. This is illustrated in Figure 10.3, where it is shown that the anomaly in the specific heat, the loss of superfluidity and the change in OL all occur at the same temperature. 3.5 3DXY f=0 Γ=7

3.0 2.5 2.0

C/k B

1.5 ϒz

1.0 0.5

OL 0 0

0.5

1.0

1.5

2.0

2.5

T′

Figure 10.3 Specific heat capacity C, helicity modulus ϒz and vortex-connectivity probe OL as functions of temperature. Note how the the anomaly in C, the vanishing of ϒz , and the onset of OL all occur at the same temperature.

306

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

10.7 Fractal dimension of a vortex-loop tangle One great advantage of the dual field theory formulation of the previous section is that it allows us to obtain information about critical exponents of the (dual) field theory by investigating geometric properties of the vortex-loop tangle. To see this, we first introduce the quantity P (x, y, N ) which is the probability of being able to perform a walk from the point x to the point y via a connected path of vortex segments in precisely N steps. Now, from this we can can derive several useful quantities. The one we shall focus on here is the probability distribution D(N ) of finding vortex loops of perimeter N . This is nothing but the probability of starting in point x and ending up in the same point in N steps, summed over all possible starting points x along the closed loop, normalizing to the number of starting points along the loop, which is just N . That is, we have D(N ) ∝

1 P (x, x, N ) ∝ N −α N x

(10.66)

This relation defines the geometric exponent α describing the vortex-loop tangle. (It should not be confused with the specific heat exponent.) Note also that all contributions in the above sum are equal, by translational invariance. Hence, we may pick out an arbitrary contribution to the sum, and invert to obtain P (x, x, N ) ∝ N 1−α

(10.67)

Note also that we have so far been careful to denote the configurations of vortex segments closing on themselves as vortex-loops, not vortex-rings. In fact the loops we are describing turn out to be highly crinkled line-objects which do not resemble rings at all. They are instead fractal objects with a Hausdorff dimension DH that can be computed from α. Not only that, but we may compute the anomalous scaling dimension ηφ for the dual matter field φ, from α. Let us demonstrate explicitly how this close connection between geometry and criticality in superconductors and superfluids can be found. Let us start with the simplest case, that of a tangle of non-interacting vortex segments. Then an analytic exact expression for P (x, x, N ) would be given by

1 (x − y)2 P (x, y, N ) ∝ d exp − (10.68) N N 2 with = 1/2. In analogy with this, we write down a scaling Ansatz for P (x, y, N ) for the general case of interacting loops as follows

|x − y| 1 (10.69) P (x, y, N ) ∝ d F N N 2

307

FRACTAL DIMENSION OF A VORTEX-LOOP TANGLE

where F is some scaling function and is some exponent, often called the wandering exponent, to be determined. This exponent is defined via the relation between the linear extent L of a walk and the number of steps N in the same walk, namely L ∼ N (10.70) Conversely, the number of links in a path of linear extent L is given by N ∼ L1/ ∼ LDH

(10.71)

where DH is the so-called Hausdorff dimension, or fractal dimension, of the vortex-loop tangle in the thermodynamic limit. For the non-interacting case, it can be shown that DH = 2. This follows immediately from what we have stated above, DH = 1/ = 2. If we merely add a steric repulsion to this, passing from Eq. 10.55 to Eq. 10.54, the effect must surely be to push vortex segments apart, thus reducing the Hausdorff-dimension, hence for this case we have DH < 2. Physically, this corresponds to the dual case of a charged three-dimensional superconductor. On the other hand, if we start out with a neutral superfluid, then the correct dual description is given by Eq. 10.52 with e2 = 0. In this case, in addition to having a steric repulsion between vortex segments we also have a long-range anti-Biot–Savart interaction between vortex segments. This latter interaction tends to produce a long-range attraction between vortex segments that are oppositely directed. This interaction will tend to compress the vortex tangle compared to the case with only steric repulsion. Moreover, we expect the long-range interaction to overcompensate the dilution of the tangle produced by the local steric repulsion such that in fact the tangle is even more compact than the non-interacting case. Thus, we expect that for the dual of a three-dimensional neutral superfluid, DH > 2. The various cases described above are illustrated in Figure 10.4.

Charged condensate

Gaussian loops

Neutral condensate

Figure 10.4 A schematic illustration of vortex loops in three cases. The three fractal dimenG < D (e = 0), where D G is the fractal sions are ordered according to: DH (e = 0) < DH H H dimension corresponding to a Gaussian field theory, i.e. random loops. Qualitively the three loops are self-avoiding, random and self-seeking.

308

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

We will be interested in the scaling function for |x − y| = 0. By combining Eqs 10.67 and 10.69 we find by simple inspection the scaling relation d = 1 − α

(10.72)

Let us now connect these geometrical properties of the vortex-loop tangle to statistical physics and critical properties. To do this, we consider the two-point correlation function for the dual field φ(x). We have G(x, y) = φ(x)φ ∗ (y)

(10.73)

This correlation function (propagator) is nothing but the probability amplitude of going from the point x to the point y via any connected vortex path. Hence, we have P (x, y, N ) (10.74) G(x, y) ∝ N

The sum over N in Eq. 10.74 cannot be performed exactly; however we will now focus on long loops such that the discrete character of the excursions of the vortex segments on the lattice can be neglected. We therefore replace the sum by an integral such that

1 (|x − y|) 1 G(x, y) ∼ dN d F (10.75) = N N 2 |x − y|d−1/ Close to criticality, on the other hand, we have the standard scaling Ansatz for the two-point correlation function G(x, y) ∼

1 |x − y|d−2+ηφ

(10.76)

which defines the anomalous scaling dimension ηφ . By comparing Eqs 10.72, 10.71, 10.75, and 10.76 we obtain the following scaling relations connecting geometric exponents of the vortex tangle to critical exponents of the dual field theory d =α−1 DH ηφ + DH = 2

(10.77)

For computational purposes it is most convenient to compute the geometric exponent α in simulations. The reason is that this quantity appears to have less finite-size effects than for instance those observed in direct computations of DH . However, once α is determined, DH and ηφ follow.

309

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

Table 10.1 Value of the loop-size distribution exponent, as determined from simulations Exponent

Gaussian

e=0

e = 0

α DH ηφ

5/2 2 1/2 0

2.312 ± 0.003 2.287 ± 0.004 0.437 ± 0.001 −0.287 ± 0.004

2.56 ± 0.03 1.92 ± 0.04 0.52 ± 0.01 0.08 ± 0.04

Limit α>2 DH < 3 > 1/3 ηφ > −1

The remaining exponents have been calculated using scaling relations Eq. 10.77. Gaussian results are exact, and confirmed for the different exponents independently.

In Table 10.1 we show results of large-scale Monte Carlo simulations [148] where the vortex-loop distribution exponent α has been computed, and scaling relations used to derive DH and ηφ . The qualitative picture described is Eq. 10.71 is confirmed by the results shown in Table 10.1. For the original charged case e = 0, corresponding to a dual theory which only features a steric repulsion, we indeed find DH 2, ηφ 0, while for the original neutral case corresponding to the dual charged case, we find DH 2, ηφ 0.

10.8 Type I versus type II, briefly revisited In this section, we will revisit the issue of type I versus type II superconductivity [45, 149]. As we have noted earlier, the distinction between the two is given in terms of the Ginzburg–Landau parameter κ = λ/ξ . At the mean-field level, the value of κ separating type I from type II behaviour is given by 1 κ=√ 2

(10.78)

Note also that when we speak of stable vortices as excitations in a superconductor, we are implicitly talking about type II superconductors. The reason is that in type I superconductors, vortices are not stable. This is due to the fact that for too small values of κ, the vortex-attraction of range ξ , overwhelms the vortexrepulsion due to circulating currents around each individual vortex, a repulsion of range λ. Alternatively, therefore, type I and type II superconductors can be viewed as superconductors where vortices interact attractively and repulsively, respectively. In this section, we start out with the Ginzburg–Landau model once again, but unlike the type II case studied in previous sections of this chapter, we do not ignore amplitude fluctuations of the superconducting order parameter. What we shall find is that the value of κ that separates type I from type II behaviour

310

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

is not precisely given by the mean-field estimate, but rather by [45, 149] κ=

0.76 ± 0.04 √ 2

(10.79)

This may be seen by reasoning as follows. We start out by performing large-scale Monte Carlo simulations on the full Ginzburg–Landau model, including amplitude fluctuations and phase-fluctuations in , as well as gauge-field fluctuations. As the system is warmed up, it passes from a low-temperature superconducting state to a high-temperature disordered state with no Meissner effect, which we obviously identify as the normal state. Now, we may compute the latent heat of this phase-transition as a function of κ. A first order phase transition has a non-zero latent heat, i.e. a jump in the entropy of the systems across the transition, whereas a second order phase transition does not. What is found is that the latent heat is finite deep in the type I regime, κ 1. The latent heat is zero deep in the type II regime, κ 1. The latent heat is found to vanish at a critical value of κ κ = κtri

(10.80)

where the numerical value is given in Eq. 10.79. We have denoted this critical value of κ by κtri , since it is the value that separates a first order phase transition from a second order one. A critical endpoint terminating a first order phasetransition line and where a second order phase-transition line commences, is a tricritical point. The above numerical result is in rather remarkable agreement with an early analytical calculation [144], which gave √ 3 3 4 " π #4 0.798 (10.81) κtri = 1− = √ 2π 9 3 2 Now, let us use the results of the previous sections to connect this change in character of the phase transition, from a first order to a second order on the one hand, to the notion of type I and type II superconductivity on the other. We will follow the discussions of Refs. [45, 149]. Because the critical fluctuations in a superconductor are vortex-loops, criticality at the phase transition from the superconducting state to the normal metallic state requires stable vortices to exist. I. e. they must interact repulsively. By the previous discussion, this requires the vortex tangle to have Hausdorff dimension DH ≤ 3 [148, 45]. A Hausdorff dimension equal to 3 would imply that the vortex tangle fills space in a compact manner, which is just another way of stating that the vortex system has collapsed on itself. Hence, if we were to monitor the vortex-loop distribution function in the first order regime, we would find DH = 3. By the scaling relation DH + ηφ = 2, we would conclude that ηφ = −1. Now, we may use the well-known Rushbrooke scaling law

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

311

2β = ν(d − 2 + ηφ ) to conclude that the order parameter exponent β = 0. That is, the order parameter vanishes discontinuously, the hallmark of a first order phase transition. On the other hand, for repulsive vortex interactions and a stable vortex tangle, DH < 3, ηφ < 1, and β > 0. This means that the superconducting order parameter vanishes in a continuous fashion, which is the hallmark of a second-order phase transition. Thus, via the connection between geometry and criticality, we find a first-order phase transition when vortices attract each other, and a second-order phase transition when vortices repel each other. However, as noted above, attractive and repulsive vortex interactions are precisely the characteristics of type I and type II superconductivity, respectively. Hence, we conclude that the distinction between type I and type II superconductivity is conceptually the same as the distinction between superconductors undergoing first order and second order phase transitions, respectively. The transition from one type of behaviour to the√ other happens at κtri , which is slightly renormalized from the mean field value 1/ 2. It should be noted that the latent heat even deep in the type II regime is tiny, and hence extremely precise measurements close to the critical temperature would be necessary in order to see the first order character. However, liquid crystals are described by a similar Ginzburg–Landau theory, as Eq. 10.7. In that case the Ginzburg–Landau parameter κ can be varied by varying the chemical compositions of the liquid crystal compounds and the latent heat involved in the smectic-A to nematic phase transition is sizeable. For such systems it has indeed been found experimentally that both first and second order phase transitions take place, depending on the value of κ [150]. We may summarize the discussion on effects of fluctuations in the Ginzburg– Landau model as follows. If we perform a mean-field analysis of the Ginzburg– Landau model, we arrive at the conclusion that the superconductor-normal metal transition is a second order phase transition with classical critical exponents. We may include effects of fluctuations both in the order parameter and the gaugefield A, arriving at different conclusions depending on what fluctuations we take into account. Historically, the first attempt at seriously considering fluctuation effects in the Ginzburg–Landau model were made by Halperin and co-workers who froze the superconducting order parameter ψ and considered only gauge-field fluctuations [43]. This is a procedure valid for extreme type I superconductors. The result is that this generates a term |ψ|3 in the free energy, with a negative coefficient. Since this now contains a cubic invariant, a first order phase-transition is inevitable. For the superconductors present at the beginning 1980s the critical region is extremely narrow, however the predicted jump in the entropy across the first order transition is found to be small, of order 0.01k per degree of freedom, where k is Boltzmann’s constant. Consequently the question was difficult to settle experimentally. However there is an isomorphism between superconductors and liquid crystals first discussed by Halperin and co-workers [151, 152], and on this system experiments can be done [153, 150].

312

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

Table 10.2 A schematic view of some important results regarding the order of the phase transition in the GL model Description 1 At the mean field level the model reduces to the |ψ|4 theory, i.e. the effect of the gauge field vanishes completely. 2 |ψ|4 theory is a well known theory, which is much studied [154]. 3 To study the effect of the gauge field Halperin, Lubensky and Ma integrated out the gauge field exactly, this gives a cubic term in the remaining effective φ theory. This is a sound approach in the κ 1, i.e. strongly type I regime. 4 Dasgupta and Halperin studied the combined effects of phase and gauge field fluctuations, excluding amplitude fluctuations [155]. Various duality relations were derived, and the concept of an inverted XY transition was introduced. Excluding amplitude fluctuations is a valid approximation in the κ 1, i.e. strongly type II regime. 5 For the superconductors present at the beginning 1980s the critical region is extremely narrow, and the predicted jump across the first order transition very small. Consequently the question was difficult to settle experimentally. However there is an isomorphism between superconductors and liquid crystals [151, 152], and on this system experiments can be done [153, 150].

Fluctuations

Order

None

2.

|ψ|, arg ψ

2.

A

1.

arg ψ, A

2.

|ψ|, arg ψ, A (Experiment)

1. and 2.

Especially from cases 3 and 4 one can conclude that there must be a κtri separating first order and second order transitions. It is also important to realize that a correct description of this feature of the GL model requires a full description, including fluctuations in |ψ|, arg ψ and A. Adapted from Ref. [156].

The next serious step at considering fluctuation effects in superconductors was taken by Dasgupta and Halperin [155]. Here, they took the opposite approach, and ignored the gauge-field fluctuations altogether, focusing on the fluctuations in ψ of a specific type, namely phase fluctuations. As we have seen, this is a sensible procedure in extreme type II superconductors. A second order phase transition in the inverted three-dimensional XY universality class is found, i.e. a three-dimensional XY phase transition with inverted temperature axis (and a negative anomalous scaling exponent). In fact, we may also include the gaugefield fluctuations with the phase fluctuations, and the result is always a secondorder phase transition, as we have seen above [45, 149, 148]. Moreover, we may include amplitude fluctuations with phase fluctuations only, the result is still a permanent second order phase transition [154]. Thus, as long as we

TYPE I VERSUS TYPE II, BRIEFLY REVISITED

313

y Normal state Tricritical point ytri

y c(x)

Type-I superconductor

Type-II superconductor x c(y)

xtri

0.5

x

Figure 10.5 Phase diagram of the Ginzburg–Landau model in the (x, y) plane (parameters as in Eq. 10.7). The value xtri = 0.295 ± 0.025, corresponding to a tricritical value of the √ . The solid line is the phase transition Ginzburg–Landau parameter given by κtri = 0.76±0.04 2 line from superconducting to normal state. The dashed line xc (y) is a line separating type I from type II superconductivity. The tricritical point separates a first-order phase transition (thick solid line) from a second-order phase transition (thin solid line), and also separates type I from type II superconductivity. The mean field value separating type I from type II superconductivity is given by x = 1/2. Note how it is possible to cross over from type I to type II behaviour in one and the same compound, for moderate values of κ, as the temperature is increased!.

ignore amplitude fluctuations in the order parameter ψ, a second-order phase transition always is obtained, either in the three-dimensional XY universality class (gauge-field fluctuations not included) or in the inverted three-dimensional XY universality class (gauge-field fluctuations included). Kleinert [135] then considered an attempt at combining gauge-field fluctuations and phase fluctuations with amplitude fluctuations by mimicking the amplitude fluctuations using a fluctuating temperature in the Ginzburg–Landau model. He then found that the superconductor–normal metal phase transition changes from first to second order as κ passes through the tricritical value given by Eq. 10.81. The next step was taken by Bartholomew who considered the Ginzburg–Landau model in Monte Carlo simulations, including all fluctuations in phase, amplitude, and gauge fields, finding a second √ order phase transition when κ is larger than some tricritical value κtri = 0.4/ 2 [44]. This value was improved on in Refs [45, 149] using very large scale Monte Carlo simulations in conjunction with sophisticated finite-size scaling techniques, finding a first order phase transi√ tion below κ = 0.76/ 2 and a second order phase transition above it. This is in rather remarkable agreement with Eq. 10.81.

314

DUAL DESCRIPTION OF THE SUPERCONDUCTING PHASE TRANSITION

All of the above may be put into a table showing various descriptions of the Ginzburg–Landau theory, including which fluctuations are taken into account at the superconductor–normal metal transition, and what the character of the resulting phase-transition is. This is shown in Table 10.2. In terms of the parameters used in Eq. 10.7, the phase diagram of the Ginzburg–Landau model is given in Figure 10.5.

PART III

Selected Applications

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

11 Small Scale Applications As a common introductory for the two chapters on applications we should motivate the contents as follows: Superconductor technology divides naturally into two main categories: small scale, usually electronic components or devices, and large scale where magnets and energy applications are of most importance. The applied part of this book intends to review some selected examples of superconductor applications. The entire spectrum of implemented and potential applications is so great today, that a comprehensive review is far beyond the scope of any physics text. However, there is a need to see the physics of superconductivity in the context of applications which is a major driving force in research on superconductors today. To this end, some examples of applications are given, and in important cases the underlying theory is worked out in some detail. A characteristic for superconductor-based technology is often that it is either superior to alternative methods, or only possible using superconductors. It should be emphasized that the potential for future applications other than those discussed in Chapters 11 and 12, or for improvements of existing ones, is enormous. Usually the question whether a demonstrated new superconductor technology is finally brought to the market is one of economy. This is always the case when alternative technologies are available, for instance in electric energy transport and storage, and in magnet technology. Long-term reliability and safety is another important consideration. The situation is somewhat different in areas where superconductor technology is unique, i.e. when no real comparable alternative exists. This is clearly the case with regard to some of the technologies based the Josephson junction. Although only a few examples have been chosen here, they suffice to demonstrate existing and future superconductor technology on scales ranging from micrometres in the Josephson junction to tens of kilometres in electric energy transport and maglev passenger movement.

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

318

SMALL SCALE APPLICATIONS

11.1

More JJ-junction and SQUID basics

11.1.1

Introductory remarks

In the present chapter we will discuss some further basic properties and how these are important for applications of superconductivity on a small scale, as well as giving outstanding examples of present day use.1 The most important small scale electronic device applications so far are based on Josephson junctions, a topic we already encountered in Chapter 5. Among these, the squid has reached by far the widest range of useful implementations due to its unique property as the most sensitive and versatile device for detection and measurement of magnetic flux. The SQUID has been under continuous development and improvements during several decades. It owes its sensitivity to the properties of the superconducting wavefunction phase which provides the basis for both flux quantization and Josephson tunnelling. The broad versatility is due to the possibility it offers for high resolution measurements of any physical quantity which can be converted into magnetic flux. This is the case with quantities like magnetic field, magnetic susceptibility, magnetic field gradient, electric current, voltage, and displacement. Therefore, a wide range of uses are open to the use of SQUID technology. A better understanding of the SQUID can only be reached through a good understanding of the Josephson effect. We therefore proceed to discuss the Josephson junction further, and then again turn to the SQUID and other applications.

11.1.2

RSJ – the resistively shunted Josephson junction

We showed in Chapter 5 that the current trough an unbiased Josephson junction can be expressed as I = I0 sin γ ,

(11.1)

where I0 is the maximum supercurrent the junction can sustain, usually referred to as the critical current, and γ = φ1 − φ2 is the difference in superconducting phase across the junction. We also discovered that while the current I could be expected to flow at zero voltage, another new phenomenon would appear when the current was forced to exceed I0 : A voltage V developed across the junction, and the phase γ became time dependent, giving an AC current with so-called Josephson frequency ωJ according to ωJ = ∂γ /∂t = (2e/)V = 2π V /0 . The current across the junction should now be written I = I0 sin[γ0 − (2eV /)t]

(11.2)

1 Suggested additional reading: S¨ app¨a H, Ryh¨anen T, Ilmoniemi R and Knuutila J, in Fossheim K., (ed) Superconducting Technology. 10 case studies, World Scientific Publishing, 1991.

MORE JJ-JUNCTION AND SQUID BASICS

319

where γ0 in the phase across the junction without the voltage V present. In junctions of high structural perfection the I –V characteristic is often found to be hysteretic as shown in graphs (b) and (c) of Figure 11.1. We will return to the details of this figure later on. For a junction to be practical in a squid it cannot be allowed to have such characteristics. Experience and theoretical analysis have taught us that the problem can be solved by shunting the junction, i.e. by adding an external resistance in parallel. This modification is commonly referred to as the RSJ-model (resistively shunted junction), as shown in Figure 11.2. One identifies from left to right: The current source, the resistive shunt R, the Josephson junction, the self-capacitance C bound to be present in the layered SIS junction structure, and finally the voltage V . We take the current source to be in a current controlled mode. This forces the phase γ in the equation I = I0 sin γ to adjust itself accordingly. The current now determines the phase difference across the junction, and not vice versa. We might further take into account the possibility that there is a fluctuating noise current In (t) associated with the components of the circuit, as is commonly true. The equation of motion for the circuit is then C

dV V + I0 sin γ + = I + In (t) dt R

(11.3)

Current i

1.5

1.0

0.5

0

0

0.5

bc = 3.0 Γ=0 Γ = 0.05

bc = 1.6

bc = 0.7

1.0

0

0.5

(a)

1.0

0

0.5

1.0 (c)

(b) Voltage v

Figure 11.1 Numerically calculated current-voltage characteristics of Josephson junctions with βc = 0.7, 1.6 and 3.0 at zero temperature, i.e. = 0 (solid lines), and with = 0.05 (dashed lines). (For reference, see the footnote at the foot of the opposite page). Parameters βc and are defined below.

I

I

R

I0

C

V

Figure 11.2 The RSJ model for a Josephson junction.

320

SMALL SCALE APPLICATIONS

an equation first studied by Stewart [157] and McCumber [158]. We choose first to analyze the differential equation (Eq. 11.3) under the assumption that In (t) can be neglected. We use the previously found relationship ∂γ /∂t = (2e/)V and write Eq. 11.1 as C γ¨ + γ˙ = I − I0 sin γ . 2e 2eR

(11.4)

Upon defining the quantity 0 (I γ + I0 cos γ ) 2π

(11.5)

C 2e ∂U γ¨ + γ˙ = − 2e 2eR ∂γ

(11.6)

U =− Eq. 11.4 may be written as

This is recognized as the equation of motion for a mass point moving down a corrugated surface, often referred to as a ‘washboard potential’, where U is a function of γ . Two characteristic situations are illustrated in Figure 11.3, I < I0 , and I > I0 respectively. In the first case the point mass gets trapped in one of the potential minima, and oscillates locally there. In the other case it goes on sliding. The first of these situations corresponds to zero time average phase difference, i.e. γ˙ = 0. This corresponds to the average voltage across the junction being zero. The second type of motion arises when the tilt is increased to make I > I0 . In this case the time average is γ˙ > 0, in other words, the point mass keeps sliding down the washboard. It is helpful also to note that in the mechanical analogue the capacitance C represents the particle mass, and 1/R is proportional to the friction coefficient, or damping of the motion.

U(g)

I > I0

I < I0

g

Figure 11.3 The washboard potential with a sliding point mass. Here I represents the tilt of the washboard as can be seen from Eq. 11.5.

MORE JJ-JUNCTION AND SQUID BASICS

321

Numerical analysis of Eqs 11.3–11.6 shows that hysteresis is controlled by the parameter βc , called the Stewart–McCumber parameter βc =

2π I0 R 2 C 0

(11.7)

Hysteresis is found for βc > 1. Calculations of current versus voltage is shown in Figure 11.1 for different values of βc . Distinct hysteresis appears for βc > 1. Further properties of Figure 11.1 will be discussed later. It requires highly qualified laboratory expertise to create junctions which meet the particular requirement βc < 1 for hysteresis-free junctions. Until now we neglected the current noise In (t). For a better understanding of the Josephson contact and SQUID physics the In (t) term should be reintroduced, and its consequences analysed. The full equation of motion is now: C γ¨ + γ˙ + I0 sin γ = I + In (t) 2e 2eR

(11.8)

The effects of noise are usually discussed in terms of noise spectral density SI (f ) of In (t). The meaning of SI (f ) is ‘noise power per bandwidth due to current noise In (t)’. Theoretical analysis shows that the noise spectral density of In (t) is given by the Nyquist result: SI (f ) = 4kB T /R

(11.9)

Since the current I represents the tilt of the washboard potential, the physical effect of In (t) is to cause fluctuations in that tilt. If these fluctuations become large enough they will cause the particle to escape from is local trapping site. This creates a condition for γ˙ to differ from zero, which again means that a voltage will appear, in this case corresponding to the appearance of voltage noise with increasing temperature. This will cause a rounding of the I –V curve before the steeper onset of current driven by the external voltage V . The noise corresponds to an additional voltage dVn and a total effective voltage V + dVn , causing the precursor “noise- rounding” effect in the I –V characteristic observed in the calculations of Figure 11.1. This current noise has an additional effect of lowering the effective critical current value, a potentially harmful consequence of noise since the critical current I0 must be above a certain value for proper operation of the junction. A criterion for I0 to be large enough to maintain a coherent supercurrent or ‘coupling of the junction’ is that the coupling energy exceeds the available thermal energy, expressed by the relation I0 0 /2π kT

(11.10)

322

SMALL SCALE APPLICATIONS

The quantity I0 0 /2π is what we referred to as the coupling energy of the junction. It is a measure of the energy associated with the current pattern for each flux quantum in the junction. A typical value of I0 is in the µA range at low temperatures, a small but easily measured current.

11.1.3

Further modelling of the Josephson junction

Having discussed the Josephson junction in rather simple terms above, let us examine it a little further. Before we rewrite the equation of motion, we remark first on the presence of the resistance R. Going back to the Josephson result for the current, we should, to be accurate, add a term coming from quasiparticle current in the presence of a voltage. The total current is now: I = I0 sin γ + V /Rq

(11.11)

Rq is a voltage dependent quasiparticle resistance. The term I0 sin γ still determines the main properties of the junction. Next, we rewrite the equation of motion by defining new, normalized variables: t ∗ = (2π I0 R/0 )t;

in (t ∗ ) = In (t)/I0

(11.12)

We assume further that the total resistance R, which is formed by Rq in parallel with the shunt resistance, satisfies the condition R Rq . For such cases the equation of motion (Eq. 11.8) describes the junction accurately. The thermal noise current In is the current in the resistance R. Its autocorrelation function is In (t + τ )In (t) = 2kT δ(τ )/R, where δ(τ ) is the Dirac delta function. With a little effort one finds the following reduced form of the equation of motion: βc

dγ d d2γ + ∗ = − (−iγ − cos γ ) + in (t ∗ ) ∗2 dt dγ dt

(11.13)

The current in (t ∗ ) = In /I0 is expressed as a Langevin function describing the thermal noise, and according to standard treatment obeys the relation in (t ∗ + τ ∗ )in (t ∗ ) = 2δ(τ ∗ )

(11.14)

where = 2π kT /I0 0 is the normalized thermal energy. The parameter βc is now analogous to mass, and inversely proportional to the damping of the system. Numerical analysis of Eq. 11.13 yields further insight into the current–voltage characteristics, as seen in Figure 11.1. What was computed there were the quantities i = I /I0 , and corresponding values of v¯ = v = V¯ /RI0 , resulting in the function v(i). ¯ V¯ is the time averaged voltage over the current-biased SQUID.

MORE JJ-JUNCTION AND SQUID BASICS

323

The graphs demonstrate the dependence of the I –V characteristics, here expressed as i versus v, ¯ on the two parameters and βc . First, we observe that embodies the rounding effect at finite temperatures mentioned above. It is therefore referred to as the noise rounding parameter, and the phenomenon itself as noise rounding. Second, as pointed out before, at βc ≤ 1 the characteristics is hysteresis free when = 0, but at higher values of βc there is distinct hysteresis even when = 0. This result defines one of the main technical challenges in applications of the Josephson effect: To control the parameter βc and thereby the characteristics of the junction. The use of Josephson contacts in the SQUID, requires that hysteresis is absent, as mentioned. This provides the important design criterion 2π I0 R 2 C/0 < 1. Fortunately, this nontrivial requirement on the I0 R 2 C product can be met in practice.

11.1.4

The autonomous DC SQUID

Next, we proceed to describe the structure, properties, and operational principles of the double junction DC SQUID, consisting of a superconducting loop interrupted by two identical junctions, both resistively shunted to avoid hysteresis. In the absence of hysteresis the state of the junctions and the DC SQUID are unambiguously determined by the applied voltage. Furthermore, since the flow patterns of supercurrent are characteristically different when the ring encloses an integral number n of flux quanta as opposed to (n + 12 ) quanta, the corresponding two I –V characteristics are also distinctly different. This fact provides the basis for practical use of the DC SQUID. We will now analyse the double-junction DC SQUID by extending the RSJ model to this case. This procedure neglects some technical aspects. But the DC SQUID is in reality such a complex device that one should make some initial simplifications to gain insight into the basic properties. Next, further aspects can be discussed on that basis. For instance, when it comes to practical implementation one cannot avoid considering the coupling of the SQUID to the external world in order to fully understand and control the properties. But it is not a good idea to include all such problems in the first basic analysis. Hence we start the analysis by using the RSJ model equation for both junctions simultaneously. First we note that in each junction, hereafter numbered i = 1, 2, the current Ii is Ii =

d2 γi dγi C + I0 sin γi + In,i + 2e dt 2 2eR dt

(11.15)

This provides us with two equations. First we observe that the total current through the DC SQUID is I = I1 + I2 , and next that the total magnetic flux

324

SMALL SCALE APPLICATIONS

threading the ring is =

0 (γ1 − γ2 ) = a + L(I1 − I2 )/2 2π

(11.16)

In other words, the flux in the ring it is the sum of the applied flux and the flux generated by the (difference of) currents I1 and I2 . a is as before, the external applied flux. The quantities C, R and I0 take on the same meaning as discussed in the RSJ model discussed before. L is the inductance of the ring, and In,i is the thermal noise current in the shunt resistance Ri . The junctions are characterized by the phase differences γi . For further analysis we combine the equations of motion for the two junctions by once adding them, and once subtracting one from the other. This allows us to study the behaviour of the quantities γ1 + γ2 and γ1 − γ2 , which turns out to be a useful procedure. To this end we define the quantities ν = (γ1 + γ2 )/2; φ = (γ1 − γ2 )/2

(11.17)

The instantaneous voltage across the two junctions is now V = RI0 dν/dt ∗ , using the previously defined rescaled, dimensionless time variable t ∗ = 2π RI0 t/ 0 , and the total flux is = 0 φ/π . Using the previously defined parameter βc , and introducing a new parameter βL = 2π LI0 /0

(11.18)

we combine the equations as described, to obtain two new equations of motion. Looking at the case where we add the equations for junction 1 and junction 2 we find d2 d C 2 (γ1 + γ2 ) + (γ1 + γ2 ) 2e dt 2eR dt + I0 (sin γ1 + sin γ2 ) + In,1 + In,2 .

I = I1 + I2 =

Upon introducing ν = (γ1 + γ2 )/2 and φ = (γ1 − γ2 )/2 we find d2 ν dν γ1 + γ2 I= C 2 + + 2I0 sin e dt eR dt 2 γ1 − γ2 × cos + In,1 + In,2 2 I d2 ν dν ≡i = C 2 + + sin ν cos φ + in,ν 2I0 2eI0 dt 2eRI0 dt

(11.19)

(11.20) (11.21)

with in,ν = (In,1 + In,2 )/2I0 . By rescaling the time variable and introducing t ∗ as explained we finally obtain βc

dν d2 ν + ∗ + sin ν cos φ = i + in,ν (t ∗ ) ∗2 dt dt

(11.22)

MORE JJ-JUNCTION AND SQUID BASICS

325

(The change of sign for in,ν (t ∗ ) is unimportant since this is a quantity which fluctuates around zero.) Proceeding in a similar manner when taking the difference I1 − I2 we find βc

dφ 2 d2 φ + ∗ + cos ν sin φ + (φ − φa ) = in,φ (t ∗ ) ∗2 dt βL dt

(11.23)

where we introduced the quantity φa = π(/0 ). The Langevin functions for in,ν , and in,φ represent uncorrelated thermal noise sources, and each of them are characterized by the correlation property in,ν (t ∗ + τ )in,ν (t ∗ ) = in,φ (t ∗ + τ )in,φ (t ∗ ) = δ(τ ). is again the noise rounding parameter defined previously. The equations developed here describe what is called the ‘autonomous DC SQUID’, i.e. one that is operating in a magnetic field with an external current I applied, but without other coupling to external devices, like a signal coil or control circuit, feedback circuit etc.

11.1.5

Simplified model of the DC SQUID

Numerical analysis of Eqs 11.22 and 11.23 has given much insight into the properties of the DC SQUID. For instance, under the assumption that the loop inductance L is very small, corresponding to βc 0, the equations can be expanded as a series, from which the voltage, the circulating current, and the transfer function ∂ V¯ /∂a can be estimated. Under the condition that L is negligible so that βL 1 and βc ≈ 0, the total flux in the ring is ≈ a . According to Eq. 11.22 the voltage can now be written as V ≈ RI0 (i − cos φa sin ν)

(11.24)

By integration of V over the period T of the Josephson oscillation, the average voltage across the current-biased DC SQUID is found [53], 1 V¯ = T

0

T

RI V dt ≈ 2

1−

2I0 π a cos I 0

2 12 (11.25)

In this limit the double junction DC SQUID behaves like a single Josephson junction with resistance R/2, and with an effective critical current Ic,eff = 2I0 cos(π a /0 ), in other words a flux-dependent critical current, with a modulation depth I0,eff = 2I0 when βL 1 and βL ≈ 0. This is seen by comparison with the I–V characteristics found for a single junction.

326

SMALL SCALE APPLICATIONS

The transfer function ∂ V¯ /∂a can be estimated on the basis of the above analysis by differentiation of Eq. 11.25 at a = 0 /2 and I = 2I0 which approximates the usual point of operation in a feedback circuit. To obtain realistic estimates one needs to relax the condition βL 1. RSJ model simulations indicate that at βL = π the modulation depth of critical current is approximately equal to I0 . This leads to the conclusion that ∂ V¯ /∂a ∝ I0,eff is reduced by approximately a factor of 2 for βL = π . The result is that the transfer function can be approximated as R ∂ V¯ ≈ ∂a 2L

(11.26)

√ Similarly, the dynamic resistance can be estimated as Rdyn = ∂ V¯ /∂I ≈ R/ 2 Operational properties The most important aspects of the DC SQUID with regard to operational properties are sketched in Figure 11.4. From left to right is shown the resistive shunting of each junction, and with a capacitance C associated with each, followed by a sketch of the two typical I –V characteristics, once with a flux a = n0 and once with a = (n + 12 )0 applied. This leads to a periodically varying voltage vs. applied flux, with a period 0 as shown in the right figure. These insights can be gained through numerical calculations, using the equations of motion discussed above. Looking through the mathematics of these equations, it is not easy to see from them why the I–V characteristics behave as shown in Figure 11.4. Clarke [159] has given a ‘simplistic’ analysis with a minimum amount of mathematics. We refer here to Figure 11.5, and also to Figure 11.4: we take the two junctions in the SQUID to be arranged symmetrically, one on each side of the loop, as is always done in a DC SQUID. The bias current I is then divided equally I

I

Φ

R I0

C

R V C

V Φ = n Φ0

IB

I0 Φ = (n + 1/2)Φ0 V

(a)

(b)

0

1 Φ/Φ0

2

(c)

Figure 11.4 (a) The DC SQUID; (b) I –V characteristics; (c) V vs. /0 at constant bias current IB . After Clarke [159].

327

MORE JJ-JUNCTION AND SQUID BASICS I

J I 2

Φ0 2L

−J

Φ0 /L

J I 2

+J

V

Im 1

2

Φ/Φ0 (a)

(b)

0

1 Φ/Φ0

2

(c)

Figure 11.5 Simplistic view of the DC SQUID: (a) a magnetic flux generates a circulating current J that is periodic in as shown in (b); as a result (c), the maximum supercurrent Im is also periodic in . After Clarke [159].

between the two paths, with I /2 in each. As long as the current in a junction is below the critical current I0 , a supercurrent tunnels through the junction at zero potential difference. If we allow an arbitrary amount of flux a to be applied to the ring, an additional supercurrent Icirc is set up, creating a self-generated flux LIcirc in the ring. Recalling that the total flux in a superconducting ring or loop is quantized as n0 , the following relation now applies: = a + LIcirc = n0

(11.27)

Taking the starting values of the applied flux as a = 0 or a = n0 , the circulating current according to Eq. 11.27 is initially zero. On increasing the applied flux, a finite circulating current JI circ = (a − n0 )/L develops in order to keep the total flux through the loop at its starting, quantized value. This internally generated, circulating current adds to the externally applied bias current I /2 in junction 1, and subtracts in the other, junction 2. The individual junction currents are related as I1 = I2 + 2Icirc and I2 = I1 − 2Icirc . Since the circulating current flows in opposite sense relative to the bias current in the two junctions, the junctions will respond differently to the same amount of externally applied flux. Junction 1 switches to the voltage state, i.e. a voltage develops across it, when it carries a total current equal to the critical current (see Figure 11.1). This happens when I1 = I /2 + Icirc = I0 . At this point the device current is I = 2I0 − 2Icirc . This is to be regarded as the device critical current at this applied flux. The maximum value clearly is 2I0 . What is important for use of the device is how it further responds to applied flux: At the same time as a increases from zero to 0 /2, Icirc increases from zero to 0 /2L according to Eq. 11.27, and the device critical current diminishes to 2I0 − 0 /L. We see from this that the critical current of the device as a whole has decreased by the amount 0 /L. Next, as we increase the applied flux beyond 0 /2 the SQUID makes a transition from the flux state n = 0 to n = 1, with reversal of the sign of Icirc . As a is increased to 0 , the critical current again increases

328

SMALL SCALE APPLICATIONS

to its maximum value 2I0 . The sequence discussed is depicted in Figure 11.5. It repeats periodically with increasing flux, and thereby results in the behavior of the DC SQUID illustrated in Figure 11.4. As Figure 11.4 also indicates, a practical device is biased at a constant current IB . This bias is above the critical current and therefore puts the entire DC SQUID in the voltage state, which is what we need in order to make it a flux to voltage transformer. It is the resulting voltage response to applied flux, shown in the right figure, which is so extensively exploited in practical applications of the device. An important question is how this device which is so sensitive, can be used both in low and high magnetic fields. The answer is that a combination of several factors make this possible: The sensitivity of the the transfer function ∂ V¯ /∂ at the bias current IB , combined with compensating feedback circuitry, as well as the use of a flux transformer that amplifies the flux detected at the observation point and transfers it to the SQUID, usually located some distance away. The DC SQUID is typically operated in socalled flux-locked loop. A simplified example is shown in Figure 11.6. The operating point of the SQUID is chosen at the steepest point on one of the periodic oscillations of the V –curve seen in Figure 11.4. In this design the SQUID is coupled to an external compensation inductor controlled by feedback from the SQUID output, thus causing the flux felt by the SQUID to be constant during operation even in a strongly varying external field. The feedback circuit also produces a voltage proportional to the flux that the circuit compensates. When calibrated, this voltage then measures the field detected by the device. In many uses of the SQUID other types of detector coils are used, such as first-order or second-order gradiometers. Gradiometers are used to eliminate spatially homogeneous external noise superimposed on the signal, like electromagnetic noise in the environment. A simplified but realistic and detailed sketch of a DC SQUID with signal coil attached is shown in Figure 11.7. The development of the SQUID has been a long battle against noise of many kinds. Noise may be environmental type, it may come from the components of the SQUID itself, and from the detecting circuitry and amplifier. Since the SQUID is a non-linear device, thermal noise has a dramatic effect on the dynamics. Figure 11.1 already gave some IB

Amplifier

Lock-in detector

Integrator

SQUID V 100 kHz oscillator

Figure 11.6

Modulation and feedback circuit for the DC SQUID. After Clarke [159].

SQUID APPLICATIONS Current nodes

329

I DC SQUID

Signal coil

High frequencies Low frequencies Parasite capacitance Base electrode I

Josephson junctions Counter electrode

Figure 11.7 Simplified structure of a planar DC SQUID together with a signal coil. The sites for the current nodes of the microstrip resonance and for the effective capacitance coupling are indicated. The directions of the current in the different signal-coil turns at frequencies lower and higher than the microstrip line resonance frequency are shown. After S¨app¨a et al. [160].

information on the influence of noise through the parameter as an example. According to careful studies [160] the autonomous DC SQUID discussed above √ has an optimal energy resolution ≈ 12kB T LC at βc ≈ 0.7. This expression can be interpreted as the ratio of thermal energy 12 kB T divided by the so-called effective noise bandwidth of the SQUID, 14 R/L. We conclude that a low-noise DC SQUID should have small junction capacitance, small loop inductance, and proper damping of the junctions. Examples of typical values are: C = 1 pF and L = 20–40 pH. In Figure 11.7 it is seen that the design attempts to meet these requirements. Obviously, the junction capacitance is made very small. DC SQUIDS may be shunted in several ways. We have only discussed one of these, the resistively shunted DC SQUID. In addition both capacitive and inductive shunting are possible, and have been well characterized.

11.2 SQUID applications 11.2.1

Biomagnetism: neuromagnetic applications

Introductory remarks2 Magnetic fields produced by living organisms has become one of the most wide-spread applications of the SQUID. Especially important is magnetoencephalography (MEG) which is a method for studying brain functions by mapping of the magnetic field produced by neural currents in the human brain. 2 Suggested additional reading: Ahonen A.I, et al., in Fossheim, K. ed. Superconducting Technology. 10 case studies, World Scientific Publishing, 1991 [161].

330

SMALL SCALE APPLICATIONS Action potential

Postsynaptic potential

Propagation

Synapse

Figure 11.8 Schematic illustration of an action potential, essentially consisting of two nearby opposite current dipoles propagating towards a synapse and the resulting postsynaptic potential corresponding to a single stationary current dipole. After Ahonen et al. [161].

Such magnetism is referred to as neuromagnetism. The function of the brain involves activity on the millisecond timescale. For such study there are two main windows: Electroencephalography (EEG) and magnetoencephalography (MEG). In EEG the potential distribution over the head is measured by electrodes attached to the scalp. In MEG the weak electromagnetic fields of typical amplitude 50–500 fT generated by the human brain are measured in order to locate the current sources generating the magnetic fields associated with cortical activity. Magnetoencephalography is a noninvasive tool for such study, offering spatial resolution on the millimetre scale and time resolution on the millisecond scale. A particular advantage of the MEG is its ability to locate cortical activity at deeper levels and spatially more accurately than EEG. The EEG is strongly influenced by currents in the scalp, which the MEG is not. Hence MEG offers superior quality with regard to locating accuracy. There are two types of signals from the brain: spontaneous activity, and evoked response to external stimuli. The principle of neuromagnetism The basis for MEG lies in concepts of action potential and postsynaptic potential. Information is carried from one neuron to another by the action potential via the synapse, mediated by the release of transmitter molecules which increase the permeability of the postsynaptic membrane as illustrated in Figure 11.8. Due to an interaction between chemical and electrical gradients there is a net current flow through the membrane and a change in voltage, called the postsynaptic potential (PSP). To a first approximation PSP is an intracellular current dipole oriented along the neuron, while the action potential may be described as a current quadrupole. In order for a resulting magnetic field to be detectable outside the head, a large

SQUID APPLICATIONS

331

number of neurons need to be activated, and to act in unison. The strength of a PSP current dipole is only 10−14 A. The observed magnetic field is believed to be mostly due to PSP cells which are perpendicular to the cortex. The field due to the action potential is very short range due to its quadrupolar nature. In addition, the dipolar PSP lasts an order of magnitude longer. The observed equivalent dipole is of the order of 10−8 A, which means that tens of thousands of neurons are activated at the same time. Dipoles which are observed in spontaneous activity, like in elliptic foci, may be an order of magnitude larger still. In order to calculate the field outside the head, resulting from cortical activity, some model assumptions have to be made. The head is often described as spherical symmetric, filled by a conductive medium with conductivity σ (r). The magnetic field outside such a body has important simplifying properties: (1) radial dipoles and their volume currents cancel each other and thus do not generate a magnetic field outside the body, (2) the radial component of magnetic field is produced by the primary current density only, and (3) both radial and tangential field components are independent of the conductivity profile. During measurement, the evoked response signal is usually assumed to be composed of the true source signal plus gaussian noise. By repeated sampling, say N = 100 times, the signal part is integrated up proportional to√N , the total number of samples, while the noise integrates up proportional to N . Thus an acceptable signal to noise ratio can be achieved. Instrumentation The SQUID is the only instrument with sufficient sensitivity to perform neuromagnetic studies. Usually, the external field is coupled into the SQUID by a a superconducting flux transformer, i.e. a pickup loop coil and a signal coil in series, shown in principle in Figure 11.9. Normally the signal is orders of magnitude smaller than the environmental noise. Therefore, the transformer usually has a gradiometer coil on the detecting side, sensitive only to the derivative of the magnetic field, ∂Bz /∂z, and insensitive to environmental noise with electromagnetic wavelength much longer than the size of the coil. An illustration of such a coil is shown in Figure 11.10. It consist of two identical coils in series, but oppositely wound. The first part may be regarded as the signal detector, and the second part as a compensator coil. In a case when spatially homogeneous noise is detected by the first coil, it is compensated by the second one, and the resulting signal picked up by the gradiometer is zero. If on the other hand an inhomogeneous field is present, the gradiometer coil detects a signal proportional to the spatial derivative along the coil axis. Depending on the design one may choose to make gradiometers that measure tangential derivatives ∂Bz /∂x and ∂Bz /∂y. Usually the whole device is placed in a magnetically shielded room. However, more and more sophisticated designs have made it possible to operate the

332

SMALL SCALE APPLICATIONS Pickup coil

Signal coil

→ Bext

→ Bcoupled

SQUID

Figure 11.9 Transformer. After Ahonen et al. [161]. Li Mi

L

Js Flux-locked SQUID

Li Mi

L

z Js Flux-locked SQUID y x

Li Mi

L

Js Flux-locked SQUID

Figure 11.10 Examples of gradiometers coupled to flux-locked SQUID. After Clarke [159].

SQUID in unshielded environment. For a more widespread use of SQUIDs in diagnostics, it is essential to avoid the use of shielded rooms for the sake of cost reduction. A potentially interesting area for the future is in cardiology. The capability to obtain high quality signals from the heart cycle is well established even using high-Tc superconductor SQUIDs. However, sensitivity to the positioning of the device is one of the problems with this method. During the 1990s a new development took place. Multichannel SQUID systems, containing well over 100 SQUIDs were built to be placed over the head, and

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

333

Figure 11.11 Multichannel SQUID system for neuromagnetic studies of the brain. With permission from Neuromag.

allowing a very detailed recording of brain activity in the entire brain. These systems are commercially available, and becoming increasingly important as a tool for brain diagnostics, and as a research tool for the study of brain function more generally. Figure 11.11 shows an example of multichannel squid system for neuromagnetic studies of the brain. Determining the precise location of epileptic foci before surgical treatment is an established clinical application of such systems.3

11.3 Superconducting electrodynamics in the two-fluid model 11.3.1

Frequency dependent conductivity in the two fluid model

Electrical current in the Meissner phase is confined to the penetration depth λ. This obviously is the DC limit of response to an electromagnetic field. Therefore, any theory for the low frequency response must have Meissner screening 3 Recommended further reading: See two review articles by Clarke J. (1) In Weinstock, H. ed. SQUID Sensors: Fundamentals, Fabrication and Applications. NATO ASI Series. Kluwer Academic Publishers, Dordrecht, The Netherlands 1996, and (2) In Weinstock, H. ed. Applications of Superconductivity. NATO ASI Series. Kluwer Academic Publishers, Dordrecht, The Netherlands 2000. These reference treat the rf SQUID.

334

SMALL SCALE APPLICATIONS

as its limiting low frequency behaviour. We will now treat electrodynamics in the situation where a superconductor surface is exposed to an AC electromagnetic field. Relevant cases may be electromagnetic radiation incident on the superconductor surface, for instance at normal incidence, or an electromagnetic wave traveling along the superconductor surface. This latter case will correspond to the situation in the technologically very important planar wave-guides and filters used in high frequency communications. We treat a superconducting half-space first as the basic entity. In the course of this treatment penetration depths for electromagnetic field in both normal and superconducting materials will be introduced. Furthermore, we need a model description of the superconducting electron gas. It turns out that the so-called two-fluid model is adequate for this purpose over a wide frequency range. The two-fluid model was historically introduced by Gorter and Casimir in 1934 [67]. It proposes to divide the mobile charges in the superconducting state of a metal into two distinct entities: A normal component of concentration nn with properties like those of the electron in the normal state, and a superfluid component of concentration ns whose properties are responsible for the observed screening of a static magnetic field in the Meissner phase. The total concentration of mobile charge is then (11.28) n = nn + ns where both nn and ns have to be temperature dependent in order to account for the temperature dependence of the penetration depth λ. Corresponding to this division one also foresees that currents are composed of two parts, a normal part Jn associated with nn , and a superconducting part, Js , associated with ns . For the total current then J = Jn + Js

(11.29)

Experimentally one finds in low-Tc superconductors that the London penetration depth λL obeys the following simple relation for its temperature dependence − 1 2 λL (T ) = λL (0) 1 − (T /Tc )4

(11.30)

This can be interpreted as a consequence of a density of normal component nn /n = (T /Tc )4 , and a corresponding density of superfluid component ns /n = 1 − (T /Tc )4

(11.31)

1 Since λL = ms /µ0 ns (T )qs2 2 , substituting ns from Eq. 11.31 reproduces Eq. 11.30. We define λL (0), the London penetration depth at 0 K, as 1

λL (0) = (ms /µ0 ns (0)qs2 ) 2

(11.32)

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

335

How does this relate to conductivity? Using Newton’s second equation for the case of zero friction we have ms

dv = qs E dt

(11.33)

The current density Js may be expressed as J s = ns qs v

(11.34)

Hence we can rewrite Eq. 11.33 as

dJ s −E =0 dt

(11.35)

which is the first London equation where = ms /ns qs 2 . In case of a sinusoidal field of frequency ω we expect a resulting sinusoidal current. After performing the derivation in Eq. 11.35 we obtain Js =

1 E = σs E iω

(11.36)

where we have defined a conductivity σs : σs =

1 1 = iω iµ0 ωλ2L

(11.37)

Since σs is expressed for a condition of zero loss (without a damping term in Newton’s equation of motion) it is a purely imaginary quantity. Also, if we assume low frequency, as when ωτ 1, we can take the usual DC expression for the normal state conductivity to apply for the normal component of the electron gas, with the normal current being in phase with the driving field: Jn = σn E = and the total current

J = Jn + Js =

nn qn2 τ E mn

nn qn2 τ 1 −i mn µ0 ωλ2L

(11.38) E

(11.39)

The conductivity is now a complex expression: σ = σ1 − iσ2 =

nn qn2 τ 1 −i mn µ0 ωλ2L

(11.40)

The response to an AC field in a superconductor clearly is out of phase with the applied E-field.

336

SMALL SCALE APPLICATIONS

11.3.2

Surface impedance and AC loss

Because of the altered screening effects resulting from the foregoing analysis there is a need to apply a different concept, adequate for this situation, in addition to Meissner screening. This is the concept of a (complex) surface impedance Z, measured in units of , defined by Z=

E|| J dz

(11.41)

where E|| is the electric field in the surface, driving the current J along the surface, and integration is from the surface (z = 0) to (in principle) infinity inside the conductor. Using Maxwell’s equation one derives for a normal metal, as we will show later, Zn = Rn + iXn 1 Rn = Xn = (µ0 ω/2σn ) 2

(11.42)

Consequently, the resistive and reactive parts of the surface impedance in a normal conductor are equal, and, since σ is frequency independent in the range we are considering, both go like ω1/2 . These results have been well verified experimentally. In the superconducting state matters are different due to the difference in AC conductivity discussed in the previous section. Since we already used London’s first equation to establish an expression for σ in the superconducting state, and in addition invoked the two-fluid model, superconductivity is built into the σs we derived above. We therefore now only need to use Maxwell’s equations, and the surface impedance takes the same form both in the superconducting and normal states when expressed in terms of σs . We have for the superconductor: Zs = Rs + iXs = We will show later that

iµ0 ω σs

1 Rs = µ20 ω2 λ2L σn 2 Xs = µ0 ωλL

1 2

(11.43)

(11.44) (11.45)

where we used the symbol σn for the conductivity of the superconductor in its normal state, corresponding to nn = n. We also note that the reactive part Xs of the surface impedance Zs is purely inductive. The usual expression for such impedance is X = ωL. In the present case therefore, we can conclude that Ls = µ0 λL , usually called the equivalent inductance, known also as the kinetic inductance. We now proceed to deduce the results briefly mentioned above, first

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

337

for the normal state. We want to find the intrinsic impedance Z. This quantity may be defined from Maxwell’s equations ∇ × H sn = Jns + iωεE sn

(11.46)

where the second term on the right-hand side is the displacement current due to bound charges, or

and by use of

∇ × H sn = (σn + iωε)E sn

(11.47)

∇ × E sn = −iωµ0 H sn

(11.48)

In all cases the superscript s here refers to ‘surface’ rather than ‘superconducting’ while subscript n refers to the normal state. Combining Eqs 11.47 and 11.48 by taking the curl of the second one and inserting the result in the first, and further s e−(α+iβ)z = E s e−γ z one finds writing Ens = En,o n,o γn2 = (σn + iωε) iωµ0

(11.49)

which can be written in the form

1 σn 12 γn = iω (µ0 ε) 2 1 − i ωε

(11.50)

In a good metal the displacement current density is very small compared to that caused by free charges. Numerically, therefore, one finds even for normal metals that σn /ωε 1. Hence, the general expression for γn can be approximated by

σ 1 1 1 n 2 γn = iω (µ0 ε) 2 −i = i (−iωµ0 σn ) 2 ωε 1

= (1 + i) (ωµ0 σn /2) 2 = (1 + i) /δn

(11.51)

where δn is the classical normal state skin depth, defined here as δn =

2 ωµ0 σn

1 2

(11.52)

We also note that under this approximation, since γn = αn + iβn is a complex quantity, we have for αn and βn αn = β n =

1 ωµ0 σn 2

1 2

=

1 δn

(11.53)

338

SMALL SCALE APPLICATIONS

These quantities are again closely related to the intrinsic impedance, a quantity we will deduce next. The complex surface impedance Z ≡ R + iX defined as indicated previously (Eq. 11.41), or alternatively by the relation Z≡

s e−γ z Ex,o s Hyz

(11.54)

here specifically referring to an electromagnetic AC field applied at normal incidence to the surface whose normal is along z. Using ∇ × E s = −iωµ0 H s one finds 1

Z=

(iωµ0 ) 2 1

(σ + iωε) 2

=

µ 1

1

ε

(1 − i (σ/ωε)) 2

0

2

1

=

µ ω1 2 0 (1 + i) 2σ

(11.55)

We can at this point easily distinguish between the normal and superconducting states. In the normal state the conductivity is a real quantity σn , and we find in this case for Zn = Rn + iXn , the corresponding terms in Zn =

ωµ0 2σn

1 2

+i

ωµ0 2σn

1 2

(11.56)

Next, introduce σ in the superconducting state as a complex quantity σs = σ1 − iσ2 as we did before. Inserting this, we have: Zs = Rs + iXs =

iωµ0 σ1 − iσ2

1 2

(11.57)

Since in the superconductor σ1 σ2 we can expand the root, and find, using the expressions for σ1 and σ2 from Eq. 11.40 Zs = Rs + iXs = 1 Rs = µ20 ω2 σn λ3L 2 Xs = µ0 ωλL

µ20 ω2 λ3L nn qn2 τ + iµ0 ωλL 2mn

(11.58) (11.59) (11.60)

We notice in particular that the surface resistance predicted by this model increases as the square of the frequency, compared to the square root dependence in the normal case. Observations confirm these predictions with good accuracy in, respectively, normal metals, and in high quality LTS superconductors. In HTS the frequency dependence is sometimes influenced by non-ideal structures. The agreement with predictions is therefore not as good in such cases. Examples of observations are given in Figure 11.12.

SUPERCONDUCTING ELECTRODYNAMICS IN THE TWO-FLUID MODEL

11.3.3

339

Surface resistance measurement

The most crucial information needed in order to evaluate the quality of superconducting surfaces or thin films for use in high frequency communication systems is the surface resistance Rs . This quantity will determine the loss properties, and this is the essential information to obtain. Several methods have been established for such purposes. As far as high-Tc materials are concerned, due to the anisotropic structure of these materials, measurements must be done on planar surfaces. This is contrary to well-established methods for low-Tc materials, which are often measured in cylindrical cavities including the walls. Since the planar sample can very well be used in both cases we describe briefly the so-called endwall replacement method. Figure 11.13 shows a sketch of a vertical cut through a cylindrical TE011 mode cavity with input and output signal attached as indicated. The short centre lead sticking into the cylinder are antennas for the excitation of the electromagnetic cavity, and for measurement of the response on the ‘out’ side. While the cylindrical walls and the bottom part are made of high quality copper, the top flange can be exchanged, placing here in one case a copper plate, and in the other case a high-Tc film deposited on some appropriate substrate. By sweeping across a certain frequency range around the resonance frequency f0 of the cavity, the detecting antenna will register a varying field response due 102

K Optical waveguide

Waveguide 77 K WR-15 u C eline Strip l cable a i x a Waveguide 9 Co RGWR-28

1

K

)

10−1

K

)

77

2 4.

Optical fiber (Silica)

3S

n

eY

(N b K 27 O eY

BC

10−5

in

10−4

BC

Sa w

O

(×

10−3

K

3. 7

×

(N

b

10 −

4. 2

)

5

10−2

St rip el

Attenuation (dB/cm)

u 300

line C

Stripe

10

Atmospheric propagation at sea level

St

rip

el in

10−6 10−7 0.1

1 10 Frequency (GHz)

100

Figure 11.12 Loss per meter as a function of frequency for various transmission media. (The surface acoustic wave propagation losses on LiNbO3 have been scaled to make a realistic comparison and represent dB/µs of delay for an equivalent electromagnetic wave in a media with εr = 10). After Lyons and Withers [162].

340

SMALL SCALE APPLICATIONS HTS sample TE011 cavity

In

Out

Absorber

Figure 11.13 Cross-section of a TE011 mode cylindrical cavity for measurements of surface resistance. After Shen [163].

to the finite width f of the resonance. This width is a measure of the quality of the cavity as a resonator, called its Q-value, defined by ω0 f0 2πf0 W ω0 W = ≡Q= = ω f P P

(11.61)

We can regard this as a measure of how much energy is dissipated per second (P ) relative to how much energy is put into the cavity per second. Here W is the stored energy, which, after multiplication by frequency essentially measures the rate of energy put into the cavity. Therefore, a measurement of the Q-value defined here is an appropriate way to characterize the quality of the cavity. These aspects are determined fully by the loss properties of the material. The next question is now how a measurement of the Q-value as described above gives access to the surface resistance Rs . First we have to replace the upper Cu flange by the superconductor. The change of Q will tell us how the materials differ. A relative measure of the surface resistance r of the superconductor compared to that of copper is often expressed as r=

Rs (Cu) k = Rs (SC) k + Q0 (Cu)/Q0 (SC) − 1

(11.62)

Here, k is a geometrical constant of the cavity. k=

1 2 + PSw (Cu)/Pew (Cu)

(11.63)

where PSw (Cu) is the power lost in the sidewall of the copper cavity while Pew (Cu) is the power lost in the end wall when the Cu end wall is in place. We did not prove these results. They are referred to here only to show that the analysis can be completed. The important relation is that expressed by r. Clearly, if all that is needed to determine the surface resistance of the superconductor, relative to that of copper, is a measurement of quality factors as explained, with the

HIGH-FREQUENCY RADIO TECHNOLOGY

341

10−1

Surface resistance (Ω)

10−2

10−3

10−4

10−5 0 10

1.2 cm substrate 5.1 cm substrate Rs a f 2 Cu 101 102 Frequency (GHz)

103

Figure 11.14 Relationship between surface resistance Rs at 77 K and frequency in a Tl2 Ba2 CaCu2 O8 film and in Cu. After Holstein et al. [164].

upper wall in place, once as a superconductor and once as a copper wall. Since copper is the standard by which metallic resistance is gauged, this does the job. What is found, is that although copper is a very good conductor, with low resistance, a superconductor is often 1000 or more times better, i.e. Rs is 103 to 104 times lower than that of copper at room temperature. This is a drawback for the method described, making it one of relatively low sensitivity. Other techniques have been devised to allow the superconductor to play a larger role in determining the total Q of the cavity. We refer to more specialized literature on this subject. Figure 11.14 shows results of measurement of surface resistance carried out on Tl2 Ba2 CaCu2 O8 film. We notice in particular that the square law for surface resistance discussed before is verified, even using different substrates. The validity of the result of the two-fluid theory is confirmed even in this high frequency range.

11.4 High-frequency radio technology 11.4.1

Microstrip filters and delay lines

Introduction Superconductors can have a dramatic impact on selected passive microwave device applications because of two properties that differ greatly from those of

342

SMALL SCALE APPLICATIONS

normal metals at high frequencies. First, much lower surface resistances is available using superconductors, a fact that transforms into much lower loss and much higher Q-values in superconducting microwave system components. Second, superconductors have a practically frequency independent penetration depth in the microwave frequency range. This has the important consequence that superconductors introduce no dispersion into a microwave device up 1 THz frequency in low-Tc superconductors, and well above this in high-Tc superconductors due to their larger gap frequency. The improvement over normal conducting performance is substantial. Superconductor passive devices may work quite well in cases where normal conductor devices would function very poorly or not at all. A normal metal component would, in many cases, have several orders of magnitude higher conductor loss than the superconducting ones. Important passive microwave device components are bandpass filters, which are becoming essential components in mobile phone base stations. Other uses are in chirp filters which can provide improved resolution in radar images, and delay lines used in various contexts. As we discussed previously in this chapter, the two-fluid model is adequate for an engineering representation of the physical properties of superconductors in the present context. Figure 11.15 shows how the surface impedance can be represented graphically in a circuit analysis. The surface resistance, which we previously found in Eq. 11.59, can be expressed as follows: 4 − 32 4 T 1 2 2 3 T Rs = µ0 ω λL (0)σn 1− 2 Tc Tc

(11.64)

where the temperature dependencies of nn /n and λL , respectively, have been inserted in the two parentheses. According to this expression the surface resistance goes to zero at T = 0. In reality this does not happen. Instead a limiting value is reached at low temperatures, independent of temperature but dependent on frequency. This effect is typically caused by small inclusions of normal phase. For niobium the residual resistance falls below 10−8 in the GHz range at about 1.2 K. High-Tc superconductors have a much shorter coherence length than low-Tc ones. The residual resistance is therefore a more serious problem Normal current path Surface impedance Ln

Rn Lsurf

Rsurf

Lsc Supercurrent path

Figure 11.15 Two-fluid model for the bulk impedance of superconductors and its equivalent surface impedance.

HIGH-FREQUENCY RADIO TECHNOLOGY

343

in high-Tc superconductors. We refer again to Figure 11.12 for examples of the improved surface resistance properties in superconductors compared to copper, in particular in high-Tc , in the 1–100 GHz range. For YBCO film the calculated curves are based on the two-fluid model. The potential improvement compared to Cu at 77 K is enormous. Although part of the improvement is lost when patterning is performed, compared to the unpatterened continuous film, a substantial advantage remains. Another important aspect is the loss per meter during signal transmission. Figure 11.12 leaves no doubt about the advantage of superconducting transmission media over surface acoustic wave signal transport, normal coaxial cable, and Cu stripline. This figure does not take into account dielectric losses, nor does it take into account transducer and conversion losses in the SAW device. Comparison to Nb and Nb3 Sn at 4.2 K is made. Implementation: filters and delay lines Figure 11.16 shows the design of a 4-pole so-called Chebyshev bandpass filter with 3% bandwidth, 0.05 dB passband ripple, and 4 GHz centre frequency. The filter was made by deposition of YBCO film on 425 µm thick LaAlO3 substrate. Data in Figure 11.17 shows a passband insertion loss of only 0.3 dB at 77 K and 0.1 dB at 13 K. Nb filters showed similarly 0.1 dB insertion loss at 4.2 K. Gold filters had an insertion loss of 2.8 dB at 77 K. The superconductor filters have far steeper skirts than gold filters, a very important feature to prevent cross-talk between channels, in particular when used as filters for mobile phone communication. Another important application of superconductor passive devices is in analogue signal processing where the high frequencies and wide bandwidths required place a premium on conductor loss. The tapped delay line architecture developed at Lincoln Laboratory is illustrated in Figure 11.18. A tapped delay line provides temporary storage and sampling of the input signal at intervals τi . The samples are multiplied by weights wi and coherently combined by spatial summation or time integration. Such delay lines are used to implement chirp 66 µm

165 µm

0.100”

Figure 11.16 Four-pole superconductive microstrip filter layout. The filters were fabricated on LaAlO3 substrates using gold, niobium and YBCO signal lines. After Lyons and Withers [162].

344

SMALL SCALE APPLICATIONS

Transmission (dB)

0

T = 77 K

−10 −20 −30 −40 −50

4.0

4.2 4.4 Frequency (GHz)

4.6

Figure 11.17 Measured transmission response at 77 K of a filter fabricated with a postannealed YBCO signal line and ground plane on a 425 µm thick LaAlO3 substrate. Passband insertion loss is 0.3 dB. After Lyons and Withers [162].

Input

t1

t2 w1

t3 w2

t4 w3

t5 w4

w5

Figure 11.18 Architecture of a transverse filter, where τi are time delays and wi are fixed or programmable tap weights. After Lyons and Withers [162].

Signal line conductor

Dielectric

Figure 11.19 Various transmission line geometries considered for the implementation of YBCO delay lines. After Lyons and Withers [162].

filters, matched filtering, correlation and Fourier transformation. The number of information cycles of the waveform gathered coherently in the filter determines the signal processing gain, i.e. the time-bandwidth product. Delay line transmission geometries are illustrated in Figure 11.19, in various combinations of signal line, dielectric and ground. Generally, the various structures perform very much in agreement with predictions.

HIGH-FREQUENCY RADIO TECHNOLOGY

11.4.2

345

Superconducting high-frequency devices

Introductory remarks Superconducting tunnel junctions are well suited for use in low-noise high frequency detectors. The noise level in the these quantum mechanical based detectors can be well below those of competing state-of-the-art detectors. The most demanding applications for mm- and sub-mm observations in radio astronomy already take advantage of these low-noise receivers. According to Dicke’s famous radiometer formula [165], the signal to noise ratio for a given bandwidth ( f ) and a given integration time ( t) is S Ts = f t N TR

(11.65)

where Ts is the equivalent blackbody temperature of the signal, and TR is the receiver noise temperature. From this formula we observe that for a given signal to noise ratio the integration time needed to observe a particular source is reduced by a factor of 4 if the receiver noise temperature is reduced by a factor of 2. Since the integration time sets the time scale of the telescope observation time, this transforms into far more efficient use of an expensive satellite telescope with moderate improvement of the detector. Superconducting device components are therefore of great interest. It turns out that the greatest advantage is obtained at several hundred GHz, i.e. in the mm and sub-mm wavelength regime, an interesting range for radio astronomy in space or on the ground. Phase sensitive heterodyne detectors normally use a mixer to down-convert a high frequency signal to an intermediate frequency (if) range where low noise semiconductor amplifiers are available. To perform the down-conversion a high frequency local oscillator (lo) is needed. For semiconductor mixers which need about 1 mW power above 200 GHz, these oscillators are rather heavy equipment. In contrast, a superconducting detector needs only low lo power. Furthermore, a large number of receivers can use the same lo. It is therefore possible to construct an array of detectors for radio astronomy used in satellite telescopes, that can scan the sky simultaneously in several directions. This gives another factor of 10 in efficiency. Lightweight low power lo solutions are also available for SIS mixers. For space use the ideal technology will be to build integrated all superconductor receivers, i.e. local oscillator, mixer and preamplifier on the same chip. The particular property of SIS junctions which makes them useful in the context outlined above, is their extremely sharp non-linear I –V characteristics. According to the physical properties we have discussed in Chapters 4 and 5, there are two distinct possibilities, either the quasiparticle tunnelling I –V characteristic near the gap Vg , or the Josephson effect pair tunneling characteristic at zero voltage, V = 0. Both may be used.

346

SMALL SCALE APPLICATIONS

Mixer principle It is the lack of broadband low-noise amplifiers for signals above ≈100 GHz that drives the need for superconductor technology in the mm to sub-mm range of radiowaves. When a local oscillator voltage is applied to a nonlinear element, in our case an SIS tunnel junction, a periodic variation of the small signal conductance dI /dV is produced, giving rise to a number of current components at the fundamental and harmonic frequencies of the lo. Combining the received signal voltage at frequency fs with the lo signal at flo the non-linear characteristic of the detector gives a product response at Fourier component frequencies fm = |mflo + fif | where fif = |fs − flo | is the so-called intermediate frequency signal, or if signal for short. This means that power is transferred to sum and difference frequencies of the two signals that are mixed in the SIS non-linear device. The situation is illustrated in Figure 11.20. From this new spectrum of frequencies the important signal is the one whose frequency has been downconverted to the range accessible to conventional low-noise amplifiers, the last stage before viewing the resulting telescope output. We will briefly outline a simplified mathematical description of the mixing process. The current through the nonlinear element can be written as a power expansion in the voltage V : I (V ) = a1 V + a2 V 2 + a3 V 3 + · · ·

(11.66)

The input signal consist of three parts: (1) the DC bias voltage V0 , which places the device at the correct operating point on the I –V curve, here the gap voltage Vg , (2) the lo-voltage vlo = Vlo cos (ωlo t), and (3) the weak signal we want to retrieve, vs = Vs cos (ωs t) where ω = 2πf . When these voltages are inserted into the expansion, Eq. 11.66, the resulting terms can be gathered according to their common coefficients ai . The sum of terms with the coefficient a1 is a scaled replica of the sum of all inputs. This is not what we are searching. Rather, the term we are interested in is found in the sum with the a2 coefficient: 2Vlo Vs cos ωlo t cos ωs t = Vlo Vs {cos(ωlo − ωs )t + cos(ωlo + ω)t}

2flo

Power

flo fif = |fs − flo|

0

fi

−1

(11.67)

fs

+1 Frequency

|3flo − fs|

−2

|flo + fs|

+2

Figure 11.20 Power spectrum for a mixer with the local oscillator (lo) and the signal frequencies applied. Note also the intermediate and image frequencies.

HIGH-FREQUENCY RADIO TECHNOLOGY

347

Here, the down-converted if voltage at fif = |fs − flo | is present, as well as a correspondingly up-converted one. By adjusting the local oscillator frequency ωlo various received signals can now all be converted to the same if frequency and amplified at the same frequency. The point is here that a single state-of-the art if amplifier optimized just for one frequency can handle a wide range of signal frequencies. A sweep of lo frequencies will give access to a range of received signal frequencies. The SIS junction has a pronounced microwave response, as illustrated in Figure 11.21, where the characteristics are shown both with and without lopower applied. At low-frequency radiation, the I –V curve is smeared at the gap singularity, the current increases at sub-gap voltages, and the DC Josephson current is depressed. Photon induced steps appear as the rf frequency is increased. These are of two kinds. Figure 11.21 (b) indicates photon-induced steps in the quasiparticle current at voltages 2 /e ± mhflo /e. They occur as photons are absorbed (or emitted) in the tunnelling process, thus allowing electrons to tunnel into the high density of states above the energy gap. The photon-induced structure increases in strength with microwave power until superconductivity is quenched. The other kind of steps (Figure 11.21(d)), is due to Josephson mixing products falling at zero intermediate frequency for bias voltages corresponding to multiples of the applied frequency (2eVk / h = fJ = kflo ). The amplitude of

(f) C RSJ

R SH 40 (e)

Current (µA)

Ic 20

h f lo e

(b)

(d)

(a)

0

2∆ e

−20 −40

(c) hf lo e

dVg

−4

−2

0

2

4

−2

0

2

4

Voltage (mV)

Figure 11.21 Typical I –V curves for SIS tunnel junctions. For a low critical current junction (or with an applied magnetic field) the left-hand curves show the I –V curve without (a) and with (b) lo applied (∼240 GHz). The right hand curves show how the Josephson effect changes the I –V curves without (c) and with (d) lo applied (∼240 GHz). Outlined in the figure is the I –V curve of a resistively shunted tunnel junction (RSJ), and the corresponding electrical circuit (e resp. f ). A Josephson mixer could also be biased at the open circle. After Winkler et al. [166].

348

SMALL SCALE APPLICATIONS

these Shapiro steps vary as Bessel functions, Jn (α1 ), with normalized microwave amplitude α1 = 2eVlo / hflo . Josephson junctions can be used in a number of applications, based on the effects that relate current and voltage via the phase difference across the junction. Some prominent examples are high frequency oscillators, voltage standards, parametric amplifiers, Josephson video detectors and mixers.4

4 Further

recommended reading may be found in the review by Winkler et al. [166].

12 Superconducting Wire and Cable Technology 12.1

Low-Tc wire and cable

12.1.1

Introductory remarks

Technical superconductors for energy and magnet applications1 consist of composite wires of superconducting and normal conducting material, both in high-Tc (HTS) or low-Tc (LTS) applications. To stabilize the superconducting state the superconductor is subdivided into a multi-filamentary structure embedded in low resistivity normal conducting matrix. As far as LTS applications is concerned, only the intermetallic stoichiometric compound Nb3 Sn and the alloy NbTi are important. In both of these the matrix consists of low resistance Cu matrix. Filament diameters range from a few µm to about 100 µm, and the filament number can be as high as 100 000. Wire diameters are between 0.1 mm and 2 mm, and the current capacity range is from a few ampere to 1000 A in fields up to 20 T in the liquid helium range at or below 4.2 K. The fabrication process includes bundling of components into a billet, with subsequent extrusion and drawing. Conductors for high current use are produced in the form of fully transposed cables. Depending on the design, additional stabilizer material of copper and aluminium, as well as strengthening members and cooling channels may be added. Wires of ceramic high-Tc cuprates are mostly manufactured by the powderin-tube method. Here the leading first generation technology is based on the development and use of BiSrCaCuO/Ag wires. These can tolerate magnetic 1 Based largely on the review by Krauth in Fossheim: Superconducting Technology. 10 case studies. [167] For further reading we recommend Buckel: Supraleitung [168], Wilson Superconducting magnets [169], R. P. Reed and Clark Materials at Low Temperature [170], Collings Applied Superconductivity, Metallurgy and Physics of Titanium Alloys [171] and Foner and Schwartz: Superconductor Material Science [172].

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

350

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

fields up to more than 20 T at 4.2 K. Even at 77 K the quality of these conductors is becoming interesting for some applications, as we will give examples of in the following. A second generation of superconductor tapes, manufactured by film deposition on a suitable substrate is emerging, and should be expected to take over the market.

12.1.2

General design considerations

The primary characteristics in the design and fabrication of technical superconductors may be broken down into three groups: 1. Superconductor properties

Critical temperature Tc Upper critical field Bc2 Critical current density Jc

2. Design of composite wire: Superconductor filaments in normal matrix

Stability against transition to normal state (quenching) AC losses Mechanical characteristics

3. Fabrication technology

Fabrication of multi-filamentary composites Fabrication of high current conductor cables with additional stabilization, mechanical reinforcement and cooling channels Compatibility of conductor properties with magnet fabrication technologies.

In the following we will discuss these three areas of wire and cable technology in turn, and give examples of results obtained.

12.1.3

Basic superconductor properties

The transition from normal-conducting to superconducting state is determined by three critical parameters, the critical temperature Tc , the upper critical field Bc2 , and the critical current density Jc . The first two are determined by the electronic properties, including the pairing mechanism for Cooper pair formation. In typical low-Tc materials of technical importance these parameters cannot be manipulated to any important extent. In high-Tc cuprate materials they can be manipulated first by choice of material composition, of which there are now a great number, and next by doping of the chosen material. However, in reality only optimally

LOW-Tc WIRE AND CABLE

351

Table 12.1 Development of the highest known Tc as a function of time. Tc and Bc2 values of some prominent materials Superconductor Nb NbZr NbTi V3 Ga Nb3 Sn (Nb, Ta)3 Sn Nb3 Ge PbMo6 S8 Y1 Ba2 Cu3 O7 Bi2 Sr2 Ca1 Cu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 Ca2 Cu3 O10

Tc 9.2 K 10.8 K 10.2 K 16.5 K 18 K 18 K 23 K 14 K 90 K 90 K 110 K 125 K

Bc2 (4.2 K) 0.27 T 11 T 11 T 22 T 22 T 25 T 30 T 45 T Highly anisotropic ≥50 T, BCu-O-layers ≥200 T, B ⊥Cu-O-layers

doped materials, to the highest achievable Tc are technically interesting. For values of Tc and Bc2 in important materials, we refer to Table 12.1. The critical current density Jc is strongly dependent on temperature and magnetic field in all classes of materials. In high-Tc materials Jc is in addition, strongly anisotropic, and depends critically on grain boundary alignment (texturing) and on successful introduction of pinning centres. Clearly, these aspects bring processing technology to the forefront as the key to achieving successful material control during manufacture of wires and cables. Optimization of Jc is a demanding task in all bulk superconductor applications, but specially so in the high-Tc cuprates. The great potential advantages of high-Tc materials are their high critical temperature and high upper critical fields. These advantages are easily lost unless extremely careful processing methods are developed to meet the challenges mentioned. In recent years much progress has been made in making multi-filamentary wires even of high-Tc superconductors, especially Bi2223 and Bi2212, by the powder-in-tube method. A new generation of highTc wires and cables is under development by superconductor film deposition on non-superconducting substrates with matching lattice constant. The ultimate success of high-Tc applications in the area of wires and cables will depend crucially on the outcome of this extremely demanding processing development. Only the solid solution alloy NbTi- and the Nb3 Sn-based binary intermetallic compound have so far reached the stage of an industrially produced commercial superconductor. The optimum composition of NbTi contains about 47 to 50 wt. per cent Ti. The exact critical parameters of Nb3 Sn depend on the composition and the perfection of the superconducting A15 phase. In ternary compounds like (NbTa)3 Sn or (NbTi)3 Sn Bc2 can be enhanced without sacrificing too much in Tc and workability. Adding 7.5 wt. per cent Ta to the Nb results in a Bc2 shift of about 3 T. According to the Bc2 values NbTi conductors can be used up to field levels of 10 T and Nb3 Sn-based conductors up to about 20 T. Possible candidates

352

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

for applications beyond 20 T are Chevrel phases, like PbMo6 S8 , or HTS like Bi2 Sr2 Ca2 Cu3 O10 and Bi2 Sr2 Ca1 Cu2 O8 when operated at low temperature. Due to their crystal structure with the superconductivity mainly in the CuO2 planes, the behaviour of HTS in a magnetic field is highly anisotropic, leading to much higher Bc2 values when the magnetic field is parallel to the CuO2 planes as compared with the field perpendicular to these planes. A high critical current density Jc at operational field is a precondition for most applications. Usually Jc values of 105 to 106 A/cm2 are desirable. A lower limit is 104 A/cm2 . A type II superconductor is penetrated by the magnetic field in form of quantized flux lines. Only the volume outside the flux line remains superconducting. Bc2 is reached when the flux lines fill up the total volume. An ideal type II superconductor can not carry a superconducting current because the flux lines move by the Lorentz force. This movements leads to electric fields and therefore to losses. The superconductor must therefore be hardened by microstructural features acting as pinning centres for flux lines. Effective pinnings centers can be for instance precipitates of normal conducting phase, like in NbTi, or grain boundaries as in Nb3 Sn. But grain boundaries may at the same time act as weak links, thus impeding the current flow from one grain to its neighbour. Thus it is possible to have high intragrain Jc , yet at the same time low intergrain Jc in the same material, giving low overall transport critical current density. High-Tc materials are well known for such problems, among them YBCO. As we have discussed in Chapter 8 the critical current density Jc is defined at the point where the Lorenz force begins to exceed the pinning force, i.e. at the onset of flux flow . In this regime, above Jc , current transport is no longer lossless. But even at low current density another loss mechanism is active. This is the flux creep process. The presence of such effects is seen in the decay of magnetization with time. The creep effect is usually very small in the liquid helium range, but becomes more and more significant as the temperature is increased. This is a well-known problem in all high-Tc materials operating at elevated temperatures up to 77 K or higher. We refer to the Topical Contribution by Muralidhar and Murakami (Section 13.4) showing how a sophisticated interplay between composition and processing can improve pinning up to 77 K in YBCO-type high-Tc materials. Another important phenomenon related to flux penetration and flux pinning is so-called flux jump. This phenomenon, which can lead to severe instabilities, may be suppressed by appropriate design. Due to inhomogeneities of the material the onset of flux flow is not a sharp criterion for determination of critical current. A practical criterion is therefore used: Jc is defined as the current density at the point where a 1 µV/cm electric field is observed across the sample in the transport direction. In small laboratory scale experiments the criterion is often set simply as 1 µV. A corresponding criterion using resistivity measurements is to identify the current where the resistivity reaches 10−14 to 10−13 m. Often the transition from superconducting to

LOW-Tc WIRE AND CABLE

353

107 0.1 µV/cm

Nb3Sn

(NbTa)3Sn

Jc non Cu [A/cm2]

106

10−14 Ωm

NbTi

4.2 K 2K 4.2 K 2K 4.2 K 2K

105

104

103

102 0

2

4

6

8 10 12 14 16 18 20 22 24 26 B [T]

Figure 12.1 Critical current density as a function of magnetic field and temperature for metallic superconductors: NbTi, Nb3 Sn, (NbTa)3 Sn at 4.2 K and 1.8 K, respectively. In case of Nb3 Sn-based conductors the bronze area is included in the calculation of Jc .

normal transport can be described by a power law, as discussed in Chapter 8, i.e. E ∝ I n . The higher the exponent n, the higher quality of a technical superconductor. A high value of the exponent n reflects uniform pinning and generally uniform material conditions. In Figure 12.1 Jc values of commercial grade NbTi, Nb3 Sn, and (NbTa)3 Sn are shown as a function of magnetic field at 4.2 K and 1.8 K. In Nb3 Sn the conductors were produced by the bronze route, as will be explained below. In this case the bronze area is included in the calculation of Jc . An estimate of Jc in the superconductor is obtained by multiplying the Jc value by a factor of 3.

12.1.4

Design of technical superconductors

The starting point for the mechanical design of a technical superconductor is its behaviour in a magnetic field. This field may be of external or of internal origin

354

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(self-field). According to the Bean model the full penetration field Bp , which is the maximum field that can be shielded is, as shown in Chapter 8 Bp = 2µ0 Jc a

(12.1)

in a slab of thickness 2a. We have referred to this condition as the critical state. Figure 12.2 and the discussion of the Bean model in Chapter 8 should be consulted for a better understanding of how this model describes flux penetration under different external fields Bm . In the Bean model, as we have

Bext

Jc

Jc

B T2

Bext Bp

Bext

T1

2

−a

+a

Bm

(1)

2a (b)

(a)

(c)

Bp

Bm

(2)

(a)

(b)

(c)

(d)

Figure 12.2 Field pattern in a superconducting slab according to the Bean model. Upper: field and current directions and field patterns for two temperatures T2 > T1 , (Jc (T2 ) < J (T1 )). Lower: Field pattern for a time varying field with amplitude Bm /2: (1) Bm < Bp , (2) Bm > Bp .

355

LOW-Tc WIRE AND CABLE

seen, Jc is defined by the field gradient, which is taken to be constant, i.e. dB = µ0 Jc dx

12.1.5

(12.2)

Stabilization

The Bean model does not say anything about stability. In reality there is always a decay of currents. This means that the field profile will flatten out, or ‘thermalize’, given sufficient time. The time taken for this process can vary by many orders of magnitude depending on the controlling factors for flux creep: temperature and pinning barriers. In addition, strong external disturbances can cause flux jumps with large energy dissipation, which can lead to quench of the superconductor. Such severe disturbances can be of magnetic, thermal, or mechanical nature leading to a positive feedback. Functional breakdown events due to such effects may be avoided by appropriate prevention measures. (i) Reduction of available magnetic energy by fine subdivision of the superconductor volume so that the heat capacity of the superconductor and its nearest surrounding matrix is high enough to limit the temperature increase T following the flux jump event. The technical term for this is adiabatic stabilization. (ii) Damping of the rate of flux change by highly conducting surrounding normal conducting matrix, Cu or Al. This ensures both a reduced heat generation and efficient heat removal to the coolant. The technical term for this is dynamic stabilization. The subdivision required to achieve these goals can be calculated by accounting for both energy and power balance, respectively. In case a magnetic field is perpendicular to the wire axis, the adiabatic stabilization requirement on the superconducting filament diameter d is 2 d< Jc

CT µ0

1 2

(12.3)

c where C is the volumetric specific heat, and T = dJ−J . Usually Jc decreases c /dT linearly with temperature so that T = Tc (Bop ) − Top , where Bop and Top are operational field and temperature, respectively. For typical parameter values of NbTi at 4.2 K this results in d < 100 µm filament diameter. When this criterion is used at 77 K for HTS systems one finds that much larger diameters are allowed due to the far higher heat capacity of both the superconductor and the matrix. Obviously, such thin filaments have a quite low current carrying capacity. Therefore a large number of them may be needed, bundled together and embedded in a normal conducting matrix. If this matrix is electrically and thermally highly conductive, one can achieve dynamic stabilization according to the above analysis. To avoid an unacceptable temperature increase inside a

356

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

filament, the following criterion must be fulfilled to prevent flux jumps: d

1 the result is B2 Qh = m 2µ0

For

Bm Bp

Bp 2 − Bm 3

Bp Bm

2 (12.9)

1 this gives, when combined with the Bean equation (Eq. 12.1) Qh = Bm Jc an

(12.10)

The demagnetization factor n has been included here. For circular filaments in a transverse field configuration n = 2. As can be seen from Eq. 12.10 magnetization and hysteresis losses can only be kept small by using fine filaments. For most applications d = 5–10 µm is sufficient, but for 50 Hz applications sub-micrometre filaments are required. The coupling losses Qc can be estimated for slow field changes, i.e. for Tm τ , according to B 2 8τ (12.11) Qc = m 2µ0 Tm

LOW-Tc WIRE AND CABLE

359

where Tm is the field rise time and τ is the conductor time constant given by τ=

2 µ0 lp 8π 2 ρtr

(12.12)

Here lp is the twist pitch (or transposition length lt ) as before, and ρtr is the effective transverse resistivity of the matrix (or of the cable or braid). Since lp typically is limited to values larger than about 10 times the respective diameter if each stage (strand or cable stage), the only means to reduce the coupling losses further is by introduction of resistive barriers, for instance CuNi, into the composite.

12.1.7

Mechanical characteristics

Important design criteria are related to mechanical loads that a superconductor has to accommodate during building and operation, i.e. during coil winding, cool-down, operation, and warm-up. The stresses during operation are dominated by magnetic forces. Typically the stress level is given by σ = JBR

(12.13)

where J is the overall current density, B is the magnetic field, and R is the coil radius. The conductor must withstand these stresses without mechanical damage and without degradation of the critical current density. NbTi conductors show little degradation of Jc as a function of stress and strain. Nb3 Sn-based conductors are much more sensitive to strain, especially in high magnetic fields. Also, Nb3 Sn conductors are very brittle after reaction (discussed below) and allow only strain levels below 0.3% for safe operation.

12.1.8

Fabrication technology

As described above, a technical superconductor consists of a composite of superconducting filaments and a stabilizing matrix, with additional optional components. A suitable fabrication process must be capable of producing long length of composite conductors in a reliable and economic way. The process must allow to optimize the superconducting properties, especially the current carrying capacity. The completed composite wire must be processable into more complex conductor geometries, like cables and magnet coils. In spite of the fact that many superconducting materials are known, the complexity of all these requirements has so far resulted in only two low-Tc materials of technical importance for bulk applications. These are the ductile alloy NbTi and the brittle intermetallic compound Nb3 Sn. Due to its difficult handling Nb3 Sn is only used at high fields

360

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(greater than 10 T) where the current carrying capacity of NbTi decreases very strongly. The fabrication of a multi-filamentary wire is shown schematically in Figure 12.5. In the case of NbTi/Cu composite, prefabricated NbTi and Cu parts are bundled inside a Cu-tube to form a billet with an outer diameter of typically 100–200 mm. The billet is evacuated and warm extruded to a rod of 20–70 mm diameter. Further area reduction is achieved by cold working on drawing benches, bull blocs, and multiple drawing machines. Twisting of the wire is performed close to final dimension. The number of NbTi filaments and the copper to superconductor ratio is chosen according to the application. The composite wire can be further processed into rectangular and other profiles and cables required for special applications. Co-processing of NbTi and Cu is possible because both materials are quite ductile and are similar with respect to hardness and resistance to deformation. With other, less favourable materials combinations other solutions had to be found. In some cases stabilization with ultrapure aluminum is desirable due to very low residual resistance. A process to achieve Al-stabilized conductor is by co-extrusion of Al onto a prefabricated NbTi/Cu composite wire or cable as shown in Figure 12.6. In Figure 12.7 some examples of NbTi conductors may be seen. The brittle Nb3 Sn compound cannot be processed by either coldworking or warmworking. The solution is to use a composite of ductile precursor materials and to develop the superconducting phase after the deformation process. The most reliable method is by the bronze route where Nb rods are embedded in a CuSn bronze, and the Nb3 Sn is formed by solid sate diffusion and reaction

Billet

Extrusion

Drawing

Twisting

Figure 12.5 Fabrication of a multifilamentary conductor. Conductors with a very large number of filaments (>10 000) are produced by a two stage bundling and extrusion.

Aluminium

Conductor

Profiling

Cabling

Co-extrusion

Figure 12.6 Examples of processing of multifilamentary wires for special applications (rectangular profiling, cabling, co-extrusion with aluminium).

LOW-Tc WIRE AND CABLE

(a)

(b)

(c)

(d)

361

Figure 12.7 Configuration of NbTi conductors. (a) Standard conductor with 54 filaments and a Cu:NbTi ratio α = 1.35 for Nuclear Magnetic Resonance (NMR) and laboratory magnets. Typical wire diameter 0.7 mm. (b) Conductor with 24 filaments and α = 6.5 for whole body magnetic resonance imaging (MRI) magnets. Typical wire diameter 1 to 2 mm. (c) Conductor with 6000 filaments with 5 µm diameter at a wire diameter of 0.65 mm for accelerators with low magnetization requirements for the filaments. (d) Conductor with 1200 filaments with 10 µm diameter and mixed Cu/CuNi matrix with low hysteresis and coupling losses e.g. for pulsed field applications. After Krauth in Fossheim [167].

process at about 700 ◦ C. This is the reason why the Nb3 Sn configuration differs from that of the NbTi conductor. To allow effective transformation of the Nb into Nb3 Sn within a reasonable time, in practice a few days, the filament diameter is limited to about 3 to 5 µm. Consequently, a very high number of filaments is required, typically 10 000, such that the bundling and deformation process has to be performed twice. In addition, the CuSn matrix does not stabilize and protect the conductor, so that additional copper has to be added, preferentially in the second bundling process. The pure Cu has to be protected from poisoning by Sn during the reaction heat treatment by means of a diffusion barrier, for instance of Ta. Figure 12.8 shows examples of resulting multi-filamentary wires. Optimization of critical current density is part of the conductor fabrication process. It is determined by the microstructure, and can therefore be controlled during the fabrication process. Optimization of Jc is achieved by introduction of finely dispersed microstructural features acting as pinning centres. In the case of NbTi normal conducting α-Ti precipitates in the superconducting β-phase are

362

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

(a)

(b)

(c)

(d)

Figure 12.8 Configuration of Nb3 Sn conductors with Ta diffusion barriers. (a) Standard conductor with 6000 filaments in a bronze matrix and internal Cu stabilization. (b) Conductor with 20 000 filaments and external Cu stabilization. Fully transposed flat (keystoned) cables for accelerator magnets (dipoles and quadrupoles). (c) 23 NbTi strands with 0.84 mm diameter. (d) 36 Nb3 Sn strands with 0.92 mm diameter. After Krauth in Fossheim [167].

known as the most effective pinning centres. In the case of Nb3 Sn the grain boundaries act as pinning centres. A microstructure with fine grains is therefore required to get high Jc -values. This is achieved by performing the reaction heat treatment at about 700 ◦ C for three days. The reaction treatment can be performed either before the coil winding (react-and-wind) or after coil winding (wind-and-react). The latter is mostly used for small magnets, and the former for large magnets with low bending strain during coil winding.

12.2 High-Tc wire and cable 12.2.1

High-Tc wire and tape

Successful development of high-Tc wire as a basis for high current transport was so far achieved by use of Bi2223, and to some extent using Bi2212 material. The dominating methodology is to produce wires by the powder-in-tube (PIT)

HIGH-Tc WIRE AND CABLE

363

technique. This is done by filling the pre-reacted powder into silver a tube. Its dimension will determine how long length can eventually be produced. The resulting filled tube is extruded and drawn to several times its original length. Continued drawing leads to a single filamentary wire which may be rolled to the dimension of about 3 mm width and 0.3 mm thickness. After processing at temperatures approaching 900 ◦ C in oxygen atmosphere, and subsequent cooling to room temperatures at varying rates, a superconducting wire results. In the next stage multi-filamentary wires of 100-odd superconducting tape wires of kilometre lengths is produced. Production of such wires involves a repetition of the drawing stage in which the first extruded and partially drawn tube is cut into short lengths of metre size, and packed into a second Ag tube. The drawing and rolling process is now repeated, resulting in a multi-filamentary tape shaped wire. Thermal processing is similar to the single filament case. To illustrate the sophistication required to develop second generation of conductors of the quality required on a large scale, we refer to the Topical Contribution, by Thompson and Christen (Section 13.9).

12.2.2

Full-scale high-Tc cable

The technology for high-Tc cable manufacturing is maturing gradually. Several projects are under way. Full scale cables have so far been manufactured from Bi2223 tapes only. The next generation of tapes based on deposition of YBCO film is expected to provide great improvements in the long run. The speed of the manufacturing process is still far too low for this next generation of tapes to be applicable in cables. A good example of high-Tc cable implementation using Bi2223 tapes is the Danish HTS power cable project [173], the first HTS cable operated in a public network. In 2001 installation of a 30-m, 30 kVrms , and 2000 A three-phase HTS cable was carried out in a substation of the Copenhagen utility network. One year later, the operating experiences were deemed satisfactory. The cable supplied electric energy corresponding to the average consumption of about 25 000 households, over 100 000 MWh of energy. The advantages seen for a HTS power cable may be listed as follows • High current and power rating • Compact cable dimensions and low weight (about 1/3 of conventional cable) • Low losses • No thermal or magnetic interaction with surroundings. HTS power cables have a potential for reduced cost per transferred unit of energy compared to conventional technology due to low material consumption and potentially lower installment cost. The cables may be used as short internal

364

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY

Figure 12.9 The Danish HTS cable design [173]. Reproduced with the authors’ permission.

substation connections and retrofits (replacement) of low capacity conventional cables in existing ducts. They may further be applied for urban feeder cables, bulk power transmission, low-voltage high-current cables, DC power, etc. The design of the Danish HTS cable is shown in Figure 12.9. The superconducting tapes are wound in a helical pattern on the inner corrugated flexible steel tube. The superconductor is cooled by liquid nitrogen flowing through the steel tube at a rate of 700 kg/hour at 4 bar. The HTS tapes are nowhere in direct contact with liquid nitrogen. The main structure from inner to outer layers is briefly characterized by the following sequence: The inner tube, called the ‘former’, on which the superconducting tapes are wound, has an outer diameter of 30 mm. Then follow first the superconductor tape layers, next a thermal insulation layer, an electrical insulation layer, an electrical Cu-screen, and finally a polyethylene sheath of ID/OD dimensions 95/105 mm. The critical current Ic was measured as 2770 A at 79 K, and 5000 A at 66 K. No degradation was detected during one year of operation.

12.2.3

HTS induction heater

Electromagnetic induction heating is commonly used for industrial heating of metals. Figure 12.10 illustrates the principle involved in induction heating [174]. A metal workpiece is placed inside a solenoidal coil, and when an AC current is passed through the windings, the time-varying magnetic field generated by the coil induces electric currents in the metal, causing resistive dissipation and

HIGH-Tc WIRE AND CABLE

365

Figure 12.10 Principles of billet heating using a superconducting coil [174]. Reproduced with the authors’ permission.

heating of the workpiece. For aluminum extrusion the typical billets used for extrusion are of about 20 cm diameter and 1–2 m length. The billet is heated to temperatures of around 500 ◦ C in about 2 min to soften the metal just before extrusion takes place. Runde and coworkers [174] have introduced a new concept in induction heating by use of high-temperature superconductor (HTS) windings in the induction coil. The great advantage is that the losses in the coil can be reduced to a small fraction of those in conventional coils. A simple analysis shows that the overall electrical efficiency η may be expressed as 1

η= 1+

ρc ρw µw

(12.14)

where ρc and ρw are the resistivities of the coil and the workpiece, respectively, and µw is the permeability of the workpiece. From Eq. 12.14 we observe that if the resistivities of the workpiece and the coil are similar, the efficiency approaches 1/2. However, if the resistivity in the coil is eliminated, the efficiency approaches 1, or 100%. These are of course ideal values, but the effect is in any case very significant. A demonstrator HTS induction heater has been shown to work as expected. The coils were of so-called stacked pancake design made of stainless steel reinforced multi-filamentary Bi-2223/Ag tape with a self-field

366

SUPERCONDUCTING WIRE AND CABLE TECHNOLOGY Epoxy cryostat

Superinsulation

Flux diverters HTS coils

LN2

Al billet

Thermal insulation

Figure 12.11 Cross-sectional view of the induction heater. The heater is concentrically built up around the dash-dotted symmetry line. The current leads and various structural parts made in fibreglass reinforced epoxy are not included in the drawing [174]. Reproduced with the authors’ permission.

critical current of 115 A. Figure 12.11 shows the design used. The reduced scale demonstrator prototype reached 500 ◦ C in about 5 minutes. In the original tests, DC HTS tapes were used. With AC tapes one would expect to be able to apply higher currents, and reduce the heating period substantially. An important feature of the design is the insertion of iron rings at each end of the coil. These are placed there to prevent solenoidal stray field from taking a short route through the coil near its ends. This would have allowed some field to cross the pancake coil windings normal to the tape, a field configuration which has a strongly detrimental effect on the critical current in Bi2223 tapes.

12.3

Magnet technology

Superconducting magnet technology is a mature field today, and well described in textbooks. In the present context we have found it interesting to present two outstanding unconventional examples of recent development in superconductor

MAGNET TECHNOLOGY

367

magnet applications. The frist one is a description of a fullscale complex magnet system, the worlds strongest, 45 T, stationary field hybrid magnet, built and operated by the National High Magnetic Field Laboratory at Florida Sate University in Tallahassee, Florida. For this outstanding example of magnet technology we refer to the Topical Contribution by Schneider-Muntau in Section 13.5. The second example is a pure materials development which has been carried out at the Superconductivity Research Laboratory at ISTEC in Tokyo. Murakami has led the efforts to tailor the pinning properties of YBCO-type cuprate superconductors for storage of truly high magnetic field. We refer to the topical contribution in by Muralidhar and Murakami (Section 13.4) on this subject.

PART IV

Topical Contributions

Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

13 Topical Contributions This Chapter contains nine invited contributions written for this book by particularly outstanding scientists from Europe, Japan and USA in various fields of superconductor research. The authors have been asked to write their contributions in as short form as seemed pedagogically possible. These examples highlight specific subjects at the forefront of research and development at the time of writing this textbook. Scientific references belonging to this chapter are given at the end of the chapter.

13.1

Spin-Triplet superconductivity by Y. Maeno

What is the spin triplet superconductivity? When two electrons form a pair in the superconducting state, the total spin of the pair is either S = 0 (spin singlet) or 1 (spin triplet). Because of the symmetry relation for the permutation of electrons as Fermions, the state vector of a Cooper pair | = χ (k 1 , k 2 )|σ1 , σ2 must be antisymmetric with respect to the exchange of the two electrons involved. Here k i and σi are the momentum and spin of an electron and χ is the orbital wave function. For spin-singlet state with antisymmetric spin part, | ↑↓ − | ↓↑, the orbital wave function has to be symmetric so that the allowed orbital angular momentum L of a pair contains even-number components only: L = 0 is called the s-wave, L = 2 the d-wave, etc. It is in principle possible to form spin-triplet pairs. In this case the spin state is symmetric, | ↑↑, | ↑↓ − | ↓↑, or | ↓↓, corresponding to Sz = 1, 0, or −1, respectively. Thus the orbital wave function has to be antisymmetric with the orbital angular momentum L = odd number: L = 1 is called the p-wave, L = 3 the f-wave, etc. Conventional superconductors are in the spin-singlet s-wave state. However, a number of unconventional non-s-wave superconductors have been found. For Superconductivity: Physics and Applications Kristian Fossheim and Asle Sudbø c 2004 John Wiley & Sons, Ltd ISBN 0-470-84452-3

372

TOPICAL CONTRIBUTIONS

example, it has been shown that even the high-transition temperature copperoxide (high-Tc cuprate) superconductors have spin-singlet electron pairs, but the pairing is in the d-wave symmetry.

Which superconductors are spin triplet? Investigation of spin-triplet superconductivity started soon after the birth of the BCS theory [1]. It has been well established that superfluidity of 3 He is carried by Cooper pairs of 3 He atoms with their nuclear spins forming spin-triplet states [2]. However, it has not been easy to prove whether a candidate superconductor is in fact spin triplet, mainly because the Meissner effect masks the magnetic susceptibility of the electron spins. Nevertheless, there are a number of superconductors for which the spin-triplet pairing is strongly suggested [3]. An earlier example is the heavy Fermion superconductor UPt3 , for which there are three superconducting phases when the magnetic field and temperature are varied. Recently, a new class of superconductors have been found in which superconductivity occurs below the transition temperature of ferromagnetic ordering and coexists with the ferromagnetism. A good example of this class of superconductors is UGe2 . A layered ruthenate Sr2 RuO4 [4] is a unique example because it is probably the only oxide for which spin-triplet nature has been confirmed so far. As shown in Figure 13.1, its crystal structure is common to the first high-Tc cuprate superconductor discovered by Bednorz and M¨uller, La2−x Bax CuO4 , but the Tc of Sr2 RuO4 is 1.5 K, much lower than the corresponding high-Tc cuprate. Since the electronic properties of its normal state is characterized in detail, it is arguably the most extensively and quantitatively characterized spin-triplet superconductor [3]. From the nuclear magnetic resonance (NMR) Knight shift, the spin susceptibility for the magnetic field parallel to the RuO2 layer was found to be unchanged on entering the superconducting state, marking the definitive evidence for the spin-triplet pair formation with Sz = 0 [5]. In addition, from the muon-spin relaxation measurements, spontaneous internal magnetic field was found to emerge below Tc [6]. This suggests that the time-reversal symmetry (TRS) is broken in the superconducting state. The origin of the broken TRS is attributed to the unquenched orbital angular momentum of the pairs; thus Lz = +1 or −1. Taking into consideration of consistencies with a number of other experimental results, as well as with theoretical requirements, it is believed that the pairing state is described as S = 1, Sz = 0; L = 1, Lz = +1 or −1. Such spin and orbital state for this p-wave superconductivity is schematically represented in Figure 13.2. The mechanism of the spin-triplet formation has not been fully understood, but it is believed by many that the strong electron correlations due to Coulomb interactions among the 4d electrons of ruthenium ions play the essential role in the pairing, rather than the conventional electron-phonon interactions.

SPIN-TRIPLET SUPERCONDUCTIVITY BY Y. MAENO

Sr2RuO4

La2-cBacCuO4

Sr

La (Ba)

Ru

Cu

O

373

O

C

a a

Figure 13.1 The layered crystal structure common to the spin-triplet ruthenate superconductor and high-Tc cuprate superconductor. Image is by K. Deguchi.

Orbital angular momentum

Electron

Spin

c (z) b a

Figure 13.2 The representation of the spin triplet electron pairs in Sr2 RuO4 . Small arrows depict the spins of an electron pair, while the large arrow represents the orbital angular momentum. Image is by K. Deguchi.

New physics expected with spin-triplet superconductivity For spin-triplet superconductors, not only the charge degree of freedom, but also the spin degree of freedom exhibits “superfluidity”. Thus a variety of phenomena not present in spin-singlet superconductors are expected. Because of the internal degree of freedom of the triplet pairs, multiple superconducting phases are excepted to emerge and they are in fact observed in Sr2 RuO4 , as well as in UPt3 [3]. Although not reported in any superconductor so far, induction of collective motions of spin or orbital moments without breaking the pairs is also expected. For Sr2 RuO4 the phase of the wave function should vary with the

374

TOPICAL CONTRIBUTIONS

azimuthal angle and effects sensitive to this phase are also expected in the tunneling. Furthermore, the TRS broken state is characterized by “chirality”, with all the Cooper pairs within a single superconducting domain having a common sign of their orbital moments (plus or minus). If the chirality can be externally controlled, it may be used as a quantum bit, a nanoscale unit for future quantum devices.

13.2 π -SQUIDs – realization and properties by J. Mannhart The predominantly dx 2 −y 2 -pairing symmetry of the high-Tc superconductors influences fundamental properties of Josephson junctions and Josephson junction-based devices, such as Superconducting Quantum Interference Devices (SQUIDs). Notably, it offers the possibility to fabricate Josephson junctions which in equilibrium are biased by a phase shift of π , and dc π -SQUIDs which consist of such a π -Josephson junction and a conventional junction connected in a loop [7]. The electrical characteristics of these devices provide detailed insight into the symmetry of the superconducting order parameter, tracing for example possible admixtures of sub-dominant symmetry components. Furthermore, the devices present novel building blocks for superconducting quantum electronics [8]. All-high-Tc dc π -SQUIDs have been fabricated according to the design illustrated in Figure 13.3. A detailed description has been provided in [7]. Exploiting the bicrystal technology [9], the devices are based on two ∼10 µm wide, symmetric 45◦ [001]-tilt grain boundaries formed by ∼100 nm thick, c-axis oriented YBa2 Cu3 O7−δ -films grown on SrTiO3 -tetracrystals. Due to the orientation of the grain boundaries, across one of the junctions order parameter lobes with opposite signs face each other. This π -phase difference defines the π -junction. In practice the π -junction is the junction with the smaller critical current, because it has the smaller Josephson coupling energy. The current-voltage, I (V )-characteristics of the π -SQUIDs follow the behavior expected according to the resistively shunted junction model, with additional self-induced resonances which disappear for small applied magnetic fields, as shown in Figure 13.4 [10]. The magnetic field dependencies of the π -SQUIDs critical currents Ic (H ) (see Figure 13.5) are characterized by a minimum at small fields, exactly opposite to the behavior of the standard SQUIDs’ critical currents, which for vanishing applied fields are maximal. This characteristic effect is expected for superconductors with a pure dx 2 −y 2 -symmetry. The Ic (H )dependencies for larger applied magnetic fields are highly symmetric, proving that the measurements are not influenced by spurious trapped magnetic flux [7]. The self-induced resonances shown by the π -SQUIDs’ I (V )-characteristics reveal that in the voltage state the dx 2 −y 2 -wave symmetry induces circulating

π -SQUIDS – REALIZATION AND PROPERTIES BY J. MANNHART

375

Figure 13.3 Sketch of a π-SQUID fabricated by using the bicrystal technology (after [7]).

200

p- SQUID 4.2 K 0 µT

100

V (µV)

2.55 µT 0

−100

−200 −30

−20

−10

0 I (µA)

10

20

30

Figure 13.4 Current-voltage characteristics of a π-SQUID measured at 4.2 K at zero field and at the smallest magnetic field that causes a maximum of Ic (from [10]).

ac-currents, which oscillate with the Josephson frequency in the π -ring configuration. This provides evidence that the π -shift as well as the order parameter symmetry are maintained for Josephson frequencies up to several tens of GHz [10]. The technology to fabricate π -Josephson junctions and π -SQUIDs is extendable to the design of circuits with larger numbers of π -type junctions. Well operating π -SQUIDs have now also been fabricated by using the ramp-type Josephson junction technology [11].

376

TOPICAL CONTRIBUTIONS 0 - SQUID 15

0.4

10

0.2

5 Ic (µA)

Ic (µA)

p- SQUID 0.6

0.0

0

−0.2

−5

−0.4

−10

−0.6

−6

−4

−2 0 2 m0H (µT)

4

6

−15

−6

−4

−2 0 2 m0H (µT)

4

6

Figure 13.5 Dependencies of the critical current on applied magnetic field of a π-SQUID and of a standard SQUID at 77 K (from [7]).

This work was performed together with H. Bielefeldt, B. Chesca, B. Goetz, H. Hilgenkamp, A. Schmehl, C.W. Schneider, and R.R. Schulz. Support by the BMBF (project EKM 13N6918) and by the ESF (Pishift-Project) is gratefully acknowledged.

13.3 Doppler effect and the thermal Hall conductivity of quasiparticles in d-wave superconductors by N.P. Ong At temperatures very close to absolute zero, all the electrons in a superconductor are paired. The collection of Cooper pairs constitutes the condensate or superfluid. At finite temperatures T , however, a few of the Cooper pairs break up to form a gas of ‘singles’ called Bogolyubov quasiparticles (the entropy of the quasiparticle gas lowers the sample’s free energy). With increasing T , the quasiparticle population nqp (T ) increases rapidly until all the pairs become singles at the critical transition temperature Tc . The thermal conductivity κ has proved to be a fruitful way to study the transport properties of quasiparticles. In a temperature gradient −∇T , the flow of quasiparticles towards the cooler end generates a thermal current Je (as the condensate itself has zero entropy, it does not contribute to the thermal conductivity). However, the gradient also produces a parallel phonon current Jph which greatly complicates the interpretation of measurements of κ. First, let us consider the normal state of a conventional metal such as Pb. κ is the sum of the electronic term κe and the phonon term κph , viz. κ = κe + κph (κe is about 100 times larger than κph in Pb, but κe is 5-8 times smaller than κph in the cuprates). As T falls below Tc in Pb, the rapid (exponential) decrease of

DOPPLER EFFECT AND THE THERMAL HALL CONDUCTIVITY

377

50

κ (W/mK)

40 0.5 40 K

30 20 10

0.4 0 0

κxy (W/mK)

50

100 50 T(K)

150

0.3

60

0.2

70 0.1 75 K 0.0

0

2

4

6 8 m0 H(T)

10

12

14

Figure 13.6 (Main Panel) Curves of κxy versus the applied field H at selected temperatures in high-purity YBa2 Cu3 O7 . At high T , κxy is linear in H , but as T decreases, its field profile displays a prominent peak. The initial slope limH →0 κxy /H increases by a factor of 1000 between 85 and 40 K. The inset shows the zero-field thermal conductivity κ versus T . A prominent peak appears below Tc = 93 K [adapted from 13].

nqp leads to a sharp decrease in κe . However, this is partially compensated by an increase in κph because the decreasing nqp results in a marked decrease in the scattering of phonons. Hence the total κ in a typical s-wave superconductor decreases rather gradually below Tc . If the sample is of exceptional purity, this gradual decrease is interrupted by a resurgent κ ∼ κph which rises to a prominent peak below ∼ 12 Tc . The phonons, now largely free of any scattering by quasiparticles, develop exceedingly long mean-free-paths (mfp) limited only by the size of the crystal. Eventually, at very low T , κph vanishes as T 3 , reflecting the specific heat of the phonon gas. A major puzzle in the high-Tc cuprates became apparent shortly after the 1987 discovery of the ‘90-K’ superconductor YBa2 Cu3 O7 . Instead of decreasing below Tc , κ is observed to rise sharply, reaching a peak value 2–3 times larger than the value just above Tc = 93 K (inset of Figure 13.6). The origin of the giant anomaly in κ has been a source of debate. Recalling κ in Pb, many investigators initially identified the giant anomaly with a strong enhancement of the mfp of phonons. However, this identification was unconvincing because the quasiparticle population in the cuprates falls quite slowly below Tc (in contrast

378

TOPICAL CONTRIBUTIONS

with Pb). How can we distinguish the phonon and quasiparticle currents in the cuprates? Let us consider applying a magnetic field B normal to the plane of the crystal. The field pierces the condensate as an array of vortices. Quasiparticles do not ‘see’ the applied magnetic field, but they scatter from the vortices (which act like impurities in the otherwise uniform condensate). A quasiparticle incident on a vortex line strongly scatters from the steep decrease in the pair potential at the core. More germane to our discussion, it interacts with the intense azimuthal supercurrent surrounding the core. Generally, the energy of a quasiparticle is shifted in the presence of a superflow. If the quasiparticle moves in a direction parallel to that of the local superfluid velocity (co-moving), its velocity relative to the lattice is increased (this so-called Doppler effect is analogous to viewing a pedestrian walking on a moving ramp). Conversely, a quasiparticle moving against the superfluid has its velocity lowered. The difference in kinetic energies implies that quasiparticles prefer to go around a vortex in the direction against the azimuthal superfluid velocity. If the superflow is clockwise (viewed from above), the incident quasiparticle is preferentially scattered to the left, whereas it is scattered to the right when the flow is counterclockwise. The resulting ‘skew’ scattering produces a net ‘Hall entropy current’ (if −∇T is applied along x with H z, the Hall current is along y and given by Jy = κyx (−∇T ), where κxy is called the thermal Hall conductivity). Phonons, which are charge-neutral, do not experience this asymmetric scattering. Hence the thermal Hall effect acts very much like a selective filter that ignores the phonon current. The thermal Hall effect was detected in high-purity crystals of YBa2 Cu3 O7 and investigated in detail from ∼12 K to temperatures slightly above Tc [12, 13]. In weak fields, κxy increases linearly with H (main panel of Figure 13.6). In high-purity crystals, this linear field dependence evolves into a profile with a prominent peak. The profile is consistent with a very long quasiparticle meanfree-path when the field is absent. If we plot the initial slope κxy /H (H → 0) against T , we find that it displays a remarkable thousand-fold increase [13] between Tc and 30 K that dwarfs the corresponding increase in κ. This is consistent with an increase in of over 100 within this temperature interval. The steep increase is sufficient to produce a giant peak in κe that matches the observed giant anomaly. The thermal Hall effect presents the strongest evidence to date that the giant anomaly derives entirely from the quasiparticles.

13.4 Nanometer-sized defects responsible for strong flux pinning in NEG123 superconductor at 77 K by M. Muralidhar and M. Murakami The bulk superconductor composite of (Nd0.33 Eu0.38 Gd0.28 )Ba2 Cu3 Oy with 5 mol% (Nd0.33 Eu0.33 Gd0.33 )2 BaCuO5 , 0.5 mol% Pt, and 10 wt% Ag2 O exhibits

NANOMETER-SIZED DEFECTS RESPONSIBLE FOR STRONG FLUX PINNING

379

80

Jc (kA cm−2)

2000

60

T = 77K, Hc-axis

1500 1000

Jc (kA cm−2)

500 0

13

40

13.4 13.8 m0Ha (T)

16

Birr (T)

12

20

8 4 0

80

85 90 Ι (Κ)

95

0 0

2

4

6 8 m0Ha (T)

10

12

14

Figure 13.7 Field dependence of the critical current density (Jc ) for the (Nd0.33 Eu0.38 Gd0.28 )Ba2 Cu3 Oy sample with 5 mol% NEG-211, 0.5 mol% Pt, and 10 wt% Ag2 O at 77 K and H ||c-axis. The bottom inset shows the extrapolation of Birr (T).

the irreversibility field (Birr ) over 14 T for B//c axis at 77 K [14]. The critical current density reached 70, 49, and 22 kA/cm2 at 4.5, 7, and 10 T, respectively (see Figure 13.7). The extrapolation of temperature dependence of irreversibility field between 79 K and 94 K measured with a vibrating sample magnetometer indicated the actual Birr value at 77 K about 15 T (bottom inset of Figure 13.7). Structural analyses made by transmission electron microscopy (TEM) revealed a nanometer-scale modulation structure, which had a lamellar structure with spacing of a few nanometers. Similar nano-structures were observed in the NEG123/NEG211 composite samples with 3-7 mol% NEG-211. All the samples exhibited very high irreversibility fields over 12T at 77K [15]. Chemical analysis of the matrix showed that there is a chemical fluctuation in the (Nd+Eu+Gd)/Ba ratio on a nanometer scale. Scanning tunneling microscopy (STM) also confirmed the presence of nano-scale structure as shown in Figure 13.8a. Here its average spacing is around 3.5 nm, which is close to the coherence length of YBCO at 77K (ξab (77 K) ≈ 4.5 nm) [16]. The observation with higher magnification showed that the structure consisted of rows of aligned clusters of slightly off stoichiometric composition of 3–4 nm in size (see Figure 13.8b). These clusters were identified by EDX analysis as (NEG)1.015 Ba1.985 Cu3 Oy . Tunneling current spectra taken on the RE-rich clusters, and the regular matrix showed similar conductivity of both regions. This shows that the composition of the clusters is not much different from that of the 123 matrix.

380

TOPICAL CONTRIBUTIONS

(a)

(b)

Figure 13.8 STM images of the sample with 5 mol% NEG-211 [(a)-(b)]. The image was recorded with bias voltage Vs = 1 V and tunneling current It = 0.3 nA. The black arrows in (a) mark some nanolamellas. Note the presence of arrays of clusters around 3 to 4 nm in diameter dispersed in an organized manner in the NEG-123 matrix.

Thus superior flux pinning of NEG123/NEG211 composites at higher fields and temperatures is ascribed to the formation of new type of nanometer-scale lamellar array of RE-rich clusters. These new pinning medium led to an increase of Birr up to 15 T at 77 K and thus will make it possible to construct a superconducting magnet generating >10 T at liquid nitrogen temperature.

13.5 Hybrid Magnets by H. Schneider-Muntau A hybrid magnet is a combination of a powered resistive magnet (insert) with a surrounding superconducting magnet (outsert). Hybrid magnets are built with the goal to produce the highest continuous magnetic fields possible [17–21]. Design and construction of hybrid magnets are a considerable technological and logistical challenge. Besides the sheer size of the magnet, the interaction of the subsystems, the magnitude of the forces within and between the resistive and the superconducting magnet, the cryogenic requirements, and safe and reliable operation of such a complex system require detailed attention and very specific capabilities in several disciplines. The essential components of a hybrid magnet are: superconducting magnet, the cryostat, the resistive insert, and the quench detection and protection system (see Figure 13.9). The superconducting magnet (Figure 13.10, 13.11) surrounds the resistive magnet. Because of its bore size of 360 mm (Sendai, Nijmegen), 610 mm (Tallahassee) and 800 mm (Grenoble), the magnet becomes impressive in size,

HYBRID MAGNETS BY H. SCHNEIDER-MUNTAU

381

Cryostat housing 80 K shield Resistive coils Superconducting coil (NbTi) Superconducting coils (Nb3Sn) Support column Connection to vacuum pump

Mounting flange

20 K shield

Superfluid helium cunduit

Connection to supply cryostat Superconductor joint box

Access tube Resistive housing

Burst disk

Current connection Helium exhaust Cooling water connection

Figure 13.9 Cross-sectional view of the hybrid magnet at NHMFL. It generates the highest continuous field of 45 T in a bore of 32 mm since June 2000 and has since then provided more than 2000 h per year of measuring time to the international science community.

Figure 13.10 The outsert in construction. It generates 15 T in 615 mm.

382

TOPICAL CONTRIBUTIONS

Figure 13.11 The outsert being put on the central bore tube.

especially if the field contribution is above 8 T. Even more dramatic is the increasing stored energy (in round numbers): from 10 MJ (Nijmegen) to 60 MJ (Tsukuba and future Grenoble hybrid) to 110 MJ (Tallahassee). The energy content and, even more important, the coupling between the two magnet systems make a hybrid outsert much more challenging than a stand-alone, large-bore superconducting magnet. The most important design issues for the outsert are: (a) Changes of the field of the resistive insert result in induced currents. Field changes also induce eddy current heating and coupling losses between the filaments in the superconductor. They are proportional to (dB/dt)2 and define specific requirements for the coupling time constant between filaments. The worst case is an insert trip from full field which can result into an energy deposition of over 20 kJ. (b) The ramp time of the outsert should not be more than approximately one hour in view of its operation in a user facility. The hysteresis losses are proportional to the maximum field and are independent of the ramp rate and define a requirement for the maximum admissible energy deposition as a

HYBRID MAGNETS BY H. SCHNEIDER-MUNTAU

383

function of its evacuation time. These losses can reach values of up to 100 kJ for a high field magnet. Wires with a small effective diameter have lower hysteresis losses. (c) To limit the magnet size, the conductor should operate as closely as possible to its critical current. A high index number will reduce the heating from current sharing. (d) The stability of a magnet against quench depends, among other things, on the amount of stabilizer and the available enthalpy. The presence of helium, especially superfluid helium, within or beside the conductor, increases the margin considerably. (e) In case of a quench, the energy must be extracted from the magnet and discharged into an outer resistor. An alternative solution is to dissipate the energy equally over the volume by firing heaters to quench the magnet uniformly. It is obvious from above that the worst case scenario, for which the outsert magnet must be designed, is an insert trip after a ramp to full field, plus heating through current sharing. The heat must be absorbed and transported out of the conductor with only modest excursion in the local temperature. Therefore, important design criteria are, (a) the operating temperature, and (b) the temperature gradients between current carrying filaments, conductor matrix, surrounding helium, main helium buffer and refrigerator. Three different approaches have been developed for the design of the outsert in response to the requirements listed above. They can be distinguished by the superconductor they employ: the solid, cable-in-conduit and Rutherford cable conductor. The cryostat, together with the cryogenic system, must provide the environment for safe and reliable operation of the superconducting magnet. The operating temperature of the magnet has an important impact on the design of the cryostat and magnet performance. A bath-cooled, ventilated magnet wound from solid conductor and operated at about 4.2 K represents the standard technique and has the great advantage of simplicity. However, operation of the magnet at superfluid helium with its extremely high thermal conductivity and low viscosity, increases magnet performance considerably. The heat transfer between conductor and liquid and, therefore, conductor stability and margin to external disturbances is essentially improved. Also, the critical current density in the superconductor is much higher at lower temperatures. A subcooled 1.8 K superfluid helium bath, including magnet, at atmospheric pressure can be achieved if a 1.8 K heat exchanger is introduced into the main bath. Such a cryostat system consists of a 1.8 K vessel housing the magnet, a 1.8 K heat exchanger, and two radiation shields which are at intermediate temperatures between 4.2 and 100 K, optimized for minimum losses. The magnet is kept at 1.8 K by a thermal exchange loop through expansion of 4.2 K helium in a JouleThomson valve using a vacuum pump. The forces between and within the two magnet systems, the superconducting magnet and the resistive insert, must be considered in the case of axial and radial misalignment of any of the magnetic coil centers. These forces are generated between the current carrying conductors of all coils, and are transmitted through the coil winding and support structure

384

TOPICAL CONTRIBUTIONS

and the cryostat. In case of a major failure, they can reach alarming magnitudes of several MN, which is many times the weight of the superconducting magnet system. The resistive insert magnets have lower efficiency than do stand-alone magnets without background fields (Figure 13.12). The major difficulties are: (a) The reduced volume in which the electric power must be dissipated. For economic

Figure 13.12 The hybrid magnet with view on the support and cooling water connections of the resistive insert. It consumes 30 MW, 300l/s of cooling water are needed. The superconducting magnet is located in the top vessel.

MAGNETO-OPTICAL IMAGING OF VORTEX MATTER BY T.H. JOHANSEN

385

reasons, the magnet engineer has to choose the bore of the superconducting magnet as small as possible and, therefore, the resistive magnet must be very compact and efficiently cooled. (b) The additional field from the outer magnet. The background (booster) field from the superconducting magnet increases the Lorentz forces as the insert experiences the sum of its own and the outer field. Therefore, special high-strength conductors, a multi-coil design and an adequate support structure are required. (c) The high alignment forces between the coils. Impressive forces are generated within the insert and, to a lesser extent, between the insert and the outsert. (d) The forces resulting from the termination of the winding. These endforces are extremely large, resulting from the high fields and the high operating currents. They impact strongly on the design because of their magnitude and the limited space available. An early detection of a quench is important to avoid uncontrolled growth of the resistive zone and destruction through excessive heating. Detecting a quench is difficult because the small resistive voltages must be separated from the large inductive voltages induced when either magnet is swept. The inductive voltages are up to a factor of 1000 higher. Inductive voltages can be cancelled if the magnet is divided into zones of equal inductance and the voltages are compared in bridge fashion, for instance, between taps connected to the winding. In the event of a quench, the protection system must be capable of extracting enough energy from the system that high stresses from differential thermal expansion or even overheating/melting are precluded. This is done by discharging the magnet with a defined time constant into an external resistor. Limiting the maximum or hot-spot temperature to about 150 K and the discharge voltage for fully impregnated coils to 5 kV and for ventilated coils to 3 kV results in time constants of between 3 and 20 seconds, depending on the coil energy. The quench detection and control system of a superconducting outsert is best done with several industrial quality computers. As part of the total control system and its reliability, the safety devices such as the power supply, discharge resistor, breakers, and computers, must be checked continuously for their operational conditions.

13.6 Magneto-Optical Imaging of Vortex Matter by T.H. Johansen Space-resolved magnetic measurements have during the last decades proved increasingly useful in revealing micro-structural features and physical phenomena that control the overall electromagnetic behavior of superconductors. Among the various methods, scanning probe magnetometry, Bitter decoration etc., the technique of magneto-optical (MO) imaging has two major advantages, namely it allows easy zoom from cm-scale field-of-view down to micron resolution, and secondly, the time response is very quick (

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close